SOLID STATE PHYSICS VOLUME 60
Founding Editors FREDERICK SEITZ DAVID TURNBULL
SOLID STATE PHYSICS Advances in Resea...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

SOLID STATE PHYSICS VOLUME 60

Founding Editors FREDERICK SEITZ DAVID TURNBULL

SOLID STATE PHYSICS Advances in Research and Applications

Editors HENRY EHRENREICH FRANS SPAEPEN

Division of Engineering and Applied Sciences Harvard University Cambridge, Massachusetts

VOLUME 60

AMSTERDAM • BOSTON • HEIDELBERG • LONDON • NEW YORK • OXFORD PARIS • SAN DIEGO • SAN FRANCISCO • SINGAPORE • SYDNEY • TOKYO Academic Press is an imprint of Elsevier

Academic Press is an imprint of Elsevier 84 Theobald’s Road, London WC1X 8RR, UK Radarweg 29, PO Box 211, 1000 AE, Amsterdam, The Netherlands 30 Corporate Drive, Suite 400, Burlington, MA 01803, USA 525 B Street, Suite 1900, San Diego, California 92101-4495, USA ∞ This book is printed on acid-free paper

Copyright © 2006, Elsevier Inc. All rights reserved No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means electronic, mechanical, photocopying, recording or otherwise, without the prior written permission of the publisher. Permissions may be sought directly from Elsevier’s Science and Technology Rights Department in Oxford, UK: phone: (+44) (0) 1865 843830; fax: (+44) (0) 1865 853333; e-mail: [email protected] You may also complete your request on-line via the Elsevier homepage (http://www.elsevier.com), by selecting ‘Customer Support’ and then ‘Obtaining Permissions’ ISBN-13: 978-0-12-607760-5 ISBN-10: 0-12-607760-6 ISSN: 0081-1947 For information on all Academic Press publications visit our web site at http://books.elsevier.com Printed and bound in USA 05 06 07 08 09 10

10 9 8 7 6 5 4 3 2 1

Contents C ONTRIBUTORS TO VOLUME 60 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . P REFACE . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

vii ix

Strongly Correlated Electrons P. F ULDE , P. T HALMEIER AND G. Z WICKNAGL I. II. III. IV. V. VI. VII. VIII. IX.

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Special Features of Strong Correlations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Kondo Lattice Systems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Phase Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Partial Localization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Charge Ordering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Geometrically Frustrated Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . High-Energy Excitations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Acknowledgment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

2 8 14 30 48 66 122 147 176 179

Defect-Induced Dynamic Pattern Formation in Metals and Alloys Y. B RÉCHET AND C. H UTCHINSON I. II. III.

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Free Energy Changes, Driving Forces and Energy Input . . . . . . . . . . . . . . . . . . . . . . . . . . Chemical Patterning: Interface-Mediated Transformations: Eutectoid Decomposition and Discontinuous Precipitation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . IV. Structural Defect Patterning: Grain Growth, Recovery and Recrystallization . . . . . . . . . V. Structural Defect Patterning: Irradiation and Plastic Deformation . . . . . . . . . . . . . . . . . . VI. Spatio-Temporal Patterning in Plasticity: The Portevin–Le Chatelier Effect . . . . . . . . . . VII. Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

182 188 192 233 248 273 285

AUTHOR I NDEX . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . S UBJECT I NDEX . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

289 303

This page intentionally left blank

Contributors to Volume 60 Numbers in parentheses indicate the pages on which the authors’ contributions begin.

Y VES B RÉCHET (181) Laboratoire de Thermodynamique et Physico-Chimie Métallurgiques, Institut National Polytechnique de Grenoble, 38402, St. Martin D’Hères, France P ETER F ULDE (1) Max-Planck-Institut für Physik komplexer Systeme, 01187 Dresden, Germany C HRISTOPHER H UTCHINSON (181) Department of Materials Engineering, Monash University, Clayton, 3168, Vic, Australia P ETER T HALMEIER (1) Max-Planck-Institut für Chemische Physik fester Stoffe, 01187 Dresden, Germany G ERTRUD Z WICKNAGL (1) Institut für Mathematische Physik, Technische Universität Braunschweig, 38106 Braunschweig, Germany

This page intentionally left blank

Preface

The article by Fulde, Thalmeier and Zwicknagl traces many of the recent developments in the field of strongly correlated many electron systems. It is very useful both as a reference and a pedagogical exposition since it places these developments into a historical context beginning with early developments in the electron theory of solids. Together with its extensive references and its formal elucidation of important theoretical subjects, the article supplies an excellent entry point into the field which is closely coupled to the classic works on the subject. Many early important ideas, such as Hückel and Heitler–London theory, the Wigner lattice, metal-insulator transitions originated in the thirties and were extensively developed in the sixties when it came to be realized that transition and rare earth metals with their characteristic d and f electrons respectively should be viewed as at least moderately strongly correlated systems requiring more sophisticated theoretical treatments than those supplied by the simplest band theories. The development of the relevant theories are associated with Hubbard and Mott among many others. They introduced model Hamiltonians, which were amenable to easily performed calculation whose results exhibited metal-insulator transitions for appropriate choices of the inter- and intra-atomic physical parameters. The Hubbard Hamiltonian, for example, motivated by lattices containing transition metal constituents has remained, in the authors’ words one of the “working horses of many studies of strongly correlated” electron systems. Even though early conventional applications are limited to d electrons, many of the generic effects of strongly correlated electrons are captured by its solutions. A principal impetus for the development of the field is associated with the discovery of high temperature superconductivity in copper-oxide based perovskites in 1986. Indeed, but for the strong electron correlations in hole-doped superconductors like La2−x Bax CuO4 would be metallic instead of insulating antiferromagnetic. It is the richness of the periodic table resulting from the presence of inner shell electrons in the heavier elements and their associated correlations that is responsible for these otherwise unexpected physical effects. Although superconducting phenomena play an important role in the article, we stress that the principal topic concerns the more general behavior of strongly corix

x

PREFACE

related electrons in solids. The article presents a detailed description of Kondo lattice systems and its associated heavy fermions, which preceded the discovery of high temperature superconductivity. It relates the results to a wide variety of experimental observations in real systems wherever possible. Readers having special interests in given heavy fermion materials will thus be well rewarded by browsing its pages and detailed figures of, for example, Fermi surfaces, photoemission results and phase diagrams. The article begins with a detailed exposition of the physical features that characterize strong electron correlations, and presents a detailed description of the central feature associated with strong correlations leading to the presence of energy scales low compared to the typical metallic Fermi energy possibly resulting in deviations from Fermi-liquid behavior. This introduction is followed by a detailed description of Kondo lattice systems which deal with magnetic impurities associated with spins embedded in a metal and interacting via exchange scattering. The understanding of Ce-based heavy Fermi systems present particular challenges. The authors describe theoretical techniques for describing such systems that combine ab initio approaches with a phenomenologically based Landau theory. A so-called renormalized band scheme is used for calculating realistic quasi-particle bands of materials grown and observed in the laboratory. Quantum phase transitions in localized and itinerant magnetic systems characterize many systems of direct interest here. Quantum criticality in the Kondo lattice and scaling theory close to quantum critical points are discussed in considerable detail. Charge ordering, which began with the notion of crystallization first introduced in the 30s by Wigner was subsequently observed in 2D electron systems. Originating from a variety of effects, charge ordering can occur in many types of systems. For example, Yb4 As3 , which is discussed in considerable detail from both experimental and theoretical points of view in the present exposition, exhibits charge ordering associated with 4f holes. It illustrates the formation of heavy quasiparticles caused by spin chains without involvement of the Kondo effect. Other subjects discussed here include partial localization found in some actinide-based heavy fermion compounds in which experiments are used to infer the co-existence of delocalized and localized 5f electrons, superconductivity mediated by intra-atomic excitations, geometrically frustrated lattices such as metallic spinels, fractional charges resulting from strong correlations, and high energy correlation induced excitations, for example, the appearance of shadow bands and satellites associated with nickel. Because of its significant reliance on and comparison with experiment, its frequent use of phenomenologically based theory used to calculate quasi-particle band structures and Fermi surfaces, this article is to some extent less focussed on

PREFACE

xi

fundamental microscopic theoretical aspects than on techniques leading to optimal physical insight permitting ready comparison with observations relevant to important materials systems. Clearly both types of expositions are needed. The second article in this volume, by Bréchet and Hutchinson, concerns pattern formation in metals and alloys. Spontaneous pattern formation is the development of a regularity, either in the spatial distribution of the material in a system or in its development in time, of a lower symmetry than that of its cause. These phenomena have been of considerable interest to the non-linear physics community, in particular in fluid dynamics and in chemical reactions. This article deals with pattern formation in the solid state, which is comparatively less studied. Usually, crystal defects, such as dislocations or interfaces, play an important role and the energetic cost required by their formation requires that the system be prepared or maintained far from equilibrium. Interface-mediated formation of lamellar microstructures from supersaturated solution is discussed as an example of chemical patterning in a system prepared far from equilibrium. Striking examples are the formation of pearlite and discontinuous precipitation. Grain growth, recovery and recrystallization are discussed as examples of defect pattering in a system prepared far from equilibrium. Grain growth is a rich topological subject, several aspects of which have been presented in earlier articles in this Series, such as that by Weaire and McMurry in vol. 50 and by Thompson in vol. 55. Systems that are maintained far from equilibrium can be called “driven systems”. Martin and Bellon have reviewed the chemical aspects of such systems in their article in vol. 50 of the Series. The present article therefore concentrates more on structural pattering in driven systems, such as the formation of arrays of dislocation loops and voids under irradiation or dislocation patterning in deformation. Finally, plastic deformation provides an interesting example of pattering in both space and time: the Portevin–Le Chatelier effect, which is a stick-slip effect of plastic waves that move through the sample. The authors show that this can be usefully analyzed as a case of self-organized criticality. H ENRY E HRENREICH F RANS S PAEPEN

This page intentionally left blank

SOLID STATE PHYSICS VOLUME 60

This page intentionally left blank

SOLID STATE PHYSICS, VOL. 60

Strongly Correlated Electrons

P ETER F ULDE Max-Planck-Institut für Physik komplexer Systeme, 01187 Dresden, Germany

P ETER T HALMEIER Max-Planck-Institut für Chemische Physik fester Stoffe, 01187 Dresden, Germany

G ERTRUD Z WICKNAGL Institut für Mathematische Physik, Technische Universität Braunschweig, 38106 Braunschweig, Germany

I. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . II. Special Features of Strong Correlations . . . . . . . . . . . . . . . . . . . . . . . . . . . 1. Low-Energy Scales: a Signature of Strong Correlations . . . . . . . . . . . . . . . 2. Deviations from Fermi-Liquid Behavior . . . . . . . . . . . . . . . . . . . . . . . . III. Kondo Lattice Systems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3. Fermi-Liquid State and Heavy Quasiparticles: Renormalized Band Theory . . . . . 4. Heavy Fermions in CeRu2 Si2 and CeCu2 Si2 . . . . . . . . . . . . . . . . . . . . . 5. Low-Temperature Phase Diagram of CeCu2 Si2 . . . . . . . . . . . . . . . . . . . . IV. Quantum Phase Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6. Quantum Phase Transition in Localized and Itinerant Magnets . . . . . . . . . . . . 7. Quantum Criticality in the Kondo Lattice . . . . . . . . . . . . . . . . . . . . . . . 8. Scaling Theory Close to the Quantum Critical Point . . . . . . . . . . . . . . . . . V. Partial Localization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9. Heavy Quasiparticles in UPd2 Al3 . . . . . . . . . . . . . . . . . . . . . . . . . . . 10. Microscopic Model Calculation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11. Superconductivity Mediated by Intra-Atomic Excitations . . . . . . . . . . . . . . VI. Charge Ordering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12. Wigner Crystallization in Homogeneous 2D Electron Systems . . . . . . . . . . . . 13. Generalized Wigner Lattice: Yb4 As3 . . . . . . . . . . . . . . . . . . . . . . . . . 14. Charge Ordering and 1D Spin Excitations in α -NaV2 O5 . . . . . . . . . . . . . . 15. Reentrant Charge Ordering and Polaron Formation in Double Exchange Bilayer Manganites La2−2x Sr1+2x Mn2 O7 . . . . . . . . . . . . . . . . . . . . . . . . . . . VII. Geometrically Frustrated Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16. Metallic Spinels: LiV2 O4 — a Metal with Heavy Quasiparticles . . . . . . . . . .

2 8 10 12 14 18 19 23 30 32 38 45 48 51 54 59 66 69 74 91 108 122 125

1 ISBN 0-12-607760-6 ISSN 0081-1947/06

© 2006 Elsevier Inc. (USA) All rights reserved.

2

P. FULDE ET AL.

17. Structural Transition and Charge Disproportionation: AlV2 O4 18. Fractional Charges Due to Strong Correlations . . . . . . . . . VIII. High-Energy Excitations . . . . . . . . . . . . . . . . . . . . . . . . 19. Projection Operators . . . . . . . . . . . . . . . . . . . . . . . . 20. The Hubbard Model: Appearance of Shadow Bands . . . . . . 21. Marginal Fermi Liquid Behavior and Kink Structure . . . . . . 22. Nickel and its Satellite . . . . . . . . . . . . . . . . . . . . . . . 23. Multiplet Effects in 5f Systems . . . . . . . . . . . . . . . . . 24. Excitations in Copper-Oxide Planes . . . . . . . . . . . . . . . IX. Summary and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . Acknowledgment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . List of Acronyms . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

133 139 147 149 151 153 163 168 171 176 179 179

I. Introduction

The field of strongly correlated electron systems has been constantly growing for almost three decades. A milestone in its development was the discovery by Andres, Graebner and Ott1 of heavy-quasiparticle excitations in CeAl3 . Additional verve came from the discovery of superconductivity in the related compounds CeCu2 Si2 ,2 UBe13 3 and UPt3 .4 But a real great push for the field was provided by the discovery of high-temperature superconductivity in the copperoxide based perovskites.5 Were it not for strong electron correlations La2 CuO4 , one of the key compounds of that class of materials and the basis of the hole doped superconductors La2−x Bax CuO4 and La2−x Srx CuO4 would be metallic. Instead it is an antiferromagnet which remains insulating even above the Néel temperature where the unit cell is not doubled anymore. Therefore, electron correlations are apparently so strong that the metallic character of the material is suppressed in favor of an insulating state. That electron correlation may induce a metal to insulator transition had been suggested long before the discovery of heavy quasiparticles and high-Tc cuprates. The names of Mott6 and Hubbard7 stand for that phenomenon. At their time the interests in the effects of strong correlations resulted from the transition metal oxides and their various phase transitions. It is 1 K. Andres, J. E. Graebner, and H. R. Ott, Phys. Rev. Lett. 35, 1779 (1975). 2 F. Steglich, J. Aarts, C. D. Bredl, W. Liecke, D. Meschede, W. Franz, and H. Schäfer, Phys. Rev.

Lett. 43, 1892 (1979). 3 H. R. Ott, H. Rudigier, Z. Fisk, and J. L. Smith, Phys. Rev. Lett. 50, 1595 (1983). 4 G. R. Stewart, Z. Fisk, J. O. Willis, and J. L. Smith, Phys. Rev. Lett. 52, 679 (1984). 5 J. G. Bednorz and K. A. Müller, Z. Phys. B 64, 189 (1986). 6 N. F. Mott, Metal–Insulator Transition, Taylor and Francis, London (1990), 2nd ed. 7 J. Hubbard, Proc. R. Soc. London A 276, 238 (1963).

STRONGLY CORRELATED ELECTRONS

3

worth recalling that the famous Verwey8 transition in magnetite Fe3 O4 falls into the same category. One may even go back to Wigner9 or Heitler and London10 who dealt with strongly correlated electrons long before corresponding experiments were available. While Wigner pointed out that electrons may form a lattice when their correlations become sufficiently strong, Heitler and London developed a theory for chemical bonding based on strongly correlated electrons. It is the opposite limit of Hückel’s theory11–13 based on molecular orbitals in which electron correlations are completely neglected. This raises the question of how to quantify the strength of electronic correlations. For example, one would like to know how much more strongly electrons are correlated in LaCu2 O4 than, e.g., in iron or nickel or in transition metal oxides. The differences between systems with strongly and with weakly correlated electrons may be seen by considering the ground state of the simplest possible example, i.e., of a H2 molecule in the Heitler–London- and in the molecular orbital limit. The Heitler–London form of the ground-state wavefunction is 1 ψHL r1 , r2 = φ1 (r1 )φ2 (r2 ) + φ2 (r1 )φ1 (r2 ) (α1 β2 − β1 α2 ) 2

(1.1)

where the single-electron wavefunctions φ1,2 (r) are centered on atoms 1 and 2 of the molecule and α and β denote spinors for up and down spins. In distinction to Eq. (1.1) the molecular-orbital form of the ground-state wavefunction is ψMO (r1 , r2 ) =

1 φ1 (r1 )φ1 (r2 ) + φ1 (r1 )φ2 (r2 ) + φ2 (r1 )φ1 (r2 ) (1.2) + φ2 (r1 )φ2 (r2 ) (α1 β2 − β1 α2 ).

23/2

It is seen that ψMO (r1 , r2 ) but not ψHL (r1 , r2 ) contains ionic configurations φ1 (r1 )φ1 (r2 ) and φ2 (r1 )φ2 (r2 ). In Eq. (1.2) they have equal weight as the nonionic configurations. But ionic configurations cost additional Coulomb repulsion energy of the electrons. Therefore they are completely suppressed in the Heitler– London- or strong correlation limit. This demonstrates an important feature of electron correlations, namely a partial suppression of electronic charge fluctuations on an atomic site. The former are called interatomic correlations because charge fluctuations at an atomic site are caused by an overlap of wavefunctions of 8 E. J. W. Verwey and P. W. Haayman, Physica 8, 979 (1941). 9 E. Wigner, Phys. Rev. 46, 1002 (1934). 10 W. Heitler and F. London, Z. Phys. 44, 455 (1927). 11 E. Hückel, Z. Phys. 70, 204 (1931). 12 E. Hückel, Z. Phys. 72, 310 (1931). 13 E. Hückel, Z. Phys. 76, 628 (1932).

4

P. FULDE ET AL.

different atoms. They are favored by a kinetic energy gain due to electron delocalization. Reducing them compared with uncorrelated electrons keeps the Coulomb repulsions small. In addition to interatomic correlations we must also consider intra-atomic correlations. Consider an atom of a solid in a configuration with a given number of electrons, for example, a C atom in diamond with, e.g., 4 or 5 valence electrons. Those electrons will optimize their on-site Coulomb repulsions by arranging according to Hund’s rules and by in-out correlations. Hund’s rules ensure that electrons on an atom are optimally distributed over the angular segments of the atom, so that their repulsions are as small as possible. In-out correlations achieve the same by proper radial distribution of the electrons. Intra-atomic correlations are strongest for 4f electrons, i.e., for atoms or ions of the lanthanide series. But also in actinides or transition-metals they play a big role. Large overlaps with atomic wavefunctions of the chemical environment will weaken them. This is understandable: before the electrons can fully establish intra-atomic correlations they leave for the neighboring sites by hopping off the site. Interatomic correlations can be strong even when intra-atomic correlations are moderate or weak. Let us make a gedanken experiment and consider a Si crystal with artificially enlarged lattice parameter. The intra-atomic correlations on a Si site are fairly moderate, but the interatomic correlations are becoming strong when the lattice constant is increased, i.e., when the limit of separate atoms is approached. In that case fluctuations in the electron number at a site reduce to zero. From the above considerations it follows that a suitable measure of the interatomic correlation strength is the reduction of electron number fluctuations on a given atom. An independent-electron or Hartree–Fock description implies too large fluctuations. Let |ψ0 denote the exact ground state of an electronic system and |SCF the corresponding self-consistent field (SCF) or Hartree–Fock (HF) state. The normalized mean-square deviation of the electron number ni on atom i is given by (i) =

SCF |(ni )2 |SCF − ψ0 |(ni )2 |ψ0 SCF |(ni )2 |SCF

(1.3)

where ni = ni − n¯ i and n¯ i denotes the average value. One notices that 0 (i) 1. When (i) = 0 the interatomic correlations vanish, i.e., the Coulomb repulsions between the electrons can be treated in mean-field approximation. In a solid atoms or ions with strongly correlated electrons have (i) values near unity. One can also define a correlation strength for different bonds instead of atoms. In that case the denominator is modified when heteropolar bonds are considered. Then we must subtract from SCF |(ni )2 |SCF a term (n)2pc . It takes into account that some number fluctuations are required even when the electrons are perfectly correlated in order to ensure a heteropolar charge distribution within

STRONGLY CORRELATED ELECTRONS

5

the bond. Let αp denote the bond polarity. It is defined by the difference in the average occupation numbers of the two half-bonds 1 and 2 which form the heteropolar bond, i.e., n¯ 1(2) = (1 ± αp ). In that case (n)2pc = αp (1 − αp ). Those considerations apply to a solid as well as to a molecule. For the H2 molecule one checks immediately that approximating |ψ0 by ψMO (r1 , r2 ) gives = 0 while a replacement by ψHL (r1 , r2 ) yields = 1 since ψ0 |(n)2 |ψ0 = 0 in that case. For a C=C or N=N π bond one finds ≈ 0.5 while for a C–C or N–N σ bond = 0.30 and 0.35, respectively. Let us consider the ground state of La2 CuO4 and let P (dν ) denote the probability of finding ν 3d electrons on a given Cu site. Within the independent electron or Hartree–Fock approximation the average d count is found to be n¯ d 9.5 and the probabilities of different configurations are P (d10 ) = 0.56, P (d9 ) = 0.38 and P (d8 ) = 0.06. When correlations are included, i.e., the correlated ground state |ψ0 is used the average d electron number changes to n¯ d 9.3 and P (d10 ) = 0.29, P (d9 ) = 0.70 while P (d8 ) = 0.0. One notices that the d8 configurations are almost completely suppressed in agreement with photoemission experiments. The fluctuations between the d9 and d10 configurations are fixed by the value of n¯ d . A similar analysis for the oxygen atoms reveals that there the 2p4 configurations are not completely suppressed because the Coulomb integrals are not as large as for Cu. Indeed, these configurations are important for superexchange to occur, which determines the antiferromagnetic coupling between Cu ions. In accordance with the above consideration one finds (Cu) 0.8 and (O) 0.7.14 So indeed, correlations are quite strong in La2 CuO4 . On the other hand, they are still smaller than those of 4f electrons in a system like CeAl3 . A measure for the strength of intra-atomic correlations is more difficult to define. One way is by finding out to which extent Hund’s rule correlations are building up on a given atomic site i. A possible measure for that is the degree of spin alignment at a given atomic site i (1.4) Si2 = ψ0 S2 (i)ψ0 where S(i) = ν sν (i) and sν (i) is the spin operator for orbital ν. The quantity Si2 should be compared with the values when the SCF ground-state wavefunction |SCF is used and when instead the ground state |loc in the limit of complete suppression of interatomic charge fluctuations is taken, i.e., for large atomic distances. Therefore we may define Si2 =

ψ0 |S2 (i)|ψ0 − SCF |S2 (i)|SCF loc |S2 (i)|loc − SCF |S2 (i)|SCF

14 A. Ole´s, J. Zaanen, and P. Fulde, Physica B 148, 260 (1987).

(1.5)

6

P. FULDE ET AL.

as a possible measure of the strength of intra-atomic correlations. Note that 0 Si2 1. For example, for the transition metals Fe, Co and Ni Si2 is approximately 0.5. Those findings show that the much discussed transition metals are just in the middle between the limits of uncorrelated and strongly correlated electrons. Hund’s rule correlations are important in them but relatively large overlaps of atomic wavefunctions on neighboring sites prevent their complete establishment. Starting from the work of Slater15 and Van Vleck16 in particular Friedel,17 Gutzwiller,18,19 Hubbard20 and Kanamori21 have discussed their effects in detail. One of the outcomes of the studies of transition metals is the Hubbard Hamiltonian. It was in fact used independently also by Gutzwiller and in a slightly modified version by Kanamori. This Hamiltonian was extensively treated in various approximations. The multiband Hubbard model has remained until present times the working horse of many studies of strongly correlated electrons.22,23 The shortcomings of that model are known. For example, it considers d electrons only, i.e., s electrons are neglected. Also it cannot provide for orbital relaxations when electrons hop on or off a site because only one basis function per atomic orbital is used. Nevertheless, it is believed that it covers the most important generic effects of strongly correlated electrons. The valence electrons which are most strongly correlated are the 4f ones because their atomic wavefunction is close to the nucleus and the tendency to delocalize is very small. In fact, in intermetallic rare-earth compounds only f -electrons in Ce or Yb ions show a noticeable degree of itineracy. The consequence are new low-energy scales which may appear in those compounds and as a result heavy-quasiparticle excitations. Not always do quasiparticles show conventional Fermi liquid behavior which governs the low-temperature thermodynamic properties of many metals. In a number of cases one observes what is called non-Fermi liquid behavior, i.e., quantities like the temperature dependence of the specific heat or of the susceptibility deviate from normal metallic behavior. In particular this holds true near a quantum critical point where apparently no characteristic energy scale is prevailing. Fermi liquid behavior requires that at low temperatures all thermodynamic quantities scale with kB T ∗ , a characteristic energy which in 15 J. C. Slater, Phys. Rev. 49, 537 and 931 (1936). 16 J. H. V. Vleck, Rev. Mod. Phys. 25, 220 (1953). 17 J. Friedel, The Physics of Metals: 1. Electrons, Cambridge Univ. Press, Cambridge (1969). 18 M. C. Gutzwiller, Phys. Rev. A 134, 923 (1964). 19 M. C. Gutzwiller, Phys. Rev. A 137, 1726 (1965). 20 J. Hubbard, Proc. R. Soc. London A 281, 401 (1964). 21 J. Kanamori, Progr. Theor. Phys. 30, 275 (1963). 22 M. Imada, A. Fujimori, and Y. Tokura, Rev. Mod. Phys. 70, 1039 (1998). 23 F. Mancini and A. Avella, Adv. Phys. 53, 537 (2004).

STRONGLY CORRELATED ELECTRONS

7

strongly correlated electron systems takes the role of the Fermi energy. When such a characteristic scale does not exist deviations from Fermi liquid behavior do occur. In a way it is more astonishing that to good approximation Fermi liquid behavior is observed in a number of strongly correlated electron systems than that it is not. A study of the Hubbard model shows ways for obtaining deviations from standard features of a metal. One interesting aspect of strong electron correlations is the possible occurrence of charge order. A charge ordered state minimizes the repulsive energy between electrons at the expense of the kinetic energy. Wigner was the first to study this subject by considering a homogeneous electron gas and specifying the conditions under which the formation of an electronic lattice is possible. Chances for charge ordering are larger for inhomogeneous systems, i.e., lattices than for homogeneous ones, the reason being that the kinetic energy gain of electrons due to delocalization may become very much reduced as compared with homogeneous electron systems. A prototype example is Yb4 As3 where charge order occurs close to room temperature and there are many other cases. While 4f electrons are localized in most cases and are very strongly correlated, 5f electrons are more delocalized but still more strongly correlated as, e.g., 3d electrons in transition metals. It turns out that in this case a dual picture applies: while 5f electrons become itinerant in some of the orbitals they remain localized in others. Such a model explains very well a number of experiments on U compounds. Heavy quasiparticles have also been observed in LiV2 O4 , a metal with 3d electrons. A special feature of that material is that the 3d electrons are placed on a pyrochlore or geometrically frustrated lattice. Model calculations show that charge degrees of freedom of strongly correlated electrons in frustrated lattice structures can give rise to new phenomena at special band fillings. There may exist large numbers of low-energy excitations for which Landau’s Fermi liquid approach fails and there may be even excitations with fractional electron charges. Although phenomena of this kind have not been observed yet, the theoretical results may stimulate further thinking. Strongly correlated electrons show in addition to the quasiparticle bands also satellite structures in photoemission experiments. They are contained in the incoherent part of the one-particle Green function. It appears that detailed studies of the incoherent part of Green’s function have not been done to the extent they deserve. The reason for their importance is the following. A quasiparticle in a solid can be considered as a bare particle (electron or hole) surrounded by a correlation hole. The whole object, i.e., particle plus correlation hole moves in form of a Bloch wave through the system. The internal degrees of freedom of the correlation hole give rise to excitations which are contained in the incoherent part of Green’s function. Therefore it is very instructive to study general features of

8

P. FULDE ET AL.

that incoherent part. Hubbard’s upper band can be considered a satellite feature for filling factors n < 1/2, i.e., for less than one electron per site. Other examples will be presented. It is impossible to cover all aspects of strongly correlated electrons in a review of reasonable size. Therefore selections have to be made. Naturally, authors select topics for reviews for which they feel particularly competent. These are usually areas in which they have actively worked. This holds also true here and the selection we made may do injustice to other interesting developments in fields not covered here. So we apologize for an incomplete covering of topics as well as for incomplete lists of contributions of authors to the subjects discussed here. II. Special Features of Strong Correlations

Metals with strongly correlated electrons exhibit characteristic deviations from the behavior of independent electrons. The latter are reflected in thermodynamic and transport properties as well as in the high energy spectra. Traditional electron theory of metals proceeds from the electron gas model formulated by Sommerfeld and Bethe.24 The electrons are described as a system of non-interacting fermions. The eigenstates are formed by filling single-particle levels in a manner consistent with the Pauli principle which permits at most one electron per spin direction to occupy any single-electron level. The ground state of an N electron state is obtained by filling the N/2 single particle levels with the lowest energies. It is non-degenerate and characterized by a surface in k-space separating the occupied levels from their unoccupied counterparts. The existence of this surface, the Fermi surface, follows directly for a system of independent electrons. But note that the observation of a Fermi surface does not imply that the independent electron approximation is a valid description of a system. The lowtemperature properties which are dominated by the low-energy excitations are universal, the detailed character of the system under consideration being reflected in a characteristic energy—the Fermi energy EF . The energy scale is set by the variation of the single particle levels with wave number k. A measure of it is the Fermi velocity vF . The linear variation with temperature of the specific heat, C(T ) γ T , and the temperature-independent magnetic susceptibility, χs (T ) → const are also characteristic features of free electrons. Finally, the spectrum for adding or removing a particle in a single-particle level k, σ to the ground state A(k, ω), exhibits a well-defined peak A(k, ω) = δ(ω − k )

(2.1)

24 A. Sommerfeld and H. Bethe, Elektronentheorie der Metalle, vol. 24/2 of Handbuch der Physik,

Springer, Berlin, Heidelberg (1933), 2nd ed.

STRONGLY CORRELATED ELECTRONS

9

of weight unity centered at the single-particle energy k . The independent electron model has proven to be very successful in explaining experimentally observed properties of simple metals. That was a surprise for some time since electron– electron repulsions are not weak in any metal and one might therefore expect that they modify strongly the properties of a system of independent electrons. That this is not necessarily the case was shown by Landau.25–28 The Landau theory assumes that there exists a one-to-one correspondence between the excitations of the complex interacting electron system and those of independent electron. The former are called quasiparticles and their orbitals and energies E(k) are determined from an effective Hamiltonian. It contains an effective, not necessarily local potential. The many-body aspects are contained in the construction of the effective potential which must be determined specifically for the problem under consideration. The quasiparticle energies may be altered when the overall configuration is changed. A characteristic feature of interacting Fermi liquids is that the energy dispersion E˜ σ (k) of a quasiparticle depends on how many other quasiparticles are present,

E˜ σ (k) = E(k) + fσ σ (k, k )δnσ (k ). (2.2) k σ

Here E(k) denotes the energy dispersion of a quasiparticle when there are no other quasiparticles around (dilute gas limit). In systems with strong correlations it reflects the electron interactions and hence cannot be calculated from the overlap of single-electron wave functions. Interactions among quasiparticles are characterized by the matrix fσ σ (k, k ). The deviations from a step-function-like Fermi distribution f (E(k), T = 0) are given by δnσ (k). The scattering amplitudes fσ σ (k, k ) are parameterized and the parameters are adjusted to experiments. Their form is strictly applicable only to a homogeneous translationally invariant electron system. Therefore applying it to an inhomogeneous periodic solid requires some modifications (see, e.g., Ref. [29]) which are usually not discussed. From this point of view Landau’s theory is more of a useful theoretical concept rather than a quantitative computational scheme. The assumed one-to-one correspondence of the excitations implies that the low temperature thermodynamic properties resemble those of independent electrons but with renormalized parameters such as the effective electron or hole 25 L. D. Landau, Zh. Eksp. Teor. Fiz. 30, 1058 (1956). 26 L. D. Landau, Zh. Eksp. Teor. Fiz. 32, 59 (1957). 27 L. D. Landau, Zh. Eksp. Teor. Fiz. 35, 97 (1958). 28 A. A. Abrikosov, L. P. Gorkov, and I. E. Dzyaloshinski, Methods of Quantum Field Theory in

Statistical Physics, Prentice-Hall, Englewood Cliffs, New York (1963). 29 P. Fulde, J. Keller, and G. Zwicknagl, in Solid State Physics, vol. 41, eds. H. Ehrenreich and

D. Turnbull, Academic Press, New York (1988), p. 1.

10

P. FULDE ET AL.

mass. Also the weight of the peak in the spectral density A(k, ω) is modified to Z · δ(ω − E(k)) where the renormalization factor 0 < Z 1 describes the weight of the bare electron in the quasiparticle. The latter contains in addition to the bare electron also the correlation hole around it. An interacting electron system to which Landau’s theory applies has also a Fermi surface. Luttinger has proven30 that in case that perturbation theory is applicable the volume enclosed by the Fermi surface is independent of the electron interactions. Another important property of quasiparticles is that they can be considered as ‘rigid’ with respect to low-energy and long-wavelength perturbations. That is to say that excitations involving degrees of freedom of the correlation hole show up at high energies only and are neglected as regards low-temperature properties. They are discussed in Section VIII. When electron correlations are strong the quasiparticle concept is still applicable for a number of substances. In that case the renormalization factor Z may become very small. This results in heavy quasiparticles because the Fermi velocity is reduced by the same factor. Probably in many cases the one-to-one correspondence between the excitations of a strongly correlated electron system and a corresponding system of independent electrons is only approximately fulfilled. But then the low-temperature properties of the system may still look very similar to those of independent electrons with renormalized parameters. For example, the specific heat will still be nearly linear in T at low temperatures etc. However, we want to stress that from the observation of a specific heat linear in T or a temperature independent spin susceptibility in the low temperature regime one may not conclude that the quasiparticle picture is applicable. In fact, Luttinger liquids in quasi-one-dimensional systems show many properties as quasiparticles do. This is so despite the fact that the key assumption of a one-toone correspondence of excitations to those of independent electrons is unjustified here. There are strongly correlated systems where the quasiparticle picture seems totally inappropriate. This is outlined in the following Section II.2 and discussed in more detail in various sections of this chapter. 1. L OW-E NERGY S CALES : A S IGNATURE OF S TRONG C ORRELATIONS As mentioned above, the characteristic energy scale of a free electron gas is the Fermi energy EF or, alternatively the Fermi temperature TF . A typical value for EF is 5 eV corresponding to a TF of 5 · 104 K. A special feature of strongly correlated electrons is that they introduce new low-energy scales. It is customary to associate a temperature T ∗ with them. In metals with heavy quasiparticles, i.e., with very strong electron correlations T ∗ ranges from a few Kelvin to a few 30 J. M. Luttinger and J. C. Ward, Phys. Rev. 118, 1417 (1960).

STRONGLY CORRELATED ELECTRONS

11

hundred Kelvin. As correlations become weaker T ∗ increases until it is no longer justified to speak of a separate low-energy scale. The microscopic origin of the low-energy scales can be quite different. A widely recognized case is the Kondo effect. Here T ∗ is the Kondo temperature, i.e., it is given by the binding energy of the spins of the conduction electrons to local spins. Local spins imply incomplete inner shells of an atom or ion. The fact that they remain partially filled only, when surrounded by conduction electrons is due to strong correlations. Any conduction electron which tries to enter the incomplete inner shell is expelled by strong on-site Coulomb repulsion. An example are Ce3+ ions immersed in a sea of (generally) weakly correlated conduction electron. Due to a weak hybridization the number of 4f electrons is nearly one. It forms a singlet with the conduction electrons. The aforementioned CeAl3 falls into that category. Breaking those singlets results in low-energy excitations and fixes the low-energy scale T ∗ . The lowenergy excitations make it plausible that there will be a large low-temperature specific heat. To explain heavy quasiparticles the singlet-triplet excitations on different sites must lock together and form coherent Bloch-like excitations. That takes place at a somewhat lower energy scale Tcoh . One expects that Tcoh is of order of T ∗ but no detailed theory for a relation between the two temperatures is available. There is also no theory existing which tells us that the coherent excitations are in one-to-one correspondence to excitations of (nearly) free electrons. Nevertheless this assumption has worked remarkably well. The origin of a low T ∗ is quite different in the strongly correlated semimetal Yb4 As3 . Here the Coulomb repulsion of the 4f holes in neighboring Yb ions leads to charge order in the form of well separated chains of Yb3+ ions. Spin excitations in those chains by which light mobile 4p holes of As are scattered, lead to low temperature properties which resemble very much those of other systems with heavy quasiparticles.31,32 Despite of this the system is not really a heavy Landau Fermi liquid any more as is explained in the next subsection and discussed in more detail in Section VI.13. A third mechanism is found to be responsible for a low energy scale T ∗ in U compounds like UPd2 Al3 or UPt3 . Strong intra-atomic or Hund’s rule correlations lead here to pronounced anisotropies of the effective hybridization of different 5f orbitals. As a result some of the 5f electrons remain localized while others delocalize. The crystalline environment lifts degeneracies of the localized electrons on a low energy scale. The delocalized or itinerant electrons couple to the excitations of the local system and in this way generate a low T ∗ .33 Heavy quasiparticles may also appear near a quantum critical point like in YMn2 .34 31 P. Fulde, B. Schmidt, and P. Thalmeier, Europhys. Lett. 31, 323 (1995). 32 M. Kohgi, K. Iwasa, J.-M. Mignot, A. Ochiai, and T. Suzuki, Phys. Rev. B 56, R11388 (1997). 33 G. Zwicknagl and P. Fulde, J. Phys.: Condens. Matter 15, S1911 (2003). 34 C. Pinettes and C. Lacroix, J. Phys. Cond. Mat. 6, 10093 (1994).

12

P. FULDE ET AL.

Finally, in Ce doped Nd2 CuO4 a fourth origin of a low T ∗ is observed. Here it is essentially a fluctuating internal molecular field originating from the Nd ions which causes a low energy scale in the strongly correlated d-electron system of the Cu–O planes to which is couples.35,36 It seems obvious that there will be other physical processes identified in the future resulting in low-energy scales of strongly correlated electron systems. 2. D EVIATIONS FROM F ERMI -L IQUID B EHAVIOR There is no obvious reason why strongly correlated metallic electron systems should be Fermi liquids. But as pointed out above a large number of them behave very nearly like ordinary metals, i.e., Fermi liquids with renormalized parameters like the effective mass. Even in these cases, high energy excitations show characteristic satellite structures which reflect strong correlations in partially filled inner shells. This topic is discussed in Section VIII. However, there are also numerous examples where the Fermi liquid concept for low-energy excitations is not applicable. One much discussed item is the separation of charge and spin degrees of freedom and moreover the appearance of fractional charges. Separate spin and charge excitations occur always when electron correlations are so strong that the electrons remain localized. In that case the coupling of spins on different sites leads to magnetic excitations with energies of order J , the intersite coupling constant. In contrast, charge excitations from the partially filled inner shells as observed, e.g., by photoelectron spectroscopy have much higher energies. But this kind of spin-charge separation is trivial and does not require further consideration. It is well known that in one dimension (1D) spin and charge degrees of freedom lead to different kinds of excitations even when the correlations are weak (Luttinger liquid). For a review see, e.g., Ref. [37]. Spin-charge separation is also found for kink excitations (solitons) in polyacethylene.38 Those excitations exist even within the independent electron approximation, but require inclusion of lattice degrees of freedom. Doped polyacethylene can have also excitations with fractional charges, again within the one-electron picture but requiring lattice (chain) deformations.39 In 2D electron correlations, e.g., in semiconducting inversion layers may become strong when a magnetic field is applied perpendicular to the 35 T. Brugger, T. Schreiner, G. Roth, P. Adelmann, and G. Czjzek, Phys. Rev. Lett. 71, 2481 (1993). 36 P. Fulde, V. Zevin, and G. Zwicknagl, Z. Phys. B 92, 133 (1993). 37 A. O. Gogolin, A. A. Nersesyan, and A. N. Tsvelik, Bosonization and Strongly Correlated Systems,

Cambridge University Press, Cambridge (1998). 38 W. P. Su, J. R. Schrieffer, and A. J. Heeger, Phys. Rev. Lett. 42, 1698 (1979). 39 W. P. Su and J. R. Schrieffer, Phys. Rev. Lett. 46, 738 (1981).

STRONGLY CORRELATED ELECTRONS

13

plane. The kinetic energy of the electrons is strongly reduced in a high field and therefore the Coulomb repulsions become dominant. This results in the fractional quantum Hall effect (FQHE) and quasiparticles with fractional charges.40 Thus in two dimensions electron correlations are essential for the appearance of fractional charges. The same holds true for 3D systems. There it turns out that excitations with fractional charges may exist in certain geometrically frustrated lattice structures like the pyrochlore lattice.41,42 There is also spin-charge separation. A Fermi liquid description is inapplicable here. This intriguing possibility is discussed in Section VII. Another interesting case of a breakdown of Landau’s Fermi liquid description is found in Yb4 As3 . This system is metallic in a high temperature phase and semimetallic in the low temperature phase.32,43 The change is related to a partial electronic charge order in form of well separated Yb3+ chains with an effective spin 1/2 per site. It is well known that a Heisenberg spin chain has a specific heat of the form C = γ T like a metal. It is due to spinons which obey Fermi statistics. The reader should note that in one dimension one can convert fermions into bosons and vice versa.44 The coefficient γ is large here because of a weak coupling of the spins in a chain and therefore the specific heat resembles that of heavy quasiparticles.31 But the charge carriers, which are mainly 4f holes in the high temperature phase consist of a small number of As 4p holes in the low temperature phase.45 Therefore one may speak of spin-charge separation and a breakdown of the conventional Fermi liquid picture. The one-to-one correspondence between the excitations in the low temperature phase and those of an independent electron system is no longer given. Nevertheless the system shows many properties of an ordinary metal with heavy quasiparticles at low temperature. A detailed discussion of that interesting material is found in Section VI. Another form of deviation from classical Fermi liquid behavior is found in the cuprates perovskite structures. In the underdoped regime many of their physical properties show marginal Fermi liquid behavior.46,47 This implies that they can be described by assuming a frequency dependence of the electron self-energy (ω) for small values of ω of the form Re (ω) ∼ ω ln ω,

Im (ω) ∼ |ω|

(2.3)

40 R. B. Laughlin, Phys. Rev. Lett. 50, 1395 (1983). 41 P. Fulde, Adv. Physics 51, 909 (2002). 42 E. Runge and P. Fulde, Phys. Rev. B 70, 245113 (2004). 43 A. Ochiai, T. Suzuki, and T. Kasuya, J. Phys. Soc. Jpn. 59, 4129 (1990). 44 A. Luther and I. Peschel, Phys. Rev. B 12, 3908 (1975). 45 V. N. Antonov, A. N. Yaresko, A. Y. Perlov, P. Thalmeier, P. Fulde, P. M. Oppeneer, and H. Eschrig,

Phys. Rev. B 58, 9752 (1998). 46 C. M. Varma, P. B. Littlewood, S. Schmitt-Rink, E. Abrahams, and A. Ruckenstein, Phys. Rev. Lett.

63, 1996 (1989). 47 P. B. Littlewood and C. M. Varma, J. Appl. Phys. 69, 4979 (1991).

14

P. FULDE ET AL.

instead of the Fermi-liquid form Re (ω) ∼ ω,

Im (ω) ∼ ω2 .

(2.4)

The latter would be required for the one-to-one correspondence of the excitations. The relations (2.3) hold only for T < ω. Otherwise T replaces ω. They yield, e.g., a resistivity ρ(T ) ∼ T as is observed in a number of the strongly correlated cuprates. The microscopic origin of marginal Fermi liquid behavior in the presence of strong electron correlations has been an open problem. It is also unclear down to which small ω (or T ) values the relations (2.3) must hold in order to explain the relevant experiments. It is shown in Section VIII that marginal Fermi liquid behavior is obtained for a certain parameter range of the Hubbard Hamiltonian on a square lattice near half filling when the one-site Coulomb repulsions dominate. Last but not least, non-Fermi liquid behavior is also found near a quantum critical point (QCP). It is a point in parameter space at which the system would undergo a phase transition at T = 0, if we were able to reach the limit of zero temperature. In that case quantum fluctuations instead of thermal fluctuations determine the critical behavior of the system. It is intuitively obvious that near a QCP the conventional Fermi liquid description breaks down since the self-energy is no longer expected to be of the form (2.4). Instead, quantum fluctuations down to arbitrary low wave numbers will modify this form. The scattering length of electrons diverges at a QCP while it must remain finite for a Fermi liquid. It should be emphasized that those features do not require strong electron correlations but appear also at QCPs of weakly correlated systems. An example of the latter case is the theory of Moriya48 (see also Ref. [49]) for the resistivity near a QCP of a weak ferromagnet. Quantum critical points are discussed in Section IV. III. Kondo Lattice Systems

The Kondo Hamiltonian describes magnetic impurities with free spins embedded in a metal and interacting with metal electrons via exchange scattering. The key ingredient is an antiferromagnetic interaction term Hint = J s(0) · S,

J > 0,

(3.1)

where S and s(0) are the S = 1/2 impurity spin and the conduction electron spin density at the impurity site which is taken here to be the origin. The model explains the characteristic Kondo behavior in dilute magnetic alloys which is determined by the phenomena of asymptotic freedom and confinement. They give 48 T. Moriya and A. Kawabata, J. Phys. Soc. Jpn. 34, 639 (1973). 49 K. K. Murata and S. Doniach, Phys. Rev. Lett. 29, 285 (1972).

STRONGLY CORRELATED ELECTRONS

15

rise to anomalies in the variation with temperature of equilibrium and transport properties and the “quenching” of the magnetic moment at low temperatures. The presence of a highly complex many-body ground state is highlighted by the breakdown of conventional perturbation theory which starts from free electrons and magnetic moments. The divergence of the conduction electron scattering matrix sets the low-energy characteristic scale kB TK where TK is usually referred to as the Kondo temperature. Microscopically it arises because the local degeneracy associated with the magnetic ion is removed through the exchange coupling between the conduction electrons and the impurity spin. The coupling leads to the formation of a singlet ground state and low-energy excitations which can be described in terms of a local Fermi liquid. In close analogy to confinement the local quasiparticles are composite objects formed by conduction electrons and magnetic degrees of freedom. The problem of magnetic impurities is well understood theoretically. There is a wide variety of techniques available which allow for an accurate description of the impurity contributions to physical properties. For detailed discussion, we refer to50–52 and references therein. Challenging problems are posed by work on concentrated systems, in particular on Ce-based compounds with heavy quasiparticles (heavy-fermion systems). At first glance these systems share many properties with dilute magnetic alloys. Those materials differ from ordinary metals in that there exists a characteristic temperature scale T ∗ 10–100 K, that is much smaller than the usual Fermi temperatures in ordinary metals, on which the electronic behavior of the compounds changes drastically. In the high-temperature regime for T T ∗ the systems behave like ordinary magnetic rare-earth systems which have itinerant conduction electrons with conventional masses and well-localized f -electrons. This picture is derived from the temperature dependence of the specific heat which exhibits pronounced Schottky anomalies corresponding to crystalline electric field (CEF) excitations. In addition, the magnetic susceptibility is Curie–Weiss-like reflecting the magnetic moment of the partially filled f -shell in a CEF. The low-temperature behavior, however, observed for T T ∗ is highly unusual and rather surprising: The specific heat varies approximately linearly with temperature (that is C = γ T + · · ·), and the magnetic susceptibility, χs , approaches a Pauli-like form, becoming almost independent of temperature. Values of the coefficients γ are of the order of J/mol K2 and consequently two to three orders of magnitude larger than those of ordinary metals 50 A. C. Hewson, The Kondo Problem to Heavy Fermions, Cambridge University Press (1993). 51 Y. Kuramoto and Y. Kitaoka, Dynamics of Heavy Electrons, vol. 105 of International Series of

Monographs in Physics, Clarendon Press, Oxford (2000). 52 D. L. Cox and A. Zawadowski, Exotic Kondo Effects in Metals: Magnetic Ions in a Crystalline

Electric Field and Tunnelling Centres, Taylor and Francis (1999).

16

P. FULDE ET AL. 2

which are of the order of π2 N kB T1F mJ/mol K2 . In addition, the magnetic susceptibility χs is enhanced by a factor of comparable magnitude. A recent survey of the experimental properties can be found in Refs. [53,54] and references therein. The similarities in the behavior of Ce-based heavy-fermion systems to that of dilute magnetic alloys have led to the assumption that these systems are “Kondo lattices” where the observed anomalous behavior can be explained in terms of periodically repeated resonant Kondo scattering. This ansatz provides a microscopic model for the formation of a singlet ground state and the appearance of a small energy scale characterizing the low-energy excitations. The Kondo picture has been confirmed by the observation of the Kondo resonance which forms at low temperatures.55 In contrast to the impurity case the Kondo model cannot be solved for a periodic lattice of magnetic ions. A major difficulty is the competition between the formation of (local) Kondo singlets and the lifting of degeneracies by long-range magnetic order. In the high-temperature regime the moments of the Ce 4f -shells are coupled by the RKKY interaction which can favor parallel as well as antiparallel orientation of the moments at neighboring sites. Model calculations for two Kondo impurities56–58 showed that antiferromagnetic correlations between the magnetic sites weaken the Kondo singlet formation reducing the characteristic energy scale kT ∗ to rather small values. Consequences for an extended lattice will be discussed in the subsequent section on Quantum Phase Transitions. The general difficulties in understanding the low temperature properties of Kondo lattices seem partially due to the lack of an adequate common “language” for the two regimes where local singlet formation is dominating on one side and where the magnetic intersite interactions dominate on the other. Such a language is usually provided by a mean-field theory which maps the complex quantum problem onto an appropriate classical model. In the case of the Kondo lattice separate mean-field descriptions exist for the two regimes which cannot be reconciled in a straightforward way to provide a unified approach. In the present section we focus on the heavy Fermi liquid regime. The corresponding mean-field theory was described, e.g., in Ref. [29] and references 53 P. Thalmeier and G. Zwicknagl, in Handbook of the Physics and Chemistry of Rare Earth, vol. 34,

eds. K. A. Gschneider, Jr., J.-C. Bünzli, and V. Pecharsky, Elsevier, Amsterdam (2005), p. 135. 54 P. Thalmeier, G. Zwicknagl, O. Stockert, G. Sparn, and F. Steglich, in Frontiers in Superconducting

Materials, Springer, Berlin (2005), p. 109. 55 F. Reinert, D. Ehm, S. Schmidt, G. Nicolay, S. Hüfner, J. Kroha, O. Trovarelli, and C. Geibel, Phys.

Rev. Lett. 87, 106401 (2001). 56 C. Jayprakash, H.-R. Krishna-murthy, and J. W. Wilkins, Phys. Rev. Lett. 47, 737 (1981). 57 C. Jayprakash, H.-R. Krishna-murthy, and J. W. Wilkins, J. Appl. Phys. 53, 2142 (1982). 58 B. Jones and C. M. Varma, J. Magn. Magn. Mater. 63 & 64, 251 (1987).

STRONGLY CORRELATED ELECTRONS

17

therein. The majority of recent microscopic studies of the Kondo lattice adopted the Dynamical Mean Field Theory which—by construction—explicitly neglects the subtle magnetic intersite correlations. It accounts for the complex local dynamics in terms of a local self-energy which has to be determined selfconsistently. The applications include model calculations and a study of the γ -αtransition in Ce.59 A major restriction on the general validity is imposed by the fact that the 4f valence has to be kept fixed at unity, i.e., nf = 1, throughout the calculation. The novel feature observed in stoichiometric Ce-compounds is the formation of narrow coherent bands of low-energy excitations. They give rise to the temperature dependence of the electrical resistivity which approximately follows ρ(T ) = ρ0 + AT 2 . While these findings unambiguously show that the low-energy excitations are heavy quasiparticles involving the f degrees of freedom, they nevertheless do not provide conclusive information on how the latter have to be incorporated into a Fermi liquid description. A characteristic property of a Fermi liquid is the existence of a Fermi surface whose volume is determined by the number of itinerant fermions. It is rather obvious that at high temperatures the f electrons should be excluded from the Fermi surface due to their apparent localized character. The latter, however, is lost at low temperatures. The conjecture that the f -degrees of freedom have to be treated as itinerant fermions and, consequently, have to be included in the Fermi surface was met with great scepticism.60 This hypothesis implies that the strong local correlations in Kondo lattices lead to an observable many-body effect, i.e., a change with temperature of the volume of the Fermi surface. At high temperatures, the f -degrees of freedom appear as localized magnetic moments, and the Fermi surface contains only the itinerant conduction electrons. At low temperatures, however, the f degrees of freedom are now tied into itinerant fermionic quasiparticle excitations and accordingly, have to be included in the Fermi volume following Luttinger’s theorem. Consequently the Fermi surface is strongly modified. This scenario61,62 was confirmed experimentally by measurements of the de Haas–van Alphen (dHvA) effect63–65 and recent photoemission studies.66,67 59 A. K. McMahan, K. Held, and R. T. Scalettar, Phys. Rev. B 67, 075108 (2003). 60 T. Kasuya, Prog. Theor. Phys. Supplement 108, 1 (1992). 61 G. Zwicknagl, Physica Scripta T 49, 34 (1993). 62 P. Fulde, in Narrow Band Phenomena: Infuence of Electrons with both Band and Localized Char-

acter, eds. J. C. Fuggle, G. A. Sawatzky, and J. Allen, Plenum (1988). 63 G. G. Lonzarich, J. Magn. Magn. Mat. 76–77, 1 (1988). 64 H. Aoki, S. Uji, A. K. Albessard, and Y. Onuki, Phys. Rev. Lett. 71, 2110 (1993). 65 F. S. Tautz, S. R. Julian, G. J. McMullen, and G. G. Lonzarich, Physica B 206–207, 29 (1995). 66 J. D. Denlinger, G.-H. Gweon, J. W. Allen, C. G. Olson, Y. Daliachaouch, B.-W. Lee, M. B. Maple, Z. Fisk, P. C. Canfield, and P. E. Armstrong, Physica B 281 & 282, 716 (2000). 67 J. D. Denlinger, G.-H. Gweon, J. W. Allen, C. G. Olson, M. B. Maple, J. L. Sarrao, P. E. Armstrong, Z. Fisk, and H. Yamagami, J. Electron Spectrosc. Relat. Phenom. 117 & 118, 347 (2001).

18

P. FULDE ET AL.

The present section is mainly devoted to the theoretical description of the Fermi liquid state at low temperatures. We briefly introduce the renormalized band scheme which has been devised for calculating realistic quasiparticle bands of real materials. This is achieved by combining ab initio electronic structure methods and phenomenological concepts in the spirit of Landau theory. Concerning the applications we shall not elaborate on the results for the Fermi surface and anisotropic effective masses in CeRu2 Si2 for which we refer to.61,68 We rather present recent results concerning the instabilities of the Fermi liquid state in CeCu2 Si2 . We would like to emphasize the predictive power of the renormalized band method. In both cases mentioned above (Fermi surface of CeRu2 Si2 and SDW instability in CeCu2 Si2 ) the effects were first calculated theoretically and later confirmed experimentally—sometimes with a delay of up to several years. 3. F ERMI -L IQUID S TATE AND H EAVY Q UASIPARTICLES : R ENORMALIZED BAND T HEORY The energy dispersion E(k) of a dilute gas of noninteracting quasiparticles is parameterized by the Fermi wave vector kF and the Fermi velocity vF ˆ · (k − kF ) E(k) = vF (k)

(3.2)

where kˆ denotes the direction on the Fermi surface. The key idea of the renormalized band method is to determine the quasiparticle states by computing the band structure for a given effective potential. Coherence effects which result from the periodicity of the lattice are then automatically accounted for. The quantities to be parameterized are the effective potentials which include the many-body effects. The parameterization of the quasiparticles is supplemented by information from conventional band structure calculations as they are performed for “ordinary” metals with weakly correlated electrons. The periodic potential leads to multiplescattering processes involving scattering off the individual centers as well as to propagation between the centers which mainly depends on the lattice structure and is therefore determined by geometry. The characteristic properties of a given material enter through the information about single-center scattering which can be expressed in terms of a properly chosen set of phase shifts {ηνi (E)} specifying the change in phase of a wave incident on site i with energy E and symmetry ν with respect to the scattering center. Within the scattering formulation of the band structure problem the values of the phase shifts at the Fermi energy {ηνi (EF )} together with their derivatives {(dηνi /dE)EF } determine the Fermi wave vectors kF and the Fermi velocity vF . 68 G. Zwicknagl, Adv. Phys. 41, 203 (1992).

STRONGLY CORRELATED ELECTRONS

19

A detailed description of the renormalized band method is given in Ref. [68]. The first step is a standard LDA band-structure calculation by means of which the effective single-particle potentials are self-consistently generated. The calculation starts, like any other ab initio calculation, from atomic potentials and structure information. In this step, no adjustable parameters are introduced. The effective potentials and hence the phase shifts of the conduction states are determined from first principles to the same level as in the case of “ordinary” metals. The f -phase shifts at the lanthanide sites, on the other hand, are described by a resonance type expression η˜ f arctan

˜f E − ˜f

(3.3)

which renormalizes the effective quasiparticle mass. One of the two remaining ˜ f is eliminated by imposing the condition that the free parameters ˜f and charge distribution is not significantly altered as compared to the LDA calculation by introducing the renormalization. The renormalized band method devised to calculate the quasiparticles in heavy-fermion compounds thus is essentially a one-parameter theory. We mention that spin-orbit and CEF splittings can be accounted for in a straightforward manner.68 4. H EAVY F ERMIONS IN C E RU 2 S I 2 AND C E C U 2 S I 2 The archetype heavy fermion superconductor CeCu2 Si2 as well as CeRu2 Si2 crystallize in the tetragonal ThCr2 Si2 structure. The unit cell is shown in Figure III.1.

F IG . III.1. Conventional unit cell of the ThCr2 Si2 and CeM2 X2 structure where M = Cu, Ni, Ru, Rh, Pd, Au, . . . and X = Si, Ge.

20

P. FULDE ET AL.

To study the electronic structure, we compare the results of two different models, i.e., treating the Ce 4f degrees of freedom as localized (atomic like) states and as delocalized yet strongly renormalized electrons. The first procedure provides a good quantitative description of the properties at elevated temperatures, high excitation energies, and above the metamagnetic transition. The latter ansatz yields a model for the Fermi liquid state. The low-temperature behavior of CeRu2 Si2 is well described by a paramagnetic Fermi liquid with weak residual interactions. The relevant low-energy excitations are heavy quasiparticles as inferred from the linear specific heat coefficient γ 350 mJ/mol K2 .69 In the local moment regime, the Fermi surface is determined exclusively by the conduction states. The strongly renormalized Fermi liquid state, on the other hand, is described by the renormalized band method us˜ f 10 K in Eq. (3.3) for the intrinsic width of the quasiparticle band. The ing value is consistent with inelastic neutron data70 as well as thermopower and specific heat data.69 CEF effects are accounted for by adopting a 7 ground state. The details of the calculation are described in Ref. [68]. The renormalized band scheme gives the correct Fermi surface topology for CeRu2 Si2 and thus consistently explains the measured dHvA data.61,68,71 The character of quasiparticles in CeRu2 Si2 varies quite strongly over the Fermi surface. The validity of the Fermi liquid picture is concluded from a comparison of the effective masses on Fermi surface sheets with large f contribution. From the large linear specific heat the renormalized band scheme deduces a characteristic energy kT ∗ 10 K and predicts heavy masses of order m∗ /m 100. This value was confirmed by experiments72–74 where the ψ orbit with m∗ /m 120 was observed. The corresponding Fermi surface cross-section is in agreement with estimates from the renormalized band theory. This proofs that the heavy quasiparticles exhaust the low-energy excitations associated with the f -states. The change in volume of the Fermi surface when going from T T ∗ to T T ∗ is observed by comparing the Fermi surface of CeRu2 Si2 to that of its ferromagnetic isostructural counterpart CeRu2 Ge2 where the f -states are clearly localized. In a series of beautiful experiments75 it was demonstrated that the Fermi 69 F. Steglich, U. Rauchschwalbe, U. Gottwick, H. M. Mayer, G. Sparn, N. Grewe, and U. Poppe,

J. Appl. Phys. 57, 3054 (1985). 70 L. P. Regnault, W. A. C. Erkelens, J. Rossat-Mignot, P. Lejay, and J. Flouquet, Phys. Rev. B 38,

4481 (1988). 71 G. Zwicknagl, E. Runge, and N. E. Christensen, Physica B 163, 97 (1990). 72 A. K. Albessard, T. Ebihara, I. Umehara, K. Satoh, Y. Onuki, H. Aoki, S. Uji, and T. Shimizu,

Physica B 186–188, 147 (1993). 73 H. Aoki, S. Uji, A. K. Albessard, and Y. Onuki, Phys. Rev. Lett. 71, 2110 (1993). 74 F. S. Tautz, S. R. Julian, G. J. McMullen, and G. G. Lonzarich, Physica B 206–207, 29 (1995). 75 C. A. King and G. G. Lonzarich, Physica B 171, 161 (1991).

STRONGLY CORRELATED ELECTRONS

21

F IG . III.2. Photoemission results for (a) LaRu2 Si2 in comparison to (b) CeRu2 Si2 at T = 25 K, i.e., above the Kondo temperature T ∗ = 15 K of that system. Band structures are very similar for both compounds. (After Ref. [67].)

surfaces of these two compounds are rather similar. However, the enclosed Fermi volume is smaller in the case of CeRu2 Ge2 , the difference being roughly one electron per unit cell. More direct evidence is provided by recent photoemission experiments (see Figure III.2). Denlinger et al.67 have shown that at temperatures around 25 K, the Fermi surface of CeRu2 Si2 , is that of its counterpart LaRu2 Si2 which has no f electrons. At this point the general question arises how the formation of heavy quasiparticles is reflected in the angular resolved photoelectron spectroscopy (ARPES) data. A major difficulty stems from the fact that photoemission experiments probe the occupied part of the spectrum. The most dramatic changes, however, are expected to occur in the empty part. In Figure III.3 we compare the dispersion of the heavy quasiparticle bands at low temperatures to their light high-temperature counterparts. In the occupied part the main difference is a bending close to the Fermi energy which changes the volume of the Fermi surface. The characteristic bending was recently observed in CeCoIn5 .76 76 A. Koitzsch, Priv. comm.

22

P. FULDE ET AL.

F IG . III.3. Band dispersion for CeCu2 Si2 along Z– for low temperatures T T ∗ (full lines) and high temperatures (dashed lines). The formation of the heavy quasiparticles leads to a characteristic bending in the occupied part of the spectrum.

Let us now turn to the heavy fermion superconductor CeCu2 Si2 which exhibits a highly complex phase diagram at low temperatures discussed in Section III.5. It results from an extreme sensitivity of the physical properties with respect to variations of the stoichiometry and external magnetic fields.

F IG . III.4. CeCu2 Si2 : Main Fermi surface sheet of heavy quasiparticles (m∗ /m 500) calculated with the renormalized band method. It consists of modulated columns which are oriented parallel to the tetragonal axis. The calculations adopt the CEF scheme of Ref. [77] consisting of a singlet ground state separated from an excited quartet by a CEF splitting δ 330 K. Therefore δ T ∗ 10 K (obtained from the γ -value). The nesting vector Q = (0.23, 0.23, 0.52) connects flat parts (“nesting”) of the Fermi surface. (After Refs. [78] and [79].) 77 E. A. Goremychkin and R. Osborn, Phys. Rev. B 47, 14280 (1993). 78 G. Zwicknagl and U. Pulst, Physica B 186, 895 (1993). 79 O. Stockert, E. Faulhaber, G. Zwicknagl, N. Stuesser, H. Jeevan, T. Cichorek, R. Loewenhaupt,

C. Geibel, and F. Steglich, Phys. Rev. Lett. 92, 136401 (2004).

STRONGLY CORRELATED ELECTRONS

23

To calculate the quasiparticle bands in CeCu2 Si2 by means of the renormalized band method, we adopt the doublet-quartet CEF scheme suggested in Ref. [77]. The ground state is separated from the excited quartet by δ 330 K. The results for the Fermi surface78,80 can be summarized as follows: We find two separate sheets of the Fermi surface for heavy and light quasiparticles. The light quasiparticles have effective masses of the order of m∗ /m 5. They can be considered as weakly renormalized conduction electrons. Of particular interest are heavy quasiparticles of effective masses m∗ /m 500 which are found on a separate sheet. This surface whose shape (see Figures III.4 and III.8) is rather different from the corresponding LDA surface mainly consists of columns parallel to the tetragonal axis and of small pockets. The topology of the Fermi surface suggests that the strongly correlated Fermi liquid state should become unstable at sufficiently low temperatures. Firstly, it exhibits pronounced nesting features which may eventually lead to the formation of a ground state with a spin-density modulation. This will be discussed in detail below. Secondly, the topology of this surface depends rather sensitively on the position of the Fermi energy. The band filling and hence the f -valence are critical quantities. Reducing the f -occupancy from the initial value of nf 0.95 by approximately 2% leads to changes in the topology as shown in Refs. [78,80]. As a result, the quasiparticle density of states (DOS) exhibits rather pronounced structures in the immediate vicinity of the Fermi energy which, in turn, can induce instabilities.81 5. L OW-T EMPERATURE P HASE D IAGRAM OF C E C U 2 S I 2 The phase diagram of CeCu2 Si2 contains three different phases: the A and the B phase and a superconducting phase. In some samples the superconducting phase expels the A phase while in other samples the two phases may coexist. While the A phase has been identified as a spin-density wave phase as discussed below, the character of the B phase has remained unknown. The instability may result from a reconstruction of the Fermi surface.78 Much effort has been devoted to the characterization of the A phase which originally had the appearance of a ‘hidden order’ phase. However, later a spin-density wave character was first inferred from resistivity results82 and was supported by specific heat and high-resolution magnetization measurements.83 The transition temperature TA is suppressed by increasing 80 U. Pulst, Ph.D. thesis, TH Darmstadt (1993). 81 M. I. Kaganov and I. M. Lifshits, Sov. Phys. Usp. 22, 904 (1979). 82 P. Gegenwart, C. Langhammer, C. Geibel, R. Helfrich, M. Lang, G. Sparn, F. Steglich, R. Horn,

L. Donnevert, A. Link, et al., Phys. Rev. Lett. 81, 1501 (1998). 83 F. Steglich, N. Sato, T. Tayama, T. Lühmann, C. Langhammer, P. Gegenwart, P. Hinze, C. Geibel,

M. Lang, G. Sparn, et al., Physica C 341–348, 691 (2000).

24

P. FULDE ET AL.

F IG . III.5. B–T phase diagram of CeCu2 Si2 for B a. Original version from Ref. [84], completed version from Ref. [85]. In this sample the SDW A-phase is expelled from the superconducting (SC) region (no coexistence). The nature of the B-phase is yet undetermined.

the 4f -conduction electron hybridization and eventually vanishes. This can be achieved by applying hydrostatic pressure or choosing a few percent excess of Cu. The ordered moments are expected to be rather small. The important question in this context is: What is the origin of the antiferromagnetic correlations, showing up in the A phase? How do they arise in the heavy fermion state and finally, how do they affect the heavy quasiparticles? The key to the answers comes from the Fermi surface of CeCu2 Si2 and its nesting properties. As shown in Figure III.4 there are parallel portions which are connected by a wave vector close to (1/4, 1/4, 1/2). As a consequence, the static susceptibility χ(q) exhibits a maximum for momentum transfer q close to the nesting vector (Figure III.6). Recent neutron scattering experiments79 (Figure III.6) for the stoichiometric compound (x = 0) show a spin-density wave (SDW) which forms below TN 0.7 K. The experimental propagation vector Q is close to (0.22, 0.22, 0.55) and the ordered moment amounts to μ 0.1μB . These findings show that the SDW in CeCu2 Si2 arises out of the renormalized Fermi liquid state. The transition is driven by the nesting properties of the heavy quasiparticles. 84 G. Bruls, D. Weber, B. Wolf, P. Thalmeier, B. Lüthi, A. de Visser, and A. Menovsky, Phys. Rev.

Lett. 65, 2294 (1990). 85 F. Weickert, Private comm. (2003).

STRONGLY CORRELATED ELECTRONS

25

F IG . III.6. Upper panel: Neutron diffraction intensity in CeCu2 Si2 at temperature above and below the A-phase transition temperature TA . Incommensurate peak is at Q = (0.22, 0.22, 0.55). (After Ref. [79].) Lower panel: Nesting of heavy FS columns (Figure III.4) leads to a peak in the static susceptibility χ(q) at q = Q. Intensity map of χ(q) (value increasing from dark to bright) in the reciprocal (h, h, l)-plane as calculated for the renormalized bands at T = 100 mK. The experimental Q at 50 mK from the left panel shows perfect agreement with the calculated maximum position of χ(q).

Having classified the nature of the A phase we next turn to the question how the latter competes with superconductivity. Itinerant electron antiferromagnetism as realized in the A phase and superconductivity both form in the system of the heavy quasiparticles. Their interplay therefore depends sensitively on the geometric properties of the paramagnetic Fermi surface and the symmetries of the ordered phases. This can be seen from realistic model calculations investigating the

26

P. FULDE ET AL.

F IG . III.7. Temperature dependence of the superconducting (SC) and magnetic A (SDW) order parameters in a AS crystal. The sublattice magnetization M = h0 (T ) and the amplitude 0 of the SC order parameter are calculated from Eq. (3.23) using realistic quasiparticles and the experimentally determined propagation vectors for the A phase. A SC order parameter (k) = 0 (cos kx a − cos ky a) (1)

can form in the A phase. Below the superconducting transition temperature T < Tc < TN the two order parameters coexist and compete. Itinerant SDW antiferromagnetism is expelled at a temperature (2) TN < Tc . (After Ref. [86,87].)

variation with temperature of the two order parameters in crystals where the two ordering phenomena coexist in some temperature range (“AS-type” crystals).86,87 Figure III.7 summarizes the results for an unconventional superconducting state with 3 (d-wave) symmetry of the gap function, i.e., (k) ∼ (cos kx a − cos ky a). The theory leading to the results displayed in Figure III.7 starts from the model Hamiltonian H = H0 + Hint where the free quasiparticles are described by

† H0 = E(k)ckσ ckσ .

(3.4)

(3.5)

kσ

The creation (annihilation) operators for quasiparticles with wavevector k, † (pseudo) spins σ = ±1 and energy E(k) are denoted by ckσ (ckσ ). The energies which are measured relative to the Fermi level are calculated within the Renormalized Band Scheme. The residual interactions in the strongly renormalized Fermi liquid are assumed to be repulsive for short separations while being attractive for two quasiparticles of opposite momenta on neighboring sites. The former favors 86 M. Neef, Master Thesis, Technische Universität Braunschweig (2004). 87 M. Neef, M. Reese, and G. Zwicknagl, preprint (2004).

STRONGLY CORRELATED ELECTRONS

27

the formation of a SDW while the latter gives rise to a superconducting instability. Adopting a mean-field approximation yields Hint → HSDW + HSC

(3.6)

where

σ † ck+Qj σ + h.c. h(Qj )ckσ 2

(3.7)

1 † † σ σ (k)ckσ c−kσ + h.c. . 2

(3.8)

HSDW = −

kσ

Qj

and HSC =

kσ σ

The periodically modulated magnetization associated with the SDW with propagation vectors Qj as well as the superconducting pair potential σ σ have to be determined selfconsistently h(Qj ) =

U σ † c ckσ L 2 k+Qj σ

(3.9)

kσ

and σ σ (k) =

1

gsσ σ ;σ σ (k, k )c−k σ ck σ , L

(3.10)

kσ σ

where the strength U of the local Hubbard-type repulsion is of the order of the quasiparticle band width kB T ∗ and gσ σ ;σ σ (k, k ) is the effective pair attraction. The k-summation runs over the entire paramagnetic Brillouin zone and L denotes the number of lattice sites. The expectation values denoted by · · · have to evaluated with the eigenstates of the mean-field Hamiltonian HMF = H0 + HSDW + HSC , and consequently depend upon the order parameters. Therefore the self-consistency equations are coupled. The mean-field Hamiltonian implicitly assumes that the amplitudes of both order parameters are small. In particular, we neglect here the pairing amplitudes of the form c−kσ ck+Qj σ . The latter are important when the gaps introduced by the antiferromagnetic order into the quasiparticle spectrum are large on the scale set by superconductivity. For a discussion of this point we refer to Refs. [88,89]. 88 G. Zwicknagl and P. Fulde, Z. Phys. B 43, 23 (1981). 89 P. Fulde and G. Zwicknagl, J. Appl. Phys. 53, 8064 (1982).

28

P. FULDE ET AL.

The periodically modulated magnetization associated with the SDW acts on the conduction electrons like a periodic spin-dependent potential which we approximate by

h(Qj )eiQj ·r (3.11) h(r) = Qj

with the same amplitudes h(Qj ) = h0 for the eight commensurate wave vectors π π Qj ∈ {(± 2a , ± 2a , ± πc )}. The magnetic superstructure breaks the translational invariance of the underlying lattice but preserves the point group symmetry. The mean-field Hamiltonian, however, is invariant under translations with a1 = (2a, 2a, 0),

a2 = (2a, −2a, 0),

a3 = (2a, 0, c).

(3.12)

The volume of the magnetic supercell is 16 times the volume of the paramagnetic unit cell. As a result the Brillouin zone is reduced and the quasiparticle states are modified by extra Bragg reflections. The opening of new gaps is important at sufficiently low temperatures T TN where TN is the ordering (Néel) temperature. The order parameter σ σ behaves as a two-fermion wave function in many respects. This is expressed by the fact that an off-diagonal long-range order (ODLRO) parameter is not the thermal expectation value of a physical observable but rather a complex pseudo- wave function describing quantum-phase correlations on the macroscopic scale of the superconducting coherence length. Its phase is a direct signature of the broken gauge invariance in the superconducting condensate. Experiment (strongly) suggests that superconductivity in CeCu2 Si2 occurs with anisotropic even-parity (pseudo-) spin singlet pairing. We therefore restrict ourselves to this case characterized by a scalar order parameter σ σ (k) = φ(k)(iσ2 )σ σ

(3.13)

were φ(k) is a complex amplitude and σ2 denotes the Pauli matrix in spin space. Since the two ordering temperatures, i.e., the antiferromagnetic Néel temperature TA and the superconducting Tc are very close to each other we focus on pair states which are compatible with the translational symmetry of the paramagnetic lattice. The corresponding functions are listed in Refs. [68,90–92]. In the explicit calculations we restrict ourselves to one-dimensional representations for simplicity. The generalization to multi-dimensional representations is rather straightforward.86 Finally, the variation with momenta k and k of the quasiparticle attraction g(k, k ) is expanded in terms of the basis functions belonging to the κ-th row, κ = 90 M. Sigrist and K. Ueda, Rev. Mod. Phys. 63, 239 (1991). 91 R. Konno and K. Ueda, Phys. Rev. B 40, 4329 (1989). 92 M. Ozaki and K. Machida, Phys. Rev. B 39, 4145 (1989).

STRONGLY CORRELATED ELECTRONS

29

1, . . . , d(), of the d()-dimensional irreducible representation of the symmetry group g(k, k ) =

g

d()

ϕκ (k)ϕ∗ κ (k ).

(3.14)

κ=1

We further simplify the problem by focusing on the states φ (k) with the symmetry which yields the strongest quasiparticle attraction g . Assuming that this most stable order parameter is non-degenerate the self-consistency condition is 1 ∗ φ(k) = −g0 ϕ0 (k) ϕ (k )c−k ↓ ck ↑ . (3.15) L 0 k

To solve the mean-field Hamiltonian Eqs. (3.7) and (3.8) we adopt the Nambu formalism which allows us to reduce the mean-field Hamiltonian to single-particle form in particle–hole space, i.e., H=

AFBZ

ˆ τˆ3 + h1 ˆ + (k) ˆ k† E(k) τˆ1 k .

(3.16)

k

The Nambu spinors k have 32 components and are defined as † † k† = ck↑ , ck+Q1 ↑ , . . . , c−k↓ , c−k−Q ,... . 1↓

(3.17)

They account for the coherent superposition of particles and holes which is the ˆ τˆ1 and τˆ3 denote the characteristic feature of the superconducting state. Here 1, unit matrix and the Pauli matrices in particle–hole space. The sixteen wave vectors Q0 = 0, Q1 , . . . , Q15 are the reciprocal lattice vectors appearing in the antiferromagnetic phase. The set includes the eight propagation vectors of the SDW and their higher harmonics. The k-summation is restricted to the reduced Brillouin zone (AFBZ) of the antiferromagnetic state defined by the SDW. The structure of the Hamiltonian in particle–hole space is

ˆ ˆ E(k) + hˆ ˆ H (k) = (3.18) ˆ ˆ −E(k) + hˆ where the 16 × 16-diagonal matrix contains the quasiparticle energies of the paramagnetic normal phase ˆ E(k) = δQi Qj E(k + Qi ). (3.19) QQ i

j

The SDW acts like an effective magnetic field. The modulated spin density leads to Umklapp scattering which is accounted for by the matrix ˆ hˆ = −h0 (T )m.

(3.20)

30

P. FULDE ET AL.

ˆ is a purely geometric quantity specifying the possible UmkThe 16 × 16 matrix m lapp processes while the temperature-dependent amplitude h0 (T ) has to be determined self-consistently. The diagonal matrix ˆ (k) = δQi Qj 0 (T )ϕ0 (k + Qi ) Qi Qj ˆ (3.21) ≡ 0 (T ) (k) QQ i

j

contains the superconducting order parameters with the given k-dependent function φ (k) and a temperature-dependent amplitude 0 (T ). The self-consistency Eqs. (3.9) and (3.10) can be formulated in terms of the off-diagonal elements of the 32 × 32-matrix Green’s function ˆ n , k) = in 1ˆ − Hˆ (k) −1 G(i (3.22) according to h0 (T ) =

c AFBZ

1 U

ˆ n , k) ˆ 1ˆ G(i T Tr m L 16 k

n

0 (T ) = −

c AFBZ

1 g

ˆ )τˆ1 τˆ3 G(i ˆ n , k )τˆ3 . T Tr (k L 2 n

(3.23)

k

Here n = πT (2n + 1) denote the T -dependent Matsubara frequencies and c is the energy cut-off required in weak-coupling theory. The coupling constants U and g as well as the cut-off c are eliminated in the usual way in favor of the (0) (0) observable quantities TN and Tc . Solving the self-consistency equations for φ3 (k) ∼ cos kx a − cos ky a yields the results displayed in Figure III.7. It shows that both order parameters coexist in a finite temperature interval. This is due to the fact they have their maximum amplitudes on different parts of the Fermi surface (see Figure III.8). At sufficiently low temperatures the A-phase is finally expelled by superconductivity as shown in Figure III.7. This was confirmed by neutron diffraction which shows a suppression of magnetic Bragg peaks further below Tc . IV. Quantum Phase Transitions

Most phase transitions in condensed matter are governed by the appearance of a spontaneously broken symmetry below a certain transition temperature Tc . The low temperature phase is then characterized by an order parameter belonging to a single nontrivial representation of the high temperature symmetry group. In the simplest case the order parameter is of the density type (diagonal long range order), for instance charge density n(r) or spin density m(r). Approaching Tc from

STRONGLY CORRELATED ELECTRONS

31

F IG . III.8. CeCu2 Si2 : Variation of the SC gap function amplitude |(k)|/0 (T ) = |φ3 (k)| for the (pseudo-) singlet wave function with 3 -symmetry φ3 (k) ∼ cos kx a − cos ky a on the heavy quasiparticle sheet of the paramagnetic Fermi surface. The amplitude of this SC order parameter is maximal on the kidney-shaped surfaces centered along the direction which are almost unaffected by the formation of the A phase. The dominant contributions to the latter come from the nesting parts on the heavy columns where the superconducting amplitude is small. Dark and light grey indicate large and small amplitudes, respectively.

above the correlation length of spatial order parameter fluctuations, the associated order parameter susceptibility and other thermodynamic quantities diverge. The divergence is characterized by critical exponents that depend only on spatial dimension d, on the range of interactions and number of order parameter components n which define the universality class of the model. In such finite temperature or ‘classical’ phase transitions the underlying microscopic quantum fluctuations of charge and spin densities etc. are not important ingredients for the long-range order because their coherence is destroyed by thermal fluctuations over time scales longer than h¯ /kTc . However, the broken symmetry state may not only be reached by lowering the temperature. Instead at T = 0 the tuning of a physical control parameter X, e.g., due to applied hydrostatic or chemical pressure via doping may drive the compound from the disordered to the ordered state and vice versa (see Figure IV.6). The corresponding value Xc defines the quantum critical point (QCP) where a quantum phase transition (QPT) takes place. In the latter the T = 0 quantum fluctuations can be coherent over arbitrary long time scales. For this reason the effective dimension for order parameter fluctuations close to a QPT is given by deff = d + z where z is the dynamic exponent which characterizes the scaling of energies of quantum fluctuations with system size. The contribution of quantum fluctuations has therefore profound consequences for the critical exponents of thermodynamic and transport quantities. For example, in strongly correlated metals close to an antiferromagnetic QCP along the quantum critical line (X = Xc

32

P. FULDE ET AL.

or |r| = 0) in Figure IV.6 an anomalous non-Fermi liquid (NFL) temperature dependence of physical quantities like χ(T ), C(T )/T and ρ(T ) emerges. Its origin and theoretical description has been the subject of much recent investigations and controversy.93,94 An additional important discovery is the observation that superconductivity often appears in a dome-like shape around the QCP. Viewed differently, it may be a successful strategy to look for unconventional superconducting states in searching around magnetic QCPs of suitable materials. The presence of strong electronic correlations is by no means essential for the appearance of a quantum phase transition. Historically they have been first studied in weakly correlated metals without calling them explicitly with their modern name. As an introduction we will briefly discuss some early examples of QPTs. Subsequently well understood model theories for QPTs in local moment systems, notably the Ising model in a transverse field will be discussed. Then we come to QPTs in the strongly correlated systems where theoretical work has focused on the Kondo-lattice type models both with and without charge degrees of freedom. Finally the phenomenological scaling and Ginzburg–Landau theories applicable close to the QCP will be discussed. They are important for the interpretation of a large body of experimental work near the QCP of heavy-fermion compounds. 6. Q UANTUM P HASE T RANSITION IN L OCALIZED AND I TINERANT M AGNETS The idea that tuning of a control parameter may drive an insulator or metal from the paramagnetic state to a magnetically ordered state at zero temperature is indeed a very old one. The classical Stoner–Wolfarth theory of itinerant ferromagnetism (FM)95,96 identifies this control parameter as X = I N(EF ) where I is the exchange integral of itinerant conduction electrons and N (EF ) the conduction electron DOS per spin direction. In the paramagnetic regime with X < Xc = 1 the exchange interaction is too weak to cause an exchange splitting of conduction bands and stabilize a spin polarization. However the incipient FM order has its effect on the spin fluctuation spectrum. The typical life time τsf of a quantum fluctuation of magnetic moments diverges when X → Xc . This may be seen from the dynamical susceptibility, calculated from the single-band Hubbard model for 93 S. Sachdev, Quantum Phase Transitions, Cambridge University Press (1999). 94 M. A. Continentino, Quantum Scaling in Many-Body Systems, World Scientific (2001). 95 E. Stoner, Proc. Roy. Soc. A165, 372 (1938). 96 E. Stoner, Proc. Roy. Soc. A169, 339 (1939).

STRONGLY CORRELATED ELECTRONS

33

a parabolic band within random-phase approximation (RPA). Close to the QCP (X Xc ) the spectrum of FM spin fluctuations with q → 0 is given by:97,98 Im χ−+ (ω) =

(π/4)N (EF )ω/qvF [1 − I N(EF )]2 + [(π/4)N (EF )I ω/qvF ]2

(4.1)

where vF is the Fermi velocity. When X → Xc this spectrum is strongly peaked at the ‘paramagnon’ frequency (S 1) ωP =

4 vF q. π S

(4.2)

Here S = (1 − I N(EF ))−1 is the ‘Stoner parameter’ which governs the softening of the spin fluctuation spectrum in Eq. (4.1) on approaching the QCP. It also gives the enhancement of the static susceptibility χ = Sχ0 as compared to the free Pauli susceptibility χ0 . In addition the paramagnon excitations lead to a deviation from the linear specific heat behavior of the Fermi liquid described by98,99 C(T )/T = γ0 [m∗ /m + S(T /TSF )2 ln(T /TSF )]

(4.3)

where m∗ /m is the mass enhancement due to paramagnons98 and TSF is the spin fluctuation temperature given by TSF = EF /S. Equivalently one may say that χ−+ (ω) has a pole at the purely imaginary frequency iωP . This represents a collective overdamped spin fluctuation mode. When X is tuned through the critical value Xc = 1 by pressure or alloying, the imaginary spin fluctuation pole moves to the real axis and becomes the FM spinwave pole with frequency (q kF , ms n) ω(q) = Dq 2 ,

D ∼ (I 2 /EF )kF−2 nms .

(4.4)

Simultaneously a spontaneous FM moment caused by the spin polarization ms = n↑ − n↓ of conduction bands appears. Here D is the spin wave stiffness constant and n = n↑ + n↓ is the number of conduction electrons per site. This collective spin excitation is undamped for small q because it is the Goldstone mode associated with the continuous SO(3) symmetry of the FM order parameter and therefore in the hydrodynamic limit it is protected by a conservation law against decay. For X only marginally above the FM QCP Xc = 1 one has only weak ferromagnetism (WFM) and anomalous thermodynamic and transport behavior due to paramagnon excitations was observed.97,98 The first theory beyond the Hartree–Fock RPA level to address such quantum critical phenomena in itinerant 97 N. F. Berk and J. R. Schrieffer, Phys. Rev. Lett. 17, 1171 (1966). 98 S. Doniach and S. Engelsberg, Phys. Rev. Lett. 17, 750 (1966). 99 C. P. Enz, A Course on Many-Body Theory Applied to Solid-State Physics, vol. 11 of Lecture Notes in Physics, World Scientific (1992).

34

P. FULDE ET AL.

ferromagnets was Moriya’s self consistent renormalization (SCR) theory48,100,101 for the WFM and the theory by Hertz102 on which much of the later developments are based. The best known example of an enhanced paramagnetic metal which is close to a FM quantum critical point is palladium metal. In this case one has a large susceptibility enhancement of S 10.103 Indeed, alloying with only 0.5% Fe immediately leads to FM order.104 According to band structure calculations a (linear) expansion of the lattice of pure Pd by ∼ 7% should lead to a FM ground state. Experimentally Au–Pd–Au sandwiches have been prepared where an estimated volume expansion of 2.3% of Pd due to the larger lattice constant of Au leads to huge Pd Stoner factors of S ∼ 103 –104 ,105 but FM order is still not achieved. The classical, enhanced paramagnetism in Pd and associated QPT in Pd alloys has been complemented by Laves phase compounds AB2 like TiBe2 106 and ZrZn2 107 which are slightly on the overcritical side, i.e., I N(EF ) 1 and thus weak itinerant ferromagnets. By doping with Cu the alloy series TiBe2−x Cux exhibits a QCP at xc 0.155 where ferromagnetism disappears. The compound ZrZn2 has already been known for a long time and has recently been investigated with renewed interest because it exhibits a FM QCP as function of hydrostatic pressure at pc = 21 GPa. As in UGe2 it was found that surprisingly superconductivity coexists within the FM phase, albeit with a small Tc .108 Quite another quantum phase transition to a magnetically ordered state has been known since a long time in localized moment systems. It was studied under the name ‘induced moment magnetism’ without actually stressing that it is a generic type of quantum phase transition as we shall see. In localized (4f - or 5f -) magnetic compounds with uniaxial symmetry the lowest CEF states of non-Kramers ions may consist of a nonmagnetic singlet ground state |1 and a nonmagnetic singlet (or doublet) excited state |2 at an energy . They are both characterized by a vanishing moment, i.e., n|Jz |n = 0 (n = 1, 2) with Jz denoting the total angular momentum component of the localized 4f or 5f states. Therefore there are no pre-existing localized moments that might order as in a conventional AF 100 T. Moriya and A. Kawabata, J. Phys. Soc. Jpn. 35, 669 (1973). 101 T. Moriya, Spin Fluctuations in Itinerant Electron Magnetism, vol. 56 of Springer Series in Solid-

State Sciences, Springer-Verlag, Berlin (1985). 102 J. A. Hertz, Phys. Rev. B 14, 1165 (1976). 103 W. Gerhardt, F. Razavi, J. S. Schilling, D. Hüser, and J. A. Mydosh, Phys. Rev. B 24, 6744 (1981). 104 J. A. Mydosh, J. I. Budnick, M. P. Kawatra, and S. Skalski, Phys. Rev. Lett. 21, 1346 (1968). 105 M. B. Brodsky and A. J. Freeman, Phys. Rev. Lett. 45, 133 (1980). 106 F. Acker, Z. Fisk, J. L. Smith, and C. Y. Huang, J. Magn. Magn. Mater. 22, 250 (1981). 107 B. T. Matthias and R. M. Bozorth, Phys. Rev. 109, 604 (1958). 108 C. Pfleiderer, M. Uhlarz, S. M. Hayden, R. Vollmer, H. v. Löhneysen, N. R. Bernhoeft, and G. G. Lonzarich, Nature 412, 58 (2001).

STRONGLY CORRELATED ELECTRONS

35

phase transition. The local moments themselves have to be induced at any given site at TN . This is possible if a nondiagonal matrix element α = 1|Jz |2 exists. The effective RKKY inter-site exchange J (q) then mixes the two states, thereby creating an induced ground state moment. If J (q) is maximal at a wave vector Q this happens spontaneously at a temperature TN =

2 tanh−1 ( ξ1 )

,

here ξ =

α 2 J (Q) 2

(4.5)

is the control parameter of the quantum phase transition to an induced moment state. It takes place for ξ > ξc = 1. In general the ordered state has an incommensurate modulation with wave vector Q. In the paramagnetic phase the magnetic singlet-singlet excitations disperse into a magnetic exciton band given by α 2 J (q) (4.6) ω(q) = 1 − 2 The onset of the QFT is signified by a softening of the exciton mode as function of ξ at the incipient ordering vector Q which is given by ω(Q) = [1 − ξ ] and vanishes at ξc = 1. The control parameter contains the CEF splitting which is susceptible to pressure. The latter may therefore be used to tune the singletsinglet system through the QCP. Phase transitions of the induced moment type under ambient conditions as well as under pressure have been found in a number of rare earth systems like Pr3 Tl, TbSb (for a review see Ref. [109]) and dhcp Pr metal.110,111 It also describes the AF order in the actinide compound UPd2 Al3 with partly itinerant and partly localized 5f-electrons (see Section V). In fact dhcp Pr, which is approximately a singlet-doublet CEF system, is of special interest. There the critical mode softening and modulated moment appearance under uniaxial pressure shown in Figure IV.1 correspond to the modern concept of a quantum phase transition due to variation of a microscopic control parameter. However, this aspect was not stressed or realized at that time. This is remarkable because it was found earlier that the simplest Hamiltonian which describes induced moments in the singlet-singlet system (though not precisely dhcp Pr) is of the type

H = Tix + I Tiz Tiz (4.7) i

ij

109 P. Fulde, in Handbook of the Physics and Chemistry of Rare Earth, vol. 2, eds. K. A. Gschneider, Jr. and L. Eyring, North-Holland, Amsterdam (1979), chap. 17, p. 295. 110 J. Jensen, K. A. McEwen, and W. G. Stirling, Phys. Rev. B 35, 3327 (1987). 111 J. Jensen and A. R. Mackintosh, Rare Earth Magnetism: Structures and Excitations, Clarendon Press, Oxford (1991).

36

P. FULDE ET AL.

F IG . IV.1. Left panel: paramagnetic (PM) to incommensurate magnetic (ICM) quantum phase transition as function of uniaxial pressure in dhcp Pr. The quantum critical point is at pc ∼ 0.7 kbar. Circles are the experimental first harmonic of the ICM moment corresponding to modulation wave vector Q = 0.12a∗ . Dashed and solid lines correspond to model calculations. Right panel: Optic (open circles) and acoustic (closed circles) exciton mode frequencies which give the energy scale of quantum fluctuations. Close to the quantum critical point at pc and for the ordering wave vector Q this energy scale vanishes. (After Ref. [110].)

where the two orientations | ↑, | ↓ of the pseudo-spin Tz correspond to the CEF singlets n = 1, 2 respectively. Indeed, this is the n.n. Ising model in a transverse field (ITF), a genuine model for quantum phase transitions. The last term establishes AF order of Ising spins with a twofold degenerate ground state due to Z2 symmetry. The first transverse field term introduces quantum fluctuations of the spins and destroys long-range order if the control parameter ξ = I /(2) exceeds ξc = 1. This model is exactly solvable in 1D112,113 and therefore is a reference point for the theory of QPTs. If one adds an infinitesimal staggered field term to 112 E. Lieb, T. Schultz, and D. Mattis, Ann. Phys. (N. Y.) 16, 407 (1961). 113 P. Pfeuty, Ann. Phys. (N.Y.) 57, 79 (1970).

STRONGLY CORRELATED ELECTRONS

37

F IG . IV.2. Pseudo spin correlation functions for the ITF according to Eqs. (4.8), (4.9) as function of inverse control parameter 1/ξ = 2/I . Order parameter mz = |Tz | with critical (pressure) exponent 1/8 is also shown. (After Ref. [114].)

Eq. (4.7) one obtains a finite order parameter Tz given in Section VI.14 provided ξ > ξc . The critical exponent of the order parameter is 1/8. In addition the correlation functions may be calculated exactly. In good accuracy they are given by112,113 (j = i ± 1): z z Ti T j = k z , where 1 kz = − 4π

0

π

ξ + cos(q) dq , q

x x Ti Tj = m2x ,

1 mx = 2π

π

dq 0

(4.8)

1 + ξ cos(q) x (4.9) = Ti q

1 2

with q = (1 + ξ 2 + 2ξ cos q) . These correlation functions together with the order parameter are plotted in Figure IV.2. It shows nicely that long range order mz is destroyed when the transverse quantum fluctuations characterized by m2x overwhelm the longitudinal correlations given by kz . The ITF is a generic model for QPTs that may be applied to quite different physical systems. For example, in the case of induced magnetic moment ordering discussed above the two pseudospin states correspond to the two CEF singlet states, the Ising interaction is due to the nondiagonal exchange between them and the transverse field is associated with the CEF splitting energy. On the other hand the same model may be applied to the problem of charge ordering in insulators with a 2D ladder type structure 114 V. Yushankhai and P. Thalmeier, Phys. Rev. B 63, 064402 (2001).

38

P. FULDE ET AL.

like α -NaV2 O5 . In this case the pseudo-spin describes resonating, singly occupied 3d states within the rung of a ladder, the Ising interaction corresponds to the inter-site Coulomb interaction between d-electrons in different rungs and the transverse field is provided by the intra-rung kinetic (hopping) energy. The ITF then describes a quantum phase transition where charge ordering in the rungs is destroyed by the increase of the intra-rung kinetic energy. This will be discussed in detail in Section VI.14. The induced moment magnetism can also appear in a different context in compounds with localized 3d-electrons. Instead of singlet-singlet CEF states as before one may have here singlet-triplet level systems with a splitting due to preformed dimers of S = 1/2 3d-spins. When the inter-dimer exchange coupling is slightly subcritical the magnetic exciton mode with a minimum at the wave vector Q has a finite but small energy and the compound is paramagnetic. Application of a magnetic field splits off one triplet component and the excitation energy at Q is driven to zero at a critical field Hc . There a quantum phase transition to an incommensurate magnetic phase takes place. An example is TlCuCl3 where the Cu2+ spins form dimers.115 Since for 3d spins the orbital degrees are quenched, the inter-dimer coupling is of the Heisenberg- rather than Ising type where the latter has a discrete Z2 symmetry as discussed above. This makes an essential difference since the continuous SU(2) symmetry of the former allows the exchange Hamiltonian to be mapped to a hard-core boson Hamiltonian for the singlet-triplet boson excitations.116 Then the field-driven QPT in TlCuCl3 can be interpreted as Bose–Einstein condensation (BEC) of the singlet-triplet excitations. Another, even cleaner example of magnetic order through BEC, though with different microscopic details was recently identified in Cs2 CuCl4 .117 Actually the mapping to the boson model is already possible for the xy-exchange model with U(1) symmetry in a transverse field which applies to dhcp Pr.111 Thus the appearance of an incommensurate phase under pressure in Figure IV.1 may perhaps also be described within the BEC framework. This has not been investigated yet. 7. Q UANTUM C RITICALITY IN THE KONDO L ATTICE As mentioned in the introduction a great part of the interest on QPTs is focused on strongly correlated metallic systems which exhibit pronounced non-Fermi liquid 115 C. Ruegg, N. Cavadini, A. Furrer, H. U. Güdel, K. Krämer, H. Mutka, A. Wildes, K. Habicht, and P. Vorderwisch, Nature 423, 62 (2003). 116 M. Matsumoto, B. Normand, T. M. Rice, and M. Sigrist, Phys. Rev. B 69, 054423 (2004). 117 T. Radu, H. Wilhelm, V. Yushankhai, D. Kovrizhin, R. Coldea, T. Lühmann, and F. Steglich, Phys. Rev. Lett. 95, 127202 (2005).

STRONGLY CORRELATED ELECTRONS

39

(NFL) behavior. This is found frequently close to pressure- (hydrostatic or chemical) and field-induced QPTs from the paramagnetic to the antiferromagnetic phase of Ce- or Yb-based heavy fermion metals. The schematic phase diagram for such compounds is shown in Figure IV.6. Prominent examples are found among the class of Ce122, Ce115 and Ce218 intermetallic compounds and alloys.54 Classical cases are CePd2 Si2 ,118 CeNi2 Ge2 119 and more recently YbRh2 Si2 .120 Most Ce compounds also exhibit dome-shaped superconductivity, sometimes with very small Tc . It appears in the NFL regime around the quantum critical point of AF order. For an example see Figure IV.6 (right panel). The generic model to describe the quantum critical Ce HF compounds is the Kondo lattice model given by

† k ckσ ckσ + JK si Si . (4.10) HKL = kσ

i

The first term describes conduction electrons with a dispersion k and bandwidth W . The second term is a local AF (JK > 0) coupling of conduction electron spins si to localized spins Si . There are two competing effects. Firstly, the solutions of the Kondo impurity model (a single spin Si=0 coupled to the Fermi sea) shows that below the Kondo temperature TK = W exp(−1/JK N (0)) the local moment is screened. A singlet is formed which extends to a distance ξK ∼ hv ¯ F /TK from the impurity site.50 Secondly, in the lattice the polarization of conduction electrons due to an on-site exchange induces an effective RKKYtype interaction between localized spins. This leads to a tendency to magnetic order at a temperature of the order TRKKY ∼ JK2 χ(2kF ) where χ(q) is the conduction electron susceptibility. When TRKKY TK local but overlapping singlets form a nonmagnetic state and below a coherence temperature Tcoh < TK they disperse into quasiparticle bands as indicated in Figure IV.6 (see also Section III). For TRKKY TK the singlet formation is inhibited and magnetic order sets in at TN . When the two temperature scales are about the same size one expects a quantum phase transition between the magnetically ordered and nonmagnetic heavy Fermi liquid state. This criterion is only a heuristic guide because TK is the nonperturbative energy scale (the singlet binding energy) of the impurity problem, whereas TRKKY is the perturbative energy scale on the lattice. The control parameter of the model is X = JK /W which may be assumed to vary linearly with pressure. This behavior is illustrated in the Doniach-type phase diagram around 118 F. M. Grosche, I. R. Walker, S. R. Julian, N. D. Mathur, D. M. Freye, M. J. Steiner, and G. G. Lonzarich, J. Phys. Condens. Matter 13, 2845 (2001). 119 R. Küchler, N. Oeschler, P. Gegenwart, T. Cichorek, K. Neumaier, O. Tegus, C. Geibel, J. A. Mydosh, F. Steglich, L. Zhu, and Q. Si, Phys. Rev. Lett. 91, 066405 (2003). 120 J. Custers, P. Gegenwart, H. Wilhelm, K. Neumaier, Y. Tokiwa, O. Trovarelli, C. Geibel, F. Steglich, C. Pepin, and P. Coleman, Nature 424, 524 (2003).

40

P. FULDE ET AL.

the QCP (Figure IV.6). The wedge above the QCP is the region where NFL behavior of thermodynamic coefficients and transport properties is observed. This qualitative picture is hard to quantify. In fact the Kondo lattice model is an unsolved problem and only various approximative and numerical methods have been applied to it. The problem may be somewhat simplified by eliminating the charge degrees of freedom. This was proposed in Ref. [121] for the 1D Kondo chain. Using a Jordan–Wigner transformation the 1D conduction electrons may be replaced by a second spin system with xy-type inter-site coupling in addition to the local Kondo spins. The model then reads

y y τix τjx + τi τj + δτiz τjz + JK τ i Si . (4.11) HKN = 2J ij

i

The 1D ‘Kondo necklace’ model based on the Jordan–Wigner transformation of HKL has δ = 0. But later this was generalized to δ > 0 in arbitrary dimension and treated as a model for the competition of AF order (J ) and local singlet formation (JK ) in its own right. The control parameter is now X = JK /2J . The constant 2J associated with interacting spins corresponds to the bandwidth W of conduction electrons in the original HKL . The approximate quantum critical phase diagram of this model may be obtained with the help of the bond operator method.122 It starts from the observation that the four singlet-triplet basis states of a local pair of spins τ i , Si may be represented by singlet-triplet boson creation operators according to |s = s † |0 and |tα = tα† |0 (α = x, y, z). The spin operators may then be expressed in terms of singlet and triplet boson operators: 1 † † sn − iαβγ tnβ tnγ Sn,α = sn† tn,α + tn,α 2 1 † † τn,α = −sn† tn,α − tn,α (4.12) sn − iαβγ tnβ tnγ . 2 † These operators have to fulfill the local constraint sn† sn + α tnα tnα = 1 at every site n. Using the above transformation in HKN one obtains various bosonic interaction terms which may be decoupled by a mean field approximation both in the Hamiltonian and in the constraint. In the strong coupling region where X = JK /2J is large the ground state is characterized by the molecular field s¯ = s corresponding to a condensation of the local singlet bosons. The decoupling then leads to a bilinear Hamiltonian in the triplet bosons which may be diagonalized and yields the triplet excitation energies ωk . From the excitation spectrum the singlet amplitude s¯ (X) and the chemical potential μ(X) (to satisfy the mean-field constraint) are determined self-consistently. Then the minimum 121 S. Doniach, Physica B 91, 231 (1977). 122 G. M. Zhang, Q. Gu, and L. Yu, Phys. Rev. B 62, 69 (2000).

STRONGLY CORRELATED ELECTRONS

41

triplet excitation energy is at the AF zone boundary vector q = Q, and it is equivalent to the spin gap in the Kondo singlet phase. It is given by (z = coordination number)

1 SP = JK + μ/JK 1 − zd/2 4 d=

s¯ 2 2J JK ( 14 + μ/JK )

(4.13)

where the dimensionless parameter d(X) is determined by the self-consistent equation 4J 1 ω0 d= 1− JK 2N ωk ωk = 1 + dγk ω0

k

with γk =

cos kα .

(4.14)

α

When the intermediate coupling regime is approached by decreasing X −1 = 2J /JK the spin gap eventually collapses and a magnetically ordered phase is established. The solution of the above equations is shown in Figure IV.3 for the

F IG . IV.3. Spin gap s in the Kondo singlet (KS) phase and staggered magnetization ms in the AF phase as function of the inverse control parameter 1/X = 2J /JK . Full line is the mean field result for HKN in 2D for the xy case (δ = 0). The dotted line is obtained from Monte Carlo simulations. The QCP is at 1/Xc 0.7. (After Ref. [122].)

42

P. FULDE ET AL.

2D case. Indeed it exhibits a QPT at a critical value Xc ∼ 1.43. For larger X, i.e., in the AF regime an analogous calculation may be performed leading to the staggered magnetization ms shown in the previous figure. In 3D results are similar but the scaling exponents for SP (X) and ms (X) close to the QCP are different. We note that the boson representation employed here for the Kondo-necklace type model is identical to the one used in the spin-dimer problem in TlCuCl3 .116 Therefore the transition from spin gap to AF phase may also be interpreted as a BEC of triplet bosons. The mean-field boson treatment confirms the qualitative conjectures made above on the quantum critical phase diagram by simply comparing the energy scales of singlet formation and magnetic order. Because it respects the local constraint for bosons only on the average this method is however completely inadequate to investigate how the on-site singlet and inter-site magnetic correlations compete as function of control parameter X and also as function of temperature. For this purpose one has to use advanced numerical approaches like the finite temperature Lanczos method123 for finite size clusters. This method has recently been employed to Kondo lattice like models given by HKL and also HKN with δ = 1, i.e., in the Heisenberg limit for the interacting τ -spins.124 Because each site has 4 states, the possible cluster sizes for exact diagonalization are limited. The 8-site cluster of the square lattice with periodic boundary conditions was investigated and correlation functions and specific heat were calculated.124 The Lanczos procedure is repeated 400 times for random starting vectors in the 4N (N = 8)-dimensional Hilbert space until convergence for thermodynamic quantities is achieved. The specific heat results are shown in Figure IV.4 (upper panel) for various values of the control parameter X = JK /2J . For JK = 0 the broad upper maximum corresponds to the AF correlations of the ‘itinerant’ τ -spins. When JK is turned on a lower much sharper maximum rapidly evolves which shifts to higher temperatures and for X ∼ 1.5 eventually merges with the upper maximum. The origin of the lower sharp maximum becomes clear if one monitors the on-site singlet correlation τ 1 · S1 and the induced ‘RKKY’ correlations S1 · S2 between the localized (but non-interacting) spins at n.n. sites 1 and 2. These correlations are shown in Figure IV.5 as function of temperature. For JK = 0 both correlations are absent. When JK is turned on τ 1 · S1 develops AF on-site singlet correlations with a limiting value of −0.75 in the strong coupling limit (upper panel). Due to the inter-site coupling of τ -spins the local singlet formation also induces AF inter-site correlations of the previously uncoupled Si spins (lower panel). In the strong coupling limit when on-site singlets are formed, however, the inter-site correlations of Si spins are diminished again. The sharp maximum in CV is well correlated with the inflection point of the induced inter-site correlations. Therefore 123 G. Jaclic and N. B. Prelovsek, Adv. Phys. 49, 1 (2000). 124 I. Zerec, B. Schmidt, and P. Thalmeier, Physica B, in press.

STRONGLY CORRELATED ELECTRONS

43

F IG . IV.4. Upper panel: The specific heat CV of the 8-site cluster. Lower panel: ‘Phase diagram’ of the 8-site cluster (inset) obtained from tracing the characteristic maxima of CV (full lines) and inflection points of correlation functions (from Figure IV.5) as function of control parameter X = JK /2J . PM = paramagnetic phase, ‘AF’ = phase with AF correlations of τ -spins. ‘LAF’ = phase with AF correlations of local spins S. ‘Local Singlet’—phase with Kondo spin gap. (After Ref. [124].)

in the thermodynamic limit it may be interpreted as the CV -anomaly due to AF order of partially Kondo-screened local moments. For larger JK the sharp lower CV maximum merges with the broad upper maximum but the inflection point in S1 · S2 may still be identified. Following these characteristic temperatures as function of X a ‘phase diagram’ of the Kondo-lattice type model HKN (δ = 1) may be constructed as shown in Figure IV.4 (lower panel). For small values of JK one finds a correlated state of ‘itinerant’ τ spins (‘AF’) below the temperature of the broad maximum in CV . Below the sharp maximum temperature one has induced antiferromagnetic correlations of the local S spins (‘LAF’). For larger

44

P. FULDE ET AL.

F IG . IV.5. Upper panel: On-site correlations show singlet formation at low temperatures. Lower panel: Simultaneously inter-site ‘RKKY’ correlations are induced for moderate JK and suppressed again for large JK . (After Ref. [124].)

values of JK both maxima merge but correlations of the LAF state are still visible (dotted line). For even larger JK the ‘Local Singlet’ formation dominates correlation and specific heat behavior. Of course, due to the finite cluster size one may not strictly speak about thermodynamic phases and phase boundaries. However, the qualitative evolution of correlations and thermodynamic anomalies as function of control parameter X may be expected to survive in the thermodynamic limit. It is interesting to compare these findings with the previous mean-field calculation for the quantum phase transition as function of X. In the cluster calculation one would identify the ‘QCP’ with the value of X = JK /2J where the correlations show a cross-over from inter-site (‘LAF’) to ‘Local Singlet’ type behavior along the T = 0 line in Figure IV.4 (lower panel). This is found to be at Xc ∼ 1–1.5 and

STRONGLY CORRELATED ELECTRONS

45

compares reasonably well with the value Xc = 1.43 of the mean-field calculation (where however δ = 0 was taken). 8. S CALING T HEORY C LOSE TO THE Q UANTUM C RITICAL P OINT The previous calculations give an insight into the microscopic mechanism of singlet formation vs magnetic order in the Kondo lattice. These results are, however, still far removed from explaining the most common experiments around the QCP, notably the temperature and field scaling for specific heat, susceptibility, resistivity, etc. Assuming the existence of a QCP some insight into the dependence of physical quantities on temperature and control parameters close to it (see Figure IV.6) may be obtained within a simple phenomenological scaling theory. A Kondo impurity in a metallic host shows all the signatures of a local Landau Fermi liquid state50 at temperatures T T ∗ , notably a scaling of the free energy density with T /T ∗ . This leads to universal relations among low temperature thermodynamic quantities irrespective of the microscopic details. This idea has been successfully extended to the Fermi liquid phase of heavy fermion and

F IG . IV.6. Left panel: Schematic phase diagram for Kondo compounds with a QCP (r = 0) separating AF (left) and LFL (right) phases (full line). Scaling of characteristic temperatures is indicated (broken lines). (After Ref. [125].) Right panel: Hydrostatic pressure induced AF to HF liquid QPT in CePd2 Si2 . The AF structure is indicated. At the critical pressure pc = 2.86 GPa the resistivity shows pronounced NFL behavior ρ(T ) ∼ T n with n = 1.2 down to the superconducting transition (inset). (After Ref. [118].) 125 M. A. Continentino, Brazilian Journal of Physics 35, 197 (2004).

46

P. FULDE ET AL.

mixed-valent compounds in a phenomenological scaling ansatz.126–128 The aim was to explain observed relations between quantities like specific heat, thermal expansion, magnetostriction and others. It is natural to apply these ideas also to the vicinity of the QCP, where the characteristic energies T ∗ (p) and Tc (p) themselves depend on the distance r to the QCP which then appears as a further scaling variable.129 The associated correlation length (ξ ) and time scales of quantum fluctuations (τ ) diverge on approaching the phase transition. Their critical exponents are universal, depending only on dimension and the degrees of freedom of the order parameter. We define the quantities r=

X − Xc , Xc

t=

T − Tc Tc

(X = p or H )

(4.15)

which measure the distance to the critical control parameter Xc and the transition temperature Tc respectively. On approaching the QCP at T = 0, r = 0 the correlation length, fluctuation time and free energy scale like94,125

T H . (4.16) ξ ∼ |r|−ν , τ ∼ |r|−νz , f ∼ |r|2−α f˜ , T ∗ H∗ Here H ∗ has the meaning of ‘metamagnetic’ field scale. For fields H H ∗ the heavy quasiparticle state is destroyed by breaking the Kondo singlet state. For QPTs the hyperscaling relation which relates critical exponents to the effective dimension is given by94 2 − α = νdeff ,

deff = d + z.

(4.17)

In the case of a Gaussian fix point appropriate for deff > 4 one has ν = 12 . In the free energy of Eq. (4.16) which is a generalization of the one used in126–128 the characteristic temperature (T ∗ ) and metamagnetic field (H ∗ ) have scaling relations T ∗ ∼ |r|νz ,

H ∗ ∼ |r|φh .

(4.18)

In the magnetically ordered regime T ∗ has to be replaced by the magnetic transition temperature which scales as Tc ∼ |r|ψ where ψ is the shift exponent. Below the upper critical dimension, i.e., for deff < dc = 4 the hyperscaling relation Eq. (4.17) is equivalent to the assumption ψ = νz.125 In this case Tc (r) and T ∗ (r) 126 R. Takke, M. Niksch, W. Assmus, B. Lüthi, R. Pott, R. Schefzyk, and D. K. Wohlleben, Z. Phys. B

44, 33 (1981). 127 P. Thalmeier and P. Fulde, Europhys. Lett. 1, 367 (1986). 128 A. B. Kaiser and P. Fulde, Phys. Rev. B 37, 5357 (1988). 129 L. Zhu, M. Garst, A. Rosch, and Q. Si, Phys. Rev. Lett. 91, 066404 (2003).

STRONGLY CORRELATED ELECTRONS

47

scale symmetrically around the QCP (Figure IV.6), however for deff > 4 in general one has ψ = νz. This is known as ‘breakdown of hyperscaling’. Within a generalized Landau–Ginzburg–Wilson approach this may be understood as the effect of a dangerously irrelevant quartic interaction. Although it scales to zero for deff > 4, it changes nevertheless the scaling behavior at finite T leading to a modified shift exponent ψ = z/(deff − 2) for deff > dc . From an experimental viewpoint the most interesting aspect is the temperature dependence of physical properties at the QCP (r = 0) in the non-Fermi liquid regime. Very useful quantities are specific heat C = (T /V )(∂S/∂T )p and thermal expansion α = (1/V )(∂V /∂T )p .119,129 At the QCP (r = 0) they scale with temperature like C(T ) ∼ T d/z ,

1

α(T ) ∼ T (d− ν )/z

and =

1 α ∼ T − νz . C

(4.19)

This means that the temperature dependence of the critical ‘Grüneisen ratio’ (r = 0) is controlled by the exponent which directly determines the time scale of quantum fluctuations in Eq. (4.16). Using this important relation a consistent explanation of experiments in the NFL compound CeNi2 Ge2 can indeed be given (Figure IV.7). Tables of the scaling behavior of the quantities in Eq. (4.19) for various d, z have been given in Ref. [129]. The exponent νz determines at the same time pressure scaling (Eq. (4.18)) of the characteristic temperature T ∗ on the nonmagnetic side of the QCP. On the other hand the pressure scaling exponent φh of the characteristic field H ∗ is an independent quantity within the scaling ansatz. Experimentally it has been investigated in detail for CeRu2 Si2 which has a metamagnetic field scale H ∗ (p = 0) = 7.8T (H c). It was found empirically that φh = 2 − α = νz is fulfilled. According to the free energy in Eq. (4.16) this implies with m = (∂f/∂H ) that m(H ∗ ) = const independent of pressure. This was indeed found experimentally.130 The empirical relation 2 − α = νz may be interpreted as quantum hyperscaling relation with dimension d = 0 according to Eq. (4.17). The empirical validity of such a relation points to a dimensional crossover as function of pressure close to the QCP which is caused by the different divergence of spatial and temporal correlations.125 An explicit calculation of scaling exponents close to the QCP demands the use of effective field theories based on Ginzburg–Landau type action functionals for the spatial and temporal order parameter fluctuations. Such theories are not specific for strongly correlated electron systems and therefore are beyond the scope of this review. As mentioned before they have indeed first been constructed for 130 A. Lacerda, A. de Visser, P. Haen, P. Lejay, and J. Flouquet, Phys. Rev. B 40, 8759 (1989).

48

P. FULDE ET AL.

F IG . IV.7. Thermal expansion showing the suppression of NFL behavior as function of field. The inset shows that for B = 0 the critical contribution to the Grüneisen ratio of CeNi2 Ge2 scales like ∼ 1/T νz with νz = 1. According to Eq. (4.19) this means (assuming z = 2 for AF SDW) a mean field correlation length exponent ν = 1/2 which is in agreement with deff = d + z = 5 for the effective dimension. (After Ref. [119].)

weakly correlated metals in Refs. [48,100,101] and Ref. [102] and have been reinvestigated later in hindsight of QPTs in strongly correlated metals.131 Until now the results and even starting assumptions of these field theoretical approaches are controversial and will not be discussed here. V. Partial Localization

The concept of orbital-selective localization applies to correlated systems with orbital degeneracies. Important examples are transition metal oxides132–135 and 5f compounds. In these materials, the intra-atomic correlations as described by Hund’s rules play an important role. Nevertheless the physics of partial localization in transition metal oxides and 5f systems is quite different. In compounds 131 A. J. Millis, Phys. Rev. B 48, 7183 (1993). 132 V. I. Anisimov, I. A. Nekrasov, D. E. Kondakov, T. M. Rice, and M. Sigrist, Eur. Phys. J. B 25,

191 (2002). 133 A. Koga, N. Kawakami, T. M. Rice, and M. Sigrist, Phys. Rev. Lett. 92, 216402 (2004). 134 A. Liebsch, Phys Rev. Lett. 95, 116402 (2005). 135 M. S. Laad, L. Craco, and E. Müller-Hartmann, Europhys. Lett. 69, 984 (2005).

STRONGLY CORRELATED ELECTRONS

49

with d electrons the large crystalline electric field (CEF) set up by the surroundings of a transition metal ion plays a major role. It is often larger than the bandwidth as, for example in the manganites (Section VI.15). In case of a cubic lattice it splits the five d orbitals into a t2g triplet and an eg doublet and the corresponding subbands are well separated. When the Hund’s rule energy is larger than this splitting and when the orbital energy of the t2g is lower than that of the eg states the t2g states will be occupied by the first three d electrons. Those three d electrons remain localized in a high-spin state with S = 3/2. Additional d electrons occupy eg states and remain delocalized. The situation differs when the CEF splitting is larger than Hund’s rule coupling. In that case the t2g subband can accommodate six electrons. When the d electron count per ion nd is larger than six, i.e., nd > 6 only (nd − 6) d electrons will be itinerant and contribute to metallic behavior. In 5f compounds we are facing a different situation. Since the 5f atomic wavefunctions are closer to the nuclei than d electron wavefunctions are, CEF splittings are smaller and less important. But Hund’s rule energies are larger. Therefore when we deal with a situation where the 5f count per actinide ion nf exceeds two, i.e., nf > 2 only those 5f electrons will delocalize which enable the remaining ones to form a Hund’s rule state. Otherwise the Coulomb interaction is increased so much that delocalization is disadvantageous as far as energy is concerned. Therefore Hund’s rule correlations may strongly enhance anisotropies in the kinetic energy and eventually lead to the co-existence of band-like itinerant 5f states with localized atomic-like ones. The central focus of the present section is the dual model for actinide-based heavy fermion compounds which assumes the co-existence of delocalized and localized 5f electrons. Initially, the dual character has been conjectured for UPd2 Al3 where the variation with temperature of the magnetic susceptibility points to the coexistence of CEF-split localized 5f states in a heavy fermion system with 5f -derived itinerant quasiparticles. Direct experimental evidence for the co-existence of 5f -derived quasiparticles and local magnetic excitations is provided by recent neutron scattering experiments.136 There is clear evidence that the presence of localized 5f states is responsible for the attractive interaction leading to superconductivity.137 In addition the dual model could allow for a rather natural description of heavy fermion superconductivity co-existing with 5f -derived magnetism. For a recent review of experimental facts see Refs. [53,54]. Heavy quasiparticles have been observed by de Haas–van Alphen (dHvA) experiments in a number of U compounds. The experiments unambiguously confirm 136 A. Hiess, N. Bernhoeft, N. Metoki, G. H. Lander, B. Roessli, N. K. Sato, N. Aso, Y. Haga, Y. Koike, T. Komatsubara, et al., cond-mat/0411041 (2004). 137 N. Sato, N. Aso, K.. Miyake, R. Shiina, P. Thalmeier, G. Varelogiannis, C. Geibel, F. Steglich, P. Fulde, and T. Komatsubara, Nature 410, 340 (2001).

50

P. FULDE ET AL.

that some of the U 5f electrons must have itinerant character. It has been known for quite some time that the 5f -states in actinide intermetallic compounds cannot be considered as ordinary band states. Standard bandstructure calculations based on the Local Density Approximation (LDA) to Density Functional Theory fail to reproduce the narrow quasiparticle bands. On the other hand the LDA bandwidths are too small to explain photoemission data.138,139 These shortcomings reflect the inadequate treatment of local correlations within ordinary electron structure calculation. Theoretical studies aiming at an explanation of the complex low-temperature structures lay emphasis on the partitioning of the electronic density into localized and delocalized parts.140,141 Concerning the low-energy excitations it has been shown that the dual model allows for a quantitative description of the renormalized quasiparticles—the heavy fermions—in UPd2 Al3 . The measured dHvA frequencies for the heavy quasiparticle portions as well as the large anisotropic effective masses can be explained very well by treating two of the 5f electrons as localized. The central goal of the present section is (1) to demonstrate that the dual model allows to determine the heavy quasiparticles in U compounds without adjustable parameters and (2) to give a microscopic justification for the underlying assumptions. Before turning to a discussion of the dual model, its results and their implications we should like to add a few comments. In referring to the dual model one has to keep in mind that the latter provides an effective Hamiltonian designed exclusively for the low-energy dynamics. As such it seems appropriate for typical excitation energies hω ¯ below ∼ 10 meV. In general, effective low-energy models are derived from the underlying microscopic Hamiltonians—to borrow the language of Wilson’s renormalization group— by integrating out processes of higher energies. In the case of 5f systems the conjecture is that the hybridization between the conduction electrons and the 5f states effectively renormalizes to zero for some channels while staying finite for others. We shall show that the physical mechanism leading to the orbital-dependent renormalization of the hybridization matrix elements are the intra-atomic correlations which are often described by Hund’s rules. To focus on the role of the intra-atomic correlations we consider model Hamiltonians for the 5f subsystem where the hybridization with the conduction 138 J. W. Allen, in Synchrotron Radiation Research: Advances in Surface and Interface Science, Plenum Press, New York (1992), vol. 1, chap. 6, p. 253. 139 S. Fujimori, Y. Saito, M. Seki, K. Tamura, M. Mizuta, K. Yamaki, K. Sato, T. Okane, A. Tanaka, N. Sato, et al., J. Electron Spectrosc. Relat. Phenom. 101–103, 439 (1999). 140 L. Petit, A. Svane, W. M. Temmerman, Z. Szotek, and R. Tyer, Europhys. Lett. 62, 391 (2003). 141 J. M. Wills, O. Eriksson, A. Delin, P. H. Andersson, J. J. Joyce, T. Durakiewicz, M. T. Butterfield, A. J. Arko, D. P. Moore, and L. A. Morales, J. Electron Spectrosc. Relat. Phenom. 135, 163 (2004).

STRONGLY CORRELATED ELECTRONS

51

electrons is accounted for by introducing effective 5f hopping. The orbitaldependent suppression of hybridization then translates into orbital-selective localization. The concept of correlation-driven partial localization in U compounds has been challenged by various authors (see, e.g., Ref. [142]). The conclusions are drawn from the fact that conventional band structure calculations within the Local Density Approximation (LDA) which treat all 5f -states as itinerant can reproduce ground state properties like Fermi surface topologies and densities. The calculation of ground state properties, however, cannot provide conclusive evidence for the delocalized or localized character of the 5f -states in actinides. First, the presence of localized states can be simulated in standard band calculations by filled bands lying (sufficiently far) below the Fermi level. Second, the Fermi surface is mainly determined by the number of particles in partially filled bands and the dispersion of the conduction bands which, in turn, depends mainly on the geometry of the lattice. A change in the number of band electrons by an even amount does not necessarily affect the Fermi surface since a change by an even number may correspond to adding or removing a filled band. As such, the Fermi surface is not a sensitive test of the microscopic character of the states involved. Unambiguous proof of the dual character can be provided by an analysis of the spectral function. Of particular importance are characteristic high-energy features associated with transitions into excited local multiplets. A detailed discussion of these features will be given in Section VIII. 9. H EAVY Q UASIPARTICLES IN UP D 2 A L 3 Within the dual model the strongly renormalized quasiparticles in U -based heavy fermion compounds are described as itinerant 5f electrons whose effective masses are dressed by low-energy excitations of localized 5f states. We refer to Refs. [33,54] for a detailed description which proceeds in three steps. The latter include (a) a band structure calculation to determine the dispersion of the bare itinerant 5f states (b) a quantum chemical calculation which yields the localized 5f multiplet states and, in particular, their coupling to their itinerant counterparts and, finally, (c) a standard (self-consistent) many-body perturbation calculation to determine the renormalized effective mass. We should like to emphasize, however, that we treat all 5f electrons as quantum mechanical particles obeying Fermi anticommutation relations. The scheme has been successfully applied to UPd2 Al3 and UPt3 as can be seen from the comparison between the calculated and measured dHvA frequencies and 142 I. Opahle, S. Elgazzar, K. Koepernik, and P. M. Oppeneer, Phys. Rev. B 70, 104504 (2004).

52

P. FULDE ET AL.

the effective masses in Figure V.1 and Table V.1, respectively. It is important to note that the data are derived from a parameter-free calculation. To show this we examine the individual steps as described above. First, the bare 5f band dispersion is determined from a parameter-free ab initio calculation by solving the Dirac equation for the self-consistent LDA potentials

F IG . V.1. Upper panel: Fermi surface of UPd2 Al3 calculated within the dual model.33 The main cylinder part has effective masses with m∗ = 19–33m, the highest masses are found on the torus. Lower panel: Comparison of experimental dHvA frequencies (black symbols) from Ref. [143] and calculated frequencies (open symbols) (After Ref. [33]). The large parabola corresponds to the main FS cylinder. 143 Y. Inada, H. Yamagani, Y. Haga, K. Sakurai, Y. Tokiwa, T. Hinma, E. Yamamoto, Y. Onuki, and T. Yanagisawa, J. Phys. Soc. Jpn. 68, 3643 (1999).

STRONGLY CORRELATED ELECTRONS

53

TABLE V.1. E FFECTIVE M ASSES IN UP D 2 A L 3 FOR H c. N OTATION FOR FS S HEETS AND E X VALUES FROM R EF. [143], m0 I S THE F REE E LECTRON M ASS . T HEORETICAL VAL UES FROM R EF. [33]

PERIMENTAL

FS sheet

m∗ /m (exp.)

ζ γ β 2 3 β

65 33 19 18 12 5.7

m∗ /m (theory) 59.6 31.9 25.1 17.4 13.4 9.6

but excluding two U 5f (j = 52 ) states from forming bands. The apparent absence of Kramers’ degeneracy in this compound suggests to treat an even number of 5f electrons as localized. The calculations yield the dHvA frequencies which can be directly compared with experimental data. At this point we should like to briefly comment on the strategy to account for long-range antiferromagnetic order. The two examples, UPd2 Al3 and UPt3 , represent two different categories. In UPd2 Al3 localized 5f moments order antiferromagnetically at TN 14.5 K with the induced moment being 0.83μB per U. The heavy quasiparticles form in the magnetically ordered state. As a consequence, the calculation of the bare 5f bands employs the experimentally observed antiferromagnetic structure. The superstructure strongly affects the Fermi surface topology for the heavy quasiparticles. The corresponding paramagnetic model cannot reproduce the heaviest orbit. In the second step, the localized U 5f states are calculated by diagonalizing the Coulomb matrix in the restricted subspace of the localized 5f states. Assuming the j -j coupling scheme, the Coulomb matrix elements are evaluated using the radial functions of the ab initio band structure potentials. The coupling between the localized and delocalized 5f electrons is directly obtained from the expectation values of the Coulomb interaction in the 5f 3 states. Finally, the renormalization of the effective masses which results from the coupling between the two 5f subsystems is estimated. The itinerant 5f states scatter off the low-energy excitations of the localized 5f 2 configurations. The situation resembles that in Pr metal where a mass enhancement of the conduction electrons by a factor of 5 results from virtual crystal field (CEF) excitations of localized 4f 2 electrons.144 The effective masses in Table V.1 are obtained from an isotropical renormalization of the band mass mb is given by m∗ ∂ |ω=0 . =1− mb ∂ω 144 R. White and P. Fulde, Phys. Rev. Lett. 47, 1540 (1981).

(5.1)

54

P. FULDE ET AL.

F IG . V.2. Self-energy diagram due to local intra-atomic excitations leading to a mass enhancement. Solid double line: full Green’s function of the conduction electrons. Dashed lines: effective intra-atomic two-level states |α, |β separated by an excitation energy δ¯ = 7 meV. Triangles: matrix elements a|M|.

The local self-energy of the delocalized 5f states (ω) is displayed in Figure V.2. The explicit expressions are given in.33 The mass enhancement is calculated selfconsistently inserting values for the density of states at the Fermi level N (0) = 2.76 states/(eV cell spin) obtained from the bandstructure, when two 5f electrons are kept localized. The vertex is given by a|M| = 0.084 eV where the prefactor a denotes the 5f weight per spin and U atom of the conduction electron states near EF . The matrix element M describes the transition between the localized states |4 and |3 due to the Coulomb interaction UCoul with the delocalized 5f electrons. These are the two lowest eigenstates of the localized 5f 2 system in the presence of the CEF. They have J = 4 in accordance with Hund’s rule and are combinations of |Jz = | ± 3. Finally, the dynamical susceptibility is approximated by that of an effective two-level system with an excitation energy δ¯ 7 meV. 10. M ICROSCOPIC M ODEL C ALCULATION To illustrate the orbital selection by intra-atomic correlations we consider a simple molecular model consisting of two actinide atoms at sites a and b. The strong Coulomb interaction among the 5f electrons at the same site leads to well-defined ionic configurations f n with energies E(f n ). To model U compounds we assume that the total number of 5f electrons in the cluster be five corresponding to an averaged f -occupation of 2.5 per U site. The ground state will be a linear combination of states |a; f 3 |b; f 2 and |a; f 2 |b; f 3 , respectively. These two sets of states are coupled by the hopping term. Since both atoms have more than one

STRONGLY CORRELATED ELECTRONS

55

electron in their 5f shells intra-atomic correlations come into play. The two sets of basis functions split into groups of states characterized by the total angular momenta J (a) and J (b), respectively, the energy differences being of the order of the 5f exchange constant, i.e., approximately 1 eV. Since the spin-orbit interaction is large we use j -j coupling and restrict ourselves to 5f states with j = 5/2. We are aiming at the low-energy subspace which is spanned by the states |a; f 3 , J (a) = 9/2|b; f 2 , J (b) = 4 and |a; f 2 , J (a) = 4|b; f 3 , J (b) = 9/2, in close analogy to Hund’s rules. Transferring an electron from site a to site b changes the local f occupation and the total angular momenta a; f 3 , J (a) = 9/2 b; f 2 , J (b) = 4 → a; f 2 , J (a) b; f 3 , J (b) (5.2) and the resulting final state will usually contain admixtures from excited multiplets. The transfer of a 5f electron from site a to site b causes intra-atomic excitations against which the gain in kinetic energy has to be balanced. The crucial point is that the overall weight of the low-energy contributions to the final state depends upon (a) the orbital symmetry of the transferred electron, i.e., on jz and (b) on the relative orientation of J(a) and J(b). The latter effect closely parallels the “kinetic exchange” well-known from transition metal compounds. The requirement that the gain in energy associated with the hopping be maximal leads to orbital selection. The dynamics in the low-energy subspace is described by an effective single-particle Hamiltonian where some of the transfer integrals are renormalized to zero while others are reduced yet remain finite. These qualitative considerations are the basis for microscopic model calculations which proceed from the simple model Hamiltonian H = Hband + HCoul . The local Coulomb repulsion part 1

HCoul = Ujz1 ,jz2 jz3 jz4 cj†z (a)cj†z (a)cjz3 (a)cjz4 (a) 1 2 2 a

(5.3)

(5.4)

jz1 ,...,jz4

is written in terms of the usual fermionic operators cj†z (a) (cjz (a)) which create (annihilate) an electron at site a in the 5f -state with total angular momentum j = 5/2 and z-projection jz . Considering the fact that the spin-orbit splitting is large we neglect contributions from the excited spin-orbit multiplet j = 7/2 and adopt the j -j coupling scheme. The Coulomb matrix element Ujz1 jz2 jz3 jz4 for jzi = −5/2, . . . , 5/2

J Jz JJ Ujz1 jz2 jz3 jz4 = UJ C5/2,j C z (5.5) z1 ;5/2,jz2 5/2,jz3 ;5/2,jz4 J ... and the Coulomb are given in terms of the usual Clebsch–Gordan coefficients C... parameters UJ . Here J denotes the total angular momentum of two electrons

56

P. FULDE ET AL.

and Jz = jz1 + jz2 = jz3 + jz4 . The sum is restricted by the antisymmetry of the Clebsch–Gordan coefficients to even values J = 0, 2, 4. The kinetic energy operator describes the hopping between all pairs at neighboring sites ab

tjz cj†z (a)cjz (b) + h.c. + f cj†z (a)cjz (a). (5.6) Hband = − ab,jz

a,jz

We assume the transfer integrals tjz to be diagonal in the orbital index jz . While this is certainly an idealization it allows us to concentrate on our main interest, i.e., the interplay of intra-atomic correlations and kinetic energy. Finally, we account for the orbital energy f which determines the f -valence of the ground state. Due to the local degeneracy, the Hilbert space increases rapidly with the number of lattice sites and exact (numerical) solutions are possible only for relatively small clusters. For extended systems, i.e., for periodic solids the ground state and the low-lying excitations can be determined within a mean-field approximation.145 The slave-boson functional integral method allows for a discussion of various ground states and co-operative phenomena starting from realistic bare electronic band structures. The orbital-dependent separation of the low-energy excitations into dispersive quasiparticle bands and incoherent background is observed in the spectral functions of a linear chain calculated by means of Cluster Perturbation Theory.146 Itineracy is reflected in a discontinuity of the orbital-projected momentum distribution function (5.7) njz (k) = dω f (ω)Ajz (k, ω) where Aj z (k, ω) is the single-particle spectral function while f (ω) denotes the Fermi distribution. Here we discuss the qualitative features derived for two-site clusters where we can find simple approximate forms for the ground-state wavefunction in limiting cases. In order to quantify the degree of localization or, alternatively, of the reduction of hopping of a given jz orbital by local correlations, the ratio of the jz -projected kinetic energy Tjz and the bare matrix element tjz

Tjz = gs | cj†z (a)cjz (b) + h.c. |gs (5.8) tjz ab,

The ground-state wavefunction |gs contains the strong on-site is correlations. A small ratio of Tjz /tjz indicates partial suppression of hopping for electrons in the ±jz orbitals. Two kinds of correlations may contribute to that calculated.33

145 J. Jedrak and G. Zwicknagl, preprint (2005). 146 F. Pollmann, and G. Zwicknagl, Phys Rev. B 73, 035121 (2006).

STRONGLY CORRELATED ELECTRONS

57

process. The first one is based on the reduction of charge fluctuations due to the large values of the isotropically averaged Coulomb repulsion which results in an isotropic renormalization of the kinetic energy. As this is a typical high-energy effect we defer the discussion to Section VIII. In the strong-coupling limit the reduction of charge fluctuation is accounted for by restricting the ground state to the well-defined atomic configurations. The quantity of interest here is the orbitaldependent reduction Tjz /tjz which is due to intra-atomic correlations. As the latter are local in nature, even small clusters should adequately describe the important qualitative features. The results for Tjz /tjz 33 —initially obtained perturbatively for a two-site cluster—as well as their interpretation are confirmed by detailed calculations based on exact diagonalization for small clusters.147 Figure V.3 displays the reduction factors for a two-site cluster. The model parameters U4 = UJ =4 − UJ =0 = −3.79 eV U2 = UJ =2 − UJ =0 = −2.72 eV.

(5.9)

are chosen appropriate for UPt3 . These findings demonstrate that in particular Hund’s rule correlations strongly enhance anisotropies in the hopping. For a certain range of parameters this may result in a complete suppression of the effective hopping except for the largest one, which remains almost unaffected. This provides a microscopic justification of partial localization of 5f electrons which is observed in a number of experiments on U intermetallic compounds. As the relevant correlations are local, the general results qualitatively agree with those found for a three-site cluster and four-site clusters.148 The magnetic character, however, is affected by finite size effects. This can be seen by varying the cluster sizes and the boundary conditions. Although the total angular momentum component Jz may be different for periodic and open boundary conditions we can identify the following different regimes in the strong-coupling limit. In the strongly anisotropic limit with dominating transfer integral |t3/2 | |t1/2 | = |t5/2 | the high-spin states with ferromagnetic inter-site correlations are energetically most favorable. In the two-site cluster, the ground state has a very simple form

1 t † † † † † † | = √ c3/2 (a) + c3/2 (b) c5/2 (a)c1/2 (a)c5/2 (b)c1/2 (b)|0 |t| 2

(5.10)

being simultaneously an eigenstate of the Coulomb energy and of the kinetic energy. It can be considered as a bonding jz = 3/2 state in a ferromagnetically aligned background. The high-spin phases are followed by complicated 147 D. V. Efremov, N. Hasselmann, E. Runge, P. Fulde, and G. Zwicknagl, Phys. Rev. B 69, 115114 (2004). 148 M. Reese, F. Pollmann, and G. Zwicknagl (2006), unpublished.

58

P. FULDE ET AL.

F IG . V.3. Left panel: Values Tjz /tjz for a two-site cluster along a line connecting linearly the points written below the figure. (After Ref. [147].) Right panel: Variation with wave number of (Ajz (k , ω) + A−jz (k , ω)) in the low-energy regime calculated for a two-site cluster with five electrons. The corresponding values of the transfer integrals are those of the left panel. The full line and the dotted line refer to k = 0 and k = π , respectively. Spectral weight is transferred to local excitations (valence transitions and transitions into excited atomic multiplets) which are not displayed here. The Lorentzian broadening is η = 0.03 (After Ref. [146].)

intermediate-spin phases as the isotropic limit t1/2 = t3/2 = t5/2 is approached. In the case with subdominant |t3/2 | |t1/2 | = |t5/2 | low-spin phases with antiferromagnetic intersite correlations are formed. In a two-site cluster, they involve linear combinations of † † † † † (a)c±5/2 (a)c±3/2 (a)c∓5/2 (b)c∓1/2 (b)|0, c1/2 † † † † c±5/2 (a)c±3/2 (a)c∓5/2 (b)c1/2 (b)|0.

The splitting of the low-energy excitations into dispersive quasiparticle states and incoherent background is reflected in the single-particle spectral functions Ajz (k , ω) where the discrete set of quantum numbers k = 0, π labels the singleparticle eigenstates of the two-site cluster. The variation with the transfer integrals is displayed in Figure V.3. The jz -channels with dominant hopping exhibit dispersive narrow peaks while those with subdominant hopping yield an incoherent background. Considerable spectral weight is transferred to the high-energy excitations not shown here.

STRONGLY CORRELATED ELECTRONS

59

11. S UPERCONDUCTIVITY M EDIATED BY I NTRA -ATOMIC E XCITATIONS Since the discovery of the isotope effect149,150 and the work of Fröhlich151 the electron–phonon interaction has been considered the main cause of Cooper-pair formation. By exchanging virtual phonons, electrons may attract each other and form Cooper pairs. Later it was pointed out that phonons need not be the only bosons the exchange of which results in electron attraction. Also magnetic excitations such as paramagnons were considered as candidates for generating superconductivity, although not necessarily in a conventional s-wave pairing state.97,152 Also it had been pointed out that crystalline electric field (CEF) excitations in rareearth ions like Pr have a pronounced effect on superconductivity153–155 when such ions are added to a conventional superconductor and furthermore, that those excitations can be either pair-breaking or pair forming depending on matrix elements between different CEF levels. The experimental observation of those effects, e.g., in doped LaPb3 and LaSn3 156,157 demonstrated not only the reality but also the magnitude of that kind of boson exchanges between conduction electrons. After the discovery of high-temperature superconductivity in some of the cuprate perovskites and even before for some of the heavy-fermion superconductors numerous suggestions of non-phononic pairing interactions were made.158–166 But they were mainly qualitative rather than quantitative and therefore remained inconclusive. For reviews see Refs. [54,167]. Therefore it is of interest that for UPd2 Al3 experimental evidence exists for a non-phononic mechanism causing superconductivity. It has a transition temperature Tc of Tc = 1.8 K; which is 149 E. Maxwell, Phys. Rev. 78, 477 (1950). 150 C. A. Reynolds, B. Serin, W. H. Wright, and L. B. Nesbitt, Phys. Rev. 78, 487 (1950). 151 H. Fröhlich, Phys. Rev. 79, 1950 (845). 152 D. Fay and J. Appel, Phys. Rev. B 16, 2325 (1977). 153 P. Fulde, L. L. Hirst, and A. Luther, Z. Phys. 238, 99 (1970). 154 J. Keller and P. Fulde, J. Low Temp. Phys. 4, 289 (1971). 155 J. Keller and P. Fulde, J. Low Temp. Phys. 12, 63 (1973). 156 F. Heiniger, E. Bucher, J. P. Maitra, and L. D. Longinotti, Phys. Rev. B 12, 1778 (1975). 157 R. W. McCallum, W. A. Fertig, C. A. Luengo, M. B. Maple, E. Bucher, J. P. Maitra, A. R.

Schwedler, L. Mattix, P. Fulde, and J. Keller, Phys. Rev. Lett. 34, 1620 (1975). 158 D. J. Scalapino, E. Loh, and J. E. Hirsch, Phys. Rev. B 34, 8190 (1986). 159 K. Miyake, S. Schmidt-Rink, and C. M. Varma, Phys. Rev. B 34, 6554 (1986). 160 P. W. Anderson, Science 235, 1196 (1987). 161 J. Spalek, Phys. Rev. B 38, 208 (1988). 162 T. Moriya, Y. Takahashi, and K. Ueda, J. Phys. Soc. Jpn. 59, 2905 (1990). 163 P. Monthoux, A. V. Balatsky, and D. Pines, Phys. Rev. Lett. 67, 3448 (1991). 164 P. Monthoux and G. G. Lonzarich, Phys. Rev. B 59, 14598 (1999). 165 P. Monthoux and G. G. Lonzarich, Phys. Rev. B 63, 054529 (2001). 166 P. Monthoux and G. G. Lonzarich, Phys. Rev. B 66, 224504 (2002). 167 N. M. Plakida, High-Temperature Superconductivity, Springer, Berlin, Heidelberg (1995).

60

P. FULDE ET AL.

below the onset of antiferromagnetic (AF) order with a Néel temperature of TN = 14.3 K. Some evidence for a non-phononic pairing mechanism is provided by UPd2 Al3 –Al2 O3 –Pb tunneling measurements.168 The differential conductivity dI /dV shows structure in the regime of 1 meV demonstrating that there are low-energy bosons which result in a frequency dependence (ω) of the order parameter. For phonons this structure would be an order of magnitude higher in energy. The Debye energy of UPd2 Al3 is 13 meV. In addition inelastic neutron scattering (INS) experiments show that the CEF based magnetic excitation energy ωE (q) at q = Q is between 1–1.5 meV depending on temperature.136,137,169,170 It has been argued that these excitations show up in (ω) and cause superconductivity. This is seen in Figure V.4 which shows the INS data as well as the tunneling density of states. The strong coupling of those AF excitons to conduction electrons is also demonstrated in these experiments. The AF structure of UPd2 Al3 consists of ferromagnetic hexagonal planes with a moment of μ = 0.83μB per U ion pointing in [100] direction and stacked antiferromagnetically along the c-axis.171,172 This corresponds to an AF wave vector Q = (0, 0, 1/2). The large moment supports the dual model with two localized 5f electrons. As discussed before the Hund’s rule ground-state multiplet of the 5f 2 localized electrons is J = 4. In a CEF only the two lowest singlets |3 and |4 have to be taken into account. The Hamiltonian is then of the form

† H= kσ ckσ ckσ + δ |4 4 |i kσ

− Jff

i

Ji Jj − 2I0 (geff − 1)

ij

si Ji

(5.11)

i

where kσ = ⊥ (k⊥ σ ) − 2t cos kz

(5.12)

serves as a model for the Fermi surface of UPd2 Al3 in the paramagnetic state. Figure V.3 shows that the Fermi surface in the AF state consists of a cylindrical part and a torus. The torus has the highest effective mass. For simplicity we will neglect it here and model the paramagnetic Fermi surface by a cylinder. The 168 M. Jourdan, M. Huth, and H. Adrian, Nature 398, 47 (1999). 169 N. Sato, N. Aso, G. H. Lander, B. Roessli, T. Komatsubara, and Y. Endoh, J. Phys. Soc. Jpn. 66,

1884 (1997). 170 N. Bernhoeft, N. Sato, B. Roessli, N. Aso, A. Hiess, G. H. Lander, Y. Endoh, and T. Komatsubara,

Phys. Rev. Lett. 81, 4244 (1998). 171 A. Krimmel, P. Fischer, B. Roessli, H. Maletta, C. Geibel, C. Schank, A. Grauel, A. Loidl, and F. Steglich, Z. Phys. B 86, 161 (1992). 172 H. Kita, A. Dönni, Y. Endoh, K. Kakurai, N. Sato, and T. Komatsubara, J. Phys. Soc. Jpn. 63, 726 (1994).

STRONGLY CORRELATED ELECTRONS

61

F IG . V.4. Upper panel: Magnetic exciton dispersion from INS along c∗ (0, 0, ql ) and a ∗ (qh , 0, 0.5) around the AF zone center Q = (0, 0, 0.5) for T = 2 K just above Tc = 1.8 K. A flat dispersion with a corresponding high DOS is observed for q Q. For T < Tc the additional quasielastic response (open circles at zero energy) evolves into sharp resonance peaks within the gap. (After Ref. [136].) Lower panel: Differential conductivity dI /dV for tunneling current along c. The additional hump at V 1.5 meV has been associated with the magnetic exciton mode at Q in the upper panel. This feature is due to a frequency dependent gap (ω) caused by a strong coupling of quasiparticles to magnetic excitons. However the evaluation of the tunneling data needs additional justification (J. Geerk, private communication). (After Ref. [168].)

antiferomagnetic coupling to the conducting electrons is considerably larger than in systems like TbMo6 S8 173 and HoNi2 B2 .174 One should also keep in mind that 173 M. Ishikawa and Ø. Fischer, Solid State Comm. 24, 747 (1977). 174 A. Amici, P. Thalmeier, and P. Fulde, Phys. Rev. Lett. 84, 1800 (2000).

62

P. FULDE ET AL.

in accurate determination of Tc is anyway out of reach and that the aim is here to demonstrate that the non-phononic pairing mechanism yields the right order of magnitude for Tc . Returning to Eq. (5.12) we note that t determines the amount of corrugation of the cylinder. The second term in Eq. (5.11) denotes the CEF splitting with δ = 6–7 meV. The coupling between localized 5f electrons on nearest-neighbor sites is given by Jff and the on-site exchange between localized and itinerant electrons is described by the last term of Eq. (5.11). The effective Landé factor geff refers to the localized 5f electrons. The total intersite exchange is therefore J (q) = Jeff (q) + I02 (geff − 1)2 χe (q)

(5.13)

where χe (q) is the spin susceptibility of the itinerant electrons. Due to that intersite interaction the susceptibility of the system becomes χ(q, ω) =

u(ω) 1 − J (q)u(ω)

(5.14)

where u(ω) is the single-ion susceptibility175 and the CEF excitation energy goes over into an excitation band (magnetic exciton). When J (q) has its maximum value at q = Q and J (Q) ≡ Je exceeds a critical value, i.e., Je > Jcrit the system becomes an induced AF. In that case the Néel temperature TN is given by TN =

δ 2

tanh−1 (J

c /Je )

.

(5.15)

UPd2 Al3 is an induced AF and one finds that Je /Jc = 1.015. The critical value is given by Jc = δ/2M 2 where M = 24 |Jx |3 i . For temperatures T < TN the susceptibility is again of a form similar to Eq. (5.14) but now the single-ion susceptibility contains the effect of the AF molecular field acting on the |4 , |3 states. In that case the magnetic excitations form a band of AF magnons. For a review see, e.g., Refs. [109,176]. They have originally been measured177 with relatively low resolution and later with much better one, see Refs. [136,137] and [178]. Their dispersion has also been derived theoretically in Ref. [179] by in175 B. R. Cooper, Phys. Rev. 163, 444 (1967). 176 J. Jensen and A. R. Mackintosh, Rare Earth Magnetism, Structures and Excitations, Clarendon

Press, Oxford (1991). 177 T. E. Mason and G. Aeppli, Matematisk-fysiske Meddelelser. 45, 231 (1997). 178 N. Bernhoeft, Eur. Phys. J. B 13, 685 (2000). 179 P. Thalmeier, Eur. Phys. J. B 27, 29 (2002).

STRONGLY CORRELATED ELECTRONS

63

cluding the molecular field as well as the anisotropic exchange and agreed nicely with the measured ones. An approximate form is (5.16) ωE (qz ) = ωex 1 + β cos(cqz ) with ωex = 5 meV, β = 0.8 and c denoting the lattice constant perpendicular to the hexagonal planes. The corresponding boson propagator K(qz , ων ) in Matsubara frequency notation (ων = 2πT , ν = integer) replaces the phonon propagator when the superconducting properties are calculated.180 It is of the form K(qz , ων ) = g

2 ωex (ωE (qz ))2 + ων2

(5.17)

where g denotes the coupling constant between conduction electrons and magnetic excitons. Their interaction Hamiltonian Hc−f can be written in a pseudospin notation by introducing for the two levels |3 i and |4 i of a U site i the + 1 pseudospin τ i , so that τiz |3(4) i = (−) 2 |3(4) i . Then we may write

Hc−f = I σiz τix (5.18) i

where σi refers to the itinerant 5f electron. The two coupling constants g and I are related through

I 2 1 p02 1 (5.19) g= 4 c 2π ωex where p0 is the radius of the circle in the px , py plane which contains the same area as the hexagon defining the Brillouin zone. We are now in the position to write down and solve Eliashberg’s equations for the conduction electron self-energy (pz , ωn ) and order parameter (pz , ωn ). (pz , ωn ) =

dp⊥ T

K(pz − pz ; ωn − ωm ) G(p⊥ , pz , ωm ) Nz (2π)2 pz ,m

(pz , ωn ) = −

T

K(pz − pz ; ωn − ωm )(pz , ωm ) Nz

×

pz ,m

dp⊥ G(p , p , ωm )2 ⊥ z 2 (2π)

180 P. McHale, P. Fulde, and P. Thalmeier, Phys. Rev. B 70, 014513 (2004).

(5.20)

64

P. FULDE ET AL.

where Nz is the number of lattice sites along the z-axis and ωn = 2πT (n + 1/2). It has been assumed that the order parameter has even parity (singlet channel). The electron Green function has the usual form G−1 (p, ωn ) = iωn − p − (pz , ωn )

(5.21)

with p given by Eq. (5.12). integration in Eq. (5.20) has been done the equations reduce After the dp⊥ to a one-dimensional problem. Thereby it is essential that the kernel K(qz , ων ) is strongly peaked at qz = π/c and ων = 0. Therefore, loosely speaking the gap equation is of the form

π (pz , πT ) = −C(pz ) pz − , πT (5.22) c where C(pz ) is a smooth positive function. This suggests the form (p) = cos(cpz )

(5.23)

with A1g symmetry. The symmetry allows also for a multiplication of the righthand side by a fully symmetric function f (px , py ). The order parameter has lines of nodes at the AF zone boundary pz = ±Qz /2 = ±π/(2c). One finds that Eliashberg’s equations yield also an odd-parity solution of the form (pz ) = sin(cpz )

(5.24)

|χ = (2)−1/2 (|↑ ↓ + |↓ ↑)

with a spin part and the same Tc . Note that because of the Ising-like interaction (5.18) rotational symmetry in spin space is broken. A more general study of possible order parameters due to pair potentials based on magnetic excitons was undertaken in Ref. [179]. It turned out that in the weak coupling limit, i.e., without taking retardations into account, one of the odd-parity triplet states has lower energy than the singlet one. However this could be a consequence of the weak coupling assumption which does not apply to UPd2 Al3 . There is strong experimental evidence discussed below that the order parameter has indeed A1g symmetry (see Eq. (5.23)) and therefore we discard the A1u solution (5.24). In the following we discuss the parameters which are required within this simplified model to explain the anisotropic effective mass and the ones which are needed to explain the observed Tc . For the DOS at the Fermi energy a value of N (EF ) 2 states/(eV-cell-spin) seems appropriate. This includes also the torus. The local intra-atomic excitations responsible for the mass enhancement are characterized by δ 7 meV33 and ωex 5 meV.180 With these values it turns out that a value of I 2 N (EF ) = 0.026 eV

(5.25)

STRONGLY CORRELATED ELECTRONS

65

F IG . V.5. Left panel: The dependence of the superconducting Tc on the electron-magnetic exciton coupling constant g (Eq. 5.19). Parameter values are ωex = 0.01⊥ , α = −0.1, β = 0.8. The full curve corresponds to opposite spin pairing states |χ (Sz = 0) A1g and A1u with gap functions given in Eqs. (5.23), (5.24) and node lines at kz = ± πc and kz = 0 respectively. The dashed curve is a less favorable state with |Sz | = 1 and more node lines. For a value g/⊥ ∼ 2 which leads to the observed mass enhancement m∗ /mb 10 one obtains a calculated Tc 2.9 K (from the full curve). This value is somewhat larger than the experimental Tc = 1.8 K. (After Ref. [180].)

corresponding to g/⊥ = 2 is required in order to reproduce the experimentally observed mass enhancement within the simplified scheme applied to Eliashberg’s equations. With this value a superconducting transition temperature Tc = 2.9 K is obtained while the true value is 1.8 K. The dependence of the superconducting Tc on the dimensionless coupling strength g/⊥ is shown in Figure V.4. Taking into account that the strong mass anisotropies were derived theoretically without adjustable parameters (see Table V.1) it is gratifying to find that when the parameter I 2 N (EF ) (or g/⊥ ) of a simplified model is adjusted so as to reproduce the mass anisotropies, a superconducting transition temperature of the right order of magnitude is obtained. As regards the experimental situation the superconducting state of UPd2 Al3 has been studied in great details for which we refer to the review Ref. [54]. Here we point out merely those experiments which allow for a determination of the symmetry of the order parameter. This applies in particular to the studies of the anisotropic thermal conductivity in an applied magnetic field. As pointed out in Ref. [181] measurements of the thermal conductivity under rotating magnetic field with heat current perpendicular to the rotation plane yield information on 181 K. I. T. Watanabe, Y. Kasahara, Y. Haga, Y. Onuki, P. Thalmeier, K. Maki, and Y. Matsuda, Phys.

Rev. B 70, 184502 (2004).

66

P. FULDE ET AL.

the k-space position of gap nodes. Corresponding measurements on single crystals of UPd2 Al3 181 and their analysis182 have indeed shown that (p) has node lines perpendicular to the c-axis. However these experiments cannot distinguish π at the AF zone boundary or at pz = 0 at the zone between a node line at pz = ± 2c center, i.e., which one of the theoretically favored gap functions of Eq. (5.23) or Eq. (5.24) is realized. Other evidence for node lines was pointed out by Bernhoeft.178 He argued that the symmetry property (p ± Q) = −(p) is required in order to explain the large intensity of a low energy quasiparticle-like peak in the inelastic neutron scattering spectrum below Tc . This again implies a line of nodes perpendicular to the c axis but cannot distinguish between the two candidates. However already before these results became available a pronounced Knight shift reduction below Tc was found in UPd2 Al3 .183 A naive interpretation of this result advocates for the even parity A1g gap function in Eq. (5.23) whose antisymmetric spin function corresponds to the spin singlet state in models with isotropic pairing interaction. In concluding this section we want to summarize the above findings. It has been shown that in UPd2 Al3 superconductivity is due to non-phononic bosons. Intraatomic excitations of localized 5f electrons in U ions, a consequence of strong correlations and described within the dual model provide the glue for the Cooper pairs. We want to stress that their interaction with the itinerant 5f electrons (see Eq. (5.18)) is not time-reversal invariant. Nevertheless Cooper pairs may form but a sign change of the order parameter along the c-direction is mandatory. Otherwise the interaction would not be pair forming but rather act as a pair breaker. It is likely that a similar pairing mechanism, mediated by the exchange of quadrupolar excitons, is operative in the Pr-skutterudite cage compound. VI. Charge Ordering

The concept of charge order in electronic systems was introduced by Wigner in the early 1930s.9 He considered a homogeneous electron gas, i.e., a system in which the positively charged background is distributed uniformly over the sample. Wigner showed that in the limit of low densities the Coulombic repulsion energy between the electrons will always dominate their gain in kinetic energy due to delocalization. Therefore at sufficiently low temperatures electrons will form a lattice. This way they minimize their mutual repulsions. Following the original proposal of Wigner a number of systems have been discovered which show electronic charge order. The cleanest realization of Wigner 182 P. Thalmeier, T. Watanabe, K. Izawa, and Y. Matsuda, Phys. Rev. B 024539, 72 (2005). 183 Y. Kitaoka, H. Tou, K. Ishida, N. Kimura, Y. Onuki, E. Yamamoto, Y. Haga, and K. Maezawa,

Physica B 281–282, 178 (2000).

STRONGLY CORRELATED ELECTRONS

67

crystallization is observed in a classical 2D sheet of electrons generated on a liquid-He surface where the electron density can be varied by an applied electrical field.184 In constrained geometries like quantum dots clear signatures of Wigner crystallization may be found already for small electron numbers.185 The most common systems which exhibit this type of electronic charge order have an underlying atomic lattice as an important ingredient in distinction to Wigner’s homogeneous positive background. When valence electrons are situated close to an atomic nucleus the overlap with orbitals from neighboring sites is expected to be small. This implies that the associated kinetic energy gain is small when electrons delocalize. Therefore the mutual repulsions between electrons on neighboring sites will dominate the kinetic energy gain at a higher density than it is the case for a uniformly distributed positive background. But a resulting electronic charge order must here be commensurate with the underlying atomic lattice. The 3d-valence electrons of transition metal compounds are most amenable to this kind of charge order. The latter may occur within a metallic (or at least conducting) state as in the prominent example of magnetite Fe3 O4 or within an already insulating state as in α -NaV2 O5 . Since the number of d-electrons in 3dcompounds may commonly be changed by doping, a large variety of commensurate 3d-charge ordered states can be achieved, for example in the cuprate (parent compound LaCu2 O4 ) and single layer and bilayer manganite families (parent compound LaMnO3 and half-doped compound LaSr2 Mn2 O7 , respectively). The amplitude of the total charge order parameter or charge disproportionation on the inequivalent 3d-sites is typically small of the order 0.1 electron per site or less. This is due to the screening of the large 3d-orbital occupation changes by the valence electrons of ligands, as can be clearly seen from LSDA+U calculations. Experimentally the amount of charge disproportionation is extremely difficult to determine. This is mostly done via the empirical valence-bond analysis of X-ray results in the ordered phase, where the change in bond distances is linked to the valence charge disproportionation. In some 3d-oxide compounds like, e.g., the bilayer-manganites one must be aware that 3d-charges are dressed by strong distortions of the surrounding lattice leading to (small) polaron formation. It is then the latter which exhibit the ordering transition. Charge ordering is less common in 4f -compounds, because the intersite Coulomb interaction necessary for charge order is well screened and in genuine metallic compounds the hybridization with conduction electrons tends to favor a site-independent 4f -occupation. This leads to a metallic mixed-valent or heavy fermion state. There is however an important case where 4f -charge order may occur. In insulating or semimetallic 4f compounds which are homogeneous valence fluctuators at high temperatures, the intersite Coulomb interaction may be 184 G. Adams, Phys. Rev. Lett. 42, 795 (1979). 185 A. V. Filinov, M. Bonitz, and Y. E. Lozovik, Phys. Rev. Lett. 17, 3851 (2001).

68

P. FULDE ET AL.

strong enough to lead to a 4f -charge disproportionation, i.e., an inhomogeneous mixed-valent state at low temperatures with different 4f -orbital occupations on inequivalent sites. Again the amplitude of the total charge order including the effect of ligand screening charges is much smaller than the bare 4f -charge disproportionation. An important class of compounds where this charge-order (CO) transition occurs are members of the R4 X3 series (R = rare earth Yb, Sm, Eu and X = As, Bi, P, Sb), notably the semimetal Yb4 As3 discussed in Section VI.13. An attractive feature of CO transitions in these 3d or 4f compounds is the possibility of lowering the effective dimension of the arrangement of magnetic ions, for example to a family of 1D chains, planes of zig-zag chains or ladders and stripes. The effect of low dimensionality has then important consequences for the spin excitation spectrum, e.g., the appearance of a two-spinon continuum in the case of spin chains. When this type of electronic charge order in 3d and 4f systems is compared with the original suggestion of Wigner one notices two differences. As pointed out before, the lattice structure of the positive background is very important but also the repulsions between electrons on neighboring sites are not purely Coulombic. Instead they may be modified due to the electrons in inner closed shells which leads to strongly screened Coulomb interactions that usually extend only to nearest and next nearest neighbors. Another type of charge ordering which does not break spatial symmetries is obtained in systems which can be described by a Hubbard Hamiltonian at half filling. Here it is the on-site Coulomb interaction expressed by an energy U which is competing with electron hopping processes and the associated energy gain. While the repulsion energy U favors single occupancy of sites, and suppresses double occupancies the kinetic energy gain favors a sizeable fraction of sites with double occupations. Without electron correlations 25% of them would be doubly occupied in order to optimize the kinetic energy. For sufficiently large values of U charge order in the form of strongly suppressed on-site charge fluctuations will take place leading to a Mott–Hubbard metal to insulator (M-I) transition. Again, similarities to the previously considered cases are obvious but so are the differences. Repulsions between electrons on different sites are completely neglected in the Hubbard model and it is crucial to have precisely one electron per site in order to obtain charge order. A similar requirement does not exist in the previously considered cases. Finally, charge order can also occur via formation of a charge density wave (CDW) in metals. In this case the instability is driven by minimizing the kinetic (band) energy of conduction electrons leading to a reconstruction of the Fermi surface. A prerequisite is the presence of nesting properties in the Fermi surface. The generally incommensurate vector Q which connects the nesting parts determines wavelength and direction of a corresponding CDW. Note that strong elec-

STRONGLY CORRELATED ELECTRONS

69

tron correlations are not required for a CDW to form. Summarizing we distinguish between the following electronic charge ordering processes: (a) (b) (c) (d) (e)

Wigner crystallization in the homogeneous electron gas or liquid Charge order due to weak hybridizations and strong intersite interactions Mott–Hubbard charge order due to strong on-site interaction Charge density waves due to nesting properties of the Fermi surface Charge ordering in polaronic systems

In this overview we will not address the genuine Mott–Hubbard M-I transition which is reviewed in existing articles, e.g., Ref. [186]. It demands a considerable technical effort based on the recently developed dynamical mean field theory (DMFT). Low dimensional metallic CDW systems will also not be included, since this topic is well represented in the literature187 and should be discussed together with spin-density waves and superconductivity which is beyond the scope of this chapter. 12. W IGNER C RYSTALLIZATION IN H OMOGENEOUS 2D E LECTRON S YSTEMS The electron gas may be subject to many different instabilities depending both on the background (lattice) potential and the resulting shape of the Fermi surface as well as the strength and range of the screened Coulomb interactions. A convenient way to characterize the relevant regime is the Brueckner parame− 13 ter rs = a10 ( 4π which is the ratio of average electron distance to the Bohr 3 n) radius a0 (n = electron density). In the two limits of small and large rs the electron system exhibits radically different behavior. At large density (small rs ) the system is in a metallic state dominated by the kinetic (Fermi) energy and the Coulomb interactions between electrons are well screened. If the Fermi surface has parallel (quasi-1D) sections, ‘nested’ by a wave vector Q, the residual Coulomb interactions may lead to a condensation of electron–hole (Peierls) pairs into a charge- or spin-density wave state with translational and possibly other symmetries broken. Part or all of the nested Fermi surface sheets are then removed by the self-consistent potential in the condensed state. For a conventional density wave spontaneous modulation of the charge- or spin density with period 2π/Q takes place which may be identified by common methods like X-ray or neutron diffraction. Since real metallic materials have high densities and small or moderate rs this type of instability is frequently encountered. It often competes or coexists with an alternative condensation mechanism, 186 A. Georges, G. Kotliar, W. Krauth, and M. J. Rosenberg, Rev. Mod. Phys. 68, 13 (1996). 187 G. Grüner, Density Waves in Solids, Addison-Wesley (1994).

70

P. FULDE ET AL.

namely electron–electron (Cooper) pair formation leading to a superconducting state. In the opposite limit of small density and large rs the long range Coulomb interaction is badly screened and it dominates the small kinetic energy gain due to delocalizations. At low enough temperatures the electron liquid condenses in real space, forming a Wigner solid9 which also breaks translational symmetry. This is complementary to condensation in the k-space as found in the previous density wave case. For a two dimensional (2D) homogeneous electron liquid in a uniform positive background the appropriate Hamiltonian H = T + V is

1

† † † (k)ckσ ckσ + vq cp+qσ ck−qσ (6.1) H= ckσ cpσ 2 kσ

pkq;σ σ

2

where (k) = k2 /2m is the kinetic energy and vq = 4πe (1 − δq0 ) is the Coulomb q2 interaction. The Kronecker delta δq0 ensures that due to the positive background vq = 0. Furthermore is the volume. For practical calculations on a lattice and for finite systems the Ewald summation technique has to be used to obtain the real space Coulomb potential V (r). The qualitative shape of the n–T phase boundary for the liquid-solid transition has been given in Ref. [188]. It is derived from the intuitive notion that at the phase transition the average potential and kinetic energies of electrons should be comparable, i.e., V /T ≡ 0 . This leads to a parametrically (z = exp(−βμ)) determined n–T phase boundary (μ = chemical potential) shown in Figure VI.1. In 2 √πn. Then the classical limit (kT μ) one has T = kT , furthermore V = e √ the melting curve is simply given by n(T ) = (kT 0 / π e2 )2 with an unknown parameter 0 . In a homogeneous background the 2D electron liquid solidifies in a trigonal (hexagonal) lattice structure.189 In the static approximation without ki−1/2 which is lower netic energy the ground-state energy is EGS = −3.921034e2 ac √ than for any other of the five 2D Bravais lattices. (Here ac = ( 3/2)a02 is the hexagonal cell area with a0 denoting the lattice constant, the density is n = 1/ac .) This result is simple to understand because of all 2D lattices the trigonal one has the largest lattice spacing for a given density and therefore minimizes the total energy if the latter is dominated by the Coulomb repulsion as in the small density regime. Stability analysis shows that the trigonal lattice is stable under longitudinal and transverse (shear) distortions and the corresponding two phonon branches have real frequencies. In the long wavelength limit they are isotropic, i.e., they depend only on q = (qx2 + qy2 )−1/2 and are given by ω1 (q) = ωp (a0 q)1/2 and ω2 (q) = 0.19ωp a0 q for longitudinal and transverse modes respectively. Here 188 P. M. Platzmann and H. Fukuyama, Phys. Rev. B 10, 3150 (1974). 189 L. Bonsall and A. A. Maradudin, Phys. Rev. B 15, 1959 (1977).

STRONGLY CORRELATED ELECTRONS

71

F IG . VI.1. Schematic Fermi liquid–Wigner solid phase diagram of the 2D electron system. Estimates of critical density and temperature are given by nc = (4/πa02 )(1/ 02 ) and Tc = (2e4 m/ 02 ). (After Ref. [188].) 2

−1 is the 3D plasma frequency of a slab of thickness 2a. While ωp = 4πe m∗ (2ac a0 ) the Wigner lattice structure and stability is well understood, the melting into the liquid state, both classical melting (as function of T ) and quantum melting at T = 0 (as function of the control parameter rs ) is much less clear. The situation sketched in Figure VI.1 is certainly oversimplified in one aspect: In both cases presumably an intermediate phase between Wigner solid and Fermi liquid appears which is characterized by the loss of long range translational order but preserves quasi-long range orientational order. In the case of classical melting of 2D trigonal lattices this intermediate phase is known as the ‘hexatic phase’.190 In the case of quantum melting (at T = 0) as function of density (rs ) a similar precursor phase to the liquid seems to appear. This can only be investigated by numerical techniques like Quantum Monte Carlo (QMC) simulations. It was known from earlier QMC results191 that for rs > 37 ± 5 the Fermi liquid state becomes instable. A more recent investigation of phases as function of rs was undertaken in Ref. [192] with a fixed-node QMC approach. A variational trial or guiding wave function for the ground state of H (Eq. (6.1)) on a grid (Lx , Ly ) was used. It has the following 190 B. I. Halperin and D. R. Nelson, Phys. Rev. Lett. 41, 121 (1978). 191 B. Tanatar and D. M. Ceperley, Phys. Rev. B 39, 5005 (1989). 192 H. Falakshahi and X. Waintal, Phys. Rev. Lett. 94, 046801 (2005).

72

form

P. FULDE ET AL.

J |ri − rj | . (r1 , r2 , . . . rN ) = Det φi (rj )

(6.2)

i<j

The single particle wave functions φi (rj ) in the Slater determinant Det[φi (rj )] are taken as plane waves in the liquid state and localized Gaussian orbitals on trigonal sites in the Wigner lattice case. The Jastrow function J (|ri − rj |) describes correlations and consists of modified Yukawa functions. It takes the Coulomb correlations into account by keeping the electrons apart. √ The range of correlations scales with the average electron distance d = 1/ πn where n = N/Lx Ly denotes the density. With this trial wave function one would obtain indeed the instability of the liquid state at rs∗ 40 since for rs > rs∗ its energy exceeds that of the Wigner solid (see Figure VI.2). However, the latter with its localized wave functions is still not the most stable state in that range of rs . This may be seen if one uses instead trigonal lattice Bloch states for the single particle functions φi (rj ) but with k constrained to the first BZ. This implies an orientational symmetry breaking in k space, i.e., a trigonally shaped Fermi surface. But the static density correlation function has still no fully developed Bragg peaks like in the crystal in analogy to the classical melting scenario. This intermediate or hybrid state has indeed a lower energy than the Wigner solid in the range rs∗ < r < rs∗∗ with rs∗ 30 and rs∗∗ 80. For still higher values of rs the Wigner solid with fully

F IG . VI.2. Energy differences in units of 2π N nt (t = hopping energy, n = N/Lx Ly = average density) of liquid and intermediate (or hybrid) phases with respect to the Wigner crystal phase. Here Eliquid –Ecrystal (circles) and Ehybrid –Ecrystal (triangles) are plotted as function of rs for N = 72 electrons on a Lx = 48 × Ly = 84 grid. Critical values are rs∗ ∼ 30 and rs∗∗ ∼ 80. Inset: density–density correlation function with reference particle in the center. (After Ref. [192].)

STRONGLY CORRELATED ELECTRONS

73

localized functions φi (rj ) finally becomes stable. There is no symmetry change involved in going from the intermediate to the Wigner solid state. Therefore it is not clear whether there is a real quantum phase transition at rs∗∗ , as there is at rs∗ , or simply a crossover to more pronounced density correlations (see inset of Figure VI.2). The picture of the intermediate phase is also supported by QMC calculations for mesoscopic 2D electron systems in a harmonic trap. There a similar two-step transition is found from liquid to orientational and finally to fully developed lattice correlations.185 Finally we note that at even larger values of rs the Wigner lattice becomes spin-polarized due to a ferromagnetic ring exchange in the trigonal lattice.193 The experimental realization of the genuine Wigner lattice formation in the 2D electron liquid has been attempted along two alternative approaches. The more successful route is the accumulation of electrons in a monolayer on the surface of liquids such as helium. The accumulation is achieved by applying an electrical pressing field perpendicular to the surface. Its strength allows to vary the electron density in the monolayer over several orders of magnitude. The lower part of the classical melting curve in Figure VI.1 has been determined in Ref. [184] by a rfresonance method. For the ratio of potential to kinetic energy at the phase boundary a surprisingly large value of 0 ∼ 137 was found in agreement with early MC simulations. Due to a finite surface tension the pressing field deforms the liquid surface around the electrons thereby leading to single electron ‘dimples’. This induces an effective attraction between electrons which has to be added to the Coulomb repulsion. It has been proposed that this attraction may lead to a structural phase transition of the Wigner lattice from trigonal to square lattice for sufficiently low density and high pressing fields.194 The second route to generate 2D electron systems are semiconductor heterojunctions. It has been much less conclusive because the evidence for Wigner lattice formation in transport properties is obscured by the 2D localization effects caused by impurities.195 Computational results presented before show that the genuine Wigner lattice formation takes place at rs values which are more than an order of magnitude larger than those found in real solids. But in real crystals with inhomogeneous electron densities the condition for a Wigner type of lattice formation may be much easier to fulfill. In case that the overlap of atomic wavefunctions of neighboring atoms is small the gain in kinetic energy due to electron delocalization is also small. The mutual Coulomb repulsion of electrons on neighboring sites can become more easily dominant in that case than in a homogeneous electron gas. 193 D. M. Ceperley, The Electron Liquid Paradigm in Condensed Matter Physics, IOS Press, Amsterdam (2004), p. 3. 194 M. Haque, I. Paul, and S. Pankov, Phys. Rev. B 68, 045427 (2003). 195 E. Abrahams, Rev. Mod. Phys. 73, 251 (2001).

74

P. FULDE ET AL.

Neighboring rare earth ions have a particularly small overlap of their 4f wavefunctions. Therefore they are particularly good candidates for the formation of charge ordered Wigner like lattices196 as will be discussed in the next section. Furthermore in 3d/4f compounds the Coulomb interactions are strongly screened whereas in the two-step classical and quantum melting of a 2D Wigner lattice the long range part of the Coulomb interactions is most important. Indeed, charge ordering in compounds usually takes place at a well defined temperature and is mostly of first order. It is driven by a competition between short range next and next nearest neighbor Coulomb interactions and the kinetic energy. Also some compounds are already in a Mott–Hubbard insulating state due to large on-site Coulomb repulsion before charge order caused by the inter-site Coulomb interactions appears. Therefore, for real compounds like vanadates and manganites the extended Hubbard type models are a better starting point than the Hamiltonian in Eq. (6.1) to describe the multitude of charge ordering phenomena in solids. Nevertheless, loosely speaking one may refer to them as a kind of generalized Wigner lattice formation.196 13. G ENERALIZED W IGNER L ATTICE : Y B 4 A S 3 The intermetallic compound Yb4 As3 is a perfect example of a system in which charge order takes place, here of 4f holes. Yb4 As3 has a cubic anti-Th3 P4 struc¯ ture with a I 43d space group. Due to the special lattice structure charge order in this three-dimensional system results in the formation of well separated chains of Yb3+ ions. They act like one-dimensional spin chains. The net result is that Yb4 As3 shows all the signs of a low-carrier-density heavy fermion system which here is due to the properties of the spin chains. This is a good example for the formation of heavy quasiparticles caused by electronic charge order. The Kondo effect plays no role in this compound. We start out by summarizing some experimental facts and results. Yb4 As3 and other family members of R4 X3 were first systematically investigated by Ochiai et al.43 A compilation of more recent results may be found in Ref. [197]. By counting valence electrons one notices that since As has a valency of −3, three of the Yb ions must have a valency of +2 while one ion has a valency of +3, i.e., one expects Yb4 As3 → (Yb2+ )3 (Yb3+ )(As3− )3 . But Yb2+ has a filled 4f shell. Thus there is one 4f hole per formula unit. The Yb ions occupy four families of 196 P. Fulde, Ann. Phys. (Leipzig) 6, 178 (1997). 197 B. Schmidt, H. Aoki, T. Cichorek, J. Custers, P. Gegenwart, M. Kohgi, M. Lang, C. Langhammer,

A. Ochiai, S. Paschen, et al., Physica B 300, 121 (2001).

STRONGLY CORRELATED ELECTRONS

75

F IG . VI.3. Left panel: Anti-Th3 P4 structure of Yb4 As3 . Large and small spheres symbolize Yb and As ions, respectively. The Yb ions are residing on four interpenetrating families of chains oriented along cubic space diagonals. Right panel: Dense rod packing representation of the Yb-chains. In the CO structure only one family of chains carries Yb3+ ions with pseudo-spin S = 1/2 whereas the other three families are occupied with S = 0 Yb2+ ions. (After Ref. [197].)

interpenetrating chains which are pointing along the diagonals of a cube (see Figure VI.3). This is often referred to as body-centered cubic rod packing.198 It is important to notice that the distance between two neighboring Yb ions along a chain is larger than the distance between ions belonging to different chains. This implies that nearest neighbor Yb ions belong to different families of chains. At sufficiently high temperatures, i.e., above 300 K the 4f holes move freely between sites and the system is metallic. Measurements of the Hall coefficient RH confirm that the carrier concentration is approximately one hole per unit cell in that temperature range. The situation is different at low temperatures where the measured Hall coefficient has a value of RH = 7 · 1018 cm−3 implying approximately one hole per 103 Yb ions (see Figure VI.4). Thus the system changes from a metal to a semimetal as the temperature decreases. This is particularly seen in measurements of the resistivity ρ(T ) (see Figure VI.4). While for T > 300 K a linear temperature dependence is observed, one notices that near Tc 292 K a first-order phase transition is taking place with a corresponding increase in resistivity. At low temperatures ρ(T ) = ρ0 + AT 2 is found, i.e., the semimetal is a Fermi liquid. Despite the low carrier concentration of order n 10−4 per cell obtained from the Hall constant, Yb4 As3 shows all the signs of a heavy-quasiparticle system at low temper198 Y. M. Li, N. d’Ambrumenil, and P. Fulde, Phys. Rev. Lett. 78, 3386 (1997).

76

P. FULDE ET AL.

F IG . VI.4. Left panel: Hall coefficient RH (T ) for Yb4 As3 . The inset shows the change at the phase transition temperature Tc . Right panel: resistivity ρ(T ). At Tc = 295 K a phase transition due to charge ordering is taking place. Solid line: extrapolation of ρ(T ) ∼ T . (After Ref. [43].)

atures. The γ -coefficient of the specific heat is γ 200 mJ/(mol K2 ), the Sommerfeld–Wilson ratio is RW = 4π 2 kB2 /3(gμB )2 (χ/γ ) 1 implying an equally enhanced spin susceptibility and the Kadowaki–Woods ratio A/γ 2 is similar to that of other heavy quasiparticle systems. If one were to postulate an origin of the heavy mass within the Kondo lattice mechanism, this may seem very strange in view of the fact that this semimetal has a very low density of charge carries. The phase transition at Tc 300 K is accompanied by a trigonal distortion and a change of the space group to R3c. This structural transition is volume conserving and is triggered by charge order of the 4f holes. The angle between orthogonal axes in the cubic phase changes to α = 90.8◦ in the trigonal phase for T Tc (Figure VI.5). Associated with this change is a spontaneous elastic strain below Tc which is proportional to the charge order parameter. The structural instability is accompanied by a softening of the c44 elastic mode above Tc .199 This suggests that the trigonal elastic strain yz , zx , xy with 5 symmetry plays a crucial role. The temperature dependence of the c44 mode may be obtained from a Ginzburg–Landau expansion of the free energy in terms of the strains and the charge ordering parameter components (Qyz , Qzx , Qxy ).199 The latter are defined by expanding the charge ρ = ρ0 + ρ in the form ρ = Qyz ρyz (5 ) + Qzx ρzx (5 ) + Qxy ρxy (5 ).

(6.3)

Here ρ0 is the part of the charge distribution which remains unchanged by the phase transition while ρij (5 ) are the charge fluctuation modes of 5 symmetry. 199 T. Goto, Y. Nemoto, and A. Ochiai, Phys. Rev. B 59, 269 (1999).

STRONGLY CORRELATED ELECTRONS

77

F IG . VI.5. Upper panel: Unit cell angle α = 90◦ + δ (open symbols) as function of T showing first order trigonal distortion at the CO transition temperature Tc 288 K together with linear thermal expansion a/a (full symbols). After Ref. [200]. Lower panel: temperature dependence of the elastic constant c44 (T ). Above the structural phase transition temperature Tc a strong softening is observed described by Eq. (6.6) and caused by coupling to the 5 type charge order parameter. Due to the first-order nature of the transition the theoretical mean-field transition temperature Tc0 = 247 K is smaller than the actual Tc . (After Ref. [199].)

It is Qij = 0 for T > Tc and Qij = 0 for T < Tc . Up to a constant the free energy contains three different contributions. One (FQ ) is due to the order parameter, a second one (Fel ) is due to the elastic energy of the lattice and the third one (FQ-el ) describes the interactions of the order parameter with the lattice. For the 200 K. Iwasa, M. Kohgi, N. Nakajima, R. Yoshitake, Y. Hisazaki, H. Osumi, K. Tajima, N. Wakabayashi, Y. Haga, A. Ochiai, et al., J. Mag. Mag. Mat. 177–181, 393 (1998).

78

P. FULDE ET AL.

c44 elastic constant we obtain201 α FQ = F0 + Q2xy + Q2xz + Q2yz 2

β 3 2 4 4 4 2 2 2 Qxy + Qxz + Qyz − Qxy + Qxz + Qyz + 4 5 Fel =

0 c44 2 2 2 xy + xz + yz 4

FQ-el = −g(Qxy xy + Qxz xz + Qyz yz ).

(6.4)

Near a phase transition α = α0 (T − ) changes sign at a characteristic temperature . The fourth-order terms in Qij stabilize the ordered state of the system. For T > the softening of the elastic constant is obtained by neglecting the terms ∼ Q4ij in the free energy and minimizing F = FQ + Fel + FQ-el by setting ∂F /∂Qij = 0. For β > 0 this leads to a trigonal charge order parameter Qt = √1 (Qxy , Qxz , Qyz ). It also leads to a proportionality between Qij and the 3 strain ij which may be used to rewrite the free energy in the form

2 1 0 g2 2 2 c − xy + xz . (6.5) + yz F = F0 + 2 44 α0 (T − ) Therefore the renormalized elastic constant is

T − Tc0 g2 0 where Tc0 = + c44 = c44 0 T − α0 c44

(6.6)

denotes the theoretical mean-field transition temperature in the presence of the strain interaction. The explanation of a first-order phase transition at Tc > Tc0 requires the inclusion of higher order terms in Qij in (6.4). A detailed grouptheoretical analysis of different measured elastic constants is found in Ref. [199]. At temperatures T > Tc the 4f holes are equally distributed over the chains. But at low temperatures the system avoids nearest-neighbor Yb3+ –Yb3+ sites in order to minimize the mutual short-range inter-site repulsion of 4f holes. This is accomplished by an accumulation of 4f holes in one family of chains, i.e., by charge order. This way nearest-neighbor repulsions of 4f holes are reduced. In the idealized case one expects that for T → 0 one family of chains consists of Yb3+ sites while in the three remaining families of chains all sites are in a Yb2+ configuration. This explains the trigonal distortion (Figure VI.5) which is accompanying charge ordering of the 4f holes. Since Yb3+ ions have a smaller ionic radius than Yb2+ ions the sample is shrinking in the direction of the chains containing the Yb3+ ion. In order to keep the volume of the unit cell constant (other201 T. Goto and B. Lüthi, Adv. Phys. 52, 67 (2003).

STRONGLY CORRELATED ELECTRONS

79

wise a too large amount of elastic energy would be necessary) the remaining three families of chains must expand correspondingly. It was first pointed out in Ref. [31] that the origin of the heavy quasiparticles are spin excitations (spinons) in the chains of Yb3+ ions and that it is not due to the Kondo effect as previously thought. This physical model was beautifully confirmed by inelastic neutron scattering experiments (INS).32,202 They demonstrated that the magnetic excitations are those of an isotropic antiferromagnetic Heisenberg chain. They agree with the spectrum of two-spinon excitations lying within the lower and upper boundaries ωL (q) and ωU (q) respectively, given by

π 1 (6.7) ωL (q) = J sin(q) and ωU (q) = πJ sin q 2 2 with q measured in units of inverse lattice constants d −1 . The lower boundary ωL (q) was calculated long before by des Cloizeaux and Pearson203 (see Figure VI.6). Note that unlike in the classical spin chain there is no sharp spin wave excitation for a given momentum q but instead a two-spinon continuum. Its corresponding dynamic spin-structure factor (Figure VI.6) is proportional to the INS

F IG . VI.6. Spectral function S(q, ω) of the two-spinon excitation spectrum of a Heisenberg chain in the q, ω-plane. It is nonzero in the shaded region above the lower bound ωL (q) calculated by Ref. [203] and the below the upper bound ωU (q) given by Eq. (6.8). S(q, ω) diverges at ωL (q) approximately with a root singularity. The step-like cutoff at ωU (q) is an artefact of the approximate form in Eq. (6.8). The lattice constant is set equal to unity. (After Ref. [204].) 202 M. Kohgi, K. Iwasa, J.-M. Mignot, N. Pyka, A. Ochiai, H. Aoki, and T. Suzuki, Physica B 259– 261, 269 (1999). 203 J. des Cloizeaux and J. J. Pearson, Phys. Rev. 128, 2131 (1962). 204 M. Karbach, G. Müller, and A. H. Bougourzi, Phys. Rev. B 55, 12510 (1997).

80

P. FULDE ET AL.

cross-section and may be approximated by204 S(q, ω) =

(ω − ωL (q))(ωU (q) − ω) . 2 (q) ω 2 − ωL

(6.8)

This spectrum diverges at the lower boundary with a square root singularity and therefore has a very asymmetric appearance as function of energy transfer ω (see Figure VI.6). The total integrated intensity, i.e., the frequency integral of S(q, ω) is linear in q for q π and diverges like [− ln(1 − q/π)]α for q → π , where α = 1 for the approximation in Eq. (6.8) and α = 3/2 is the exact result. Therefore the two-spinon continuum should appear in INS as a spectrum strongly peaked at ωL (q) with an asymmetric tail reaching up to ωU (q) and a strongly increasing total intensity for q → π . This is precisely what has been found in the INS experiments of Kohgi et al. (see Figure VI.7) and constitutes a proof for the 1D character of spin excitations in Yb4 As3 . That the interacting crystal field ground-state doublets of Yb3+ behave like an isotropic Heisenberg system is not immediately obvious. It was shown

F IG . VI.7. Left panel: Experimental S(q, ω) from INS202 for momenta q = 1 and 0.8 (here q is given in units of π/d where d is the Yb distance in the chain). The asymmetric shape of the two-spinon spectrum in Figure VI.6 is clearly observed. For q < 1 the resolution limited peak position corresponds to the lower boundary ωL (q) of the spinon spectrum. Right panel: Dispersion of ωL (q) from INS experiments for different directions of the momentum transfer. Here q is the projection of momenta on the 111 chain direction. All data points fall on the dashed curve which is the theoretical ωL (q) = π2 J sin dq with J /kB = 25 K. In addition to the asymmetric shape of S(q, ω) this proves the 1D character of magnetic excitations in Yb4 As3 . (After Ref. [32,202].)

STRONGLY CORRELATED ELECTRONS

81

independently in Refs. [205] and [206]. Thereby the local symmetry of the crystalline electric field was properly accounted for. Spin fluctuations of Heisenberg chains can explain the observed heavy quasiparticle excitations as they appear in the specific heat C = γ T and spin susceptibility χS . They are given by γ=

2 kB R 3 J

and χS =

4μ2eff R (π 2 J )

(6.9)

(see Ref. [207]). Here J is the AF coupling constant of nearest-neighbor sites in the effective S = 12 spin chain described by the 1D Heisenberg Hamiltonian

H =J Si Sj . (6.10) ij

Furthermore, R is the gas constant and μeff is the effective magnetic moment of a Yb3+ site. Therefore one finds RW = 2 for the Sommerfeld–Wilson ratio. When the experimental value of J /kB = 25 K (from Figure VI.7) is used in (6.9) the observed size of the γ coefficient is well reproduced. Having described the underlying physics we discuss a model description for the compound. For that purpose we neglect the electron hopping terms between different chains as it was done, e.g., in the Labbé–Friedel model for A-15 compounds like V3 Si or Nb3 Sn.208 There one is dealing with three families of intersecting chains while here we have four types of chains. The effective 4f -model Hamiltonian31 is then written as

+ fiμσ fj μσ + h.c. + U niμ↑ niμ↓ H = −t μ ij σ

+

μ

iσ

μ

μ niμσ +

i

N c 2 . 4

(6.11)

The first term describes effective 4f -hole hopping due to hybridization with As 4p ligand states within a chain of a family μ = 1–4 from site i to a nearest neighbor site j . From LDA calculations one can deduce that 4t 0.2 eV. The second + fiμσ term is due to the on-site Coulomb repulsion of 4f holes with niμσ = fiμσ 4+ 12 and ensures that in the large U limit Yb states with 4f configurations are excluded. The third term describes the volume conserving coupling of the f bands 205 G. Uimin, Y. Kudasov, P. Fulde, and A. Ovchinnikov, Eur. Phys. J. B 16, 241 (2000). 206 H. Shiba, K. Ueda, and O. Sakai, J. Phys. Soc. Jpn. 69, 1493 (2000). 207 D. C. Mattis, The Theory of Magnetism, vol. 17 of Springer Series in Solid State Sciences, Springer-Verlag, Berlin (1981), 2nd ed. 208 J. Labbé and J. Friedel, Journ. Phys. (Paris) 27, 153, 303 (1966).

82

P. FULDE ET AL.

to the trigonal strain > 0 with = 5 . It leads to a deformation potential of the form (6.12) μ = (4δμ1 − 1) 3 for 4f holes situated in chains, e.g., in [111] direction denoted by μ = 1. Since the Yb3+ ions are smaller than the Yb2+ ions, the distance between Yb ions shrinks for μ = 1 while it expands in the other chain directions denoted by μ = 2, 3, 4. As previously pointed out the origin of the deformation potential is the Coulomb repulsion between holes on neighboring sites. It is treated here as an effective attraction Veff between holes on nearest-neighbor sites of a chain. The fourth term in (6.11) is the elastic energy in the presence of a trigonal distortion, where N is the number of sites and c is the background elastic constant. A reasonable value is c / = 4 · 1011 erg/cm3 where denotes the volume of a unit cell with a lattice constant of a0 = 8.789 Å. The Hamiltonians for chains μ with an interaction Veff can be written in the form

+ Hμ = −tμ fiμσ fj μσ − Veff (niμ − n)(n ¯ j μ − n) ¯ (6.13) ij σ

ij

where n¯ is the average occupancy of all sites in the system. Within a molecularfield approximation the Hamiltonian reduces to

N + fiμσ fj μσ − 2Veff (n¯ μ − n) (niμ − n) ¯ + Veff (n¯ μ − n) ¯ 2. HμMF = −tμ 4 ij σ

ij

(6.14) We denote the distinct chains with μ = 1 and note that with the correspondence 4 = −2Veff (n¯ 1 − n); ¯ 3

2 9 = Veff c 4

(6.15)

the Hamiltonians (6.14) and (6.11) become the same. This serves as a justification for the band Jahn–Teller type of description chosen above. When a distortion is taking place the hopping matrix elements also depend on μ, according to tμ = t+ δμ1 + t− (1 − δμ1 ) t+ = teλ ,

t− = teλ /3 .

(6.16)

But this μ dependence of t is not essential. The Hamiltonian (6.11) is well suited for describing the lattice distortion caused by charge ordering. The distortion is described here like a collective band Jahn– Teller effect. The four-fold degeneracy of the f bands is lifted by the spontaneous appearance of a trigonal strain which lowers the symmetry. For the purpose of

STRONGLY CORRELATED ELECTRONS

83

F IG . VI.8. Temperature dependence (T ) of the (secondary) strain order parameter. Shown in the inset are the corresponding changes in the population of the different families of chains. Q = n1 − n2 is the primary charge order parameter. (After Ref. [31].)

demonstration we consider first the case of U = 0. This neglects the effects of strong on-site correlations on the band Jahn–Teller effect. Near the charge ordering transition where each of the chains contains nearly 25% of Yb3+ sites this approximation is justified. However, it is no longer acceptable for low temperatures when nearly all of the sites in the μ = 1 chains are Yb3+ . The condition for a collective band Jahn–Teller effect taking place is 2 /(t ) > 3.31 Choosing = 5 eV results in a transition temperature of Tc 250 K which is close to the experimental value of 300 K. This value of corresponds to a Grüneisen parameter of G ≡ /(4t) = 25 which is of a comparable size found in other 4f -mixed valence systems. The symmetry strain as function of reduced temperature T /Tc is shown in Figure VI.8. As a consequence of a finite strain the four degenerate onedimensional f bands split into a lower and three upper bands. Their centers of gravity differ by (4/3)| | with the equilibrium strain given by = −/(2c ) 0.02. The changes in the population of the chains with μ = 1 and μ = 1 with decreasing temperature are shown in the inset of Figure VI.8. The transition is of first order due to the singular DOS of the effective 1D f-bands. Let us reemphasize that those changes are caused by the Coulomb repulsion of holes and drive (T ) and not vice versa. Band refillings by a band Jahn–Teller transition and crystallization of holes are alternative points of view of the respective descriptions here.

84

P. FULDE ET AL.

F IG . VI.9. Yb4 As3 : Site selective values of Yb valence/hole concentration (data points) as obtained from the 303¯ reflection in the vicinity of the Yb L3 X-ray absorption edge. Full line: guide to the eye. Dashed line: model calculation from Ref. [198]. Dotted line: from the angular deviation δ(T )200 in Figure VI.5. (After Ref. [209].)

There have been experiments which directly observed one-dimensional charge order.209 This was achieved, e.g., by resonant X-ray diffraction on the Yb L3 absorption edge. Below Tc forbidden reflections appear in the slightly rhombohedrally distorted cube. From their intensity one can deduce an effective valency for the short and long chains (see Figure VI.9). The discontinuities at the first-order phase transition are even larger than the above model calculation predicts. We return to the Hamiltonian in Eq. (6.11) and consider the effects of a large on-site interaction U in the charge ordered state for T Tc . For this purpose we transform to a t–J Hamiltonian for the chains μ = 1. The exclusion of Yb4+ configurations (2 holes) due to U is taken into account by a projector P which projects onto 0 and 1 hole occupations of sites. To lowest order in t/U we obtain

1 + Si Sj − ni1 nj 1 (6.17) P fi1σ fj 1σ + h.c. P + J Hμ=1 = −t 4 ij σ

ij

+ where J = 4t 2 /U and furthermore Si = αβ fi1α σ αβ fi1β , ni1 = σ ni1σ . For U = 10 eV we find J = 1·10−3 eV. A slight band-narrowing effect due to the 209 U. Staub, B. D. Patterson, C. Schulze-Briese, F. Fauth, M. Shi, L. Soderholm, G. B. M. Vaughan, and A. Ochiai, Europhys. Lett. 53, 72 (2001).

STRONGLY CORRELATED ELECTRONS

85

lattice distortion (see Eq. (6.16)) has been neglected here. The Hamiltonian Hμ=1 can be treated within the slave-boson approximation. Thereby the projector P is replaced by an auxiliary boson bj+ which generates a configuration without a hole, i.e., a Yb2+ site. By treating the boson field in mean-field approximation one obtains an effective mass of the quasiparticles m∗ t = mb tδ + (3/4)χJ

(6.18)

where mb is the bare band mass and χ = ( π2 ) sin( π2 (1 − δ)). Furthermore, δ is the deviation of the chains μ = 1 from half filling. When δ = 0, i.e., for the half-filled case we find (J = 4t 2 /U ) m∗ π U 2π t = = mb 6 t 3 J

(6.19)

which is a large mass enhancement of order 102 . In this case the heavy quasiparticles are spinons as we are dealing with an antiferromagnetic Heisenberg chain. The low temperature thermodynamics is completely determined by these spin degrees of freedom and we have an example of spin-charge separation here. A de Haas–van Alphen experiment should not yield heavy quasiparticle masses here and the Fermi-liquid relation between the γ coefficient and a renormalized mass of (nearly) free electrons is violated. This becomes obvious when Yb4 (As1−x Px )3 (x = 0.3–0.4)210,211 is considered. In distinction to Yb4 As3 this is a charge ordered insulator but it has nevertheless a similar large linear specific heat coefficient γ . The latter is caused by spin excitations in Heisenberg chains as in Yb4 As3 . It is interesting to note that the Hamiltonian (6.11) can be solved exactly by adaptation of Lieb and Wu’s solution of the one-band Hubbard model. The solution is based on the Bethe ansatz. This is possible since the different bands are not coupled directly with each other. One interesting finding is that the increase in the strain order parameter just below Tc is much steeper than in Figure VI.8 and therefore in better agreement with experiments. For more details we refer to the original literature.212 This brings us to the question: why is Yb4 As3 at low temperatures still a semimetal and not an insulator? From the present model we would naively expect that at zero temperature Yb4 As3 is an insulator. Charge order should be complete and a half-filled Hubbard chain is an insulator at sufficiently low temperatures for any positive value of U . In reality this is not the case due to incomplete charge order, 210 H. Aoki, T. Suzuki, and A. Ochiai, unpublished (2005). 211 A. Ochiai, H. Aoki, T. Suzuki, R. Helfrich, and F. Steglich, Physica B 230–232, 708 (1997). 212 Y. M. Li, N. d’Ambrumenil, and P. Fulde, Phys. Rev. B 57, R14016 (1998).

86

P. FULDE ET AL.

F IG . VI.10. LDA+U energy bands for Yb4 As3 . A small number of As 4p holes appears at the -point. The flat band has Yb 4f -character. (After Ref. [45].)

i.e., the Hubbard chains are not half-filled but doped. Within the model one possible explanation for incomplete charge order would be self-doping. Indeed, as function of U the exact solution of the Hamiltonian (6.11) shows a regime in the c vs. total electron concentration n0 plane where charge ordering is incomplete. However, in Yb4 As3 the true reason for the observed semimetallic behavior is found when bandstructure calculations within the local spin-density approximation plus U approach (LSDA+U) are performed. They show a rigid pinning of the Fermi energy to states close to the top of the As 4p band (see Figure VI.10). The filled 4f shell of Yb2+ is treated as a core shell and the interaction U = 9.6 eV between two 4f holes was adjusted to obtain the proper number of charge carriers. Because of a large gap between the As 4p and Yb 5d bands, the 4f hole band is pinned to the top of the As 4p band. This allows for charge transfer between Yb and As. As a result a small amount of As 4p holes is created, which act as mobile charge carriers with a corresponding reduction of Yb 4f holes. The calculated cyclotron masses of the almost spherical hole sheet of the As p states are in the range of 0.6 to 0.8 times the free electron mass m0 , in good agreement with the value of mexp = 0.72m0 obtained from cyclotron-resonance experiments while a value of 0.275m0 was obtained from Shubnikov–de Haas oscillations.213 However, the calculated mass should still be renormalized due to electron–phonon interactions. We want to draw attention to the fact that the relation between the large γ coefficient in the specific heat and the mass of the charged quasiparticles responsible for charge transport is lost here. This calls in question one fundamental requirement 213 P. Gegenwart, H. Aoki, T. Cichorek, J. Custers, N. Harrison, M. Jaime, M. Lang, A. Ochiai, and F. Steglich, Physica B 312–313, 315 (2002).

STRONGLY CORRELATED ELECTRONS

87

of Landau’s Fermi liquid theory. Its basis is a one to one correspondence between the excitations of an interacting electron system and those of a free electron system with renormalized parameters such as the quasiparticle mass. In the case of Yb4 As3 this correspondence holds only when the charge of the free electrons is renormalized to zero, i.e., when we deal with neutral fermions. This is due to the fact that the low-lying excitations are those of a Heisenberg chain which are of magnetic origin and can be described either by bosons or alternatively by neutral fermions. In addition to the neutral fermionic excitations in the chains which are spinon-like there are charged fermions (the As 4p-holes), i.e., electrons with a low density of states which provide for charge transport. The large A coefficient in ρ(T ) results from scattering of the charged fermions by the neutral ones, while the thermal conductivity is dominated by the neutral ones (spinons). This special feature is amplified when instead of Yb4 As3 semiconducting mixed crystals Yb4 (As1−x Px )3 with x = 0.3–0.4 are considered. These crystals also exhibit charge order like Yb4 As3 forming spin chains below the ordering temperature. The Sommerfeld constant is γ = 250 mJ/(mol K2 ) despite the fact that at T = 0 there are no charge carriers in the system.211 The LSDA+U calculations also show that one must be careful in finding the correct ordered structure by comparing Madelung energies. In competition with the trigonal phase considered here is a cubic P21 3 phase with chains of sequence – Yb3+ –Yb2+ –Yb2+ –Yb2+ –Yb3+ –Yb2+ – . The Madelung energy of this structure is slightly lower than the one of the trigonal structure. It does not couple to the 5 strain and therefore cannot explain the observed softening of the elastic constant c44 . But when the self-consistent charges are calculated one finds a slight charge disproportionation of 0.05 electrons between the center Yb2+ ion and the two adjacent Yb2+ ions. This changes the Madelung energy difference in favor of the trigonal structure. When a magnetic field H is applied to an isotropic antiferromagnetic spin chain (S = 12 , g = 2), the excitations remain gapless as long as the field remains smaller than gμB HS = J beyond which the system becomes a fully polarized ferromagnet with a Zeeman gap.214 It was therefore a surprise when it was found that the specific heat of Yb4 As3 depends strongly on H.215 Experimental results for γ (H) are shown in Figure VI.11. Likewise strong anomalies in the thermal expansion were found215 which is related to the specific heat via the Ehrenfest relation. A number of possible explanations of these observations have been proposed. One is based on magnetic interchain interactions.216 Another model calcu214 J. D. Johnson, J. Appl. Phys. 52, 1991 (1981). 215 M. Köppen, M. Lang, R. Helfrich, F. Steglich, P. Thalmeier, B. Schmidt, B. Wand, D. Pankert,

H. Benner, H. Aoki, et al., Phys. Rev. Lett. 82, 4548 (1999). 216 B. Schmidt, P. Thalmeier, and P. Fulde, Europhys. Lett. 35, 109 (1996).

88

P. FULDE ET AL.

F IG . VI.11. Yb4 As3 : Experimental field dependence of the specific heat γ coefficient (full circles) at T 0.5 K and theoretical results based on interchain interactions: lower and upper solid lines: H ⊥[111] and H [111]. The dashed curve is for T = 5 K. A ratio J /J = 10−4 was used. (After Ref. [216].)

lation advocates a staggered field mechanism due to the Dzyaloshinsky–Moriya interaction206 and a third one suggests that the dipolar interactions within a chain are responsible for the decrease of γ with increasing external field.205 In all three cases a magnetic field applied perpendicular to the Yb3+ chains is opening a gap in the excitation spectrum while the excitations remain gapless when the field is pointing along the chains. But they differ in details, e.g., in the way the gap opens. When a small interchain coupling J is assumed between adjacent Yb3+ chains a field perpendicular to the chains induces a gap ∼ (|J J |)1/2 . For J /J = 10−4 one obtains a decrease of the γ coefficient with increasing field of the observed size (see Figure VI.11). The two other models are based on independent Heisenberg chains. The model based on the Dzyaloshinsky–Moriya interaction exploits the fact that the Yb3+ sites are not centers of inversion (see Figure VI.12). The local C3 symmetry together with a glide reflexion and a glide vector parallel to the chains allows for the following features: a uniaxial anisotropy for the symmetric part of the spin– spin interaction and an antisymmetric Dzyaloshinsky–Moriya (DM) interaction. However due to the hidden symmetry they are not independent.206 A transformation consisting of staggered rotations with angle θ around the chain direction (z) makes this more apparent: The pseudo-spin Hamiltonian for the lowest Yb3+

STRONGLY CORRELATED ELECTRONS

89

F IG . VI.12. Yb4 As3 : Absence of a center of inversion in Yb3+ chains. The distance Yb(1)–As(1) (or Yb(2)–As(2)) is smaller than the distance Yb(1)–As(2) (or Yb(2)–As(1)). Atoms with equal gray scale are equivalent. (After Ref. [206].)

Kramers’ doublet, expressed in rotated spin operators, is then given by

Heff = J g Siz Hz + cos θg⊥ (Six Hx + Siy Hy ) Si Sj − ij

i

+ (−1)i sin θg⊥ (Siy Hx − Six Hy ) .

(6.20)

Here the C3 doublet wavefunction has associated anisotropic g-factors g,⊥ whose ratio is 2.5.206 The angle θ is adjustable and in principle determined by the C3 CEF parameters. Thus for zero field one has indeed an isotropic spin chain (S = 1/2) Hamiltonian despite involving strongly anisotropic wave functions of the lowest Kramers’ doublet state. This leads to the gapless spinon excitation spectrum discussed previously. When a magnetic field is applied perpendicular to the chain a staggered field perpendicular to both chain and applied field is induced by the DM interaction described by the last term in Eq. (6.20): Hs = g⊥ sin θ [n × H].

(6.21)

Here n is a unit vector in chain direction and g⊥ = 1.3 is the corresponding g factor. Due to the staggered field the uniform physical susceptibility χ⊥ (0) is a mixture of q = 0 (uniform) and q = π (staggered) susceptibilities χ1D of the (S = 12 , g = 2) isotropic Heisenberg chain according to 2 2 χ⊥ (0) = g⊥ cos (θ )χ1D (0) + sin2 (θ )χ1D (π) . (6.22) Since the latter diverges ∼ 1/T at low temperatures this should lead to a Curielike upturn also in the homogeneous χ⊥ (0, T ). This behavior was indeed found and in principle the value of tan2 (θ ) = 0.04 may be extracted from the analysis of

90

P. FULDE ET AL.

F IG . VI.13. Upper panel: Spin excitations (ωL (q)) from INS in an Yb3+ chain in a magnetic field perpendicular to the chains and without it. Note the gap opening at q = π/d. After Ref. [217]. Lower panel: Gap as function of applied field. A scaling exponent 2/3 corresponding to quantum sine-Gordon equation is found (full line: (H ) ∼ Es (H ) ∼ H 2/3 ). Here Es (H ) is the gap from thermodynamic and transport quantities and (H ) is the gap obtained in INS. (After Ref. [197].)

the upturn. The most important effect of the staggered field is the appearance of an induced gap in the excitation spectrum with a field dependence 2/3

(H ) 1.8J 1/3 Hs

∼ H 2/3 .

(6.23)

This gap was seen in thermodynamic and transport properties like specific heat, thermal expansion, etc.215,213 and the field scaling exponent 2/3 was indeed identified (Figure VI.13). A field dependence of this form has also been directly observed by inelastic neutron scattering (INS) on a single crystal at T = 1.9 K. A gap 217 M. Kohgi, K. Iwasa, J.-M. Mignot, B. Fak, P. Gegenwart, M. Lang, A. Ochiai, H. Aoki, and T. Suzuki, Phys. Rev. Lett. 86, 2439 (2001).

STRONGLY CORRELATED ELECTRONS

91

was found to open up at q = πd when the field was perpendicular to the short, i.e., Yb3+ chains (see Figure VI.13). This supports the above model. In passing we note that the above excitations can also be described by a sine-Gordon equation associated with moving domain walls as applied to Cu-benzoate.218 But when the magnetic field is parallel to the chain, gapless modes at finite q = πd (1±2σ ) (σ = magnetization) are expected219,220 which so far have not been seen and this casts some doubt on the theory. This brings us to the third model which is based on the weak dipolar interaction of the Yb3+ sites. For that purpose the DM interaction is neglected. The dipolar interaction is

Ji Jj − 3(Ji e)(Jj e) Hdip = g 2 μ2B (6.24) |Ri − Rj |3 i<j

where e = (Ri − Rj )/|Ri − Rj | and only the ground state doublet of the Yb3+ is taken into account. This leads to an effective, slightly anisotropic Heisenberg antiferromagnet in an applied field. In a transverse field a gap opens up.221 A special feature is that at high fields the gap should close again. Measurements up to H = 30 T reveal this effect. Indeed a strong reduction of the gap below the (H ) ∼ H 2/3 scaling curve (Figure VI.13) was observed already above H = 10 T.213 When H is parallel to the chains a Zeeman splitting is expected and there should be no incommensurate peaks appearing, in agreement with experiments. In summary it seems that the magnetic field effects are not yet fully understood. 14. C HARGE O RDERING AND 1D S PIN E XCITATIONS IN α -NAV 2 O 5 In quasi-1D metals such as organic charge transfer salts or the famous KCP chain compound187 it is known that the ground state exhibits a spontaneous dimerization due to the instability of the 1D Fermi surface. It is signified by a diverging electronic susceptibility at wave number q = 2kF . In real compounds this instability, the ‘Peierls-transition’ takes place at a finite transition temperature controlled by the interchain-coupling. Amazingly a similar ‘spin-Peierls’ transition may occur in insulating quasi-1D spin chains with antiferromagnetic nearest neighbor (n.n.) coupling. This is most conveniently understood for an xy-type exchange interaction model which can be exactly mapped by a Jordan–Wigner transformation 218 D. C. Dender, P. H. Hammar, D. N. Reich, C. Broholm, and G. Aeppli, Phys. Rev. Lett. 79, 1750 (1997). 219 G. Müller, H. Thomas, H. Beck, and J. C. Bonner, Phys. Rev. B 24, 1429 (1981). 220 H. Shiba, K. Ueda, O. Sakai, and S. Qin, Physica B 312–313, 309 (2002). 221 D. V. Dmitriev, V. Y. Krivnov, and A. A. Ovchinnikov, Phys. Rev. B 65, 172409 (2002).

92

P. FULDE ET AL.

(JW) to a model of free spinless 1D fermions at half filling.222 Naturally this leads to a chain dimerization via the same ‘electron’–phonon coupling as in the case of real conduction electrons. Adding the z-term of the Heisenberg exchange interaction one obtains an interacting fermion model after the JW transformation but the basic mechanism of dimerization is unchanged. The spin-Peierls transition has originally been found in a number of organic spin chain compounds and has been theoretically investigated first in Ref. [223] within a mean-field treatment and later in Ref. [224] using the Heisenberg exchange and its coupling to the lattice in the fermionic (JW) representation. Surprisingly the spin-Peierls transition rarely occurs in inorganic 1D-spin chain compounds, presumably because magnetic order due to interchain–exchange is preferred in most cases. The only such spin-Peierls compound known until recently was CuGeO3 225 where the S = 12 spins of Cuchains undergo dimerization at TSP = 14 K. The corresponding dimerization of the exchange integral along the chain then creates an isotropic spin excitation gap. The ensuing isotropic drop in the spin susceptibility below the transition temperature is therefore the most direct method to identify the spin-Peierls mechanism. Actually this is not unambiguous because the presence of n.n.n exchange interactions J with a ratio J /J > 0.24 where J is the n.n. exchange also leads to a spin gap and this issue is still controversial in CuGeO3 . Therefore the discovery of a structural phase transition in the layered perovskite insulator α -NaV2 O5 at Tc 34 K with a corresponding isotropic spingap formation226 has created enormous interest and activity, both experimental and theoretical. This compound was seen as a second candidate for an inorganic spin-Peierls system which seemed to be consistent with the original crystal structure determination227 that suggested the existence of S = 1/2 V4+ spin chains along the crystal b-axis (every second V chain in Figure VI.14), isolated by intervening nonmagnetic V5+ (S = 0) chains. Both belong to V-V ladders formed by the oxygen pyramids, where neighboring ladders are shifted by b/2. In the ab-plane this leads to a Trellis lattice structure shown in Figure VI.14. Exchangedimerization of the S = 1/2 V chains due to the spin-Peierls mechanism below Tc would then lead to the isotropic spin gap. This interpretation was however much too naive as became clear subsequently. It turned out that the structural phase transition is not of the simple chain dimerization type but leads to a very low symmetry (monoclinic) structure that can only be understood if in addition a charge 222 G. Beni and P. Pincus, J. Chem. Phys. 57, 3531 (1972). 223 E. Pytte, Phys. Rev. B 10, 4637 (1974). 224 M. C. Cross and D. S. Fisher, Phys. Rev. B. 19, 402 (1979). 225 M. Hase, I. Terasaki, and K. Uchinokura, Phys. Rev. Lett. 70, 3651 (1993). 226 M. Isobe and Y. Ueda, Phys. Soc. Jpn. 65, 1178 (1996). 227 A. Carpy and J. Galy, Acta Crystallogr. B 31, 1481 (1975).

STRONGLY CORRELATED ELECTRONS

93

F IG . VI.14. Upper panel: Layered perovskite structure of α -NaV2 O5 consisting of chains of oxygen pyramids that contain the V atoms aligned along the crystal b axis. The layers are stacked along c axis. Na atoms (grey spheres) are centered above the ladder plaquettes. Lower panel: ab-plane Trellis lattice structure of V-V ladders alternatingly shifted along b by half a lattice constant. This leads to a quasi-‘triangular’ structure for V-V rung units. Orthorhombic high temperature unit cell is indicated.

ordering transition of V4+ /V5+ is present, starting from a homogeneous high temperature insulating mixed valence (V4.5+ ) state, in contrast to the first assumption in Ref. [227]. Nevertheless above Tc the susceptibility exhibits the typical Bonner–Fisher maximum of 1D spin chains.226,228 This compound therefore is another example of an intricate relation between charge ordering and quasi-1D spin excitations which in the present case are gapped. In this section we first discuss the result of the increasingly more detailed X-ray analysis of the high and low temperature structure of α -NaV2 O5 , nevertheless no final agreement on the low-T structure has been reached. Electronic structure calculations are essential to construct an effective Hamiltonian for the charge ordering. We will argue that this transition and the ensuing spin 228 P. Horsch and F. Mack, Eur. Phys. J. B 5, 367 (1998).

94

P. FULDE ET AL.

gap formation requires the inclusion of lattice degrees of freedom which lead to the appearance of two inequivalent V-V ladder types in the perovskite layers. The gapped spin excitation spectrum in the distorted CO phase will be discussed within a simple dimer-RPA approach and a comparison with INS results is given which also advocates the inequivalent ladder model. Finally we briefly mention the stacking of CO layers along c and the destruction of CO by Na deficiency doping or substitution of Na by Li or Ca and in connection with the nature of the insulating state in α -NaV2 O5 . In this section we will not review the various alternative theoretical models that have been proposed for α -NaV2 O5 . We also will exclude the discussion of most optical experiments, since this is not the ideal method to investigate spin excitations. The determination of the crystal structure of α -NaV2 O5 , both above and below Tc , is fundamental for constructing a microscopic model for the phase transition and spin gap mechanism. This was surprisingly controversial and has led to much confusion, mostly for the low- but even for the high-temperature structure. The latter was originally thought to have non-centrosymmetric symmetry227 already above Tc leading to the assumption of V5+ /V4+ in-line charge disproportionation on each V-V rung of the ladders from the outset. However later it was discovered229 that the proper high temperature structure belongs to the centrosymmetric Pmmn space group. Due to the reflection plane containing y both V-sites in the rungs must be equivalent, i.e., they are in a mixed valence state V4.5+ . The structure of the low temperature phase (T Tc ) proved even more controversial. In Refs. [230–232] an orthorhombic space group Fmm2 with a 2a × 2b × 4c supercell was proposed. In the low temperature phase the modulation (atomic shifts of V, O and Na atoms with respect to high temperature structure) strongly differs for neighboring ladders A and B. Loosely speaking the atomic positions on A are modulated while on B they are not (see Figure VI.17). Subsequently it was shown233 that the symmetry is even lower, characterized by the monoclinic space group A112 which does not contain an inversion symmetry. This implies the existence of a spontaneous dipole moment (induced ferroelectric order parameter) below the phase transition which has indeed been observed by measuring the dielectric function. The two space groups differ in the number of inequivalent atoms 229 H. G. von Schnering, Y. Grin, M. Knaupp, M. Somer, R. K. Kremer, O. Jepsen, T. Chatterji, and

M. Weiden, Z. Kristallographie 213, 246 (1998). 230 J. Lüdecke, A. Jobst, S. van Smaalen, E. Morré, C. Geibel, and H. G. Krane, Phys. Rev. Lett. 82, 3633 (1999). 231 S. van Smaalen and J. Lüdecke, Europhys. Lett. 49, 250 (2000). 232 J. L. deBoer, S. A. Meetsma, J. Baas, and T. T. M. Palstra, Phys. Rev. Lett. 84, 3962 (2000). 233 H. Sawa, E. Ninomiya, T. Ohama, H. Nakao, K. Ohwada, Y. Murakami, Y. Fuji, Y. Noda, M. Isobe, and Y. Ueda, J. Phys. Soc. Jpn. 71, 385 (2002).

STRONGLY CORRELATED ELECTRONS

95

per unit cell, e.g., 6 V sites in two inequivalent layers a, b for Fmm2 and 8 V sites again in two layers for A112. Likewise there are 6 vs. 8 inequivalent Na atoms and 16 vs. 20 inequivalent O atoms in both cases respectively. Nevertheless, the full refinement of the modulated crystal structure with A112 and Fmm2 space group leads to almost identical atomic positions.233 This raises the question how the valences, most importantly of V-atoms should be assigned in the low temperature structure. Unfortunately the modulated structure has not yet been investigated within LDA+U calculations. Therefore one has to resort to the empirical valence-bond method.234 In this approach every atom at an inequivalent site is assigned a formal valence Vi (or oxidation number) which may be thought of as the number of electrons it contributes to all the bonds connected to ligand atoms according to the prescription

R0 − Rij (6.25) vij with vij = exp |Vi | = B j

where vij is the valence of a given central atom-ligand bond which depends on the bond length. Here R0 and B are empirical parameters characteristic of a given type of chemical bond, e.g., V–O bond, independent of the material. The optimal parameters R0 and B may however be weakly temperature dependent. Using the sum rule in Eq. (6.25) and identifying valence with the number of electrons contributing to bonds the valence of constituents may be determined. In α -NaV2 O5 we are primarily interested in the number of electrons in the V-dxy orbital because the 3dxy -bands are well separated from all other bands as seen below. Its orbital occupation is then given by ndxy = 5–Vi , assuming that bonding takes place mainly with the lower lying O3p orbitals. This quantity is the most interesting to study in view of possible charge ordering. We now discuss a few basic observations that prove the connection between charge ordering and spin gap formation at the structural phase transition. It has been proposed early from thermal expansion measurements235 that actually there are two separate but close by phase transitions at Tc1 33 K and Tc2 32.7 K which are of first and second order respectively. These values depend considerably on sample quality and may be higher (see Figure VI.15) than those given above. Detailed investigation of NMR frequencies and Knight shifts have shown236 that Tc1 and Tc2 may be associated with charge ordering on V-sites and a spin-gap formation respectively (Figure VI.15). In the following we will denote the whole 234 J. D. Brown, Acta Cryst. B 48, 553 (1992). 235 M. Köppen, D. Pankert, R. Hauptmann, M. Lang, M. Weiden, C. Geibel, and F. Steglich, Phys.

Rev. B 57, 8466 (1998). 236 Y. Fagot-Revurat, M. Mehring, and R. K. Kremer, 84, 4176 (2000).

96

P. FULDE ET AL.

F IG . VI.15. Upper panel; V-Knight shift 51 Kcc and Na-Knight shift 23 Kcc as well as quadrupolar frequency 23 νcc of α -NaV2 O5 . The first reflects charge order, the second the opening of the spin gap and the third the lattice distortion around Na-sites. Since 23 Kcc and 23 νcc behave synchronously below Tc2 this suggests that spin gap formation is connected with exchange dimerization due to Na-shifts. After Ref. [236]. Lower panel: Magnetic susceptibility for single crystalline α -NaV2 O5 showing the isotropic spin gap opening below Tc2 . (After Ref. [237].)

region of these close transitions simply by ‘Tc ’. At the lower transition the critical exponent of the spin-gap opening SP ∼ (1 − T /Tc )β is β ∼ 0.34 close to 2 the theoretical value 0.33 obtained from SP ∼ δ 3 (see Ref. [224]) and a mean1 field chain and exchange dimerization behavior δ ∼ (1 − T /Tc ) 2 . This suggests indeed a spin-Peierls dimerization at the lower transition. The first transition on 237 M. Weiden, R. Hauptmann, C. Geibel, F. Steglich, M. Fischer, P. Lemmens, and G. Güntherod, Z. Phys. B 103, 1 (1997).

STRONGLY CORRELATED ELECTRONS

97

the other hand has a 2D-Ising character, as indicated by a logarithmic peak in the specific heat superposed by the jump of the second transition. Furthermore, according to temperature dependence of X-ray satellites the total lattice distortion has a temperature exponent β ∼ 0.2 closer to the Ising value 1/8 than to the mean-field exponent. In summary, these findings suggest that the Tc1 -transition leads to charge ordering on the V-sites and has partly 2D Ising character. Its field dependence is smaller than for an Ising transition but larger than for a pure structural transition. At Tc1 the main lattice distortion takes place. At the slightly lower Tc2 the spin gap opens with a spin-Peierls like exponent and connected with an additional exchange dimerization along the charge ordered chains. Before discussing microscopic models for these peculiar transitions results of the electronic structure calculations for α -NaV2 O5 have to be summarized. So far they were only done for the undistorted structure. Both LDA calculations238 and spin polarized LDA+U calculations239 for the charge ordered (but undistorted) case have been performed. In both cases it is found that the planar V dxy bands are well separated from hybridized Vd-Op-bands which are fully occupied or empty as shown in Figure VI.16. In the LDA calculation the Fermi level is centered in the dxy band predicting a metallic state, contrary to the fact that even without CO above Tc α -NaV2 O5 is an insulator. As in the undoped cuprates this is due to a neglect of on-site Coulomb correlations in LDA. In the LDA+U treatment they are simulated by breaking the orbital symmetry, i.e., by using an orbital-occupation dependent one-electron potential

1 LDA+U LSDA (6.26) − nασ |ασ ασ | = Vσ + (U − J ) Vσ 2 α where U, J are the on-site Hubbard and exchange energy and α denotes the 3dorbitals. In a charge ordered state the different orbital occupations of inequivalent V-sites cause relative shifts of their orbital energies. As shown in Figure VI.16 this leads to a dxy subband splitting with a charge transfer gap CT . It moves the Fermi level to the top of the lower subband, thus creating a charge transfer insulator in the CO phase. The size of the gap is CT 0.5–1 eV. A gap of this size was indeed found in optical conductivity measurements.240 Calculation of the total LDA+U energy for various CO structure favors the zig-zag structure in one ladder,239 however so far it cannot say anything on the arrangement of adjacent CO ladders or whether only every second ladder exhibits CO as proposed in 238 H. Smolinsky, C. Gros, W. Weber, U. Peuchert, G. Roth, M. Weiden, and C. Geibel, Phys. Rev. Lett. 80, 5164 (1998). 239 A. N. Yaresko, V. N. Antonov, H. Eschrig, P. Thalmeier, and P. Fulde, Phys. Rev. B 62, 15538 (2000). 240 C. Presura, D. van der Marel, M. Dischner, C. Geibel, and R. K. Kremer, Phys. Rev. B. 62, 16522 (2000).

98

P. FULDE ET AL.

F IG . VI.16. Left panel: LDA+U DOS of α -NaV2 O5 with U = 4.1 eV and J = 1.1 eV exhibits two isolated 3dxy subbands due to enforced charge order with a charge transfer gap CT ∼ 0.5–1 eV between them. Right panel: Tight binding (TB) fit to LDA bands (CT = 0) with full V-O basis corresponding to effective hopping elements tR = 0.380 eV, tL tD = 0.085 eV for the effective V-V TB model with only dxy -states included. Note that within LDA a metallic state is predicted with EF lying in the lower dxy band. (After Ref. [239].)

the structure model of Ref. [230] and others. The nature of the insulating phase above Tc is an unsolved problem since every rung is only singly occupied, i.e., one has quarter filled V-ladders. Even without CO when CT vanishes there is an excitation gap for double occupancy of V-V rungs. An interpretation as a simple Mott–Hubbard insulator in an effective dxy -one band model based on the molecular orbital (bonding) state of a rung seems inadequate. An interpretation of the insulating state in terms of an extended Hubbard model has been proposed in Ref. [241]. Such microscopic models require as an input the effective hopping parameters obtained from a mapping of LDA band structure to a tight binding model. It was shown in Ref. [239] that an adequate mapping requires a basis of both V dxy and O px , O py orbitals. The result is shown in Figure VI.16 for the full basis. Nevertheless in a crude approximation this may be further simplified by mapping to an effective dxy model containing only three hopping parameters tR , tL and tD along the rung, leg and diagonal of a single ladder (inset of Figure VI.17). Their values are given in Figure VI.16. It is found that tL tD . This leads to the essentially flat upper band in Figure VI.16 (right) and therefore tD cannot be neglected. It is also essential to obtain the proper exchange Hamiltonian for the zig-zag CO structure [111] which will be discussed now. The description of the coupled CO and exchange dimerization in α -NaV2 O5 starts from an extended Hubbard model containing hopping terms discussed before, the on-site effective Coulomb energy Ueff 3 eV and unknown intersiteCoulomb energies VR , VL and VD for the same bonds as the hopping integrals 241 A. Bernert, Ph.D. thesis, TU Dresden (2001).

STRONGLY CORRELATED ELECTRONS

A

B

A

99

B

F IG . VI.17. Charge order and dimerization in α -NaV2 O5 . Left panel: Shift of V-positions in distorted a-layer below Tc1 . Stacking along c is of aaa a type. In a -layers A shifts have the same phase and B shifts are moved by one lattice constant along b (ladder direction). Each layer has three inequivalent V (full, open and gray circles), leading to 6 inequivalent V. Charge order (zig-zag) happens mainly on A, ladder dimerization on B. Below Tc2 the A ladders also dimerize and V sites on B become inequivalent leading to 8 inequivalent V sites altogether. Right panel: Variation of effective spin exchange along the ladder (b-direction) with V charge order parameter 2δCO for zig-zag CO (A). 0 is the actual charge order parameter for α -NaV O on A-ladders corresponding to J = 440 K δCO A 2 5 (37.9 meV). Inset shows TBA hopping elements tR (along rung a), tL (along leg b) and tD (along diagonal) on a ladder plaquette. The same convention for inter-site Coulomb interactions VR , VL and VD is used. (After Ref. [242].)

(inset of Figure VI.17). For an investigation of CO, this model may be reduced to a much simpler one taking for granted an insulating state with double occupancies of rungs prohibited. Then the charge degrees of freedom are described by a pseudo spin T = 12 where Tz = ± 12 describes a dxy electron that occupies the left (− 12 ) or right (+ 12 ) V-atom of a rung.243 The projected Hamiltonian in the charge sector then has the form244

ij

ij HITF = KLz Tiz Tjz + KI L Tiz Tjz + 2t˜Ri Tix (6.27)

i,j L

i,j I L

i

which is the Ising model in a transverse field (ITF) whose role is plaid by the renormalized intra-rung hopping t˜Ri . In the spin sector one has a Heisenberg Hamiltonian with exchange between the spins on neighboring rungs and legs ij ij (Eq. (6.30)). Like the Ising interaction ‘constants’ KLz (intra-ladder) and KI L 242 A. Bernert, P. Thalmeier, and P. Fulde, Phys. Rev. B 66, 165108 (2002). 243 P. Thalmeier and P. Fulde, Europhys. Lett. 44, 242 (1998). 244 A. Bernert, T. Chatterji, P. Thalmeier, and P. Fulde, Eur. Phys. J. B 21, 535 (2001).

100

P. FULDE ET AL.

(inter-ladder) t˜Ri is related to the original Hubbard parameters which are renormalized by terms that depend on the spin configuration:242 ij

KLz = 2VL + δKLz (Si , Sj ) ij

KI L = −VI L + δKI L (Si , Sj )

δ t˜R (Si , Sj ). t˜R = tR +

(6.28)

ij L

In this model the charge (T) degrees of freedom and spin (S) degrees of freedom are coupled through the renormalized interaction constants of Eq. (6.28) that depend on the spin configuration. As a consequence, even above Tc the optical conductivity which probes the (rung) charge excitations also shows a signature of coupled spin excitations.245 For the moment, considering only the possibility of charge ordering we may freeze the spins in an AF or FM configuration along or between the ladders according to the sign of the spin exchange obtained in LDA+U calculations.239 This leads to values t˜R = −0.19 eV and KLz −KI L = 0.68 eV.242 One might expect that the Hamiltonian in Eq. (6.27) on the rigid Trellis lattice describes charge order in a natural way, however this is not so obvious. It is true that the ITF on a single ladder (first and last term in Eq. (6.27)) has a (doubly degenerate) ground state with staggered ‘AF’ (KLz > 0) pseudo-spins corresponding to zig-zag charge order along the ladder if the magnitude of the ‘transverse field’ t˜R is smaller than a critical value 4t˜Rc = KLz . This value defines the quantum critical point λc = 1 of the ITF model93 with the dimensionless control parameter λ = KLz /4t˜R . For λ > λc , and assuming an infinitesimal staggered field to lift the twofold ground-state degeneracy, the order parameter of zig-zag CO is given by the exact solution of the 1D ITF:

2 1 8 z λc i1 1− Ti = (−1) = (−1)i δCO (λ). (6.29) 2 λ However due to the Trellis lattice structure (Figure VI.14) the rungs of a ladder form a trigonal covering lattice and therefore the inter-ladder coupling KI L frustrates the zig-zag charge ordering on a given ladder. Therefore the critical λc (KI L ) increases monotonously with the inter-ladder coupling which defines a quantum critical line for zig-zag CO at T = 0 in the KLz –KI L plane. At finite temperature the presence of frustration prevents zig-zag CO to occur. If KI L becomes equal to the intra-ladder KLz , CO melts and for some range of KI L even at T = 0 a disordered state appears. Finally if KI L increases even further one obtains again a CO state, but now with in-line order with parallel alignment of pseudo spins 245 M. V. Mostovoy, D. I. Khomskii, and J. Knoester, Phys. Rev. B 65, 064412 (2002).

STRONGLY CORRELATED ELECTRONS

101

along a ladder, i.e., V4+ configurations are on one side of the ladder and V5+ on the other side. These conclusions have been drawn from an exact diagonalization study of the 2D model with finite KI L .246 The LDA+U results for α -NaV2 O5 (see Ref. [239]) imply a relation 2VL − VI L 0.027 eV meaning KLz KI L . Therefore α -NaV2 O5 is indeed close to the quantum critical line for zig-zag charge order and purely Coulombic interactions cannot lead to a phase transition at finite temperature in this compound due to geometric frustration. This is rather similar to the charge ordering in the pyrochlore- or spinel lattices (or their 2D analogue, the checkerboard lattice) where charge ordering is also prohibited by the inherent geometric frustration due to corner sharing tetrahedra of V- or other 3d ions of different valencies (Section VII). In such structures CO requires the lifting of macroscopic degeneracy of the charge configurations by a lattice distortion as is the case in AlV2 O4 (see Section VII.17). Something similar happens in α -NaV2 O5 . The driving mechanism for the lattice distortion is here the spin superexchange energy between singly occupied rungs along a ladder. Due to the quarter-filled ladders the superexchange does not only contain terms coming from intermediate states with doubly occupied sites but also contributions from rungs with two singly occupied sites. The latter depend on the pseudospin configurations, which is the complementary effect as compared to Eq. (6.28). Therefore the effective spin exchange constants will depend on the degree of charge order. One obtains

Jij Sij Si+1j Hex = i,j

Jij = 1 +

α

uαi+ 1 ,j ∇ αi+ 1 ,j 2 2

z J Tijz , Ti+1j

ij z z J Tijz , Ti+1j = J0 1 + f Tijz , Ti+1j uij =

λq

λ† 1 λ . exp iqRij bqj + bqj 1/2 (mN )

(6.30)

The summation runs over the atomic shifts uij of neighboring atoms (α = O, Na) with respect to V which modulate the superexchange. In addition the latter depends on the charge configuration. Therefore spin (Si ), charge (Ti ) and lattice λ ) degrees of freedom are now coupled via Eq. (6.30). The spin exchange in (bqj Eq. (6.30) has to be added to Eq. (6.27) to get the total Hamiltonian HISSP of the z ) Ising-spin Peierls model for α -NaV2 O5 . To simplify the model the J (Tijz , Ti+1j 246 A. Langari, M. A. Martin-Delgado, and P. Thalmeier, Phys. Rev. B 63, 144420 (2001).

102

P. FULDE ET AL. ij

dependence is approximated by Jij = J0 (1 − 4Tjz 2 ). This reduction of superexchange (Figure VI.17) with increasing charge order was explained before. The remaining spin-lattice part is treated within the Cross–Fisher theory.224 The combined spin-Peierls transition and charge ordering takes place at Tc1 . At that temperature the renormalized frequency of the VO-bond dimerization mode with wave vector q0 = π/b along the ladder given by 2 (6.31) ω˜ q20 (T ) = ωq20 − 0.26gVO (q0 ) T −1 − 4gI2s χq0 (T ) becomes soft, i.e., when ω˜ q20 (Tc1 ) = 0. Here the last term is determined by the pseudo-spin susceptibility χq0 (T ) of HITF where gI s is a coupling constant that describes the change of the transverse pseudo-spin field with lattice distortion. It may be shown that inclusion of a spin-Zeeman term leads to the proper field dependence of Tc1 (H ) observed in experiment. It is found to be much weaker than for a pure spin Peierls transition. The choice of the precise order parameter and distortion pattern between the ladders below Tc1 is determined by the minimization of the total free energy. On a given ladder there is a competition between the exchange dimerization energy gain of the spin Peierls distortion and the zig-zag charge order because the former is proportional to J and the latter reduces J as just discussed (Figure VI.17). This can be avoided by generating two inequivalent types of ladders A and B below Tc1 where one (A) is mainly charge ordered and the other (B) mainly dimerized.242 At the same time this reduces the symmetry of the Trellis lattice in such a way that geometric frustration is reduced and long range charge order is stabilized at a finite temperature. Indeed, X-ray results230,233 show that the distortion of B-type ladders is much stronger as of Atype ladders, independent of whether orthorhombic Fmm2 or monoclinic A112 space groups are used for the structure refinement (Figure VI.17, left panel). At this stage, slightly below Tc1 one has a large spin gap on B ladders but none on the zig-zag spin chains on the A ladders. However the rapidly growing charge order δCO (T ) on A-type ladders below Tc1 modulates the hopping integrals and orbital energies via Na- and rung O- shifts. This occurs in such a way that an additional but smaller exchange dimerization is also induced on the A-type ladders. It grows with δCO (T ). Once it is big enough it leads to a further dimerization below Tc2 on the A-type ladders which is now of the pure spin-Peierls type and opens the spin gap seen in experiment (Figure VI.15). This interpretation is supported by the appearance of additional Na-NMR splittings caused by the shifts of Na atoms on top of the A-ladders for T < Tc2 . They correspond to 8 instead of 6 inequivalent Na positions below Tc2 which is indeed compatible with the monoclinic A112 structure from X-ray analysis.233 Although the mechanism for the phase transitions is intricate, involving charge, spin and lattice degrees of freedom and their competing coupling effects, the low temperature (T Tc ) spin dynamics is quite simple again. With charge order and

STRONGLY CORRELATED ELECTRONS

103

lattice distortion saturated only the pure spin part in Eq. (6.30) of the original ISSP Hamiltonian remains. Thereby the existence of two inequivalent A,B-type ladders and their low temperature (T Tc1 ) distortions in the parameterization of exchange constants has to be taken into account. Since the B ladders are strongly exchange dimerized with a δB ∼ 0.25 and J = JB (1 ± δB ) they have a large spinexcitation gap B = 38 meV.242 It is not visible in the inelastic neutron scattering (INS) results which show a minimum excitation energy around 10 meV. It must therefore result from excitations on the more weakly dimerized (δA δB ) A-type CO ladders. Consequently the low temperature spin Hamiltonian comprises only slightly dimerized 1D zig-zag S = 1/2 spin chains (on A) with an intra-chain exchange JA (1 ± δA ) along the b-direction. Since they are separated by intervening B-ladders the A-ladders are only weakly coupled with Ja JA in the transverse a-direction. One therefore would expect gapped quasi-1D spin excitations in α NaV2 O5 . Indeed it was found that their dispersion is much stronger along b than along a.247,248 As mentioned earlier the stacking of layers along c is of the aaa a type.249 Therefore the zig-zag chains on A are in-phase on aa (and a a ) bilayers and out-of-phase between aa . In the c-direction one may therefore assume an exchange Jc within the bilayers and neglect coupling between them. Using this effective exchange model with parameter set (JA , δA , Ja , Jc ), where Ja = Ja − 4JD is an effective intra-chain exchange along a, the magnetic excitations have been calculated within a local dimer approach. It is applicable here since JA Ja , Jc . The susceptibility of an isolated dimer pair in the bilayer is given by u± (ω) =

2(JA (1 + δA ) ∓ Jc ) . (JA (1 + δA ) ∓ Jc )2 − ω2

The collective susceptibility of the bilayers in RPA is then expressed as −1 q , ω) = 1 − J ( q )u± (ω) u± (ω). χ ± (

(6.32)

(6.33)

The dispersion of spin excitations in the ab plane may be obtained from the poles q , ω) as of χ ± ( 2 2 ω± (qx , qy ) = JA (1 + δA ) ∓ Jc − JA (1 + δA ) ∓ Jc × JA (1 − δA ) cos 2qy ± Ja cos(qx − qy ) − 4JD cos qx cos qy . (6.34) 247 B. Grenier, L. P. Regnault, J. E. Lorenzo, T. Ziman, J. P. Boucher, A. Hiess, T. Chatterji, J. Jegoudez, and A. Revcolevschi, Phys. Rev. Lett. 86, 5966 (2001). 248 T. Yosihama, M. Nishi, K. Nakajima, K. Kakurai, Y. Fuji, M. Isobe, C. Kagami, and Y. Ueda, J. Phys. Soc. Jpn. 67, 744 (1998). 249 K. Ohwada, Y. Fuji, K. Y. J. Muraoka, H. Nakao, Y. Murakami, H. Sawa, E. Ninomiya, M. Isobe, and Y. Ueda, Phys. Rev. Lett. 94, 106401 (2005).

104

P. FULDE ET AL.

The comparison of mode dispersions with experimental results is shown in Figure VI.18. Using the low temperature JA = 440 K (see Ref. [248]) which corresponds to the charge order parameter 2δCO = 0.32 in Figure VI.17 the remaining parameters may be determined from three of the four observed gaps ω± (0, 12 ) and ω± (0, 1) in Figure VI.18. The fourth (lowest) gap is then correctly calculated as ω− (0, 1) = 8.14 meV. The exchange dimerization obtained is δA = 0.03 δB . The model calculation explains a number of observations from INS:

F IG . VI.18. Dispersion of spin excitations in α -NaV2 O5 (qx a and qy b given in r.l.u. 2π/a and 2π/b respectively). Comparison of theoretical fit after Eq. (6.34) with experimental results from Ref. [247]. Full lines: qy0 = 12 , broken lines q0y = 1. Upper panel: ω+ (qx )-dispersion (top) and ω− (qx )-dispersion (bottom). From extremal values at qx = 0 model parameters δA = 0.03, Ja = 0.21 meV and Jc = 0.43 meV are obtained. Lower panel: Dispersion along b with exchange JA = 37.9 meV (440 K) along zig-zag chain on A. (After Ref. [242].)

STRONGLY CORRELATED ELECTRONS

105

(i) The dispersion along b is much larger than along a because Ja JA due to weak coupling of A-ladders through intervening B-ladders. (ii) The a-dispersion of ω+ (qx , qy0 ) is considerably smaller than for ω− (qx , qy0 ) with qy0 = 12 or 1. (iii) Contrary to earlier results248 the high resolution experiments247 presented in Figure VI.18 show a finite gap between lower and upper mode +− 1 meV which is determined by a combination of JA and Jc . It provides strong evidence for the inequivalent A-B ladder model. If only equivalent A-ladders were present, the gap should vanish, i.e., ω+ (qx , qy0 ) and ω− (qx , qy0 ) would touch with their minima and maxima and the dispersion would have twice the observed period along a.250 We conclude that α -NaV2 O5 presents another example where charge ordering may lead to pronounced 1D character of spin excitations below Tc , here they are gapped due to exchange dimerization caused by the complicated nature of the associated lattice distortions. It has become clear that CO in α -NaV2 O5 is severely inhibited by effects of geometric frustration. In fact its comparatively low Tc 33 K indicates that it is close to the quantum critical point of the ITF model, where the CO is of essentially 1D Ising type. The true 2D ordered state at finite T is then established by a staggered longitudinal pseudo spin field set up by the distortions of the neighboring ladders. In this scenario it is suggestive that even small perturbations of the 1D Ising spin correlations along the ladder might suppress the CO state in α -NaV2 O5 . This can be achieved by reducing the filling factor n of the 1D ladders below 14 by doping with holes. This introduces “empty” rungs into the ladder which cut the Ising bonds. The ensuing destruction of long-range 1D correlations should then strongly reduce Tc as function of the hole concentration δh (n = 14 − δh ). This has indeed been found by introducing holes into the ladders through Na-deficiency doping251 where a few per cent holes are sufficient to destroy the CO state and the associated spin Peierls transition. Rapid suppression of charge order has also been found in various other doping series, i.e., replacing Na by Li and K (isoelectronic) or Ca (electron-doping).252 This may be observed directly by specific heat measurements252 which show a progressive suppression of C(Tc ) with increasing doping. It is also seen in the susceptibility251 which exhibits a closing of the spin gap associated with CO. Most importantly, in this doping range α -Nax V2 O5 remains an insulator. This is not easy to understand within a Hubbard like model for the quarter filled ladder.244,242 Possibly 1D localization and polaronic effects play a role, indeed the conductivity was found to exhibit variable-range hopping behavior251 for hole doping. It was shown in 250 C. Gros and R. Valenti, Phys. Rev. Lett. 82, 976 (1999). 251 M. Isobe and Y. Ueda, J. Alloys Compounds 261–263, 180 (1997). 252 M. Dischner, C. Geibel, E. Morré, and G. Sparn, J. Magn. Magn. Mat. 226–230, 405 (2001).

106

P. FULDE ET AL.

Ref. [253] that even for the (hole-) doped case the CO problem may be treated with an extended pseudo-spin model. In order to incorporate the possibility of empty rungs on a ladder a pseudo spin T = 1 is introduced where the |Tz = ±1 states describe occupation of the right or left V dxy orbital of a rung respectively, and in addition |Tz = 0 the empty (hole-doped) rung. The total effective T = 1 Hamiltonian of a single ladder is then given by

H= ( − μ)Tzi2 + tR Txi2 − Tyi2 − h0si Tzi i

+ 2tL

j† i i† j Ozy Ozy + Ozy Ozy ij

+ V−

Tzi Tzj + V+

ij

Tzi2 Tzj2 .

(6.35)

ij

= h0s (−1)i is a longitudinal stagHere is the on-site orbital energy and gered pseudo-spin field that simulates the effect of distortion connected with CO and the coupling to neighboring ladders, ij denotes n.n. rungs along the ladder. Here Ozy = iTz Ty may be interpreted as a quadrupolar operator in the T = 1 pseudo-spin space. Furthermore is the dxy orbital energy and μ, a ‘chemical potential’ to fix the number of holes δ = 1 − n (n = number of d-electrons per rung) at a value determined by the doping. Interaction parameters are defined as V± = 12 (VL ± VD ). If the ladder diagonal term VD is neglected then V± = 12 VL leads to a control parameter λ = 2tR /VL (to stay in accordance with Ref. [253] the inverse value of the previous definition for λ is used here). In isospin language the (staggered) CO parameter δCO and the hole doping δh are given by δCO = Tz1 = −Tz2 , (6.36) δh = 1 − Tz2 . h0s (i)

Here i = 1, 2 denote the two 1D sublattices along the ladder direction b. The selfconsistent mean-field solution of the model is shown in Figure VI.19 (lower panel). Its usefulness relies on the Ising type nature of the ordered state. It shows that close to the QCP λc = 1 the charge order parameter is rapidly suppressed with increasing doping which is also evident from the δh -dependence of the slope shown in the inset. This behavior corresponds qualitatively to the rapid reduction of CO in Na-deficiency doped α -Nax V2 O5 where the spin-gap and hence the associated charge order is suppressed by a few per cent Na-deficiency 1 − x. For small doping one may assume that the latter is equal to the average hole concentration δh in the V-rungs. 253 P. Thalmeier, Physica B 334, 60 (2003).

STRONGLY CORRELATED ELECTRONS

107

F IG . VI.19. Upper panel: Melting of charge order by Na-deficiency (1 − x) (hole) doping seen from the rapid closing of the spin gap in χ(T ) with increasing 1 − x (corresponding nominally to δh ). (After Ref. [251].) Lower panel: Calculated melting of CO with hole doping δh for various λ = 2tR /VL given in decreasing order. The absolute slope value −(dδCO /dδh ) increases strongly when approaching the quantum critical point λc = 1 of CO; this is shown in the inset. (After Ref. [253].)

Finally we briefly discuss the β-vanadium bronzes β-Na0.33 V2 O5 with large but stoichiometric (1 − x = 2/3) Na deficiency doping. Their crystal structure is different but it still contains the Trellis lattice layers. For high temperatures these compounds are 1D metals (only in the stoichiometric case) along the b-axis and

108

P. FULDE ET AL.

exhibit a CDW-instability at TCDW = 136 K into an insulating state.254 While the Wigner-lattice type CO transition discussed for α -NaV2 O5 is due mostly to intersite Coulomb interaction energies of localized 3d electrons, the CDW Fermisurface instability in β-Na0.33 V2 O5 is driven by the kinetic energy of 1D conduction electrons. Under pressure the CDW transition may be suppressed again and around pc 8 GPa the TCDW (p)-line ends in a quantum critical point with an associated superconducting dome around a maximum superconducting Tc of about 10 K. 15. R EENTRANT C HARGE O RDERING AND P OLARON F ORMATION IN D OUBLE E XCHANGE B ILAYER M ANGANITES L A 2−2x S R 1+2x M N 2 O 7 The layered perovskite manganites have been at the center of 3d-oxide research since the discovery of the colossal magnetoresistance effect (CMR).255 Its signature is a change in the resistivity over several orders of magnitude under comparatively small magnetic field changes for doped metallic manganites close to the ferromagnetic phase transition. The investigation of CMR has led to a global survey of doped manganite compounds. Their structures consist of MnO6 octahedra corner-linked to layers that may be stacked in different fashions. As in the cuprates, the parent compounds are AF Mott–Hubbard insulators and hole doping destroys the AF order. However, the metallic state is not superconducting but ferromagnetic. In the manganites the doping with holes only reduces the Mn-moments, rather than creating non-magnetic Zhang–Rice singlets as in the cuprates. The Mn moments then order ferromagnetically via the double exchange (DE) mechanism256,257 that lowers kinetic energy of eg conduction electrons when their spins are aligned with spins of localized Mn-t2g spins (see Figure VI.25). The physics of manganites, especially those derived from the infinite layer parent compound LaMnO3 , has been reviewed in many articles, e.g., Ref. [22]. In this chapter we shall focus exclusively on aspects of the bilayer manganites with half-doped insulating compound LaSr2 Mn2 O7 that are related to charge ordering and possible polaronic effects. In addition we discuss magnetic excitations in the doped metallic ferromagnetic bilayer compounds which give evidence for the double exchange mechanism that is central to the physics of magnetic phases and magnetotransport. This topic has also been more extensively reviewed in 254 K. Okazaki, A. Fujimori, T. Yamauchi, and Y. Ueda, Phys. Rev. B 69, 045103 (2004). 255 Y. Moritomo, Z. Asamitsu, and Y. Tokura, Nature 380, 141 (1996). 256 C. Zener, Phys. Rev. B 82, 403 (1951). 257 P. W. Anderson and H. Hasegawa, Phys. Rev. B 100, 675 (1955).

STRONGLY CORRELATED ELECTRONS

109

F IG . VI.20. Left panel: Crystal structure of LaSr2 Mn2 O7 and La2−2x Sr1+2x Mn2 O7 consisting of MnO6 octahedra and (La,Sr)-cations (circles). Lattice constants are (x = 0.5) a = 3.874 Å, c = 19, 972 Å. The space group is I4/mmm. Right panel: Structural and magnetic phase diagram of bilayer La2−2x Sr1+2x Mn2 O7 in the doping range 0.3 < x < 1.0. Charge order (CO) appears for 0.5 x 0.65. Around x = 0.7 magnetic order is absent. (After Ref. [258].)

Ref. [259]. We first give a brief summary of structural properties. The manganites belong to the Ruddlesden–Popper phases which may be described by intergrowth of rock-salt like MnO slabs and n slabs of the perovskite LaMnO3 . For n = ∞ one has the infinite layer LaMnO3 perovskite, while n = 2 corresponds to the bilayer manganite La2−2x Sr1+2x Mn2 O7 considered here. Its structure is shown in Figure VI.20. In the (hypothetical) compound with x = 0 La and Sr are tri- and divalent cations which implies a Mn3+ (S = 2) state for the magnetic cations. Replacing La by Sr according to the chemical formula La2−2x Sr1+2x Mn2 O7 is equivalent to hole doping and creates Mn4+ (S = 3/2) with a nominal concentration of x holes/Mn site. For x = 0.5 one has a stoichiometric mixed-valent compound LaSr2 Mn2 O7 with a 1:1 ratio of Mn3+ /Mn4+ ions. This suggests the possibility of charge (and orbital) ordering leading to an insulating state. In the possible concentration range 0.2 < x < 1 the crystal structure remains the same although the Mn–O bond lengths depend on x due to the Jahn–Teller distortion of 258 X. Qiu, S. J. L. Billinge, C. R. Kmety, and J. F. Mitchell, cond-mat/0307652 (2003). 259 T. Chatterji, G. Jackeli, and N. Shannon, in Colossal Magnetoresistance Manganites, Kluwer Aca-

demic Publishers (2004), chap. 8, p. 321.

110

P. FULDE ET AL.

the octahedrons containing Mn3+ . The AF (x = 0.5) and FM (x < 0.4) structures are shown later in Figure VI.25. Electronic structure calculations for LaSr2 Mn2 O7 within LSDA+U (see Ref. [260]) lead to a quasi-2D band structure that is close to that of a half metal. The gap between majority and minority spin bands is ↑↓ = 2.7 eV. The influence of possible charge ordering has been neglected in this calculation. Due to the CEF splitting of 3d states into t2g and eg states, the lower lying t2g bands, which are ∼ 1 eV below EF are almost dispersionless while the bands crossing EF have mainly eg character. This allows one to use a simple model for the electronic structure: While the eg electrons are described in a nearest neighbor (n.n.) tight-binding (TB) approximation, the t2g electrons are treated as localized with the intra-atomic exchange aligning their spins to a total spin S (S = 3/2) (see Figure VI.25). Furthermore, there is a Hund’s rule coupling of strength JH which tries to align localized t2g and itinerant eg spins. Finally on-site (U ) and inter-site (V ) Coulomb interaction terms for the eg electrons have to be added. Then one obtains the total Hamiltonian

†

H= tij ciσ cj σ + h.c. + U ni↑ ni↓ + V ni nj ij σ

− JH

i

Si si + J

i

ij

Si Sj .

(6.37)

ij

Here the first three terms describe eg conduction electrons (ciσ ) where niσ = † ciσ ciσ and ni = ni↑ + ni↓ , the fourth term describes FM Hund’s rule coupling (JH > 0) between eg -spins (s) and t2g spins (S) and the last one a superexchange between the localized t2g spins. Note that i = (l, λ) where λ = 1, 2 is the bilayer index and l the site within a layer. The model is able to describe both the charge ordering and magnetism in the manganites. The orbital degree α = 1, 2 of eg electrons is still missing. It is too complex to be solved in full generality, we therefore treat CO and magnetic aspects separately and disregard the possibility of simultaneous orbital order. To investigate charge order as function of the eg band filling n we take into account only the first three terms which constitute an extended Hubbard model (EHM) for the eg electrons. Assuming identical CO in both layers the problem reduces to the EHM on a 2D square lattice. Magnetic order will be suppressed and two-sublattice (A,B) charge order is assumed. In the limit U t > V this model may be treated261 by a combination of Hartree–Fock approximation for the inter-site term (V ) and a CPA approximation for the on-site Hubbard term (U ). 260 P. K. de Boer and R. A. de Groot, Phys. Rev. B 60, 10758 (1999). 261 A. T. Hoang and P. Thalmeier, J. Phys. Condens. Matter 14, 6639 (2002).

STRONGLY CORRELATED ELECTRONS

111

The latter rests on the alloy-analogy, i.e., the EHM is replaced by a single-particle Hamiltonian with diagonal (sites 1,2 within each layer) disorder of eg orbital en(1,2) (1,2) ergies EA/Bσ and corresponding probabilities pA/Bσ on each sublattice. Accordingly, (1)

EA/Bσ = zV nA/B (2)

(1)

with pA/Bσ = 1 − nA/B−σ

EA/Bσ = zV nA/B + U

(2)

with pA/Bσ = nA/B−σ .

(6.38)

The Green’s functions of the equivalent single-particle Hamiltonian is then configuration averaged within CPA, i.e., requiring the average T -matrix of the system to vanish. This leads to averaged Green’s functions tk2 ¯ A/B (k, ω) = ω − A/B (ω) − (6.39) G ω − B/A (ω) where tk = (t/2)(cos kx + cos ky ). The corresponding self-energies are given by ¯ A/B (ω) zV NB/A A/B (ω) = E¯ A/B − zV nB/A − A/B (ω) G + U − A/B (ω) . (6.40) Here E¯ A/B = zV nB/A + 12 U nA/B are the effective orbital energies on A/B sublattices. On the bipartite lattice CO has to be symmetric which leads to the restriction nA/B = n ± nCO . This requires only a single averaged Green’s function defined ¯ A/B (ω). From the above equations the self energies may be by G(±nCO , ω) = G eliminated. One obtains a cubic equation for G from which the order parameter nCO may be calculated as function of filling n and Coulomb interaction parameters U, V by requiring charge conservation. Setting nCO = 0 the phase boundary between CO and homogeneous phase is obtained as a surface in (n, U, V ) space. It is obtained as an implicit solution of the equations 2 n=− dω f (ω) Im G(0, ω) and π 2 (6.41) dω f (ω) Im G (0, ω) 1=− π where the derivative is defined as G (ω) = ∂G(nCO , ω)/∂nCO |nCO =0 and f (ω) is the Fermi function. The self-consistent solution for charge order has been determined for the 2D square lattice (z = 4 and W = 4t = half bandwidth). The resulting n–V and V –T phase diagrams for CO are shown in the left and right part of Figure VI.21 respectively. In the n–V phase diagram we notice two regions. For n < n∗ ∼ 0.67 the CO boundary Vc (n) is almost independent of U while for n > n∗ when the half filled case n = 1 is approached CO is strongly suppressed with increasing U . This is due to the fact that in a Mott–Hubbard in-

112

P. FULDE ET AL.

F IG . VI.21. Left: n–V phase diagram of charge order (CO) for the 2D EHM (T = 0, W = 4t ≡ 1) and U = 0, 0.5, 1.5, ∞ corresponding to dotted, long-dashed, dashed and solid lines respectively. Right: V –T phase diagram of CO for U = 2 and various band filling n = 0.3, 0.5, 0.65 and 0.8 corresponding to solid, dash-dotted, dotted and dashed curves respectively. The CO regime is to the right of the boundary for each value of n. Energies and temperature are given in units of t . (After Ref. [261].)

sulator charge fluctuations are already strongly suppressed and additional spatial symmetry breaking CO then needs a larger threshold value Vc . On the other hand for n < n∗ , e.g., quarter filling n = 1/2 the Vc ∼ 0.25W = t is determined essentially by the hopping t. The minimum Vc where CO is most easily achieved is obtained around n = n∗ . The V –T phase diagram shows an interesting aspect: For each value of U a range of V values exists for which the CO transition is reentrant as function of temperature. For such a V value the ground state is homogeneous while CO appears in an intermediate temperature range. This behavior cannot be obtained by treating the EHM in Hartree–Fock approximation and thus it is a genuine correlation effect. However, as we shall see, another mechanism based on polaron formation may also lead to reentrant CO. In the present model the absolute value of transition temperatures is unrealistically large because only the n.n. interaction V is assumed. This may be improved by including also a competing n.n.n. Coulomb repulsion which reduces the CO temperature as shown later. The predicted phase diagram of charge order qualitatively agrees with experimental observations, keeping in mind that due to electron–hole symmetry the calculated phase diagram can be used for the hole doped case of La2−2x Sr1+2x Mn2 O7 (x = 1 − n). One must note however that there is no unanimous agreement on doping range and temperature behavior of CO in this compound. Both depend considerably on the experimental method used to detect CO, e.g., X-ray, electron diffraction or transport measurements. In the latter case one

STRONGLY CORRELATED ELECTRONS

113

F IG . VI.22. Structure of charge and orbital order in stoichiometric (x = 0.5) LaSr2 Mn2 O7 corresponding to wave vector Q = ( 14 , 14 , 0). (After Ref. [262,263].)

finds CO in a broad range of doping (0.44 x 0.8) at TCO ∼ 200 K.264 Another observation is the collapse of CO or reentrance of the homogeneous phase at lower temperatures. Surprisingly a second reentrance of CO appears below 50 K as concluded from an upturn in the resistivity. From diffraction experiments the doping range of CO is somewhat smaller (0.5 x 0.65).258 For the stoichiometric case x = 0.5 (Mn3+ /Mn4+ = 1) the CO has first been observed in Ref. [262] by X-ray diffraction. If one had only CO one would expect a simple two-sublattice structure with Mn3+ /Mn4+ ordering corresponding to a commensurate superstructure with Q = ( 12 , 12 , 0). However one rather observes Q = ( 14 , 14 , 0). This is due to additional orbital ordering of Mn3+ eg orbitals in a staggered fashion (d3x 2 −r 2 /d3y 2 −r 2 ) on top of CO (see Figure VI.22). The Q = ( 14 , 14 , 0) superlattice reflexions are then due to the associated JT distortion of the crystal structure. The additional orbital order is not contained in the above single-orbital model. Below 100 K the superstructure reflections vanish, indicating melting of both CO and orbital order as conjectured from transport.264 Later X-ray experiments on LaSr2 Mn2 O7 (x = 0.5) have shown that there is also evidence for a CO reentrance below 50 K (see Ref. [265]) in agreement with Ref. [264]. This evidence for the second (CO) reentrance is seen in Figure VI.23. The intensity of reflexions in the reentrant CO region below 50 K is however much smaller, indicating much weaker CO. In fact, it seems sample dependent since it was not observed in other experiments. The possible existence of the second CO reentrance cannot be 262 T. Kimura, R. Kumai, Y. Tokura, J. Q. Li, and Y. Matsui, Phys. Rev. B 58, 11081 (1998). 263 Y. Wakabayashi, Y. Murakami, I. Koyama, T. Kimura, Y. Tokura, Y. Moritomo, Y. Endoh, and

K. Hirota, J. Phys. Soc. Jpn. 72, 618 (2003). 264 J. Dho, W. S. Kim, H. S. Choi, E. O. Chi, and N. H. Hur, J. Phys. Condens. Matter 13, 3655 (2001). 265 T. Chatterji, G. J. McIntyre, W. Caliebe, R. Suryanarayanan, G. Dhalenne, and A. Revcolevschi, Phys. Rev. B 61, 570 (2000).

114

P. FULDE ET AL.

F IG . VI.23. Temperature variation of superlattice reflexion intensities in LaSr2 Mn2 O7 corresponding to wave vector Q = ( 14 , 14 , 0) (cf. inset of Figure VI.24). Right: CO and first reentrance of homogeneous state. Left: second possible reentrance of CO below 50 K. (After Ref. [265].)

explained by the purely electronic EHM model. In fact around x = 1 − n∗ there is not even the first reentrance found to the homogeneous phase. Instead the charge order parameter increases monotonously with decreasing temperature as may be inferred from the V –T phase diagram (n = 0.65) in Figure VI.21. We note that Mn3+ /Mn4+ charge order has also been observed in the infinitelayer manganites, typically around the half-doped (x = 0.5) compounds, e.g., in La0.5 Ca0.5 MnO3 and R0.5 Sr0.5 MnO3 (R = Pr, Nd). For the Pr-compound CO was observed in a large doping range (0.3 x 0.7) similar as in the bilayer La2−2x Sr1+2x Mn2 O7 . The reentrance into the homogeneous phase was also observed in Pr0.5 Sr0.5 MnO3 , again only away from half doping (x = 0.5). It becomes especially pronounced in the presence of magnetic fields up to 10 T.266 There is no evidence for a second CO reentrance in the infinite layer compounds. To explain these phenomena in the stoichiometric bilayer LaSr2 Mn2 O7 a more extended but still single-orbital based theory is apparently needed. It was proposed in Ref. [267] that in this case CO is profoundly affected by polaron formation caused by a strong coupling to the lattice. This is suggestive since polaron formation changes the ratio of kinetic vs. intersite Coulomb energy of the holes and thus affects the conditions of CO. The electron–lattice coupling is due to the modulation of pd-hybridization along the in-plane bond directions caused by vibrations of oxygen atoms that form corner-sharing octahedra around the Mn ions. 266 Y. Tomioka, A. Asamitsu, H. Kuwahara, Y. Moritomo, and Y. Tokura, Phys. Rev. B 53, R1689

(1996). 267 Q. Yuan and P. Thalmeier, Phys. Rev. Lett. 83, 3502 (1999).

STRONGLY CORRELATED ELECTRONS

115

Effectively this leads to a coupling of the Mn3+ -eg level shift to a bond-stretching vibration of the oxygen. The latter may be assumed dispersionless with a frequency ω0 . We note that this refers to conventional Holstein-type polarons. They differ from the Jahn–Teller (JT) type polarons where the eg level is split by coupling to the JT symmetry distortions of the whole oxygen octahedron. The latter have been proposed for the slightly doped infinite layer La1−x Srx MnO3 in the region 0.1 x 0.2.268 The present Holstein-type model for the x 0.5 bilayer LaSr2 Mn2 O7 is described by

† † He−ph = g bi,δ + bi,δ (ni+δ − ni ) + ω0 bi,δ bi,δ . (6.42) i,δ

i,δ

† bi,δ

is the local vibration at oxygen site δ associated with Mn site i and g Here is the coupling constant. This has to be added to the EHM part, i.e., to the first three terms of Eq. (6.37). The latter is also generalized by including both n.n. interactions (V1 ) and n.n.n. interactions (V2 ) to achieve a realistic TCO which is controlled by the ratio (V1 − V2 )/t. In the limit of strong coupling (α ≡ g 2 /ω02 ∼ 1) the phonon coordinates may be eliminated by a combined Lang–Firsov (LF) transformation

† (ni+δ − ni ) g/ω0 bi,δ − bi,δ U1 = exp − i,δ

(see Ref. [269]), and squeezing transformation

† † U2 = exp γ bi,δ bi,δ − bi,δ bi,δ . i,δ

Here γ > 0 is a variational parameter270 determined by minimization of the ground-state energy. This leads again to an effective electronic model, but with renormalized hopping and interaction parameters. Furthermore, the on-site correlation problem is simplified by using the limit U → ∞ where the layers are fully spin polarized and we may assume spinless fermions. For x = 0.5 this implies the spinless half-filled band is realized in LaSr2 Mn2 O7 . Then, after applying U2 U1 the effective Hamiltonian reads, up to a constant,

†

Heff = −t˜ ci ci+δ + h.c. + (V1 + 2αω0 ) ni ni+δ i,δ

+ V2

i,δ

ni ni+η .

i,η 268 Y. Yamada, O. Hino, S. Nohdo, and R. Kanao, Phys. Rev. Lett. 77, 904 (1996). 269 I. G. Lang and Y. A. Firsov, Sov. Phys. JETP 16, 1301 (1963). 270 H. Zheng, Phys. Rev. B 37, 7419 (1988).

(6.43)

116

P. FULDE ET AL.

The first term describes hopping of small polarons. The essential point is that the effective hopping element t˜ = t exp[−5ατ coth(ω0 /2T )] with τ = exp(−4γ ) is strongly temperature dependent. It is small compared to the bare hopping t when T ω0 and increases for T ω0 because the occupation of the n-phonon modes decreases with T eventually until only the effect of zero-point fluctuations in t˜ is left. This T -dependent renormalization of t˜ is very important for charge ordering to take place, since the latter is determined by the balance of kinetic and intersite Coulomb energies. Treating the intersite Coulomb terms for two sublattices A,B in Hartree–Fock approximation as before and choosing ni = 1/2 ± nCO , i ∈ A, B, the condition for the CO instability line is 2V 1 tanh[2 (t˜z)2 + (V nCO )2 /T ] K( 1 − z2 ) dz (6.44) 1= 2 π 0 (t˜z)2 + (V nCO )2 where K is the complete elliptic function of the first kind and z = ε 2 − (4V nCO )2 /4t˜ with V = V12 + 2αω, V12 = V1 − V2 . For T → 0 this equation has always a solution with nCO > 0. For a reasonable parameter set (t, ω0 , V12 ) its solution leads to the α–T phase diagram shown in Figure VI.24. Depending on the size of α, both the non-reentrant and double-reentrant scenarios are possible. There is an intermediate region for α ∼ 0.65 where on lowering the temperature one obtains

F IG . VI.24. α–T phase diagram for the spinless (half-filled) case of the Holstein–EHM model with parameters V12 = 0.1, ω0 = 0.05 in units of t = 4 · 103 K. For comparison, the thin line corresponds to a t˜ which is kept constant (cf. Figure VI.23). The inset shows nCO (T ). The dotted, solid and dashed lines correspond to the three possible types of diagrams with α = 0.60, 0.65 and 0.68 respectively. (After Ref. [267].)

STRONGLY CORRELATED ELECTRONS

117

a CO phase, then a first reentrance into the homogeneous phase and subsequently a second reentrance into the CO phase. The corresponding variation of the order parameter nCO (T ) is shown in the inset of Figure VI.24 (full line). The other possible cases are also illustrated. Physically the behavior around α ∼ 0.65 may be explained as follows. First the effective hopping t˜ is reduced from the bare value and polaronic CO appears at relatively high temperatures. With decreasing temperature the kinetic energy (∼ t˜) increases until CO can no longer be maintained and the homogeneous state is stable again. For even lower temperatures CO always reappears because the n.n. tight binding Fermi surface has a nesting instability to CO for the half filled (spinless) case for arbitrary small values of V . The reentrance behavior discussed here is entirely due to the temperature dependence of the effective polaron hopping t˜ = t exp[−5ατ coth(ω/2T )]. Without it only the lowest CO transition does occur. This agrees with the previous study where no reentrance was observed for quarter filling including spin or spinless half filling. In the discussion of the reentrance behavior in La2−2x Sr1+2x Mn2 O7 we have so far invoked electronic correlation effects and polaron formation as origin but neglected the influence of coexisting magnetic order. A treatment of the full problem of CO would require the inclusion of spin degrees of freedom for finite values of U together with the last two exchange terms in Eq. (6.37) and the electron–lattice coupling. This is still an open problem. In the last part of this chapter we therefore focus on a rather complementary case: When the doping is large enough Coulomb correlation effects are less prominent and CO is absent for all temperatures. Then only the exchange terms in Eq. (6.37) are important. Double exchange (DE) illustrated in Figure VI.25 favors FM order within and between layers by optimizing kinetic energy gain for parallel eg (s = 1/2) conduction and t2g (S = 3/2) localized spins. In contrast superexchange (last term in Eq. (6.37)) favors AF orientation of moments between layers leading to the AF order in Figure VI.25 for x = 0.5. For 0.4 < x < 0.5 its competition with FM double exchange along the c-axis leads to a canting of moments out of the plane271 (CAF region in Figure VI.20) which may be interpreted as a superposition of an AF and FM structure. For x 0.4 the eg conduction bands become increasingly two-dimensional with d3z2 −r 2 character. Therefore double exchange along c increases significantly as discussed below. Consequently only the FM structure with FM bilayers remains and the last term in Eq. (6.37) may be neglected. The less than half-doped (x 0.4) metallic La2−2x Sr1+2x Mn2 O7 compounds are then described by the ferromagnetic (JH > 0) Kondo-lattice Hamil271 K. Hirota, S. Ishihara, H. Fujioka, M. Kubota, H. Yoshizawa, Y. Moritomo, Y. Endoh, and S. Maekawa, Phys. Rev. B 65, 64414 (1998).

118

P. FULDE ET AL.

F IG . VI.25. Left: AFM structure of stoichiometric (x = 0.5) CO insulator LaSr2 Mn2 O7 consisting of AF stacked FM layers along c. Right: FM structure of metallic (x = 0.4) La2−2x Sr1+2x Mn2 O7 . Moments are parallel to [110] in both cases. Center: Illustration of FM double exchange mechanism in doped manganites. FM polarization of itinerant eg spins (s = 1/2) leads to kinetic energy gain (∼ t ) due to FM Hund’s rule coupling (∼ JH ) to localized t2g spins (S = 3/2).

tonian HK = −t

† ciλα cj λα − t⊥

ij λα

− JH

† ci1α ci2α + h.c. iα

† Siλ · ciλα sαβ ciλβ .

(6.45)

iλαβ

Here t, t⊥ > 0 are the nearest neighbor hopping parameters within a layer and between the two partners (λ = 1, 2) of a bilayer along c respectively. Furthermore S and s are localized and conduction electron spins respectively with α, β =↑, ↓. In La2−2x Sr1+2x Mn2 O7 the lattice constants (x = 0.4) are a = 3.87 Å and c = 20.14 Å. The intra-bilayer splitting d a is much smaller than the distance D = 6.2 Å between adjacent bilayers (Figure VI.20). Therefore inter-bilayer hopping or exchange has been neglected above. Diagonalization of the hopping term leads to bonding and antibonding tight binding bands split by t⊥ with identical in-plane dispersion and a DOS given by σ ± (k) = − ±t⊥ + t (cos kx + cos ky ) N± () = N ( ± t⊥ );

2 1 2 2 1 N () = 2 K 1 − . W π W

(6.46)

The justification for this model and the size of its parameters can be obtained by considering the spin wave excitations below the Curie temperature TC . They have

STRONGLY CORRELATED ELECTRONS

119

been investigated by inelastic neutron scattering by various groups271–274 and analyzed in Refs. [275,276] both in the classical limit and with quantum corrections. In the manganites the condition JH t, t⊥ is fulfilled because the Hund’s rule coupling JH ∼ 2 eV is quite large. This greatly simplifies spin wave calculations because firstly the eg bands σ ± (k) will be spin-split such that only majority bands are occupied, i.e., n↑± = 1 and n↓± = 0 and secondly the large S = 3/2 local t2g spins allow for a 1/S expansion. This approach has been first applied to the cubic manganites277 and later used for the bilayer manganites.275,276 It turns out that in the limit JH → ∞, and to order 1/S one obtains classical spin waves of an effective Heisenberg model for t2g spins. The effective exchange constants are determined by the eg conduction band dispersion and filling. One obtains ωA (q) = zJ DE S[1 − γq ] ωO (q) = zJ DE S[1 − γq ] + 2J⊥DE S.

(6.47)

In two dimensions γq = 12 (cos qx + cos qy ) and ωA (q) and ωO (q) are the dispersion of acoustic (A) and optical (O) spin wave branches respectively. They have equal dispersion in the ab-plane and are split by the A-O gap AO = 2SJ⊥DE . In this approximation there is no spin-space anisotropy and therefore the A branch has no gap at k = 0. The effective Heisenberg exchange constants J DE , J⊥DE for t2g spins are given by F ±t⊥ 1 1 J DE = − 2 (0 + π ) with 0,π = N () d 2S 2z −W F ±t⊥ 1 t⊥ J⊥DE = 2 (n0 − nπ ) with n0,π = N () d. (6.48) 2S 2 −W The effective t2g exchange parameters J DE , J⊥DE termined by the eg band parameters in the limit simple result for the spin waves in the double good agreement with inelastic neutron scattering

are therefore completely deJH → ∞. This surprisingly exchange ferromagnet is in experiments on the x = 0.4

272 T. Chatterji, P. Thalmeier, G. J. McIntyre, R. van de Kamp, R. Suryanarayanan, G. Dhalenne, and

A. Revcolevschi, Europhys. Lett. 46, 801 (1999). 273 T. Chatterji, L. P. Regnault, P. Thalmeier, R. Suryanarayanan, G. Dhalenne, and A. Revcolevschi, Phys. Rev. B 60, R6965 (1999). 274 T. G. Perring, D. T. Adroja, G. Chaboussant, G. Aeppli, T. Kimura, and Y. Tokura, Phys. Rev. Lett. 87, 217201 (2001). 275 T. Chatterji, L. P. Regnault, P. Thalmeier, R. van de Kamp, W. Schmidt, A. Hiess, P. Vorderwisch, R. Suryanarayanan, G. Dhalenne, and A. Revcolevschi, J. Alloys Compounds 326, 15 (2001). 276 N. Shannon, T. Chatterji, F. Ouchni, and P. Thalmeier, Eur. Phys. J. B 27, 287 (2002). 277 N. Furukawa, J. Phys. Soc. Jpn. 65, 1174 (1996).

120

P. FULDE ET AL.

F IG . VI.26. Left panel: Acoustic and optic spin wave branches along [100] direction with a splitting AO = 6 meV and overall dispersion of 40 meV. Full lines are obtained from the classical dispersion expression in Eq. (6.47). Right panel: Acoustic spin wave dispersion along [001]. An extrapolated anisotropy gap A (0) = 0.04 meV is obtained. (After Ref. [275].)

La2−2x Sr1+2x Mn2 O7 . This is seen in the left panel of Figure VI.26. Two parallel A and O modes are observed with a maximum zone-boundary energy of ωA (qx = πa ) ∼ 40 meV and an A-O splitting of AO = 6 meV. From these values one obtains SJ DE = 10 meV and SJ⊥DE = 3 meV. Using Eqs. (6.48) this leads to eg band parameters t = 0.175 meV and t⊥ = 0.1 eV. In the present theory there is no double exchange between adjacent bilayers and hence no spinwave dispersion along the c-axis. But experimentally a small dispersion along c was found (Figure VI.26, right panel) although it is two orders of magnitude smaller than the one along the a-axis. This requires an inter-bilayer DE constant J⊥DE with J⊥DE /J⊥DE 1.5 · 10−2 (see Ref. [272]) and shows that La2−2x Sr1+2x Mn2 O7 is an almost ideal two dimensional double exchange ferromagnet. This conclusion was supported by an analysis of diffuse neutron scattering which exhibits long range FM in-plane correlations far above the Curie temperature (∼ 2.3TC ).278 Finally, Figure VI.26 shows that a small extrapolated anisotropy gap A (0) ∼ 0.04 meV for the acoustic mode exists at the zone center whose microscopic origin is not clear. The double exchange model based on the FM Kondo lattice Hamiltonian is able to describe ferromagnetism and basic properties of spin wave excitations quite well. However it has its limits. Firstly quantum corrections of order 1/S 2 can278 T. Chatterji, R. Schneider, J. U. Hoffmann, D. Hohlwein, R. Suryanarayanan, G. Dhalenne, and A. Revcolevschi, Phys. Rev. B 65, 134440 (2002).

STRONGLY CORRELATED ELECTRONS

121

not be completely neglected as discussed in Refs. [259,276] and references cited therein. They lead to two effects: (i) reduction of the overall dispersion of spin waves. In the effective Heisenberg model this would necessitate a rescaling of the parameters J DE , J⊥DE or possibly an inclusion of more parameters; (ii) the local spin moment is coupled to density fluctuations in the itinerant system which leads to damping effects not present in the classical (1/S) approximation. Comparison with experiment shows that (1/S 2 ) corrections provide still insufficient damping and also cannot explain the observed deviations from the classical q-dependence of spin waves.276 It has also been proposed that a crossing with a phonon branch might be involved in these anomalies. Another shortcoming of the model is the neglect of orbital degeneracy of eg states. This has indeed dramatic effects on the doping dependence of the A-O spin wave splitting and the resulting effective exchange constants in the FM regime x = 0.3–0.4 as shown in Ref. [274]. When x decreases from the present value x = 0.4 the effective J⊥DE strongly increases while J DE stays almost constant. In the above double exchange model the anisotropy ratio is given by

J⊥DE t⊥ W (n0 − nπ ) = − . (6.49) DE J t 0 + π Assuming a doping independent t⊥ /t the above ratio changes at most by ∼ 10% in the doping range x = 0.3–0.4, which is much too small to explain experimental observations. Therefore another mechanism must be invoked. It has been found279 that for decreasing x the MnO6 octahedra elongate significantly along the c axis due to the JT effect on eg orbitals which leads to a lower energy and hence larger occupation for d3z2 −r 2 orbitals as compared to dx 2 −y 2 orbitals. Since the former have larger overlap along the c axis, the effective t⊥ strongly increases with decreasing x. Thus it is really the prefactor (t⊥ /t) in the above equation which leads to the dramatic increase of J⊥DE and the A-O spin wave splitting with decreasing x. This effect was described phenomenologically in Ref. [276] and within a microscopic model in Ref. [280]. In our discussion of bilayer manganites we have focused on models for charge ordering which can be described as simple periodic superstructures caused by inter-site but short range Coulomb interactions supplemented by small polaron formation. We have also discussed the importance of the double exchange mechanism for explaining the spin excitations in the metallic ferromagnet away from half-doping. We have mostly neglected the complications of orbital order, JT distortions and the effect of longer range Coulomb interactions in the low doping 279 M. Kubota, H. Fujioka, K. Hirota, K. Ohoyama, Y. Moritomo, H. Yoshizawa, and Y. Endoh, J. Phys. Soc. Jpn. 69, 1606 (2000). 280 G. Jackeli and N. B. Perkins, Phys. Rev. B 65, 212402 (2002).

122

P. FULDE ET AL.

DE F IG . VI.27. Upper panel: Doping dependence of effective exchange parameters. Note that J⊥ is proportional to A-O spin wave splitting and J DE to the overall dispersion. Lower panel: Doping dependence of JT distortion JT (elongation along c) of MnO6 octahedra. (After Ref. [274].)

regime. This may lead to the important possibility of an inhomogeneous state due to phase separation of ferromagnetic metallic and charge ordered insulating regions. Such states may consist of metallic droplets or stripes of holes in an insulating environment. This possibility has been reviewed in Ref. [281]. These aspects may also be of great importance for explaining the giant magnetoresistance of the manganites.22 VII. Geometrically Frustrated Lattices

Usually the concept of frustration is used in connection with magnetic systems. When Ising spins with an antiferromagnetic interaction are placed onto certain lattices like a triangular one, the pair-wise interactions cannot be satisfied simultaneously and therefore are frustrated. Here we will associate the concept of frustration with lattice structures. We call a lattice geometrically frustrated when in case that its sites are occupied by antiferromagnetically coupled Ising spins the interactions are frustrated. Examples are in two dimensions the just mentioned triangular, the checkerboard or the Kagomé lattice. In three dimensions the pyrochlore lattice (see Figure VII.1) is the one most frequently investigated. For those lattices we want to study charge degrees of freedom, i.e., when the electron number at a lattice site is fluctuating. A frustrated 281 A. Moreo, S. Yunoki, and E. Dagotto, Science 283, 2034 (1999).

STRONGLY CORRELATED ELECTRONS

123

F IG . VII.1. Pyrochlore lattice consisting of corner-sharing tetrahedra.

lattice structure can have a degenerate ground state for special band fillings when electron correlations are strong. In fact, in the limit of large on-site and nearest-neighbor electron repulsions there exists an exponentially large number of configurations with minimal potential energy. This is particularly so when the number of electrons equals half the number of lattice sites. It is not surprising that this special feature which is closely related to a frustrated geometry leads to new theoretical models and special effects when the electrons are strongly correlated. In the center of our attention will be the above mentioned pyrochlore lattice and a two-dimensional projection of it, the checkerboard lattice. A pyrochlore lattice is a substructure of the spinels which have the composition AB2 O4 . They can be considered as face-centered cubes of O2− ions. The B ions are surrounded by an octahedron of O2− ions, i.e., BO6 and are positioned on corner-sharing tetrahedra which define the pyrochlore lattice. Here we want to consider metallic spinels in which the electrons are itinerant. They may undergo metal to insulator transitions which are usually accompanied by a structural distortion. The most studied example has been magnetite Fe3 O4 . A transition to an insulator already indicates that electron correlations may be strong in spinels but an unambiguous proof is the observed heavy-fermion behavior of LiV2 O4 at low temperatures.282 Another interesting case is AlV2 O4 . This material is either a poor metal or a semiconductor at low temperatures. It undergoes a structural phase transition at lower temperatures which apparently is caused by strong electron correlations. Finally, LiTi2 O4 is a metallic spinel which becomes supercon282 S. Kondo, D. C. Johnston, and L. L. Miller, Phys. Rev. 59, 2609 (1999).

124

P. FULDE ET AL. TABLE VII.1. S PINELS WITH A H ALF -I NTEGER VALENCY OF d I ONS M=

Li(Al)M2 O4

Ti

V

V(Cr)

Mn

LiTi2 O4

LiV2 O4

AlV2 O4

LiMn2 O4

(LiCr2 O4 ) average d-electron count per M-atom

d0.5

d1.5

d2.5

d3.5

ducting at a relatively high transition temperature of Tc = 13.7 K.283,284 Table VII.1 summarizes these materials with half-integer valency of the cations. In the following we start out with a reminder on Fe3 O4 for which a huge literature does exist. For references see, e.g., Ref. [285]. The purpose is to merely recall some of the basic facts in order to understand better the special features of strong electron correlations in LiV2 O4 , AlV2 O4 and other spinels. This is followed by a discussion of fractional charges. They are found when a model Hamiltonian describing strongly correlated electrons with strong on-site and nearest-neighbor repulsions is used and applied to a frustrated lattice. Magnetite Fe3 O4 has been much investigated because of the important role it has played in the development of magnetism and magnetic materials. It is a spinel of the form AB2 O4 with A = Fe3+ and B = Fe2.5+ sites. We assume that 50% of the B sites are in a Fe2+ and Fe3+ configuration each, i.e., that electron correlations are so strong that Fe+ or Fe4+ configurations are suppressed. Magnetite undergoes at 120 K a phase transition from a metallic high-temperature phase to an insulating low-temperature phase. This transition was first observed by Verwey and Haayman8 and is usually referred to as Verwey transition. Verwey presented also a model for its description in terms of an order-disorder transition, which is entropy driven. The implicit assumption regarding B sites is thereby that the repulsions of electrons on neighboring sites are so strong that the kinetic energy term of the electrons plays only a minor role and may be neglected when the phase transition is considered. With an average valence of the B sites of +2.5 this implies that two neighboring Fe2+ sites and also two Fe3+ sites repel each other, while Fe2+ –Fe3+ sites attract. Let us denote by Vαβ the interaction between two neighbors Feα+ –Feβ+ . An order-disorder phase transition will take place when δV = V33 + V22 − 2V23 > 0.

(7.1)

Verwey suggested a particular charge ordering for the insulating low-temperature phase in which the Fe2+ and Fe3+ sites of the pyrochlore lattice order in form of 283 D. C. Johnston, J. Low Temp. Phys. 25, 145 (1976). 284 R. W. McCallum, D. C. Johnston, C. A. Luengo, and M. B. Maple, J. Low Temp. Phys. 25, 177

(1976). 285 M. Isoda and S. Mori, J. Phys. Soc. Jpn. 69, 1509 (2000).

STRONGLY CORRELATED ELECTRONS

125

two families of chains pointing in the [110] and [110] direction, respectively. However, the situation is more complicated than that. First one should realize that in the absence of electron hopping the ground state is highly degenerate. In order to minimize the Coulomb interactions Vαβ , two of the sites of each tetrahedron of the pyrochlore structure must be occupied by a Fe2+ and two by a Fe3+ ion (tetrahedron rule). There is an exponentially large number of different configurations which satisfy this rule.286 When a small hopping of electrons is taken into account this degeneracy is partially lifted. How that is taking place remains an unsolved problem. It is possible that the electronic ground state would remain disordered, i.e., liquid like as long as the lattice is unchanged. In that case charge order could result from a structural distortion which is accompanying the metal-insulator transition. Indeed, the experimental determination of the electronic low-temperature phase has been a challenging and controversial subject as has been a proper theoretical interpretation. A recent review287 describes the development of different theoretical models starting from a Hubbardlike Hamiltonian including nearest-neighboring repulsions288 up to inclusion of electron–phonon interactions together with the tetrahedron rule.289 Calculations in the frame of density functional theory based on LDA+U and the observed low temperature lattice structure produce charge order which agrees with estimates based on a valence bond analyses.290 They also conclude that the tetrahedron rule is not strictly fulfilled. This is due to the kinetic energy, i.e., electronic hopping terms which lead to violations of that rule. Nevertheless, for a simple reason the tetrahedron rule must be satisfied to a high degree. Without considerable short-range order it would be difficult to understand the relatively low transition temperature of the Verwey transition. For a conventional order– disorder phase transition the transition temperature is given by TV = 2δV /kB , where kB is Boltzmann’s constant. This would imply a TV of several thousands of Kelvin.286 16. M ETALLIC S PINELS : L I V 2 O 4 — A M ETAL WITH H EAVY Q UASIPARTICLES In order for a spinel oxide to be conducting, the electron count of the B ions in AB2 O4 should differ from an integer number. The compounds listed in Ta286 P. W. Anderson, Phys. Rev. 102, 1008 (1956). 287 F. Walz, J. Phys. Cond. Matt. 14, R285 (2002). 288 J. R. Cullen and E. Callen, J. Appl. Phys. 41, 879 (1970). 289 D. Ihle and B. Lorenz, Phil. Mag. 42, 337 (1980). 290 I. Leonov, A. N. Yaresko, V. N. Antonov, M. A. Korotin, and V. I. Anisimov, Phys. Rev. Lett. 93,

146404 (2004).

126

P. FULDE ET AL.

ble VII.1 are therefore of special interest. As mentioned before LiTi2 O4 with d 0.5 per Ti ion is a superconductor with a transition temperature of Tc = 13.7 K. LiV2 O4 with d 1.5 per V ion is a metal with heavy quasiparticle excitations. At ambient pressure no spin- or charge order has been observed down to the lowest temperature. The compound LiCr2 O4 is not stable and therefore AlV2 O4 with d 2.5 per V ion is particularly interesting. This system becomes a charge ordered insulator by so-called valence skipping (see the next section). Finally LiMn2 O4 with d 3.5 per Mn ion is an antiferromagnetic insulator with a Néel temperature of TN = 280 K. Charge ordering is taking place in that material which has been used in batteries. In the following we will discuss LiV2 O4 in more detail. As pointed out above LiV2 O4 shows at low temperatures heavy-fermion behavior, i.e., it supports heavy quasiparticle excitations.282,291 It has been the first system where the heavy quasiparticles originate from d electrons. Experiments show that the γ coefficient of the low temperature specific heat C = γ T is strongly enhanced and of order γ 0.4 J mol−1 K−2 . The spin susceptibility is equally enhanced at low T . Over a large temperature regime it shows a behavior χS = χ0 +

C , T +

= 63 K

(7.2)

i.e., of Curie–Weiss type. The Sommerfeld–Wilson ratio RW = πkB2 χS (T = 0)/(3μ2B γ ) is found to be RW = 1.7. The temperature independent term χ0 = 0.4 · 10−4 cm3 /mol and the Curie constant is C = 0.47 cm3 K/(mol V). The sign of indicates antiferromagnetic interactions between V sites but no magnetic ordering was found down to 4.2 K. In view of the frustrated lattice this is understandable. The resistivity is found to be ρ(T ) = ρ0 + AT 2 with a large coefficient A = 2μ cm K−2 . The Kadowaki–Woods ratio A/γ 2 ,292 a hallmark of heavy quasiparticles is in the range of other heavy-quasiparticle materials.293 These findings are typical signatures of heavy fermion systems. From the specific heat data one may determine the entropy S(T ). One finds that S(T = 60 K) − S(T = 2 K) = 10 J/(mol · K) which is close to 2R ln 2 where R is the gas constant. The implication is that at 60 K the system has almost one excitation per V ion. This is inconceivable with a conventional band description of the d electrons. According to Pauli’s principle only a small fraction of them is participating in the excitations 291 S. Kondo, D. C. Johnston, C. A. Swenson, F. Borsa, A. V. Mahajan, L. L. Miller, T. Gu, A. I. Goldman, M. B. Maple, D. A. Gajewski, Phys. Rev. Lett. 78, 3729 (1997). 292 K. Kadowaki and S. B. Woods, Solid State Comm. 58, 507 (1986). 293 C. Urano, M. Nohara, S. Kondo, F. Sakai, H. Takagi, T. Shiraki, and T. Okubo, Phys. Rev. Lett. 85, 1052 (2000).

STRONGLY CORRELATED ELECTRONS

127

F IG . VII.2. Energy bands for electrons in a pyrochlore lattice with one orbital per site in the presence of nearest neighbor hopping. The upper flat band is two-fold degenerate. (After Ref. [285].)

when a one-electron picture is applied. Calculations based on the LDA show that the electrons near the Fermi energy have t2g character.294–296 These states are well separated from the eg states as well as from the oxygen states (see Figure VII.3). The width of the t2g bands is of order 2 eV and therefore at 60 K only a small fraction of the electrons in t2g states would contribute to the excitations. In fact, the calculated density of states must be multiplied by a factor of 25 in order to account for the large γ value. This provides convincing evidence for strong electron correlations in LiV2 O4 . Further support is given by the observation that the material undergoes a phase transition into a charge ordered state at approximately 6 GPa.297,298 Presumably this metal–insulator transition is again accompanied by a structural distortion as in Fe3 O4 . It is worth pointing out that the band structure of a pyrochlore lattice has interesting features, which are simple to derive when only nearest-neighbor hopping is taken into account. The Hamiltonian of noninteracting electrons with nearestneighbor hopping t is given in diagonal form by

† α (k) − μ akασ akασ (7.3) H0 = kασ

294 J. Matsuno, A. Fujimori, and L. F. Mattheiss, Phys. Rev. B 60, 1607 (1999). 295 D. J. Singh, P. Blaha, K. Schwarz, and I. I. Mazin, Phys. Rev. B 16, 359 (1999). 296 V. Eyert, K.-H. Höck, S. Horn, A. Loidl, and P. S. Riseborough, Europhys. Lett. 46, 762 (1999). 297 K. Takeda, H. Hidaka, H. Kotegawa, T. C. Kobayashi, K. Shimizu, H. Harima, K. Fujiwara,

K. Miyoshi, J. Takeuchi, Y. Ohishi, et al., Physica B 359–361, 1312 (2005). 298 K. Fujiwara, K. Miyoshi, J. Takeuchi, Y. Shimaoka, and T. Kobayashi, J. Phys.: Condens Matter 16, S615 (2004).

128

P. FULDE ET AL.

F IG . VII.3. Partial densities of states (DOS) for LiV2 O4 calculated in LDA. The flat band of Figure VII.2 corresponds to the spike at 1 eV. (After Ref. [296].)

where α = 1, . . . , 4 is a band index due to 4 atoms/unit cell and one orbital per site is assumed. The band energies are 2t, α = 3, 4 1 α (k) = 2 α = 1, 2 −2t 1 ± (1 + ηk ) ηk = cos(2kx ) cos(2ky ) + cos(2ky ) cos(2kz ) + cos(2kz ) cos(2kx ) (7.4) where kν is given in reciprocal lattice units 2π a . The bandstructure is shown in Figure VII.2. One notices a two-fold degenerate flat band which is unoccupied provided t > 0. Hopping processes beyond nearest neighbors do not give the flat band a dispersion. This is only the case when the hopping matrix elements differ for different orbitals. The essential features of the simplified bands are still visible in the bands calculated by LDA (see Figure VII.3). As regards heavy quasiparticles the crucial question is which degrees of freedom are associated with their formation. Usually one relates spin degrees of freedom with the low energy excitations giving rise to the heavy quasiparticles. This has been discussed at length, e.g., in Sections III, V and VI. However, in a frustrated lattice one might also think of charge degrees of freedom giving rise to a large number of low energy excitations. The high degeneracy of the ground state in the absence of a kinetic energy term in the Hamiltonian is lifted when hopping processes are included and the entropy can be released over a small temperature range. This is discussed in one of the next sections for the strong correlation limit. Nonetheless, the finding that the entropy at 60 K is close to 2R ln 2 suggests that here too spin degrees of freedom are responsible for the large low temperature specific heat coefficient γ .

STRONGLY CORRELATED ELECTRONS

129

In the following we give an estimate which shows that spin degrees of freedom in the pyrochlore structure are indeed able to explain the size of γ in LiV2 O4 . In setting up the Hamiltonian we include repulsive interactions between electrons on neighboring sites. In view of the observed charge ordering under pressure, the following Hamiltonian seems appropriate

†

H =− tν ciνσ cj νσ + h.c. + U niν↑ niν↓ + U niν niμ ij ν

+ J˜

iνμ

siν siμ + V

iν

ni nj +

ij

i;ν>μ

Jij (Si , Sj )Si Sj .

(7.5)

ij

Here i is a site and ν is an orbital index (ν = 1, 2, 3) denoting the different t2g orbitals. The first term is the kinetic energy or electronic hopping term. For the purpose of the intended estimate for γ we will later neglect it. The following three terms describe the intra-atomic Coulomb repulsions and spin interactions. For simplicity we have neglected the differences in the repulsions when different orbitals at site i are involved. Otherwise we would have to introduce an additional parameter U (compare with Eq. (7.7) below). Finally, the last two terms are due to the Coulomb repulsions and antiferromagnetic spin spin interactions between neighboring sites. Hereby Si = ν siν . For an estimate of the spin contributions to the γ coefficient we assume that the tν are very small so that they do not play a role. Then the d 2 configurations have spin S = 1. The Coulomb repulsions are minimized if on each tetrahedron two sites are in a d 1 configuration with S = 1/2 and two are in a d 2 configuration with S = 1. Let us pick out one of the exponentially large number of degenerate ground-state configurations (see Figure VII.4). One notices that all S = 1/2 sites form chains and rings and the same holds true for the sites with spin 1. The smallest rings consist of six sites. These features are independent of the chosen configuration. By means of constrained LDA+U calculations one can determine the nearest-neighbor spin coupling constants Jij (Si Sj ).299 One finds for J (1/2, 1/2) = 3 meV and J (1, 1) = 24 meV implying that the spin 1 sites are much stronger coupled to each other than the spin 1/2 sites. Note that spin 1 chains have a gap in the expectation spectrum, i.e., the Haldane gap H .300,301 Therefore spin 1/2 chains and rings are virtually uncoupled from each other. They can be coupled only via spin 1 chains. But the coupling between the two is frustrated and it takes a considerable energy H 0.41J (1, 1) to excite the spin 1 chains and rings. Therefore the spin 1/2 chains remain essentially uncoupled and 299 P. Fulde, A. N. Yaresko, A. A. Zvyagin, and Y. Grin, Europhys. Lett. 54, 779 (2001). 300 F. D. M. Haldane, Phys. Lett. A 93, 464 (1983). 301 F. D. M. Haldane, Phys. Rev. Lett. 50, 1153 (1983).

130

P. FULDE ET AL.

F IG . VII.4. Pyrochlore lattice: Example of a configuration satisfying the tetrahedron rule. Occupied sites with S = 1 (black dots) are connected by thick solid lines which form chains or rings. The same may be done for occupied sites with S = 1/2 (yellow dots).

we can determine directly the γ coefficient of the specific heat and the susceptibility from the relations.302 γ=

kB R 2 , 3 J (1/2, 1/2)

χs =

4μ2eff R . π 2 J (1/2, 1/2)

(7.6)

Note that the Sommerfeld–Wilson ratio is RW = 2. An experimental fit of γexp would require J (1/2, 1/2) = 1.2 meV instead of the calculated 3 meV. It is known that spin interactions are overestimated by a LDA+U calculation. But in any case, the improvement which is needed by applying the above localized electron picture to determine the γ coefficient is much less than the factor of 25 which is missing when a band approach is used. The above estimate suggests that a description of electrons in LiV2 O4 should start from the localized limit instead from the band limit because in the former case the required corrections by including tν = 0 are much less. There have been also a number of attempt to explain the heavy quasiparticle in LiV2 O4 with an on-site Hubbard interaction U only, i.e., without including Coulomb repulsions between neighboring sites. Thereby one of the t2g electrons is kept as localized while the remaining 0.5 electron per V site is treated as delocalized. The following argument is used to justify this distinction. Due to a slight 302 J. C. Bonner and M. E. Fisher, Phys. Rev. A 135, 640 (1964).

STRONGLY CORRELATED ELECTRONS

131

distortion of the oxygen octahedra surrounding the V sites the t2g states split into a lower a1g and two eg states. The splitting is much smaller than the corresponding bandwidths. Indeed, a LDA bandstructure calculation294–296 finds the total occupancies n(eg ) = 1.1 and n(a1g ) = 0.4 implying a similar population of the different t2g orbitals. But when instead a LDA+U calculation is performed303 the a1g state is singly occupied while the remaining 0.5 electrons per V site are of eg character. However, this seems to be a typical mean-field result. From an atomic point of view there is no reason why an a1g electron should not be able to hop to a neighboring site like an eg type electron. The following Hamiltonian based on the LDA+U findings has been used and investigated beyond mean-field approximation304

†

H =− t12 ci1σ cj 2σ + h.c. + U niα↑ niα↓ + U ni1 ni2 ij

− J˜

Si (σi1 + σi2 ) + J

i

iα

i

(7.7)

Si Sj .

ij

The indices 1 and 2 refer to the two eg orbitals. Due to Hund’s rule the coupling at site i between a localized a1g electron with spin Si and an eg electron with spin 1 2 σiα (α = 1, 2) is ferromagnetic. The spin–spin interactions between neighboring sites i and j are antiferromagnetic. Otherwise the system would order ferromagnetically. The on-site Coulomb repulsion of eg electrons is chosen to be different when the electrons are in the same orbital and when they are not. The spin–spin interaction between the eg electrons is neglected. A strong Hund’s rule coupling is assumed between the a1g and the eg electrons by taking the limit J˜ → ∞. The nearest neighbor spin correlations between the localized a1g electrons imply that the effective hopping matrix element t12 (S) of the eg electrons depends on the relative spin orientation of the a1g electrons, i.e., 1 + Si Sj t12 (S) = t12 . (7.8) 2S 2 The determination of Si Sj takes into account the frustrated lattice, here the pyrochlore structure 305 With the above simplification the Hamiltonian (7.7) reduces to

† † H =− t12 (S) ci1 cj 2 + ci2 cj 1 + h.c. + U ni1 ni2 . (7.9) ij

i

303 V. I. Anisimov, M. A. Korotin, M. Zölfl, T. Pruschke, K. L. Hur, and T. M. Rice, Phys. Rev. Lett. 83, 364 (1999). 304 M. S. Laad, L. Craco, and E. Müller-Hartmann, Phys. Rev. B 67, 033105 (2003). 305 B. Canals and C. Lacroix, Phys. Rev. Lett. 80, 2933 (1998).

132

P. FULDE ET AL.

The ci operators have only one additional index which takes the values 1 and 2 and acts like a pseudospin. Therefore Eq. (7.9) has the form of a Hubbard Hamiltonian with a spin dependent hopping matrix element. This Hamiltonian has been treated for the 1/4 filled case by iterated perturbation theory.304 When U is increased a Kondo-like sharp resonance is obtained at the Fermi surface resulting in heavy quasiparticles at low temperatures. Thermodynamic as well as transport properties can be expressed in terms of a cross-over temperature T ∗ , going from a heavy Fermi liquid to a spin liquid at T > T ∗ . There have been also a number of other attempts to explain the heavy quasiparticles which we want to mention. One approach starts from a Hamiltonian similar to (7.7) but replacing the two eg orbitals by a single one.306 Nearestneighbor spin correlations are treated by a mean-field ansatz Si Sj = − 32 2 and so are Hund’s rule correlations Si σ i = u2 . The mean field u is determined from a pseudo-hybridization between the a1g electron and the itinerant, i.e., eg electron. A subsidiary condition ensures that there is one a1g electron per site. Two temperatures characterize that approach. Above T = Tmag the quantity = 0 and the susceptibility is Curie–Weiss like because the intersite correlations have vanished. Similarly, a vanishing mean field u marks the second temperature THF ( 20 K) below which a narrow a1g band at EF appears giving rise to heavy quasiparticles. More details are found in Ref. [306]. The mean-field approach has been generalized by treating also the a1g electron as itinerant. The on-site Coulomb repulsion between the eg and a1g electrons is taken into account in a slave boson mean-field approximation.307 In effect the a1g bandwidth is strongly renormalized and gives rise to a sharp resonance at EF . There have been also weak coupling approaches to explain the heavy quasiparticles. One suggestion is based on multicomponent fluctuations due to the t2g and spin degrees of freedom.308 One of the consequences of the large orbital contributions to the γ coefficient of the specific heat is a small Sommerfeld–Wilson ratio of RW 0.1. Another approach treats the pyrochlore structure of the V ions as a network of Hubbard chains.309 Due to this one-dimensional feature electron correlations have strong effects on electron-hole excitations and hence on the selfenergy.

306 C. Lacroix, in Proceed. HFM 2000, Canad. J. Phys. 79, 135 (2000). 307 H. Kusunose, S. Yotsuhashi, and K. Miyake, Phys. Rev. B 62, 4403 (2000). 308 Y. Yamashita and K. Ueda, Phys. Rev. B 67, 195107 (2003). 309 S. Fujimoto, Phys. Rev. B 65, 155108 (2002).

STRONGLY CORRELATED ELECTRONS

133

17. S TRUCTURAL T RANSITION AND C HARGE D ISPROPORTIONATION : A LV 2 O 4 The spinel AlV2 O4 is of interest because the average d-electron number per V ion is 2.5 and therefore the configurations are expected to fluctuate between 3d 2 and 3d 3 . However, what actually happens is that the system undergoes a phase transition at approximately Tc = 700 K to a charge ordered state. It is associated with a change of the lattice structure from pyrochlore to alternating Kagomé and triangular planes. This is shown in Figure VII.5. In the low temperature rhombohedral phase the [111] axis is elongated while the perpendicular axes are shortened in order to keep the volume of the unit cell nearly constant. Experimental results are shown in FigureVII.6. The figure contains also a plot of the observed changes of the angle between two unit vectors of the rhombohedral lattice as the temperature

F IG . VII.5. Distortion of a pyrochlore lattice by elongation along the [111] axis. The resulting rhombohedral lattice consists of Kagomé and triangular planes.

F IG . VII.6. AlV2 O4 : Dependence of the V–O bond lengths on temperature. V1 and V2 refer to V2+ and V4+ ions while O1 and O2 are different oxygen ions. (After Ref. [310].) 310 J. Matsuno, T. Katsufuji, S. Mori, Y. Moritomo, A. Machida, E. Nishibori, M. Takata, M. Sakata, N. Yamamoto, and H. Takagi, J. Phys. Soc. Jpn. 70, 1456 (2001).

134

P. FULDE ET AL.

F IG . VII.7. Resistivity and magnetic susceptibility at 1 Tesla as function of temperature for AlV2 O4 . The left inset shows the low temperature field cooled (FC) and zero field cooled (ZFC) susceptibility in a field of 10−2 Tesla. (After Ref. [310].)

is lowered below the phase transition temperature. Note that there are three times as many sites on the Kagomé lattice than there are on the triangular one. In a simplified description the V ions have a valency of V4+ on the triangular and V2+ on the Kagomé sites corresponding to d 1 and d 3 configurations, respectively. The charge disproportionation is often called valence skipping. Of course, this is a simplified view since in reality the disproportionation is considerably less than the separation 4 × d 2.5 → 3 × d 3 + 1 × d 1 would suggest. The system avoids frustration by distorting. Unfortunately the experimental results are still sparse. It is not even clear whether AlV2 O4 is a poor metal or a small gap semiconductor at low temperatures. Resistivity measurements as well as those of the susceptibility are shown in Figure VII.7. The structural phase transition shows up in both quantities, i.e., by a small but steep increase in the resistivity and a pronounced decrease of the magnetic susceptibility. For a description of the phase transition one must set up a model Hamiltonian. It should also allow for explaining differences of charge ordering in AlV2 O4 and in LiV2 O4 under pressure. While AlV2 O4 is a semiconductor or a metal in the charge ordered state, LiV2 O4 becomes an insulator.297 Electronic structure calculations based on LDA+U provide a realistic description of magnetic insulators but are not suitable for strongly correlated paramagnetic metals. Therefore we exclude them here and start from a microscopic model Hamiltonian at the price of having to introduce adjustable parameters. Nevertheless, we can uncover this way the processes which lead to the observed structural transition and the accompanying charge order. From standard band-structure calculations it is known that only t2g states are near the Fermi energy (compare with Figure VII.3). All other bands

STRONGLY CORRELATED ELECTRONS

135

are well above or below EF . Therefore it suffices to include only t2g electrons in the model Hamiltonian. We write it in the form H = H0 + Hint + He−p , with

νν † H0 = tμμ (l, l )clμνσ cl μ ν σ lμ,l μ

(U + 2J ) Hint = nlμν↑ nlμν↓ + U nlμνσ nlμν σ¯ ν

lμ

+ (U − J )

ν>ν

nlμνσ nlμν σ +

ν>ν

V 2

nlμνσ nl μ ν σ

lμ,l μ νν σ σ

1 δμ,1 − (1 − δμ,1 ) nlμνσ + K He−p = l2 . 3 μ lνσ

(7.10)

l

Here H0 describes the kinetic energy. The electron creation and annihilation operators are specified by four indices, i.e., for the unit cell (denoted by l), the sublattice (μ = 1−4), the t2g orbital (ν = dxy , dyz , dzx ), and the spin (σ = ↑, ↓). The brackets . . . indicate a summation over nearest-neighbor sites. The term Hint describes the on-site Coulomb and exchange interactions U and J among the t2g electrons. The last term contains the Coulomb repulsion V of an electron with those on the six neighboring sites. Finally He−p describes the coupling to lattice distortions. The deformation potential is denoted by . It is due to a shift in the orbital energies of the V sites caused by relative changes in the oxygen positions. While the energy shift is positive for the V (1) sites it is negative for the V (2) sites. The elastic constant K refers to the c44 mode and describes the energy due to the rhombohedral lattice deformation. It is reasonable to assume that like in Fe3 O4 311 and Yb4 As3 199 only the c44 mode is strongly coupled with the charge disproportionation. One can give at least approximate values for all parameters except for V and . Their ratio will be fixed by the charge-ordering transition temperature while keeping the constraint V U . For the on-site Coulomb- and exchange integrals we set U = 3.0 eV and J = 1.0 eV which are values commonly used for vanadium oxides.312 Band structure calculations which we have νν between different performed demonstrate that the hopping matrix elements tμμ orbitals ν = ν are negligible. For simplicity we can therefore omit ν, ν . Then 311 H. Schwenk, S. Bareiter, C. Hinkel, B. Lüthi, Z. Kakol, A. Koslowski, and J. M. Honig, Eur. Phys. J. B 13, 491 (2000). 312 A. Fujimori, K. Kawakami, and N. Tsuda, Phys. Rev. B 38, R7889 (1988).

136

P. FULDE ET AL.

tμμ (l, l ) = −t when l, l are nearest neighbors. We will take into account the orbital dependent hopping matrix elements coming from a tight-binding fit of LDA calculations. Furthermore the c44 elastic constant is neither known for AlV2 O4 nor for LiV2 O4 , while computational methods for its ab initio calculation in the case of materials with strong electronic correlations are not mature enough. (0) Therefore a representative value c44 / = 6.1 · 1011 erg/cm3 is used for AlV2 O4 where is the volume of the cubic unit cell with a lattice constant of a = 5.844 Å. This value is close to the experimental value for Fe3 O4 which has also the spinel structure. This leads to K 1.1 · 102 eV. The deformation potential is not known but is commonly of the order of the band width. For convenience we introduce the dimensionless coupling constant λ = 2 /Kt and lattice distortion δL = /t. From LDA calculations the bandwidth is 8t = 2.7 eV, and therefore a reasonable value is λt = 2 /K = 1 eV. This means = 10.5 eV which is twice the value of Yb4 As3 .31 Not contained in the Hamiltonian (7.10) is a spin–spin interaction term between the V ions. This might turn out a shortcoming since bandstructure calculations based on a local spin-density approximation (LSDA) to density functional theory find effective exchange constants which are strongly enhanced in the low temperature phase. Estimates are Jkk = Jkt = 202 K for the high temperature phase where the subscripts k and t refer to Kagomé and triangular sites. For the low temperature phase the corresponding estimates are Jkk = 360 K and Jkt = 167 K.313 Let us first consider H0 which is easily diagonalized. With four V ions per unit cell and three t2g orbitals there are altogether 24 bands, assuming that the spin symmetry is broken. Of those twelve are dispersionless and degenerate. Furthermore, there are two sixfold degenerate dispersive bands (compare with Figure VII.2). The Fermi energy is in a region of high density of states. More details are found in Ref. [285]. The next term we discuss is He−p which describes the deformation potential coupling. When it is sufficiently strong it leads to charge ordering. There is no opening of a gap though, but only a sharp decrease of the density of states near EF , i.e., the system remains a metal. This feature does not change when the interactions U and V are included in mean-field approximation, provided we deal with a paramagnetic state. Generally U suppresses charge ordering while V enhances it. Again, no gap opens at EF but the density of states decreases in its neighborhood. In mean-field approximation the relation between the homogeneous lattice distortion δL along [111] and charge disproportionation is given by δL =

λ(n2 − n1 ) 2

313 A. Yaresko, I. Leonov, and P. Fulde, Physica B, in press.

(7.11)

STRONGLY CORRELATED ELECTRONS

137

where n1 = νσ nl1νσ is the occupational number of the triangular sites while n2 = n3 = n4 with n2 = νσ nl2νσ is the one of the Kagomé sites. A shortcoming of the mean-field analysis is that it leads to a second-order phase transition instead of the observed first-order one. This is almost certainly due to strong correlations which suppress charge fluctuations between different vanadium sites. In order to incorporate them at least approximately, one must allow for unrestricted mean-field solutions by breaking the spin symmetry. But the constraint of zero total magnetic moment has to remain. This is done by ascribing to the sites μ of a tetrahedron an occupational number nμ and a magnetization mμ = νσ nlμνσ σ . The spins are assumed to be directed towards the center of the tetrahedron in the undistorted phase. For them the [111] direction is a convenient quantization axis. In the distorted phase the spins of the V (1) sites are slightly tilted with respect to this axis so that the net magnetization remains zero. The free energy is a function of the different nμ and mμ and must be minimized with respect to both. The energy bands do now depend on spin σ . The hopping matrix elements between nearest neighbor sites must be transformed accordingly, so that the different spin directions are accounted for. For details see Ref. [314]. As a result the charge disproportionation is found as function of the various parameters. We show in Figure VII.8 the results for T = 0 as function of the ratio V /t. As usual the calculated disproportionation is larger, here by a factor of 2.5 than

F IG . VII.8. Charge disproportionation based on Eq. (7.10) as function of V /t . The nμ denote the occupation numbers of the four sites of a tetrahedron. In the inset the changes in the density of states are shown when V /t is just below and above the critical value at which charge ordering sets in. For V /t = 1.67 one has n1 = 2.5 − 3δ and ni = 2.5 + δ (i = 2–4) with a charge disproportionation δ 0.25. Here U = 3.0 eV, J = 1.0 eV, λt = 1.0 eV and 8t = 2.7 eV. (After Ref. [314].) 314 Y. Z. Zhang, P. Fulde, P. Thalmeier, and A. Yaresko, J. Phys. Soc. Jpn. 74, 2153 (2005).

138

P. FULDE ET AL.

the one obtained from a valence band analysis of the measured distorted structure. This is due to the simplified model Hamiltonian which does not allow for screening by non-d electrons. The same difficulty was found for Yb4 As3 .31,315 Also shown in Figure VII.8 as an inset is the change in the density of states in the vicinity of the critical ratio (V /t)crit = 1.6 at which the transition to a charge ordered state does occur. The strong change which one can notice might explain the observed small but steep increase in the resistivity when charge ordering sets in. The phase transition is found to be of first order when the free energy is evaluated. For V /t = 1.67 the calculated transition temperature is Tc = 660 K which is reasonably close to the observed one of Texp = 700 K. Of course, there is some arbitrariness in the particular choice of V /t. It should be pointed out that the LSDA calculations yield a value of δ = 0.17 for the disproportionation and a small hybridization gap. In the undistorted phase the point symmetry of the vanadium ions is D3d and the t2g degeneracy is reduced to an a1g singlet and an eg doublet. In the distorted, i.e., charge ordered phase the symmetry of the triangular sites remains D3d while the one of the Kagomé sites is lowered to C2h . This lifts also the eg degeneracy. It is due to an elongation of the crystal in [111] direction and a contraction perpendicular to it. While in the distorted phase of AlV2 O4 the energies of the three orbitals are nearly the same because of a very small distortion of the oxygen octahedra one expects that in LiV2 O4 the energy of the a1g orbital is highest. There the distortion of the octahedra is fairly large. Since the changes in orbital energies are small in AlV2 O4 one expects that the system remains gapless even in the charge ordered state in agreement with LDA calculations. The LDA band structure can be reproduced by a proper choice of the hopping parameters. By determining self-consistently the occupational numbers of the three V (1) sites one xy yz xy yz yz xy zx zx finds that n2 = nzx 2 > n2 , n3 = n3 > n3 and n4 = n4 > n4 in the t2g basis. This shows that the ordered orbitals on sublattices 2, 3 and 4 are perpendicular to each other. There is no orbital ordering on the V (2) sites in the charge ordered state because of the small energy difference between the a1g and eg orbitals as compared with the bandwidth. The sharp decrease of the density of states near EF as well as the order of the charge ordering phase transition are not influenced by orbital order. The same holds true for the absence of an energy gap at EF . Therefore orbital ordering is of little importance for AlV2 O4 . These findings should be compared with charge ordering observed in LiV2 O4 under pressure. A crucial difference is the average d-electron number per V site which is 1.5 for LiV2 O4 as compared with 2.5 in the case of AlV2 O4 and the distinct role of the a1g orbital. Consequently in the limit t → 0 the a1g orbital is 315 U. Staub, B. D. Patterson, C. Schulze-Briese, F. Fauth, M. Shi, L. Soderholm, G. B. M. Vaughan, E. Dooryhee, J. O. Cross, and A. Ochiai, Physica B 318, 284 (2002).

STRONGLY CORRELATED ELECTRONS

139

empty at the V (1) sites of LiV2 O4 while the split eg orbitals are singly occupied with S = 1. On the V (2) sites with d 0 also the split eg orbitals are unoccupied. Therefore a gap at EF is expected in the charge ordered state. This is what is found when the Hamiltonian (7.5) is treated in mean-field approximation with a filling factor of 1/4 instead of 5/12 as in the case of AlV2 O4 . The opening of a gap can also be inferred from measurements of ρ(T ).297 Orbital ordering is obviously not relevant here. For further details we refer to Ref. [314]. The structure in the distorted phase on which the above theory has been based was recently called into question in Ref. [316]. Instead of a low-temperature structure consisting of triangular and Kagomé planes those authors interpret their data in terms of V7 molecular clusters. The future has to show which structure is the correct one. 18. F RACTIONAL C HARGES D UE TO S TRONG C ORRELATIONS Consider the pyrochlore lattice with half as many electrons than there are number of sites. We take the limit U → ∞ and neglect for simplicity the electron spin so that we are dealing with spinless fermions. In that case half of the lattice sites are singly occupied and half of them are empty. Restricting the inter-site Coulomb repulsion to nearest neighbors the Hamiltonian is

†

H = −t ci cj + h.c. + V ni nj . (7.12) ij

ij

The ci† create spinless fermions at sites i and as usual ni = ci† cj . As discussed before, the repulsion V is minimized when in each tetrahedron two sites are occupied and two sites are empty (tetrahedron rule). Let us now add one particle to the system. Since each site belongs to two tetrahedra, the above rule is violated for two neighboring tetrahedra which now contain three electrons each. The interaction energy is increased by 4V . But when one of the four nearest neighbors of the added particle hops onto an empty site the two tetrahedra violating the rule are separated. This is shown in Figure VII.9. The important point is that the interaction energy remains unchanged by this separation, i.e., it is still 4V . When the charge of the added particle is e, each fragment must be assigned a charge e/2. Taking into account the kinetic energy term of the Hamiltonian lifts the exponentially large degeneracy of the ground state which is present when the kinetic energy term is absent. Deconfinement of the charges e/2 remains intact provided 316 Y. Horibe, M. Shingu, K. Kurushima, H. Ishibashi, N. Ikeda, K. Kato, Y. Motome, N. Furukawa, S. Mori, and T. Katsufuji, Phys. Rev. Lett. 96, 086406 (2006).

140

P. FULDE ET AL.

F IG . VII.9. Separated tetrahedra on a pyrochlore lattice after an electron has been added to the system. Occupied sites are connected by solid red lines and empty by green lines (courtesy of F. Pollmann).

t/V is sufficiently small.317–319 Since a numerical study of a pyrochlore lattice is difficult we shall investigate instead the simpler checkerboard lattice. The latter can be considered a projection of the pyrochlore lattice onto a plane. But one must keep in mind that the lower dimension of the checkerboard lattice may result in different behaviors as regards confinement or deconfinement of the fractional charges e/2. This is known from lattice gauge theories which are closely related to the present problem317,320 Also the statistics of fractionally charged excitations may differ in two and three dimensions. In two dimensions the wavefunction of the particles belongs to a representation of the braid group while in three dimensions it is one of the permutation group. Figure VII.10 shows one of the ground state configurations. They have the form of string nets (see also Ref. [321]). In the absence of hopping the degeneracy is Ndeg = (4/3)3N/4 where N = Nx Ny and Nx , Ny are the number of lattice sites in x and y direction. In order to study numerically the ground state of the system for large ratios of V /t it is advantageous to introduce an effective Hamiltonian42 which acts on the different configurations obeying the tetrahedron rule. They form what will be called the allowed subspace 317 A. M. Polyakov, Gauge Fields and Strings, vol. 3 of Contemporary Concepts in Physics, Harwood Academic Publ. (1993), 5th print. 318 P. Fulde, K. Penc, and N. Shannon, Ann. Phys. (Leipzig) 11, 892 (2002). 319 J. Betouras, F. Pollmann, and P. Fulde, to be published (2006). 320 E. Fradkin, Field Theories of Condensed Matter Systems, Addison-Wesley Publ., Redwood City (1991). 321 M. Levin and X.-G. Wen, Phys. Rev. B 73, 035122 (2006).

STRONGLY CORRELATED ELECTRONS

141

F IG . VII.10. Ground-state configuration of a checkerboard lattice with half-filling of spinless fermions. Occupied sites are connected by solid lines and empty sites by dashed lines. Hopping takes place along thin lines with matrix element −t .

of all configurations. An effective Hamiltonian allows for the diagonalization of much larger clusters than does the full H . To leading order in t/V one finds that the energy is lowered for all allowed configurations by an amount of 4t 2

ni . (7.13) E = − V i

Therefore it does not lift the degeneracy and one has to go to the next higher order term. Different allowed configurations are connected through ring hopping processes. The smallest non-vanishing process is 3 − 6t (7.14) + Heff = (+) 2 V where filled dots denote occupied and empty dots empty sites, respectively. The site in between can be empty or occupied. The arrows stand for particle hopping. With tring = this Hamiltonian can be written as Heff = tring

12t 3 V2

(7.15)

cj†6 cj†4 cj†2 cj5 cj3 cj1 .

(7.16) 7 Hopping on larger rings implies higher orders in t/V . The matrix elements of Heff with respect to different allowed configurations |i and |j are j |Heff |i = (−1)n0 tring

(7.17)

142

P. FULDE ET AL.

where n0 is the occupation number of the site inside the ring. It is worth realizing that the sign dependence of j |Heff |i is absent when instead of a checkerboard lattice the pyrochlore lattice is considered. In the latter structure there is no lattice site inside a 6-ring loop. The partial lifting of the degeneracy of the ground-state manifold by Heff can be understood with the help of the height representation. For that purpose one divides the crisscrossed squares of the checkerboard lattice into sublattices A and B and assigns a clockwise and counter-clockwise orientation to them. To each occupied site is attached a unit vector the direction of which is in accordance with the orientation of the corresponding crisscrossed squares. At each empty site the vector is pointing into opposite direction. This defines a vector field f(r) where r is defined with respect to the uncrossed plaquettes. Because of the tetrahedron rule, i.e., two sites are occupied and two are unoccupied on a crisscrossed square, the vector sum over a closed loop vanishes, implying curl f = 0. Therefore f can be written as the gradient of a scalar field h(r), i.e., a potential which is called height field. It allows for the introduction of two topological quantum numbers κx and κy . They quantify the difference in the potential at the upper and lower boundary and at the right and left one. Their values cover the range −Nx /2 κx Nx /2 and −Ny /2 κy Ny /2. In Figure VII.11 an example is given of the change of the height field h(r) defined on the uncrossed squares. On a torus κx and κy are winding numbers. An important point is that the application of Heff does not change the topological quantum numbers of a configuration. Therefore the degenerate ground-state configurations are divided into different classes according to (κx , κy ). The matrix i|Heff |j reduces into block matrices characterized by (κx , κy ). It turns out that Heff does not necessarily connect all configurations within a class. Therefore the matrix (Heff )ij for the class (κx , κy ) may reduce further to irreducible blocks (κx(α) , κy(α) ). This holds true in particular for the class (0, 0) which has the largest

F IG . VII.11. Values of the height field h for a part of a given configuration: solid and empty dots mark occupied and empty sites, respectively.

STRONGLY CORRELATED ELECTRONS

143

number of elements. It is found that for a system of size 8 × 8 with Nf = 32 spinless fermions the ground state has topological quantum numbers (0, 0). The subclass to which it belongs has more than 105 elements. The ground state is twofold degenerate and the two states are related by particle–hole symmetry. Note that Heff has this symmetry while H does not have it. The two states are charge ordered along one of the diagonals and can be transformed into each other by a rotation of 90 degrees. This invalidates a supposition in Ref. [42]. The participation ratio (PR) of a wavefunction is a measure of how extended that function is. With

|ψ = αν |ν (7.18) ν

where |ν denotes different configurations the participation ratio is 1 . 4 ν |αν |

PR[ψ] =

(7.19)

For the ground state |ψ0 of the 8 × 8 system this ratio is very large, i.e., PR[ψ0 ] = 46.9 · 103

(7.20)

indicating that many configurations contribute to it. The largest possible value of PR[ψ0 ] in a Hilbert space of dimension N is PR[ψ0 ] = N . The total density of state is

ρtot (E) = δ(E − El ) (7.21) l

where El are the eigenvalues of H . From it we can compute the specific heat C(T ) according to ∂ dE Eρtot (E)e−βE C(T ) = . (7.22) ∂T dE ρtot (E)e−βE Numerical results for different system sizes are shown in Figure VII.12. One notices an almost linear in T behavior. This suggests that a large quasiparticle mass in geometrically frustrated lattices may possibly be due to charge instead of spin degrees of freedom, the usual source of heavy quasiparticles. The large number of low lying excitations causing the steep linear increase of the specific heat with temperature is here due to a release of entropy (3/4) ln(4/3) ≈ 0.22 per site over a temperature range of kB T 2tring . In the following we want to go beyond the space of allowed configurations which obey the tetrahedron rule. When a particle is hopping to a neighboring empty site (vacuum fluctuation) the tetrahedron rule is broken for two tetrahedra: now one tetrahedron contains three particles, while another contains one only (see

144

P. FULDE ET AL.

F IG . VII.12. Specific heat per particle for a checkerboard lattice of spinless fermions at half filling for various system sizes. Inset: corresponding entropies, the arrow marks the value of 2(3/4) ln(4/3). (After Ref. [42].)

Figure VII.13a). For the corresponding uncrossed squares curl f = 0. By subsequent hopping these two objects can separate carrying a charge of ±e/2 each. As a result of the vacuum fluctuation the vector field f(n) contains a vortex–antivortex pair. An insulator to metal transition may be viewed as a proliferation of such pairs and resembles a Kosterlitz–Thouless transition. It is difficult to compute numerically the ratio V /t at which this transition takes place, but an estimate yields a critical ratio of (V /t)cr 7. This is considerably larger than the value obtained by conventional equations of motion methods in Hubbard I-type approximation.322

F IG . VII.13. (a) Vacuum fluctuation. One criss-crossed square (tetrahedron) contains three particles while another one contains one particle only; (b) particle added to the otherwise half-filled checkerboard lattice; (c) after a hop of one of the electrons the two squares with three particles each have separated. (After Ref. [318].) 322 Y. Z. Zhang, M.-T. Tran, V. Yushankhai, and P. Thalmeier, Eur. Phys. J. 44, 265 (2005).

STRONGLY CORRELATED ELECTRONS

145

When an extra particle is added to the system two neighboring criss-crossed squares contain three occupied sites each (see Figure VII.13b). These two special squares separate from each other when one of the electrons is hopping to a neighboring site (see Figure VII.13c). There is no change in the particle repulsions associated with this separation of the two. Since the charge of the added particle is e, each of the separated squares must have charge e/2. The reason for that is easily seen. When a square with three particles moves in the checkerboard lattice plane, the squares left behind must again satisfy the tetrahedron rule. Inspection shows that this requires the backflow of a charge e/2, thus reducing the charge flow due to hopping of an electron from e to e/2. For the checkerboard lattice it turns out that ring hopping processes cause a (weak) restoring force on the two particles with fractional charge e/2.323 We have not discussed the issue of the spin here but instead have considered spinless or fully polarized fermions. In passing we point out that not only do we have spin-charge separation when the spin is included but also is the spin distributed over parts of the sample. For more details we refer to Ref. [318]. The spectral density is a quantity which is expected to show signatures of fractional charges. For that reason we determine the integrated spectral density

ψ N +1 c† ψ N .2 δ ω − E N +1 + E N . S(ω) = (7.23) 0 kν 0 kν kν kν N +1 |ψkν

are the different excited states characterized by momentum k Here N +1 are the corresponding and band index ν of the N + 1 particle system and Ekν † create particles energies. The energy of the N -particle ground state is E0N . The ckν in quantum states k, ν. For a 32 sites checkerboard cluster with N = 16 spinless fermions and V /t = 25 the integrated spectral density is shown in Figure VII.14a. When one includes only configurations of the N + 1 particle system in which the added particle is not disintegrated like in Figure VII.14a one obtains the spectral density shown in Figure VII.14b. A comparison with Figure VII.14a shows a considerable reduction of the width of the excitation spectrum and an absence of the low frequency part. Therefore we may conclude that hopping processes leading to a separation of the charge e into two parts have an important effect on the spectral density and constitute further evidence for the appearance of fractional charges. The above considerations suggest that in 2D there are also other lattices than the checkerboard one allowing for charge fractionalization. That holds particularly true for the Kagomé lattice which at 1/3 filling can support excitations with charge e/3 and 2e/3 when a spinless fermion is added.323 The requirement hereby is a short-range repulsion V ni nj when i and j are on the same hexagon. 323 F. Pollmann and P. Fulde, Europhys. Lett., in print.

146

P. FULDE ET AL.

F IG . VII.14. Integrated spectral density as function of energy for a 36 sites checkerboard system with 18 particles and V /t = 25. (a) When the excited states are fully accounted for and (b) when only configurations are used in which the added particle remains an entity. (After Ref. [324].)

The fermionic character of the particles discussed here makes the present model different from related spin models and models for hard core bosons. Nevertheless, there exist also similarities between the problem of fractional charges and resonating valence bonds (RVB). For example, Kalmeyer and Laughlin325 have shown that the ground-state wavefunction of an antiferromagnetic Heisenberg Hamiltonian with nearest-neighbor interactions on a triangular lattice is practically the same as the fractional quantum Hall effect (FQHE) wavefunction for bosons. As the ground-state of a Heisenberg Hamiltonian on a frustrated lattice is of the RVB type, the two phenomena, i.e., FQHE effect and RVBs are closely related. RVB systems support spinons, i.e., a spin flip with sz = 1 breaks up into two spinons with spin 1/2 each.326–329 The situation resembles the one in Figure VII.13 in particular when an Ising Hamiltonian us used. Spins up and down on a checkerboard lattice correspond to occupied and unoccupied sites and a state with total z = 0 has a half-filled lattice of hard-core bosons as analogue. While a spin Stot large body of work exists connecting RVB models with confined and deconfined phases of compact gauge theories (see, e.g., Refs. [320,326,330]) corresponding work for fermionic systems is still missing. 324 F. Pollmann, E. Runge, and P. Fulde, Phys. Rev. B 73, 125121 (2006). 325 V. Kalmeyer and R. B. Laughlin, Phys. Rev. B 39, 11879 (1989). 326 R. Moessner and S. L. Sondhi, Phys. Rev. B 63, 224401 (2001). 327 L. Balents, M. P. A. Fisher, and S. M. Girvin, Phys. Rev. B 65, 224412 (2002). 328 O. I. Motrunich and T. Senthil, Phys. Rev. Lett. 89, 277004 (2002). 329 G. Misguish and C. Lhuillier, Frustrated Spin Systems, World Scientific, Singapore (2004). 330 M. Hermele, M. P. A. Fisher, and L. Balents, Phys. Rev. B 69, 064404 (2004).

STRONGLY CORRELATED ELECTRONS

147

F IG . VII.15. String (marked in red) of an odd number of sites (here five) connecting two particles with charge e/2.

Finally we want to comment on some modifications which occur when the spin of the fermions is included. The question may be asked where the spin of an added electron goes when the excitation falls into two parts with charge e/2 each. The answer is found by looking at Figure VII.15 where periodic boundary conditions are used. The two charges e/2 are connected by a spin chain containing an odd number of sites. The ground state of that chain is two-fold degenerate and represents the spin degrees of freedom. Thus one may state that the spin is smeared over parts of the system as is the connected spin chain. This is a rather novel feature which we have not met before in condensed matter physics to the best of our knowledge. It should be also noticed that in the presence of spins the lowest order ring exchange process on a checkerboard lattice involves four sites instead of six. This is different for the pyrochlore lattice where the smallest possible ring involves six sites (see Figure VII.4). So the ground-state degeneracy is lifted in order t 2 /V . VIII. High-Energy Excitations

In Section II we demonstrated that strong electron correlations generate characteristic low energy scales. They are much smaller than the Fermi energy, the typical energy scale in a metal. But it is well known that strong correlations influence high-energy excitations as well. Hereby the expression high energy is used quite flexible. For example, it may include satellite structures or peaks as they are found in the photoelectron spectra of Ni metal331,332 or of the high temperature superconducting cuprates. But it also includes energies which are larger than the one 331 S. Hüfner and G. K. Wertheim, Phys. Lett. A 47, 349 (1974). 332 W. Eberhardt and E. W. Plummer, Phys. Rev. B 21, 3245 (1980).

148

P. FULDE ET AL.

at which Fermi liquid behavior breaks down. In practice this may be a rather low energy or temperature. These effects are best studied by investigating the oneparticle Green’s function. In Dyson’s representation it reads Gν (k, z) =

1 . z − ν (k) − ν (k, z)

(8.1)

The energy ν (k) describes the dispersion of electrons in band ν within an effective single-electron approximation while the self-energy ν (k, ω) contains all effects beyond that approximation. In case that ν (k) describes the Hartree– Fock bands, ν (k, ω) contains the electronic correlations. When Landau’s Fermi liquid theory does apply, the low-energy excitations near the Fermi energy are quasiparticles. They are obtained from G(k, ω) =

Z + Ginc (k, ω). ω − qp (k) − iγk sgn ω

(8.2)

For convenience we have omitted the band index ν. The first term contains the quasiparticle pole at ω = qp (k) + iγk

(8.3)

with the quasiparticle dispersion qp (k) and lifetime γk . The second term is the incoherent part which is of special interest here. Usually it is not further discussed but we want to draw attention to its importance and to significant features when electron correlations are strong. We may think of it as being due to the internal degrees of freedom of the correlation hole which is surrounding an electron. The bare electron has weight Z < 1 in the quasiparticle. The reduction is due to the interaction of the electron (or hole) with the surroundings. The internal degrees of freedom of the modified surroundings, i.e., the correlation hole shows up in the integrated spectral density in form of quasiparticle damping and satellite structures. Those structures have generally a k dependence which is much weaker than the one of the quasiparticles. An example is the shadow band in the Hubbard model when the Hubbard I approximation7 is made. The internal degrees of freedom of the correlation hole are best described by the projection operator method. The idea is to select those particular operators which describe the most important microscopic processes in setting up the correlation hole. Green’s function is determined within that restricted operator space. The Hubbard I approximation to the Hubbard model is the simplest example. Here + only one operator, i.e., ciσ ni−σ where i is the site index is used in order to describe the correlation hole. More interesting cases are discussed in the following subsections.

STRONGLY CORRELATED ELECTRONS

149

We want to draw attention to the zero-point fluctuations of internal excitation modes of the correlation hole. A well known example is Gaskell’s ansatz333 for the ground-state |ψ0 of a homogeneous electron gas. It is of the form

† |ψ0 = exp (8.4) τ (q)ρ ρq SCF q

0

q

where |SCF 0 is the Hartree–Fock ground state and ρq are the density fluctuations of wavenumber q. Furthermore τ (q) ∼ q −2 when q → 0. Here the zero-point fluctuations of plasmons are taken into account which are the internal excitation modes of the correlation hole when the latter is described within the random phase approximation (RPA). It is well known that the RPA models very well the longrange part of the correlation hole but fails to describe properly the short-range part. Zero-point fluctuations of other modes, in particular of those associated with the short-range part of the correlation hole enter in a similar way the (Jastrow) prefactor in Eq. (8.4). We start out by describing the projection operator formalism before we discuss a number of applications. 19. P ROJECTION O PERATORS In the following we shall use the retarded Green function in order to determine the excitations of the system. It is given by † (8.5) GR νσ (k, t) = −i(t) ψ0 cνσ (k, t), cνσ (k) + ψ0 where |ψ0 is the exact ground state and (t) is the step function, i.e., (t) = 1 for t 0 and zero otherwise. The superscript R will be left out in the following discussion for simplicity. We assume that the Fourier transforms of the most important microscopic processes for the generation of the correlation hole are represented by a set of operators {Aμ (k)}, the dynamical variables. But we want to † (k). Explicit examples for proper include in this set also the original operators cνσ choices of the Aμ (k) will be given when specific applications of this method are discussed. Within that reduced operator space 0 spanned by the {Aν (k)} we define the Green function matrix (8.6) Gμν (k, t) = −i(t) ψ0 A†μ (k, t), Aν (k, 0) + ψ0 . Note that the Green function (8.5) is just a diagonal element of that matrix. It is convenient to introduce the following notation (8.7) (A|B)+ = ψ0 A† , B + ψ0 . 333 T. Gaskell, Proc. Phys. Soc. 72, 685 (1958).

150

P. FULDE ET AL.

This enables us to rewrite (8.6) after a Fourier transformation in the condensed form

1 Aν Gμν (k, z) = Aμ (8.8) z−L + where z = ω + iη and η is a positive infinitesimal number. The Liouvillian L corresponds to H and is defined by its action on an arbitrary operator A through LA = i

dA = [H, A]− dt

(8.9)

so that A(t) = eiLt A(0).

(8.10)

By making use of the identity 1 1 1 1 = − b a+b a a a+b we can rewrite (8.8) in the form of the following matrix equation z1 − L + M(z) χ−1 G(z) = χ

(8.11)

with matrix elements χμν = (Aμ |Aν )+ Lμν = (Aμ |LAν )+ ,

1 QLAν . Mμν (z) = Aμ LQ z − QLQ +

(8.12)

The matrix M(z) is called memory function.334,335 It couples the relevant operators {Aν } to the remaining degrees of freedom. The operator Q

Q=1− |Ai )+ χij−1 (Aj | (8.13) ij

projects onto those remaining degrees, i.e., onto an operator space perpendicular to the {Aν }, i.e., Q|Aν )+ = 0. Setting M(z) = 0 implies that the dynamics of the system is approximated by the {Aν } and takes place within 0 . One may either choose a large basis {Aν } and set M(z) = 0 or work with a small basis and keep M(z). Examples are given below. If not stated otherwise we shall set M(z) = 0. The dimension of the matrix Eq. (8.11) equals the number of dynamical variables Aν (k). The energy resolution of the excitation spectrum depends on the size of the set {Aν (k)}. For high-energy excitations a relatively small number of dynamical variables is sufficient. By increasing their number one can increase the energy resolution of the spectral density calculated from Eq. (8.8). 334 H. Mori, Progr. Theor. Phys. 33, 423 (1965). 335 R. Zwanzig, Lectures in Theoretical Physics, Interscience, New York (1961), vol. 3.

STRONGLY CORRELATED ELECTRONS

151

20. T HE H UBBARD M ODEL : A PPEARANCE OF S HADOW BANDS The Hubbard model shows particularly well a number of generic features caused by strong electron correlations. Among them are the appearance of satellite structures, shadow bands and a marginal Fermi liquid like behavior close to half filling. The Hamiltonian is of the well known form

† ciσ cj σ + h.c. + U ni↑ ni↓ H = −t ij

i

= H0 + HI

(8.14)

in standard notation. In the following we discuss solely for pedagogical and illustrative reasons the spin-density wave (SDW) and Hubbard I approximation by applying projection operators. The simplest case in which a shadow band does appear, is a square lattice at half filling when a spin-density wave (SDW) approximation is made. This simple approximation leads to an antiferromagnetic ground state |AF . Charge fluctuations are suppressed here on a mean-field level by symmetry breaking. Breaking a symmetry can reduce intersite charge fluctuations similarly as strong correlations do without symmetry breaking. Therefore features of strong correlations show up already in this simple mean-field scheme. From the kinetic energy term in (8.14) one obtains the dispersion (k) = −2t (cos kx + cos ky ). The lattice constant has been set equal to unity. Therefore, at half filling the Fermi surface is nested and the ground state in mean-field approximation is a spin density wave. One finds † † uk ckσ + σ vk ck+Qσ |0 (8.15) |AF = kσ † † where Q is a reciprocal lattice vector and ckσ is the Fourier transform of ciσ . Furthermore u2k + vk2 = 1 with

(k) (k) 1 1 2 2 1− , vk = 1+ uk = 2 E(k) 2 E(k) 1

m2 U 2 2 E(k) = (k)2 + 0 . (8.16) 4

Here m0 is the staggered magnetization. The latter has to be calculated selfconsistently. In order to calculate the excitations we choose for the relevant dynamical variables {Aν } † A1 (k) = ckσ ,

† A2 (k) = ck+Qσ .

(8.17)

152

P. FULDE ET AL.

When the 2 × 2 matrix (8.11) with M(z) = 0 is evaluated one finds G11 (k, z) =

u2k z − ( U2 − E(k))

+

vk2 z − ( U2 + E(k))

and for the spectral density

U U D(k, ω) = u2k δ ω − + E(k) + vk2 δ ω − − E(k) . 2 2

(8.18)

(8.19)

For each k point there are two contributions to D(k, ω), i.e., one δ-function peak with a large weight and one with a small one. The peaks with the smaller weight form a shadow band Esb (k) = −E(k) which complements the band resulting from the peaks with large weight.336,337 Because of the mean-field level the shadow band disappears for temperatures higher than the Néel temperature. This is in reality not the case and therefore one would like to reproduce a shadow band also for arbitrary filling factors and for the paramagnetic state. This can be done, of course, only by accounting for the strong correlations. They are described in the simplest way by the Hubbard I7 approximation. In that case the following choice is made for the dynamical variables {Aν } 1 ikRi † † , A2 (k) = √ e ciσ δni−σ (8.20) A1 (k) = ckσ N0 i with δni−σ = ni−σ − ni−σ . The Ri denote the positions of the N0 lattice sites. Again, we want to determine G11 (k, ω) from (8.8) by setting M(z) = 0. The 2 × 2 matrix equation can be easily solved and one finds −1

U Uˆ G11 (k, z) = z − (k) − n 1 + (8.21) 2 z − Uˆ where n is the number of electrons per site and Uˆ = U (1 − n/2). G11 (k, ω) has two poles centered at z = 0 and z = U . Neglecting terms of order U −1 we can rewrite (8.21) as G11 (k, z) =

n 1 − n2 2 . n + z − (k)(1 − 2 ) z − U − (k) n2

(8.22)

The poles give raise to two bands, i.e., the upper and the lower Hubbard band. Their widths differ except for n = 1. For n = 0.25 the upper Hubbard band is reduced to a satellite structure with a k-dependent dispersion. This is illustrated in Figure VIII.1 and is well known. The reason for repeating these facts here is 336 A. P. Kampf and J. R. Schrieffer, Phys. Rev. B 42, 7967 (1990). 337 A. P. Kampf, Phys. Rev. 249, 219 (1994).

STRONGLY CORRELATED ELECTRONS

153

F IG . VIII.1. Schematic representation of the two bands resulting from the two variables of Eq. (8.20), i.e., the upper and the lower Hubbard band. The electron number per site is n, the broadening is artificial.

that we want to proceed similarly when we discuss the satellite structure in Ni or the spectral density of electrons in Cu–O planes. We want to emphasize the point of view that the incoherent part of a Green function is the superposition of satellite peaks which have a small k-dependence each. But before, we demonstrate that for special band fillings a Hubbard model can exhibit marginal Fermi liquid behavior. This is shown explicitly for a square lattice. 21. M ARGINAL F ERMI L IQUID B EHAVIOR AND K INK S TRUCTURE The Coherent Potential Approximation (CPA) has been widely used in electronic structure calculations of disordered systems.338–343 Here we want to combine it with the projection operator technique and apply it to the Hubbard model. We remind the reader that a CPA was introduced first by Hubbard when treating his 338 P. Soven, Phys. Rev. 156, 809 (1967). 339 D. W. Taylor, Phys. Rev. 156, 1017 (1967). 340 B. Velický, S. Kirkpatrick, and H. Ehrenreich, Phys. Rev. 175, 747 (1968). 341 F. Yonezawa, Progr. Theor. Phys. 40, 734 (1968). 342 R. J. Elliott, J. A. Krumhansl, and P. L. Leath, Rev. Mod. Phys. 46, 465 (1974). 343 H. Ehrenreich and L. M. Schwartz, in Solid State Physics, vol. 31, Academic Press, New York

(1976).

154

P. FULDE ET AL.

Hamiltonian.20 In the following we want to treat the many-electron problem as accurately as possible for a number of sites which need not be connected. This ˜ cluster is embedded in a medium with a coherent potential (ω). The potential is determined self-consistently so that it agrees with the momentum integrated selfenergy (k, ω) of the cluster. It is known344,345 that the local projection operator method combined with the CPA346 is equivalent to the Many-Body CPA,347 the Dynamical CPA348,349 as well as to the Dynamical Mean Field Theory (DMFT) which is based on many-body physics in infinite dimensions.350,351 For reviews of the latter, see Refs. [186,352]. Here we want to discuss the more general nonlocal version of the projection operator method353 combined with the CPA. It is based on a decomposition of the scattering matrix of the system into one-site, two-site etc. scattering matrices. This way the scattering matrix can be calculated successively in terms of increments, a method successfully applied in the theory of wavefunction based electronic structure calculations of solids. For a review of that method, see Refs. [354,41]. We apply the theory to the Hubbard model on a square lattice near half filling.7,20 The results are interesting. A marginal Fermi liquid behavior is found for large U values and small hole doping and a corresponding phase diagram is worked out.355 It is also found that for similar parameters the excitation spectrum (or real part of the self-energy) has a kink near EF .356 Such a structure was observed in a number of underdoped cuprates like Bi2 Sr2 CaCuO8+δ or La2−δ Srδ CuO4 .357,358 It has been attributed to electron– phonon interactions358–361 and also to the interaction with a magnetic resonance 344 Y. Kakehashi, Adv. Physics 53, 497 (2004). 345 Y. Kakehashi, Phys. Rev. B 66, 104428 (2002). 346 Y. Kakehashi and P. Fulde, Phys. Rev. B 69, 045101 (2004). 347 S. Hirooka and M. Shimizu, J. Phys. Soc. Jpn. 43, 70 (1977). 348 Y. Kakehashi, J. Magn. Magn. Mater. 104–107, 677 (1992). 349 Y. Kakehashi, Phys. Rev. B 45, 7196 (1992). 350 W. Metzner and D. Vollhardt, Phys. Rev. Lett. 62, 324 (1989). 351 E. Müller-Hartmann, Z. Phys. B: Cond. Matt. 74, 507 (1989). 352 T. Pruschke, M. Jarrell, and J. Freericks, Adv. Phys. 44, 187 (1995). 353 Y. Kakehashi and P. Fulde, Phys. Rev. B 70, 195102 (2004). 354 H. Stoll, B. Paulus, and P. Fulde, J. Chem. Phys. 123, 144108 (2005). 355 Y. Kakehashi and P. Fulde, Phys. Rev. Lett. 94, 156401 (2005). 356 Y. Kakehashi and P. Fulde, J. Phys. Soc. Jpn. 74, 2153 (2005). 357 P. V. Bogdanov, A. Lanzara, S. A. Keller, X. J. Zhou, E. D. Lu, W. J. Zheng, G. Gu, J.-I. Simoyama,

K. Kishio, H. Ikeda, et al., Phys. Rev. Lett. 85, 2581 (2000). 358 T. Chuk, D. H. Lu, X. J. Zhou, Z.-X. Shen, T. P. Devereaux, and N. Nagaosa, Phys. Stat. Sol. (b) 242, 11 (2005). 359 Z.-X. Shen, A. Lanzara, S. Ishihara, and N. Nagaosa, Philos. Mag. B 82, 1349 (2002). 360 S. Verga, A. Knigavko, and F. Marsiglio, Phys. Rev. B 67, 054503 (2003). 361 S. Ishihara and N. Nagaosa, Phys. Rev. B 69, 144520 (2004).

STRONGLY CORRELATED ELECTRONS

155

mode observed by inelastic neutron scattering.362–365 But as it turns out, also strong electron correlations in a 2D Hubbard model can produce it. To reach our goal we start out by choosing for the {Aν } simply the operators † but we keep this time the memory matrix, i.e., M(z) = 0. In that case we write ciσ for a paramagnetic system G(k, z) =

1 . z − (k) − U 2 M(k, ω)

(8.23)

The matrix L in (8.11) gives only a constant energy shift and is neglected here. For convenience a factor U 2 has been extracted from M(k, z). We decompose

M(k, z) = Mj0 (z)eikRj (8.24) j

and write for the reduced memory matrix according to (8.12)

1 † † Mij (z) = ciσ δni−σ c δnj −σ , z − L¯ j σ +

(8.25)

† † where L¯ = QLQ with the projector Q = 1 − iσ |ciσ )+ (ciσ |. Stopping at this stage, i.e., neglecting the new memory function in the denominator of (8.25) would bring us back to the Hubbard I approximation. In order to establish a connection to the CPA we define the Hamiltonian of an effective medium through

˜ H˜ (z) = H0 + (z) ni (8.26) i

˜ i.e., LB ˜ = [H˜ (z), B]− for arbitrary operawith the corresponding Liouvillian L, tors B. The aim is to account efficiently for local as well as nonlocal correlations ˜ by means of an effective medium characterized by (z). ˜ The coherent potential (z) is determined self-consistently from ˜ (z) =

U2

M(k, z) N

(8.27)

k

362 M. Eschrig and M. R. Norman, Phys. Rev. Lett. 85, 3261 (2000). 363 P. D. Johnson, T. Valla, A. V. Fedorov, Z. Yusof, B. O. Wells, Q. Li, A. R. Moodenbaugh, G. D.

Gu, N. Koshizuka, C. Kendziora, et al., Phys. Rev. Lett. 87, 177007 (2001). 364 M. Eschrig and M. R. Norman, Phys. Rev. B 67, 144503 (2003). 365 E. Schachinger, J. J. Tu, and J. P. Carbotte, Phys. Rev. B 67, 214508 (2003).

156

P. FULDE ET AL.

where N is the number of sites. With this in mind we decompose

˜ + ˜ Q U δni↑ δni↓ − (z)n L¯ = QLQ i Q i

= L0 (z) +

(i)

LI (z)

i

= L0 (z) + LI (z).

(8.28)

¯ −1 in terms of a scattering (super)operator T as Next we express (z − L) 1 1 1 1 + T = z − L0 z − L0 z − L0 z − L¯ = g0 (z) + g0 (z)T g0 (z)

(8.29)

with T = LI + L I g 0 L I + · · · . The T -operator can be decomposed into a sequence of many-sites increments

T= Ti + δTij + δTij k + · · · . (8.30) i

ij

ij k

Those increments are closely related to the T operators Ti , Tij , Tij k , . . . of single-site, 2-sites, 3-sites, etc. clusters. It is δTij = Tij − Ti − Tj δTij k = Tij k − δTij − δTik − δTj k − Ti − Tj − Tk .. .

(8.31)

This enables us to introduce retarded memory functions for clusters

1 (c) † † Mij (z) = ciσ δni−σ c δnj −σ . z − L¯ (c) j σ +

(8.32)

These matrices have dimensions 1 × 1 when c = i (one-site cluster) and 2 × 2 when c = (i, j ), i.e., in the 2-site cluster approximation. The Liouvillian L¯ (c) (z) is given by L¯ (c) = L0 (z) +

Nc

(n)

LI (z).

(8.33)

n∈c

The sum over n involves all Nc sites belonging to a given cluster c. Within (n) zeroth-order renormalized perturbation theory (RPT-0) only that part of LI (z)

STRONGLY CORRELATED ELECTRONS

157

(n) † is used which projects onto the operators ciσ δni−σ , i.e., P¯ LI (z)P¯ with the projector.

† c δni−σ χ −1 c† δni−σ (8.34) P¯ = iσ iσ + i iσ

and χi = ni−σ (1 − ni−σ ). With this simplification the memory matrix can be expressed in terms of a “screened” one as −1 Mij(c) (z) = g · 1 − L(c) . (8.35) I g ij The screened memory matrix is given by

1 † gij (z) = ciσ cj†σ δnj −σ . δni−σ z − L0 (z) +

(8.36)

(c)

The cluster memory matrix Mij (z) describes a Hubbard cluster embedded in a uniform medium with a Hamiltonian H˜ (z) (see the left side in Figure VIII.2). The ˜ interactions in the embedded cluster are given by ic (U δni↑ δni↓ − (z)n i ). We start from a uniform medium described by H˜ (z) (see Eq. (8.28) and the right side of Figure VIII.2). An alternative would have been to start from the same medium but with cavities at the sites of the cluster (see the middle of Figure VIII.2), i.e., from a Hamiltonian H˜ (c) with ˜ H˜ (c) = H˜ (z) − (z)

Nc

ni .

(8.37)

n∈c

In this case the interaction in the cluster would be n∈c U δni↑ δni↓ . (c) The diagonal matrix LI in (8.35) describes the atomic excitations. The ma(j ) (i) (i) trix elements are given by [LI , LI , . . .]. It has one element LI = U (1 − (j ) 2ni−σ )/[ni−σ (1 − ni−σ )] when c = i and a second one LI when c = (i, j ). The incremental cluster expansion is depicted in Figure VIII.3. With the above approximations the theory reproduces two limiting cases exactly, i.e., the limit of

F IG . VIII.2. Left side: Cluster with on-site Coulomb repulsion U embedded in a medium. Middle: ˜ Cavities replacing the sites of the cluster. Right side: Uniform medium with self-energy (ω). (After Ref. [353].)

158

P. FULDE ET AL.

F IG . VIII.3. Schematic drawing of the multisite cluster expansion of Green’s function. From left to right: single-site, two-sites and three-sites contributions. Note that the sites of a cluster need not be nearest neighbors.

small U when perturbation theory is applicable as well as the atomic limit. This is an important feature of the present theory. In the limit of large clusters the memory functions are independent of the medium. But since the cluster expansion must be truncated in practical applications there is a dependence of the memory functions on the medium and we must make an optimal choice for it. When correlation effects on the static matrix elements are neglected one can write down an explicit expression for the screened memory function of the form gij(c) (z) = Aij

d d d ρ (c) ()ρ (c) ( )ρ (c) ( )χ(, , ) ij ij ji z − − +

(8.38)

with Aii = [ni−σ (1 − ni−σ )]/[ni−σ c (1 − ni−σ c )] and Ai=j = 1. Here (c) ρij () is the density of states of a system with one or two empty sites (depending ˜ on the cluster c) embedded in a medium with a coherent potential (z). More specifically ρij(c) (z) = −

−1 1 Im z − H˜ (c) . ij π

Furthermore

niσ c =

(8.39)

(c)

d ρii ()f ()

where f () is the Fermi function. Moreover χ(, , ) = f (−)f (− )f (− ) + f ()f ( )f (− ). These approximations are used in order so solve Eq. (8.27) self-consistently whereby M(k, z) is replaced by Eq. (8.35). We reemphasize that in the two-site cluster approximation for fixed site i, all sites j are taken into account until convergence is achieved. For the Hubbard model on a square lattice this includes sites which are more than ten lattice vectors apart! In this respect the present theory resembles incremental schemes which

STRONGLY CORRELATED ELECTRONS

159

have been applied in the treatment of solids by quantum chemistry methods.366 For a review see Ref. [41]. The self-consistent projection method (SCPM) provides an interesting link between treatments of model Hamiltonians in solid state theory and true ab initio calculations with controlled approximations based on methods used in quantum chemistry. Our theory differs from extensions of the DMFT such as the Dynamical Cluster Approximations367 or the Cellular Dynamical Mean-Field Theory368 where clusters of connected sites are treated. They require a truly impressive amount of numerical work and have been carefully reviewed in Ref. [369]. Determining M(k, ω) might look like a very demanding computational problem too, but that is not really the case. In fact, we can calculate M(k, ω) directly without a numerical analytic continuation from the imaginary axis as is the case in other schemes.369 Therefore a high numerical resolution as regards energy and momentum can be obtained. The following results are obtained for U = 8|t| and T = 0 in the underdoped regime, i.e., for n 1. At half-filling, the system will always be an antiferromagnetic insulator due to nesting. But in the effective medium approach described here one finds in addition also a paramagnetic metallic solution. We use the latter here, being aware of the fact that an arbitrarily small temperature or doping concentration will destroy antiferromagnetic order in two dimensions (Mermin– Wagner theorem). A metallic solution does exist only for U < Ucrit where in single-site approximation Ucrit 14|t| is obtained. Therefore with a value of U = 8|t| we are still in the metallic regime. We find that a flat quasiparticle band is crossing the Fermi energy EF . There is also an empty upper Hubbard band found which is centered around the M point and there is incoherent spectral density near the point resulting from the lower Hubbard band. The results compare well with those of Quantum Monte Carlo (QMC) calculations for finite temperatures.370–372 This is seen in Figure VIII.4. The Fermi surface for n = 0.95 (underdoped regime) is found to be hole like. This is due to a collapse of the lower Hubbard band which causes a portion of the flat quasiparticle band near the X point to sink below EF . These findings are contrary to expectations from the Hubbard I approximation. From (8.22) it is seen that within that approximation the spectral weight of the lower Hubbard band increases while that of the upper Hubbard band decreases in case of hole doping n < 1. In the present, improved approximation this is not the 366 H. Stoll, Phys. Rev. B 46, 6700 (1992). 367 M. H. Hettler, M. Mukherjee, M. Jarrell, and H. R. Krishnamurthy, Phys. Rev. B 61, 12739 (2000). 368 G. Kotliar, S. Savrasov, G. Pallson, and G. Biroli, Phys. Rev. Lett. 87, 186401 (2001). 369 T. Maier, M. Jarrell, T. Pruschke, and M. H. Hettler, Rev. Mod. Phys. 77, 1027 (2005). 370 N. Bulut, D. J. Scalapino, and S. R. White, Phys. Rev. Lett., Phys. Rev. 73, 50, 748, 7215 (1994). 371 R. Preuss, W. Hanke, and W. von der Linden, Phys. Rev. Lett. 75, 1344 (1994). 372 C. Gröber, R. Eder, and W. Hanke, Phys. Rev. B 66, 4336 (2000).

160

P. FULDE ET AL.

F IG . VIII.4. Single-particle excitations at zero temperatures for the Hubbard model on a square lattice in units of the nearest-neighbor transfer integral t . Dashed line: Hartree–Fock result. Open circles with error bars: QMC results for T = 0.33.372 (After Ref. [355].)

case for small hole doping and implies that Luttinger’s Theorem30 does not apply here. It would require a reduction of the volume enclosed by the Fermi surface with increasing hole concentration. For n = 0.8 (overdoped regime) an electronlike Fermi surface is found. These results are in agreement with the Dynamical Cluster Approximation373 and with QMC calculations.370–372 An important finding is that for doping less than 2% the effective mass mk changes strongly between the M point, i.e., [π, π] where it is minimal and the X point, i.e., [π, 0] where it has its maximum. It is computed numerically from mk = 1 − U 2 Re ∂M(k, ω)/∂ω|ω=0+ . Near the X point one finds that the smaller the δω steps are in computing the derivative, the larger becomes mk=X . One finds that approximately mk ∼ ln δω, indicating marginal Fermi liquid behavior. The marginal Fermi liquid theory46,47,374,375 had been designed in order to explain a number of features, observed in the normal state of the high-Tc cuprates where electron correlations are strong. They deviate from normal Fermi liquid behavior. Most noticeable is a linear temperature dependence of the resistivity ρ(T ) ∼ T which has been observed, e.g., in doped La2 CuO4 materials. It is suggestive to associate this dependence with a quasiparticle scattering rate 1/τ (T ) ∼ ρ(T ), i.e., τ −1 ∼ Im (T ) ∼ T . Then it is plausible to assume that for T < |ω| the corresponding expression is Im (ω) ∼ |ω|. Indeed, optical reflectivity measurements 373 T. A. Maier, T. Pruschke, and M. Jarrell, Phys. Rev. B 66, 075102 (2002). 374 C. M. Varma, P. B. Littlewood, S. Schmitt-Rink, E. Abrahams, and A. Ruckenstein, Phys. Rev.

Lett. 64, 497 (1990). 375 G. T. Zimanyi and K. S. Bedell, Phys. Rev. B 48, 6575 (1993).

STRONGLY CORRELATED ELECTRONS

161

F IG . VIII.5. Phase diagram for the Hubbard model on a square lattice as function of hole doping δn. In the upper shaded region two self-consistent solutions are found one of which corresponds to a marginal and the other to a normal Fermi liquid. In the lower shaded region two slightly different marginal Fermi liquid solutions are found. (After Ref. [355].)

on YBa2 Cu3 O4 are in accordance with this form.376 But also the frequencydependent spin susceptibility at low T shows marginal Fermi liquid behavior. Real and imaginary part of (k, ω) are related to each other via a Kramers– Kroning relation from which is follows that Re (ω) ∼ ω ln(ω/ω0 ) where ω0 is a cut-off parameter. From this form of Re (ω) we conclude that the residuum of the Green’s function pole (see Eq. (8.2)) is Z(ω) ∼ 1/| ln(ω/ω0 )| and that the quasiparticle mass mk diverges at the Fermi energy like mk ∼ | ln(ω/ω0 )|. The above treatment shows that a marginal Fermi liquid type of behavior can be obtained from a Hubbard Hamiltonian on a square lattice, provided one is in a certain U dependent doping regime. We expect that this region will be enlarged when long-range antiferromagnetic correlations are taken into account which have been neglected here. The phase diagram in the U vs. δn plane is shown in Figure VIII.5, where δn denotes hole doping. There are two small regions in which two self-consistent solutions are found. They separate the marginal Fermi liquid regime from the normal Fermi liquid one. For smaller U values the cross-over between the two regimes is continuous. It is instructive to consider the origin of the marginal Fermi-liquid like behavior of the self-energy. For half-filling a van Hove singularity shows up in the density of states at EF which leads, as is well known, to a self-energy of marginal Fermi liquid type. With hole doping this singularity moves rather fast away from EF pro376 R. T. Collins, Z. Schlesinger, F. Holtzberg, P. Chaudhari, and C. Feild, Phys. Rev. B 39, 6571

(1989).

162

P. FULDE ET AL.

F IG . VIII.6. Schematic drawing of the dispersion ω(k) near kF in the presence of a kink.

vided correlation effects are small.377–379 But when U is large as assumed here, and for small hole doping spectral density moves to high energies and therefore EF remains virtually pinned to the van Hove singularity. This changes at higher doping concentrations where EF moves to lower energies and normal Fermi liquid behavior is recovered. It is interesting that for small hole doping the calculations for U = 8|t| show a kink in the excitation spectrum at approximately ωkink = −0.8|t|. A kink has been observed in high-resolution photoemission experiments in the quasiparticle band dispersion of high-Tc cuprates.357,358 It was found that along the nodal direction (0, 0) − (π, π) the effective Fermi velocity vF as defined by the form ω(k) = vF (k)(|k| − kF ) is neither sensitive to the type of cuprate, nor to doping concentration or isotope substitution380 as long as ω < ωkink (= 60–70 meV). But when ω > ωkink a strong dependence of vF on those quantities as well as on k is observed. The form of the dispersion is schematically shown in Figure VIII.6. There have been two possible explanations advanced for this experimental observation. One is based on a coupling of electrons to the longitudinal optical phonon mode found in inelastic neutron scattering experiments.358 The other is based on a coupling of the electronic quasiparticles to spin fluctuations, in particu377 A. Virosztek and J. Ruvalds, Phys. Rev. B 42, 4064 (1990). 378 H. Schweitzer and G. Czycholl, Z. Phys. B 83, 93 (1991). 379 G. Kastrinakis, Physica C 340, 119 (2000). 380 G.-H. Gweon, T. Sasagawa, S. Y. Zhou, J. Graf, H. Takagi, D.-H. Lee, and A. Lanzara, Nature

430, 187 (2004).

STRONGLY CORRELATED ELECTRONS

163

F IG . VIII.7. Hubbard model on a square lattice near half-filling. Contours of spectral function of excitations along M– for hole doping δn = 0.01 showing a kink. (After Ref. [356].)

lar to an observed resonance mode.362,363,381 No consensus has been reached yet. So it is interesting to note that a kink is also obtained from the Hubbard model on a square lattice for small doping concentrations. Here it is based on long-ranged electron correlations. In Figure VIII.7 we show the excitation spectrum near EF for a small hole concentration of δn = 0.01 and U = 8|t| as before356 (compare with Figure VIII.4). As before, the calculations assume a paramagnetic ground state. The kink structure becomes weaker as the doping concentration increases while the kink position changes little with δn. For δn = 0.05 the kink has disappeared together with the remnants of the lower Hubbard band. The ratio of the Fermi velocities vF /vF above and below ωkink is found to be vF /vF = 1.8 for δn = 0.01 and 1.5 for δn = 0.02. The kink is caused by a hybridization of the quasiparticle excitation with short-range antiferromagnetic fluctuations. With decreasing antiferromagnetic correlations, e.g., by hole doping the kink structure does also decrease and eventually disappears. Whether or not it provides an explanation for the observed kink in the underdoped regime of La2−x Srx CuO4 remains an open question. 22. N ICKEL AND ITS S ATELLITE Photoelectron spectroscopy has revealed a pronounced satellite structure in Ni metal which is approximately 6 eV below the Fermi energy EF .331 It is due to 381 A. V. Chubukov and M. R. Norman, Phys. Rev. B 70, 174505 (2004).

164

P. FULDE ET AL.

strong electron correlations and a number of different theoretical model calculations have been performed to explain it. The simplest way of including correlations is by calculating the self-energy in second-order perturbation theory.382,383 This results in a d-band narrowing effect as well as in a satellite structure. However, for a quantitative comparison with experiments this is not sufficient. Another well known method is the t-matrix approach of Kanamori.21 It accounts for multiple scattering of two d-holes, but it is strictly valid only in the cases of small or almost complete band filling. It has been used to explain the satellite structure384,385 and was subsequently extended to include also multiple electronhole scattering.386–388 These calculations establish also a link to calculations based on couplings of a hole to magnons.389–392 There have been also numerical diagonalizations based on a 4-sites tetrahedral cluster with five d-orbitals per site.393 A correctly positioned multiplet structure was obtained for ferromagnetic Ni but more detailed information is beyond the scheme of that approach. Other calculations were based on a LDA+DMFT approach394 and on a Gutzwiller projected wavefunction.395 In the latter case band narrowing but no satellite structure was obtained. Here we want to start from a five-band Hubbard model and to calculate the spectral density for paramagnetic Ni with the help of the projection operator method.396 It gives good insight into the relevant microscopic processes which contribute to the satellite and are described by the set of operators {Aν } (see Eq. (8.6)). The results are found to be similar to those obtained when the twohole one-electron t matrix is solved by employing Faddeev’s equations.397

382 G. Treglia, F. Ducastelle, and D. Spanjaard, J. Phys. (Paris) 41, 281 (1980). 383 G. Treglia, F. Ducastelle, and D. Spanjaard, J. Phys. (Paris) 43, 341 (1982). 384 D. R. Penn, Phys. Rev. Lett. 42, 921 (1979). 385 A. Liebsch, Phys. Rev. Lett. 43, 1431 (1979). 386 A. Liebsch, Phys. Rev. B 23, 5203 (1981). 387 J. Igarashi, J. Phys. Soc. Jpn. 52, 2827 (1983). 388 J. Igarashi, J. Phys. Soc. Jpn. 54, 260 (1985). 389 L. Roth, Phys. Rev. B 186, 428 (1969). 390 J. A. Hertz and D. M. Edwards, J. Phys. C 3, 2174 (1973). 391 J. A. Hertz and D. M. Edwards, J. Phys. C 3, 2191 (1973). 392 H. Matsumoto, L. Umezawa, S. Seki, and M. Tachiki, Phys. Rev. B 17, 2276 (1978). 393 R. H. Victora and L. M. Falicov, Phys. Rev. Lett. 55, 1140 (1985). 394 A. I. Lichtenstein, M. I. Katsnelson, and G. Kotliar, Phys. Rev. Lett. 87, 067205 (2001). 395 J. Bünemann, F. Gebhard, T. Ohm, R. Umstätter, S. Weiser, W. Weber, R. Claessen, D. Ehm, A. Harasawa, A. Kakizaki, et al., Europhys. Lett. 61, 667 (2003). 396 P. Unger, J. Igarashi, and P. Fulde, Phys. Rev. B 50, 10485 (1994). 397 J. Igarashi, P. Unger, K. Hirai, and P. Fulde, Phys. Rev. B 49, 16181 (1994).

STRONGLY CORRELATED ELECTRONS

165

We write the five-band Hubbard Hamiltonian for the d electrons of Ni in the following form

H1 (l) H = H0 + H0 =

l

ν (k)nνσ (k)

kνσ

H1 (l) =

1

† † Vij mn aiσ (l)amσ (l)anσ (l)aj σ (l). 2

(8.40)

ij mn σ σ

Here l is a site index and i, j, m, n denote different d orbitals. The ν (k) with ν = 1, . . . , 5 are the energy dispersions of canonical d-bands obtained by solving a one-particle equation. We use for them the LDA bands being aware of the † ckνσ fact that they contain already some correlation effects. The nνσ (k) = ckνσ are number operators for Bloch states with quantum numbers k, ν and σ . Their † (l) through creation operators are expressed in terms of the basis operators aiσ 1

† † ckνσ =√ ανn (k)eikRl anσ (l) (8.41) N0 ln where N0 is the number of sites. The interaction matrix elements in (8.40) are of the form Vij mn = Uim δij δmn + Jij (δin δj m + δim δj n ) Uim = U + 2J − 2Jim

(8.42)

where U and J are average values of the Coulomb- and exchange interaction, respectively. The matrix Jij can be expressed in terms of J and a single anisotropic parameter J provided we deal with a cubic lattice as is the case here. For more details we refer, e.g., to Refs. [398,399]. When electronic correlations are neglected the ground state is of the form † ckνσ |0. (8.43) |0 = |k| 0 n n jz 0 n0 Ajz (k, ω) = (8.47) (N −1) cj (k) (N ) 2 δ ω + ω(−) , ω < 0 z n n 0 n0 with cjz (k) =

a

eika cjz (a),

(±) ωn0 = En(N ±1) − E0(N ) .

(8.48)

STRONGLY CORRELATED ELECTRONS

169

F IG . VIII.10. Configurational energies vs. 5f -valence for the microscopic model adopted to describe the U sites. For a qualitative discussion, the value U0 is treated as a parameter since it is screened in a metal and concomitantly will depend upon the crystallographic environment of the U site.

It yields the probability for adding (ω > 0) or removing (ω < 0) a 5f electron with energy ω in a state characterized by momentum k and angular momentum (N ) (N ) projection jz to the N -particle ground state |0 with energy E0 . The states (N ±1) (N ±1) and En , respectively. with N ± 1 and their energies are denoted by |n The notation was introduced in Section V. The structure of the spectra in the strong-coupling limit can be understood by considering the atomic limit where the system is modeled as a statistical ensemble of isolated 5f atoms. The absence of pronounced valence peaks in the photoemission and inverse photoemission spectra suggests that the energies of the f 2 - and f 3 -configurations, are (almost) degenerate i.e., E(5f 2 ) = E(5f 3 ). The variation with 5f -valence of the configurational energies E(f n ) is shown schematically in Figure VIII.10. The ground state will mainly involve 5f 2 and 5f 3 configurations. The corresponding spectral functions are obtained in close analogy to the classical work of Hubbard.7 Let us first consider the zero configuration-width approximation which neglects intra-atomic correlations. The valence transitions f 2 → f 1 and f 3 → f 4 occur at high energies set by the isotropic average of the Coulomb interaction and, concomitantly, do not affect the low-temperature behavior. The latter is determined by the low-energy peak resulting from the transitions f 2 ↔ f 3 within the f 2 - and f 3 -configurations. This peak is a direct consequence of the intermediate-valent ground state. The distribution among the peaks can be estimated from combinatorial considerations. The weight Z(f 2 → f 1 ) of the transition f 2 → f 1 equals the probability that a state with a given jz is occupied in that

170

P. FULDE ET AL.

F IG . VIII.11. Left panel: Multiplets for f 2 and f 3 configurations of the U model in the atomic limit. The levels are obtained by diagonalizing the Coulomb matrix using j -j coupling and Coulomb parameters of UPt3 . Right panel: Spectral function for the model in the atomic limit.

f 2 contribution of the mixed-valent ground-state. Following these lines one finds 1 Z f2 →f1 = , 6 3 1 Z f →f2 = , 4

1 Z f2 →f3 = 3 3 1 Z f →f4 = 4

(8.49)

The central focus is the evolution of the low-energy peak whose spectral weight sums up to 7/12 (= 1/3 + 1/4). Intra-atomic correlations which are usually described by Hund’s rules yield the multiplets displayed schematically in Figure VIII.11. The values for the excitation energies are calculated from the Coulomb parameters of UPt3 adopting j -j -coupling. In the atomic limit the model spectral function has a low-energy peak resulting from transitions between the Hund’s rule ground-state manifolds |f 2 , J = 4, Jz and |f 3 , J = 9/2, Jz as well as peaks corresponding to transitions into excited multiplets. Due to the rotational invariance of the Coulomb interaction, the spectral functions do not despectral weights for the phopend upon the magnetic quantum number jz . The 1 2 3 toemission and inverse photoemission parts, 10 Jz |f , J , Jz − jz |cjz |f , J = † 9/2, Jz |2 and 19 Jz |f 3 , J , Jz + jz |cjz |f 2 , J = 4, Jz |2 are easily obtained by expressing the matrix elements in terms of reduced matrix elements and Clebsch– Gordan coefficients. The excitation energies as well as the corresponding spectral weights are listed in Table VIII.1. We should like to mention that there is no transition into the excited multiplet |f 2 , J = 0. The model therefore predicts 5f spectral weight at 1 eV binding energy in the photoemission spectra from U-based heavy fermion compounds. The position of these 5f structures should not depend sensitively on the actual crystalline environment since they result from intra-atomic excitations. The weights, however,

STRONGLY CORRELATED ELECTRONS

171

TABLE VIII.1. P OSITIONS AND S PECTRAL W EIGHTS OF THE ATOMIC T RANSITIONS IN U RA AT Z ERO E NERGY P OSITION THE PARTICLE AND H OLE P EAKS H AVE A T OTAL W EIGHT 0.414

NIUM .

PES Position/[eV] Spectral weight

−1.06 0.054

BIS 0.00 0.196

0.00 0.218

1.60 0.032

2.73 0.083

will be altered by the reconstruction of the ground state and the low-energy excitations in an extended solid and may vary with chemical composition and temperature. These predictions seem to be in agreement with recent experiments.403 Recent photoemission studies by Fujimori et al.404 seem to indicate the presence of features in the proper energy range. The fact that they cannot be attributed to LDA energy bands further supports our interpretation in terms of multiplet side bands. An unambiguous identification, however, will require resonant photoemission experiments. 24. E XCITATIONS IN C OPPER -OXIDE P LANES It is well known that the copper-oxide based perovskites which play a major role in high-temperature superconductivity are strongly correlated electron systems. This is immediately obvious by realizing that, e.g., La2 CuO4 is an insulator and not a metal despite the fact that with one hole per unit cell one would expect a half-filled conduction band. Note that insulating behavior is found also above the antiferromagnetic transition temperature and therefore is unrelated to the doubling of the unit cell when the material becomes an antiferromagnet. Indeed, LDA calculations give an effective Coulomb repulsion of two d holes on a Cu site of Ud = 10.5 eV and a hopping matrix element of a hole from a Cu 3dx 2 −y 2 orbital to an O 2px(y) orbital of tpd = 1.3 eV. Therefore the bandwidth is small as compared with Ud . The strong correlations lead to a single-particle spectral density which is quite distinct from the one of weakly correlated electrons. In fact, the excitations are dominated by the internal degrees of freedom of the correlation hole so that the one-particle or coherent part of Green’s function plays a secondary role here. This will become clear towards the end of this section. We shall use again a model Hamiltonian although an ab initio calculation would be highly desirable. We want to write it in hole representation in the form of a 403 R. Eloirdi, T. Gouder, F. Wastin, J. Rebizant, and F. Huber, preprint (2005). 404 S. Fujimori, private communication (2005).

172

P. FULDE ET AL.

F IG . VIII.12. Cu and O orbitals accounted for in the 3-band Hubbard Hamiltonian (8.53).

three-band Hubbard or Emery model. The unit cell consists of one Cu 3dx 2 −y 2 orbital and two O 2px(y) orbitals (see Figure VIII.12). The orbital energies are d and p . Two holes on a Cu site repel each other with Ud and on a O site with Up . The hopping matrix element between a Cu orbital and an O orbital is tpd and tpp between the orbitals of the two O atoms. The parameter values can be derived from a constrained LDA calculation405 with the following results: Ud = 10.5 eV, Up = 4.0 eV, tpd = 1.3 eV, tpp = 0.65 eV, p − d = 3.6 eV. It is helpful to first introduce a basis of oxygen orbitals which is diagonal with respect to oxygen– oxygen hopping processes tpp . Let us denote the corresponding creation operators † by cmkσ where m is an oxygen band index. Those bands have a dispersion (m = 1, 2) (8.50) m (k) = p ± 2tpp cos k(r1 + r2 ) − cos k(r2 − r1 ) where the vectors r1 and r2 are shown in Figure VIII.12. Due to the different orientations of the O 2px(y) orbitals, the sign of tpp depends on the direction. It is positive in the direction r1 + r2 , −(r1 + r2 ) and negative in the direction r1 − r2 , r2 − r1 . Next we introduce a linear combination of oxygen orbitals which possesses the same symmetry on a CuO4 plaquette as the tpd -matrix elements, i.e.,

† † = φmk cmkσ , (8.51) pkσ m

with i φmk = − √ [sin kr1 ± sin kr2 ]. 2 405 M. S. Hybertsen, M. Schlüter, and N. E. Christensen, Phys. Rev. B 39, 9028 (1989).

(8.52)

STRONGLY CORRELATED ELECTRONS

173

The model Hamiltonian we shall be using can thus be written as

† m (k)cmkσ cmkσ + Up np↑ (J )np↓ (J ) H= mkσ

+ d

† dkσ dkσ + Ud

kσ

+ 2tpd

J

nd↑ (I )nd↓ (I )

I

† pkσ dkσ + h.c. .

(8.53)

kσ

As usual npσ (J ) and ndσ (I ) are the occupation number operator of the O 2px(y) orbital on site J and of the Cu 3dx 2 −y 2 orbital on site I , respectively. With the help of the above Hamiltonian we calculate the spectral density of the Cu–O planes, with and without hole doping. For that purpose we have to choose the right set of relevant operators {An (k)}. They must include the most important microscopic processes in the strongly correlated system which generate the correlation hole of an electron. First of all, the hole operators † , Ap (m, k) = pmk

† Ad (k) = dk↑ ,

m = 1, 2

(8.54)

must be part of the set. They are supplemented by a number of local operators. In order to suppress double occupancies of the d and p orbitals due to the large values of Ud and Up , we must include d¯↑† = d↑† (I )nd↓ (I ) and p¯ ↑† = pJ† ↑ np↓ (J ), i.e., their Fourier transforms 1 −ikRI ¯ † e dI ↑ Ad (k) = √ N J Ap (k) = √

1 2N

e−ikRJ p¯ J† ↑

(8.55)

J

where N is the number of Cu sites and there are two O sites per Cu site. In addition we want to account for spin flips of d holes at Cu sites in combination with spin flips at neighboring O sites. Those processes are important for the formation of a Zhang–Rice singlet.406 This is a singlet state formed by a hole at a Cu site and another one at a nearest-neighbor O site. The corresponding microscopic operator is 1 −ikRI † + e p˜ I ↑ SI Af (k) = √ N I 406 F. C. Zhang and T. M. Rice, Phys. Rev. B 37, 3759 (1988).

(8.56)

174

P. FULDE ET AL.

where 1 † † † † p1σ + p2σ (8.57) − p3σ − p4σ 2 is a superposition of the four O 2p orbitals which surround the 3d orbital of Cu site I . The operator SI+ = dI+↑ dI ↓ . For a possible formation of triplet states also the operator 1 −ikRI † Aa (k) = √ e p˜ I ↑ nd↓ (I ) (8.58) N I p˜ I†σ =

is needed. In order to describe charge transfer in the vicinity of an added hole we also include 1 −ikRI † † Ac (k) = √ e pI ↑ pI ↓ d I ↓ . (8.59) N I This completes the choice of the set {Aν (k)}. With 9 operators Aν (k) we have to diagonalize for each k point (9 × 9) matrices Lμν and χμν (see (8.12)). The static expectation values which enter the matrix elements are determined from the spectral functions to which they are related via +∞ † ψ0 Am (k)An (k) ψ0 = dω f (ω)Amn (k, ω) (8.60) −∞

with β = (kB T )−1 is the Fermi distribution function. where It can be replaced by a step function. By solving Eq. (8.60) self-consistently the static correlation functions are obtained. For more details we refer to the original literature.407,408 The resulting density of states are shown in Figure VIII.13 for the half-filled case as well as for 25% of hole doping. The two cases are supposed to simulate La2 CuO4 and La2−x Srx CuO4 , respectively. The agreement with results of exact diagonalization of a small cluster containing four CuO2 units409 is very good. It is noticed that at half filling the system is insulating and a gap is present. Around ω = 0 one notices the O 2p band and a 3d component due to hybridization. The upper Hubbard band is centered at 5tpd . The structure near −7tpd results mainly from Ad (k) and is interpreted as the lower Hubbard band. The peak near −4tpd comes mainly from Ac (k), i.e., from charge fluctuations. The structure close to 2.5tpd marks the Zhang–Rice singlet state. It is important for the interpretation of spectroscopic experiments.410 When the system is doped f (ω) = [eβω

+ 1]−1

407 P. Unger and P. Fulde, Phys. Rev. B 48, 16607 (1993). 408 P. Unger and P. Fulde, Phys. Rev. B 47, 8947 (1993). 409 T. Tohyama and S. Maekawa, Physica C 191, 193 (1992). 410 H. Romberg, M. Alexander, N. Nücker, P. Adelmann, and J. Fink, Phys. Rev. B 42, 8768 (1990).

STRONGLY CORRELATED ELECTRONS

175

F IG . VIII.13. Spectral density of Cu–O planes described by the Hamiltonian (8.53); (a) at half-filling; (b) for 25% hole doping. Solid and dashed lines show the Cu and O contributions. In the hole doped case spectral density has been shifted from the upper Hubbard band to the region near EF (dotted line). Parameters are Ud = 8, Up = 3, tpp = 0.5, tpd = 1, p − d = 4. Compare also with Figure VIII.14. (After Ref. [407].)

with holes the Fermi energy moves into the Zhang–Rice singlet band. Simultaneously there is a transfer of spectral density taking place from the upper Hubbard band to energies below EF . As mentioned at the beginning of this section we are dealing here with a situation where the internal degrees of freedom of the correlation hole dominate the spectral density. This is most clearly seen by comparing the density of states for the half-filled case with the one obtained in the independent electron approximation. The latter is shown in Figure VIII.14a. It consists of a bonding, nonbonding and antibonding part. The splitting of the d electron contributions into a lower and upper Hubbard band is schematically shown in Figure VIII.14b and the singlettriplet splitting in Figure VIII.14c. The difference between Figures VIII.13a and b demonstrates nicely the effect of the excitations of the correlation hole.

176

P. FULDE ET AL.

F IG . VIII.14. Schematic representation of the density of states of a Cu–O plane described within a 3-band Hubbard model. (a) Independent electron approximation. A, B, NB denote antibonding, bonding and nonbonding part. (b) Splitting of the d band into a lower (LHB) and upper (UHB) Hubbard band. (c) Singlet-triplet splitting (S, T) S = Zhang–Rice singlet.

IX. Summary and Outlook

The different topics we have discussed in this review concern mainly low energy effects of strongly correlated electrons, though not exclusively. In Section VIII we have also given examples of high energy features like shadow bands, satellites and kink effects which originate from strong electron correlations. Low energy effects are mainly due to heavy quasiparticles consisting of an electron with its (rigid) correlation hole. The latter is very pronounced when correlations are strong and therefore an electron moves with a reduced Fermi velocity through the system dragging the correlation hole with it. Low temperature properties are strongly influenced by the effective mass of the quasiparticles. Important examples are Ce-based heavy fermion metals where an interplay of strong on-site 4f Coulomb correlations and hybridization with conduction electrons leads to the heavy quasiparticle mass. These features may be described within Renormalized Band Theory by assuming periodic scattering with a resonant phase shift. This way one obtains the proper heavy quasiparticle bands and the Fermi surface. In recent years it has been realized that in U-based heavy fermion compounds like, e.g., UPd2 Al3 heavy quasiparticles originate from a special mechanism: the 5f electrons form a two-component system with some itinerant and some localized

STRONGLY CORRELATED ELECTRONS

177

orbitals and the renormalization of the former via intra-atomic excitations of the localized 5f electrons leads to strong mass enhancements. In fact, this mechanism has also been identified as the origin of superconductivity in UPd2 Al3 which is not based on electron–phonon interactions. We have also given examples where the low energy excitations cannot simply be described by a Fermi liquid of heavy quasiparticles. In general, even in weakly correlated metals, one expects non-Fermi liquid behavior close to quantum phase transitions. The earliest examples are the logarithmic corrections to the linear specific heat term coming from electrons dressed by paramagnon excitations close to a ferromagnetic quantum critical point. By now numerous examples of mostly Ce-based heavy fermion metals have been found where the vicinity to an AF quantum phase transition leads to pronounced non-Fermi liquid anomalies. Their microscopic understanding is still at an early stage. A different type of deviation from the Fermi liquid picture emerges in strongly correlated electron compounds which exhibit Wigner-lattice type charge order as is the case, e.g., in Yb4 As3 . Here spin and charge degrees of freedom which are responsible for low energy excitations may belong to different types of electrons, i.e., they appear to be separated. In the example of Yb4 As3 the spin degrees of freedom involve 4f holes of Yb while the charge degrees of freedom were found to be due to As 4p holes. The spins of 4f holes are aligned along chains and the 1D neutral spinon excitations cause the large linear specific heat term while light 4p holes carry the current. Quite generally charge ordering in 3d or 4f mixed-valent systems is a promising route to obtain low-dimensional spin structures. An example is NaV2 O5 . There the 1D spin excitations that emerge via charge ordering interact with the lattice leading to a spin-Peierls type dimerization and spin-gap formation. An even stronger kind of lattice coupling occurs in the manganites which leads to polaron formation. The intersite Coulomb correlations then drive charge order of polaronic quasiparticles as observed in the bilayer-manganites. The nonstoichiometric compounds of this class are examples of strong Hund’s rule correlations of itinerant (eg ) and localized (t2g ) electrons. This leads to almost ideal 2D ferromagnetic order driven by kinetic or double exchange mechanisms. Another deviation from a simple Fermi liquid heavy-quasiparticle description was found for the Hubbard model on a square lattice at a particular range of doping and for U above the critical value of the metal–insulator transition at half filling. Here the excitations were of a form previously termed marginal Fermi liquid and suggested to explain some of the properties of layered cuprates. High-energy features of strongly correlated electrons result on the other hand from excitations of internal degrees of freedom of the correlation hole. While the slowly moving quasiparticle has a low excitation energy the internal excitations of its cloud correspond to high energies and show up as satellite structures in photoelectron spectroscopy. Examples were given in Section VIII.

178

P. FULDE ET AL.

In which direction will research on the theory of strongly correlated electrons develop in the future? Here one can only speculate at the risk of being completely wrong. Firstly, there is the field of electronic structure calculations. After LDA based density functional calculations turned out to describe insufficiently strongly correlated electrons they were combined successfully with other approaches to improve on the shortcomings. As discussed in this review Renormalized Band Structure calculations showed considerable predictive power. But also LDA+U and LDA+GW schemes have been applied and yielded insight into strongly correlated electrons. However the more corrections are added to the original approximation to density functional theory like LDA, the less controlled the results are. Double counting of correlation contributions or screening is one of the uncertainties, accounting for the spatial extend of the correlation hole is another. The latter is a problem which also dynamical mean-field theory (DMFT) is facing in its present form. Extensions of that theory to clusters369 are desirable but difficult to realize in practice. This suggests that over the long run wavefunction-based approaches using quantum chemical methods may be a possible solution to the problem. They are technically very demanding but they are well controlled and allow for a detailed understanding of different correlation processes. They may have a great future.41 Exact diagonalizations will certainly also play their role in the future. Usually they use model Hamiltonians with model parameters obtained from single particle LDA(+U) calculations. With increasing possibilities to treat larger clusters they will lead to much new insight into the nature of the correlated ground state as well as the excitations responsible for low temperature thermodynamic anomalies. Analyses of the excitation spectrum of correlation holes seem to be a very promising field. By projecting the calculations onto a few selected variables which represent the most important degrees of freedom, insight may be gained about the relative importance of different correlations. We expect considerable extensions of our understandings of elementary excitations here. As was shown in Section VII in special lattices (here geometrically frustrated ones) it may happen that an electron added to the system may separate into two parts when correlations are strong. This may give raise to charge fractionalization, a phenomenon known from the fractional quantum Hall effect (FQHE).40 Even if there is a weak restoring force between the two parts we would have “quasiparticles” of considerable spatial extent. They would have little in common with the usual picture of an electron surrounded by a correlation hole. Interestingly enough, certain analogies to field theories in elementary particle physics do appear here when dealing with confinement and deconfinement.317,320 After all, why should nature restrict itself to realize certain basic properties only in one particular field of physics and not in others too?

STRONGLY CORRELATED ELECTRONS

179

Acknowledgment

We thank Prof. Y. Kakehashi for a critical reading of Section VIII and for helpful comments. Last not least we thank Mrs. Regine Schuppe for carefully preparing the manuscript. L IST OF ACRONYMS AF ARPES BEC BZ CDW CEF CMR CO CPA DE dHvA DOS DM DMFT EHM e-p FL FM FQHE FS HF ICM INS ISSP ITF JT JW KS LDA LSDA n.n. n.n.n.

antiferromagnet angle resolved photoemission spectroscopy Bose–Einstein condensation Brillouin zone charge density wave crystalline electric field colossal magnetoresistance charge order coherent potential approximation double exchange de Haas–van Alphen density of states Dzyaloshinsky–Moriya dynamical mean-field theory extended Hubbard model electron–phonon Fermi liquid ferromagnet fractional quantum Hall effect Fermi surface heavy fermion or Hartree–Fock incommensurate magnet inelastic neutron scattering Ising-spin-Peierls Ising model in transverse field Jahn–Teller Jordan–Wigner Kondo singlet local density approximation local spin density approximation nearest neighbor next nearest neighbor

180

NCA NFL NMR ODLRO PM QCP QMC QPT RPA RKKY SCF SCPM SDW TB WFM

P. FULDE ET AL.

non-crossing approximation non-Fermi liquid nuclear magnetic resonance off-diagonal long range order paramagnet quantum critical point quantum Monte Carlo quantum phase transition random phase approximation Ruderman–Kittel–Kasuya–Yoshida self-consistent field self-consistent projection method spin density wave tight binding weak ferromagnet

SOLID STATE PHYSICS, VOL. 60

Defect-Induced Dynamic Pattern Formation in Metals and Alloys

Y VES B RÉCHET Laboratoire de Thermodynamique et Physico-Chimie Métallurgiques, Institut National Polytechnique de Grenoble, 38402, St. Martin D’Hères, France

C HRISTOPHER H UTCHINSON Department of Materials Engineering, Monash University, Clayton, 3168, Vic, Australia

I. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1. Chemical Patterning . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2. Structural Patterning in Systems Prepared Far from Equilibrium . . . . . . . . . . . 3. Structural Patterning in Systems Maintained Far from Equilibrium . . . . . . . . . . 4. Spatio-Temporal Patterning in Plasticity . . . . . . . . . . . . . . . . . . . . . . . . . II. Free Energy Changes, Driving Forces and Energy Input . . . . . . . . . . . . . . . . . . 5. Systems Prepared Far from Equilibrium . . . . . . . . . . . . . . . . . . . . . . . . . 6. Systems Maintained Far from Equilibrium by the Continuous Input of Energy . . . . III. Chemical Patterning: Interface-Mediated Transformations: Eutectoid Decomposition and Discontinuous Precipitation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7. Steady State Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8. The Spacing Selection Problem . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9. Non-Steady State Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10. Coarsening and Related Morphological Evolution . . . . . . . . . . . . . . . . . . . 11. Multilayer Stability . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . IV. Structural Defect Patterning: Grain Growth, Recovery and Recrystallization . . . . . . . 12. Grain Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13. Recovery and Recrystallization of Dislocation Structures . . . . . . . . . . . . . . . V. Structural Defect Patterning: Irradiation and Plastic Deformation . . . . . . . . . . . . . 14. Irradiation Induced Patterning . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15. Plasticity Induced Patterning . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . VI. Spatio-Temporal Patterning in Plasticity: The Portevin–Le Chatelier Effect . . . . . . . . 16. Phenomenology of Portevin–Le Chatelier Effect . . . . . . . . . . . . . . . . . . . . 17. Statistical Analysis of Serrated Flow: An Example of Self Organized Criticality (SOC) 18. Portevin–Le Chatelier Effect: An Example of Deterministic Chaos . . . . . . . . . . VII. Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

182 185 186 187 187 188 188 191 192 197 213 218 225 232 233 234 240 248 249 255 273 274 276 282 285

181 ISBN 0-12-607760-6 ISSN 0081-1947/06

© 2006 Elsevier Inc. (USA) All rights reserved.

182

Y. BRÉCHET AND C. HUTCHINSON

I. Introduction

There has recently developed within the non-linear physics community, a deep interest in the formation of ‘patterns’ in condensed matter systems driven far from equilibrium. Patterns are a concept somewhat vague and subjective. We will speak of spontaneous pattern formation when a spatial distribution of matter, or the temporal response of a solid to an external stimulus presents some sort of regularity which has a lower symmetry than its cause. The ideal regularity is periodicity, but one may also consider the possible order in apparently chaotic behavior, or the length scales appearing in an initially homogeneous body. After the extensive work done in fluid mechanics where numerous examples of spontaneous pattern formation may be found (e.g., see Refs. [1,2]), and where the non-linear equations to be solved are well established, solidification seemed to be another of these areas to which the non-linear physicist could apply his methods to model the spontaneous emergence of patterns (dendritic forms and cellular and eutectic structures). Since the classic review paper by Langer,3 a number of new mathematical techniques (e.g., solvability theory) or numerical methods (phase field, cellular automata)4 have been developed to describe and predict the shapes and scales observed when going from the liquid to the solid. For both fluid mechanics and solidification, the dynamic equations to be solved (Navier–Stokes equation, and mass and heat transfer equation) are defined without ambiguity, and the problem is primarily to analyze and solve them. Similarly, the spontaneous patterning (both in space and time) that can be observed in chemical reactions has also attracted significant recent attention, particularly from the ‘Belgian school’. These systems have been labeled ‘dissipative structures’5–7 and in such situations, the transport of matter is often by a diffusion mechanism. The variety of possible ‘intermediate reactions’ leads to a much wider range of partial differential equations than in fluid mechanics or solidification, but the methods currently used to find the conditions for instabilities and their development are quite similar. 1 S. Chandrasekhar, Hydrodynamic and Hydromagnetic Stability, Dover (1981). 2 P. Berge, Y. Pomeau, and C. Vidal, Order within Chaos: Towards a Deterministic Approach to

Turbulence, Wiley, New York (1987). 3 J. S. Langer, Rev. Mod. Phys. 52, 1 (1980). 4 H. Muller-Krumbhaar, W. Kurz and E. A. Brener, in Phase Transformations in Materials, ed. G. Kostorz, Wiley–VCH, Weinheim (2001), p. 81. 5 G. Nicolis and I. Prigogine, Self-Organization in Nonequilibrium Systems: From Dissipative Structures to Order Through Fluctuations, Wiley, New York (1977). 6 D. Walgraef, Spatio-Temporal Pattern Formation: With Examples from Physics, Chemistry, and Materials Science, Springer, New York (1997). 7 C. Vidal and H. Lemarchand, La Reaction Creatrice, Hermann, Paris (1988).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 183

Comparatively less studied by the physics community is the spontaneous patterning in the solid state. This field is also very rich in examples, but there is no equivalent of a ‘Navier–Stokes equation’ which would apply to all the patterns observed. In addition, unlike liquids, crystalline solids also contain structural defects of various dimensions (point defects (0d), dislocations (1d), grain boundaries (2d)), and these defects bring both a new complexity and a new richness to the field. The approach we will take is to present an outline of the relevant phenomena and, where they exist, to summarize the possible equations used to describe the observations and the current models developed by materials scientists to capture the complexity of the problem. The guide line of this chapter, which at the same time gives it its unity and limits its scope, is ‘spontaneous pattern formation’ in solids driven far from equilibrium, involving explicitly the role of structural defects. It is well recognized that there is an energetic cost associated with pattern formation that involves a multiplication of interfaces. This is one fundamental reason for which being far from equilibrium seems to be a necessary condition for obtaining patterns. Solids can be either prepared out of equilibrium, or maintained out of equilibrium by a continuous injection of energy from outside the system. Both cases are possible for metallic alloys, and both lead to pattern formation. For example, preparing a solid far from equilibrium can be achieved by rapidly cooling below a phase boundary of the phase diagram: the high temperature structure is then out of equilibrium. Maintaining a system out of equilibrium can be accomplished either by plastic deformation or by irradiation: we refer to such systems as ‘driven systems’ and again, in these cases, patterns may spontaneously appear. In metallic alloys, pattern formation in space can be manifested in two ways: it can be a patterning of phases of different chemical composition, such as in the decomposition of solid solutions, or it can be a patterning of the structural defects themselves as in the case of plastically deformed materials. Pattern formation in time is well know in chemistry, and ‘chemical clocks’ have been central to the development of the methods of non-linear physics.5,8 To our knowledge there is no equivalent in the solid state (except perhaps in periodic oxidation, but it is translated in space under the form of layered oxides9 ). However, under special circumstances, we can observe an equivalent in the plastic behavior of materials: ‘serrated yielding’. 8 H. Haken, Synergetics: An Introduction: Nonequilibrium Phase Transitions and Self-Organization in Physics, Chemistry, and Biology, Springer, New York (1983). 9 G. Bertrand, Solid State Phenomena 3–4, 257 (1988).

184

Y. BRÉCHET AND C. HUTCHINSON

TABLE I.1. C LASSIFICATION OF THE PATTERNING E XAMPLES P RESENTED IN THIS C HAPTER Structural defects patterning

Chemical patterning

Systems prepared far Grain growth, recovery and from equilibrium recrystallization (Section IV)

Interface-mediated phase transformations: Pearlite and Discontinuous precipitation (Section III)

Systems maintained far from equilibrium

Driven systems10 Irradiation induced precipitation and order/disorder transition, Ball milling amorphization11 Fatigue induced dissolution12

Spatial patterning (Section V) Dislocation and void self organization under irradiation. Pattern formation in plasticity (creep, fatigue...) Temporal patterning (Section VI) Serrated yielding (Portevin–Le Chatelier effect)

We have classified the various phenomena to be presented in this chapter in Table I.1. We do not claim to be exhaustive (e.g., neither pattern formation in dynamic fracture nor pattern formation in martensitic transformations is treated here, and the case of chemical patterning under irradiation has recently been reviewed in the same series10 ), but we aim to present examples which are representative both of the phenomena occurring in the solid state involving structural defects as central actors, and of the current tools used for their understanding. For systems prepared far from equilibrium that produce patterns whilst approaching the equilibrium state, thermodynamics is a natural guide: it indicates the end point of the transformation, and computing the ‘driving force’ for the evolution is meaningful. For systems maintained far from equilibrium, the situation is much more confusing, and the input of energy into the system is a key parameter, together with the ability of the system to store it or to dissipate it as heat. In these driven systems, the kinetics of the defects becomes a central issue, and therefore the modelling is bound to be much more ‘system and problem specific’. Depending on the nature of the departure from equilibrium (initially imposed or constantly maintained) the questions of driving forces and energy input must be addressed differently along with the consequences on relevant kinetic mechanisms. In a driven system, besides the natural atomic movements due to thermal activation, extra mobilities associated either with irradiation damage or with 10 G. Martin and P. Bellon, in Solid State Physics, vol. 50, eds. H. Ehrenreich and F. Spaepen, Acad-

emic Press (1997), p. 189. 11 P. Pochet, L. Chaffron, P. Bellon, and G. Martin, Ann. Chimie 22, 363 (1997). 12 Y. Brechet, F. Louchet, C. Marchionni, and J. L. Vergergaugry, Phil. Mag. A 56, 353 (1987).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 185

dislocation motion must also be taken into account. The evaluation of the contributions to the driving force and the relative magnitudes compared to the input energies will be discussed in Section II. Within this scheme, the examples to be treated can be put into perspective with other systems more familiar to the physics community. We will consider successively: chemical patterning, structural defect patterning, and spatio-temporal patterning in plasticity. 1. C HEMICAL PATTERNING There is often a thermodynamic requirement that alloys decompose, i.e., to produce, from an initially homogeneous mixture of different atomic species, phases with different compositions well separated in space. This process of decomposition, which reflects the competition between the entropic term which wins at high temperature and the enthalpic terms which dominate at low temperature, tends to bring the alloy closer to thermodynamic equilibrium. In these situations, there is a thermodynamic potential which ‘shows the way’, the free energy, and the possible kinetic paths for the alloy lead to a succession of microstructures that are spatially heterogeneous. One class of these phenomena, the diffusional decomposition of a solid solution by precipitation and/or spinodal decomposition, is familiar to the physics community. The process generates length scales and kinetic scaling laws which have been extensively studied, experimentally, theoretically, and with computer simulations (for a review, see Refs. [13,14]). At this level of generality, it does not really matter if the decomposition is in a solid or in a liquid. However, the specificity of the solid being able to sustain shear and usually having a crystalline structure introduces a new richness through the elastic effects and crystal anisotropy. Pattern formation under these conditions has been extensively studied,15–17 and leads to specific behavior as far as coarsening rates and shapes are concerned. Again, the classical tools of statistical mechanics and computer simulations have led this field to a state of maturity, and it will not be reviewed here. When decomposition is thermodynamically possible, there are various possible kinetic pathways, all compatible with the thermodynamics. One of them is to 13 R. Wagner, R. Kampmann, and P. W. Voorhees, in Phase Transformations in Materials, ed. G. Kos-

torz, Wiley–VCH, Weinheim (2001), p. 309. 14 K. Binder and P. Fratzl, in Phase Transformations in Materials, ed. G. Kostorz, Wiley–VCH, Wein-

heim (2001), p. 409. 15 P. Fratzl, O. Penrose, and J. Lebowitz, J. Stat. Phys. 95, 1429 (1999). 16 F. Larche, in Dislocations in Solids, ed. F. R. N. Nabarro, North-Holland, Amsterdam, Netherlands

(1979), p. 135. 17 A. G. Khachaturian, Theory of Structural Transformations in Solids, Wiley, New York (1983).

186

Y. BRÉCHET AND C. HUTCHINSON

take advantage of the defects in the material to find short circuits toward thermodynamic equilibrium. The decomposition, instead of taking place by a homogeneous nucleation and growth process, may take advantage of existing interfaces in the solid (most often grain boundaries) or it may proceed by creating an interface and propagating a front into the non-transformed region, to approach thermodynamic equilibrium more closely. These interface-mediated transformations lead to very nice regular patterns, which bear some similarities to those observed in solidification.18 These patterns have attracted considerable interest in materials science and we will attempt to summarize this form of solid state patterning in Section III. 2. S TRUCTURAL PATTERNING IN S YSTEMS P REPARED FAR FROM E QUILIBRIUM Metals and alloys are rarely in their state of thermodynamic equilibrium. This would be given by the phase distributions predicted by the phase diagram, and given an infinite length scale, would, in principle, lead to an interfacial energy contribution equal to zero. Even the simplest case of a solidified pure metal, usually consists of a polycrystalline structure, i.e., it contains grain boundaries which are surface defects with an associated surface energy. This is the simplest possible out of equilibrium situation which may lead to defect patterning. The phenomenon of grain growth, in spite of its simplicity, presents some features of pattern forming systems which are worth further investigations.19,20 The difference with the classical ‘domain growth with non-conserved order parameter’ familiar to the statistical physicist will be reviewed. Relying on recent simulations, some open questions on grain growth will be addressed in Section IV.12. Another way of introducing extra energy in a simple system is through plastic deformation. The dislocations stored in the material after a deformation step tend to annihilate during further annealing, bringing the system closer to thermodynamic equilibrium. This procedure may be smooth and lengthy, or it may be discontinuous and rapid. The two phenomena, referred to as recovery and recrystallization,21 are different pathways to thermodynamic equilibrium, and although they do not generate organized patterns, they lead to the evolution of patterns which in itself reveals some important differences between deformation 18 G. R. Purdy and Y. J. M. Brechet, in Phase Transformations in Materials, ed. G. Kostorz, Wiley–

VCH, Weinheim (2001), p. 481. 19 D. Weaire and S. McMurry, Solid State Physics 50, 1 (1997). 20 C. V. Thompson, Solid State Physics 55, 269 (2000). 21 F. J. Humphreys, Recrystallization and Related Annealing Phenomena, Elsevier Science, New York

(2003).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 187

structures and equilibrium structures. These aspects will be discussed in Section IV.13 with a view to understanding the patterns formed during plastic deformation (Section V.15). 3. S TRUCTURAL PATTERNING IN S YSTEMS M AINTAINED FAR FROM E QUILIBRIUM A system may be maintained out of equilibrium by a continuous input of energy. Two cases will be investigated in this section. In Section V.14 we investigate the remarkable patterns arising from irradiation damage. The input of energy is transformed at least partially into point defects and the dynamical evolution of this population (its aggregation into dislocation loops or cavities) leads to patterns which are striking by their regularity (both in scale and in crystallographic orientation). The regular networks of dislocation loops or voids and bubbles is one of the most convincing cases of pattern formation in driven systems in metallurgy. The classical methods of ‘chemical kinetics’ have been remarkably successful in explaining them. This ‘success story’ is to be contrasted with the case described in Section V.15: pattern formation in plasticity. The patterns observed are also very nice although less regular, but our understanding of them is much less complete. The comparison with pattern formation under irradiation will help in identifying both the necessary ingredients to be included in a future theory for pattern formation during plastic deformation, and the limits of the ‘chemical reaction’ approach. Recent developments from intensive computer simulations as well as stochastic approaches will be presented. 4. S PATIO -T EMPORAL PATTERNING IN P LASTICITY Patterning at the microstructural scale is only one feature of plasticity. The distribution of plastic deformation in space may not be homogeneous, and in some situations, well defined ‘plastic waves’ may travel through the sample. The stressstrain curve is then no longer smooth and the observation of ‘serrated yielding’ presents some complex features strongly reminiscent of ‘stick-slip’ behavior. We will focus our attention on the Portevin–Le Chatelier (PLC) effect, and illustrate the existence of a regime of self-organized criticality (SOC),22 and of deterministic chaos.2 22 H. J. Jensen, Self-Organized Criticality, Cambridge University Press, Cambridge (1998).

188

Y. BRÉCHET AND C. HUTCHINSON

II. Free Energy Changes, Driving Forces and Energy Input

We have classified the different flavors of defect-induced solid state patterning according to whether they occur in systems prepared far from equilibrium whilst approaching equilibrium or whether they occur in systems that are maintained far from equilibrium by some external input of energy (Table I.1). This classification not only provides a nice physical picture of the differences between the two types of patterning systems but also highlights the important fundamental difference that necessitates different theoretical approaches. As we shall see in the coming chapters, the relative success we have had in describing and explaining the patterning observed in the solid state, accurately reflects the relative maturity of the theoretical framework available for the two types of systems. 5. S YSTEMS P REPARED FAR FROM E QUILIBRIUM The systems in which patterning is observed during an approach to equilibrium include interface-mediated chemical patterning and defect patterning in grain growth, recrystallization and recovery. Under isothermal conditions, these systems can be considered to be ‘closed’ in a thermodynamic sense and well defined initial and final states can be identified using classical thermodynamics. A thermodynamic potential, ‘the free energy’, can be defined and the change in this potential in going from the initial state to the final state can be quantified. The contributions to this free energy change that are interest to us are usually classified as chemical energy, strain energy and interfacial (surface) energy and we shall discuss these further in a moment. However, we are interested in dynamic pattern formation. This is the spontaneous patterning that occurs during the change from the initial to the final state and these changes are intrinsically irreversible. Even though the initial and final states may be well defined, classical thermodynamics tells us nothing about these irreversible changes. To describe the changes we resort to kinetic descriptions of the underlying physical processes (diffusion, dislocation glide, etc.) and then the theory of irreversible thermodynamics23–25 provides us with a means of linking these irreversible microstructural changes to the equilibrium descriptions of the initial and final states. Our ability to describe the changes that occur depends on our ability to describe the initial and final states and on our understanding and ability to accu23 W. Yourgrau, A. van der Merwe, and G. Raw, Treatise on Irreversible and Statistical Physics, MacMillan, New York (1966). 24 S. R. DeGroot and P. Mazur, Non-Equilibrium Thermodynamics, North-Holland, Amsterdam, (1962). 25 R. Haase Thermodynamics of Irreversible Processes, Addison-Wesley, Reading, MA (1969).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 189

rately describe the fundamental physical processes underlying the changes that occur within the material. This approach has been very successful at describing, for example, the kinetics of phase transformations13,14 where mass transport by diffusion is the primary process governing change. The kinetic descriptions of the underlying physical processes are usually based on the assumption that the rate of the process is linearly related to the gradient in a relevant thermodynamic potential. This is not a consequence of the theory of irreversible thermodynamics, but is a hypothesis that appears to be experimentally well supported. Fick’s first law of diffusion (Eq. (2.1)) in an n component system is a good example: Ji =

n

−Lij grad(μj ),

(2.1)

j =1

Lij are phenomenological coefficients and μj is the chemical potential of component j . In this case the solute flux is proportional to the gradient in the chemical potential of the solute species. We usually refer to the gradient in the thermodynamic potential as the ‘driving force’ and the gradient in the chemical potential is the driving force for solute diffusion. These driving forces are not independent of the free energy change associated with the initial and final states of the material but neither are they the same. The driving forces are locally defined and should be associated with some particular physical process. Nevertheless, we usually categorize the driving forces in the same way as we categorize the free energy changes and it is worthwhile summarizing these different contributions.

a. Chemical Energy: The Free Energy of Strain-Free Regions of a Phase When the compositions and/or the structures of the phases in a system deviate from the equilibrium values under the conditions examined a driving force for solute redistribution and/or crystal structure change arises. The classic example may be the cooling of pure Fe below the allotriomorphic phase transformation temperature of 1183 K. The change in free energy associated with the crystal structure change is of the order of 1 kJ/mol (140 MJ/m3 ). Other microstructural changes driven by chemical free energy familiar to the physicist include the precipitation of a second phase from a metastable homogeneous solid solution.13 In this case the chemical free energy change attending the reaction is typically somewhere in the range 0.1–3 kJ/mol (∼10–300 MJ/m3 ) and is used to drive both the crystal structure change and the necessary solute redistribution.

190

Y. BRÉCHET AND C. HUTCHINSON

b. Strain Energy: The Increase in Free Energy Caused by Short and Long Range Elastic Strains When a metal or alloy is deformed most of the work done is liberated as heat. However, a small amount (which is less than 10% and decreases with increasing strain) is stored within the material in the form of lattice strains and imperfections. The most important of these are dislocations which have a long range strain field. In most cases the entropic contribution to the free energy of the material from dislocations is negligible compared with the strain energy contribution and we can approximate the increase in free energy with the strain energy of the dislocation ensemble. The elastic stored energy of a single isolated edge dislocation is:

μb2 r ED = , (2.2) Ln 4π(1 − ν) r0 μ is the shear modulus of the material, b is the burgers vector, r is the outer cut-off radius (which could be the specimen surface), r0 is the inner cut-off radius and ν is Poisson’s ratio. In addition to the elastic stored energy of the long range strain field, we also associate a ‘core’ energy with the dislocation with a magnitude similar to the elastic contribution. Often, the total is approximated as 12 ρμb2 . An ensemble of dislocations, ρ, can reduce its free energy contribution from ρED by reducing r through the rearrangement into stress-screening arrays. Clearly both the density and the distribution of dislocations must be known to calculate the free energy contribution from the dislocations. For a typical metal deformed at room temperature and containing a high dislocation density of 1 · 1015 m−2 we may estimate the upper limit to the total strain energy (ρED ) as of the order of 10–20 J/mol (1–3 MJ/m3 ). It is this free energy that drives the recovery and recrystallization processes to be discussed in Section IV.13. Unlike solute diffusion, where the kinetic processes are relatively well described (Eq. (2.1)), dislocation motion is much more problematic. Dislocations motion is restricted to well defined crystallographic planes and dislocations are non-conserved quantities. They move by a dislocation glide process which occurs more readily than diffusion. These kinetic aspects as well as the difficulty in defining a local driving force for dislocation motion (which depends on the density and distribution of all other dislocations) will be discussed in later chapters and highlights the difficulties faced in describing dislocation patterning.

c. Interfacial (Surface) Energy: The Extra Free Energy of Atoms at Interfaces Between Phases and at Grain Boundaries The extra energy associated with the atoms at the interfaces between phases and at grain boundaries is a free energy. This excess free energy is usually expressed

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 191

as an energy per unit area of interface and gives rise to a driving force to reduce the interfacial area. This reduction occurs through interface migration and the local driving force is usually expressed in terms of a chemical potential difference on either side of an interface: 2σ μ = , (2.3) r σ is the interfacial free energy per unit area and r is the radius of curvature of the interface (which can be generalized to two principle radii of curvature for an arbitrary boundary). It is the interfacial contribution to the free energy of the system that drives the grain growth processes to be discussed in Section IV.12. A typical grain boundary energy in a metal may be expected to lie somewhere between 0.4–1 J/m2 and for a grain size of 10 µm, this would give rise to a local driving force acting over the interface of the order of 1 J/mol (0.1 MJ/m3 ). The kinetic description of interface motion is usually based on an assumed proportionality between this driving force and the interface velocity. The above separation of the driving forces into chemical, strain and interfacial energies is useful for discussion purposes but it is of course artificial. Not only is there usually more than one type of contribution present, but the contributions often also represent retarding forces that need to be overcome for the physical process to proceed. For example, a concentration gradient in an otherwise perfect crystal will have contributions to the driving force from both chemical and strain energies. The latter arises from the concentration dependence of the molar volume of the lattice. In the case of the interface-mediated transformations to be discussed in Section III, the transformation (which is driven by the chemical free energy change) results in the generation of interfaces and strains (because of differences in molar volumes of the phases). The associated interfacial and strain energies must be ‘paid for’ by the chemical free energy driving the transformation. When considering the contributions (driving or retarding) from chemical, strain and interfacial energies, it is useful to bear in mind the relative magnitudes. Although the driving forces usually evolve in time, in general we find that the typical chemical contribution is one or two orders of magnitude larger than a typical strain energy contribution which is usually at least an order of magnitude larger than the interfacial energy contribution. 6. S YSTEMS M AINTAINED FAR FROM E QUILIBRIUM BY THE C ONTINUOUS I NPUT OF E NERGY For those systems that are continuously maintained far from equilibrium by the input of energy, no general framework such as that offered by classical and irreversible thermodynamics discussed above exists. It is not meaningful to define

192

Y. BRÉCHET AND C. HUTCHINSON

an initial and final state of the material. The system is dynamic and the external input of energy input plays a vital role in the identification and the stability of any stationary states. The defect patterning that occurs during irradiation and during plastic deformation both belong to these types of systems. The energetic contributions to the driving forces discussed above (chemical, strain and interfacial) all still apply to driven systems but an additional two factors must also now be considered. The first is the input of energy into the systems and the means of storing this energy. In the case of plastic deformation, the energy is stored in the form of dislocations and represents less than 10% of the energy expended in deformation. In the case of irradiation, the equivalent quantity is the displacement per atom induced by irradiation. The energy is stored in the form of point defects (vacancies and interstitials) and the only way to evaluate the quantities in an irradiation cascade is through molecular dynamics simulations. This continuous input of energy during plastic deformation or irradiation modifies the ‘potential landscape’ in which the system evolves. Any attempts at identifying stationary states must consider the effect of this input energy on the landscape being sampled. In addition, the defects introduced by plastic deformation and irradiation modify the kinetic processes governing the changes in the material. Therefore, not only is the ‘potential landscape’ modified but the kinetic pathways available for searching the landscape are also changed. Both of these aspects must be considered in dealing with microstructural evolution in driven systems. As we shall see in Section V.14, some success has been achieved in dealing with patterning under irradiation. In these cases a ‘chemical kinetics’ approach was adopted which shows some good agreement with experiment. In Section V.15, we discuss patterning during plastic deformation and we shall see that our understanding is much less complete. The difficulties in identifying the local driving force for dislocation motion and in mimicking the dislocation transport (glide) process currently present some barriers to progress. III. Chemical Patterning: Interface-Mediated Transformations: Eutectoid Decomposition and Discontinuous Precipitation

Probably the best known of all solid state patterns formed in the science of metals and alloys, and certainly the most thoroughly studied, is that arising from the pearlite phase transformation in steels. The reaction belongs to the class of eutectoid transformations (the solid state equivalent of the eutectic transformation) and involves the decomposition of the face-centered cubic austenite (γ ) phase into a lamellar pattern of body-centered cubic carbon-poor ferrite (α) and carbon-rich orthorhombic cementite (Fe3 C) behind a migrating interphase boundary. γ → α + Fe3 C

(3.1)

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 193

In this case, the defect involved in the pattern formation is the interface which is created between the growing product phases and the parent phase. The transformation usually begins at the prior γ grain boundaries or other structural heterogeneities and an example taken from an Fe-0.8C (wt.%) alloy is shown in Figure III.126 together with the phase diagram illustrating the three phases involved in the transformation. Although the pearlite transformation in steels is by far the best known and studied of the eutectoid transformations, the formation of lamellar patterns from eutectoid decomposition in systems other than those based on Fe-C are also well known (e.g., Cu-Al,27–30 Zn-Al,31 Cu-In,32 Au-In33 ). In all cases, the parent phase transforms into two different product phases and growth involves the redistribution of solute from the solute-poor product phase to the solute-rich phase. An important input into the theoretical treatments of growth is an identification of the ‘path’ taken by the redistributing solute. In some cases, such as in the Cu-Al system,29 it has been quite well established that the diffusion occurs in the parent phase ahead of the migrating interface. In other cases (e.g., Cu-In32 ), it has been concluded that the solute redistribution occurs by shortcircuit diffusion within the migrating interphase boundary itself where the atomic arrangement is comparatively disordered.34,35 In the overwhelming majority of cases of pearlite growth, the necessary solute redistribution from the solute poor phase to the solute rich is restricted to the vicinity of the transformation interface and no long range solute diffusion either to or from the parent phase is observed. The pearlite aggregate forms with the same overall composition as the parent phase and growth occurs at a constant rate with a constant interlamellar spacing. It is these two characteristics of the pattern formation in eutectoid decomposition that have attracted the interest of researchers in materials science. In the solid state, a lamellar pattern resembling the pearlite transformation in appearance can also arise as the product of a simple precipitation reaction involving only two crystallographically distinct phases. The transformation is referred 26 L. S. Darken and R. M. Fisher, in Decomposition of Austenite by Diffusional Processes, eds.

V. F. Zackay and H. I. Aaronson, Interscience, New York (1962), p. 249. 27 G. V. T. Ranzetta and D. F. R. West, J. Inst. Metals 92, 12 (1964). 28 M. K. Asundi and D. F. R. West, J. Inst. Metals 94, 19 (1966). 29 D. Cheetham and N. Ridley, Metall. Mater. Trans. A 4, 2549 (1973). 30 M. J. Whiting and P. Tsakiropoulos, Acta mater. 45, 2027 (1997). 31 D. Cheetham and N. Ridley, J. Inst. Metals 99, 371 (1971). 32 A. Das, S. K. Pabi, I. Manna, and W. Gust, J. Mat. Sci. 34, 1815 (1999). 33 A. Das, W. Gust, and E. J. Mittemeijer, Mat. Sci. and Tech. 16, 593 (2000). 34 Y. Mishin, C. Herzig, J. Bernardini, and W. Gust, Int. Mat. Rev. 42, 155 (1997). 35 I. Kaur and W. Gust, Diff. and Def. Data A 66–69, 765 (1989).

194

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.1. (a) Optical micrograph of a pearlite colony in an Fe-0.8C (wt.%) alloy partially transformed at 700 ◦ C. The lamellar pattern consists of alternating plates of Fe3 C (dark) and α (light) separated from the parent γ phase by an interphase boundary. (b) The Fe-rich end of the binary Fe-C phase diagram illustrating the three phases involved in eutectoid decomposition. The C content of the α phase is so low that the single α phase field cannot be resolved for the domain of C contents chosen for illustration.

to as ‘discontinuous’ precipitation to distinguish it from the competitive ‘continuous’ mode of relieving the supersaturation of the parent phase, familiar to the physicist.13,14 Discontinuous precipitation also usually begins at grain bound-

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 195

F IG . III.2. (a) Bright field transmission electron microscopy image of discontinuous precipitation in an Al-22Zn (at.%) alloy partially transformed at 478 K. The lamellar pattern consists of alternating plates of β-Zn and a solute depleted α-Al phase separated from the supersaturated α0 phase (parent phase) by a grain boundary. (b) The binary Al-Zn phase diagram illustrating the two phases involved in discontinuous precipitation.

aries in the supersaturated parent phase (α0 ) and forms as a regular aggregate of alternating compound phase (β) and a solute depleted matrix phase (α) growing behind a migrating grain boundary which separates the product from the parent phase (e.g., Figure III.2a). α0 → α + β

(3.2)

196

Y. BRÉCHET AND C. HUTCHINSON

The solute depleted matrix phase (α) is identical in structure to the parent phase (α0 ) and differs only in solute content and crystal orientation across the transformation interface. The solute content and orientation appear to change ‘discontinuously’ across the grain boundary and it is from this change that the transformation derives its name. The solute redistribution from the solute depleted product phase to the solute rich compound phase occurs by short circuit diffusion within the transformation interface and volume diffusion in the parent phase is thought to play little role in the transformation. Like most cases of the pearlite transformation, under isothermal conditions the discontinuous precipitation product usually forms with the same overall composition as the parent phase and growth at a constant rate with a constant interlamellar spacing is observed. Discontinuous precipitation has now been identified in more than 150 binary and ternary systems. A comprehensive review of theses systems was recently compiled by Manna et al.36 and a thorough discussion of many aspects of the reaction can be found in the monograph by Pawlowski and Zieba37 and in several recent reviews.18,38 An example taken from the Al-Zn system39 is shown in Figure III.2 along with a section of the corresponding binary phase diagram. In the transmission electron micrograph shown, discontinuous precipitation of the β-Zn phase and the Zn poor α-Al matrix lamellar phase grow behind a migrating grain boundary into the parent phase. Unlike eutectoid decomposition, where pearlite formation is associated with a definite feature of the phase diagram (the eutectoid), it is not well understood under which conditions a supersaturated solution will decompose solely in a discontinuous manner, solely in a continuous manner or both together in a competitive manner. The result depends on the competition between the nucleation and growth of the continuous and discontinuous products. Although the growth aspects of both of these problems are now reasonably well understood, a reliable quantitative understanding of the rates of nucleation of the two products is lacking. This is especially true for the initiation of the discontinuous reaction. Several initiation mechanisms have been proposed over the years36,37,39–42 but so far no single origin is consistent with all of the experimental observations. 36 I. Manna, S. K. Pabi, and W. Gust, Int. Mat. Rev. 46, 53 (2001). 37 A. Pawlowski and P. Zieba, Phase Transformations: Controlled by Diffusion at Moving Boundaries,

Polish Academy of Sciences, Warszawa (1991). 38 D. B. Williams and E. P. Butler, Int. Metals Rev. 26, 153 (1981). 39 I. G. Solorzano, G. R. Purdy, and G. C. Weatherly, Acta metall. 32, 1709 (1984). 40 G. Meyrick, Scripta metall. 10, 649 (1976). 41 S. F. Baumann, J. Michael, and D. B. Williams, Acta metall. 29, 1343 (1981). 42 H. I. Aaronson and C. S. Pande, Acta mater. 47, 175 (1998).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 197

The pearlite and discontinuous reactions shown in Figures III.1 and III.2 give rise to lamellar patterns. The pattern takes the form of alternating plates of the product phases and this is indeed the most commonly observed morphology. Less frequently, products of both the discontinuous and eutectoid decomposition reactions have also been observed to adopt ‘rod-like’ morphology; examples include the discontinuous precipitation reaction in Cu-Co43 and the pearlite (α + Mo2 C) formed in Fe-C-Mo.44 As is the case for eutectic solidification, the choice of morphology depends on the relative volume fraction of phases formed and the energy of the interface between the product phases.4 In the following discussion, we shall restrict ourselves to treatments of the more common lamellar morphology. The regularity of the patterns formed from the pearlite and discontinuous precipitation reactions has led many theoreticians to search for a quantitative description of the pattern repeat distance and the growth rate. In Section III.7, we review the most popular treatments and then in Section III.8 consider the attempts to resolve the central unanswered growth related question: ‘the spacing selection problem’. A brief discussion of lamellar pattern formation under non-steady state conditions is presented in Section III.9 and some illustrations of the resulting patterns are provided. Since the products of both the pearlite and the discontinuous precipitation reactions are highly non-equilibrium structures, a significant driving force exists for coarsening processes. In Section III.10 we summarize the known mechanisms responsible for the changes in shape and scale of the lamellar products during coarsening. Finally, a short discussion on the possibility of using artificially created metallic multilayers to investigate some of the fundamental aspects of the selection and evolution of solid state patterns in interface-mediated transformations is presented. 7. S TEADY S TATE G ROWTH

a. Theoretical Treatments The pearlite and discontinuous precipitation products shown in Figures III.1 and III.2 were formed isothermally under steady state conditions with an approximately constant (average) growth rate and interlamellar spacing. This problem of the steady state growth of a lamellar pattern has a long history and has been

43 A. Perovic and G. R. Purdy, Acta metall. 29, 53 (1981). 44 R. E. Hackenberg and G. J. Shiflet, Acta mater. 51, 2131 (2003).

198

Y. BRÉCHET AND C. HUTCHINSON

considered by many authors.45–66 In the following, we will present a selection from the sequence of models which have appeared in the literature, each model representing a response to the limitations of its predecessors. The reason for this approach is not only to provide a clearer insight into the necessary ingredients for a full solution of the problem, but also to give the reader access to the simplest model possible for interpreting their experimental observations. If only the growth kinetics and length scales are to be interpreted, then Zener’s47 approach is sufficient. If local chemical analysis between lamellae is to be analyzed, then the full solution of the diffusion equation provided by Cahn50 is necessary. If the shapes of the moving boundaries are available to experimental investigation, then the treatment developed by Hillert49,57,60,64 is necessary. If the full selection problem is to be investigated, then a complete solution of the diffusion equations, coupled with appropriate thermodynamic data and a local force balance at every position along the transformation interface is required. We start with the simplest approaches and progressively proceed toward the more sophisticated ones, but want to emphasize that for a given set of experimental observations the appropriate theory may not be the most sophisticated one. At the outset it is worth emphasizing the difference between the pearlite and discontinuous precipitation reactions. Even though both processes give rise to a lamellar pattern and the diffusion geometry is similar in both cases, one reaction is 45 W. H. Brandt, J. Appl. Phys. 16, 139 (1945). 46 E. Scheil, Z. Metallkd. 37, 123 (1946). 47 C. Zener, Trans. AIME 167, 550 (1946). 48 D. Turnbull, Acta metall. 3, 55 (1955). 49 M. Hillert, Jernkont. Ann. 141, 757 (1957). 50 J. W. Cahn, Acta metall. 7, 18 (1959). 51 K. A. Jackson and J. D. Hunt, Trans. AIME 236, 1129 (1966). 52 K.-N. Tu and D. Turnbull, Scripta metall. 1, 173 (1967). 53 H. I. Aaronson and Y. C. Liu, Scripta metall. 2, 1 (1968). 54 B. E. Sundquist, Acta metall. 16, 1413 (1968). 55 J. M. Shapiro and J. S. Kirkaldy, Acta metall. 16, 579 (1968). 56 J. Petermann and E. Hornbogen, Z. Metallkunde 59, 814 (1968). 57 M. Hillert, in Mechanism of Phase Transformations in Solids, vol. 33, The Institute of Metals

(1968), p. 231. 58 B. E. Sundquist, Acta metall. 17, 967 (1969). 59 M. Hillert, Acta metall. 19, 769 (1971). 60 M. Hillert, Metall. Mater. Trans. A 3, 2729 (1972). 61 M. P. Puls and J. S. Kirkaldy, Metall. Mater. Trans. A 3, 2777 (1972). 62 G. Bolze, M. P. Puls, and J. S. Kirkaldy, Acta metall. 20, 73 (1972). 63 B. E. Sundquist, Metall. Trans. A 4, 1919 (1973). 64 M. Hillert, Acta metall. 30, 1689 (1982). 65 A. Bogel and W. Gust, Z. Metallkd. 79, 296 (1988). 66 L. Klinger, Y. J. M. Brechet, and G. R. Purdy, Acta mater. 45, 5005 (1997).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 199

a precipitation reaction and involves only two different phases, whereas the eutectoid decomposition reaction involves three different phases. The thermodynamic situation in the two cases is very different and this difference must be considered in the development of models that attempt to explain the observed growth. Nevertheless, there are many common assumptions made in the derivations and it is also worth summarizing these commonalities. In all cases, the model derivations are based on the isothermal growth of a perfectly regular lamellar aggregate. The isothermal assumption includes all areas of the transformation interface and it is assumed that the heat liberated by the reaction can be conducted away from the transformed volume quickly enough that any local rises in temperature can be ignored. It is usually assumed that all of the phases involved in the reaction have equal molar volumes and that any local stresses developed upon transformation have a negligible influence upon the growth. Finally, it is usually assumed that any interfacial energies that enter into the derivation are isotropic. One of the earliest theoretical treatments was due to Zener47 who was interested in describing the kinetics of the pearlite transformation in steels (Eq. (3.1), Figure III.1). Zener provided an approximate treatment that assumed the growth rate of the pattern was controlled by the redistribution of carbon from the ferrite (α) to the cementite (Fe3 C) and that this occurred entirely by volume diffusion in the parent austenite (γ ) phase, Figure III.3. The diffusion was driven by the difference in carbon composition in the γ at the γ /α and γ /Fe3 C interfaces, (X γ /α − X γ /Fe3 C ). If the γ /α and γ /Fe3 C interfaces are planar and assuming dilute solution thermodynamics, then the driving force for carbon redistribution is given by the difference in interfacial carbon contents which are usually assumed to be the equilibrium values (local equilibrium assumption) found from the metastable extensions of the γ /(γ + α) and γ /(γ + Fe3 C) phase boundaries into the (α + Fe3 C) two phase field of the phase diagram (dotted lines, Figure III.1b). Zener realized that not all of this driving force could be used to drive the C diffusion because during growth some must be spent on the creation of the new α/Fe3 C interfaces. The driving force, G, spent on the creation of the interlamellar interface is 2σ Vm , (3.3) λ λ is the interlamellar spacing (pattern repeat distance), σ is the surface energy of the α/Fe3 C interface and Vm is the molar volume assumed to be the same for all phases. A critical interlamellar spacing, λc , can be identified for which all the free energy available would be spent on creating α/Fe3 C interfaces and the growth rate of the aggregate would fall to zero. For interlamellar spacings greater than λc , = Gsurface m

200

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.3. Schematic illustration of the diffusion geometry for lamellar pattern formation under conditions where the solute redistribution occurs by volume diffusion in the parent phase.

the net driving force for diffusion could then be approximated by multiplying the total driving force for the reaction by a scaling factor, (1 − λc /λ). Combining this driving force for C diffusion with a characteristic diffusion distance (which was assumed proportional to the lamellar thickness), a carbon flux can be evaluated and when combined with a solute mass balance across the interface, an expression for the growth rate of the regular lamellar aggregate can be written:47,60

γ /α γ /Fe C λc Xe − Xe 3 1 2D γ 1− , (3.4) ν = α Fe C λ λ f f 3 X Fe3 C − X α v is the growth rate, D γ is the C diffusivity in γ , λα and λFe3 C are thicknesses of the α and Fe3 C lamellae respectively, the interlamellar spacing λ = λα + λFe3 C , f α and f Fe3 C are the mol fractions of α and Fe3 C in the aggregate, X α and X Fe3 C are the C compositions of the growing α and Fe3 C phases, both assumed to be γ /α γ /Fe C constant, and Xe and Xe 3 are the C compositions in the γ at the γ /α and γ /Fe3 C interfaces, usually assumed to be the local equilibrium values found from the phase diagram. Zener’s treatment, like almost all subsequent treatments, provides a relationship between the growth velocity, the interlamellar spacing and the boundary

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 201

conditions of the diffusion problem. After a choice of appropriate interfacial compositions, an additional criterion is still required to decouple the interface velocity from the interlamellar spacing to obtain a unique velocity/spacing pair. This is referred to as the ‘spacing selection’ problem. Zener invoked a maximum growth rate hypothesis to remove the degeneracy of the problem and it is clear from Eq. (3.4) that the maximum growth rate occurs at an interlamellar spacing, λ = 2λC , (i.e., when half of the free energy driving the process is stored as interfacial energy). According to Zener’s reasoning this would be the real pearlite growth rate. A consequence of Zener’s assumed proportionality between the observed lamellar spacing and the critical spacing (Eq. (3.3)) is that we should expect a plot of the reciprocal interlamellar spacing versus the driving force to give a straight line. The driving force usually shows good proportionality with the undercooling from the eutectoid temperature and indeed plots of the reciprocal spacing versus undercooling do fall on a straight line describing well the smaller interlamellar spacings that are observed in pearlite formed at lower and lower temperatures (e.g., Figures III.6b and III.8b). In principle, either the interlamellar interfacial energy (σ ) or the proposed proportionality between the observed lamellar spacing and the critical spacing (and therefore the optimization principle) could be extracted from the slope of such plots but unfortunately neither is currently known with sufficient certainty for meaningful conclusions to be drawn. Certainly, reliable theoretical calculations of the interlamellar interfacial energy could shed some valuable light on the question of optimization principles. The first treatment applicable to discontinuous precipitation appeared in 1955 by Turnbull48 who was interested in interpreting his growth kinetic results for a Pb-Sn alloy.67 Turnbull first used Zener’s treatment for the pearlite transformation with boundary conditions for the diffusion problem appropriate for discontinuous precipitation and found that his kinetics was around eight orders of magnitude faster that those calculated assuming volume diffusion of Sn. Turnbull subsequently modified Zener’s treatment by assuming that the diffusion path for the solute was the transformation interface itself (Figure III.4) instead of volume diffusion in the parent phase as assumed by Zener for the pearlite transformation. He neglected the effect of surface energy and made some approximations in his evaluation of the net driving force for diffusion and obtained an expression for the pattern growth rate in discontinuous precipitation:

α/β D i δ X bulk − Xe , (3.5) ν= α 2 (λ ) X bulk X bulk is the initial composition of the supersaturated parent phase, D i is the solute diffusivity within the reaction interface and δ is the width of the interface itself. 67 D. Turnbull and H. N. Treaftis, Acta metall. 3, 43 (1955).

202

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.4. Schematic illustration of the diffusion geometry for lamellar pattern formation under conditions where the solute redistribution occurs by short-circuit diffusion within the migrating interface. α/β

λα is the width of the solute depleted lamella and Xe is the local equilibrium solute concentration in the α at the α/β interface. Turnbull found satisfactory agreement with his experimentally observed growth rates when using an activation energy for grain boundary diffusion that was a little less than half of that for bulk diffusion. This was consistent with the early findings for other metals and has since been found to be typically representative.34,35,68 However, the experimentally observed lamellar spacing was much larger than that predicted using Zener’s maximum growth rate hypothesis. Even though the diffusional treatment of the problem seemed adequate, Zener’s solution to the spacing selection problem did not appear to be satisfactory. Furthermore there was an indication that the discontinuous precipitation reaction resulted in an incomplete relief of the supersaturation of the parent phase and therefore the local equilibrium assumption for the boundary conditions of the diffusion problem may not be appropriate. The next steps in the theoretical treatments of lamellar growth came very soon after Turnbull’s treatment and represented major theoretical advances that put the diffusion problem on a much sounder mathematical basis. Hillert49 was the first 68 P. Zieba and W. Gust, Interface Sci. 10, 27 (2002).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 203

to present his treatment which was developed with the pearlite transformation in mind, again assuming that the C redistribution occurred only through the γ . He realized that in solving the diffusion problem all the carbon concentrations in the austenite should be considered and not only the compositions at the γ /α and γ /Fe3 C interface (Figure III.3) as was done in Zener’s approximate treatment. Hillert, building on the work of Brandt45 and Scheil46 obtained a Fourier series expression for the C diffusion field in the γ as a solution to the steady state twodimensional carbon diffusion equation. He included the effect of capillarity from the curved γ /pearlite transformation interface but to apply the boundary condition at the interface and solve for the unknown Fourier coefficients in the C field expression required knowledge of the shape of the transformation interface which was, a priori, unknown. By assuming a relatively flat interface and mechanical equilibrium at the γ /α/Fe3 C triple junction (Figure III.3), Hillert was able to obtain an analytic growth rate expression which turned out to be very similar to the approximate expression obtained by Zener (Eq. (3.4)): ν=

γ /α γ /Fe C λc π 3 D γ f α f Fe3 C Xe − Xe 3 1 1 − , b λ λ X Fe3 C − X α

(3.6)

b is a constant that depends on the ratio of the lamellar widths and typically has a value ∼ 0.5. Furthermore, Hillert’s treatment allowed for a detailed calculation of the interphase boundary shape. This had previously only been calculated by Brandt.45 To solve the spacing selection problem, Hillert, like Zener, assumed a maximum growth rate hypothesis. Soon after Hillert’s treatment, Cahn50 provided a general treatment for lamellar growth applicable to both pearlite and discontinuous transformations under conditions where it was assumed that the solute redistribution occurs solely by shortcircuit diffusion in the migrating interface (Figure III.4). Turnbull’s experiments in the Pb-Sn system67 had provided an indication that during the discontinuous precipitation reactions, the solute redistribution between the growing phases was incomplete and a non-negligible supersaturation remained in the matrix lamellar phase. With this in mind, Cahn wrote his differential equation for grain boundary interface solute transport but solved it under conditions where the composition of the product phases could vary across the lamellar (i.e., perpendicular to the growth direction). Cahn realized that equilibrium could not be maintained at the moving curved interface and that this resulted in non-equilibrium solute partitioning between the product phases. He solved his steady state diffusion problem and obtained an expression for the solute concentration profile within the solute depleted lamellae as a function of the growth rate, v, the interlamellar spacing, λ,

204

Y. BRÉCHET AND C. HUTCHINSON

and the solute transport properties of the interface (Figure III.4): √

y α X bulk − X α (y) cosh λα √ = X bulk − X α/β cosh 2α

where α =

kvλ2 , Di δ

(3.7)

X(y) is the solute content in the solute depleted α lamellae behind the migrating interface as a function of position, X α/β is the solute concentration in the α at the α/β interlamellar interface which is usually taken as the equilibrium value from the phase diagram, D i is the solute diffusivity in the migrating boundary, δ is the boundary width and k is a proportionality constant that relates the concentration in the thin slab of interface, X i , to the solute concentration inherited by the product phase, X α . Cahn assumed that the interface velocity was simply proportional to the net Helmholtz energy change across the interface, F , which can be calculated from a knowledge of the system thermodynamics, the solute profiles retained within the lamella and the interfacial energy of the interlamellar interfaces: ν = MF,

(3.8)

M is a macroscopic kinetic parameter (friction) which is a measure of the response of the interface to the applied driving force. Again, Cahn adopted an optimization principle (optimal rate of free energy dissipation) to remove the degeneracy of the problem and select a velocity/spacing pair. Cahn’s derivation of the solute profile left behind the migrating interface is applicable to both pearlite and discontinuous precipitation products. However, by nature of the system thermodynamics, the composition gradients which can be sustained in pearlite, and still result in a net free energy decrease during growth, are very limited. In contrast, in the discontinuous reaction, the ranges of available compositions allowed for a supersaturated solution are much wider. The difference is shown in Figure III.5. In the top figure the free energy curves for the precipitation reaction are shown. For a bulk alloy composition X0 , the chemical part of the free energy will decrease in a precipitating system as long as the precipitate, β, forms with a composition greater than X , regardless of how little precipitates and therefore how little the α phase changes composition. For the eutectoid composition shown below, the new α and β phases cannot take compositions anywhere near the original γ matrix composition. Segregation to at least Xα and Xβ is necessary to give a decrease in the free energy of the system. The exact solution for the solute diffusion profile between two lamellae provided by Cahn’s approach proved to be both theoreti-

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 205

F IG . III.5. Schematic free energy curves for (a) precipitating and (b) eutectoid systems.50

cally important, and possible to test experimentally by local chemical analysis, in discontinuous reaction products, e.g., see Refs. [69–73]. Hillert criticized Cahn’s treatment because it did not consider the force actually pulling the grain boundary in the first place and therefore did not really explain how discontinuous precipitation occurs. In addition, Cahn prescribed a flat interface, whereas, in principle, not only the spacing between lamellae, but also the shape of the moving grain boundary should be part of the solution of the problem. Hillert57,60,64 then provided treatments for the pearlite and discontinuous transformations under conditions where the solute redistribution was restricted to the 69 D. A. Porter and J. W. Edington, Proc. Roy. Soc. London A 358, 335 (1977). 70 P. Zieba and W. Gust, Int. Mat. Rev. 43, 70 (1998). 71 P. Zieba and W. Gust, Mikrochimica Acta 132, 295 (2000). 72 P. Zieba and W. Gust, Z. Metallkd. 92, 645 (2001). 73 P. Zieba Mat. Chem. and Phys. 62, 183 (2000).

206

Y. BRÉCHET AND C. HUTCHINSON

transformation interface, by considering the necessary diffusion and a detailed balance of surface tensions across the interface during growth. The treatments of Cahn and Hillert can respectively be characterized as ‘global’ and ‘detailed’ in the sense that, in Cahn’s treatment the interface is a high diffusivity reaction path and its mobility controls the rate at which the interface moves in response to the existing driving force; whilst in Hillert’s treatments of lamellar growth, detailed knowledge of the interface and its properties is often necessary for application of the growth rate expressions. The theoretical treatments of Hillert and Cahn, made in the 1950s and 1960s, remain to this day the treatments used most frequently. Since this time, contributions to the theory of lamellar growth have concentrated on extending these original treatments to include such effects as: ternary solute additions,58,59 non-uniformity in the compositions of the lamella phases in pearlite,62 coherency stresses60 and resolution of the spacing selection problem.61,66,74

b. Experimental Observations Many aspects of the theoretical treatments discussed above can be compared with experimental data. These include metallographic measurements of lamellar growth rates and interlamellar spacings and more recently, analytical electron microscopy measurements of the solute concentrations inherited by the growing phases. For both the pearlite transformation and the discontinuous precipitation reaction, much of the experimental data has been collected and compared with the theoretical predictions in periodical reviews of the subject (pearlite: see Refs. [61, 75,76]; discontinuous precipitation: see Refs. [36–38]). Here we present a couple of selected examples to illustrate the types of comparisons that are usually made. Pearlite. Traditionally, researchers have been interested in describing both the growth rate and the repeat distance of the evolving pattern. These are the two quantities that are experimentally measured. The growth rates are usually calculated from a representative width of the pearlite colonies in a series of isothermally transformed specimens and the results are then compared with the predictions of one of the models discussed above. The first example is taken from the Cu-Al system. The transformation rate in a Cu-12Al (wt.%) alloy has been measured by several authors27–29 and the experimental growth rates and interlamellar spacings as a function of temperature are shown in Figure III.6. 74 J. S.Kirkaldy, Phys. Rev. B 30, 6889 (1984). 75 R. F. Mehl and W. C. Hagel, Prog. Met. Phys. 6, 74 (1956). 76 J. W. Cahn, in Decomposition of Austenite by Diffusional Processes, eds. V. F. Zackay and H. I. Aaronson, Interscience, New York (1962), p. 131.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 207

F IG . III.6. Experimentally measured (a) pearlite growth rates and (b) interlamellar spacings in a Cu-11.8Al (wt.%) alloy as a function of temperature.29 .

For the data shown, Cheetham and Ridley29 then applied Hillert’s volume diffusion growth rate equation (Eq. (3.4)) using the experimentally observed interlamellar spacings to examine the agreement between theory and observation. To

208

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.7. Comparison of the growth rate data in Figure III.6a with the theoretical predictions calculated assuming local equilibrium interfacial compositions, volume diffusion of the components and using the experimentally observed interlamellar spacings.29 The results using both the maximum growth rate hypothesis of Zener47 and the optimal rate of entropy production of Kirkaldy61 are shown.

make the comparison, a choice must be made concerning the relationship between the observed lamellar spacing and the critical spacing. The calculated results using both Zener’s maximum growth rate hypothesis (λ = 2λc ) and Kirkaldy’s maximum rate of entropy production (λ = 3λc ) are compared with the experimental results in Figure III.7. The agreement in both cases is considered to be quite good. On the basis of such comparisons it is now fairly well accepted that the solute redistribution in this reaction occurs predominantly by volume diffusion in the parent phase ahead of the interface but considering the uncertainty in experimental measurements and the thermodynamic and kinetic quantities entering into Eq. (3.4), solid conclusions cannot be drawn concerning the operative optimization principle. The second example concerns the pearlite reaction in binary Fe-C steels. There has been much discussion in the literature concerning the diffusion path for C in this reaction.47,49,50,54,57,76 During the 50s, 60s and 70s when much of the experimental work was carried out, the accuracy with which the relevant thermodynamic and kinetic data was known was insufficient to draw any solid conclusions about the C diffusion path through comparisons with theory. Nevertheless, many authors had tentatively suggested that the experimental growth rates appear to be at least an order of magnitude faster than those predicted by the volume diffusion con-

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 209

F IG . III.8. Experimentally observed pearlite (a) growth rates and (b) interlamellar spacings in a series of binary Fe-C alloys as a function of temperature. The theoretical predictions assuming local equilibrium interfacial conditions, a maximum growth rate hypothesis and both volume diffusion control and boundary diffusion control are shown in (a). The volume diffusion controlled kinetics is approximately an order of magnitude slower than the experimental observations. The boundary diffusion controlled kinetics was calculated using a sD i δ triple product with an activation energy ∼ 0.5 of that for bulk C diffusion. (Continued on next page.)

trolled models.47,49,54,76 Today, our knowledge of the relevant thermodynamic and kinetic parameters is much better and we have carried out a new series of calculations using the existing data to shed some light on this issue. The experimentally measured growth rates77–79 and interlamellar spacings79 are shown in Figure III.8. The theoretical prediction using the experimental lamellar spacings and assuming both volume diffusion of C and Zener’s maximum growth rate hypothesis is also shown. It is clear that the kinetics are indeed at least an order of magnitude slower than the experimental values, suggesting a diffusion path for C other than the parent γ phase must be contributing to solute redistribution. Hillert49 77 F. C. Hull, R. A. Colten, and R. F. Mehl, Trans. AIME 150, 185 (1942). 78 J. H. Frye, E. E. Stansbury, and D. L. McElroy, Trans. AIME 197, 219 (1953). 79 D. Brown and N. Ridley, J. Iron and Steel Inst. 204, 811 (1966).

210

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.8. (Continued.)

and Cahn76 have discussed the possibility of different diffusion paths for the C and it now seems the most likely candidate is the moving interphase boundary itself (as is the case for the discontinuous precipitation reaction). The theoretical treatments of growth according to this diffusion path have also been made but the problem lies in the lack of knowledge of the thermodynamic and kinetic quantities of the moving boundary region. Hillert’s57 expression for the growth rate of pearlite according to boundary diffusion control is:

γ /α

γ /Fe C 12sD i δ Xe − Xe 3 λc 1 ν = α Fe C . (3.9) 1 − λ f f 3 X Fe3 C − X α λ2 Our problem is that neither D i , δ or s are known with any certainty. Instead, what is usually done, is to extract an effective triple product, sD i δ, from the experimental results using one of the models for growth and then to make a judgment about whether this seems reasonable for boundary diffusion control. If so, it is then usually concluded that the diffusion path for the solute is probably the moving boundary. We have made such calculations and find that using a segregation coefficient (s) of 1 and a grain boundary width (δ) of 0.5 nm, the experimental data can be adequately described by assuming Zener’s maximum growth rate hypothesis (λ = 3λc /2 in the case of boundary diffusion control) with an activation

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 211

energy for boundary diffusion of C that is approximately 0.7 of that for C diffusion in the bulk (Figure III.8a). In the case of substitutional elements diffusing in migrating interfaces, experimental measurements have found that the activation energy for diffusion is indeed approximately 0.5–0.7 of the corresponding value in the bulk.34,35,68 Whether the same should be true for C which diffuses interstitially in the bulk it is not clear. Nevertheless, this example illustrates the difficulty encountered in making any solid conclusions about the transformation when considerable uncertainty exists in the knowledge of either the optimization principle or the interlamellar interfacial energy and the relevant thermodynamic and kinetic data for the migrating boundary region. Kaur et al.80 have compiled a large set of interphase boundary diffusion data for those systems that have been experimentally examined and as we shall see in the next section, much of this data is obtained through back calculation from the results obtained in discontinuous precipitation reactions. During the last 20 years, it has become possible to use advanced electron microscopy techniques to directly measure solute concentrations in the vicinity of the transformation interface. Indeed, the state of the art instruments today are capable of making measurements in the sub-nm range. This would be an ideal, direct way of identifying the solute diffusion path in these reactions. This has been done for several cases and it has recently been shown that for the pearlite formed in Fe-C-Mn alloys,81 the diffusion path for the redistributing substitutional Mn element is the reaction interface itself and volume diffusion of Mn plays little role in the reaction. However, because of the very low C contents that are encountered in eutectoid steels and the contamination of the surface of the thin-foil samples for electron microscopy during preparation, it is currently not possible to measure with sufficient accuracy the C concentrations in these specimens. In this respect, progress in our understanding of some of the fundamental aspects of the pearlite transformation in steels has not been able to take advantage of the technological advances that techniques like analytical electron microscopy have been able to bring to other transformations, such as the discontinuous precipitation reaction to be discussed below. Discontinuous Precipitation. In making comparisons between theory and experiment in the discontinuous precipitation reaction we are not faced with the question of the solute diffusion path. From the earliest theoretical treatments it 80 I. Kaur and W. Gust, Fundamentals of Grain and Interphase Boundary Diffusion, John Wiley &

Sons, New York (1995). 81 C. R. Hutchinson, R. E. Hackenberg, and G. J. Shiflet, Acta mater. 52, 3565 (2004).

212

Y. BRÉCHET AND C. HUTCHINSON

was assumed that the path was the reaction interface itself and this is now experimentally well established. However, the comparisons are complicated by the nonequilibrium segregation of solute at the transformation interface. The solute depleted matrix lamella does retain some level of residual supersaturation. For comparisons between experimentally measured growth rates and interlamellar spacings with theoretical predictions, many of the models proposed require a quantification of this non-equilibrium segregation. Cahn provided an expression describing the solute profile across the lamella behind the transformation interface as a function of the growth rate, the interlamellar spacing, the bulk solute content and the transport properties of the boundary. This is one area where progress in our understanding has benefited from recent advances in analytical electron microscopy. There are now many experimental studies that have directly measured the solute profiles behind the migrating boundary and have found that Cahn’s equation is well obeyed. Many of these studies have recently been summarized in a series of reviews, e.g., Refs. [36,37,72]. An example taken from the work of Duly et al.82 on the discontinuous precipitation reaction in an Mg-18.8Al (at.%)) alloy is shown in Figure III.9. The data shows solute profiles measured at two distances behind the reaction interface and the solid curve is the best-fit (in α and Xα/β , Eq. (3.7)) using Cahn’s equation. From the value of α obtained, and the experimental measurements of the growth rate and interlamellar spacing of the lamellar pattern, values for the sD i δ, triple product can be extracted and a judgment can be made concerning the reasonableness of these values. Clearly, depending on which of the theoretical models for growth is chosen for comparison, different values of this triple product can be obtained. Amir and Gupta83 have nicely presented the possible differences calculated for each of the different models using data for an Mg-7Al (at.%) alloy. They metallographically measured the growth rate and interlamellar spacing as a function of temperature and used X-ray diffraction techniques to estimate the level of nonequilibrium solute segregation, all as a function of temperature. They then extracted the triple products necessary to reproduce the experimental data for each of the different models and compared these. They are shown in Figure III.10. The three most sophisticated models (Cahn,50 Hillert60,64 and Sundquist63 ) all give quite similar activation energies for boundary diffusion, ∼ 70 kJ/mol. The activation energy for chemical diffusion in dilute Mg-Al alloys is reported to be ∼ 143 kJ/mol. The proposed boundary diffusion value is then ∼ 0.5 of that for volume diffusion and is consistent with the findings in other alloys. The extraction of boundary diffusion parameters from the analysis of the discontinuous precipitation reaction has now become one of the prime sources of boundary diffusion data. However, as is clear from Figure III.10, the values obtained depend on the model used to describe the discontinuous reaction. 82 D. Duly, M. C. Cheynet, and Y. Brechet, Acta metall mater. 42, 3843 (1994). 83 Q. M. Amir and S. P. Gupta, Can. Metall. Qrty 34, 43 (1995).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 213

F IG . III.9. Plots of Al composition as a function of position across the solute depleted lamellae at two distances behind the reaction interface; (a) at 380 nm and (b) at 200 nm during discontinuous precipitation in an Mg-18.8Al (at.%) alloy treated at 220 ◦ C for 16 h. The profiles were measured using electron energy loss spectroscopy and a scanning transmission electron microscope.82 In both cases, the profiles are well described by Cahn’s equation (solid line) using the same Xα/β and α values.

8. T HE S PACING S ELECTION P ROBLEM In each of the theoretical treatments of steady state lamellar pattern growth discussed above, a relation between the growth velocity, ν, the interlamellar spacing, λ, and the boundary conditions for the diffusion problem is obtained. After ap-

214

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.10. Extracted triple product (sD i δ) values as a function of 1/T (K−1 ) according to each of the different discontinuous precipitation models for experimental growth rate and interlamellar spacing data from a Mg-7Al (at.%) alloy treated at a variety of temperatures.83

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 215

propriate boundary conditions have been chosen, an additional criterion must still be invoked to decouple the growth velocity, ν, and the interlamellar spacing, λ. This problem of ‘spacing selection’ is the central unanswered question in the formation of lamellar patterns in the solid state. Traditionally a global optimization principle has been invoked. Zener47 and Hillert49 used the maximum growth rate hypothesis, Kirkaldy61 has considered an optimal rate of entropy production and Cahn50 has considered an optimal rate of free energy dissipation. If we consider, for example, the pearlite transformation, according to volume diffusion control, the optimal lamella spacing according to Zener’s maximum growth rate hypothesis and Kirkaldy’s maximum rate of entropy production are λ = 2λc and λ = 3λc . For boundary diffusion controlled growth, the corresponding values are λ = 1.5λc and λ = 2λc . The differences in spacing predicted by the two hypotheses differ only by a small factor. The accuracy with which diffusion coefficients are known does not allow us to differentiate between these two heuristic principles and, as is often the case with these pattern selection problems, the very question of the existence of a selected spacing is still open. Gust et al.84 have carefully measured the interlamellar spacing in selected discontinuous precipitation reactions and found that under isothermal conditions, not a single spacing but a Gaussian distribution of spacings is experimentally observed (Figure III.11). Similar observations were made by Duly et al.85 in their investigations of the discontinuous reaction in Mg-Al alloys. Solorzano and Purdy86 have examined Cahn’s maximum rate of free energy dissipation hypothesis by comparing the theoretical predictions with experimental results from the Mg-Al system. These authors calculated a dissipation function, GNET · ν as a function of interface velocity and interlamellar spacing. They did indeed find a maximum in the dissipation function for a particular velocity and that this maximum was highest for a particular interlamellar spacing. Example calculations for the Mg-9Al (wt.%) alloy at two temperatures are shown in Figure III.12. The numbers on the curves refer to the interlamellar spacings. Given the experimentally observed growth rates and interlamellar spacings and an estimate of the thermodynamic and kinetic properties of the boundary extracted from experimentally measured solute concentration profiles, Solorzano and Purdy estimated the remaining supersaturation in the lamella behind the moving interface and calculated GNET . The observed interlamellar spacings could then be compared with those predicted by a maximum rate of free energy dissipation by identifying the theoretical spacing which gave the highest value in the dissipation function for the 84 W. Gust, B. Predel, and U. Roll, Z. Metallkd. 68, 117 (1977). 85 L. Klinger, Y. Brechet, and D. Duly, Scripta mater. 37, 1237 (1997). 86 I. G. Solorzano and G. R. Purdy, Metall. Trans. A 15A, 1055 (1984).

216

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.11. Experimentally measured distribution of lamellar spacings in a Ni-31.7Zn (at.%) alloy treated for 24 h at 600 ◦ C.84 The distribution is well described as Gaussian.

experimentally observed velocity. It was found that from the myriad of possible kinetic states, the velocity/spacing pair selected were within a factor of ∼ 2 of that which would give a maximum in the rate of free energy dissipation. Considering the uncertainties in the thermodynamic quantities, in particular interfacial energies, the agreement was deemed encouraging.

a. Klinger’s Alternative for Discontinuous Precipitation Only recently, an alternative treatment of the diffusion problem for the discontinuous precipitation reaction has been supplied by Klinger et al.66 which provides a unique velocity/spacing pair and for which an additional ‘optimization’ criteria is not necessary. Klinger et al. realized that the degeneracy of the problem could be removed by invoking an additional local condition in the derivation rather than imposing an optimization principle on a relation between the interface velocity and the lamella spacing. The conditions imposed were all local in nature and relied on thermodynamic assumptions of local equilibrium, which may be arguable, but are at least clearly stated. The starting point of the approach is that both the α and the β lamellae must grow at the same rate, and that both these rates are diffusion controlled. The thermodynamic difference between the α0 /α interface and the α0 /β interfaces, which parallels the previously stated difference between

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 217

F IG . III.12. Computed variation of the dissipation function, (GNET .ν), as a function of discontinuous precipitation cell velocity in an Mg-9Al (wt.%) alloy. The calculations are performed at (a) 485 K and (b) 550 K for a range of interlamellar spacings (labelled).86

218

Y. BRÉCHET AND C. HUTCHINSON

pearlite and discontinuous precipitation, requires different treatments for the diffusion problem. In previous treatments of the reaction, the solute diffusion from the solute poor lamella to the solute rich lamellae was assumed to occur within the α/α0 grain boundary and was driven by concentration gradients. The nature of the β/α0 interface and the driving force for solute diffusion within this interface was not usually considered. Klinger et al. treated the growth of the α and β phases simultaneously, subject to conditions of equal growth velocities, but assumed that the diffusion in the α/α0 grain boundary was driven by concentration gradients and diffusion within the β/α0 interface boundary was driven by gradients in curvature. Such an assumption for the β/α0 interface boundary is physically based since the compound phase in discontinuous precipitation is very often a stoichiometric phase which offers very little range for concentration gradients. The treatment of the grain boundary followed the classical treatments of Cahn50 and Hillert57 and that of the interphase boundary followed the treatment of Mullins.87 An assumption of local equilibrium and diffusional flux continuity at the α/β/α0 triple junction was sufficient to remove the degeneracy of the problem and select a unique velocity/spacing pair. Klinger et al. compared their treatment with the available experimental data in the Al-Zn system and found good agreement using reasonable values of the unknown parameters. Klinger’s approach can be seen as an idealized, but tractable version of the problem. Each of the assumptions made can be relaxed through a more sophisticated treatment: local equilibrium assumptions can be modified to account for attachment kinetics, the thermodynamic model for the solid solution can be made more realistic, the shape of the moving interface can be left free: however, the solution is no longer analytic and numerical calculations are needed which show a rich variety of behavior. The important issue is that the intrinsic degeneracy of the spacing selection problem can be relieved by local assumptions and does not require the introduction of an additional optimization principle. 9. N ON -S TEADY S TATE G ROWTH In each of the theoretical treatments of growth discussed above, it is assumed that the lamellar pattern formed under steady state conditions of constant interlamellar spacing and growth rate. There are at least two sets of circumstances where the steady state hypothesis has been called into question and each will be briefly discussed. The first concerns the recent suggestions that growth is not a continuous process with a constant rate but rather a ‘stop and go’ process and as a result, the average growth rate, determined for example from metallographic measurements, 87 W. W. Mullins, J. Appl. Phys. 28, 333 (1957).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 219

must be differentiated from the instantaneous growth rate. The second case concerns the formation of so-called divergent lamellar aggregates. Observations of isothermal lamellar growth with a rate that decreases in time and an interlamellar spacing that increases in time have been observed in both the pearlite and discontinuous precipitation reactions and the theory is qualitatively well understood.

a. ‘Stop and Go’ Interface Motion On the basis of preliminary in-situ high voltage electron microscopy studies of the discontinuous precipitation reaction in an Al-Zn alloy, Bogel and Gust65 proposed that the reaction interface does not migrate in a continuous manner with a constant velocity but rather by a ‘stop and go’ process. Subsequent electron microscopy studies88 showed that this was observed experimentally and the plot of interface displacement versus time in Figure III.13 clearly shows the start-stop nature of the interface.

F IG . III.13. Interface migration distance as a function of time during discontinuous precipitation in an Al-15Zn (at.%) alloy transformed at 160 ◦ C.88 The measurements were made during the in-situ elevated temperature high-voltage electron microscopy observations. The stop-start nature of the interface migration is clearly shown in the plot. 88 S. Abdou, G. Solorzano, M. ElBoragy, W. Gust, and B. Predel, Scripta mater. 34, 1431 (1996).

220

Y. BRÉCHET AND C. HUTCHINSON

Bogel and Gust claim that the difference between the instantaneous interface velocity and the average value can be up to three orders of magnitude. Further indirect experimental evidence in support of the ‘stop and go’ motion was collected in Duly’s studies of the discontinuous precipitation reaction in the Mg-Al system.85 They found, as with previous investigators, that within a given lamellar colony, a range of lamella spacings is observed. When the solute profiles within the lamellae behind the reaction interface were measured, they could be fitted to Cahn’s equation (Eq. (3.7)) using an approximately constant α parameter. If cooperative motion does occur in a continuous and constant manner, then everywhere along a reaction front where the lamellar spacing changes, so too should the α parameter necessary to describe the solute profile left behind. For lamellar spacings that range from S/2 to 2S, we should expect to see a variation in the α parameter of a/4 to 4a, a factor of 16. Klinger et al.85 reinterpreted the observed chemical profiles in terms of a ‘stop and go’ motion of the interface and found that the approximately constant α parameter across a lamellar colony with varying lamellar spacing could be rationalized assuming the non-steady state type of growth proposed by Bogel and Gust.65

b. Divergent Lamellar Growth The second case of non-steady state lamella growth worth considering is the formation of aggregates with diverging lamellae. The lamellar product of eutectoid decomposition or discontinuous precipitation usually inherits the same overall composition as the parent phase and therefore it is assumed that a constant (average) growth prevails. Indeed, this is experimentally confirmed in most cases. However, if for some reason the growing aggregate is constrained to inherit a composition different from that of the parent phase then long range solute diffusion is necessary between the growing lamellar aggregate and the parent phase and growth with a constant rate cannot prevail. Non-steady state growth of both pearlite and discontinuous precipitation is possible and both have been observed. These observations are restricted to multi-component systems and the examples considered below are each taken from Fe-based systems containing both a substitutional and interstitial solute. We first consider non-steady state growth of pearlite, using the Fe-C-Mn system as an example before examining a counterpart discontinuous precipitation reaction found in high N austenitic stainless steels. Pearlite. Under conditions of constant temperature and pressure, the three phase equilibrium between the γ , α, and Fe3 C in the binary Fe-C system occurs at a single ‘eutectoid’ temperature (Figure III.1b). At temperatures below the eutectoid, the γ phase is unstable and the growing (α + Fe3 C) pearlitic aggregate consumes 100% of the parent γ phase and therefore is obliged to inherit the bulk

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 221

composition. However, in multi-component systems, the three phase equilibrium between the γ , α and M3 C (M = Fe + X), exists over a temperature range and a (γ + α + M3 C) three phase field is observed. It is within this (γ + α + M3 C) three phase field that non-steady state pearlite formation can occur. Two sections of the ternary Fe-C-Mn phase diagram are shown in Figure III.14.

F IG . III.14. (a) Isoplethal section of the Fe-C-Mn system sectioned at 5.42 (wt.%) Mn. The (γ + α + M3 C) three phase field is clearly labelled. (b) Fe-rich corner of an isothermal section of the Fe-C-Mn phase diagram sectioned at 625 ◦ C. Two alloy compositions are labelled. Alloy A lies within the (γ + α + M3 C) three phase field and Alloy B, within the (α + M3 C) two phase field.

222

Y. BRÉCHET AND C. HUTCHINSON

The isopleth shown in (a) is taken at a constant Mn content of 5.4 (wt.%) and the isotherm shown in (b) corresponds to a temperature of 625 ◦ C. In both diagrams the (γ + α + M3 C) three phase field is clearly labelled. For an alloy with the composition labelled A in Figure III.14b, the equilibrium compositions of the three phases correspond to the three corners of the three phase tie-triangle (bold). It is clear that for equilibrium to be achieved, significant Mn redistribution must occur from the α to the M3 C, and to a lesser degree to the γ and substantial C redistribution must occur from the α to the M3 C and a smaller redistribution from the γ to the growing lamellar aggregate. The case of Fe-C-Mn is a little more complicated because C diffusion in γ occurs 106 times faster than Mn at these temperatures and, in practice, the growing pearlite colony does inherit the bulk Mn content of the austenite (there is no long range Mn diffusion to or from the γ ). The Mn redistribution from the α to the M3 C occurs via short circuit diffusion in the reaction interface. Nevertheless, the short circuit Mn redistribution is still much slower than the significant long range C diffusion which must occur from the γ to the growing pearlite aggregate in addition to the short range C redistribution from the α to the M3 C, and the lamellar aggregate grows into what it sees to be a parent phase with a C content that decreases in time. As a result, the local equilibrium interfacial compositions (the boundary conditions of the diffusion problem) at the pearlite/γ interface change in time. The consequence is that the compositions inherited by both phases in the lamellar aggregate also continually changes in time and growth occurs with a rate that decreases in time and an interlamellar spacing that increases in time. The effect was first observed by Cahn and Hagel in 196276 and has since been observed in Fe-C-Si89 and Fe-C-Mo90 systems and has been discussed in detail by Hillert.91 If instead, an alloy composition such as B in Figure III.14b is chosen, which lies within the (α + M3 C) two phase field

F IG . III.15. (a) Optical micrograph of ‘divergent pearlite’ formed in an Fe-0.55C-5.42Mn (wt.%) alloy transformed for 384 h at 625 ◦ C. The M3 C phase contrast is dark and the α phase is light. The alloy composition is marked, A, in the Fe-C-Mn isothermal section (Figure III.14b). Pearlite growth for compositions lying within the (γ + α + M3 C) three phase field occurs with an interlamellar spacing that increases in time and a growth rate that decreases in time. (b) Scanning electron microscopy secondary electron image of a section of a pearlite colony in an Fe-0.54C-3.51Mn (wt.%) alloy treated at 625 ◦ C for 5 h. In this case, the M3 C phase contrast is light and the α phase is dark. The alloy composition, B, lies within the (α + M3 C) two phase field as marked in the isothermal section (Figure III.14b). For such alloy compositions, growth occurs with an approximately constant interlamellar spacing and rate. 89 J. Fridberg and M. Hillert, Acta metall. 18, 1253 (1970). 90 J. Fridberg and M. Hillert, Acta metall. 25, 19 (1977). 91 M. Hillert, in Solid Solid Phase Transformations, eds. H. I. Aaronson, D. E. Laughlin, R. F. Sekerka,

and C. M. Wayman, AIME (1981), p. 789.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 223

224

Y. BRÉCHET AND C. HUTCHINSON

of the phase diagram, γ is not stable, and as was the case for the binary Fe-C system, the growing pearlite is obliged to inherit the bulk alloy composition and steady state growth can be established. The Fe-C-Mn system has recently been analyzed in detail81 and micrographs of the pearlite formed in alloys A and B (Figure III.14b) and measurements of their growth rates at 625 ◦ C are shown in Figures III.15 and III.16, respectively. The divergency of the lamellar spacing of alloy A (Figure III.15a) and a growth rate which decreases in time (Figure III.16) are clearly contrasted with the steady state conditions which prevail for Alloy B (Figure III.15b). Discontinuous Precipitation. As was the case for the non-steady state pearlite growth described above, the occurrence of non-steady state discontinuous precipitation arises from conditions that result in the growing aggregate inheriting an overall composition different from the bulk parent phase (i.e., long range diffusion to or from the parent phase is necessary in addition to the short range redistribution between the lamella phases). The most thoroughly studied case

F IG . III.16. Experimentally measured pearlite growth rates as a function of time at 625 ◦ C in the alloy compositions marked A and B in the Fe-C-Mn isothermal section in Figure III.14b. Alloy A, located within the (γ + α + M3 C) three phase field forms with a growth rate that decreases in time. Alloy B, located within the (α + M3 C) two phase field, forms with an approximately constant growth rate.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 225

is the precipitation of Cr2 N in some Cr-Ni austenitic stainless steels. In a series of studies, Kikuchi92–94 examined the discontinuous precipitation of Cr2 N in several Fe-20Ni-25Cr (wt.%) alloys with varying N contents and measured the growth rates and interlamellar spacings at several temperatures. These are shown for a series of alloys treated at 1073 K in Figure III.17. For a given alloy, the isothermal growth rate of the lamellar aggregate can change by 4 orders of magnitude and the interlamellar spacing can increase four fold during the reaction. Using arguments based on Hillert’s theoretical discussion of the formation of divergent pearlite,91 Kikuchi et al.94 argues that for the alloys examined, under conditions where no long range diffusion of Ni or Cr occurs between the parent γ and the growing lamellar aggregate, to maintain local equilibrium between the lamellar phases, long range diffusion of N from the parent γ phase to the aggregate is necessary. Kikuchi et al.93,94 have shown experimentally that indeed no bulk diffusion of the substitutional solutes is observed for most of the reaction time and that the N content of the parent phase does decrease with time. As a result of the long range N diffusion, the lamellar aggregate grows into a parent phase whose composition is continually changing. The consequence is a continuous change in both the interfacial conditions at the moving boundary and the compositions inherited by the growing phases and results in lamellar aggregate growth with a velocity that decreases in time and an interlamellar spacing that increases in time. 10. C OARSENING AND R ELATED M ORPHOLOGICAL E VOLUTION The lamellar patterns arising from eutectoid decomposition and discontinuous precipitation are highly non-equilibrium structures. In both cases, energy is stored in the form of the interlamellar interfaces. In the case of the pearlite transformation, the compositions of the phases formed are usually relatively close to the equilibrium compositions found from the phase diagram and little chemical supersaturation generally exists (Figure III.5). However, the solute depleted lamellar phase in the discontinuous reaction necessarily retains some level of supersaturation and the non-equilibrium nature of this product is due to both the free energy stored in the interfaces and the residual chemical supersaturation. The relative contribution to the driving force from the chemical and surface terms will be system specific 92 M. Kajihara, S. Choi, M. Kikuchi, R. Tanaka, Y. Seo, T. Okumura, and Y. Kondoh, Z. Metallkd. 77, 515 (1986). 93 M. Kikuchi, T. Urabe, G. Cliff, and G. W. Lorimer, Acta metall. 38, 1115 (1990). 94 M. Kikuchi, M. Kajihara, and S. Choi, Mat. Sci. and Eng. A 146, 131 (1991).

226

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.17. (a) Experimentally measured discontinuous precipitation growth rates in a series of N containing Fe-25Cr-20Ni (wt.%) alloys transformed at 800 ◦ C.94 The growth rate decreases during growth. (b) Corresponding interlamellar spacings showing an increase in spacing during growth.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 227

and depend on the primary transformation conditions, but in most cases it is expected that the volumetric chemical term will dominate the surface term. Fournelle95 has estimated the magnitudes of the two contributions to the driving force for coarsening in a Fe-30Ni-6Ti (wt.%) alloy and found that for his conditions, the chemical term was two orders of magnitude larger than the surface term. For both types of lamellar products, the available stored energy provides a driving force for coarsening processes. The return towards equilibrium can take on two aspects: (a) the decrease in interfacial energy and (b) additionally for the discontinuous precipitation product, a decrease in the remaining supersaturation. The decrease in interface energy has obvious consequences in terms of the morphology and scale of the product phases. Just as is the case for precipitation, it can occur either continuously, or discontinuously through the migration of an interface.

a. Spheroidization The reduction in total interface area can be obtained at almost constant scale through a shape change. Since Lord Rayleigh’s96 seminal work on the stability of fluid jets, it is known that a cylinder can reduce its surface area by a continuous growth of perturbations towards the production of a series of spheres: this process is spontaneous (i.e., there is no energy barrier to be overcome) and is called ‘spheroidization’. The equivalent in the solid state has been analyzed by Nicols and Mullins.97 By contrast, a perfect lamellar structure of infinite extent is stable with respect to infinitesimal fluctuations (although the sphere of equivalent volume has an obvious advantage in terms of reduced surface energy). However, real lamellar structures are not perfect: the lamellae contain both boundaries and defects. The morphological instabilities of lamellar structures are bound to initiate at boundaries and defects and several different types of instabilities leading to spheroidization have been observed. Werner98 has recently reviewed these processes. By nature of the difference in interface curvature, a driving force exists for solute transport from the edge of a lamella plate to the flat face of the plate. This solute transport in itself can lead to the direct cylinderization of a plate, and the cylinder is then unstable with respect to the type of perturbations discussed by Lord Raleigh, giving rise to the formation of an aligned row of spheres, Figure III.18a.99 95 R. A. Fournelle, Acta metall. 27, 1147 (1979). 96 Lord Rayleigh, Proc. Lon. Math. Soc. 10, 4 (1879). 97 F. A. Nichols and W. W. Mullins, Trans. AIME 233, 1840 (1965). 98 E. Werner, Z. Metallkd. 81, 790 (1990). 99 T. H. Courtney and J. C. M. Kampe, Acta metall. 37, 1747 (1989).

228

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.18. Schematic illustration of the primary instability modes for an isolated plate.99 (a) A terminated plate may evolve into a cylinder as a result of capillarity driven mass transfer from the edges to the broad faces of the plate. Following ‘cylinderization’, a Raleigh instability causes the cylinder to decompose into a row of spheres. (b) The shape evolution gives rise to the pinching-off of a row of spheres along the edges of the plate (edge spheroidization). The spheres form as a result of perturbations developed along the ridge which forms at the edges during the first stages of mass transfer to the broad faces. (c) If boundaries are present in the plate, plate splitting may occur by sustained mass transport from boundary grooves to the broad face of the plate. Cylinderization and Raleigh instabilities can then follow.

Alternatively, part way through the cylinderization process of a plate, ridges may form along the edges and the partial cylinders at the edge of the plate may then decompose to rows of spheres directly on either side of the plate through the Raleigh instability. This process is shown schematically in Figure III.18b and is usually referred to as ‘edge spheroidization’. Both of these processes lead to a change in shape at approximately the same scale and arise naturally from the solute transfer driven from the curved boundaries of plates to the flat faces. Clearly, the boundaries from which transport occurs could equally be holes in the plates themselves rather than external edges. Lamella plates also often contain boundaries. These can be the result of faulting during growth, or boundaries formed during recovery and recrystallization. In either case, these boundaries can also act as sites for the splitting of plates through a ‘boundary grooving’ mechanism which has been discussed in detail by Mullins.87,100,101 The curvature of the 100 W. W. Mullins, Acta metall. 6, 414 (1958). 101 W. W. Mullins, Trans. AIME 218, 354 (1960).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 229

F IG . III.19. Schematic illustration of ‘fault migration’ during coarsening of lamellar structures.102 (a) Initial geometry, (b) migration of the faults and (c) bulged plate. The driving force for mass transfer is the difference in curvature at the termination and the branch.

surface of the plate in the vicinity of the boundary can be sufficient to drive solute away from the boundary region. To maintain the balance of surface tensions at the triple point between the boundary and the interlamellar interface, in the presence of solute transfer, the groove continually deepens along the boundary until it is entirely removed and the plate is split in two. This process is shown schematically in Figure III.18c. Each of the instabilities shown in Figure III.18 involves the splitting of individual plates; it is a change is shape at approximately the same scale and we shall refer to them all under the umbrella of spheroidization. The reduction in surface energy can also be obtained by increasing the scale of the microstructure. This increase in scale requires diffusional mass transport and the standard means is by bulk diffusion. This is the process of Oswald ripening which has been extensively studied, both experimentally and theoretically, and has been excellently reviewed many times (e.g., see Ref. [103]). An additional mechanism for accomplishing the change in scale involves the interactions between adjacent plates and is referred to as fault migration.102 In this case, the difference in curvature at the end of a terminated plate and on the broad face of an adjacent plate drives the dissolution of the faulted plate and the 102 H. E. Cline, Acta metall. 19, 481 (1971). 103 P. W. Voorhees, Ann. Rev. Mat. Sci. 22, 197 (1992).

230

Y. BRÉCHET AND C. HUTCHINSON

thickening of the adjacent plate by volume diffusion of the atomic species until the faulted region is entirely removed (Figure III.19). As we shall see below, when volume diffusion of solute is too slow, an alternative mechanism can take over.

b. Discontinuous Coarsening When bulk diffusion is too slow, the change in scale can be accomplished through discontinuous coarsening. This is a solution involving interface migration and interface diffusion and can take over from continuous coarsening (Ostwald ripening), just as discontinuous precipitation can take over from continuous precipitation in similar situations. Discontinuous coarsening is a moving boundary reaction that converts a fine lamellar pattern into a structurally and morphologically similar, but distinctly coarser pattern. As is the case for the very similar discontinuous precipitation, the solute redistribution during the discontinuous coarsening reaction occurs via short circuit diffusion in the migrating boundary and a discontinuous change in crystal orientation is observed across the boundary. Coarsening by this mode has been observed for lamellar products of both discontinuous precipitation and eutectoid decomposition and Manna et al.36 reports that it has been identified in more than 30 different alloy systems. A classic example104 of the discontinuous coarsening of a eutectoid lamellar aggregate in the Co-Si system is shown in Figure III.20. The kinetics of the coarsening process were first treated theoretically by Livingston and Cahn104 who were interested in the thermal stability of Co-Si, Cu-In and Ni-In aligned eutectoids. They were able to derive an expression for the velocity of the interface based on a solution to the diffusion equation and considering the change in interlamellar spacing, λ.

λOR sδD b σ Vm 8X β νDC = β , (3.10) 1 − X − X e fα2 fβ2 λ2DC λOR RT λDC X β is the equilibrium composition of the β phase, λOR is the lamellar spacing of the initial pattern and λDC is the spacing of the coarsened pattern. Livingston and Cahn were considering the coarsening of eutectoid products. They assumed that the driving force in this case arises mostly from a reduction in the interfacial energy stored in the interlamellar interfaces. However, for discontinuous coarsening of discontinuously precipitated lamellar aggregates the driving force for the coarsening process must include the contribution from the chemical 104 J. D. Livingston and J. W. Cahn, Acta metall. 22, 495 (1974).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 231

F IG . III.20. An optical micrograph of the discontinuous coarsening reaction in a Co-Si alloy treated for 4 days at 1000 ◦ C.104 The direction of grain boundary motion is indicated by the arrows.

supersaturation remaining in the aggregate. Fournelle,95 modified a previous treatment for discontinuous precipitation,56 and derived an expression for the coarsening rate that allows for the inclusion of both contributions to the driving force. νDC =

8GDC sδD b , RT λ2DC

(3.11)

GDC is the total driving force for the coarsening process and includes contributions from both the remaining chemical supersaturation and the interlamellar interfaces. Under conditions where the chemical supersaturation remaining in the lamellar aggregate after the initial reaction is very close to zero, Eq. (3.11) reduces to an expression very similar to that derived by Livingston and Cahn (Eq. (3.10)). It is clear from Eqs. (3.10) and (3.11), that a relation between the interface velocity and the interlamellar spacing is obtained. The two quantities are coupled and an identical spacing selection problem exists for the discontinuous coarsening reaction as for the discontinuous precipitation and pearlite transformations discussed in Section III.8.

232

Y. BRÉCHET AND C. HUTCHINSON

11. M ULTILAYER S TABILITY The pearlite and discontinuous precipitation reactions discussed in this chapter give rise to a solid state lamellar pattern with a characteristic spacing behind a migrating interphase or grain boundary. Some aspects of the problems are still not well understood (especially aspects concerning the initiation processes) and in an effort towards this goal, Klinger et al.105–107 has suggested that several fundamental questions could be addressed through studies of the thermal stability of multilayers. Carefully controlled multilayer fabrication using techniques such as molecular beam epitaxy (MBE) provide a convenient means of examining the evolution of heterogeneous systems far from equilibrium. To date, much of the work has concentrated on the evolution of the systems controlled by bulk diffusion (an example is the precise determinations of low temperature solute diffusivities108,109 ), but multilayer growth on bi-crystal substrates that would result in a boundary that penetrates the entire structure could provide a means of examining interface-mediated pattern evolution under conditions where the boundary can act as a short circuit diffusion path for solute. Klinger et al.105 have considered the homogenization of a fully miscible multilayer by boundary migration and have computed the boundary shape and velocity (pattern selection) as a function of the system dimensions and the relevant thermodynamic and kinetic parameters. They identify different homogenization ‘modes’ illustrated schematically in Figure III.21. At one extreme (a) the homogenization may occur by the steady state motion of the boundary and at the other (c) through the instability of the boundary and a resulting ‘fingering’ solution. They were concerned with the conditions that would lead to the different patterns. More recently, they have considered cases were a third phase may form at the interfaces in the multilayer and have calculated the resulting shape and velocity of the interface between the three phases.107 Experiments of the type proposed by Klinger et al. may well provide a means of addressing such questions as velocity and pattern selection in well controlled systems as a function of the thermodynamics and kinetics of the system chosen and could certainly lead to a deeper understanding of the evolution of the lamellar patterns discussed in this chapter. 105 L. Klinger, Y. Brechet, and G. Purdy, Acta mater. 45, 4667 (1997). 106 L. Klinger, Y. Brechet, and G. Purdy, Acta mater. 46, 2617 (1998). 107 L. Klinger, Y. Brechet, and G. Purdy, Acta mater. 47, 325 (1999). 108 A. L. Greer, Curr. Opin. Sol. State. Mat. Sci. 2, 300 (1997). 109 A. L. Greer, Ann. Rev. Mat. Sci. 17, 219 (1987).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 233

F IG . III.21. The different possibilities for discontinuous homogenization of a multilayer containing a moving grain boundary:105 (a) steady state motion of the grain boundary, (b) sinusoidal instability of the grain boundary and (c) fingering instability of a moving grain boundary.

IV. Structural Defect Patterning: Grain Growth, Recovery and Recrystallization

In the previous section, the patterning examined was of a chemical nature. The structural defect involved was an interface which separated the transformed (patterned) region from the untransformed and in some cases provided a short-circuit diffusion path for solute. In the following sections we will consider the patterning of the structural defects themselves in systems that can be considered to be nominally chemically homogeneous. The structural defects encountered in metals and alloys are of three types: point defects (vacancies and interstitials), line defects (dislocations), and planar defects (grain boundaries, interfaces and surfaces). Point defects have a low energetic cost and a high configurational entropy: they are weakly interacting and only at short distances. Vacancies have a finite equilibrium concentration which can be reached when the material is cooled very slowly. Transport occurs by diffusion, in response either to a gradient in concentration, or to a gradient in stress (the latter being responsible for diffusional creep). Line defects (dislocations) are much more disturbing for the theoretician: they have a high energetic cost and their configurational entropy is restricted by topological requirements (a dislocation line can’t end within the crystal). Their equilibrium density is virtually zero at any temperature, but nevertheless, even if the material is cooled very slowly, dislocations are almost always present (e.g., Frank

234

Y. BRÉCHET AND C. HUTCHINSON

network). The reason for their persistence is the threshold force required to move them. The existence of this ‘solid friction’, together with the topological requirements and the crystallographic constraints to their motion (glide and cross slip on definite planes) prevents the simple definition of a relevant thermodynamic potential which drives their evolution. To make the things worse, dislocations are associated with a long range stress field (which decreases as 1/r) and present short range reactions (junctions). Both of these aspects are crucial to the theory of plasticity: the long range stress field couples to the applied stress to give the Peach–Kohler force for dislocation motion under stress and the short range interaction and junction formation are responsible both for the work hardening of the material and for the very existence of the sources which produce the dislocations. Any physicist interested in plasticity should absolutely resist the temptation to forget either of these aspects. We have to deal both with out of equilibrium, long range interacting, non-conserved entities, and with short range reactions. The natural mode of dislocation motion is to glide in well defined crystallographic planes in response to a local stress which results from the superposition of the applied stress and of the stress arising from all of the surrounding dislocations. Grain boundaries are somewhat more tractable. Like dislocations, they are nonequilibrium entities, but they have no long range stress field. Except for some very special grain boundaries which have a limited mobility and a low energy, their structure is such that they can have enough flexibility and ability to move so that the thermodynamic situation of having no boundary is, in principle, attainable. The specific differences in these three basic defect entities will help explain the characteristics of the patterns they produce and the ease with which they can be explained. 12. G RAIN G ROWTH Grain growth is the simplest of the pattern forming systems.110 There is a well defined thermodynamic state to be reached (infinite grain size) and the entities to be eliminated have no long range interaction. This apparent theoretical simplicity is less obvious from the experimental investigations. Grain growth is a 3D phenomenon, however very few 3D experimental studies have been reported in the literature.111,112 Most experimental studies are made using 2D slices. In addition, the theoretical predictions are derived under the assumption of a linear relation between the boundary mobility and the local driving force (which is the 110 A. P. Sutton and R. W. Balluffi, Interfaces in Crystalline Solids, Oxford University Press, Oxford (1996). 111 F. N. Rhines and B. R. Patterson, Metall. Trans. A 13A, 985 (1982). 112 F. C. Hull, Mat. Sci. and Tech. 4, 778 (1988).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 235

reduction in grain boundary curvature, cf. Section II). Under these assumptions, the theories113–115 predict that the length scale should behave as t 1/2 and that the size distribution of the grains, when scaled with the average grain size, should be invariant. Experimentally, the 1/2 exponent is almost never observed, although numerical simulations predict it, regardless of whether the boundary mobilities and energies depend on boundary misorientation. This suggests that the linear relationship between the velocity and the driving force is not valid. Natural reasons could be the impurity drag on moving boundaries116 or the reduced mobility of triple junctions and quadruple points.117 However, in spite of the disagreement between the predicted and experimentally observed exponents, the existence of an invariant scaled grain size distribution is observed both experimentally and in computer simulations. Patterning in grain growth is to be understood as the characteristics of this self-similar behavior: (i) The existence and shape of an invariant scaled size distribution. (ii) Topological relations such as the relation between the average size of the neighboring grains, or the number of neighbors of a grain of given size. Since all simulations relying on a linear relation between local driving force and velocity must give a kinetic law in t 1/2 , the issues on patterning are rather on these two characteristics. Extensive reviews of the topological characteristics of ‘cellular structures’ can be found in the articles by Weaire and McMurry19 and Thompson.20 Here we will focus on some of the open questions related both to theoretical pattern formation, and to some of the specifics of ‘real systems’. Two types of computer simulations dominate the literature on grain growth. On one side are those based on an adaptation of the Potts model,118–120 and on the other are those based on a discretization of grain boundaries, called the ‘vertex model’.121–125 Both models have been run in 2D and 3D and give similar results, 113 J. E. Burke and D. Turnbull, Prog. Met. Phys. 3, 220 (1952). 114 W. W. Mullins, J. Appl. Phys. 27, 900 (1956). 115 M. Hillert, Acta metall. 13, 227 (1965). 116 J. W. Cahn, Acta metall. 10, 789 (1962). 117 G. Gottstein and L. S. Shvindlerman, Acta mater. 50, 703 (2002). 118 M. P. Anderson, D. J. Srolovitz, G. S. Grest, and P. S. Sahni, Acta metall. 32, 783 (1984). 119 M. P. Anderson, G. S. Grest, and D. J. Srolovitz, Phil. Mag. B 59, 293 (1989). 120 A. D. Rollett, D. J. Srolovitz, and M. P. Anderson, Acta metall. 37, 1227 (1989). 121 K. Fuchizaki, T. Kusaba, and K. Kawasaki, Phil. Mag. B 71, 333 (1995). 122 F. J. Humphreys, Scripta metall. mater. 27, 1557 (1992). 123 C. Maurice and F. J. Humphreys, in Proceedings of an International Conference on Thermomechanical Processing in Theory, Modelling and Practice, ed. B. Hutchinson, The Society, Stockholm (1997), p. 201. 124 D. Weygand, Y. Brechet, and J. Lepinoux, Phil. Mag. B 78, 329 (1998). 125 D. Weygand, Y. Brechet, J. Lepinoux, and W. Gust, Phil. Mag. B 79, 703 (1999).

236

Y. BRÉCHET AND C. HUTCHINSON

as far as the size distribution and topological relations are concerned. We will place emphasis on the vertex models since the input quantities are continuum ones (such as boundary energies or mobilities) which, in principle, can be derived from experimental measurements. In both 2D and 3D, a scaled grain size distribution is obtained in the computer simulations as shown in Figure IV.1. However, this distribution does not corresponds to Hillert’s distribution which is a sort of mean field distribution (i.e., it assumes that the average size around a given grain is the average grain size in the system). It seems that Louat’s distribution, which relies on the unrealistic assumption of the totally random motion of a grain in the space of grain sizes126 is much closer to the simulated distribution, whereas the experimental distributions are often observed to be Log Normal. The ubiquity of Log Normal distributions (also observed in precipitation) is a puzzle in metallurgy. It seems that, although they do not correspond to steady state solutions of the Normalized Fokker–Planck equation, the transient to depart from them is very long. However, the reason for their appearance in the first place remains unknown. The second item used to characterize the patterns, are local correlations. Two may be considered: (i) Grains larger than average are more likely to be surrounded by grains smaller than average (Figure IV.2a). (ii) Grains larger than average tend to have a larger number of neighbors (Figure IV.2b). The correlations captured in item (i) are not included in Hillert’s derivation and may be the reason for the discrepancies between computer simulations and Hillert’s prediction. The correlations included in item (ii) are necessary in the Ryum–Hunderi scaling theory127 which makes use of the Mullins–Von Neumann equation114 to calculate the growth rate of an individual grain. The scaling theory of Ryum–Hunderi127 describes very accurately the distribution observed in the simulation (Figure IV.3), but there is currently no analytical derivation of the correlation given in Figure IV.2b. Even in this simplest case of pattern formation (scaling in grain growth), the distributions predicted both by the theory and the simulations are not in agreement, and they both disagree with the experimental data which appears to be a Log Normal distribution. Besides the pure ‘statistical physics’ problem, which amounts to investigating domain sizes in a conserved order parameter system, one can also consider 126 N. P. Louat, Acta metall. 22, 721 (1974). 127 O. Hunderi and N. Ryum, J. Mat. Sci. 15, 1104 (1980).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 237

F IG . IV.1. (a) Scaled grain size distribution obtained from a 2D vertex dynamics simulation.124 The log normal distribution as well as the distributions predicted by Hillert115 and Louat126 are shown for comparison. (b) Scaled grain size distribution obtained from a 3D vertex dynamics simulation125 and the comparison with the log-normal distribution and a previous simulation by Fuchizaki et al.121

238

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.2. 2D vertex dynamics simulations illustrating: (a) the average size of the neighbors of a grain of a given size128 and (b) the average number of neighbors of a grain of given size.124

materials science specific issues: the anisotropy of grain boundary energies and mobilities, the finite mobility of triple junctions, pinning points, etc. For the sake 128 D. Weygand, PhD, Institut National Polytechnique de Grenoble, Grenoble (1998).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 239

F IG . IV.3. Grain size distribution of the 2D vertex dynamics simulation compared to the distribution from the Ryum–Hunderi scaling theory.128

of illustration, let us consider the effect of particle pinning on the patterns formed by an evolving grain structure.129 Of course, the pinning by particles (Zener Pinning) is known to lead to a stabilized grain size. The kinetics, as simulated by the vertex model, saturate toward this ultimate grain size according to a kinetic law corresponding to a subtraction from the capillary forces due to Zener pinning (which in itself is a surprising result since Zener pinning is in principle a threshold force). The simulated kinetics and the results of an analytical expression are shown in Figure IV.4. The distributions are of course non-scale invariant, but the final distributions can be accurately fitted by a log normal distribution (Figure IV.5). A perhaps more striking result is the behavior of the topological characteristics.128,130 As shown in Figure IV.6, the correlation between the grain size of the neighbors and the average grain size is expected to be exactly opposite that predicted for grain growth in the absence of particles. For this simple patterning system it seems that two ingredients are missing for a complete understanding: the analytical derivation of the local spatial correlations, and the reasons for the apparent stability of the Log Normal distribution for grain sizes. However, the tools developed for understanding the evolution of capillary driven structures does allow us to obtain a new insight into recrystallization and 129 D. Weygand, Y. Brechet, and J. Lepinoux, Acta mater. 47, 961 (1999). 130 D. Weygand, J. Lepinoux, and Y. Brechet, in ed. J. Driver, Annecy, France, in press (2004).

240

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.4. Vertex dynamics simulation of the kinetics of grain growth in the presence of pinning particles.129 The grain size has been normalized to its saturation value and the time has been rescaled accordingly.

recovery, which in turn will provide some important inputs for the understanding of pattern formation in plasticity. 13. R ECOVERY AND R ECRYSTALLIZATION OF D ISLOCATION S TRUCTURES When heavily deformed, metals store large quantities of dislocations, in more or less organized structures (see Section V for the origin of this patterning). This certainly increases the free energy of the system, and provided some sufficient mobility is available to the defects, they will tend to move in order to reduce this energy. Accordingly, the dislocation density decreases, the substructures evolves and the hardness of the material decreases. This evolution of the structural defects during annealing can be followed by the evolution of the hardness of the material. Two situations are possible: either the evolution is slow in time (typically logarithmic) and occurs approximately everywhere at the same time and is referred to as ‘recovery’, or it is rapid in time, occurs heterogeneously, and corresponds to the nucleation of new grains free from defects (recrystallization). A detailed review of these mechanisms and their experimental studies can be found in Refs. [21,131]. 131 R. D. Doherty, D. A. Hughes, F. J. Humphreys, J. J. Jonas, D. J.Jensen, M. E. Kassner, W. E. King, T. R. McNelley, H. J. McQueen, and A. D. Rollett, Mat. Sci. and Eng. A A238, 219 (1997).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 241

F IG . IV.5. Vertex dynamics simulations of the grain size distribution in the presence of particles, compared to the initial distribution.129

In the following, we will highlight some observations which may lead to a better insight into plastically induced patterning from their further thermal stability. The first remark concerns the role of fluctuations, whereas the second and third remarks concern the definition of a driving force for structural evolution. The first set of comments concerns the nucleation of recrystallization. It is tempting to consider the nucleation of a dislocation free grain as a classical nucleation process where the gain in bulk energy pays for the cost in surface energy. The size of nuclei is such that the classical theory would predict a ridiculously low nucleation rate.21 Recrystallization nucleation is often associated with preexisting heterogeneities in the material: undeformable particles or initial grain boundaries. It seems natural to assume that gradients in stored energy are responsible for the motion of a grain boundary which delimits the new grain. This is perfectly understandable for particle nucleated grains, since geometrically necessary dislocations accumulate around the undeformable particles. However, it is more difficult to envisage in the vicinity of the grain boundary. Even if there is some crystalline anisotropy which may lead to different stored energies depend-

242

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.6. The grain size correlation function for particle inhibited grain growth compared to the correlation for normal grain growth.128 With increasing grain size, the average grain size of the neighboring grains increases in the presence of particles. The opposite behavior is observed for normal grain growth.

ing on the crystallographic orientation of the grains, these differences would tend to vanish when plastic deformation increases to the level attained in cold rolling. The paradox is that it is precisely when the strain increases that the nucleation of new grains at the boundary becomes easier. The dislocations stored in the material during cold rolling organize themselves into subgrains. The subgrain misorientations will increase, and their size will decrease when the strain in increased. An estimate of the stored energy can be obtained from the average subgrain size and the average misorientation. A vertex type simulation was performed in a situation where, across a grain boundary, a difference in stored energy was mimicked by a difference in subgrain size.132 Sure enough, the bowing of the grain boundary was triggered by this somewhat artificial gradient. But another simulation can be made, with no macroscopic gradient between the two grains, but simply accounting for the fact that sub-boundaries have a lower energy and a lower mobility that a general grain boundary.133 With these simple ingredients, it is found that, below a critical subgrain size or above a critical subgrain misorientation (which both can be understood as a critical strain) the nucleation of new grains by bowing out 132 F. J. Humphreys, Acta mater. 45, 4231 (1997). 133 D. Weygand, Y. Brechet, and J. Lepinoux, Phil. Mag. B 80, 1987 (2000).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 243

occurs naturally (Figure IV.7). It is not the gradient in the average quantity, but the fluctuation in the quantity which drives the nucleation of a new pattern. The importance of the fluctuations, and the fact that they have been too neglected in the current treatments, is a remark we will come back to. The second remark comes from measurements of the kinetics of recovery. If the sub-boundaries arising from deformation were low energy equilibrium structures, then the subsequent evolution of the microstructure would be simple subgrain growth. There would be no qualitative difference between subgrain growth and grain growth (it has been shown that the introduction of the dependence of the energy and mobility on grain boundary misorientation may change the prefactor, but the power law in t 1/2 should survive). Since the yield stress scales as the inverse subgrain size, the decrease in hardness should also follow a power law behavior, and not logarithmic kinetics. The experimentally observed logarithmic kinetics indicates that subgrain growth is slower, and suggests that the sub-boundary energy is decreasing during recovery. From this fact we can infer that (i) the sub-boundaries formed during plastic deformation where not a minimum in energy, and (ii) the sub-boundaries probably tend to a structure with minimum energy during recovery. The third set of remarks relies on some experimental observations of recovery in Al-2.5%Mg alloys. These observations will also be useful to understand the nature of the patterns emerging from deformation. Recovery processes are in principle simple in the sense that the main parameter governing the evolution is time and not strain, and the system is out of equilibrium but not maintained far from equilibrium. The pertinent questions are: What is the evolution of dislocation density? How is it correlated to the evolution of internal stresses? What is the remaining stored energy in a system having undergone static recovery? Microdensity and resistivity134 can be used to measure dislocation densities, the analysis of X-ray broadening allows us to evaluate the screening of dislocations in their substructure and calorimetry allows us to measure the stored dislocation energy which is released during recrystallization. Combining these measures on deformed samples, recovered for different times, provides information both on the pattern emerging from deformation, and its subsequent stability.135–138 134 M. Verdier, PhD, Institut National Polytechnique de Grenoble, Grenoble (1992). 135 M. Verdier, I. Groma, L. Flandin, J. Lendvai, Y. Brechet, and P. Guyot, Scripta mater. 37, 449

(1997). 136 M. Verdier, M. Janecek, Y. Brechet, and P. Guyot, Mat. Sci. and Eng. A 248, 187 (1998). 137 M. Verdier, Y. Brechet, and P. Guyot, Acta mater. 47, 127 (1998). 138 M. Verdier, F. Bley, M. Janecek, F. Livet, J. P. Simon, and Y. Brechet, Mat. Sci. and Eng. A 234,

258 (1997).

244

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.7. The bulging mechanism for the nucleation of recrystallization calculated with 2D vertex dynamics simulations with no subgrain size misfit.133 (a) Initial configuration and (b)–(f) evolution sequence.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 245

The evolution of the dislocation density as a function of the cold rolling strain (ε) in an Al-Mg alloy is shown in Figure IV.8a. The dislocation storage is not simply proportional to the strain but involves also dynamic recovery taking place during deformation. As a consequence, the net dislocation storage rate decreases at large strains. Figure IV.8b shows the evolution of the dislocation density during recovery annealing. The behavior of the dislocation density with annealing time is characteristic of the recovery kinetics: a fast initial decrease followed by a slower decay at longer annealing times. The results from resistivity and from microdensity measurements are consistent. For each sample deformed and recovered, the density of dislocations is known. In order to check that the broadening of the Bragg peak was mainly due to dislocations, the line width at half maximum has been measured for various peaks. After recovery annealing, the broadening of the peak decreases. In order to extract some useful information about the dislocation microstructure from the X-ray broadening, one has to postulate a model for the spatial arrangement of the dislocations. Instead, some information can be obtained directly from the behavior of the tail of the peak. Ideally, for an infinite straight dislocation the asymptotic decay of the intensity at large scattering vectors (q) would behave as q −3 , whereas for a dislocation dipole configuration, because of the screening of the strain fields, the intensity would decrease more slowly, as q −2 . The asymptotic behavior of the intensity for large q therefore gives information about the screening of the dislocation interactions. After static recovery, the tails at large q exhibit a slower decrease. This evolution can be interpreted as a consequence of the rearrangement of the dislocations into self screened structures of lower energy (Figure IV.9). The density of dislocations can be estimated via the resistivity measurements which are directly related to the total length of dislocation core. The stored energy in a given state can be measured by the total energy released in the calorimeter when a sample is fully recrystallized. Figure IV.10 shows the stored energy as function of the dislocation density for increasing strains. Not only does the rough estimation of the stored energy given by ρμb2 /2 (ρ is the dislocation density, μ is the shear modulus and b is the burgers vector) tend to overestimate the true value, but including the logarithmic correction term (Ln(bρ 1/2 )) is also insufficient. This clearly shows that, while deformation increases, and as dislocation structures become better defined, the dislocation stress fields are more and more efficiently screened. This effect parallels the screening effect evidenced by the X-ray analysis. During recovery, the dislocation density decreases, as expected. But the decrease in energy is much lower than would be expected from the simple estimates from the relation between dislocation density and energy in a cold rolled sample. Everything behaves as if there was a ‘marginal cost’ to incorporate and remove a dislocation from a given structure. This ‘chemical potential’ for dislocations governs the decrease of stored energy during recovery, as seen in Figure IV.11.

246

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.8. The evolution of the dislocation density (a) as a function of the cold rolling strain, ε, in an Al-Mg alloy and (b) during annealing of deformed Al-Mg samples at 160 ◦ C and 220 ◦ C.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 247

F IG . IV.9. Evolution of the X-ray Bragg peak during recovery of a deformed Al-Mg alloy after cold rolling to ε = 3.

F IG . IV.10. Comparison between the measured stored energy (EDSC ) and the calculated E(ρ) using the classical expression with a cut-off radius Re = 1/vρ, as a function of the dislocation density at different cold rolling strains in an Al-Mg alloy.

248

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.11. Evolution of the stored energy during cold rolling and after recovery of ε = 3 at T = 220 ◦ C as a function of the dislocation density in an Al-Mg alloy.

The main points to be retained from these results are the following: (i) The dislocations structures emerging from cold deformation are not low energy structures: recovery leads to lower energy structures as well as to the reduction of their number per unit volume. (ii) Dislocation density is not a sufficient variable to characterize a deformed state and the associated microstructure: as far a stored energy is concerned, the self screening of dislocations is an essential parameter. These facts will provide guidelines to evaluate the existing models for dislocation patterning. V. Structural Defect Patterning: Irradiation and Plastic Deformation

From the previous statements, one can infer that two factors will plague the understanding of patterns associated with dislocations. On one hand, the screening of the long range interactions between dislocations must be considered and this will be a key issue for understanding patterning. On the other hand, the motion of dislocations in response to an applied stress field must also be adequately addressed. Both of these aspects present current difficulties for the theoretician. In this sense, irradiation and plasticity are quite different. Irradiation induced dislocations are loops whose far field elastic stresses are much smaller than those

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 249

associated with long dislocations generated by plasticity. Furthermore, whereas the point defects generated by irradiation are mobile entities, irradiation loops are effectively immobile. As a result of these two ‘simplifications’ our understanding of patterning in irradiation is more advanced than our understanding of patterns obtained during plastic deformation. 14. I RRADIATION I NDUCED PATTERNING The main effect of irradiation is the generation of point defects (both interstitials and vacancies139 ). These defects, far in excess of the equilibrium concentrations, tend to agglomerate140 in the form of either irradiation loops or voids.139,141 An example in an irradiated stainless steel142 is shown in Figure V.1. The defects visible in Figure V.1 are clearly not well organized. However, under particular conditions, these structural defects generated from the excess point defects do tend to self-organize into strikingly regular patterns as shown in Figure V.2.143,144

a. The Experimental Facts: Dislocation Carpets and Void Lattices Detailed accounts of the experimental characteristics of irradiation patterns can be found in numerous reviews (Refs. [145–148] for voids and bubble lattices, Refs. [149–152] for dislocation patterning). We will focus our attention on the main features relevant to the modeling of irradiation patterns as dynamic instabilities. The patterns shown in Figure V.2 have two seemingly contradictory characteristic features: their scale is very small, but still much larger than the interatomic 139 M. T. Robinson, J. Nucl. Mat. 216, 1 (1994). 140 A. Barbu and G. Martin, Solid State Phenomena 30–31, 179 (1993). 141 A. Barbu, G. Martin, and L. Howe, in Basic Mechanical Properties and Lattice Defects of Inter-

metallic Compounds, eds. J. Westbrook and R. Fleisher, Wiley and Sons, New York (2000), p. 181. 142 C. Pokor, Y. Brechet, P. Dubuisson, and J. P. Massoud, J. Nucl. Mat. 326, 19 (2004). 143 W. Jager, P. Ehrhart, and W. Schilling, Solid State Phenomena 3–4, 279 (1988). 144 G. L. Kulcinski and J. L. Brimhall, in Effects of Irradiation on Substructure and Mechanical Properties of Metals and Alloys, ed. J. Mateff, ASTM (1973), p. 258. 145 J. H. Evans, Nature 229, 403 (1971). 146 J. H. Evans, Solid State Phenomena 3–4, 303 (1988). 147 J. H. Evans, Rad. Eff. 10, 55 (1971). 148 S. L. Sass and B. L. Eyre, Phil. Mag. 27, 1447 (1973). 149 D. J. Mazey and J. H. Evans, J. Nucl. Mat. 138, 16 (1986). 150 J. O. Stiegler and K. Farrell, Scripta metall. 8, 651 (1974). 151 W. Jager, P. Ehrhart, and W. Schilling, Rad. Eff. Def. Solids 113, 201 (1990). 152 R. Bullough, B. L. Eyre, and K. Krishan, Proc. Roy. Soc. London A 346, 81 (1975).

250

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.1. (a) Irradiation loops and (b) irradiation voids in an irradiated stainless steel.142

F IG . V.2. Self-organizing patterns under irradiation. (a) Dislocation carpets in Cu (periodic arrays of vacancy loops).143 (b) Nb void lattices: electron micrograph showing a BCC void superlattice in Nb irradiated with Ta+ ions at 800 ◦ C.144 The foil orientation is near 111.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 251

252

Y. BRÉCHET AND C. HUTCHINSON

spacing (at least two orders of magnitude) and their alignment reflects the underlying crystallography of the lattice. In Figure V.2a, the dislocation vacancy loops generating the ‘carpet pattern’ in irradiated Cu are aligned along (001) planes. The 3D void lattice in irradiated Nb shown in Figure V.2b has the same symmetry and orientation as the underlying crystalline host lattice. The obvious question is what mechanism could transfer anisotropy at the atomistic level into patterns at a scale two orders of magnitude larger. These well organized patterns are not observed under all irradiation conditions. The dislocation patterns become regular when the irradiation flux exceeds some critical value which is an increasing function of the irradiation temperature. However, the wave length developed seems to depend little on the irradiation conditions. If the flux exceeds a second critical value, the dislocation microstructure loses its regular patterning. The values of these two critical fluxes depend on the system and on the material purity. The void lattice (Figure V.2b) seems to nucleate first at random, and then to order at a later stage when the irradiation dose has become sufficiently high. The conditions for void ordering also depend on the level of purity of the alloys and on their gas content. The void lattice parameter seems to depend on temperature and irradiation flux mainly through the total fraction of voids generated after a given irradiation dose.

b. The Framework of a ‘Reaction Diffusion’ Approach The main effect of irradiation is to generate point defects (and possibly gases). These entities interact to create the mesoscopic defects whose patterning is of interest here: the point defects can generate dislocation loops and vacancies and gases can form bubbles. The point defects can also interact with the defects they have already formed. For example, the diffusion of vacancies or interstitials to the stationary dislocation loops and voids can give rise to absorption events. These mechanisms provide a framework for a ‘chemical kinetics’ approach to the evolution of the population of defects. A set of rate equations can be written to describe the evolution of the defect populations. The point defects (vacancies or interstitials) will be indexed by r, and the microstructural features (dislocation loops, vacancies clusters, voids) by q. Each defect in concentration, Cr , will be generated at a rate Pr by irradiation damage, and can be annihilated or created on either pre-existing sinks (such as grains boundaries) or those created by irradiation. Annihilation may also occur by pairs of vacancies/interstitials. A further feature of the rate equations is that the absorption of point defects by features such as dislocations presents a bias in favor of the interstitials. The rate of absorption is related to the mobility of point defects and therefore to their diffusion coefficients, whereas the relevant microstructural features are the defect densities and sizes.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 253

The volume fraction Qq occupied by a given type of microstructural feature (e.g., voids) may either grow or decay from the absorption or emission of point defects. The details of these equations will depend on the nature of the microstructural features under consideration, but the form of the equations is quite general. The form of the ‘rate equations’ for the point defects and the microstructural features can be written: C˙ r = Pr − AC1 C2 + r (Cr , Qq ) (5.1) ˙ q = Pq + (Cr , Qq ). Q These general ‘rate equations’, initially defined by Bullough et al.,152–154 can be used to study the evolution of the specific features one is attempting to describe. For example, if the evolution of the distribution of dislocation loops is of concern, a detailed solution of the problem, using a Fokker–Plank approach, allows for a description of the number and size distribution.142 If patterning (dislocation patterning or void patterning) is the phenomenon which has to be described, a spatial variable must be added. This appears as a diffusion term in the rate equation for the point defects. The microstructural features such as voids and dislocations are not supposed to move in space and their patterning reflects only the patterning in the field of the point defects. An example of such an approach was proposed by Murphy154 for the patterning of vacancy loops. The technique used is always the same: one searches for a homogeneous steady-state solution to the rate equations, and then performs a linear stability analysis with respect to infinitesimal perturbations periodic in space. When at least one eigenvalue of the linearized equations in Fourier space has a positive real part, the corresponding eigenmode will grown and lead to a periodic pattern. This very simple linear stability analysis is able to provide a qualitative understanding of dislocation loop patterning, but is unable to provide a quantitative prediction for the selected wavelength. In order to go further, a non-linear analysis of the same set of rate equations must be performed. In a series of papers, Ghoniem and Walgraef155–158 have thoroughly investigated this problem, both with weakly non-linear analysis (the next term in the expansion in terms of the amplitude of the perturbation) and with numerical simulations. They investigated the influence of defect densities (initial dislocation network) on the wavelength. The values of the parameters which lead to patterning have been derived and the ratio of the absorption bias to the emission bias 153 K. Krishan, Solid State Phenomena 3–4, 267 (1988). 154 S. M. Murphy, Solid State Phenomena 3–4, 295 (1988). 155 N. M. Ghoniem, D. Walgraef, and S. J. Zinkle, J. Comp. Aid. Mat. Des. 8, 1 (2002). 156 D. Walgraef and N. M. Ghoniem, Phys. Rev. B 39, 8867 (1989). 157 N. M. Ghoniem and D. Walgraef, Mod. Sim. Mat. Sci. and Eng. 1, 569 (1993). 158 D. Walgraef, J. Lauzeral, and N. M. Ghoniem, Phys. Rev. B 53, 14782 (1996).

254

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.3. Comparison between experimental data and theoretical predictions for the temperature and dose rate dependence of defect cluster wall observations in irradiated Ni.155 The filled symbols denote conditions where defect cluster wall formation was observed.

seems to play a key role. The anisotropy of diffusion of self interstitial atoms is held responsible for the crystallographic nature of the patterning of both the dislocation loops and the voids. It was also shown that this anisotropy need not to be larger than 1% to give a very well defined crystallographic organization. The conditions for patterning appear to be that the rate of point defect absorption exceeds their mutual annihilation, and that cascade induced vacancy cluster densities are above some critical value. These conditions lead to the prediction of the ranges in temperature and irradiation conditions for which dislocation patterning is expected (Figure V.3).155 When the temperature is too high, the cluster evaporation decreases the net absorption rate by dislocation loops and when the temperature is too low the recombination between vacancies and interstitials dominates. Dislocation patterning is observed only within these two limiting temperatures. The case of void formation is somewhat different: voids seem to nucleate ‘at random’, and progressively organize.146 The crystallographic organization of the void lattice has also been interpreted as a consequence of the anisotropy of self interstitial diffusion. Furthermore, it has been shown that when a void is slightly displaced from its position in a regular lattice, it will tend to grow in an anisotropic

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 255

manner, to bring it back to a central position.159 This amounts to having a drift force on the void mediated by the diffusion field of point defects. In the case of the dislocation carpets discussed above it is assumed that spatial motion is only possible for the point defects. The dislocations themselves are assumed stationary. Such models are bound to fail in describing pattern formation for entities which are nucleated at random with a substantial size. For void patterning, it seems that the long range repulsive forces described above play a key role, more so than a diffusional instability. A similar situation will be suggested for dislocation patterning in plasticity. 15. P LASTICITY I NDUCED PATTERNING The first feature which arises from dislocation patterning in plasticity, especially when compared to the dislocation patterns issued from irradiation, is their relatively coarse scale (for an overview of experimental results for F.C.C. metals, see Ref. [160]). The scale is at least one order of magnitude larger than the ‘carpet structures’ developed under irradiation. This in itself can be seen as a sign of the long range elastic interactions between dislocations, and as a consequence of the dislocation glide transport mechanism which is far more efficient than diffusion.

a. The Experimental Facts When plastic deformation takes place in a polycrystal, multiple slip systems are generally activated. The dislocations generated on these different slip systems interact and the material hardens. Eventually the flow stress reaches a saturation level where the annihilation of dislocations balances the accumulation. At large enough strains (or more accurately for large enough dislocation densities, i.e., when the interaction between dislocations exceeds the lattice friction) a cellular structure will form. The material is a composite structure of regions virtually free of dislocations (cell interiors) separated by regions of high dislocation densities (cell walls). The experimental conditions (T , ε) for the emergence of a cell structure in Fe are shown in Figure V.4.161 At low temperatures the lattice friction is difficult to overcome and the dislocation pattern remains planar rather than cellular. For F.C.C. materials, the lattice friction stress is generally negligible and cellular patterns emerge more readily than in BCC and HCP metals. When alloying 159 P. Benoist and G. Martin, in Proceedings of an Internations Conference on Fundamental Aspects of Radiation Damage in Metals, Gatlinberg, Tennessee (1975), p. 1236. 160 B. Bay, N. Hansen, D. A. Hughes, and D. Kuhlmann-Wilsdorf, Acta metall mater. 40, 205 (1992). 161 A. S. Keh and S. Weissmann, in Electron Microscopy and Strength of Metals, eds. G. Thomas and G. Washburn, Interscience, New York (1963), p. 231.

256

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.4. The transition between uniform and cellular dislocation structures in α-Fe as a function of strain and temperature.161

elements are added, any phenomenon which promotes the planarity of the slip (e.g., decreases the stacking fault energy, presence of shearable precipitates, etc.) will postpone to larger strains and larger dislocation densities the emergence of a cellular structure. The higher the deformation temperature, the better defined are the cells, i.e., the narrower are the cell walls.162 Some examples taken from Ni, Cu and Al are shown in Figure V.5.163 The cell structure has a scale D which is inversely proportional to the flow stress, as shown in Figure V.6.164 The relation between D (normalized by the Burgers vector b) and σ (normalized by the shear modulus μ) is given by Eq. (5.2). The constant K is close to 20. b σ =K μ D

(5.2)

The 3D patterns developed during large strains have been extensively reviewed. They show the emergence of patterns elongated in the direction of cold rolling and the initiation of bands of intense localization of plastic strains, probably associated with crystalline rotations.160 In addition to this self imposed ‘scale’, more recent detailed examination of the apparent length scales at different magnifications have revealed the existence of a 162 M. R. Staker and D. L. Holt, Acta metall. 20, 569 (1972). 163 I. Barker, N. Hansen, and B. Ralph, Mat. Sci. and Eng. A A113, 449 (1989). 164 S. V. Raj and G. M. Pharr, Mat. Sci. and Eng. 81, 217 (1986).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 257

(a)

(b)

(c)

F IG . V.5. Bright field transmission electron microscope images of some FCC metals deformed to a true strain of 0.1.163 (a) Ni, (b) Cu and (c) Al.

258

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.6. The relation between reduced cell size, D/b, and reduced flow stress, σ/μ, in (a) Fe and (b) Al.164

fractal structure in the dislocation cells.165 The scaling works over two orders of magnitude for the cell sizes and the fractal dimension of the 2D slices of the cell structure ranges between 1.6 to 1.8 (with increasing flow stress), Figure V.7. As pointed out by Kubin,166 the scaling relation between the flow stress and the dislocation cell size (Eq. (5.2)) can be readily obtained either from the dependence in 1/r of the dislocation stress field, or from the dependence in 1/D of the activation stress for a source whose pinning points are separated by a distance D. Therefore, any acceptable theory for pattern formation should lead to this scaling law. The differentiation between the different theories should be made on the basis of both their predictions for the constant K and their ability to predict the conditions under which patterning is observed.

b. The Limits of Classical Approaches for Pattern Formation Let us begin by summarizing a few key features of the formation of dislocation cells. • Since dislocation patterning occurs during plastic deformation, and well before the saturation stress is reached, it should be considered as a dynamic instability, not an organization of a given number of dislocations. 165 P. Hähner, K. Bay, and M. Zaiser, Phys. Rev. Letts. 81, 2470 (1998). 166 L. P. Kubin, in Materials Science and Technology: Vol. 6 Plastic Deformation and Fracture of

Materials, ed. H. Mughrabi, VCH, Weinheim (1993), p. 138.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 259

F IG . V.7. (a) Bright field transmission electron micrograph of the dislocation cell structure in a Cu single crystal after tensile deformation along a [100] direction at room temperature to a stress of 75.6 MPa. (b) Analysis of the cell structure shown in (a) by determining the ‘box dimension’ DB .165

260

Y. BRÉCHET AND C. HUTCHINSON

• Since cell formation is postponed by planarity of slip, and multiple slip seems necessary for the appearance of cells, the local reactions between different dislocation families must be a key ingredient for pattern formation. • Since cellular patterns are observed only when the long range stresses between dislocations overcome the short range lattice friction stress, it is also necessary to include the stress field of a dislocation distribution as a crucial ingredient for pattern formation. The classical approaches to dislocation patterning all fail in at least one of the above respects. The first theory for dislocation patterning, due to Holt,167 considers the formation of a cellular structure as an instability in a population of a given density of dislocations. He considers a two-dimensional distribution of supposedly infinite dislocation lines, and no short range reactions are allowed. The correlation function between dislocations is assumed to vanish on distances which are of the order of ρ −1/2 where ρ is the dislocation density. Under these conditions, the system is expected to spontaneously ‘un-mix’ by a spinodal-like instability, the fastest growing wavelength being proportional to the cut-off radius. Since the flow stress is proportional to ρ 1/2 , this gives the expected scaling law. However, besides the simplistic 2D realization, the model is fundamentally flawed in two respects: (a) the dislocations are assumed to respond to the internal stress only, whereas they should also be responding to the applied stress, and (b) the dislocation density is assumed to be constant, whereas this is obviously not generally the case during plastic deformation. Furthermore, in order to write the appropriate ‘diffusion-like’ equation for dislocation motion, the existence of a cut-off radius is crucial, and this gives the emergence of a characteristic length. The question of the spontaneous emergence of the screening length appears as a crucial issue in the problem of patterning and must be solved in a self consistent manner, not imposed ‘a priori’. The Holt model is, in essence, a model to minimize the energy of a closed system, whereas dislocation patterning is a dynamic instability in an open system. Along similar lines of a minimization of the total energy at constant dislocation density and in the absence of an external applied stress, is the family of models known as LEDS (Low Energy Dislocation Structures).168–172 These 167 D. L. Holt, J. Appl. Phys. 41, 3197 (1970). 168 D. Kuhlmann-Wilsdorf, Metall. Trans. A 16A, 2091 (1985). 169 D. Kuhlmann-Wilsdorf, Trans. AIME 224, 1047 (1962). 170 N. Hansen and D. Kuhlmann-Wilsdorf, Mat. Sci. and Eng. 81, 141 (1986). 171 D. Kuhlmann-Wilsdorf, Mat. Sci. and Eng. A A113, 1 (1989). 172 U. F. Kocks, T. Hasegawa, and R. O. Scattergood, Scripta metall. 14, 449 (1980).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 261

models describe the scaling law, which only means that they are dimensionally correct, but they cannot describe the dynamic nature of the instability. A completely different route was proposed by Kocks.173,174 Whereas the previous models insisted on the forces acting on the dislocations, Kocks insisted on including the short range reactions between dislocations in their glide plane when they interact with the forest made by dislocations from other glide planes. The key idea is that the building up of a cell structure is intrinsically a statistical problem: regions where the forest trees are to narrowly spaced will not be penetrable by the gliding dislocations, which will leave around these regions loops which will make them even more impenetrable. Since the only length scale in the problem is ρ −1/2 , the distance between hard points will scale as this distance, which will indeed give the correct scaling law, since the flow stress scales as ρ 1/2 . The simulations performed by Kocks confirm this finding. However the flaw in the approach is in two respects. On the one hand, dislocation patterning occurs in multiple slip and the forest dislocation density is certainly not constant, as is assumed in stage II work hardening. On the other hand, the hard points created by the mere fact that forest dislocations are too close together, are not really so hard. They may be too hard to be penetrated by the applied stress, but once a loop is left behind, they may be penetrated by the combined effect of the applied stress and the line tension. In order to stabilize these hard points, local reactions due to recovery are necessary to create sessile obstacles. The dynamic nature of dislocation patterning and the non-conserved character of dislocations (i.e., their ability to annihilate by pairs or to multiply via various source mechanisms) has triggered interest in a ‘chemical kinetics’ approach. Various detailed sets of equations have been proposed,174–182 but the framework always remains the same. The density of dislocations is divided into different ‘species’, ρi , each with a flux, Ji . The reaction terms (annihilation, 173 U. F. Kocks, in Dislocations and Properties of Real Materials, The Institute of Metals, London

(1985), p. 125. 174 U. F. Kocks, A. S. Argon, and M. F. Ashby, Prog. Mat. Sci. 19, 1 (1975). 175 D. Walgraef and E. C. Aifantis, J. Appl. Phys. 58, 688 (1985). 176 L. P. Kubin and J. Lepinoux, in Proceedings of an International Conference of the Strength of Metals and Alloys (ICSMA8), Vol. 1, eds. P. O. Kettunen, T. K. Lepisto, and M. E. Lehtonen, Pergamon, Tampere, Finland (1988) p. 35. 177 U. Essmann and K. Differt, Scripta metall. 22, 1337 (1988). 178 K. Differt and U. Essmann, Mat. Sci. and Eng. A A164, 295 (1993). 179 G. Malygin, Soviet Physics State Solid 31, 96 (1989). 180 G. Malygin, Physics-Uspekhi 42, 887 (1999). 181 Y. Estrin and L. P. Kubin, Acta metall. 34, 2455 (1986). 182 L. P. Kubin, in NATO ASI Series: Stability of Materials, eds. A. Gonis, P. E. A. Turchi, and J. Kudrnovsky, Plenum, New York (1995), p. 99.

262

Y. BRÉCHET AND C. HUTCHINSON

multiplication. . .) are embedded into a function R(ρi , ρj , σ ) and the evolution equations can then be written as: ∂ρi + div(Ji ) = R(ρi , ρj , σ ) ∂t

(5.3)

In some cases, when only dynamic processes are involved (i.e., when R is proportional to the velocity of dislocations), the differential equation can be written in terms of derivatives with respect to ε. The difficulty in the approach is in the expression of Ji . The flux is obviously related to the dislocation densities and velocities, and the velocities are related to the applied stress, σa , and to the internal stress, σint , due to the other dislocations by an ‘effective’ dislocation mobility, M. Ji = ρi V = ρi M(σa − σint )

(5.4)

All the difficulty lies in the evaluation of the internal stress. Since the dislocation field is long ranged, the expression for the internal stress is given by an integral, and only an expansion of this integral in terms of gradients in ρ allows us to reach an expression for σint which is local. Under this very questionable assumption, the basic equation can be reduced to a ‘reaction diffusion’ approach for which the standard techniques can be applied. Another simplified condition under which a ‘diffusion’ term can be obtained is the case of spreading of the dislocation density via random events such as double cross-slip. But again, this procedure hides the fundamental fact that dislocations are gliding and not diffusing, and that the long range fields cannot be assumed to be screened without further justification. This is probably the reason why ‘reaction diffusion’ approaches have never been able to present for dislocation patterning the same success they have shown for irradiation patterning. In spite of these pitfalls, the various ‘classical approaches’ presented above have brought to the forefront the key issues that need to be addressed by a future ‘theory of dislocation patterning’: – local reactions must be accounted for, and in particular, the non-conservative nature of dislocation densities; – long range stresses have to be accounted for, and the self-screening of dislocations, which can even be measured experimentally,183,184 must be derived as part of the solution of the problem. 183 T. Ungar, L. S. Toth, J. Illy, and I. Kovacs, Acta metall. 34, 1257 (1986). 184 T. Ungar, H. Mughrabi, D. Ronnpagel, and M. Wilkens, Acta metall. 32, 333 (1984).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 263

As a result of the difficulty in addressing these questions in an analytical manner, without making unreasonable assumptions, computer simulations of dislocation dynamics have been proposed to investigate the collective behavior of dislocation populations, and in particular, their tendency to patterning.185

c. Computer Simulations of Pattern Formation The principle of all simulations described below is first to compute for each dislocation segment the local stress arising from the applied stress and from the interactions with other dislocations in the system. Under this local stress, each dislocation will move at a particular velocity. The simulations differ in the variety of local reactions allowed (multiplications, annihilation, junction formation), on the degree of naivety with which they are described and in the range of strains (or equivalently dislocation densities, or volume simulated) they can treat in a reasonable computing time. The first simulation,186,187 a cellular automaton carried out in two dimensions, included, for reasons of computational efficiency, a cut-off radius for dislocation interactions. Calculations were made with and without an externally applied stress. When no external stress was applied, but with the dislocation interactions artificially screened, the instabilities occur, and a length scale emerges which is related to the cut-off radius. When the long range interactions were accounted for without an imposed cut-off radius, as was done in another group of simulations using Molecular Dynamics techniques,188,189 the patterning disappears. In any case, a partial self-screening is observed, in the sense that during relaxation, the net interaction stress with other dislocations is decreasing. When an external stress is applied, and no cut-off radius is artificially imposed, no clear patterning seems to occur. The definitions of the local rules for multiplication, which are randomly positioned in an artificial manner, are obviously too naïve to capture the spatial organization. In spite of the numerical and topological difficulties associated with the 3D aspect of dislocation dynamics, it seemed necessary to go one step further and to explicitly include the long range dislocation interactions, the friction stress, the junction formation, dislocation multiplications and the various glide and cross 185 L. P. Kubin, Y. Estrin, and G. Canova, in NATO ASI: Patterns, Defects and Material Instabilities,

ed. D. Walgraef, Kluwer (1989). 186 J. Lepinoux and L. P. Kubin, Scripta metall. 21, 833 (1987). 187 J. Lepinoux, Solid State Phenomena 3–4, 389 (1988). 188 N. M. Ghoniem and R. J. Amodeo, Solid State Phenomena 3–4, 377 (1988). 189 R. J. Amodeo and N. M. Ghoniem, Phys. Rev. B 41, 6958 (1990).

264

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.8. (a) Thin (111) slice (1 μm thickness) extracted from the simulated dislocation structure of a [100] aluminium crystal after deformation. (b) The corresponding mapping of the internal shear stress field resolved in the same plane.196

slip processes.190–195 The details of the 3D dislocation simulation, known as DDD (Discrete Dislocation Dynamics) can be found in Ref. [196]. This ambitious program has been developed over the years and has finally led to the simulation of an emerging dislocation structure associated with a spatial patterning of the internal stress.196,197 An example is shown in Figure V.8. The limitations in terms of plastic strain attainable in a reasonable computational time, as well as the rather poorly defined cellular structure, prevents testing of the scaling law for cell size as function of the flow stress, although the length scale observed is reasonable. The lesson to be learnt from both the 2D and the 3D simulations is that both long range stresses and short distance reactions are necessary to obtain patterning, and that the short range reactions must be described with a sufficient spatial accuracy. The fact that a source is unlikely to operate 190 L. P. Kubin and G. Canova, Scripta metall. mater. 27, 957 (1992). 191 L. P. Kubin and G. Canova, in Electron Microscopy in Plasticity and Fracture Research of Mate-

rials, eds. F. Appel and U. Messerschmidt, Akademie-Verlag, Berlin (1989), p. 23. 192 L. P. Kubin, G. Canova, M. Condat, B. Devincre, V. Pontikis, and Y. Brechet, Diff. and Def. Data B 23–24, 455 (1992). 193 B. Devincre and L. P. Kubin, Mod. Sim. Mat. Sci. and Eng. 2, 559 (1994). 194 H. M. Zbib, M. Rhee, and J. P. Hirth, Int. J. Mech. Sci. 40, 113 (1998). 195 D. Weygand, L. H. Friedman, E. Van der Giessen, and A. Needleman, Mod. Sim. Mat. Sci. and Eng. 10, 437 (2002). 196 L. P. Kubin and B. Devincre, in Deformation-Induced Microstructures: Analysis and Relation to Properties. Proceedings of 20th International Symposium on Materials Science, 6–10 Sept. 1999, Riso Nat. Lab, Roskilde, Denmark (1999), p. 61. 197 R. Madec, B. Devincre, and L. P. Kubin, Scripta mater. 47, 689 (2002).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 265

when dislocations in the surrounding region are closely spaced must be taken into account (e.g., distributing sources randomly will not be sufficient). More recently, 2D simulations have been revised198–201 with the idea of incorporating information from the 3D simulations, to simultaneously benefit from the much greater speed of the 2D calculations and the possibility of rigorously treating the mechanical boundary conditions, together with the necessity of relating the local rules to the local environment. Furthermore, lattice rotations can be naturally included.202 Figure V.9 illustrates an emerging dislocation pattern in Cu

F IG . V.9. (a) Evolution of the bulk dislocation structure in [110] tension of crystal A at a strain of ε = 0.03. (b) The corresponding contours of lattice rotation, θ (in degrees).202 198 H. H. M. Cleveringa, E. Van der Giessen, and A. Needleman, Acta mater. 45, 3163 (1997). 199 A. Needleman, Acta mater. 48, 105 (2000). 200 A. Needleman and E. Van der Giessen, Mat. Sci. and Eng. A 309, 1 (2001). 201 J. Y. Shu, N. A. Fleck, E. Van der Giessen, and A. Needleman, J. Mech. Phys. Solids 49, 1361

(2001). 202 A. A. Benzerga, Y. Brechet, A. Needleman, and E. Van der Giessen, Mod. Sim. Mat. Sci. and Eng.

12, 159 (2004).

266

Y. BRÉCHET AND C. HUTCHINSON

together with the local lattice rotations for a plastic strain of 3%. In this simulation, no artificial cut-off radius was imposed. When the rules for multiplication and annihilation are not defined according to the local environment, dislocation patterning does not emerge.

d. Necessary Ingredients for a Theory of Plastically Induced Pattern Formation The situation concerning our understanding of dislocation patterning during plastic flow can be summarized in the following way. The energetic models and statistic models capture only one part of the problem and both fail to account for the long range interactions between dislocations which is a key ingredient. The local reactions must be explicitly accounted for, including their dependence on the local environment. The ‘reaction diffusion’ approaches oversimplify the dynamics of dislocation glide. In addition, one aspect which is not accounted for is the appearance, together with cell formation, of lattice rotations which may modify the dislocation dynamics on either side of a cell wall. Each of these ingredients are necessary for a future theory for pattern formation. Recent work by Hähner and collaborators203–211 has highlighted a completely new feature that may also need to be considered in the problem of dislocation patterning. Hähner emphasizes the importance of the stochastic aspect in dislocation dynamics. The local fluctuations in the shear rate, γ˙ , and the effective shear stress, τeff , are related to the internal shear stress, τint , and to the strain rate sensitivity, S, in the following way: S = γ˙

∂τa ∂γ˙

(5.5)

Through an equivalent of the fluctuation dissipation theorem: (δτeff )2 = Sτint

and δ γ˙ 2 /γ˙ 2 = τint /S.

(5.6)

203 P. Hähner, Appl. Phys. A 62, 473 (1996). 204 M. Zaiser, Mat. Sci. and Eng. A 309, 304 (2001). 205 S. Bross and P. Hähner, in NATO ASI Series: Thermodynamics, Microstructures and Plasticity, eds. A. Finel, D. Maziere, and M. Veron, Kluwer, Dordrecht (2002), p. 313. 206 P. Hähner, Acta mater. 44, 2345 (1996). 207 M. Zaiser, M. Avlonitis, and E. C. Aifantis, Acta mater. 46, 4143 (1998). 208 M. Zaiser, K. Bay, and P. Hähner, Acta mater. 47, 2463 (1999). 209 M. Zaiser and P. Hähner, Mat. Sci. and Eng. A 270, 299 (1999). 210 P. Hähner and M. Zaiser, Mat. Sci. and Eng. A 272, 443 (1999). 211 P. Hähner, Scripta Materialia 47, 415 (2002).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 267

Zaiser, Bay and Hähner208 then write an evolution equation for the dislocation density which is in fact a stochastic equation incorporating the noise in the local strain rate. The detailed form of the deterministic equation can be discussed, but the key feature is the following: the probability distribution of the dislocation density changes from a peaked distribution for small values of the noise (i.e., small internal stresses compared to the applied stress) to a power law distribution at larger values of the noise. In this approach, the cell size distribution is expected to show a fractal like behavior, and is to be understood as a noise induced phase transition, where the strain-rate sensitivity and the internal stress compared to the applied stress play a crucial role.208,211 In addition to the requirements concerning long range stresses and local reactions, the theory for dislocation cell formation still to be discovered will have to incorporate these stochastic aspects.

e. The Special Case of Patterning in Fatigue Fatigue loading is quite special in plasticity. By a periodic reversal of the applied stress, dislocations are forced to move back and forth, and the resulting microstructure depends on the degree of irreversibility of this motion. As fatigue cycles accumulate, dislocation dipoles are formed, and these entities have elastic fields which are less extended in space. By the very construction of the fatigue dislocations, the long range interaction stresses tend to be naturally screened. The patterns observed in fatigue are very regular, much more so than the patterns obtained in monotonic plasticity. Since the phenomenon of plastic localization in fatigue was discovered,212 the dislocations structures associated with intense localization have been extensively studied,213–219 both by conventional TEM to characterize the structure, and by in-situ deformation, to observe the mode of operation.220 We will summarize only the main features, since they have

212 A. T. Winter, Phil. Mag. 30, 719 (1974). 213 J. G. Antonopoulos, L. M. Brown, and A. T. Winter, Phil. Mag. 34, 549 (1976). 214 U. Essmann and H. Mughrabi, Phil. Mag. A 40, 731 (1979). 215 U. Essmann, U. Gosele, and H. Mughrabi, Phil. Mag. A 44, 405 (1981). 216 F. Ackermann, L. P. Kubin, J. Lepinoux, and H. Mughrabi, Acta metall. 32, 715 (1984). 217 R. Wang, H. Mughrabi, S. McGovern, and M. Rapp, Mat. Sci. and Eng. 65, 219 (1984). 218 J. Lepinoux and L. P. Kubin, Phil. Mag. A 54, 631 (1986). 219 H. Mughrabi, Acta metall. 31, 1367 (1983). 220 J. Lepinoux and L. P. Kubin, Phil. Mag. A 51, 675 (1985).

268

Y. BRÉCHET AND C. HUTCHINSON

been extensively reviewed in Refs. [221–226]. Since the motion of dislocations is responsible for pattern formation, the most informative studies have been performed by applying a constant plastic strain amplitude to single crystals oriented for single slip. Below a threshold amplitude, the dislocation structure is formed of ‘veins’ rich in dislocations separated by ‘channels’ of equivalent volume fraction, poor in dislocations. This is referred to as the ‘matrix structure’, and the plastic deformation at the macroscopic level is homogeneous in space. When a critical threshold amplitude is attained, plastic deformation becomes strongly localized into so-called ‘persistent slip bands’ (PSB) which exhibit a very regular ‘ladder structure’. This strikingly regular structure shown in Figure V.10214 has been thoroughly studied and is one of the nicest and simplest examples of dislocation patterning in plasticity. It is especially simple compared to the cellular patterns discussed in Section V.15.a–c since it is a structure developed while single crystals are fatigued so that a single burgers vector is activated. This dislocation structure appears to be extremely efficient at carrying the important strains in the Persistent Slip Bands (PSB). Furthermore, the situation corresponds to a true steady state: in a test with constant applied plastic strain amplitude, it corresponds to the saturation of the applied stress amplitude, and to a steady state in the dislocation density. This implies that any creation of dislocation length has to be balanced by an equivalent annihilation process. The overall functioning of the structure is now well understood. The rungs in the ladder structure are of edge character, and the dislocations moving in the channels are of screw character (Figure V.10b). The rungs are formed by dislocation dipoles. Under the applied stress, the dipoles act as sources and emit dislocations in the channels. The screw dislocations moving in the channels leave new edge dislocations in the walls. The creation processes just described are counterbalanced by annihilation processes: dipoles in the walls can collapse by climb, annihilating edge dislocations, and two screw dislocations of opposite signs in the channels can annihilate by cross slip. The annihilation by climb in the walls requires the emission of point defects, which is the origin of the ‘swelling’ of the PSB as a whole, creating extrusions and intrusions. The operating stress of the structure is governed by the stress necessary to emit a dislocation from the wall and to propagate it in the channel. 221 L. M. Brown, in Proceedings of an International Conference on the Dislocation Modelling of

Physical Systems, eds. M. Ashby, R. Bullough, C. S. Hartley, and J. P. Hirth, Pergamon, Gainesville, Florida, USA (1980), p. 51. 222 Z. S. Basinski and S. J. Basinski, Prog. Mat. Sci. 36, 89 (1992). 223 T. Magnin, J. Driver, J. Lepinoux, and L. P. Kubin, Rev. de Phys. 19, 467 (1984). 224 T. Magnin, J. Driver, J. Lepinoux, and L. P. Kubin, Rev. de Phys. 19, 483 (1984). 225 L. M. Brown, Mat. Sci. and Eng. A A285, 35 (2000). 226 L. P. Kubin, C. Fressengeas, and G. Ananthakrishna, in Dislocations in Solids, Vol. 11, eds. F. R. N. Nabarro and M. S. Duesbery, Elsevier, Amsterdam (2002), p. 101.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 269

F IG . V.10. (a) Persistent slip bands (PSB) formed in Cu crystal subject to fatigue loading. The PSB and ‘matrix’ structures are clearly labeled.214 (b) Schematic representation of the dislocation arrangement within a PSB.215

270

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.11. Saturation peak resolved shear stresses of Cu crystals fatigued at various constant plastic strain amplitudes and temperatures.227

Therefore the structure operates at a stress amplitude which scales as the inverse spacing of the ladder rungs. In the domain of strain amplitude where the PSBs are observed, the applied saturation stress amplitude is constant and the volume fraction of PSBs is proportional to the strain227 (Figure V.11). This qualitative description of the functioning of the structure has been cast into the format of a ‘chemical kinetics approach’ for the density of dislocations in the walls and in the channels by Differt and Essmann.177,178 Even though the functioning of the structure is well understood, its spontaneous emergence is still not clear. It has been studied in the framework of the ‘reaction diffusion approach’ in a series of papers by Walgraef and Aifantis, which can be seen as the most sophisticated examples of this type of modeling in plasticity.175,228–232 Two dislocation populations, the fast and the slow, 227 Z. S. Basinski, A. S. Korbel, and S. J. Basinski, Acta metall. 28, 191 (1980). 228 D. Walgraef and E. C. Aifantis, Int. J. Eng. Sci. 23, 1351 (1985). 229 D. Walgraef and E. C. Aifantis, Int. J. Eng. Sci. 23, 1359 (1985). 230 D. Walgraef and E. C. Aifantis, Int. J. Eng. Sci. 23, 1365 (1985). 231 D. Walgraef and E. C. Aifantis, Int. J. Eng. Sci. 24, 1789 (1986). 232 E. C. Aifantis, Solid State Phenomena 3–4, 397 (1988).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 271

F IG . V.12. Bifurcation diagram in the WA model.175 A is the amplitude of the modulation of the immobile dislocation density and is the stress at saturation during cycling. The heavy lines indicate the range of stability of each of the three possible solutions, a uniform structure (0), a ‘vein’ structure (1) and a ‘ladder’ structure (2).

with two different ‘effective diffusion coefficients’ evolve in a coupled manner. In fact, the exact form of the reaction terms is more inspired by the so called ‘Brussellator’5,6 than by any precise dislocation mechanism. The control parameter in this model is the applied stress and a sequence of instabilities is predicted via a ‘Turing-type’ scenario: from a homogeneous distribution, to a ‘rod-like’ distribution (identified as the so-called ‘vein structure’) to a ‘ladder-like’ distribution (Figure V.12). Qualitatively, the sequence is indeed the observed one. However one may be surprised that in the set of equations studied by Walgraef and Aifantis, there are no terms specific to fatigue. It would predict the same kind of patterning in monotonic loading in single slip, which is known not to occur. In the current framework, the only difference in fatigue would be the ability to maintain the strain long enough so that saturation can indeed be reached and the control parameter increased sufficiently. However, very large flow stresses can be obtained in monotonic loading, and the PSB structure is never observed. This highlights the limitations of phenomenological approaches such as those developed in the reaction diffusion approach: it is necessary to incorporate some of the microstructural features which are known to be important.

272

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.13. Simulated dipolar pattern viewed in a section perpendicular to the slip plane and parallel to the slip direction.233

One of these features specific to fatigue is the existence of a large density of dipoles. These dipoles are naturally created by the back and forth motion of dislocations during fatigue loading. An attempt to propose a working mechanism to generate dipole clusters, as incipient features of pattern formation, has been proposed by Kratochvil et al.233–237 The basic idea is that a dipole drifts in a stress gradient generated by the moving screw dislocations. This drift tends to accumulate dipolar loops which in turn enhance the bowing of the dislocations and provoke further accumulation. This mechanism has been seen to operate in the 3D dislocation simulations,233 and the simulation of dipole clustering shown in Figure V.13 shows that it may be considered as a possible mechanism for generating structures. However, we are still far from the nice regular structures we have described for the PSB.

233 A. Franek, R. Kalus, and J. Kratochvil, Phil. Mag. A 64, 497 (1991). 234 J. Kratochvil, Rev. de Phys. 23, 419 (1988). 235 J. Kratochvil and M. Saxlova, Scripta metall. mater. 26, 113 (1992). 236 V. Gregor, J. Kratochvil, and M. Saxlova, Mat. Sci. and Eng. A 234, 209 (1997). 237 J. Kratochvil, Mat. Sci. and Eng. A 309, 331 (2001).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 273

VI. Spatio-Temporal Patterning in Plasticity: The Portevin–Le Chatelier Effect

After having examined the spatial organization of dislocations under various loading conditions, we finally consider a case of spatio-temporal instability in mechanical behavior. In this section, we consider patterning at scales which are much larger (∼mm) than typical dislocation spacings. At this scale, plastic deformation is normally homogeneous. Two stabilizing factors ensure this homogeneity: work hardening and a positive strain-rate sensitivity. When a material deforms, it hardens, and therefore a region which is more deformed tends to deform less easily. This is true for low strains (up to 10%) and is referred to as work hardening. When the strain is larger, and therefore when the stress has increased, the reduction in sample area associated with enhanced plastic deformation may overcome the work hardening rate (which decreases as deformation proceeds): this is the origin of the macroscopic instability called ‘Necking’ which ends any tensile test of a ductile material. Similarly, the textural evolutions associated with large strains may lead to a ‘strain softening’ and to the formation of deformation bands where deformation is much higher than in the rest of the sample. These are both instabilities in mechanical behavior. When a material is deformed at a faster rate, the stress necessary is in general higher and this is referred at as ‘positive strain-rate sensitivity’. However, in some alloys, a negative strain-rate sensitivity can be observed, leading at the same time to a serrated stress-strain curve and to the spatial localization of plastic deformation. This phenomenon, called the ‘Portevin–Le Chatelier’ (PLC)238 effect has been interpreted239 as the interplay between the diffusion of impurity solutes toward dislocations, and de-pinning of the dislocations. The underlying physics is relatively clear. For a given applied strain rate, a given dislocation density spends part of the time waiting at obstacles (other dislocations), and part of the time flying towards another obstacle. While arrested at obstacles, dislocations attract mobile impurity solutes. The greater the concentration of impurities segregated to the dislocation core, the higher the stress necessary to unpin it for further flight. Therefore two characteristic times have to be considered: the diffusion time for impurities, and the waiting time for dislocations. When the diffusion time is very large compared to the waiting time, dislocations move with almost no solute interaction, with a high mobility, and a positive strain-rate sensitivity is observed. When the diffusion time is very small compared to the waiting time, dislocations are permanently loaded with solute, they will have a low mobility, but still a positive strain-rate sensitivity. When the two times are of the same order, the longer the waiting time (lower strain rate), 238 H. Le Chatelier, Rev. de Metall. 6, 914 (1909). 239 A. Cottrell, Dislocations and Plastic Flow in Crystals, England, Carendon, Oxford (1953).

274

Y. BRÉCHET AND C. HUTCHINSON

the greater the concentration of impurities that will segregate to the dislocation, and the lower will be its mobility, meaning a higher stress is needed to make it move at a given velocity: this results in a negative strain rate sensitivity. Since the waiting time depends on the dislocation density and the applied strain rate, and the diffusion time depends on both the temperature and dislocation density, this simple analysis allows for a basic understanding of why the PLC effect is observed only in a closed domain of strain-rates and temperatures, and only beyond a critical strain. This approach has been thoroughly explored, using rate equations for dislocation densities (mobile and immobile) and well established segregation kinetics for impurities at dislocations. The questions of conditions for serrated yielding (another name for PLC) in terms of strain rate, temperature and critical strain can be considered to be solved.240,241 Similarly, a formal description of the range of negative strain-rate sensitivity,242 together with spatial dependences in gradients of the stress or the strain rate243,244 have allowed for a continuum description of the propagative plastic waves. The recent advances in the subject are related to the non-periodic serrated flow, and with the associated spatial aspects of strain localization. In this section we will consider only the detailed features of the spatial organization of plasticity and the statistics of the serrated flow. After summarizing the variety of experimentally observed phenomena, we will outline two recent approaches: PLC as an example of self organized criticality (SOC), and PLC as an example of deterministic chaos. 16. P HENOMENOLOGY OF P ORTEVIN –L E C HATELIER E FFECT The PLC effect has two manifestations: a serrated stress-strain curve and a localized deformation pattern. Three types of stress strain curves are commonly distinguished, and they correspond to three different types of spatial organization of plasticity.245–247 Type A serrations are associated with repetitive continuous propagation of deformation bands, nucleated at one end of the sample. Type B serrations correspond to a hopping propagation of localized bands in the axial direction of the sample. Type C serrations correspond to the nucleation of bands in a spatially non-correlated manner. The typical appearances of the various types of serrations are shown in Figure VI.1. 240 L. P. Kubin and Y. Estrin, Acta metall. 33, 397 (1985). 241 L. P. Kubin and Y. Estrin, Acta metall mater. 38, 697 (1990). 242 P. Penning, Acta metall. 20, 1169 (1972). 243 V. Jeanclaude and C. Fressengeas, Comp. Rendue Acad. des Sci. 315, 7 (1992). 244 V. Jeanclaude and C. Fressengeas, Comp. Rendue Acad. des Sci. 316, 867 (1993). 245 K. Chihab, Y. Estrin, L. P. Kubin, and J. Vergnol, Scripta metall. 21, 203 (1987). 246 E. Pink and A. Grinberg, Mat. Sci. and Eng. 51, 1 (1981). 247 L. P. Kubin, K. Chihab, and Y. Estrin, Acta metall. 36, 2707 (1988).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 275

F IG . VI.1. Examples of the different types of serrated yielding seen in an Al-5Mg (wt.%) polycrystal deformed at room temperature with different imposed strain rates, ε˙ .226 Type C serrations: ε˙ = 5 × 10−6 /s. Type B serrations: ε˙ = 5 × 10−4 /s. Type A serrations: ε˙ = 5 × 10−3 /s.

The stress drops during serrated yielding have also been examined and the statistical analysis248 in various situations can also lead to three types of histograms: the peak shaped distribution (type p), the asymmetric distribution (type as) and an intermediate distribution which presents both a peak and an asymmetry (type i) (Figure VI.2).

F IG . VI.2. Examples of ‘stress-drop’ histogram shapes for room temperature deformation:249 (a) polycrystalline specimen, ε˙ = 1.3 × 10−5 /s (type p); (b) single crystal, ε˙ = 1.3 × 10−5 /s (type i); (c) polycrystalline specimen, ε˙ = 6.1 × 10−4 /s (type as). 248 M. A. Lebyodkin, Y. Brechet, Y. Estrin, and L. P. Kubin, Phys. Rev. Letts. 74, 4758 (1995). 249 M. Lebyodkin, L. Dunin-Barkowskii, Y. Brechet, Y. Estrin, and L. P. Kubin, Acta mater. 48, 2529

(2000).

276

Y. BRÉCHET AND C. HUTCHINSON

F IG . VI.3. Classification of the types of serrations and stress drop statistics in an (˙ε, 1/T) map.249 The boundaries between various regions are drawn in a semi-schematic way. The area where the PLC effect occurs is delineated by the horseshoe-shaped curve.

The parameters to be considered in a first approximation as controlling the characteristics of the PLC effect are the strain rate and temperature. It is convenient to map the domain in which serrated yielding occurs in terms of the type of instability and the type of stress-drop distribution. An example for the Al-Mg system is shown in Figure VI.3. In the following sections we will consider two types of models developed to describe this rich phenomenology. The first (Section VI.17) relies on a phenomenological description, and considers as essential ingredients the negative strainrate sensitivity and the spatial coupling between slices of material deforming at different rates. The second model (Section VI) delves deeper into the detailed dynamics of dislocations responsible for the phenomena. 17. S TATISTICAL A NALYSIS OF S ERRATED F LOW: A N E XAMPLE OF S ELF O RGANIZED C RITICALITY (SOC) The existence of a negative strain-rate sensitivity, which is the origin of the PLC instabilities, is reminiscent of the behavior of a dynamic friction coefficient which decreases when the sliding velocity increases. This behavior itself generates a similar type of instability during the sliding of two solids, the ‘stick-slip’

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 277

F IG . VI.4. The distribution density function D(s) for an Al-Mg single crystal deformed at 120 ◦ C and ε˙ = 1.3 × 10−5 /s.249 The dotted line corresponds to the exponent α ≈ 1 in the dependence D(s) ≈ s −α .

instability.250–252 This sliding instability is characterized by a power law distribution for the jump in the force/displacement curve. Similarly, the distribution of stress drops, when the distribution is asymmetrical, also exhibits a power law behavior as shown in Figure VI.4. A simple model for the power law behavior in stick-slip has been proposed in the physics community: a set of blocks coupled by springs, with an appropriate friction law.250–252 By analogy a simple model has been proposed for the PLC effect:252,253 the material is ‘sliced’ into layers which may each deform at different rates. The relation between the local stress and the strain-rate is an N shaped curve which is obtained from the theory of dynamic strain aging (Figure VI.5). The local stress is the applied one corrected for ‘incompatibility stresses’ stemming from the difference in local strains. The equivalent of the position in Langer’s ‘stick-slip’ model is the strain, and the equivalent of the friction law is the N-shaped stress-strain-rate curve. The equation governing the strain in each slice (εi ) can be written: σ = hεi + F (˙εi ) − K (εi−1 − εi ) + (εi+1 − εi ) . (6.1) 250 R. Burrige and L. Knopoff, Bull. Seis. Soc. Amer. 57, 341 (1967). 251 J. M. Carlson and J. S. Langer, Phys. Rev. Letts. 62, 2632 (1989). 252 J. M. Carlson and J. S. Langer, Phys. Rev. A 40, 6470 (1989). 253 M. Lebyodkin, Y. Brechet, Y. Estrin, and L. Kubin, Acta mater. 44, 4531 (1996).

278

Y. BRÉCHET AND C. HUTCHINSON

F IG . VI.5. (a) Schematic illustration of the coupled block model sliding with a strain-rate dependent friction (F (˙ε)) and deformed with a constant total imposed strain rate ε˙ a . (b) The viscoplastic Penning’s function F (˙ε) for an Al-Mg alloy.226 In the intermediate range of strain rates, the portion of the negative slope of F describes the negative strain-rate sensitivity associated with the PLC effect.

F IG . VI.6. Schematic phase diagram of the computer model behavior illustrating the types of plastic localization and stress drop statistics.249 The dashed line separates domains of different spatial nature of strain localizations. ε˙ a1 and ε˙ a2 denote the lower and upper bounds of the applied strain rate interval where the PLC effect occurs.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 279

F IG . VI.7. The normalized distribution D(s) of stress drops for a simulated deformation curve.249 The dotted line corresponds to the exponent α ≈ −1 in the dependence D(s) ≈ s −α .

The first term is the work hardening of the slice, the second describes the strainrate sensitivity, and the third term describes the spatial coupling. This model should be able to describe not only the power law behavior in the stress drops, but also the conditions under which the PLC effect is observed (in terms of applied strain rate and test temperature). It should also predict the type of spatial localization expected. The model is solved numerically, and indeed presents the same variety of behavior as observed experimentally. When the strain-rate is increased, the stress drop distribution changes from bell-shaped to a continuously decreasing one (cf. Figure VI.2). The asymmetric distribution is indeed a power law, and the exponent depends on the coupling constant between the blocks (slices of material). The value of this coupling constant is of the order of the elastic modulus and confirms the interpretation of the coupling as resulting mainly from elastic incompatibilities. The plastic localization which is observed in the numerical simulation also evolves with increasing applied strain-rate, from spatially uncorrelated (Type C) to spatially correlated, hopping or propagating (Type B and A). The band structure predicted in each of the three cases, in relation with the stress strain curve is shown in Figure VI.8. The velocity of the propagating band has also been computed with this simple model and it is found to exhibit a non-monotonic behavior. Within this framework, the statistical behavior of the PLC instability, namely the existence of a power law distribution of stress drops can be seen, in certain

280

Y. BRÉCHET AND C. HUTCHINSON

F IG . VI.8. Stress versus time curve and the attendant deformation band patterns for (a) ε˙ a = 10−5 s −1 , (b) ε˙ a = 5 · 10−5 s −1 and (c) ε˙ a = 4 · 10−4 s −1 .253 (Continued on the next page.)

domains, as an example of Self Organized Criticality.22,254–256 However, some other experimental findings suggest another type of analysis. 254 P. Bak, C. Tang, and K. Wiesenfeld, Phys. Rev. Letts. 59, 381 (1987). 255 P. Bak, C. Tang, and K. Wiesenfeld, Phys. Rev. A 38, 364 (1988). 256 P. Bak, How Nature Works: The Science of Self-Organized Criticality, Oxford University Press,

Oxford, England (1997).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 281

F IG . VI.8. (Continued.)

F IG . VI.9. Dependence of the band propagation velocity on the imposed strain rate for three values of the coupling constant for h = 103 MPa. Curve 1: k = M, Curve 2: k = 0.5M and Curve 3: k = 0.27M. A demarcation line between the regions of the true and apparent (relay-race) propagation is shown.253

282

Y. BRÉCHET AND C. HUTCHINSON

18. P ORTEVIN –L E C HATELIER E FFECT: A N E XAMPLE OF D ETERMINISTIC C HAOS The details of the stress strain curve appear to be ‘noisy’ but what is the structure of this noise? As detailed in Ref. [226], this curve is considered as a scalar time series on which the standard techniques of chaos analysis are applied. From a series of N values of stress taken at regular intervals of time t, {σ (kt), k = 1 to N}, one constructs a vector X(k) of M values corresponding to a sampling every Lt, starting from the point σ (kt), X(k) = {σ (k + nL)t, n = 0 to M − 1}. The mapping X(k + 1) = F (X(k)) in the M-dimensional space is known as the ‘reconstructed attractor’. The embedding dimension M is a priori unknown. If M is smaller than the space in which the ‘true attractor’ lives, two points which have different orbits in the ‘true attractor’ will seem to be on the same orbit on the ‘reconstructed one’. This will influence the correlation function, C(r) namely the fraction of vectors X(k) in the M dimensional space which are closer than a distance r. When we have a fractal attractor, C(r) shows a power law behavior C(r) = r ν . The correlation dimension ν depends on the dimension M of the space in which the reconstructed attractor is built. When this space is made larger and larger (M increasing), ν tends towards a limiting value. The value of M above which the correlation dimension ceases to evolve indicates the number of variables necessary to describe the deterministic chaos. This method257 has been applied to experimental data on Portevin–Le Chatelier serrated flow. The dimension of the attractor, as obtained from the correlation function in the phase space, is shown to converge toward a value of 3.2 when the dimension M is increased beyond 5 (Ref. [258], Figure VI.10). This indicates that indeed the behavior of the time series studied is an example of deterministic chaos, and that no more than 5 variables are required to analyze this behavior. Well before this experimental proof of deterministic chaos in PLC (serrated yielding) was given, a model was proposed by Ananthakrishna,259–264 with evolution equations for the densities of mobile dislocations, of immobile dislocations and of dislocations interacting with impurity clouds, to which an equation for the stress was added. These four variables indeed show chaotic behavior. 257 F. Takens, Dynamical Systems and Turbulence, Springer-Verlag (1981). 258 S. J. Noronha, G. Ananthakrishna, L. Quaouire, C. Fressengeas, and L. P. Kubin, Int. J. Bifur.

Chaos 7, 2577 (1997). 259 G. Ananthakrishna and M. C. Valsakumar, J. Physics D 15, 171 (1982). 260 G. Ananthakrishna and M. C. Valsakumar, Phys. Letts. A 95A, 69 (1983). 261 G. Ananthakrishna, Solid State Phenomena 3–4, 357 (1988). 262 G. Ananthakrishna, Solid State Phenomena 23–24, 417 (1992). 263 G. Ananthakrishna, Scripta metall. mater. 29, 1183 (1993). 264 M. S. Bharathi, S. Rajesh, and G. Ananthakrishna, Scripta mater. 48, 1355 (2003).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 283

F IG . VI.10. Log-log plot of the correlation integral C(r) as a function of distance r in the phase space.258 Note the convergence of the slope to 3.2 (dotted line) as the embedding dimension is increased (arrow) from two to five.

A systematic statistical analysis of experimental data has shown that, depending on the loading conditions, the stress drops showed either deterministic chaos, or power law behavior, the transition being the two regimes being characterized by a multi-fractal behavior.265–269 The attractor reconstructed from experimental data on Al-Mg polycrystals, and the prediction of the model proposed by Ananthakrishna, shown in Figure VI.11 shows striking similarities, indicating that the non-linearities in this set of equations are relevant to capture the physics of the problem.270 265 G. Ananthakrishna, C. Fressengeas, M. Grosbras, J. Vergnol, C. Engelke, J. Plessing, H. Neuhauser, E. Bouchaud, J. Planes, and L. P. Kubin, Scripta metall. mater. 32, 1731 (1995). 266 G. Ananthakrishna, S. J. Noronha, C. Fressengeas, and L. P. Kubin, Phys. Rev. E 60, 5455 (1999). 267 G. Ananthakrishna, S. J. Noronha, C. Fressengeas, and L. P. Kubin, Mat. Sci. and Eng. A 309, 316 (2001). 268 M. Lebyodkin, C. Fressengeas, G. Ananthakrishna, and L. P. Kubin, Mat. Sci. and Eng. A 319, 170 (2001). 269 M. S. Bharathi, M. Lebyodkin, G. Ananthakrishna, C. Fressengeas, and L. P. Kubin, Phys. Rev. Letts. 8716, (2001). 270 S. Kok, M. S. Bharathi, A. J. Beaudoin, C. Fressengeas, G. Ananthakrishna, L. P. Kubin, and M. Lebyodkin, Acta mater. 51, 3651 (2003).

284

Y. BRÉCHET AND C. HUTCHINSON

F IG . VI.11. Type B bands. Strange attractor from experiment (a) and from model (b) in a 3D space.270 Note the striking similarity.

The spatial features of the chaotic regime need further investigation to be fully understood, as well as the mechanisms for the cross over between chaos and SOC with increasing strain rate.270–272

271 G. Ananthakrishna, M. S. Bharathi, et al., Phys. Rev. E, in press (2004). 272 P. Hähner, A. Ziegenbein, E. Rizzi, and H. Neuhauser, Phys. Rev. B 65 (2002).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 285

VII. Concluding Remarks

As we bring this chapter to a close, we wish to stress some features of the patterning problems we have examined which would certainly benefit from the input of the physics community. However, before these ‘open problems’ are outlined, we want to insist on the necessity to incorporate in any modelling those specific features which are experimentally well established. Non-linear physics has justly shown that some universal behavior can be derived without knowledge of the precise details of the equations involved and of the microscopic mechanisms. Bifurcation theory, in both its linearized and non-linear (amplitude equations) versions and Chaos theory have shown that it is possible to generate a large variety of behavior with a limited number of ingredients. Similarly, Self Organized Criticality has been claimed to provide a very general framework. However, as outlined in the previous examples, some specific features of the problems have to be incorporated: the N shape of the stress/strain rate curve in Portevin–Le Chatelier modelling brings some new features to the richness of the observed behavior and the fact that the lamellar structure in discontinuous precipitation involves two different driving forces depending on the nature of the interface has important consequences on the removal of the velocity/spacing degeneracy. The analogies between problems (PLC and solid friction, discontinuous precipitation and eutectic solidification, dislocation self-screening and ion screening in a 2D coulomb gas) have both their strengths and weaknesses. Part of the challenge in applying the methods of non-linear physics is to identify the necessary ingredients provided by a detailed knowledge of the underlying mechanisms, without being overflowed by too many details. In the problems of patterning of lamellar structures in the solid state, a key issue is to identify precisely the differences (and implication) between the solid state structures and those resulting from solidification. One of the aspects certainly lies in the difference between solids and liquids, both in their ability to sustain shear, and in the requirements imposed by crystallography. Misfit stresses may modify the driving forces, but may also drive the details of the geometry of the pattern. The crystallography of the interface determines both its energy and its mobility. In a crystalline solid, depending on the driving force, an interface can move either by lateral propagation of steps, or by normal growth. This behavior is probably associated with the ‘stop and go’ motion which has been described in Section III.7.a, but the macroscopic consequences on the patterning are still to be explored. Another feature is of course the fact that, not a single wavelength but a range of wavelengths is experimentally observed. The limited data available in the literature indicates a scaling behavior for the population of spacings observed. These results are still waiting to be modelled. Another feature, also related to the spacing selection problem, is the transition between the patterns which are nucleated and those which are growing, or the adjustment mechanisms when a change

286

Y. BRÉCHET AND C. HUTCHINSON

in the transformation conditions requires a modification of the interlamellar spacing (pattern repeat distance). Are the mechanisms operating in eutectic spacing selection still valid in systems where the anisotropy of the interface properties would make difficult any ‘tilt wave’? On the whole, patterning in phase transformations in the solid state is nevertheless on relatively solid grounds, in the sense that the relevant equations are available, and agreed upon by the community. Comparatively less advanced is the spatial patterning of structural defects. In spite of decades of experimental work and many attempts to developed models for these problems, the state of ‘irradiation patterning of dislocations’ outlined in Section V.14, where there is a relative consensus on the equations to be solved, is far from general. The role of long range stresses seems to be central to many of these ‘structural patterning’ problems. It seems crucial to explain how random nucleation of voids can lead, above a critical density, to a well organized lattice. The case of dislocation patterning in plasticity is far from being solved. The ‘reaction diffusion’ approaches have shown their limitations, due to the difficulty in mimicking a glide process by a diffusion-like description. The energetic approaches, as long as they ignore the fact that the system is maintained far from equilibrium, are unlikely to provide further contributions. Both the short range interactions and the long range interactions must be accounted for. A key issue seems to be the self-screening of dislocations. Like in ionic solutions, one could envisage a population of dislocations as a set of positive and negative entities, in principle able to screen each others field. Due to the specific forces between dislocations, it would be a sort of ‘Coulomb Gas’ with logarithmic interaction energies. But unlike ionic solution, this screening cannot be obtained from standard statistical physics: the motion of dislocations is mainly restricted to glide in certain directions, their number is not conserved since they can annihilate by pairs, and since they are generated, not spontaneously, but by source mechanisms. A proper theory of screening under such restrictions is still to be developed. Another issue put forward recently, which brings a new light to these problems, is a systematic method to account for fluctuations in plasticity. Already these approaches have led to interesting results (e.g., Refs. [133,206]). The incorporation of these ingredients together with the local events which control both the pinning and the annihilation and multiplication of dislocations is a promising route. It is likely that the intensive computer simulations developed in the last decade for dislocation dynamics will have to incorporate these stochastic features to overcome their current limitations. In the cases we have reported, spatio-temporal patterning in plasticity known as the Portevin–Le Chatelier phenomena is specially encouraging and interesting. The set of equations at the level of dislocation dynamics can be seen as sufficiently consensual to provide a realistic description of macroscopic data such as the critical strain to observe the phenomenon of serrated flow. A continuum description of band propagation has been proposed, so the ‘simplified regular PLC

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 287

effect’ can be said to be reasonably well understood. When one delves deeper into the details of the statistics of stress jumps, two regimes have been identified, corresponding respectively to a type of ‘Self Organized Criticality’ with well defined scaling laws, and to a regime of deterministic chaos, corresponding to a correctly reproduced ‘strange attractor’. However, the transition from a regime in which an infinite number of variables is required to describe the statistics, to a regime where a finite and small number of variables is sufficient, is still not understood. The phenomenon being well studied experimentally and the models to describe it at a microscopic level being reasonably safe, it could be very promising to use this problem as a prototype for understanding the transition from deterministic chaos to SOC. In any case, the variety of the patterning phenomena observable in the solid state, and associated with structural defects is certainly a driving force for new modelling approaches which could be both respectful of the underlying mechanisms but not obsessed by them.

This page intentionally left blank

Author Index

Numbers in parentheses are reference numbers and indicate that an author’s name is not cited in the text.

Asamitsu, A., 114(266) Asamitsu, Z., 108(255) Ashby, M. F., 261(174) Aso, N., 49(136, 137), 60(169, 170) Assmus, W., 46(126) Asundi, M. K., 193(28) Avella, A., 6(23) Avlonitis, M., 266(207)

A Aaronson, H. I., 196(42), 198(53) Aarts, J., 2(2) Abdou, S., 219(88) Abrahams, E., 13(46), 73(195), 160(374) Abrikosov, A. A., 9(28) Acker, F., 34(106) Ackermann, F., 267(216) Adams, G., 67(184) Adelmann, P., 12(35), 174(410) Adrian, H., 60(168) Adroja, D. T., 119(274) Aeppli, G., 62(177), 91(218), 119(274) Aifantis, E. C., 261(175), 266(207), 270, 271 Albessard, A. K., 17(64), 20(72, 73) Alexander, M., 174(410) Allen, J. W., 17(66, 67), 50(138) Amici, A., 61(174) Amir, Q. M., 212 Amodeo, R. J., 263(188, 189) Ananthakrishna, G., 268(226), 282, 283, 284(271) Anderson, M. P., 235(118–120) Anderson, P. W., 59(160), 108(257), 125(286) Andersson, P. H., 50(141) Andres, K., 2 Anisimov, V. I., 48(132), 125(290), 131(303) Antonopoulos, J. G., 267(213) Antonov, V. N., 13(45), 97(239), 125(290) Aoki, H., 17(64), 20(72, 73), 74(197), 79(202), 85(210, 211), 86(213), 87(215), 90(217) Appel, J., 59(152) Argon, A. S., 261(174) Arko, A. J., 50(141) Armstrong, P. E., 17(66, 67)

B Baas, J., 94(232) Bak, P., 280(254–256) Balatsky, A. V., 59(163) Balents, L., 146(327, 330) Balluffi, R. W., 234(110) Barbu, A., 249(140, 141) Bareiter, S., 135(311) Barker, I., 256(163) Basinski, S. J., 268(222), 270(227) Basinski, Z. S., 268(222), 270(227) Baumann, S. F., 196(41) Bay, B., 255(160) Bay, K., 258(165), 266(208), 267 Beaudoin, A. J., 283(270) Beck, H., 91(219) Bedell, K. S., 160(375) Bednorz, J. G., 2(5) Bellon, P., 184(10, 11) Beni, G., 92(222) Benner, H., 87(215) Benoist, P., 255(159) Benzerga, A. A., 265(202) Berge, P., 182(2) Berk, N. F., 33(97) Bernardini, J., 193(34) Bernert, A., 98(241), 99(242, 244) Bernhoeft, N., 49(136), 60(170), 62(178), 66 Bernhoeft, N. R., 34(108) 289

290

AUTHOR INDEX

Bertrand, G., 183(9) Bethe, H., 8, 85 Betouras, J., 140(319) Bharathi, M. S., 282(264), 283(269, 270), 284(271) Billinge, S. J. L., 109(258) Binder, K., 185(14) Biroli, G., 159(368) Blaha, P., 127(295) Bley, F., 243(138) Bogdanov, P. V., 154(357) Bogel, A., 198(65), 219, 220 Bolze, G., 198(62) Bonitz, M., 67(185) Bonner, J. C., 91(219), 93, 130(302) Bonsall, L., 70(189) Borsa, F., 126(291) Bouchaud, E., 283(265) Boucher, J. P., 103(247) Bougourzi, A. H., 79(204) Bozorth, R. M., 34(107) Brandt, W. H., 198(45), 203 Brechet, Y., 184(12), 212(82), 215(85), 232(105–107), 235(124, 125), 239(129, 130), 242(133), 243(135–138), 249(142), 264(192), 265(202), 275(248, 249), 277(253) Brechet, Y. J. M., 186(18), 198(66) Bredl, C. D., 2(2) Brener, E. A., 182(4) Brimhall, J. L., 249(144) Brodsky, M. B., 34(105) Broholm, C., 91(218) Bross, S., 266(205) Brown, D., 209(79) Brown, J. D., 95(234) Brown, L. M., 267(213), 268(221, 225) Brugger, T., 12(35) Bruls, G., 24(84) Bucher, E., 59(156, 157) Budnick, J. I., 34(104) Bullough, R., 249(152), 253 Bulut, N., 159(370) Bünemann, J., 164(395) Burke, J. E., 235(113) Burrige, R., 277(250) Butler, E. P., 196(38) Butterfield, M. T., 50(141)

C Cahn, J. W., 198, 203–206, 210, 212, 213, 215, 218, 220, 222, 230, 231, 235(116) Caliebe, W., 113(265) Callen, E., 125(288) Canals, B., 131(305) Canfield, P. C., 17(66) Canova, G., 263(185), 264(190–192) Carbotte, J. P., 155(365) Carlson, J. M., 277(251, 252) Carpy, A., 92(227) Cavadini, N., 38(115) Ceperley, D. M., 71(191), 73(193) Chaboussant, G., 119(274) Chaffron, L., 184(11) Chandrasekhar, S., 182(1) Chatterji, T., 94(229), 99(244), 103(247), 109(259), 113(265), 119(272, 273, 275, 276), 120(278) Chaudhari, P., 161(376) Cheetham, D., 193(29, 31), 207 Cheynet, M. C., 212(82) Chi, E. O., 113(264) Chihab, K., 274(245, 247) Choi, H. S., 113(264) Choi, S., 225(92, 94) Christensen, N. E., 20(71), 172(405) Chubukov, A. V., 163(381) Chuk, T., 154(358) Cichorek, T., 22(79), 39(119), 74(197), 86(213) Claessen, R., 164(395) Cleveringa, H. H. M., 265(198) Cliff, G., 225(93) Cline, H. E., 229(102) Coldea, R., 38(117) Coleman, P., 39(120) Collins, R. T., 161(376) Colten, R. A., 209(77) Condat, M., 264(192) Continentino, M. A., 32(94), 45(125) Cooper, B. R., 59, 62(175), 66, 70 Cottrell, A., 273(239) Courtney, T. H., 227(99) Cox, D. L., 15(52) Craco, L., 48(135), 131(304) Cross, J. O., 138(315) Cross, M. C., 92(224), 102

AUTHOR INDEX Cullen, J. R., 125(288) Custers, J., 39(120), 74(197), 86(213) Czjzek, G., 12(35) Czycholl, G., 162(378) D Dagotto, E., 122(281) Daliachaouch, Y., 17(66) d’Ambrumenil, N., 75(198), 85(212) Darken, L. S., 193(26) Das, A., 193(32, 33) de Boer, P. K., 110(260) de Groot, R. A., 110(260) de Visser, A., 24(84), 47(130) deBoer, J. L., 94(232) DeGroot, S. R., 188(24) Delin, A., 50(141) Dender, D. C., 91(218) Denlinger, J. D., 17(66, 67), 21 des Cloizeaux, J., 79 Devereaux, T. P., 154(358) Devincre, B., 264(192, 193, 196, 197) Dhalenne, G., 113(265), 119(272, 273, 275), 120(278) Dho, J., 113(264) Differt, K., 261(177, 178), 270 Dischner, M., 97(240), 105(252) Dmitriev, D. V., 91(221) Doherty, R. D., 240(131) Doniach, S., 14(49), 33(98), 39, 40(121) Donnevert, L., 23(82) Dönni, A., 60(172) Dooryhee, E., 138(315) Driver, J., 268(223, 224) Dubuisson, P., 249(142) Ducastelle, F., 164(382, 383) Duly, D., 212, 215, 220 Dunin-Barkowskii, L., 275(249) Durakiewicz, T., 50(141) Dzyaloshinski, I. E., 9(28) E Eberhardt, W., 147(332) Ebihara, T., 20(72) Eder, R., 159(372) Edington, J. W., 205(69)

291

Edwards, D. M., 164(390, 391) Efremov, D. V., 57(147) Ehm, D., 16(55), 164(395) Ehrenreich, H., 153(340, 343) Ehrhart, P., 249(143, 151) ElBoragy, M., 219(88) Elgazzar, S., 51(142) Elliott, R. J., 153(342) Eloirdi, R., 171(403) Endoh, Y., 60(169, 170, 172), 113(263), 117(271), 121(279) Engelke, C., 283(265) Engelsberg, S., 33(98) Enz, C. P., 33(99) Eriksson, O., 50(141) Erkelens, W. A. C., 20(70) Eschrig, H., 13(45), 97(239) Eschrig, M., 155(362, 364) Essmann, U., 261(177, 178), 267(214, 215), 270 Estrin, Y., 261(181), 263(185), 274(240, 241, 245, 247), 275(248, 249), 277(253) Evans, J. H., 249(145–147, 149) Eyert, V., 127(296) Eyre, B. L., 249(148, 152) F Fagot-Revurat, Y., 95(236) Fak, B., 90(217) Falakshahi, H., 71(192) Falicov, L. M., 164(393) Farrell, K., 249(150) Faulhaber, E., 22(79) Fauth, F., 84(209), 138(315) Fay, D., 59(152) Fedorov, A. V., 155(363) Feild, C., 161(376) Fertig, W. A., 59(157) Filinov, A. V., 67(185) Fink, J., 174(410) Firsov, Y. A., 115 Fischer, M., 96(237) Fischer, Ø., 61(173) Fischer, P., 60(171) Fisher, D. S., 92(224) Fisher, M. E., 93, 102, 130(302) Fisher, M. P. A., 146(327, 330) Fisher, R. M., 193(26)

292

AUTHOR INDEX

Fisk, Z., 2(3, 4), 17(66, 67), 34(106) Flandin, L., 243(135) Fleck, N. A., 265(201) Flouquet, J., 20(70), 47(130) Fournelle, R. A., 227, 231 Fradkin, E., 140(320) Franek, A., 272(233) Franz, W., 2(2) Fratzl, P., 185(14, 15) Freeman, A. J., 34(105) Freericks, J., 154(352) Fressengeas, C., 268(226), 274(243, 244), 282(258), 283(265–270) Freye, D. M., 39(118) Fridberg, J., 222(89, 90) Friedel, J., 6, 81 Friedman, L. H., 264(195) Fröhlich, H., 59 Frye, J. H., 209(78) Fuchizaki, K., 235(121), 237 Fuji, Y., 94(233), 103(248, 249) Fujimori, A., 6(22), 108(254), 127(294), 135(312) Fujimori, S., 50(139), 171 Fujimoto, S., 132(309) Fujioka, H., 117(271), 121(279) Fujiwara, K., 127(297, 298) Fukuyama, H., 70(188) Fulde, P., 5(14), 9(29), 11(31, 33), 12(36), 13(41, 42, 45), 17(62), 27(88, 89), 35(109), 46(127, 128), 49(137), 53(144), 57(147), 59(153–155, 157), 61(174), 63(180), 74(196), 75(198), 81(205), 85(212), 87(216), 97(239), 99(242–244), 129(299), 136(313), 137(314), 140(318, 319), 145(323), 146(324), 154(346, 353–356), 164(396, 397), 165(401), 174(407, 408) Furrer, A., 38(115) Furukawa, N., 119(277), 139(316) G Gajewski, D. A., 126(291) Galy, J., 92(227) Garst, M., 46(129) Gaskell, T., 149 Gebhard, F., 164(395)

Geerk, J., 61 Gegenwart, P., 23(82, 83), 39(119, 120), 74(197), 86(213), 90(217) Geibel, C., 16(55), 22(79), 23(82, 83), 39(119, 120), 49(137), 60(171), 94(230), 95(235), 96(237), 97(238, 240), 105(252) Georges, A., 69(186) Gerhardt, W., 34(103) Ghoniem, N. M., 253, 263(188, 189) Girvin, S. M., 146(327) Gogolin, A. O., 12(37) Goldman, A. I., 126(291) Goremychkin, E. A., 22(77) Gorkov, L. P., 9(28) Gosele, U., 267(215) Goto, T., 76(199), 78(201) Gottstein, G., 235(117) Gottwick, U., 20(69) Gouder, T., 171(403) Graebner, J. E., 2 Graf, J., 162(380) Grauel, A., 60(171) Greer, A. L., 232(108, 109) Gregor, V., 272(236) Grenier, B., 103(247) Grest, G. S., 235(118, 119) Grewe, N., 20(69) Grin, Y., 94(229), 129(299) Grinberg, A., 274(246) Gröber, C., 159(372) Groma, I., 243(135) Gros, C., 97(238), 105(250) Grosbras, M., 283(265) Grosche, F. M., 39(118) Grüner, G., 69(187) Gu, G., 154(357) Gu, G. D., 155(363) Gu, Q., 40(122) Gu, T., 126(291) Güdel, H. U., 38(115) Güntherod, G., 96(237) Gupta, S. P., 212 Gust, W., 193(32–35), 196(36), 198(65), 202(68), 205(70–72), 211(80), 215, 219, 220, 235(125) Gutzwiller, M. C., 6, 164 Guyot, P., 243(135–137) Gweon, G. -H., 17(66, 67), 162(380)

AUTHOR INDEX H Haase, R., 188(25) Haayman, P. W., 3(8), 124 Habicht, K., 38(115) Hackenberg, R. E., 197(44), 211(81) Haen, P., 47(130) Haga, Y., 49(136), 52(143), 65(181), 66(183), 77(200) Hagel, W. C., 206(75), 222 Hähner, P., 258(165), 266, 267, 284(272) Haken, H., 183(8) Haldane, F. D. M., 129 Halperin, B. I., 71(190) Hammar, P. H., 91(218) Hanke, W., 159(371, 372) Hansen, N., 255(160), 256(163), 260(170) Haque, M., 73(194) Harasawa, A., 164(395) Harima, H., 127(297) Harrison, N., 86(213) Hase, M., 92(225) Hasegawa, H., 108(257) Hasegawa, T., 260(172) Hasselmann, N., 57(147) Hauptmann, R., 95(235), 96(237) Hayden, S. M., 34(108) Heeger, A. J., 12(38) Heiniger, F., 59(156) Heitler, W., 3 Held, K., 17(59) Helfrich, R., 23(82), 85(211), 87(215) Hermele, M., 146(330) Hertz, J. A., 34, 164(390, 391) Herzig, C., 193(34) Hettler, M. H., 159(367, 369) Hewson, A. C., 15(50) Hidaka, H., 127(297) Hiess, A., 49(136), 60(170), 103(247), 119(275) Hillert, M., 198, 202, 203, 205–207, 209, 210, 212, 215, 218, 222, 225, 235(115), 236, 237 Hinkel, C., 135(311) Hinma, T., 52(143) Hino, O., 115(268) Hinze, P., 23(83) Hirai, K., 164(397) Hirooka, S., 154(347)

293

Hirota, K., 113(263), 117(271), 121(279) Hirsch, J. E., 59(158) Hirst, L. L., 59(153) Hirth, J. P., 264(194) Hisazaki, Y., 77(200) Hoang, A. T., 110(261) Höck, K. -H., 127(296) Hoffmann, J. U., 120(278) Hohlwein, D., 120(278) Holt, D. L., 256(162), 260 Holtzberg, F., 161(376) Honig, J. M., 135(311) Horibe, Y., 139(316) Horn, R., 23(82) Horn, S., 127(296) Hornbogen, E., 198(56) Horsch, P., 93(228) Howe, L., 249(141) Huang, C. Y., 34(106) Hubbard, J., 2, 6–8, 14, 27, 32, 68, 69, 74, 85, 86, 97, 98, 100, 105, 108, 110, 111, 125, 130, 132, 144, 148, 151–155, 157–161, 163–165, 167, 169, 172, 174–177, 179 Huber, F., 171(403) Hückel, E., 3 Hüfner, S., 16(55), 147(331) Hughes, D. A., 240(131), 255(160) Hull, F. C., 209(77), 234(112) Humphreys, F. J., 186(21), 235(122, 123), 240(131), 242(132) Hunderi, O., 236, 239 Hunt, J. D., 198(51) Hur, K. L., 131(303) Hur, N. H., 113(264) Hüser, D., 34(103) Hutchinson, C. R., 211(81) Huth, M., 60(168) Hybertsen, M. S., 172(405) I Igarashi, J., 164(387, 388, 396, 397) Ihle, D., 125(289) Ikeda, H., 154(357) Ikeda, N., 139(316) Illy, J., 262(183) Imada, M., 6(22) Inada, Y., 52(143)

294

AUTHOR INDEX

Ishibashi, H., 139(316) Ishida, K., 66(183) Ishihara, S., 117(271), 154(359, 361) Ishikawa, M., 61(173) Isobe, M., 92(226), 94(233), 103(248, 249), 105(251) Isoda, M., 124(285) Iwasa, K., 11(32), 77(200), 79(202), 90(217) Izawa, K., 66(182) J Jackeli, G., 109(259), 121(280) Jackson, K. A., 198(51) Jaclic, G., 42(123) Jager, W., 249(143, 151) Jaime, M., 86(213) Janecek, M., 243(136, 138) Jarrell, M., 154(352), 159(367, 369), 160(373) Jayprakash, C., 16(56, 57) Jeanclaude, V., 274(243, 244) Jedrak, J., 56(145) Jeevan, H., 22(79) Jegoudez, J., 103(247) Jensen, D. J., 240(131) Jensen, H. J., 187(22) Jensen, J., 35(110, 111), 62(176) Jepsen, O., 94(229) Jobst, A., 94(230) Johnson, J. D., 87(214) Johnson, P. D., 155(363) Johnston, D. C., 123(282), 124(283, 284), 126(291) Jonas, J. J., 240(131) Jones, B., 16(58) Jourdan, M., 60(168) Joyce, J. J., 50(141) Julian, S. R., 17(65), 20(74), 39(118) K Kadowaki, K., 76, 126 Kagami, C., 103(248) Kaganov, M. I., 23(81) Kaiser, A. B., 46(128) Kajihara, M., 225(92, 94) Kakehashi, Y., 154(344–346, 348, 349, 353, 355, 356), 165(401), 179

Kakizaki, A., 164(395) Kakol, Z., 135(311) Kakurai, K., 60(172), 103(248) Kalmeyer, V., 146 Kalus, R., 272(233) Kampe, J. C. M., 227(99) Kampf, A. P., 152(336, 337) Kampmann, R., 185(13) Kanamori, J., 6, 164 Kanao, R., 115(268) Karbach, M., 79(204) Kasahara, Y., 65(181) Kassner, M. E., 240(131) Kastrinakis, G., 162(379) Kasuya, T., 13(43), 17(60), 180 Kato, K., 139(316) Katsnelson, M. I., 164(394) Katsufuji, T., 133(310), 139(316) Kaur, I., 193(35), 211 Kawabata, A., 14(48), 34(100) Kawakami, K., 135(312) Kawakami, N., 48(133) Kawasaki, K., 235(121) Kawatra, M. P., 34(104) Keh, A. S., 255(161) Keller, J., 9(29), 59(154, 155, 157) Keller, S. A., 154(357) Kendziora, C., 155(363) Khachaturian, A. G., 185(17) Khomskii, D. I., 100(245) Kikuchi, M., 225 Kim, W. S., 113(264) Kimura, N., 66(183) Kimura, T., 113(262, 263), 119(274) King, C. A., 20(75) King, W. E., 240(131) Kirkaldy, J. S., 198(55, 61, 62), 206(74), 208, 215 Kirkpatrick, S., 153(340) Kishio, K., 154(357) Kita, H., 60(172) Kitaoka, Y., 15(51), 66(183) Kleinmann, L., 165(398) Klinger, L., 198(66), 215(85), 216, 218, 220, 232 Kmety, C. R., 109(258) Knaupp, M., 94(229) Knigavko, A., 154(360) Knoester, J., 100(245)

AUTHOR INDEX Knopoff, L., 277(250) Kobayashi, T., 127(298) Kobayashi, T. C., 127(297) Kocks, U. F., 260(172), 261 Koepernik, K., 51(142) Koga, A., 48(133) Kohgi, M., 11(32), 74(197), 77(200), 79(202), 80, 90(217) Koike, Y., 49(136) Koitzsch, A., 21(76) Kok, S., 283(270) Komatsubara, T., 49(136, 137), 60(169, 170, 172) Kondakov, D. E., 48(132) Kondo, S., 11, 14–17, 21, 32, 38–43, 45, 46, 74, 76, 79, 117, 120, 123(282), 126(291, 293), 132, 179 Kondoh, Y., 225(92) Konno, R., 28(91) Köppen, M., 87(215), 95(235) Korbel, A. S., 270(227) Korotin, M. A., 125(290), 131(303) Koshizuka, N., 155(363) Koslowski, A., 135(311) Kotegawa, H., 127(297) Kotliar, G., 69(186), 159(368), 164(394) Kovacs, I., 262(183) Kovrizhin, D., 38(117) Koyama, I., 113(263) Krämer, K., 38(115) Krane, H. G., 94(230) Kratochvil, J., 272 Krauth, W., 69(186) Kremer, R. K., 94(229), 95(236), 97(240) Krimmel, A., 60(171) Krishan, K., 249(152), 253(153) Krishna-murthy, H. -R., 16(56, 57) Krishnamurthy, H. R., 159(367) Krivnov, V. Y., 91(221) Kroha, J., 16(55) Krumhansl, J. A., 153(342) Kubin, L., 277(253) Kubin, L. P., 258, 261(176, 181, 182), 263(185, 186), 264(190–193, 196, 197), 267(216, 218, 220), 268(223, 224, 226), 274(240, 241, 245, 247), 275(248, 249), 282(258), 283(265–270) Kubota, M., 117(271), 121(279) Küchler, R., 39(119)

295

Kudasov, Y., 81(205) Kuhlmann-Wilsdorf, D., 255(160), 260(168–171) Kulcinski, G. L., 249(144) Kumai, R., 113(262) Kuramoto, Y., 15(51) Kurushima, K., 139(316) Kurz, W., 182(4) Kusaba, T., 235(121) Kusunose, H., 132(307) Kuwahara, H., 114(266) L Laad, M. S., 48(135), 131(304) Labbé, J., 81(208) Lacerda, A., 47(130) Lacroix, C., 11(34), 131(305), 132(306) Landau, L. D., 7, 9–11, 13, 18, 32, 45, 47, 76, 87, 148 Lander, G. H., 49(136), 60(169, 170) Lang, I. G., 115 Lang, M., 23(82, 83), 74(197), 86(213), 87(215), 90(217), 95(235) Langari, A., 101(246) Langer, J. S., 182, 277 Langhammer, C., 23(82, 83), 74(197) Lanzara, A., 154(357, 359), 162(380) Larche, F., 185(16) Laughlin, R. B., 13(40), 146 Lauzeral, J., 253(158) Le Chatelier, H., 184, 187, 273, 274, 282, 286 Leath, P. L., 153(342) Lebowitz, J., 185(15) Lebyodkin, M., 275(249), 277(253), 283(268–270) Lebyodkin, M. A., 275(248) Lee, B. -W., 17(66) Lee, D. -H., 162(380) Lejay, P., 20(70), 47(130) Lemarchand, H., 182(7) Lemmens, P., 96(237) Lendvai, J., 243(135) Leonov, I., 125(290), 136(313) Lepinoux, J., 235(124, 125), 239(129, 130), 242(133), 261(176), 263(186, 187), 267(216, 218, 220), 268(223, 224) Levin, M., 140(321)

296

AUTHOR INDEX

Lhuillier, C., 146(329) Li, J. Q., 113(262) Li, Q., 155(363) Li, Y. M., 75(198), 85(212) Lichtenstein, A. I., 164(394) Lieb, E., 36(112), 85 Liebsch, A., 48(134), 164(385, 386) Liecke, W., 2(2) Lifshits, I. M., 23(81) Link, A., 23(82) Littlewood, P. B., 13(46, 47), 160(374) Liu, Y. C., 198(53) Livet, F., 243(138) Livingston, J. D., 230, 231 Loewenhaupt, R., 22(79) Loh, E., 59(158) Löhneysen, H. v., 34(108) Loidl, A., 60(171), 127(296) London, F., 3 Longinotti, L. D., 59(156) Lonzarich, G. G., 17(63, 65), 20(74, 75), 34(108), 39(118), 59(164–166) Lorenz, B., 125(289) Lorenzo, J. E., 103(247) Lorimer, G. W., 225(93) Louat, N. P., 236, 237 Louchet, F., 184(12) Lozovik, Y. E., 67(185) Lu, D. H., 154(358) Lu, E. D., 154(357) Lüdecke, J., 94(230, 231) Luengo, C. A., 59(157), 124(284) Lühmann, T., 23(83), 38(117) Luther, A., 13(44), 59(153) Lüthi, B., 24(84), 46(126), 78(201), 135(311) Luttinger, J. M., 10, 12, 17, 160 M Machida, A., 133(310) Machida, K., 28(92) Mack, F., 93(228) Mackintosh, A. R., 35(111), 62(176) Madec, R., 264(197) Maekawa, S., 117(271), 174(409) Maezawa, K., 66(183) Magnin, T., 268(223, 224) Mahajan, A. V., 126(291)

Maier, T., 159(369) Maier, T. A., 160(373) Maitra, J. P., 59(156, 157) Maki, K., 65(181) Maletta, H., 60(171) Malygin, G., 261(179, 180) Mancini, F., 6(23) Manna, I., 193(32), 196, 230 Maple, M. B., 17(66, 67), 59(157), 124(284), 126(291) Maradudin, A. A., 70(189) Marchionni, C., 184(12) Marsiglio, F., 154(360) Martin, G., 184(10, 11), 249(140, 141), 255(159) Martin-Delgado, M. A., 101(246) Mason, T. E., 62(177) Massoud, J. P., 249(142) Mathur, N. D., 39(118) Matsuda, Y., 65(181), 66(182) Matsui, Y., 113(262) Matsumoto, H., 164(392) Matsumoto, M., 38(116) Matsuno, J., 127(294), 133(310) Mattheiss, L. F., 127(294) Matthias, B. T., 34(107) Mattis, D., 36(112) Mattis, D. C., 81(207) Mattix, L., 59(157) Maurice, C., 235(123) Maxwell, E., 59(149) Mayer, H. M., 20(69) Mazey, D. J., 249(149) Mazin, I. I., 127(295) Mazur, P., 188(24) McCallum, R. W., 59(157), 124(284) McElroy, D. L., 209(78) McEwen, K. A., 35(110) McGovern, S., 267(217) McHale, P., 63(180) McIntyre, G. J., 113(265), 119(272) McMahan, A. K., 17(59) McMullen, G. J., 17(65), 20(74) McMurry, S., 186(19), 235 McNelley, T. R., 240(131) McQueen, H. J., 240(131) Medrick, K., 165(398) Meetsma, S. A., 94(232) Mehl, R. F., 206(75), 209(77)

AUTHOR INDEX Mehring, M., 95(236) Menovsky, A., 24(84) Meschede, D., 2(2) Metoki, N., 49(136) Metzner, W., 154(350) Meyrick, G., 196(40) Michael, J., 196(41) Mignot, J. -M., 11(32), 79(202), 90(217) Miller, L. L., 123(282), 126(291) Millis, A. J., 48(131) Misguish, G., 146(329) Mishin, Y., 193(34) Mitchell, J. F., 109(258) Mittemeijer, E. J., 193(33) Miyake, K., 59(159), 132(307) Miyake, K. ., 49(137) Miyoshi, K., 127(297, 298) Mizuta, M., 50(139) Moessner, R., 146(326) Monthoux, P., 59(163–166) Moodenbaugh, A. R., 155(363) Moore, D. P., 50(141) Morales, L. A., 50(141) Moreo, A., 122(281) Mori, H., 150(334) Mori, S., 124(285), 133(310), 139(316) Moritomo, Y., 108(255), 113(263), 114(266), 117(271), 121(279), 133(310) Moriya, T., 14, 34, 59(162), 88, 179 Morré, E., 94(230), 105(252) Mostovoy, M. V., 100(245) Motome, Y., 139(316) Motrunich, O. I., 146(328) Mott, N. F., 2, 68, 69, 74, 98, 108, 111 Mughrabi, H., 262(184), 267(214–217, 219) Mukherjee, M., 159(367) Müller, G., 79(204), 91(219) Müller, K. A., 2(5) Müller-Hartmann, E., 48(135), 131(304), 154(351) Muller-Krumbhaar, H., 182(4) Mullins, W. W., 218, 227, 228, 235(114), 236 Murakami, Y., 94(233), 103(249), 113(263) Muraoka, K. Y. J., 103(249) Murata, K. K., 14(49) Murphy, S. M., 253 Mutka, H., 38(115) Mydosh, J. A., 34(103, 104), 39(119)

297 N

Nagaosa, N., 154(358, 359, 361) Nakajima, K., 103(248) Nakajima, N., 77(200) Nakao, H., 94(233), 103(249) Needleman, A., 264(195), 265(198–202) Neef, M., 26(86, 87) Nekrasov, I. A., 48(132) Nelson, D. R., 71(190) Nemoto, Y., 76(199) Nersesyan, A. A., 12(37) Nesbitt, L. B., 59(150) Neuhauser, H., 283(265), 284(272) Neumaier, K., 39(119, 120) Nichols, F. A., 227(97) Nicolay, G., 16(55) Nicolis, G., 182(5) Niksch, M., 46(126) Ninomiya, E., 94(233), 103(249) Nishi, M., 103(248) Nishibori, E., 133(310) Noda, Y., 94(233) Nohara, M., 126(293) Nohdo, S., 115(268) Norman, M. R., 155(362, 364), 163(381) Normand, B., 38(116) Noronha, S. J., 282(258), 283(266, 267) Nücker, N., 174(410) O Ochiai, A., 11(32), 13(43), 74, 76(199), 77(200), 79(202), 84(209), 85(210, 211), 86(213), 90(217), 138(315) Oeschler, N., 39(119) Ohama, T., 94(233) Ohishi, Y., 127(297) Ohm, T., 164(395) Ohoyama, K., 121(279) Ohwada, K., 94(233), 103(249) Okane, T., 50(139) Okazaki, K., 108(254) Okubo, T., 126(293) Okumura, T., 225(92) Ole´s, A., 5(14), 165(399) Olson, C. G., 17(66, 67)

298

AUTHOR INDEX

Onuki, Y., 17(64), 20(72, 73), 52(143), 65(181), 66(183) Opahle, I., 51(142) Oppeneer, P. M., 13(45), 51(142) Osborn, R., 22(77) Osumi, H., 77(200) Ott, H. R., 2 Ouchni, F., 119(276) Ovchinnikov, A., 81(205) Ovchinnikov, A. A., 91(221) Ozaki, M., 28(92) P Pabi, S. K., 193(32), 196(36) Pallson, G., 159(368) Palstra, T. T. M., 94(232) Pande, C. S., 196(42) Pankert, D., 87(215), 95(235) Pankov, S., 73(194) Paschen, S., 74(197) Patterson, B. D., 84(209), 138(315) Patterson, B. R., 234(111) Paul, I., 73(194) Paulus, B., 154(354) Pawlowski, A., 196 Pearson, J. J., 79 Penc, K., 140(318) Penn, D. R., 164(384) Penning, P., 274(242), 278 Penrose, O., 185(15) Pepin, C., 39(120) Perkins, N. B., 121(280) Perlov, A. Y., 13(45) Perovic, A., 197(43) Perring, T. G., 119(274) Peschel, I., 13(44) Petermann, J., 198(56) Petit, L., 50(140) Peuchert, U., 97(238) Pfeuty, P., 36(113) Pfleiderer, C., 34(108) Pharr, G. M., 256(164) Pincus, P., 92(222) Pines, D., 59(163) Pinettes, C., 11(34) Pink, E., 274(246) Plakida, N. M., 59(167) Planes, J., 283(265)

Platzmann, P. M., 70(188) Plessing, J., 283(265) Plummer, E. W., 147(332) Pochet, P., 184(11) Pokor, C., 249(142) Pollmann, F., 56(146), 57(148), 140, 145(323), 146(324) Polyakov, A. M., 140(317) Pomeau, Y., 182(2) Pontikis, V., 264(192) Poppe, U., 20(69) Porter, D. A., 205(69) Pott, R., 46(126) Predel, B., 215(84), 219(88) Prelovsek, N. B., 42(123) Presura, C., 97(240) Preuss, R., 159(371) Prigogine, I., 182(5) Pruschke, T., 131(303), 154(352), 159(369), 160(373) Puls, M. P., 198(61, 62) Pulst, U., 22(78), 23(80) Purdy, G., 232(105–107) Purdy, G. R., 186(18), 196(39), 197(43), 198(66), 215 Pyka, N., 79(202) Pytte, E., 92(223) Q Qin, S., 91(220) Qiu, X., 109(258) Quaouire, L., 282(258) R Radu, T., 38(117) Raj, S. V., 256(164) Rajesh, S., 282(264) Ralph, B., 256(163) Ranzetta, G. V. T., 193(27) Rapp, M., 267(217) Rauchschwalbe, U., 20(69) Raw, G., 188(23) Rayleigh, Lord, 227 Razavi, F., 34(103) Rebizant, J., 171(403) Reese, M., 26(87), 57(148)

AUTHOR INDEX Regnault, L. P., 20(70), 103(247), 119(273, 275) Reich, D. N., 91(218) Reinert, F., 16(55) Revcolevschi, A., 103(247), 113(265), 119(272, 273, 275), 120(278) Reynolds, C. A., 59(150) Rhee, M., 264(194) Rhines, F. N., 234(111) Rice, T. M., 38(116), 48(132, 133), 108, 131(303), 173–176 Ridley, N., 193(29, 31), 207, 209(79) Riseborough, P. S., 127(296) Rizzi, E., 284(272) Robinson, M. T., 249(139) Roessli, B., 49(136), 60(169–171) Roll, U., 215(84) Rollett, A. D., 235(120), 240(131) Romberg, H., 174(410) Ronnpagel, D., 262(184) Rosch, A., 46(129) Rosenberg, M. J., 69(186) Rossat-Mignot, J., 20(70) Roth, G., 12(35), 97(238) Roth, L., 164(389) Ruckenstein, A., 13(46), 160(374) Rudigier, H., 2(3) Ruegg, C., 38(115) Runge, E., 13(42), 20(71), 57(147), 146(324) Ruvalds, J., 162(377) Ryum, N., 236, 239 S Sachdev, S., 32(93) Sahni, P. S., 235(118) Saito, Y., 50(139) Sakai, F., 126(293) Sakai, O., 81(206), 91(220) Sakata, M., 133(310) Sakurai, K., 52(143) Sarrao, J. L., 17(67) Sasagawa, T., 162(380) Sass, S. L., 249(148) Sato, K., 50(139) Sato, N., 23(83), 49(137), 50(139), 60(169, 170, 172) Sato, N. K., 49(136) Satoh, K., 20(72)

299

Savrasov, S., 159(368) Sawa, H., 94(233), 103(249) Sawatzky, G., 166(402) Saxlova, M., 272(235, 236) Scalapino, D. J., 59(158), 159(370) Scalettar, R. T., 17(59) Scattergood, R. O., 260(172) Schachinger, E., 155(365) Schäfer, H., 2(2) Schank, C., 60(171) Schefzyk, R., 46(126) Scheil, E., 198(46), 203 Schilling, J. S., 34(103) Schilling, W., 249(143, 151) Schlesinger, Z., 161(376) Schlüter, M., 172(405) Schmidt, B., 11(31), 42(124), 74(197), 87(215, 216) Schmidt, S., 16(55) Schmidt, W., 119(275) Schmidt-Rink, S., 59(159) Schmitt-Rink, S., 13(46), 160(374) Schneider, R., 120(278) Schreiner, T., 12(35) Schrieffer, J. R., 12(38, 39), 33(97), 152(336) Schultz, T., 36(112) Schulze-Briese, C., 84(209), 138(315) Schwartz, L. M., 153(343) Schwarz, K., 127(295) Schwedler, A. R., 59(157) Schweitzer, H., 162(378) Schwenk, H., 135(311) Seki, M., 50(139) Seki, S., 164(392) Senthil, T., 146(328) Seo, Y., 225(92) Serin, B., 59(150) Shannon, N., 109(259), 119(276), 140(318) Shapiro, J. M., 198(55) Shen, Z. -X., 154(358, 359) Shi, M., 84(209), 138(315) Shiba, H., 81(206), 91(220) Shiflet, G. J., 197(44), 211(81) Shiina, R., 49(137) Shimaoka, Y., 127(298) Shimizu, K., 127(297) Shimizu, M., 154(347) Shimizu, T., 20(72)

300

AUTHOR INDEX

Shingu, M., 139(316) Shiraki, T., 126(293) Shu, J. Y., 265(201) Shvindlerman, L. S., 235(117) Si, Q., 39(119), 46(129) Sigrist, M., 28(90), 38(116), 48(132, 133) Simon, J. P., 243(138) Simoyama, J. -I., 154(357) Singh, D. J., 127(295) Skalski, S., 34(104) Slater, J. C., 6, 72 Smith, J. L., 2(3, 4), 34(106) Smolinsky, H., 97(238) Soderholm, L., 84(209), 138(315) Solorzano, G., 219(88) Solorzano, I. G., 196(39), 215 Somer, M., 94(229) Sommerfeld, A., 8, 76, 81, 87, 126, 130, 132 Sondhi, S. L., 146(326) Soven, P., 153(338) Spalek, J., 59(161) Spanjaard, D., 164(382, 383) Sparn, G., 16(54), 20(69), 23(82, 83), 105(252) Srolovitz, D. J., 235(118–120) Staker, M. R., 256(162) Stansbury, E. E., 209(78) Staub, U., 84(209), 138(315) Steglich, F., 2(2), 16(54), 20(69), 22(79), 23(82, 83), 38(117), 39(119, 120), 49(137), 60(171), 85(211), 86(213), 87(215), 95(235), 96(237) Steiner, M. J., 39(118) Stewart, G. R., 2(4) Stiegler, J. O., 249(150) Stirling, W. G., 35(110) Stockert, O., 16(54), 22(79) Stoll, H., 154(354), 159(366) Stollhoff, G., 165(399–401) Stoner, E., 32–34 Stuesser, N., 22(79) Su, W. P., 12(38, 39) Sundquist, B. E., 198(54, 58, 63), 212 Suryanarayanan, R., 113(265), 119(272, 273, 275), 120(278) Sutton, A. P., 234(110) Suzuki, T., 11(32), 13(43), 79(202), 85(210, 211), 90(217) Svane, A., 50(140)

Swenson, C. A., 126(291) Szotek, Z., 50(140) T Tachiki, M., 164(392) Tajima, K., 77(200) Takagi, H., 126(293), 133(310), 162(380) Takahashi, Y., 59(162) Takata, M., 133(310) Takeda, K., 127(297) Takens, F., 282(257) Takeuchi, J., 127(297, 298) Takke, R., 46(126) Tamura, K., 50(139) Tanaka, A., 50(139) Tanaka, R., 225(92) Tanatar, B., 71(191) Tang, C., 280(254, 255) Tautz, F. S., 17(65), 20(74) Tayama, T., 23(83) Taylor, D. W., 153(339) Tegus, O., 39(119) Temmerman, W. M., 50(140) Terasaki, I., 92(225) Thalmeier, P., 11(31), 13(45), 16(53, 54), 24(84), 37(114), 42(124), 46(127), 49(137), 61(174), 62(179), 63(180), 65(181), 66(182), 87(215, 216), 97(239), 99(242–244), 101(246), 106(253), 110(261), 114(267), 119(272, 273, 275, 276), 137(314), 144(322), 165(400) Thomas, H., 91(219) Thompson, C. V., 186(20), 235 Tohyama, T., 174(409) Tokiwa, Y., 39(120), 52(143) Tokura, Y., 6(22), 108(255), 113(262, 263), 114(266), 119(274) Tomioka, Y., 114(266) Toth, L. S., 262(183) Tou, H., 66(183) Tran, M. -T., 144(322) Treaftis, H. N., 201(67) Treglia, G., 164(382, 383) Trovarelli, O., 16(55), 39(120) Tsakiropoulos, P., 193(30) Tsuda, N., 135(312) Tsvelik, A. N., 12(37) Tu, J. J., 155(365)

AUTHOR INDEX Tu, K. -N., 198(52) Turnbull, D., 198(48, 52), 201–203, 235(113) Tyer, R., 50(140)

301

Vollmer, R., 34(108) von der Linden, W., 159(371) von Schnering, H. G., 94(229) Voorhees, P. W., 185(13), 229(103) Vorderwisch, P., 38(115), 119(275)

U W Uchinokura, K., 92(225) Ueda, K., 28(90, 91), 59(162), 81(206), 91(220), 132(308) Ueda, Y., 92(226), 94(233), 103(248, 249), 105(251), 108(254) Uhlarz, M., 34(108) Uimin, G., 81(205) Uji, S., 17(64), 20(72, 73) Umehara, I., 20(72) Umezawa, L., 164(392) Umstätter, R., 164(395) Ungar, T., 262(183, 184) Unger, P., 164(396, 397), 174(407, 408) Urabe, T., 225(93) Urano, C., 126(293) V Valenti, R., 105(250) Valla, T., 155(363) Valsakumar, M. C., 282(259, 260) van de Kamp, R., 119(272, 275) Van der Giessen, E., 264(195), 265(198, 200–202) van der Marel, D., 97(240), 166(402) van der Merwe, A., 188(23) van Smaalen, S., 94(230, 231) Varelogiannis, G., 49(137) Varma, C. M., 13(46, 47), 16(58), 59(159), 160(374) Vaughan, G. B. M., 84(209), 138(315) Velický, B., 153(340) Verdier, M., 243(134–138) Verga, S., 154(360) Vergergaugry, J. L., 184(12) Vergnol, J., 274(245), 283(265) Verwey, E. J. W., 3, 124, 125 Victora, R. H., 164(393) Vidal, C., 182(2, 7) Virosztek, A., 162(377) Vleck, J. H. V., 6 Vollhardt, D., 154(350)

Wagner, R., 185(13) Waintal, X., 71(192) Wakabayashi, N., 77(200) Wakabayashi, Y., 113(263) Walgraef, D., 182(6), 253, 261(175), 270, 271 Walker, I. R., 39(118) Walz, F., 125(287) Wand, B., 87(215) Wang, R., 267(217) Ward, J. C., 10(30) Wastin, F., 171(403) Watanabe, K. I. T., 65(181) Watanabe, T., 66(182) Weaire, D., 186(19), 235 Weatherly, G. C., 196(39) Weber, D., 24(84) Weber, W., 97(238), 164(395) Weickert, F., 24(85) Weiden, M., 94(229), 95(235), 96(237), 97(238) Weiser, S., 164(395) Weissmann, S., 255(161) Wells, B. O., 155(363) Wen, X. -G., 140(321) Werner, E., 227 Wertheim, G. K., 147(331) West, D. F. R., 193(27, 28) Weygand, D., 235(124, 125), 238(128), 239(129, 130), 242(133), 264(195) White, R., 53(144) White, S. R., 159(370) Whiting, M. J., 193(30) Wiesenfeld, K., 280(254, 255) Wigner, E., 3, 7, 40, 66–74, 91, 108, 177, 179 Wildes, A., 38(115) Wilhelm, H., 38(117), 39(120) Wilkens, M., 262(184) Wilkins, J. W., 16(56, 57) Williams, D. B., 196(38, 41)

302

AUTHOR INDEX

Willis, J. O., 2(4) Wills, J. M., 50(141) Winter, A. T., 267(212, 213) Wohlleben, D. K., 46(126) Wolf, B., 24(84) Woods, S. B., 76, 126 Wright, W. H., 59(150) Y Yamada, Y., 115(268) Yamagami, H., 17(67) Yamagani, H., 52(143) Yamaki, K., 50(139) Yamamoto, E., 52(143), 66(183) Yamamoto, N., 133(310) Yamashita, Y., 132(308) Yamauchi, T., 108(254) Yanagisawa, T., 52(143) Yaresko, A., 136(313), 137(314) Yaresko, A. N., 13(45), 97(239), 125(290), 129(299) Yonezawa, F., 153(341) Yoshitake, R., 77(200) Yoshizawa, H., 117(271), 121(279) Yosihama, T., 103(248) Yotsuhashi, S., 132(307) Yourgrau, W., 188(23) Yu, L., 40(122) Yuan, Q., 114(267) Yunoki, S., 122(281) Yushankhai, V., 37(114), 38(117), 144(322) Yusof, Z., 155(363)

Z Zaanen, J., 5(14) Zaiser, M., 258(165), 266(204, 207–210), 267 Zawadowski, A., 15(52) Zbib, H. M., 264(194) Zener, C., 108(256), 198–203, 208–210, 215, 239 Zerec, I., 42(124) Zevin, V., 12(36) Zhang, F. C., 108, 173–176 Zhang, G. M., 40(122) Zhang, Y. Z., 137(314), 144(322) Zheng, H., 115(270) Zheng, W. J., 154(357) Zhou, S. Y., 162(380) Zhou, X. J., 154(357, 358) Zhu, L., 39(119), 46(129) Zieba, P., 196, 202(68), 205(70–73) Ziegenbein, A., 284(272) Ziman, T., 103(247) Zimanyi, G. T., 160(375) Zinkle, S. J., 253(155) Zölfl, M., 131(303) Zvyagin, A. A., 129(299) Zwanzig, R., 150(335) Zwicknagl, G., 9(29), 11(33), 12(36), 16(53, 54), 17(61), 18(68), 20(71), 22(78, 79), 26(87), 27(88, 89), 56(145, 146), 57(147, 148)

Subject Index

phase diagram, 112–114 physics of, 108–110 in 3D-valence elections, 67, 68 in homogeneous 2D electron systems, 69–74 original proposal, 66–67 quasi-1D spin excitations α -NaV2 O5 , 91–107 electronic structure, 97–98 Hubbard model, 98–99 Ising-spin Peierls model, 101–107 ITF model, 99–101 Jordan–Wigner mapping, 91–92 β-vanadium bronzes, 107–108 structural phase transition, 92–93 temperature structure, 93–97 Wigner crystallization 4f model Hamiltonian, 81–87 Dzyaloshinsky–Moriya interaction, 88–91 experimental summary, 74–76 Labbé–Friedel model, 81 underlying physics, 77–81 Chemical patterning characterization, 185–186, 192–193 coarsening discontinuous, 230–231 overview, 225, 227 spheroidization, 227–230 discontinuous precipitation characterization, 194–196 divergent lamellar growth, 224–225 interface motion, 219–220 multilayer stability, 232 spacing selection, 216, 218 morphological evolution, 225, 227–230 non-steady state growth concerns, 218–219 divergent lamellar, 220–222, 224–225 interface motion, 219–220 spacing selection, 213, 215–218 steady state growth Cahn’s treatment, 204–206 discontinuous precipitation, 211–213

A AF structures, 60–61 ALV2 O4 characterization, 133–134 charge disproportionation, 136–139 structural transitions, 134–136 V ions, 134 α -NaV2 O5 coupled CO, 98–107 crystal structure, 94–95 electronic structure, 97–98 exchange dimerization in, 98–107 ground state, 91 Jordan–Winger mapping, 91–92 structural phase transition, 92–93 temperature structure, 93–97 B Bands persistent slip, 268–272 shadow, 151–153 theory, 18–19 BEC. See Bose–Einstein condensation Bilayer manganites. See Double exchange bilayer manganites Bose–Einstein condensation, 38 C Cahn’s treatment, 204–206 CeCu2 Si2 heavy fermions, 19–23 phase diagram, 23–30 CEF. See Crystalline electric fields CeRu2 Si2 , 19–23 Charge ordering 4f compounds, 67–68 concept of, 66 density in metals, 68–69 double exchange bilayer manganites as function of eg , 110–112 model, 117–122 303

304

SUBJECT INDEX

Chemical pattering (Continued) Hillbert’s treatment, 202–203 pearlite observations, 206–211 theoretical history, 197–199 Turnbull’s treatment, 202–203 Zener treatment, 199–202 transformations -discontinuous precipitation, comparison, 198–199 characterization, 193–195 divergent lamellar growth, 220–222, 224 experimental observations, 206–207 Fe-C steels, 208–208 identification, 196 multilayer stability, 232 regularity of, 193, 197 steady state growth, 206–211 CMR. See Colossal magnetoresistance effect Co-Si system, 230–231 Coarsening discontinuous, 230–231 overview, 225, 227 spheroidization, 227–230 Coherent potential approximation, 153–154 Colossal magnetoresistance effect, 108 Condensation, Bose–Einstein, 38 Cooper pairs, 59 Copper-oxide planes, 171–176 Correlated systems with orbital degeneracies, 48–51 CPA. See Coherent potential approximation Creation operators, 26–27 Crystalline electric fields characterization, 15 doublet-quartet scheme, 23, 35 in rare earth ions, 59 singlet states, 36–38 Crystallization. See Wigner crystallization Cu-Al systems, 206–207 Cuprates perovskite structures, 13–14 D Discontinuous precipitation -transformation, comparison, 198–199 chemical patterning characterization, 194–195 identification, 196

interface motion, 219–220 Klinger’s alternative, 216, 218 theory/experiment comparisons, 211–213 divergent lamellar growth, 224–225 Dislocations characterization, 233–234 patterning cell formation, 258 dynamic nature of, 261–262 first theory, 260 Hähner model, 266–267 Holt model, 260–261 Kocks model, 261 structures carpets, 249, 252 density of, 245 in PSB, 268–272 recovery density decreases, 245 kinetics, 243 processes, 243 study results, 248 recrystallization evolution of, 240–241 nucleation of, 241–243 study results, 248 void lattices, 249, 252 Divergent lamellar growth, 220–222, 224 Double exchange bilayer manganites reentrant charge ordering as function of eg , 110–112 electronic structure calculations, 110 model, 117–122 phase diagram, 112–114 physics of, 108–110 polaron formation, 114–117 structural properties, 109–110 Dynamical mean field theory, 17 Dzyaloshinsky–Moriya interaction, 88–91 E Elastic strains, 190 Energy chemical, 188–189 free, 77–78 free energy, 189–191

SUBJECT INDEX high (See High-energy excitations) interfacial, 190–191 low, scales, 10–12 madelung, 87 strain, 190 Equilibrium systems maintained far from, 191–192 systems prepared far from chemical energy, 188–189 interfacial energy, 190–191 strain energy, 190 structural patterning in, 186–187 Eutectoid decomposition, 220–222, 224–225

F Fatigue loading, 267–268, 270–272 Fault migration, 229 Fe-C steels, 208–208 Fe-C-Mn systems, 222, 224 Fe-C-Mo systems, 222, 224 Fe-C-Si systems, 222, 224 Fe3 /O4 , 124–125, 130 Fermi-liquid state CeCu2 Si2 , 19–23 CeRu2 Si2 , 19–23 high-energy excitations combined models, 153–154 findings, 159–163 methodology, 154–159 mean-field theory, 16–17 renormalized band theory, 18–19 strongly correlated electrons deviations, 12–14 Wigner crystallization, 69, 71 Fermions, heavy, 19–23 Five f systems, 168–171 Free energy at phase/grain boundary interface, 190–191 elastic strain-induced, 190 strain-free regions, 189 Free energy changes systems continuously maintained, 191–192 systems preparation characterization, 188–189 chemical energy, 189

305 interfacial energy, 190–191 strain energy, 190 G

Geometrically frustrated lattices characterization, 123 charge disproportionation, 133–139 fractional charges, 139–147 function, 122–123 metallic spinels, 124–133 structural transition, 133–139 Grain growth characterization, 234 computer models, 235–236 experiments, 234–235 log normal distributions, 236–240 Green function, 7–8 H Hähner model, 266–267 Heavy quasiparticles in U compounds dual model application, 51–54 dual model theory, 50–51 superconductivity, 59–66 High-energy excitations copper-oxide planes, 171–176 energies, 147–148 Hubbard model, 151–153 in 5f systems, multiplet effects, 168–171 kink structure, 153–163, 154–159 marginal Fermi liquid behavior combined models, 153–154 findings, 159–163 methodology, 154–159 Ni satellite structure, 163–168 projection operators, 148, 149–150 research summary, 176–178 zero-point fluctuations, 149 Hillbert’s treatment, 202–203 Holt model, 260–261 Hubbard model for high-energy excitations, 151–153 quasi-1D spin excitations, 98–99 Hückel theory, 3

306

SUBJECT INDEX I

Interatomic correlations, 3–4 Interface motion, 219–220 Interfaces at phases/grain boundaries, 190–191 Intra-atomic correlations function, 4 in superconductivity, 59–66 strength measure, 5–6 Irradiation main effect of, 252 rate equations, 253 structural defect patterning experimental characteristics, 249, 252 rate equations, 253 reaction diffusion approach, 252–255 void formation, 254–255, 258 Ising model in transverse field, 99–101 ITF. See Ising model in transverse field Itinerant ferromagnetism models, 32–37

Lamellar patterning characterization, 225, 227 discontinuous precipitation, 224–225 pearlite, 220–222, 224 spheroidization, 227–230 LaMnO3 electronic structure calculations, 110 physics, 108 structural properties, 109–110 Landau theory, 9–10 LaSr2 Mn2 O2 electronic structure calculations, 110 physics of, 108 structural properties, 109–110 LDA. See Local density approximations Line defects. See Dislocations LiV3 /O4 , 125–133 Local density approximations, 51 Log normal distributions, 236–240 Low-energy scales, 10–12

J M Jordan–Wigner transformation, 91–92 K Kink excitations, 12–13 Kink structure, 153–163 Klinger’s alternative, 216, 218 Kocks model, 261 Kondo lattice systems Ce-based compounds, 15–16 CeCu2 Si2 , 19–23 CeRu2 Si2 , 19–23 Fermi-liquid state, 18–19 function, 14–15 heavy fermions, 19–23 heavy quasiparticles, 18–19 magnetic ions, 16–17 quantum criticality in, 38–45 renormalized band theory, 18–19 scaling theory, 45–48 Kondo necklace model, 40 L Labbé–Friedel model, 81 Lamellar growth, divergent, 220–222, 224

Madelung energy, 87 Magnetic ion lattice, 16–17 Magnets, itinerant, 32–38 Magnets, localized, 32–38 Manganites. See Double exchange bilayer manganites Metallic spinels Fe3 /O4 , 124–125 LiV3 /O4 , 125–133 Metals. See also specific metals density in, charge ordering, 68–69 Landau theory, 9–10 quasiparticle energies, 8–9 transitions, 6 N Nickel satellite structure, 163–168 Non-steady state growth chemical patterning concerns, 218–219 divergent lamellar, 220–222, 224–225 interface motion, 219–220

SUBJECT INDEX O Orbital degeneracies in correlated systems dual model, 49–51 examples, 48–49 P Partial localization concept of, 48–49 in U compounds heavy quasiparticles in, 51–54 LDA, 51 microscopic model calculations, 54–58 Patterns Belgian school, 182–183 chemical (See Chemical patterning) concept of, 182 energetic costs, 183 equilibrium departure, 184 in metallic alloys, 183–184 spatio-temporal (See Spatio-temporal patterning) structural (See Structural defect patterning) Pearlite transformations -discontinuous precipitation, comparison, 198–199 characterization, 193–195 divergent lamellar growth, 220–222, 224 experimental observations, 206–207 Fe-C steels, 208–208 identification, 196 regularity of, 193, 197 steady state growth, 206–211 Persistent slip bands, 268–272 Phase diagrams CeCu2 Si2 , 23–30 charge ordering, 112–114 Phase transitions CeCu2 Si2 , 23–30 free energy, 190–191 quantum broken symmetry state, 30–32 in itinerant magnets, 32–38 in localized magnets, 32–38 structural, 92–93 Plasticity in structural defect patterning

307

classical approaches, 258, 260–263 computer simulations, 263–266 experimental facts, 255–256 fatigue loading, 267–268, 270–272 spatio-temporal patterning in chaotic behavior of, 282–284 characterization, 273–274 phenomenology of, 274–276 serrated flow, statistical analysis, 276–280 stress-strain curve, 187 PLC. See Portevin–Chatelier effect Polarons formation in double exchange bilayer manganites, 114–117 hopping element, 116 JT type, 115 Polyacethylene, 12–13 Portevin–Chatelier effect chaotic behavior of, 282–284 characterization, 273–274 phenomenology of, 274–276 serrated flow, statistical analysis, 276–280 PSB. See Persistent slip bands Pyrochlore lattice band structure, 127–128 characterization, 123 spin degrees of freedom, 129 Q QCP. See Quantum critical point QCT. See Quantum phase transitions QPC. See Quantum critical point Quantum critical point non-Fermi behavior in, 14 QPT in, 31 scaling theory, 45–48 Quantum criticality, 38–45 Quantum phase transitions broken symmetry state, 30–32, 31–32 in itinerant magnets, 32–38 in localized magnets, 32–38 onset of, 35–36 Quasi-1D spin excitations charge ordering α -NaV2 O5 , 91–107 electronic structure, 97–98 Hubbard model, 98–99

308

SUBJECT INDEX

Quasi-1D spin excitations (Continued) ITF model, 99–101 β-vanadium bronzes, 107–108 structural phase transition, 92–93 temperature structure, 93–97 Ising-spin Peierls model, 101–107 Jordan–Wigner mapping, 91–92 Quasiparticles. See Heavy quasiparticles R Raleigh instability, 227–228 Rate equations, 253 Reaction diffusion approach, 252–255 Recrystallization, 240–243 S β-Vanadium bronzes, 107–108 SDW. See Spin-density wave Self organized criticality, 276–280 Serrated flow, 276–280 Shadow bands, 151–153 SOC. See Self organized criticality Spacing selection chemical patterning discontinuous precipitation, 216, 218 problems, 213, 215–218 Spatio-temporal patterning PLC effect chaotic behavior of, 282–284 characterization, 273–274 phenomenology of, 274–276 serrated flow, statistical analysis, 276–280 stress-strain curve, 187 Spheroidization, 227–230 Spin excitations. See Quasi-1D spin excitations Spin-change separation, 12–13 Spin-density wave, 24 Steady state growth. See also Non-steady state growth chemical patterning Cahn’s treatment, 204–206 discontinuous precipitation, 211–213 Hillbert’s treatment, 202–203 pearlite observations, 206–211 theoretical history, 197–199

Turnbull’s treatment, 202–203 Zener treatment, 199–202 Stick-slip model, 277, 279 Stoner–Wolfarth theory, 32 Strain energy, 190 Strain-free regions, 189 Strong correlations, 139–147 Strongly correlated electrons charge ordering α -NaV2 O5 , 91–108 concept of, 66–69 generalized Wigner lattice, 74–91 homogeneous 2D systems, 69–74 ID spin excitations, 91–108 reentrant, 108–122 Wigner crystallization, 69–74 Yb4 As3 , 74–91 Fermi-liquid behavior deviations, 12–14 geometrically frustrated lattices characterization, 122–124 charge disproportionation, 133–139 fractional changes, 139–147 metallic spinels, 124–133 structural transitions, 133–139 high-energy excitations 5f systems, 168–171 characterizations, 147–149 copper-oxide planes, 171–176 future research, 176–178 Hubbard model, 151–153 kink structure, 153–163 marginal Fermi liquid behavior, 153–163 Ni satellites, 163–168 projection operators, 149–150 shadow bands, 151–153 Kondo lattice systems band theory, 18–19 CeCu2 Si2 , 19–30 CeRu2 Si2 , 19–23 characterization, 14–18 Fermi-liquid state, 18–19 heavy fermions, 19–23 heavy quasiparticles, 18–19 low-temperature phase, 23–30 quantum criticality, 38–45 low-energy scales, 10–12 overview, 2–8 partial localization

SUBJECT INDEX characterization, 48–51 intra-atomic excitations, 59–66 microscopic model calculation, 54–59 quasiparticles, 51–54 superconductivity, 59–66 UPd2 Al3 , 51–54 quantum phase transitions characterization, 30–32 critical point, 45–48 criticality, 38–45 itinerant magnets, 32–38 localized magnets, 32–38 scaling theory, 45–48 theories, 8–10 Structural defect patterning characterization, 233–234 dislocation structures cold rolling stain, 245, 248 density of, 245, 248 evolution, 240–241 nucleation of, 241–243 recovery kinetics, 243, 248 recovery observations, 243 grain growth characterization, 234 computer models, 235–236 experiments, 234 Log Normal distributions, 236–240 irradiation-induced experimental characteristics, 249, 252 rate equations, 253 reaction diffusion approach, 252–255 void formation, 254–255 plasticity-induced classical approaches, 258, 260–263 computer simulations, 263–266 experimental facts, 255–256, 258 fatigue loading, 267–268, 270–272 Hähner model, 266–267 Structural patterning, 186–187 Structural transition, 133–139 Superconductivity A phase interplay, 24–26 CeCu2 S2 , 24–29 intra-atomic excitations, 59–66

309 T

Transformations. See Pearlite transformations Transitions metals, 6 Turnbull’s treatment, 202–203 U U compounds AF structures, 60 heavy quasiparticles dual model application, 51–54 dual model theory, 50–51 microscopic model calculations, 54–58 superconductivity, 59–66 V Void formation, 254–255 W Wigner crystallization charge ordering 4f model Hamiltonian, 81–87 Dzyaloshinsky–Moriya interaction, 88–91 experimental summary, 74–76 Labbé–Friedel model, 81 underlying physics, 77–81 in homogeneous 2D electrons, 69–74 Y Yb4 , change ordering 4f model Hamiltonian, 81–87 elastic constant, 78–80 free energy, 77–78 interacting chains, 81 lattice structure, 74–76 Madelung energy, 87 Z Zener treatment, 199–202

This page intentionally left blank

Founding Editors FREDERICK SEITZ DAVID TURNBULL

SOLID STATE PHYSICS Advances in Research and Applications

Editors HENRY EHRENREICH FRANS SPAEPEN

Division of Engineering and Applied Sciences Harvard University Cambridge, Massachusetts

VOLUME 60

AMSTERDAM • BOSTON • HEIDELBERG • LONDON • NEW YORK • OXFORD PARIS • SAN DIEGO • SAN FRANCISCO • SINGAPORE • SYDNEY • TOKYO Academic Press is an imprint of Elsevier

Academic Press is an imprint of Elsevier 84 Theobald’s Road, London WC1X 8RR, UK Radarweg 29, PO Box 211, 1000 AE, Amsterdam, The Netherlands 30 Corporate Drive, Suite 400, Burlington, MA 01803, USA 525 B Street, Suite 1900, San Diego, California 92101-4495, USA ∞ This book is printed on acid-free paper

Copyright © 2006, Elsevier Inc. All rights reserved No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means electronic, mechanical, photocopying, recording or otherwise, without the prior written permission of the publisher. Permissions may be sought directly from Elsevier’s Science and Technology Rights Department in Oxford, UK: phone: (+44) (0) 1865 843830; fax: (+44) (0) 1865 853333; e-mail: [email protected] You may also complete your request on-line via the Elsevier homepage (http://www.elsevier.com), by selecting ‘Customer Support’ and then ‘Obtaining Permissions’ ISBN-13: 978-0-12-607760-5 ISBN-10: 0-12-607760-6 ISSN: 0081-1947 For information on all Academic Press publications visit our web site at http://books.elsevier.com Printed and bound in USA 05 06 07 08 09 10

10 9 8 7 6 5 4 3 2 1

Contents C ONTRIBUTORS TO VOLUME 60 . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . P REFACE . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

vii ix

Strongly Correlated Electrons P. F ULDE , P. T HALMEIER AND G. Z WICKNAGL I. II. III. IV. V. VI. VII. VIII. IX.

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Special Features of Strong Correlations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Kondo Lattice Systems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Quantum Phase Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Partial Localization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Charge Ordering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Geometrically Frustrated Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . High-Energy Excitations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Summary and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Acknowledgment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

2 8 14 30 48 66 122 147 176 179

Defect-Induced Dynamic Pattern Formation in Metals and Alloys Y. B RÉCHET AND C. H UTCHINSON I. II. III.

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Free Energy Changes, Driving Forces and Energy Input . . . . . . . . . . . . . . . . . . . . . . . . . . Chemical Patterning: Interface-Mediated Transformations: Eutectoid Decomposition and Discontinuous Precipitation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . IV. Structural Defect Patterning: Grain Growth, Recovery and Recrystallization . . . . . . . . . V. Structural Defect Patterning: Irradiation and Plastic Deformation . . . . . . . . . . . . . . . . . . VI. Spatio-Temporal Patterning in Plasticity: The Portevin–Le Chatelier Effect . . . . . . . . . . VII. Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

182 188 192 233 248 273 285

AUTHOR I NDEX . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . S UBJECT I NDEX . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

289 303

This page intentionally left blank

Contributors to Volume 60 Numbers in parentheses indicate the pages on which the authors’ contributions begin.

Y VES B RÉCHET (181) Laboratoire de Thermodynamique et Physico-Chimie Métallurgiques, Institut National Polytechnique de Grenoble, 38402, St. Martin D’Hères, France P ETER F ULDE (1) Max-Planck-Institut für Physik komplexer Systeme, 01187 Dresden, Germany C HRISTOPHER H UTCHINSON (181) Department of Materials Engineering, Monash University, Clayton, 3168, Vic, Australia P ETER T HALMEIER (1) Max-Planck-Institut für Chemische Physik fester Stoffe, 01187 Dresden, Germany G ERTRUD Z WICKNAGL (1) Institut für Mathematische Physik, Technische Universität Braunschweig, 38106 Braunschweig, Germany

This page intentionally left blank

Preface

The article by Fulde, Thalmeier and Zwicknagl traces many of the recent developments in the field of strongly correlated many electron systems. It is very useful both as a reference and a pedagogical exposition since it places these developments into a historical context beginning with early developments in the electron theory of solids. Together with its extensive references and its formal elucidation of important theoretical subjects, the article supplies an excellent entry point into the field which is closely coupled to the classic works on the subject. Many early important ideas, such as Hückel and Heitler–London theory, the Wigner lattice, metal-insulator transitions originated in the thirties and were extensively developed in the sixties when it came to be realized that transition and rare earth metals with their characteristic d and f electrons respectively should be viewed as at least moderately strongly correlated systems requiring more sophisticated theoretical treatments than those supplied by the simplest band theories. The development of the relevant theories are associated with Hubbard and Mott among many others. They introduced model Hamiltonians, which were amenable to easily performed calculation whose results exhibited metal-insulator transitions for appropriate choices of the inter- and intra-atomic physical parameters. The Hubbard Hamiltonian, for example, motivated by lattices containing transition metal constituents has remained, in the authors’ words one of the “working horses of many studies of strongly correlated” electron systems. Even though early conventional applications are limited to d electrons, many of the generic effects of strongly correlated electrons are captured by its solutions. A principal impetus for the development of the field is associated with the discovery of high temperature superconductivity in copper-oxide based perovskites in 1986. Indeed, but for the strong electron correlations in hole-doped superconductors like La2−x Bax CuO4 would be metallic instead of insulating antiferromagnetic. It is the richness of the periodic table resulting from the presence of inner shell electrons in the heavier elements and their associated correlations that is responsible for these otherwise unexpected physical effects. Although superconducting phenomena play an important role in the article, we stress that the principal topic concerns the more general behavior of strongly corix

x

PREFACE

related electrons in solids. The article presents a detailed description of Kondo lattice systems and its associated heavy fermions, which preceded the discovery of high temperature superconductivity. It relates the results to a wide variety of experimental observations in real systems wherever possible. Readers having special interests in given heavy fermion materials will thus be well rewarded by browsing its pages and detailed figures of, for example, Fermi surfaces, photoemission results and phase diagrams. The article begins with a detailed exposition of the physical features that characterize strong electron correlations, and presents a detailed description of the central feature associated with strong correlations leading to the presence of energy scales low compared to the typical metallic Fermi energy possibly resulting in deviations from Fermi-liquid behavior. This introduction is followed by a detailed description of Kondo lattice systems which deal with magnetic impurities associated with spins embedded in a metal and interacting via exchange scattering. The understanding of Ce-based heavy Fermi systems present particular challenges. The authors describe theoretical techniques for describing such systems that combine ab initio approaches with a phenomenologically based Landau theory. A so-called renormalized band scheme is used for calculating realistic quasi-particle bands of materials grown and observed in the laboratory. Quantum phase transitions in localized and itinerant magnetic systems characterize many systems of direct interest here. Quantum criticality in the Kondo lattice and scaling theory close to quantum critical points are discussed in considerable detail. Charge ordering, which began with the notion of crystallization first introduced in the 30s by Wigner was subsequently observed in 2D electron systems. Originating from a variety of effects, charge ordering can occur in many types of systems. For example, Yb4 As3 , which is discussed in considerable detail from both experimental and theoretical points of view in the present exposition, exhibits charge ordering associated with 4f holes. It illustrates the formation of heavy quasiparticles caused by spin chains without involvement of the Kondo effect. Other subjects discussed here include partial localization found in some actinide-based heavy fermion compounds in which experiments are used to infer the co-existence of delocalized and localized 5f electrons, superconductivity mediated by intra-atomic excitations, geometrically frustrated lattices such as metallic spinels, fractional charges resulting from strong correlations, and high energy correlation induced excitations, for example, the appearance of shadow bands and satellites associated with nickel. Because of its significant reliance on and comparison with experiment, its frequent use of phenomenologically based theory used to calculate quasi-particle band structures and Fermi surfaces, this article is to some extent less focussed on

PREFACE

xi

fundamental microscopic theoretical aspects than on techniques leading to optimal physical insight permitting ready comparison with observations relevant to important materials systems. Clearly both types of expositions are needed. The second article in this volume, by Bréchet and Hutchinson, concerns pattern formation in metals and alloys. Spontaneous pattern formation is the development of a regularity, either in the spatial distribution of the material in a system or in its development in time, of a lower symmetry than that of its cause. These phenomena have been of considerable interest to the non-linear physics community, in particular in fluid dynamics and in chemical reactions. This article deals with pattern formation in the solid state, which is comparatively less studied. Usually, crystal defects, such as dislocations or interfaces, play an important role and the energetic cost required by their formation requires that the system be prepared or maintained far from equilibrium. Interface-mediated formation of lamellar microstructures from supersaturated solution is discussed as an example of chemical patterning in a system prepared far from equilibrium. Striking examples are the formation of pearlite and discontinuous precipitation. Grain growth, recovery and recrystallization are discussed as examples of defect pattering in a system prepared far from equilibrium. Grain growth is a rich topological subject, several aspects of which have been presented in earlier articles in this Series, such as that by Weaire and McMurry in vol. 50 and by Thompson in vol. 55. Systems that are maintained far from equilibrium can be called “driven systems”. Martin and Bellon have reviewed the chemical aspects of such systems in their article in vol. 50 of the Series. The present article therefore concentrates more on structural pattering in driven systems, such as the formation of arrays of dislocation loops and voids under irradiation or dislocation patterning in deformation. Finally, plastic deformation provides an interesting example of pattering in both space and time: the Portevin–Le Chatelier effect, which is a stick-slip effect of plastic waves that move through the sample. The authors show that this can be usefully analyzed as a case of self-organized criticality. H ENRY E HRENREICH F RANS S PAEPEN

This page intentionally left blank

SOLID STATE PHYSICS VOLUME 60

This page intentionally left blank

SOLID STATE PHYSICS, VOL. 60

Strongly Correlated Electrons

P ETER F ULDE Max-Planck-Institut für Physik komplexer Systeme, 01187 Dresden, Germany

P ETER T HALMEIER Max-Planck-Institut für Chemische Physik fester Stoffe, 01187 Dresden, Germany

G ERTRUD Z WICKNAGL Institut für Mathematische Physik, Technische Universität Braunschweig, 38106 Braunschweig, Germany

I. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . II. Special Features of Strong Correlations . . . . . . . . . . . . . . . . . . . . . . . . . . . 1. Low-Energy Scales: a Signature of Strong Correlations . . . . . . . . . . . . . . . 2. Deviations from Fermi-Liquid Behavior . . . . . . . . . . . . . . . . . . . . . . . . III. Kondo Lattice Systems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3. Fermi-Liquid State and Heavy Quasiparticles: Renormalized Band Theory . . . . . 4. Heavy Fermions in CeRu2 Si2 and CeCu2 Si2 . . . . . . . . . . . . . . . . . . . . . 5. Low-Temperature Phase Diagram of CeCu2 Si2 . . . . . . . . . . . . . . . . . . . . IV. Quantum Phase Transitions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6. Quantum Phase Transition in Localized and Itinerant Magnets . . . . . . . . . . . . 7. Quantum Criticality in the Kondo Lattice . . . . . . . . . . . . . . . . . . . . . . . 8. Scaling Theory Close to the Quantum Critical Point . . . . . . . . . . . . . . . . . V. Partial Localization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9. Heavy Quasiparticles in UPd2 Al3 . . . . . . . . . . . . . . . . . . . . . . . . . . . 10. Microscopic Model Calculation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11. Superconductivity Mediated by Intra-Atomic Excitations . . . . . . . . . . . . . . VI. Charge Ordering . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12. Wigner Crystallization in Homogeneous 2D Electron Systems . . . . . . . . . . . . 13. Generalized Wigner Lattice: Yb4 As3 . . . . . . . . . . . . . . . . . . . . . . . . . 14. Charge Ordering and 1D Spin Excitations in α -NaV2 O5 . . . . . . . . . . . . . . 15. Reentrant Charge Ordering and Polaron Formation in Double Exchange Bilayer Manganites La2−2x Sr1+2x Mn2 O7 . . . . . . . . . . . . . . . . . . . . . . . . . . . VII. Geometrically Frustrated Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16. Metallic Spinels: LiV2 O4 — a Metal with Heavy Quasiparticles . . . . . . . . . .

2 8 10 12 14 18 19 23 30 32 38 45 48 51 54 59 66 69 74 91 108 122 125

1 ISBN 0-12-607760-6 ISSN 0081-1947/06

© 2006 Elsevier Inc. (USA) All rights reserved.

2

P. FULDE ET AL.

17. Structural Transition and Charge Disproportionation: AlV2 O4 18. Fractional Charges Due to Strong Correlations . . . . . . . . . VIII. High-Energy Excitations . . . . . . . . . . . . . . . . . . . . . . . . 19. Projection Operators . . . . . . . . . . . . . . . . . . . . . . . . 20. The Hubbard Model: Appearance of Shadow Bands . . . . . . 21. Marginal Fermi Liquid Behavior and Kink Structure . . . . . . 22. Nickel and its Satellite . . . . . . . . . . . . . . . . . . . . . . . 23. Multiplet Effects in 5f Systems . . . . . . . . . . . . . . . . . 24. Excitations in Copper-Oxide Planes . . . . . . . . . . . . . . . IX. Summary and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . Acknowledgment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . List of Acronyms . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

133 139 147 149 151 153 163 168 171 176 179 179

I. Introduction

The field of strongly correlated electron systems has been constantly growing for almost three decades. A milestone in its development was the discovery by Andres, Graebner and Ott1 of heavy-quasiparticle excitations in CeAl3 . Additional verve came from the discovery of superconductivity in the related compounds CeCu2 Si2 ,2 UBe13 3 and UPt3 .4 But a real great push for the field was provided by the discovery of high-temperature superconductivity in the copperoxide based perovskites.5 Were it not for strong electron correlations La2 CuO4 , one of the key compounds of that class of materials and the basis of the hole doped superconductors La2−x Bax CuO4 and La2−x Srx CuO4 would be metallic. Instead it is an antiferromagnet which remains insulating even above the Néel temperature where the unit cell is not doubled anymore. Therefore, electron correlations are apparently so strong that the metallic character of the material is suppressed in favor of an insulating state. That electron correlation may induce a metal to insulator transition had been suggested long before the discovery of heavy quasiparticles and high-Tc cuprates. The names of Mott6 and Hubbard7 stand for that phenomenon. At their time the interests in the effects of strong correlations resulted from the transition metal oxides and their various phase transitions. It is 1 K. Andres, J. E. Graebner, and H. R. Ott, Phys. Rev. Lett. 35, 1779 (1975). 2 F. Steglich, J. Aarts, C. D. Bredl, W. Liecke, D. Meschede, W. Franz, and H. Schäfer, Phys. Rev.

Lett. 43, 1892 (1979). 3 H. R. Ott, H. Rudigier, Z. Fisk, and J. L. Smith, Phys. Rev. Lett. 50, 1595 (1983). 4 G. R. Stewart, Z. Fisk, J. O. Willis, and J. L. Smith, Phys. Rev. Lett. 52, 679 (1984). 5 J. G. Bednorz and K. A. Müller, Z. Phys. B 64, 189 (1986). 6 N. F. Mott, Metal–Insulator Transition, Taylor and Francis, London (1990), 2nd ed. 7 J. Hubbard, Proc. R. Soc. London A 276, 238 (1963).

STRONGLY CORRELATED ELECTRONS

3

worth recalling that the famous Verwey8 transition in magnetite Fe3 O4 falls into the same category. One may even go back to Wigner9 or Heitler and London10 who dealt with strongly correlated electrons long before corresponding experiments were available. While Wigner pointed out that electrons may form a lattice when their correlations become sufficiently strong, Heitler and London developed a theory for chemical bonding based on strongly correlated electrons. It is the opposite limit of Hückel’s theory11–13 based on molecular orbitals in which electron correlations are completely neglected. This raises the question of how to quantify the strength of electronic correlations. For example, one would like to know how much more strongly electrons are correlated in LaCu2 O4 than, e.g., in iron or nickel or in transition metal oxides. The differences between systems with strongly and with weakly correlated electrons may be seen by considering the ground state of the simplest possible example, i.e., of a H2 molecule in the Heitler–London- and in the molecular orbital limit. The Heitler–London form of the ground-state wavefunction is 1 ψHL r1 , r2 = φ1 (r1 )φ2 (r2 ) + φ2 (r1 )φ1 (r2 ) (α1 β2 − β1 α2 ) 2

(1.1)

where the single-electron wavefunctions φ1,2 (r) are centered on atoms 1 and 2 of the molecule and α and β denote spinors for up and down spins. In distinction to Eq. (1.1) the molecular-orbital form of the ground-state wavefunction is ψMO (r1 , r2 ) =

1 φ1 (r1 )φ1 (r2 ) + φ1 (r1 )φ2 (r2 ) + φ2 (r1 )φ1 (r2 ) (1.2) + φ2 (r1 )φ2 (r2 ) (α1 β2 − β1 α2 ).

23/2

It is seen that ψMO (r1 , r2 ) but not ψHL (r1 , r2 ) contains ionic configurations φ1 (r1 )φ1 (r2 ) and φ2 (r1 )φ2 (r2 ). In Eq. (1.2) they have equal weight as the nonionic configurations. But ionic configurations cost additional Coulomb repulsion energy of the electrons. Therefore they are completely suppressed in the Heitler– London- or strong correlation limit. This demonstrates an important feature of electron correlations, namely a partial suppression of electronic charge fluctuations on an atomic site. The former are called interatomic correlations because charge fluctuations at an atomic site are caused by an overlap of wavefunctions of 8 E. J. W. Verwey and P. W. Haayman, Physica 8, 979 (1941). 9 E. Wigner, Phys. Rev. 46, 1002 (1934). 10 W. Heitler and F. London, Z. Phys. 44, 455 (1927). 11 E. Hückel, Z. Phys. 70, 204 (1931). 12 E. Hückel, Z. Phys. 72, 310 (1931). 13 E. Hückel, Z. Phys. 76, 628 (1932).

4

P. FULDE ET AL.

different atoms. They are favored by a kinetic energy gain due to electron delocalization. Reducing them compared with uncorrelated electrons keeps the Coulomb repulsions small. In addition to interatomic correlations we must also consider intra-atomic correlations. Consider an atom of a solid in a configuration with a given number of electrons, for example, a C atom in diamond with, e.g., 4 or 5 valence electrons. Those electrons will optimize their on-site Coulomb repulsions by arranging according to Hund’s rules and by in-out correlations. Hund’s rules ensure that electrons on an atom are optimally distributed over the angular segments of the atom, so that their repulsions are as small as possible. In-out correlations achieve the same by proper radial distribution of the electrons. Intra-atomic correlations are strongest for 4f electrons, i.e., for atoms or ions of the lanthanide series. But also in actinides or transition-metals they play a big role. Large overlaps with atomic wavefunctions of the chemical environment will weaken them. This is understandable: before the electrons can fully establish intra-atomic correlations they leave for the neighboring sites by hopping off the site. Interatomic correlations can be strong even when intra-atomic correlations are moderate or weak. Let us make a gedanken experiment and consider a Si crystal with artificially enlarged lattice parameter. The intra-atomic correlations on a Si site are fairly moderate, but the interatomic correlations are becoming strong when the lattice constant is increased, i.e., when the limit of separate atoms is approached. In that case fluctuations in the electron number at a site reduce to zero. From the above considerations it follows that a suitable measure of the interatomic correlation strength is the reduction of electron number fluctuations on a given atom. An independent-electron or Hartree–Fock description implies too large fluctuations. Let |ψ0 denote the exact ground state of an electronic system and |SCF the corresponding self-consistent field (SCF) or Hartree–Fock (HF) state. The normalized mean-square deviation of the electron number ni on atom i is given by (i) =

SCF |(ni )2 |SCF − ψ0 |(ni )2 |ψ0 SCF |(ni )2 |SCF

(1.3)

where ni = ni − n¯ i and n¯ i denotes the average value. One notices that 0 (i) 1. When (i) = 0 the interatomic correlations vanish, i.e., the Coulomb repulsions between the electrons can be treated in mean-field approximation. In a solid atoms or ions with strongly correlated electrons have (i) values near unity. One can also define a correlation strength for different bonds instead of atoms. In that case the denominator is modified when heteropolar bonds are considered. Then we must subtract from SCF |(ni )2 |SCF a term (n)2pc . It takes into account that some number fluctuations are required even when the electrons are perfectly correlated in order to ensure a heteropolar charge distribution within

STRONGLY CORRELATED ELECTRONS

5

the bond. Let αp denote the bond polarity. It is defined by the difference in the average occupation numbers of the two half-bonds 1 and 2 which form the heteropolar bond, i.e., n¯ 1(2) = (1 ± αp ). In that case (n)2pc = αp (1 − αp ). Those considerations apply to a solid as well as to a molecule. For the H2 molecule one checks immediately that approximating |ψ0 by ψMO (r1 , r2 ) gives = 0 while a replacement by ψHL (r1 , r2 ) yields = 1 since ψ0 |(n)2 |ψ0 = 0 in that case. For a C=C or N=N π bond one finds ≈ 0.5 while for a C–C or N–N σ bond = 0.30 and 0.35, respectively. Let us consider the ground state of La2 CuO4 and let P (dν ) denote the probability of finding ν 3d electrons on a given Cu site. Within the independent electron or Hartree–Fock approximation the average d count is found to be n¯ d 9.5 and the probabilities of different configurations are P (d10 ) = 0.56, P (d9 ) = 0.38 and P (d8 ) = 0.06. When correlations are included, i.e., the correlated ground state |ψ0 is used the average d electron number changes to n¯ d 9.3 and P (d10 ) = 0.29, P (d9 ) = 0.70 while P (d8 ) = 0.0. One notices that the d8 configurations are almost completely suppressed in agreement with photoemission experiments. The fluctuations between the d9 and d10 configurations are fixed by the value of n¯ d . A similar analysis for the oxygen atoms reveals that there the 2p4 configurations are not completely suppressed because the Coulomb integrals are not as large as for Cu. Indeed, these configurations are important for superexchange to occur, which determines the antiferromagnetic coupling between Cu ions. In accordance with the above consideration one finds (Cu) 0.8 and (O) 0.7.14 So indeed, correlations are quite strong in La2 CuO4 . On the other hand, they are still smaller than those of 4f electrons in a system like CeAl3 . A measure for the strength of intra-atomic correlations is more difficult to define. One way is by finding out to which extent Hund’s rule correlations are building up on a given atomic site i. A possible measure for that is the degree of spin alignment at a given atomic site i (1.4) Si2 = ψ0 S2 (i)ψ0 where S(i) = ν sν (i) and sν (i) is the spin operator for orbital ν. The quantity Si2 should be compared with the values when the SCF ground-state wavefunction |SCF is used and when instead the ground state |loc in the limit of complete suppression of interatomic charge fluctuations is taken, i.e., for large atomic distances. Therefore we may define Si2 =

ψ0 |S2 (i)|ψ0 − SCF |S2 (i)|SCF loc |S2 (i)|loc − SCF |S2 (i)|SCF

14 A. Ole´s, J. Zaanen, and P. Fulde, Physica B 148, 260 (1987).

(1.5)

6

P. FULDE ET AL.

as a possible measure of the strength of intra-atomic correlations. Note that 0 Si2 1. For example, for the transition metals Fe, Co and Ni Si2 is approximately 0.5. Those findings show that the much discussed transition metals are just in the middle between the limits of uncorrelated and strongly correlated electrons. Hund’s rule correlations are important in them but relatively large overlaps of atomic wavefunctions on neighboring sites prevent their complete establishment. Starting from the work of Slater15 and Van Vleck16 in particular Friedel,17 Gutzwiller,18,19 Hubbard20 and Kanamori21 have discussed their effects in detail. One of the outcomes of the studies of transition metals is the Hubbard Hamiltonian. It was in fact used independently also by Gutzwiller and in a slightly modified version by Kanamori. This Hamiltonian was extensively treated in various approximations. The multiband Hubbard model has remained until present times the working horse of many studies of strongly correlated electrons.22,23 The shortcomings of that model are known. For example, it considers d electrons only, i.e., s electrons are neglected. Also it cannot provide for orbital relaxations when electrons hop on or off a site because only one basis function per atomic orbital is used. Nevertheless, it is believed that it covers the most important generic effects of strongly correlated electrons. The valence electrons which are most strongly correlated are the 4f ones because their atomic wavefunction is close to the nucleus and the tendency to delocalize is very small. In fact, in intermetallic rare-earth compounds only f -electrons in Ce or Yb ions show a noticeable degree of itineracy. The consequence are new low-energy scales which may appear in those compounds and as a result heavy-quasiparticle excitations. Not always do quasiparticles show conventional Fermi liquid behavior which governs the low-temperature thermodynamic properties of many metals. In a number of cases one observes what is called non-Fermi liquid behavior, i.e., quantities like the temperature dependence of the specific heat or of the susceptibility deviate from normal metallic behavior. In particular this holds true near a quantum critical point where apparently no characteristic energy scale is prevailing. Fermi liquid behavior requires that at low temperatures all thermodynamic quantities scale with kB T ∗ , a characteristic energy which in 15 J. C. Slater, Phys. Rev. 49, 537 and 931 (1936). 16 J. H. V. Vleck, Rev. Mod. Phys. 25, 220 (1953). 17 J. Friedel, The Physics of Metals: 1. Electrons, Cambridge Univ. Press, Cambridge (1969). 18 M. C. Gutzwiller, Phys. Rev. A 134, 923 (1964). 19 M. C. Gutzwiller, Phys. Rev. A 137, 1726 (1965). 20 J. Hubbard, Proc. R. Soc. London A 281, 401 (1964). 21 J. Kanamori, Progr. Theor. Phys. 30, 275 (1963). 22 M. Imada, A. Fujimori, and Y. Tokura, Rev. Mod. Phys. 70, 1039 (1998). 23 F. Mancini and A. Avella, Adv. Phys. 53, 537 (2004).

STRONGLY CORRELATED ELECTRONS

7

strongly correlated electron systems takes the role of the Fermi energy. When such a characteristic scale does not exist deviations from Fermi liquid behavior do occur. In a way it is more astonishing that to good approximation Fermi liquid behavior is observed in a number of strongly correlated electron systems than that it is not. A study of the Hubbard model shows ways for obtaining deviations from standard features of a metal. One interesting aspect of strong electron correlations is the possible occurrence of charge order. A charge ordered state minimizes the repulsive energy between electrons at the expense of the kinetic energy. Wigner was the first to study this subject by considering a homogeneous electron gas and specifying the conditions under which the formation of an electronic lattice is possible. Chances for charge ordering are larger for inhomogeneous systems, i.e., lattices than for homogeneous ones, the reason being that the kinetic energy gain of electrons due to delocalization may become very much reduced as compared with homogeneous electron systems. A prototype example is Yb4 As3 where charge order occurs close to room temperature and there are many other cases. While 4f electrons are localized in most cases and are very strongly correlated, 5f electrons are more delocalized but still more strongly correlated as, e.g., 3d electrons in transition metals. It turns out that in this case a dual picture applies: while 5f electrons become itinerant in some of the orbitals they remain localized in others. Such a model explains very well a number of experiments on U compounds. Heavy quasiparticles have also been observed in LiV2 O4 , a metal with 3d electrons. A special feature of that material is that the 3d electrons are placed on a pyrochlore or geometrically frustrated lattice. Model calculations show that charge degrees of freedom of strongly correlated electrons in frustrated lattice structures can give rise to new phenomena at special band fillings. There may exist large numbers of low-energy excitations for which Landau’s Fermi liquid approach fails and there may be even excitations with fractional electron charges. Although phenomena of this kind have not been observed yet, the theoretical results may stimulate further thinking. Strongly correlated electrons show in addition to the quasiparticle bands also satellite structures in photoemission experiments. They are contained in the incoherent part of the one-particle Green function. It appears that detailed studies of the incoherent part of Green’s function have not been done to the extent they deserve. The reason for their importance is the following. A quasiparticle in a solid can be considered as a bare particle (electron or hole) surrounded by a correlation hole. The whole object, i.e., particle plus correlation hole moves in form of a Bloch wave through the system. The internal degrees of freedom of the correlation hole give rise to excitations which are contained in the incoherent part of Green’s function. Therefore it is very instructive to study general features of

8

P. FULDE ET AL.

that incoherent part. Hubbard’s upper band can be considered a satellite feature for filling factors n < 1/2, i.e., for less than one electron per site. Other examples will be presented. It is impossible to cover all aspects of strongly correlated electrons in a review of reasonable size. Therefore selections have to be made. Naturally, authors select topics for reviews for which they feel particularly competent. These are usually areas in which they have actively worked. This holds also true here and the selection we made may do injustice to other interesting developments in fields not covered here. So we apologize for an incomplete covering of topics as well as for incomplete lists of contributions of authors to the subjects discussed here. II. Special Features of Strong Correlations

Metals with strongly correlated electrons exhibit characteristic deviations from the behavior of independent electrons. The latter are reflected in thermodynamic and transport properties as well as in the high energy spectra. Traditional electron theory of metals proceeds from the electron gas model formulated by Sommerfeld and Bethe.24 The electrons are described as a system of non-interacting fermions. The eigenstates are formed by filling single-particle levels in a manner consistent with the Pauli principle which permits at most one electron per spin direction to occupy any single-electron level. The ground state of an N electron state is obtained by filling the N/2 single particle levels with the lowest energies. It is non-degenerate and characterized by a surface in k-space separating the occupied levels from their unoccupied counterparts. The existence of this surface, the Fermi surface, follows directly for a system of independent electrons. But note that the observation of a Fermi surface does not imply that the independent electron approximation is a valid description of a system. The lowtemperature properties which are dominated by the low-energy excitations are universal, the detailed character of the system under consideration being reflected in a characteristic energy—the Fermi energy EF . The energy scale is set by the variation of the single particle levels with wave number k. A measure of it is the Fermi velocity vF . The linear variation with temperature of the specific heat, C(T ) γ T , and the temperature-independent magnetic susceptibility, χs (T ) → const are also characteristic features of free electrons. Finally, the spectrum for adding or removing a particle in a single-particle level k, σ to the ground state A(k, ω), exhibits a well-defined peak A(k, ω) = δ(ω − k )

(2.1)

24 A. Sommerfeld and H. Bethe, Elektronentheorie der Metalle, vol. 24/2 of Handbuch der Physik,

Springer, Berlin, Heidelberg (1933), 2nd ed.

STRONGLY CORRELATED ELECTRONS

9

of weight unity centered at the single-particle energy k . The independent electron model has proven to be very successful in explaining experimentally observed properties of simple metals. That was a surprise for some time since electron– electron repulsions are not weak in any metal and one might therefore expect that they modify strongly the properties of a system of independent electrons. That this is not necessarily the case was shown by Landau.25–28 The Landau theory assumes that there exists a one-to-one correspondence between the excitations of the complex interacting electron system and those of independent electron. The former are called quasiparticles and their orbitals and energies E(k) are determined from an effective Hamiltonian. It contains an effective, not necessarily local potential. The many-body aspects are contained in the construction of the effective potential which must be determined specifically for the problem under consideration. The quasiparticle energies may be altered when the overall configuration is changed. A characteristic feature of interacting Fermi liquids is that the energy dispersion E˜ σ (k) of a quasiparticle depends on how many other quasiparticles are present,

E˜ σ (k) = E(k) + fσ σ (k, k )δnσ (k ). (2.2) k σ

Here E(k) denotes the energy dispersion of a quasiparticle when there are no other quasiparticles around (dilute gas limit). In systems with strong correlations it reflects the electron interactions and hence cannot be calculated from the overlap of single-electron wave functions. Interactions among quasiparticles are characterized by the matrix fσ σ (k, k ). The deviations from a step-function-like Fermi distribution f (E(k), T = 0) are given by δnσ (k). The scattering amplitudes fσ σ (k, k ) are parameterized and the parameters are adjusted to experiments. Their form is strictly applicable only to a homogeneous translationally invariant electron system. Therefore applying it to an inhomogeneous periodic solid requires some modifications (see, e.g., Ref. [29]) which are usually not discussed. From this point of view Landau’s theory is more of a useful theoretical concept rather than a quantitative computational scheme. The assumed one-to-one correspondence of the excitations implies that the low temperature thermodynamic properties resemble those of independent electrons but with renormalized parameters such as the effective electron or hole 25 L. D. Landau, Zh. Eksp. Teor. Fiz. 30, 1058 (1956). 26 L. D. Landau, Zh. Eksp. Teor. Fiz. 32, 59 (1957). 27 L. D. Landau, Zh. Eksp. Teor. Fiz. 35, 97 (1958). 28 A. A. Abrikosov, L. P. Gorkov, and I. E. Dzyaloshinski, Methods of Quantum Field Theory in

Statistical Physics, Prentice-Hall, Englewood Cliffs, New York (1963). 29 P. Fulde, J. Keller, and G. Zwicknagl, in Solid State Physics, vol. 41, eds. H. Ehrenreich and

D. Turnbull, Academic Press, New York (1988), p. 1.

10

P. FULDE ET AL.

mass. Also the weight of the peak in the spectral density A(k, ω) is modified to Z · δ(ω − E(k)) where the renormalization factor 0 < Z 1 describes the weight of the bare electron in the quasiparticle. The latter contains in addition to the bare electron also the correlation hole around it. An interacting electron system to which Landau’s theory applies has also a Fermi surface. Luttinger has proven30 that in case that perturbation theory is applicable the volume enclosed by the Fermi surface is independent of the electron interactions. Another important property of quasiparticles is that they can be considered as ‘rigid’ with respect to low-energy and long-wavelength perturbations. That is to say that excitations involving degrees of freedom of the correlation hole show up at high energies only and are neglected as regards low-temperature properties. They are discussed in Section VIII. When electron correlations are strong the quasiparticle concept is still applicable for a number of substances. In that case the renormalization factor Z may become very small. This results in heavy quasiparticles because the Fermi velocity is reduced by the same factor. Probably in many cases the one-to-one correspondence between the excitations of a strongly correlated electron system and a corresponding system of independent electrons is only approximately fulfilled. But then the low-temperature properties of the system may still look very similar to those of independent electrons with renormalized parameters. For example, the specific heat will still be nearly linear in T at low temperatures etc. However, we want to stress that from the observation of a specific heat linear in T or a temperature independent spin susceptibility in the low temperature regime one may not conclude that the quasiparticle picture is applicable. In fact, Luttinger liquids in quasi-one-dimensional systems show many properties as quasiparticles do. This is so despite the fact that the key assumption of a one-toone correspondence of excitations to those of independent electrons is unjustified here. There are strongly correlated systems where the quasiparticle picture seems totally inappropriate. This is outlined in the following Section II.2 and discussed in more detail in various sections of this chapter. 1. L OW-E NERGY S CALES : A S IGNATURE OF S TRONG C ORRELATIONS As mentioned above, the characteristic energy scale of a free electron gas is the Fermi energy EF or, alternatively the Fermi temperature TF . A typical value for EF is 5 eV corresponding to a TF of 5 · 104 K. A special feature of strongly correlated electrons is that they introduce new low-energy scales. It is customary to associate a temperature T ∗ with them. In metals with heavy quasiparticles, i.e., with very strong electron correlations T ∗ ranges from a few Kelvin to a few 30 J. M. Luttinger and J. C. Ward, Phys. Rev. 118, 1417 (1960).

STRONGLY CORRELATED ELECTRONS

11

hundred Kelvin. As correlations become weaker T ∗ increases until it is no longer justified to speak of a separate low-energy scale. The microscopic origin of the low-energy scales can be quite different. A widely recognized case is the Kondo effect. Here T ∗ is the Kondo temperature, i.e., it is given by the binding energy of the spins of the conduction electrons to local spins. Local spins imply incomplete inner shells of an atom or ion. The fact that they remain partially filled only, when surrounded by conduction electrons is due to strong correlations. Any conduction electron which tries to enter the incomplete inner shell is expelled by strong on-site Coulomb repulsion. An example are Ce3+ ions immersed in a sea of (generally) weakly correlated conduction electron. Due to a weak hybridization the number of 4f electrons is nearly one. It forms a singlet with the conduction electrons. The aforementioned CeAl3 falls into that category. Breaking those singlets results in low-energy excitations and fixes the low-energy scale T ∗ . The lowenergy excitations make it plausible that there will be a large low-temperature specific heat. To explain heavy quasiparticles the singlet-triplet excitations on different sites must lock together and form coherent Bloch-like excitations. That takes place at a somewhat lower energy scale Tcoh . One expects that Tcoh is of order of T ∗ but no detailed theory for a relation between the two temperatures is available. There is also no theory existing which tells us that the coherent excitations are in one-to-one correspondence to excitations of (nearly) free electrons. Nevertheless this assumption has worked remarkably well. The origin of a low T ∗ is quite different in the strongly correlated semimetal Yb4 As3 . Here the Coulomb repulsion of the 4f holes in neighboring Yb ions leads to charge order in the form of well separated chains of Yb3+ ions. Spin excitations in those chains by which light mobile 4p holes of As are scattered, lead to low temperature properties which resemble very much those of other systems with heavy quasiparticles.31,32 Despite of this the system is not really a heavy Landau Fermi liquid any more as is explained in the next subsection and discussed in more detail in Section VI.13. A third mechanism is found to be responsible for a low energy scale T ∗ in U compounds like UPd2 Al3 or UPt3 . Strong intra-atomic or Hund’s rule correlations lead here to pronounced anisotropies of the effective hybridization of different 5f orbitals. As a result some of the 5f electrons remain localized while others delocalize. The crystalline environment lifts degeneracies of the localized electrons on a low energy scale. The delocalized or itinerant electrons couple to the excitations of the local system and in this way generate a low T ∗ .33 Heavy quasiparticles may also appear near a quantum critical point like in YMn2 .34 31 P. Fulde, B. Schmidt, and P. Thalmeier, Europhys. Lett. 31, 323 (1995). 32 M. Kohgi, K. Iwasa, J.-M. Mignot, A. Ochiai, and T. Suzuki, Phys. Rev. B 56, R11388 (1997). 33 G. Zwicknagl and P. Fulde, J. Phys.: Condens. Matter 15, S1911 (2003). 34 C. Pinettes and C. Lacroix, J. Phys. Cond. Mat. 6, 10093 (1994).

12

P. FULDE ET AL.

Finally, in Ce doped Nd2 CuO4 a fourth origin of a low T ∗ is observed. Here it is essentially a fluctuating internal molecular field originating from the Nd ions which causes a low energy scale in the strongly correlated d-electron system of the Cu–O planes to which is couples.35,36 It seems obvious that there will be other physical processes identified in the future resulting in low-energy scales of strongly correlated electron systems. 2. D EVIATIONS FROM F ERMI -L IQUID B EHAVIOR There is no obvious reason why strongly correlated metallic electron systems should be Fermi liquids. But as pointed out above a large number of them behave very nearly like ordinary metals, i.e., Fermi liquids with renormalized parameters like the effective mass. Even in these cases, high energy excitations show characteristic satellite structures which reflect strong correlations in partially filled inner shells. This topic is discussed in Section VIII. However, there are also numerous examples where the Fermi liquid concept for low-energy excitations is not applicable. One much discussed item is the separation of charge and spin degrees of freedom and moreover the appearance of fractional charges. Separate spin and charge excitations occur always when electron correlations are so strong that the electrons remain localized. In that case the coupling of spins on different sites leads to magnetic excitations with energies of order J , the intersite coupling constant. In contrast, charge excitations from the partially filled inner shells as observed, e.g., by photoelectron spectroscopy have much higher energies. But this kind of spin-charge separation is trivial and does not require further consideration. It is well known that in one dimension (1D) spin and charge degrees of freedom lead to different kinds of excitations even when the correlations are weak (Luttinger liquid). For a review see, e.g., Ref. [37]. Spin-charge separation is also found for kink excitations (solitons) in polyacethylene.38 Those excitations exist even within the independent electron approximation, but require inclusion of lattice degrees of freedom. Doped polyacethylene can have also excitations with fractional charges, again within the one-electron picture but requiring lattice (chain) deformations.39 In 2D electron correlations, e.g., in semiconducting inversion layers may become strong when a magnetic field is applied perpendicular to the 35 T. Brugger, T. Schreiner, G. Roth, P. Adelmann, and G. Czjzek, Phys. Rev. Lett. 71, 2481 (1993). 36 P. Fulde, V. Zevin, and G. Zwicknagl, Z. Phys. B 92, 133 (1993). 37 A. O. Gogolin, A. A. Nersesyan, and A. N. Tsvelik, Bosonization and Strongly Correlated Systems,

Cambridge University Press, Cambridge (1998). 38 W. P. Su, J. R. Schrieffer, and A. J. Heeger, Phys. Rev. Lett. 42, 1698 (1979). 39 W. P. Su and J. R. Schrieffer, Phys. Rev. Lett. 46, 738 (1981).

STRONGLY CORRELATED ELECTRONS

13

plane. The kinetic energy of the electrons is strongly reduced in a high field and therefore the Coulomb repulsions become dominant. This results in the fractional quantum Hall effect (FQHE) and quasiparticles with fractional charges.40 Thus in two dimensions electron correlations are essential for the appearance of fractional charges. The same holds true for 3D systems. There it turns out that excitations with fractional charges may exist in certain geometrically frustrated lattice structures like the pyrochlore lattice.41,42 There is also spin-charge separation. A Fermi liquid description is inapplicable here. This intriguing possibility is discussed in Section VII. Another interesting case of a breakdown of Landau’s Fermi liquid description is found in Yb4 As3 . This system is metallic in a high temperature phase and semimetallic in the low temperature phase.32,43 The change is related to a partial electronic charge order in form of well separated Yb3+ chains with an effective spin 1/2 per site. It is well known that a Heisenberg spin chain has a specific heat of the form C = γ T like a metal. It is due to spinons which obey Fermi statistics. The reader should note that in one dimension one can convert fermions into bosons and vice versa.44 The coefficient γ is large here because of a weak coupling of the spins in a chain and therefore the specific heat resembles that of heavy quasiparticles.31 But the charge carriers, which are mainly 4f holes in the high temperature phase consist of a small number of As 4p holes in the low temperature phase.45 Therefore one may speak of spin-charge separation and a breakdown of the conventional Fermi liquid picture. The one-to-one correspondence between the excitations in the low temperature phase and those of an independent electron system is no longer given. Nevertheless the system shows many properties of an ordinary metal with heavy quasiparticles at low temperature. A detailed discussion of that interesting material is found in Section VI. Another form of deviation from classical Fermi liquid behavior is found in the cuprates perovskite structures. In the underdoped regime many of their physical properties show marginal Fermi liquid behavior.46,47 This implies that they can be described by assuming a frequency dependence of the electron self-energy (ω) for small values of ω of the form Re (ω) ∼ ω ln ω,

Im (ω) ∼ |ω|

(2.3)

40 R. B. Laughlin, Phys. Rev. Lett. 50, 1395 (1983). 41 P. Fulde, Adv. Physics 51, 909 (2002). 42 E. Runge and P. Fulde, Phys. Rev. B 70, 245113 (2004). 43 A. Ochiai, T. Suzuki, and T. Kasuya, J. Phys. Soc. Jpn. 59, 4129 (1990). 44 A. Luther and I. Peschel, Phys. Rev. B 12, 3908 (1975). 45 V. N. Antonov, A. N. Yaresko, A. Y. Perlov, P. Thalmeier, P. Fulde, P. M. Oppeneer, and H. Eschrig,

Phys. Rev. B 58, 9752 (1998). 46 C. M. Varma, P. B. Littlewood, S. Schmitt-Rink, E. Abrahams, and A. Ruckenstein, Phys. Rev. Lett.

63, 1996 (1989). 47 P. B. Littlewood and C. M. Varma, J. Appl. Phys. 69, 4979 (1991).

14

P. FULDE ET AL.

instead of the Fermi-liquid form Re (ω) ∼ ω,

Im (ω) ∼ ω2 .

(2.4)

The latter would be required for the one-to-one correspondence of the excitations. The relations (2.3) hold only for T < ω. Otherwise T replaces ω. They yield, e.g., a resistivity ρ(T ) ∼ T as is observed in a number of the strongly correlated cuprates. The microscopic origin of marginal Fermi liquid behavior in the presence of strong electron correlations has been an open problem. It is also unclear down to which small ω (or T ) values the relations (2.3) must hold in order to explain the relevant experiments. It is shown in Section VIII that marginal Fermi liquid behavior is obtained for a certain parameter range of the Hubbard Hamiltonian on a square lattice near half filling when the one-site Coulomb repulsions dominate. Last but not least, non-Fermi liquid behavior is also found near a quantum critical point (QCP). It is a point in parameter space at which the system would undergo a phase transition at T = 0, if we were able to reach the limit of zero temperature. In that case quantum fluctuations instead of thermal fluctuations determine the critical behavior of the system. It is intuitively obvious that near a QCP the conventional Fermi liquid description breaks down since the self-energy is no longer expected to be of the form (2.4). Instead, quantum fluctuations down to arbitrary low wave numbers will modify this form. The scattering length of electrons diverges at a QCP while it must remain finite for a Fermi liquid. It should be emphasized that those features do not require strong electron correlations but appear also at QCPs of weakly correlated systems. An example of the latter case is the theory of Moriya48 (see also Ref. [49]) for the resistivity near a QCP of a weak ferromagnet. Quantum critical points are discussed in Section IV. III. Kondo Lattice Systems

The Kondo Hamiltonian describes magnetic impurities with free spins embedded in a metal and interacting with metal electrons via exchange scattering. The key ingredient is an antiferromagnetic interaction term Hint = J s(0) · S,

J > 0,

(3.1)

where S and s(0) are the S = 1/2 impurity spin and the conduction electron spin density at the impurity site which is taken here to be the origin. The model explains the characteristic Kondo behavior in dilute magnetic alloys which is determined by the phenomena of asymptotic freedom and confinement. They give 48 T. Moriya and A. Kawabata, J. Phys. Soc. Jpn. 34, 639 (1973). 49 K. K. Murata and S. Doniach, Phys. Rev. Lett. 29, 285 (1972).

STRONGLY CORRELATED ELECTRONS

15

rise to anomalies in the variation with temperature of equilibrium and transport properties and the “quenching” of the magnetic moment at low temperatures. The presence of a highly complex many-body ground state is highlighted by the breakdown of conventional perturbation theory which starts from free electrons and magnetic moments. The divergence of the conduction electron scattering matrix sets the low-energy characteristic scale kB TK where TK is usually referred to as the Kondo temperature. Microscopically it arises because the local degeneracy associated with the magnetic ion is removed through the exchange coupling between the conduction electrons and the impurity spin. The coupling leads to the formation of a singlet ground state and low-energy excitations which can be described in terms of a local Fermi liquid. In close analogy to confinement the local quasiparticles are composite objects formed by conduction electrons and magnetic degrees of freedom. The problem of magnetic impurities is well understood theoretically. There is a wide variety of techniques available which allow for an accurate description of the impurity contributions to physical properties. For detailed discussion, we refer to50–52 and references therein. Challenging problems are posed by work on concentrated systems, in particular on Ce-based compounds with heavy quasiparticles (heavy-fermion systems). At first glance these systems share many properties with dilute magnetic alloys. Those materials differ from ordinary metals in that there exists a characteristic temperature scale T ∗ 10–100 K, that is much smaller than the usual Fermi temperatures in ordinary metals, on which the electronic behavior of the compounds changes drastically. In the high-temperature regime for T T ∗ the systems behave like ordinary magnetic rare-earth systems which have itinerant conduction electrons with conventional masses and well-localized f -electrons. This picture is derived from the temperature dependence of the specific heat which exhibits pronounced Schottky anomalies corresponding to crystalline electric field (CEF) excitations. In addition, the magnetic susceptibility is Curie–Weiss-like reflecting the magnetic moment of the partially filled f -shell in a CEF. The low-temperature behavior, however, observed for T T ∗ is highly unusual and rather surprising: The specific heat varies approximately linearly with temperature (that is C = γ T + · · ·), and the magnetic susceptibility, χs , approaches a Pauli-like form, becoming almost independent of temperature. Values of the coefficients γ are of the order of J/mol K2 and consequently two to three orders of magnitude larger than those of ordinary metals 50 A. C. Hewson, The Kondo Problem to Heavy Fermions, Cambridge University Press (1993). 51 Y. Kuramoto and Y. Kitaoka, Dynamics of Heavy Electrons, vol. 105 of International Series of

Monographs in Physics, Clarendon Press, Oxford (2000). 52 D. L. Cox and A. Zawadowski, Exotic Kondo Effects in Metals: Magnetic Ions in a Crystalline

Electric Field and Tunnelling Centres, Taylor and Francis (1999).

16

P. FULDE ET AL. 2

which are of the order of π2 N kB T1F mJ/mol K2 . In addition, the magnetic susceptibility χs is enhanced by a factor of comparable magnitude. A recent survey of the experimental properties can be found in Refs. [53,54] and references therein. The similarities in the behavior of Ce-based heavy-fermion systems to that of dilute magnetic alloys have led to the assumption that these systems are “Kondo lattices” where the observed anomalous behavior can be explained in terms of periodically repeated resonant Kondo scattering. This ansatz provides a microscopic model for the formation of a singlet ground state and the appearance of a small energy scale characterizing the low-energy excitations. The Kondo picture has been confirmed by the observation of the Kondo resonance which forms at low temperatures.55 In contrast to the impurity case the Kondo model cannot be solved for a periodic lattice of magnetic ions. A major difficulty is the competition between the formation of (local) Kondo singlets and the lifting of degeneracies by long-range magnetic order. In the high-temperature regime the moments of the Ce 4f -shells are coupled by the RKKY interaction which can favor parallel as well as antiparallel orientation of the moments at neighboring sites. Model calculations for two Kondo impurities56–58 showed that antiferromagnetic correlations between the magnetic sites weaken the Kondo singlet formation reducing the characteristic energy scale kT ∗ to rather small values. Consequences for an extended lattice will be discussed in the subsequent section on Quantum Phase Transitions. The general difficulties in understanding the low temperature properties of Kondo lattices seem partially due to the lack of an adequate common “language” for the two regimes where local singlet formation is dominating on one side and where the magnetic intersite interactions dominate on the other. Such a language is usually provided by a mean-field theory which maps the complex quantum problem onto an appropriate classical model. In the case of the Kondo lattice separate mean-field descriptions exist for the two regimes which cannot be reconciled in a straightforward way to provide a unified approach. In the present section we focus on the heavy Fermi liquid regime. The corresponding mean-field theory was described, e.g., in Ref. [29] and references 53 P. Thalmeier and G. Zwicknagl, in Handbook of the Physics and Chemistry of Rare Earth, vol. 34,

eds. K. A. Gschneider, Jr., J.-C. Bünzli, and V. Pecharsky, Elsevier, Amsterdam (2005), p. 135. 54 P. Thalmeier, G. Zwicknagl, O. Stockert, G. Sparn, and F. Steglich, in Frontiers in Superconducting

Materials, Springer, Berlin (2005), p. 109. 55 F. Reinert, D. Ehm, S. Schmidt, G. Nicolay, S. Hüfner, J. Kroha, O. Trovarelli, and C. Geibel, Phys.

Rev. Lett. 87, 106401 (2001). 56 C. Jayprakash, H.-R. Krishna-murthy, and J. W. Wilkins, Phys. Rev. Lett. 47, 737 (1981). 57 C. Jayprakash, H.-R. Krishna-murthy, and J. W. Wilkins, J. Appl. Phys. 53, 2142 (1982). 58 B. Jones and C. M. Varma, J. Magn. Magn. Mater. 63 & 64, 251 (1987).

STRONGLY CORRELATED ELECTRONS

17

therein. The majority of recent microscopic studies of the Kondo lattice adopted the Dynamical Mean Field Theory which—by construction—explicitly neglects the subtle magnetic intersite correlations. It accounts for the complex local dynamics in terms of a local self-energy which has to be determined selfconsistently. The applications include model calculations and a study of the γ -αtransition in Ce.59 A major restriction on the general validity is imposed by the fact that the 4f valence has to be kept fixed at unity, i.e., nf = 1, throughout the calculation. The novel feature observed in stoichiometric Ce-compounds is the formation of narrow coherent bands of low-energy excitations. They give rise to the temperature dependence of the electrical resistivity which approximately follows ρ(T ) = ρ0 + AT 2 . While these findings unambiguously show that the low-energy excitations are heavy quasiparticles involving the f degrees of freedom, they nevertheless do not provide conclusive information on how the latter have to be incorporated into a Fermi liquid description. A characteristic property of a Fermi liquid is the existence of a Fermi surface whose volume is determined by the number of itinerant fermions. It is rather obvious that at high temperatures the f electrons should be excluded from the Fermi surface due to their apparent localized character. The latter, however, is lost at low temperatures. The conjecture that the f -degrees of freedom have to be treated as itinerant fermions and, consequently, have to be included in the Fermi surface was met with great scepticism.60 This hypothesis implies that the strong local correlations in Kondo lattices lead to an observable many-body effect, i.e., a change with temperature of the volume of the Fermi surface. At high temperatures, the f -degrees of freedom appear as localized magnetic moments, and the Fermi surface contains only the itinerant conduction electrons. At low temperatures, however, the f degrees of freedom are now tied into itinerant fermionic quasiparticle excitations and accordingly, have to be included in the Fermi volume following Luttinger’s theorem. Consequently the Fermi surface is strongly modified. This scenario61,62 was confirmed experimentally by measurements of the de Haas–van Alphen (dHvA) effect63–65 and recent photoemission studies.66,67 59 A. K. McMahan, K. Held, and R. T. Scalettar, Phys. Rev. B 67, 075108 (2003). 60 T. Kasuya, Prog. Theor. Phys. Supplement 108, 1 (1992). 61 G. Zwicknagl, Physica Scripta T 49, 34 (1993). 62 P. Fulde, in Narrow Band Phenomena: Infuence of Electrons with both Band and Localized Char-

acter, eds. J. C. Fuggle, G. A. Sawatzky, and J. Allen, Plenum (1988). 63 G. G. Lonzarich, J. Magn. Magn. Mat. 76–77, 1 (1988). 64 H. Aoki, S. Uji, A. K. Albessard, and Y. Onuki, Phys. Rev. Lett. 71, 2110 (1993). 65 F. S. Tautz, S. R. Julian, G. J. McMullen, and G. G. Lonzarich, Physica B 206–207, 29 (1995). 66 J. D. Denlinger, G.-H. Gweon, J. W. Allen, C. G. Olson, Y. Daliachaouch, B.-W. Lee, M. B. Maple, Z. Fisk, P. C. Canfield, and P. E. Armstrong, Physica B 281 & 282, 716 (2000). 67 J. D. Denlinger, G.-H. Gweon, J. W. Allen, C. G. Olson, M. B. Maple, J. L. Sarrao, P. E. Armstrong, Z. Fisk, and H. Yamagami, J. Electron Spectrosc. Relat. Phenom. 117 & 118, 347 (2001).

18

P. FULDE ET AL.

The present section is mainly devoted to the theoretical description of the Fermi liquid state at low temperatures. We briefly introduce the renormalized band scheme which has been devised for calculating realistic quasiparticle bands of real materials. This is achieved by combining ab initio electronic structure methods and phenomenological concepts in the spirit of Landau theory. Concerning the applications we shall not elaborate on the results for the Fermi surface and anisotropic effective masses in CeRu2 Si2 for which we refer to.61,68 We rather present recent results concerning the instabilities of the Fermi liquid state in CeCu2 Si2 . We would like to emphasize the predictive power of the renormalized band method. In both cases mentioned above (Fermi surface of CeRu2 Si2 and SDW instability in CeCu2 Si2 ) the effects were first calculated theoretically and later confirmed experimentally—sometimes with a delay of up to several years. 3. F ERMI -L IQUID S TATE AND H EAVY Q UASIPARTICLES : R ENORMALIZED BAND T HEORY The energy dispersion E(k) of a dilute gas of noninteracting quasiparticles is parameterized by the Fermi wave vector kF and the Fermi velocity vF ˆ · (k − kF ) E(k) = vF (k)

(3.2)

where kˆ denotes the direction on the Fermi surface. The key idea of the renormalized band method is to determine the quasiparticle states by computing the band structure for a given effective potential. Coherence effects which result from the periodicity of the lattice are then automatically accounted for. The quantities to be parameterized are the effective potentials which include the many-body effects. The parameterization of the quasiparticles is supplemented by information from conventional band structure calculations as they are performed for “ordinary” metals with weakly correlated electrons. The periodic potential leads to multiplescattering processes involving scattering off the individual centers as well as to propagation between the centers which mainly depends on the lattice structure and is therefore determined by geometry. The characteristic properties of a given material enter through the information about single-center scattering which can be expressed in terms of a properly chosen set of phase shifts {ηνi (E)} specifying the change in phase of a wave incident on site i with energy E and symmetry ν with respect to the scattering center. Within the scattering formulation of the band structure problem the values of the phase shifts at the Fermi energy {ηνi (EF )} together with their derivatives {(dηνi /dE)EF } determine the Fermi wave vectors kF and the Fermi velocity vF . 68 G. Zwicknagl, Adv. Phys. 41, 203 (1992).

STRONGLY CORRELATED ELECTRONS

19

A detailed description of the renormalized band method is given in Ref. [68]. The first step is a standard LDA band-structure calculation by means of which the effective single-particle potentials are self-consistently generated. The calculation starts, like any other ab initio calculation, from atomic potentials and structure information. In this step, no adjustable parameters are introduced. The effective potentials and hence the phase shifts of the conduction states are determined from first principles to the same level as in the case of “ordinary” metals. The f -phase shifts at the lanthanide sites, on the other hand, are described by a resonance type expression η˜ f arctan

˜f E − ˜f

(3.3)

which renormalizes the effective quasiparticle mass. One of the two remaining ˜ f is eliminated by imposing the condition that the free parameters ˜f and charge distribution is not significantly altered as compared to the LDA calculation by introducing the renormalization. The renormalized band method devised to calculate the quasiparticles in heavy-fermion compounds thus is essentially a one-parameter theory. We mention that spin-orbit and CEF splittings can be accounted for in a straightforward manner.68 4. H EAVY F ERMIONS IN C E RU 2 S I 2 AND C E C U 2 S I 2 The archetype heavy fermion superconductor CeCu2 Si2 as well as CeRu2 Si2 crystallize in the tetragonal ThCr2 Si2 structure. The unit cell is shown in Figure III.1.

F IG . III.1. Conventional unit cell of the ThCr2 Si2 and CeM2 X2 structure where M = Cu, Ni, Ru, Rh, Pd, Au, . . . and X = Si, Ge.

20

P. FULDE ET AL.

To study the electronic structure, we compare the results of two different models, i.e., treating the Ce 4f degrees of freedom as localized (atomic like) states and as delocalized yet strongly renormalized electrons. The first procedure provides a good quantitative description of the properties at elevated temperatures, high excitation energies, and above the metamagnetic transition. The latter ansatz yields a model for the Fermi liquid state. The low-temperature behavior of CeRu2 Si2 is well described by a paramagnetic Fermi liquid with weak residual interactions. The relevant low-energy excitations are heavy quasiparticles as inferred from the linear specific heat coefficient γ 350 mJ/mol K2 .69 In the local moment regime, the Fermi surface is determined exclusively by the conduction states. The strongly renormalized Fermi liquid state, on the other hand, is described by the renormalized band method us˜ f 10 K in Eq. (3.3) for the intrinsic width of the quasiparticle band. The ing value is consistent with inelastic neutron data70 as well as thermopower and specific heat data.69 CEF effects are accounted for by adopting a 7 ground state. The details of the calculation are described in Ref. [68]. The renormalized band scheme gives the correct Fermi surface topology for CeRu2 Si2 and thus consistently explains the measured dHvA data.61,68,71 The character of quasiparticles in CeRu2 Si2 varies quite strongly over the Fermi surface. The validity of the Fermi liquid picture is concluded from a comparison of the effective masses on Fermi surface sheets with large f contribution. From the large linear specific heat the renormalized band scheme deduces a characteristic energy kT ∗ 10 K and predicts heavy masses of order m∗ /m 100. This value was confirmed by experiments72–74 where the ψ orbit with m∗ /m 120 was observed. The corresponding Fermi surface cross-section is in agreement with estimates from the renormalized band theory. This proofs that the heavy quasiparticles exhaust the low-energy excitations associated with the f -states. The change in volume of the Fermi surface when going from T T ∗ to T T ∗ is observed by comparing the Fermi surface of CeRu2 Si2 to that of its ferromagnetic isostructural counterpart CeRu2 Ge2 where the f -states are clearly localized. In a series of beautiful experiments75 it was demonstrated that the Fermi 69 F. Steglich, U. Rauchschwalbe, U. Gottwick, H. M. Mayer, G. Sparn, N. Grewe, and U. Poppe,

J. Appl. Phys. 57, 3054 (1985). 70 L. P. Regnault, W. A. C. Erkelens, J. Rossat-Mignot, P. Lejay, and J. Flouquet, Phys. Rev. B 38,

4481 (1988). 71 G. Zwicknagl, E. Runge, and N. E. Christensen, Physica B 163, 97 (1990). 72 A. K. Albessard, T. Ebihara, I. Umehara, K. Satoh, Y. Onuki, H. Aoki, S. Uji, and T. Shimizu,

Physica B 186–188, 147 (1993). 73 H. Aoki, S. Uji, A. K. Albessard, and Y. Onuki, Phys. Rev. Lett. 71, 2110 (1993). 74 F. S. Tautz, S. R. Julian, G. J. McMullen, and G. G. Lonzarich, Physica B 206–207, 29 (1995). 75 C. A. King and G. G. Lonzarich, Physica B 171, 161 (1991).

STRONGLY CORRELATED ELECTRONS

21

F IG . III.2. Photoemission results for (a) LaRu2 Si2 in comparison to (b) CeRu2 Si2 at T = 25 K, i.e., above the Kondo temperature T ∗ = 15 K of that system. Band structures are very similar for both compounds. (After Ref. [67].)

surfaces of these two compounds are rather similar. However, the enclosed Fermi volume is smaller in the case of CeRu2 Ge2 , the difference being roughly one electron per unit cell. More direct evidence is provided by recent photoemission experiments (see Figure III.2). Denlinger et al.67 have shown that at temperatures around 25 K, the Fermi surface of CeRu2 Si2 , is that of its counterpart LaRu2 Si2 which has no f electrons. At this point the general question arises how the formation of heavy quasiparticles is reflected in the angular resolved photoelectron spectroscopy (ARPES) data. A major difficulty stems from the fact that photoemission experiments probe the occupied part of the spectrum. The most dramatic changes, however, are expected to occur in the empty part. In Figure III.3 we compare the dispersion of the heavy quasiparticle bands at low temperatures to their light high-temperature counterparts. In the occupied part the main difference is a bending close to the Fermi energy which changes the volume of the Fermi surface. The characteristic bending was recently observed in CeCoIn5 .76 76 A. Koitzsch, Priv. comm.

22

P. FULDE ET AL.

F IG . III.3. Band dispersion for CeCu2 Si2 along Z– for low temperatures T T ∗ (full lines) and high temperatures (dashed lines). The formation of the heavy quasiparticles leads to a characteristic bending in the occupied part of the spectrum.

Let us now turn to the heavy fermion superconductor CeCu2 Si2 which exhibits a highly complex phase diagram at low temperatures discussed in Section III.5. It results from an extreme sensitivity of the physical properties with respect to variations of the stoichiometry and external magnetic fields.

F IG . III.4. CeCu2 Si2 : Main Fermi surface sheet of heavy quasiparticles (m∗ /m 500) calculated with the renormalized band method. It consists of modulated columns which are oriented parallel to the tetragonal axis. The calculations adopt the CEF scheme of Ref. [77] consisting of a singlet ground state separated from an excited quartet by a CEF splitting δ 330 K. Therefore δ T ∗ 10 K (obtained from the γ -value). The nesting vector Q = (0.23, 0.23, 0.52) connects flat parts (“nesting”) of the Fermi surface. (After Refs. [78] and [79].) 77 E. A. Goremychkin and R. Osborn, Phys. Rev. B 47, 14280 (1993). 78 G. Zwicknagl and U. Pulst, Physica B 186, 895 (1993). 79 O. Stockert, E. Faulhaber, G. Zwicknagl, N. Stuesser, H. Jeevan, T. Cichorek, R. Loewenhaupt,

C. Geibel, and F. Steglich, Phys. Rev. Lett. 92, 136401 (2004).

STRONGLY CORRELATED ELECTRONS

23

To calculate the quasiparticle bands in CeCu2 Si2 by means of the renormalized band method, we adopt the doublet-quartet CEF scheme suggested in Ref. [77]. The ground state is separated from the excited quartet by δ 330 K. The results for the Fermi surface78,80 can be summarized as follows: We find two separate sheets of the Fermi surface for heavy and light quasiparticles. The light quasiparticles have effective masses of the order of m∗ /m 5. They can be considered as weakly renormalized conduction electrons. Of particular interest are heavy quasiparticles of effective masses m∗ /m 500 which are found on a separate sheet. This surface whose shape (see Figures III.4 and III.8) is rather different from the corresponding LDA surface mainly consists of columns parallel to the tetragonal axis and of small pockets. The topology of the Fermi surface suggests that the strongly correlated Fermi liquid state should become unstable at sufficiently low temperatures. Firstly, it exhibits pronounced nesting features which may eventually lead to the formation of a ground state with a spin-density modulation. This will be discussed in detail below. Secondly, the topology of this surface depends rather sensitively on the position of the Fermi energy. The band filling and hence the f -valence are critical quantities. Reducing the f -occupancy from the initial value of nf 0.95 by approximately 2% leads to changes in the topology as shown in Refs. [78,80]. As a result, the quasiparticle density of states (DOS) exhibits rather pronounced structures in the immediate vicinity of the Fermi energy which, in turn, can induce instabilities.81 5. L OW-T EMPERATURE P HASE D IAGRAM OF C E C U 2 S I 2 The phase diagram of CeCu2 Si2 contains three different phases: the A and the B phase and a superconducting phase. In some samples the superconducting phase expels the A phase while in other samples the two phases may coexist. While the A phase has been identified as a spin-density wave phase as discussed below, the character of the B phase has remained unknown. The instability may result from a reconstruction of the Fermi surface.78 Much effort has been devoted to the characterization of the A phase which originally had the appearance of a ‘hidden order’ phase. However, later a spin-density wave character was first inferred from resistivity results82 and was supported by specific heat and high-resolution magnetization measurements.83 The transition temperature TA is suppressed by increasing 80 U. Pulst, Ph.D. thesis, TH Darmstadt (1993). 81 M. I. Kaganov and I. M. Lifshits, Sov. Phys. Usp. 22, 904 (1979). 82 P. Gegenwart, C. Langhammer, C. Geibel, R. Helfrich, M. Lang, G. Sparn, F. Steglich, R. Horn,

L. Donnevert, A. Link, et al., Phys. Rev. Lett. 81, 1501 (1998). 83 F. Steglich, N. Sato, T. Tayama, T. Lühmann, C. Langhammer, P. Gegenwart, P. Hinze, C. Geibel,

M. Lang, G. Sparn, et al., Physica C 341–348, 691 (2000).

24

P. FULDE ET AL.

F IG . III.5. B–T phase diagram of CeCu2 Si2 for B a. Original version from Ref. [84], completed version from Ref. [85]. In this sample the SDW A-phase is expelled from the superconducting (SC) region (no coexistence). The nature of the B-phase is yet undetermined.

the 4f -conduction electron hybridization and eventually vanishes. This can be achieved by applying hydrostatic pressure or choosing a few percent excess of Cu. The ordered moments are expected to be rather small. The important question in this context is: What is the origin of the antiferromagnetic correlations, showing up in the A phase? How do they arise in the heavy fermion state and finally, how do they affect the heavy quasiparticles? The key to the answers comes from the Fermi surface of CeCu2 Si2 and its nesting properties. As shown in Figure III.4 there are parallel portions which are connected by a wave vector close to (1/4, 1/4, 1/2). As a consequence, the static susceptibility χ(q) exhibits a maximum for momentum transfer q close to the nesting vector (Figure III.6). Recent neutron scattering experiments79 (Figure III.6) for the stoichiometric compound (x = 0) show a spin-density wave (SDW) which forms below TN 0.7 K. The experimental propagation vector Q is close to (0.22, 0.22, 0.55) and the ordered moment amounts to μ 0.1μB . These findings show that the SDW in CeCu2 Si2 arises out of the renormalized Fermi liquid state. The transition is driven by the nesting properties of the heavy quasiparticles. 84 G. Bruls, D. Weber, B. Wolf, P. Thalmeier, B. Lüthi, A. de Visser, and A. Menovsky, Phys. Rev.

Lett. 65, 2294 (1990). 85 F. Weickert, Private comm. (2003).

STRONGLY CORRELATED ELECTRONS

25

F IG . III.6. Upper panel: Neutron diffraction intensity in CeCu2 Si2 at temperature above and below the A-phase transition temperature TA . Incommensurate peak is at Q = (0.22, 0.22, 0.55). (After Ref. [79].) Lower panel: Nesting of heavy FS columns (Figure III.4) leads to a peak in the static susceptibility χ(q) at q = Q. Intensity map of χ(q) (value increasing from dark to bright) in the reciprocal (h, h, l)-plane as calculated for the renormalized bands at T = 100 mK. The experimental Q at 50 mK from the left panel shows perfect agreement with the calculated maximum position of χ(q).

Having classified the nature of the A phase we next turn to the question how the latter competes with superconductivity. Itinerant electron antiferromagnetism as realized in the A phase and superconductivity both form in the system of the heavy quasiparticles. Their interplay therefore depends sensitively on the geometric properties of the paramagnetic Fermi surface and the symmetries of the ordered phases. This can be seen from realistic model calculations investigating the

26

P. FULDE ET AL.

F IG . III.7. Temperature dependence of the superconducting (SC) and magnetic A (SDW) order parameters in a AS crystal. The sublattice magnetization M = h0 (T ) and the amplitude 0 of the SC order parameter are calculated from Eq. (3.23) using realistic quasiparticles and the experimentally determined propagation vectors for the A phase. A SC order parameter (k) = 0 (cos kx a − cos ky a) (1)

can form in the A phase. Below the superconducting transition temperature T < Tc < TN the two order parameters coexist and compete. Itinerant SDW antiferromagnetism is expelled at a temperature (2) TN < Tc . (After Ref. [86,87].)

variation with temperature of the two order parameters in crystals where the two ordering phenomena coexist in some temperature range (“AS-type” crystals).86,87 Figure III.7 summarizes the results for an unconventional superconducting state with 3 (d-wave) symmetry of the gap function, i.e., (k) ∼ (cos kx a − cos ky a). The theory leading to the results displayed in Figure III.7 starts from the model Hamiltonian H = H0 + Hint where the free quasiparticles are described by

† H0 = E(k)ckσ ckσ .

(3.4)

(3.5)

kσ

The creation (annihilation) operators for quasiparticles with wavevector k, † (pseudo) spins σ = ±1 and energy E(k) are denoted by ckσ (ckσ ). The energies which are measured relative to the Fermi level are calculated within the Renormalized Band Scheme. The residual interactions in the strongly renormalized Fermi liquid are assumed to be repulsive for short separations while being attractive for two quasiparticles of opposite momenta on neighboring sites. The former favors 86 M. Neef, Master Thesis, Technische Universität Braunschweig (2004). 87 M. Neef, M. Reese, and G. Zwicknagl, preprint (2004).

STRONGLY CORRELATED ELECTRONS

27

the formation of a SDW while the latter gives rise to a superconducting instability. Adopting a mean-field approximation yields Hint → HSDW + HSC

(3.6)

where

σ † ck+Qj σ + h.c. h(Qj )ckσ 2

(3.7)

1 † † σ σ (k)ckσ c−kσ + h.c. . 2

(3.8)

HSDW = −

kσ

Qj

and HSC =

kσ σ

The periodically modulated magnetization associated with the SDW with propagation vectors Qj as well as the superconducting pair potential σ σ have to be determined selfconsistently h(Qj ) =

U σ † c ckσ L 2 k+Qj σ

(3.9)

kσ

and σ σ (k) =

1

gsσ σ ;σ σ (k, k )c−k σ ck σ , L

(3.10)

kσ σ

where the strength U of the local Hubbard-type repulsion is of the order of the quasiparticle band width kB T ∗ and gσ σ ;σ σ (k, k ) is the effective pair attraction. The k-summation runs over the entire paramagnetic Brillouin zone and L denotes the number of lattice sites. The expectation values denoted by · · · have to evaluated with the eigenstates of the mean-field Hamiltonian HMF = H0 + HSDW + HSC , and consequently depend upon the order parameters. Therefore the self-consistency equations are coupled. The mean-field Hamiltonian implicitly assumes that the amplitudes of both order parameters are small. In particular, we neglect here the pairing amplitudes of the form c−kσ ck+Qj σ . The latter are important when the gaps introduced by the antiferromagnetic order into the quasiparticle spectrum are large on the scale set by superconductivity. For a discussion of this point we refer to Refs. [88,89]. 88 G. Zwicknagl and P. Fulde, Z. Phys. B 43, 23 (1981). 89 P. Fulde and G. Zwicknagl, J. Appl. Phys. 53, 8064 (1982).

28

P. FULDE ET AL.

The periodically modulated magnetization associated with the SDW acts on the conduction electrons like a periodic spin-dependent potential which we approximate by

h(Qj )eiQj ·r (3.11) h(r) = Qj

with the same amplitudes h(Qj ) = h0 for the eight commensurate wave vectors π π Qj ∈ {(± 2a , ± 2a , ± πc )}. The magnetic superstructure breaks the translational invariance of the underlying lattice but preserves the point group symmetry. The mean-field Hamiltonian, however, is invariant under translations with a1 = (2a, 2a, 0),

a2 = (2a, −2a, 0),

a3 = (2a, 0, c).

(3.12)

The volume of the magnetic supercell is 16 times the volume of the paramagnetic unit cell. As a result the Brillouin zone is reduced and the quasiparticle states are modified by extra Bragg reflections. The opening of new gaps is important at sufficiently low temperatures T TN where TN is the ordering (Néel) temperature. The order parameter σ σ behaves as a two-fermion wave function in many respects. This is expressed by the fact that an off-diagonal long-range order (ODLRO) parameter is not the thermal expectation value of a physical observable but rather a complex pseudo- wave function describing quantum-phase correlations on the macroscopic scale of the superconducting coherence length. Its phase is a direct signature of the broken gauge invariance in the superconducting condensate. Experiment (strongly) suggests that superconductivity in CeCu2 Si2 occurs with anisotropic even-parity (pseudo-) spin singlet pairing. We therefore restrict ourselves to this case characterized by a scalar order parameter σ σ (k) = φ(k)(iσ2 )σ σ

(3.13)

were φ(k) is a complex amplitude and σ2 denotes the Pauli matrix in spin space. Since the two ordering temperatures, i.e., the antiferromagnetic Néel temperature TA and the superconducting Tc are very close to each other we focus on pair states which are compatible with the translational symmetry of the paramagnetic lattice. The corresponding functions are listed in Refs. [68,90–92]. In the explicit calculations we restrict ourselves to one-dimensional representations for simplicity. The generalization to multi-dimensional representations is rather straightforward.86 Finally, the variation with momenta k and k of the quasiparticle attraction g(k, k ) is expanded in terms of the basis functions belonging to the κ-th row, κ = 90 M. Sigrist and K. Ueda, Rev. Mod. Phys. 63, 239 (1991). 91 R. Konno and K. Ueda, Phys. Rev. B 40, 4329 (1989). 92 M. Ozaki and K. Machida, Phys. Rev. B 39, 4145 (1989).

STRONGLY CORRELATED ELECTRONS

29

1, . . . , d(), of the d()-dimensional irreducible representation of the symmetry group g(k, k ) =

g

d()

ϕκ (k)ϕ∗ κ (k ).

(3.14)

κ=1

We further simplify the problem by focusing on the states φ (k) with the symmetry which yields the strongest quasiparticle attraction g . Assuming that this most stable order parameter is non-degenerate the self-consistency condition is 1 ∗ φ(k) = −g0 ϕ0 (k) ϕ (k )c−k ↓ ck ↑ . (3.15) L 0 k

To solve the mean-field Hamiltonian Eqs. (3.7) and (3.8) we adopt the Nambu formalism which allows us to reduce the mean-field Hamiltonian to single-particle form in particle–hole space, i.e., H=

AFBZ

ˆ τˆ3 + h1 ˆ + (k) ˆ k† E(k) τˆ1 k .

(3.16)

k

The Nambu spinors k have 32 components and are defined as † † k† = ck↑ , ck+Q1 ↑ , . . . , c−k↓ , c−k−Q ,... . 1↓

(3.17)

They account for the coherent superposition of particles and holes which is the ˆ τˆ1 and τˆ3 denote the characteristic feature of the superconducting state. Here 1, unit matrix and the Pauli matrices in particle–hole space. The sixteen wave vectors Q0 = 0, Q1 , . . . , Q15 are the reciprocal lattice vectors appearing in the antiferromagnetic phase. The set includes the eight propagation vectors of the SDW and their higher harmonics. The k-summation is restricted to the reduced Brillouin zone (AFBZ) of the antiferromagnetic state defined by the SDW. The structure of the Hamiltonian in particle–hole space is

ˆ ˆ E(k) + hˆ ˆ H (k) = (3.18) ˆ ˆ −E(k) + hˆ where the 16 × 16-diagonal matrix contains the quasiparticle energies of the paramagnetic normal phase ˆ E(k) = δQi Qj E(k + Qi ). (3.19) QQ i

j

The SDW acts like an effective magnetic field. The modulated spin density leads to Umklapp scattering which is accounted for by the matrix ˆ hˆ = −h0 (T )m.

(3.20)

30

P. FULDE ET AL.

ˆ is a purely geometric quantity specifying the possible UmkThe 16 × 16 matrix m lapp processes while the temperature-dependent amplitude h0 (T ) has to be determined self-consistently. The diagonal matrix ˆ (k) = δQi Qj 0 (T )ϕ0 (k + Qi ) Qi Qj ˆ (3.21) ≡ 0 (T ) (k) QQ i

j

contains the superconducting order parameters with the given k-dependent function φ (k) and a temperature-dependent amplitude 0 (T ). The self-consistency Eqs. (3.9) and (3.10) can be formulated in terms of the off-diagonal elements of the 32 × 32-matrix Green’s function ˆ n , k) = in 1ˆ − Hˆ (k) −1 G(i (3.22) according to h0 (T ) =

c AFBZ

1 U

ˆ n , k) ˆ 1ˆ G(i T Tr m L 16 k

n

0 (T ) = −

c AFBZ

1 g

ˆ )τˆ1 τˆ3 G(i ˆ n , k )τˆ3 . T Tr (k L 2 n

(3.23)

k

Here n = πT (2n + 1) denote the T -dependent Matsubara frequencies and c is the energy cut-off required in weak-coupling theory. The coupling constants U and g as well as the cut-off c are eliminated in the usual way in favor of the (0) (0) observable quantities TN and Tc . Solving the self-consistency equations for φ3 (k) ∼ cos kx a − cos ky a yields the results displayed in Figure III.7. It shows that both order parameters coexist in a finite temperature interval. This is due to the fact they have their maximum amplitudes on different parts of the Fermi surface (see Figure III.8). At sufficiently low temperatures the A-phase is finally expelled by superconductivity as shown in Figure III.7. This was confirmed by neutron diffraction which shows a suppression of magnetic Bragg peaks further below Tc . IV. Quantum Phase Transitions

Most phase transitions in condensed matter are governed by the appearance of a spontaneously broken symmetry below a certain transition temperature Tc . The low temperature phase is then characterized by an order parameter belonging to a single nontrivial representation of the high temperature symmetry group. In the simplest case the order parameter is of the density type (diagonal long range order), for instance charge density n(r) or spin density m(r). Approaching Tc from

STRONGLY CORRELATED ELECTRONS

31

F IG . III.8. CeCu2 Si2 : Variation of the SC gap function amplitude |(k)|/0 (T ) = |φ3 (k)| for the (pseudo-) singlet wave function with 3 -symmetry φ3 (k) ∼ cos kx a − cos ky a on the heavy quasiparticle sheet of the paramagnetic Fermi surface. The amplitude of this SC order parameter is maximal on the kidney-shaped surfaces centered along the direction which are almost unaffected by the formation of the A phase. The dominant contributions to the latter come from the nesting parts on the heavy columns where the superconducting amplitude is small. Dark and light grey indicate large and small amplitudes, respectively.

above the correlation length of spatial order parameter fluctuations, the associated order parameter susceptibility and other thermodynamic quantities diverge. The divergence is characterized by critical exponents that depend only on spatial dimension d, on the range of interactions and number of order parameter components n which define the universality class of the model. In such finite temperature or ‘classical’ phase transitions the underlying microscopic quantum fluctuations of charge and spin densities etc. are not important ingredients for the long-range order because their coherence is destroyed by thermal fluctuations over time scales longer than h¯ /kTc . However, the broken symmetry state may not only be reached by lowering the temperature. Instead at T = 0 the tuning of a physical control parameter X, e.g., due to applied hydrostatic or chemical pressure via doping may drive the compound from the disordered to the ordered state and vice versa (see Figure IV.6). The corresponding value Xc defines the quantum critical point (QCP) where a quantum phase transition (QPT) takes place. In the latter the T = 0 quantum fluctuations can be coherent over arbitrary long time scales. For this reason the effective dimension for order parameter fluctuations close to a QPT is given by deff = d + z where z is the dynamic exponent which characterizes the scaling of energies of quantum fluctuations with system size. The contribution of quantum fluctuations has therefore profound consequences for the critical exponents of thermodynamic and transport quantities. For example, in strongly correlated metals close to an antiferromagnetic QCP along the quantum critical line (X = Xc

32

P. FULDE ET AL.

or |r| = 0) in Figure IV.6 an anomalous non-Fermi liquid (NFL) temperature dependence of physical quantities like χ(T ), C(T )/T and ρ(T ) emerges. Its origin and theoretical description has been the subject of much recent investigations and controversy.93,94 An additional important discovery is the observation that superconductivity often appears in a dome-like shape around the QCP. Viewed differently, it may be a successful strategy to look for unconventional superconducting states in searching around magnetic QCPs of suitable materials. The presence of strong electronic correlations is by no means essential for the appearance of a quantum phase transition. Historically they have been first studied in weakly correlated metals without calling them explicitly with their modern name. As an introduction we will briefly discuss some early examples of QPTs. Subsequently well understood model theories for QPTs in local moment systems, notably the Ising model in a transverse field will be discussed. Then we come to QPTs in the strongly correlated systems where theoretical work has focused on the Kondo-lattice type models both with and without charge degrees of freedom. Finally the phenomenological scaling and Ginzburg–Landau theories applicable close to the QCP will be discussed. They are important for the interpretation of a large body of experimental work near the QCP of heavy-fermion compounds. 6. Q UANTUM P HASE T RANSITION IN L OCALIZED AND I TINERANT M AGNETS The idea that tuning of a control parameter may drive an insulator or metal from the paramagnetic state to a magnetically ordered state at zero temperature is indeed a very old one. The classical Stoner–Wolfarth theory of itinerant ferromagnetism (FM)95,96 identifies this control parameter as X = I N(EF ) where I is the exchange integral of itinerant conduction electrons and N (EF ) the conduction electron DOS per spin direction. In the paramagnetic regime with X < Xc = 1 the exchange interaction is too weak to cause an exchange splitting of conduction bands and stabilize a spin polarization. However the incipient FM order has its effect on the spin fluctuation spectrum. The typical life time τsf of a quantum fluctuation of magnetic moments diverges when X → Xc . This may be seen from the dynamical susceptibility, calculated from the single-band Hubbard model for 93 S. Sachdev, Quantum Phase Transitions, Cambridge University Press (1999). 94 M. A. Continentino, Quantum Scaling in Many-Body Systems, World Scientific (2001). 95 E. Stoner, Proc. Roy. Soc. A165, 372 (1938). 96 E. Stoner, Proc. Roy. Soc. A169, 339 (1939).

STRONGLY CORRELATED ELECTRONS

33

a parabolic band within random-phase approximation (RPA). Close to the QCP (X Xc ) the spectrum of FM spin fluctuations with q → 0 is given by:97,98 Im χ−+ (ω) =

(π/4)N (EF )ω/qvF [1 − I N(EF )]2 + [(π/4)N (EF )I ω/qvF ]2

(4.1)

where vF is the Fermi velocity. When X → Xc this spectrum is strongly peaked at the ‘paramagnon’ frequency (S 1) ωP =

4 vF q. π S

(4.2)

Here S = (1 − I N(EF ))−1 is the ‘Stoner parameter’ which governs the softening of the spin fluctuation spectrum in Eq. (4.1) on approaching the QCP. It also gives the enhancement of the static susceptibility χ = Sχ0 as compared to the free Pauli susceptibility χ0 . In addition the paramagnon excitations lead to a deviation from the linear specific heat behavior of the Fermi liquid described by98,99 C(T )/T = γ0 [m∗ /m + S(T /TSF )2 ln(T /TSF )]

(4.3)

where m∗ /m is the mass enhancement due to paramagnons98 and TSF is the spin fluctuation temperature given by TSF = EF /S. Equivalently one may say that χ−+ (ω) has a pole at the purely imaginary frequency iωP . This represents a collective overdamped spin fluctuation mode. When X is tuned through the critical value Xc = 1 by pressure or alloying, the imaginary spin fluctuation pole moves to the real axis and becomes the FM spinwave pole with frequency (q kF , ms n) ω(q) = Dq 2 ,

D ∼ (I 2 /EF )kF−2 nms .

(4.4)

Simultaneously a spontaneous FM moment caused by the spin polarization ms = n↑ − n↓ of conduction bands appears. Here D is the spin wave stiffness constant and n = n↑ + n↓ is the number of conduction electrons per site. This collective spin excitation is undamped for small q because it is the Goldstone mode associated with the continuous SO(3) symmetry of the FM order parameter and therefore in the hydrodynamic limit it is protected by a conservation law against decay. For X only marginally above the FM QCP Xc = 1 one has only weak ferromagnetism (WFM) and anomalous thermodynamic and transport behavior due to paramagnon excitations was observed.97,98 The first theory beyond the Hartree–Fock RPA level to address such quantum critical phenomena in itinerant 97 N. F. Berk and J. R. Schrieffer, Phys. Rev. Lett. 17, 1171 (1966). 98 S. Doniach and S. Engelsberg, Phys. Rev. Lett. 17, 750 (1966). 99 C. P. Enz, A Course on Many-Body Theory Applied to Solid-State Physics, vol. 11 of Lecture Notes in Physics, World Scientific (1992).

34

P. FULDE ET AL.

ferromagnets was Moriya’s self consistent renormalization (SCR) theory48,100,101 for the WFM and the theory by Hertz102 on which much of the later developments are based. The best known example of an enhanced paramagnetic metal which is close to a FM quantum critical point is palladium metal. In this case one has a large susceptibility enhancement of S 10.103 Indeed, alloying with only 0.5% Fe immediately leads to FM order.104 According to band structure calculations a (linear) expansion of the lattice of pure Pd by ∼ 7% should lead to a FM ground state. Experimentally Au–Pd–Au sandwiches have been prepared where an estimated volume expansion of 2.3% of Pd due to the larger lattice constant of Au leads to huge Pd Stoner factors of S ∼ 103 –104 ,105 but FM order is still not achieved. The classical, enhanced paramagnetism in Pd and associated QPT in Pd alloys has been complemented by Laves phase compounds AB2 like TiBe2 106 and ZrZn2 107 which are slightly on the overcritical side, i.e., I N(EF ) 1 and thus weak itinerant ferromagnets. By doping with Cu the alloy series TiBe2−x Cux exhibits a QCP at xc 0.155 where ferromagnetism disappears. The compound ZrZn2 has already been known for a long time and has recently been investigated with renewed interest because it exhibits a FM QCP as function of hydrostatic pressure at pc = 21 GPa. As in UGe2 it was found that surprisingly superconductivity coexists within the FM phase, albeit with a small Tc .108 Quite another quantum phase transition to a magnetically ordered state has been known since a long time in localized moment systems. It was studied under the name ‘induced moment magnetism’ without actually stressing that it is a generic type of quantum phase transition as we shall see. In localized (4f - or 5f -) magnetic compounds with uniaxial symmetry the lowest CEF states of non-Kramers ions may consist of a nonmagnetic singlet ground state |1 and a nonmagnetic singlet (or doublet) excited state |2 at an energy . They are both characterized by a vanishing moment, i.e., n|Jz |n = 0 (n = 1, 2) with Jz denoting the total angular momentum component of the localized 4f or 5f states. Therefore there are no pre-existing localized moments that might order as in a conventional AF 100 T. Moriya and A. Kawabata, J. Phys. Soc. Jpn. 35, 669 (1973). 101 T. Moriya, Spin Fluctuations in Itinerant Electron Magnetism, vol. 56 of Springer Series in Solid-

State Sciences, Springer-Verlag, Berlin (1985). 102 J. A. Hertz, Phys. Rev. B 14, 1165 (1976). 103 W. Gerhardt, F. Razavi, J. S. Schilling, D. Hüser, and J. A. Mydosh, Phys. Rev. B 24, 6744 (1981). 104 J. A. Mydosh, J. I. Budnick, M. P. Kawatra, and S. Skalski, Phys. Rev. Lett. 21, 1346 (1968). 105 M. B. Brodsky and A. J. Freeman, Phys. Rev. Lett. 45, 133 (1980). 106 F. Acker, Z. Fisk, J. L. Smith, and C. Y. Huang, J. Magn. Magn. Mater. 22, 250 (1981). 107 B. T. Matthias and R. M. Bozorth, Phys. Rev. 109, 604 (1958). 108 C. Pfleiderer, M. Uhlarz, S. M. Hayden, R. Vollmer, H. v. Löhneysen, N. R. Bernhoeft, and G. G. Lonzarich, Nature 412, 58 (2001).

STRONGLY CORRELATED ELECTRONS

35

phase transition. The local moments themselves have to be induced at any given site at TN . This is possible if a nondiagonal matrix element α = 1|Jz |2 exists. The effective RKKY inter-site exchange J (q) then mixes the two states, thereby creating an induced ground state moment. If J (q) is maximal at a wave vector Q this happens spontaneously at a temperature TN =

2 tanh−1 ( ξ1 )

,

here ξ =

α 2 J (Q) 2

(4.5)

is the control parameter of the quantum phase transition to an induced moment state. It takes place for ξ > ξc = 1. In general the ordered state has an incommensurate modulation with wave vector Q. In the paramagnetic phase the magnetic singlet-singlet excitations disperse into a magnetic exciton band given by α 2 J (q) (4.6) ω(q) = 1 − 2 The onset of the QFT is signified by a softening of the exciton mode as function of ξ at the incipient ordering vector Q which is given by ω(Q) = [1 − ξ ] and vanishes at ξc = 1. The control parameter contains the CEF splitting which is susceptible to pressure. The latter may therefore be used to tune the singletsinglet system through the QCP. Phase transitions of the induced moment type under ambient conditions as well as under pressure have been found in a number of rare earth systems like Pr3 Tl, TbSb (for a review see Ref. [109]) and dhcp Pr metal.110,111 It also describes the AF order in the actinide compound UPd2 Al3 with partly itinerant and partly localized 5f-electrons (see Section V). In fact dhcp Pr, which is approximately a singlet-doublet CEF system, is of special interest. There the critical mode softening and modulated moment appearance under uniaxial pressure shown in Figure IV.1 correspond to the modern concept of a quantum phase transition due to variation of a microscopic control parameter. However, this aspect was not stressed or realized at that time. This is remarkable because it was found earlier that the simplest Hamiltonian which describes induced moments in the singlet-singlet system (though not precisely dhcp Pr) is of the type

H = Tix + I Tiz Tiz (4.7) i

ij

109 P. Fulde, in Handbook of the Physics and Chemistry of Rare Earth, vol. 2, eds. K. A. Gschneider, Jr. and L. Eyring, North-Holland, Amsterdam (1979), chap. 17, p. 295. 110 J. Jensen, K. A. McEwen, and W. G. Stirling, Phys. Rev. B 35, 3327 (1987). 111 J. Jensen and A. R. Mackintosh, Rare Earth Magnetism: Structures and Excitations, Clarendon Press, Oxford (1991).

36

P. FULDE ET AL.

F IG . IV.1. Left panel: paramagnetic (PM) to incommensurate magnetic (ICM) quantum phase transition as function of uniaxial pressure in dhcp Pr. The quantum critical point is at pc ∼ 0.7 kbar. Circles are the experimental first harmonic of the ICM moment corresponding to modulation wave vector Q = 0.12a∗ . Dashed and solid lines correspond to model calculations. Right panel: Optic (open circles) and acoustic (closed circles) exciton mode frequencies which give the energy scale of quantum fluctuations. Close to the quantum critical point at pc and for the ordering wave vector Q this energy scale vanishes. (After Ref. [110].)

where the two orientations | ↑, | ↓ of the pseudo-spin Tz correspond to the CEF singlets n = 1, 2 respectively. Indeed, this is the n.n. Ising model in a transverse field (ITF), a genuine model for quantum phase transitions. The last term establishes AF order of Ising spins with a twofold degenerate ground state due to Z2 symmetry. The first transverse field term introduces quantum fluctuations of the spins and destroys long-range order if the control parameter ξ = I /(2) exceeds ξc = 1. This model is exactly solvable in 1D112,113 and therefore is a reference point for the theory of QPTs. If one adds an infinitesimal staggered field term to 112 E. Lieb, T. Schultz, and D. Mattis, Ann. Phys. (N. Y.) 16, 407 (1961). 113 P. Pfeuty, Ann. Phys. (N.Y.) 57, 79 (1970).

STRONGLY CORRELATED ELECTRONS

37

F IG . IV.2. Pseudo spin correlation functions for the ITF according to Eqs. (4.8), (4.9) as function of inverse control parameter 1/ξ = 2/I . Order parameter mz = |Tz | with critical (pressure) exponent 1/8 is also shown. (After Ref. [114].)

Eq. (4.7) one obtains a finite order parameter Tz given in Section VI.14 provided ξ > ξc . The critical exponent of the order parameter is 1/8. In addition the correlation functions may be calculated exactly. In good accuracy they are given by112,113 (j = i ± 1): z z Ti T j = k z , where 1 kz = − 4π

0

π

ξ + cos(q) dq , q

x x Ti Tj = m2x ,

1 mx = 2π

π

dq 0

(4.8)

1 + ξ cos(q) x (4.9) = Ti q

1 2

with q = (1 + ξ 2 + 2ξ cos q) . These correlation functions together with the order parameter are plotted in Figure IV.2. It shows nicely that long range order mz is destroyed when the transverse quantum fluctuations characterized by m2x overwhelm the longitudinal correlations given by kz . The ITF is a generic model for QPTs that may be applied to quite different physical systems. For example, in the case of induced magnetic moment ordering discussed above the two pseudospin states correspond to the two CEF singlet states, the Ising interaction is due to the nondiagonal exchange between them and the transverse field is associated with the CEF splitting energy. On the other hand the same model may be applied to the problem of charge ordering in insulators with a 2D ladder type structure 114 V. Yushankhai and P. Thalmeier, Phys. Rev. B 63, 064402 (2001).

38

P. FULDE ET AL.

like α -NaV2 O5 . In this case the pseudo-spin describes resonating, singly occupied 3d states within the rung of a ladder, the Ising interaction corresponds to the inter-site Coulomb interaction between d-electrons in different rungs and the transverse field is provided by the intra-rung kinetic (hopping) energy. The ITF then describes a quantum phase transition where charge ordering in the rungs is destroyed by the increase of the intra-rung kinetic energy. This will be discussed in detail in Section VI.14. The induced moment magnetism can also appear in a different context in compounds with localized 3d-electrons. Instead of singlet-singlet CEF states as before one may have here singlet-triplet level systems with a splitting due to preformed dimers of S = 1/2 3d-spins. When the inter-dimer exchange coupling is slightly subcritical the magnetic exciton mode with a minimum at the wave vector Q has a finite but small energy and the compound is paramagnetic. Application of a magnetic field splits off one triplet component and the excitation energy at Q is driven to zero at a critical field Hc . There a quantum phase transition to an incommensurate magnetic phase takes place. An example is TlCuCl3 where the Cu2+ spins form dimers.115 Since for 3d spins the orbital degrees are quenched, the inter-dimer coupling is of the Heisenberg- rather than Ising type where the latter has a discrete Z2 symmetry as discussed above. This makes an essential difference since the continuous SU(2) symmetry of the former allows the exchange Hamiltonian to be mapped to a hard-core boson Hamiltonian for the singlet-triplet boson excitations.116 Then the field-driven QPT in TlCuCl3 can be interpreted as Bose–Einstein condensation (BEC) of the singlet-triplet excitations. Another, even cleaner example of magnetic order through BEC, though with different microscopic details was recently identified in Cs2 CuCl4 .117 Actually the mapping to the boson model is already possible for the xy-exchange model with U(1) symmetry in a transverse field which applies to dhcp Pr.111 Thus the appearance of an incommensurate phase under pressure in Figure IV.1 may perhaps also be described within the BEC framework. This has not been investigated yet. 7. Q UANTUM C RITICALITY IN THE KONDO L ATTICE As mentioned in the introduction a great part of the interest on QPTs is focused on strongly correlated metallic systems which exhibit pronounced non-Fermi liquid 115 C. Ruegg, N. Cavadini, A. Furrer, H. U. Güdel, K. Krämer, H. Mutka, A. Wildes, K. Habicht, and P. Vorderwisch, Nature 423, 62 (2003). 116 M. Matsumoto, B. Normand, T. M. Rice, and M. Sigrist, Phys. Rev. B 69, 054423 (2004). 117 T. Radu, H. Wilhelm, V. Yushankhai, D. Kovrizhin, R. Coldea, T. Lühmann, and F. Steglich, Phys. Rev. Lett. 95, 127202 (2005).

STRONGLY CORRELATED ELECTRONS

39

(NFL) behavior. This is found frequently close to pressure- (hydrostatic or chemical) and field-induced QPTs from the paramagnetic to the antiferromagnetic phase of Ce- or Yb-based heavy fermion metals. The schematic phase diagram for such compounds is shown in Figure IV.6. Prominent examples are found among the class of Ce122, Ce115 and Ce218 intermetallic compounds and alloys.54 Classical cases are CePd2 Si2 ,118 CeNi2 Ge2 119 and more recently YbRh2 Si2 .120 Most Ce compounds also exhibit dome-shaped superconductivity, sometimes with very small Tc . It appears in the NFL regime around the quantum critical point of AF order. For an example see Figure IV.6 (right panel). The generic model to describe the quantum critical Ce HF compounds is the Kondo lattice model given by

† k ckσ ckσ + JK si Si . (4.10) HKL = kσ

i

The first term describes conduction electrons with a dispersion k and bandwidth W . The second term is a local AF (JK > 0) coupling of conduction electron spins si to localized spins Si . There are two competing effects. Firstly, the solutions of the Kondo impurity model (a single spin Si=0 coupled to the Fermi sea) shows that below the Kondo temperature TK = W exp(−1/JK N (0)) the local moment is screened. A singlet is formed which extends to a distance ξK ∼ hv ¯ F /TK from the impurity site.50 Secondly, in the lattice the polarization of conduction electrons due to an on-site exchange induces an effective RKKYtype interaction between localized spins. This leads to a tendency to magnetic order at a temperature of the order TRKKY ∼ JK2 χ(2kF ) where χ(q) is the conduction electron susceptibility. When TRKKY TK local but overlapping singlets form a nonmagnetic state and below a coherence temperature Tcoh < TK they disperse into quasiparticle bands as indicated in Figure IV.6 (see also Section III). For TRKKY TK the singlet formation is inhibited and magnetic order sets in at TN . When the two temperature scales are about the same size one expects a quantum phase transition between the magnetically ordered and nonmagnetic heavy Fermi liquid state. This criterion is only a heuristic guide because TK is the nonperturbative energy scale (the singlet binding energy) of the impurity problem, whereas TRKKY is the perturbative energy scale on the lattice. The control parameter of the model is X = JK /W which may be assumed to vary linearly with pressure. This behavior is illustrated in the Doniach-type phase diagram around 118 F. M. Grosche, I. R. Walker, S. R. Julian, N. D. Mathur, D. M. Freye, M. J. Steiner, and G. G. Lonzarich, J. Phys. Condens. Matter 13, 2845 (2001). 119 R. Küchler, N. Oeschler, P. Gegenwart, T. Cichorek, K. Neumaier, O. Tegus, C. Geibel, J. A. Mydosh, F. Steglich, L. Zhu, and Q. Si, Phys. Rev. Lett. 91, 066405 (2003). 120 J. Custers, P. Gegenwart, H. Wilhelm, K. Neumaier, Y. Tokiwa, O. Trovarelli, C. Geibel, F. Steglich, C. Pepin, and P. Coleman, Nature 424, 524 (2003).

40

P. FULDE ET AL.

the QCP (Figure IV.6). The wedge above the QCP is the region where NFL behavior of thermodynamic coefficients and transport properties is observed. This qualitative picture is hard to quantify. In fact the Kondo lattice model is an unsolved problem and only various approximative and numerical methods have been applied to it. The problem may be somewhat simplified by eliminating the charge degrees of freedom. This was proposed in Ref. [121] for the 1D Kondo chain. Using a Jordan–Wigner transformation the 1D conduction electrons may be replaced by a second spin system with xy-type inter-site coupling in addition to the local Kondo spins. The model then reads

y y τix τjx + τi τj + δτiz τjz + JK τ i Si . (4.11) HKN = 2J ij

i

The 1D ‘Kondo necklace’ model based on the Jordan–Wigner transformation of HKL has δ = 0. But later this was generalized to δ > 0 in arbitrary dimension and treated as a model for the competition of AF order (J ) and local singlet formation (JK ) in its own right. The control parameter is now X = JK /2J . The constant 2J associated with interacting spins corresponds to the bandwidth W of conduction electrons in the original HKL . The approximate quantum critical phase diagram of this model may be obtained with the help of the bond operator method.122 It starts from the observation that the four singlet-triplet basis states of a local pair of spins τ i , Si may be represented by singlet-triplet boson creation operators according to |s = s † |0 and |tα = tα† |0 (α = x, y, z). The spin operators may then be expressed in terms of singlet and triplet boson operators: 1 † † sn − iαβγ tnβ tnγ Sn,α = sn† tn,α + tn,α 2 1 † † τn,α = −sn† tn,α − tn,α (4.12) sn − iαβγ tnβ tnγ . 2 † These operators have to fulfill the local constraint sn† sn + α tnα tnα = 1 at every site n. Using the above transformation in HKN one obtains various bosonic interaction terms which may be decoupled by a mean field approximation both in the Hamiltonian and in the constraint. In the strong coupling region where X = JK /2J is large the ground state is characterized by the molecular field s¯ = s corresponding to a condensation of the local singlet bosons. The decoupling then leads to a bilinear Hamiltonian in the triplet bosons which may be diagonalized and yields the triplet excitation energies ωk . From the excitation spectrum the singlet amplitude s¯ (X) and the chemical potential μ(X) (to satisfy the mean-field constraint) are determined self-consistently. Then the minimum 121 S. Doniach, Physica B 91, 231 (1977). 122 G. M. Zhang, Q. Gu, and L. Yu, Phys. Rev. B 62, 69 (2000).

STRONGLY CORRELATED ELECTRONS

41

triplet excitation energy is at the AF zone boundary vector q = Q, and it is equivalent to the spin gap in the Kondo singlet phase. It is given by (z = coordination number)

1 SP = JK + μ/JK 1 − zd/2 4 d=

s¯ 2 2J JK ( 14 + μ/JK )

(4.13)

where the dimensionless parameter d(X) is determined by the self-consistent equation 4J 1 ω0 d= 1− JK 2N ωk ωk = 1 + dγk ω0

k

with γk =

cos kα .

(4.14)

α

When the intermediate coupling regime is approached by decreasing X −1 = 2J /JK the spin gap eventually collapses and a magnetically ordered phase is established. The solution of the above equations is shown in Figure IV.3 for the

F IG . IV.3. Spin gap s in the Kondo singlet (KS) phase and staggered magnetization ms in the AF phase as function of the inverse control parameter 1/X = 2J /JK . Full line is the mean field result for HKN in 2D for the xy case (δ = 0). The dotted line is obtained from Monte Carlo simulations. The QCP is at 1/Xc 0.7. (After Ref. [122].)

42

P. FULDE ET AL.

2D case. Indeed it exhibits a QPT at a critical value Xc ∼ 1.43. For larger X, i.e., in the AF regime an analogous calculation may be performed leading to the staggered magnetization ms shown in the previous figure. In 3D results are similar but the scaling exponents for SP (X) and ms (X) close to the QCP are different. We note that the boson representation employed here for the Kondo-necklace type model is identical to the one used in the spin-dimer problem in TlCuCl3 .116 Therefore the transition from spin gap to AF phase may also be interpreted as a BEC of triplet bosons. The mean-field boson treatment confirms the qualitative conjectures made above on the quantum critical phase diagram by simply comparing the energy scales of singlet formation and magnetic order. Because it respects the local constraint for bosons only on the average this method is however completely inadequate to investigate how the on-site singlet and inter-site magnetic correlations compete as function of control parameter X and also as function of temperature. For this purpose one has to use advanced numerical approaches like the finite temperature Lanczos method123 for finite size clusters. This method has recently been employed to Kondo lattice like models given by HKL and also HKN with δ = 1, i.e., in the Heisenberg limit for the interacting τ -spins.124 Because each site has 4 states, the possible cluster sizes for exact diagonalization are limited. The 8-site cluster of the square lattice with periodic boundary conditions was investigated and correlation functions and specific heat were calculated.124 The Lanczos procedure is repeated 400 times for random starting vectors in the 4N (N = 8)-dimensional Hilbert space until convergence for thermodynamic quantities is achieved. The specific heat results are shown in Figure IV.4 (upper panel) for various values of the control parameter X = JK /2J . For JK = 0 the broad upper maximum corresponds to the AF correlations of the ‘itinerant’ τ -spins. When JK is turned on a lower much sharper maximum rapidly evolves which shifts to higher temperatures and for X ∼ 1.5 eventually merges with the upper maximum. The origin of the lower sharp maximum becomes clear if one monitors the on-site singlet correlation τ 1 · S1 and the induced ‘RKKY’ correlations S1 · S2 between the localized (but non-interacting) spins at n.n. sites 1 and 2. These correlations are shown in Figure IV.5 as function of temperature. For JK = 0 both correlations are absent. When JK is turned on τ 1 · S1 develops AF on-site singlet correlations with a limiting value of −0.75 in the strong coupling limit (upper panel). Due to the inter-site coupling of τ -spins the local singlet formation also induces AF inter-site correlations of the previously uncoupled Si spins (lower panel). In the strong coupling limit when on-site singlets are formed, however, the inter-site correlations of Si spins are diminished again. The sharp maximum in CV is well correlated with the inflection point of the induced inter-site correlations. Therefore 123 G. Jaclic and N. B. Prelovsek, Adv. Phys. 49, 1 (2000). 124 I. Zerec, B. Schmidt, and P. Thalmeier, Physica B, in press.

STRONGLY CORRELATED ELECTRONS

43

F IG . IV.4. Upper panel: The specific heat CV of the 8-site cluster. Lower panel: ‘Phase diagram’ of the 8-site cluster (inset) obtained from tracing the characteristic maxima of CV (full lines) and inflection points of correlation functions (from Figure IV.5) as function of control parameter X = JK /2J . PM = paramagnetic phase, ‘AF’ = phase with AF correlations of τ -spins. ‘LAF’ = phase with AF correlations of local spins S. ‘Local Singlet’—phase with Kondo spin gap. (After Ref. [124].)

in the thermodynamic limit it may be interpreted as the CV -anomaly due to AF order of partially Kondo-screened local moments. For larger JK the sharp lower CV maximum merges with the broad upper maximum but the inflection point in S1 · S2 may still be identified. Following these characteristic temperatures as function of X a ‘phase diagram’ of the Kondo-lattice type model HKN (δ = 1) may be constructed as shown in Figure IV.4 (lower panel). For small values of JK one finds a correlated state of ‘itinerant’ τ spins (‘AF’) below the temperature of the broad maximum in CV . Below the sharp maximum temperature one has induced antiferromagnetic correlations of the local S spins (‘LAF’). For larger

44

P. FULDE ET AL.

F IG . IV.5. Upper panel: On-site correlations show singlet formation at low temperatures. Lower panel: Simultaneously inter-site ‘RKKY’ correlations are induced for moderate JK and suppressed again for large JK . (After Ref. [124].)

values of JK both maxima merge but correlations of the LAF state are still visible (dotted line). For even larger JK the ‘Local Singlet’ formation dominates correlation and specific heat behavior. Of course, due to the finite cluster size one may not strictly speak about thermodynamic phases and phase boundaries. However, the qualitative evolution of correlations and thermodynamic anomalies as function of control parameter X may be expected to survive in the thermodynamic limit. It is interesting to compare these findings with the previous mean-field calculation for the quantum phase transition as function of X. In the cluster calculation one would identify the ‘QCP’ with the value of X = JK /2J where the correlations show a cross-over from inter-site (‘LAF’) to ‘Local Singlet’ type behavior along the T = 0 line in Figure IV.4 (lower panel). This is found to be at Xc ∼ 1–1.5 and

STRONGLY CORRELATED ELECTRONS

45

compares reasonably well with the value Xc = 1.43 of the mean-field calculation (where however δ = 0 was taken). 8. S CALING T HEORY C LOSE TO THE Q UANTUM C RITICAL P OINT The previous calculations give an insight into the microscopic mechanism of singlet formation vs magnetic order in the Kondo lattice. These results are, however, still far removed from explaining the most common experiments around the QCP, notably the temperature and field scaling for specific heat, susceptibility, resistivity, etc. Assuming the existence of a QCP some insight into the dependence of physical quantities on temperature and control parameters close to it (see Figure IV.6) may be obtained within a simple phenomenological scaling theory. A Kondo impurity in a metallic host shows all the signatures of a local Landau Fermi liquid state50 at temperatures T T ∗ , notably a scaling of the free energy density with T /T ∗ . This leads to universal relations among low temperature thermodynamic quantities irrespective of the microscopic details. This idea has been successfully extended to the Fermi liquid phase of heavy fermion and

F IG . IV.6. Left panel: Schematic phase diagram for Kondo compounds with a QCP (r = 0) separating AF (left) and LFL (right) phases (full line). Scaling of characteristic temperatures is indicated (broken lines). (After Ref. [125].) Right panel: Hydrostatic pressure induced AF to HF liquid QPT in CePd2 Si2 . The AF structure is indicated. At the critical pressure pc = 2.86 GPa the resistivity shows pronounced NFL behavior ρ(T ) ∼ T n with n = 1.2 down to the superconducting transition (inset). (After Ref. [118].) 125 M. A. Continentino, Brazilian Journal of Physics 35, 197 (2004).

46

P. FULDE ET AL.

mixed-valent compounds in a phenomenological scaling ansatz.126–128 The aim was to explain observed relations between quantities like specific heat, thermal expansion, magnetostriction and others. It is natural to apply these ideas also to the vicinity of the QCP, where the characteristic energies T ∗ (p) and Tc (p) themselves depend on the distance r to the QCP which then appears as a further scaling variable.129 The associated correlation length (ξ ) and time scales of quantum fluctuations (τ ) diverge on approaching the phase transition. Their critical exponents are universal, depending only on dimension and the degrees of freedom of the order parameter. We define the quantities r=

X − Xc , Xc

t=

T − Tc Tc

(X = p or H )

(4.15)

which measure the distance to the critical control parameter Xc and the transition temperature Tc respectively. On approaching the QCP at T = 0, r = 0 the correlation length, fluctuation time and free energy scale like94,125

T H . (4.16) ξ ∼ |r|−ν , τ ∼ |r|−νz , f ∼ |r|2−α f˜ , T ∗ H∗ Here H ∗ has the meaning of ‘metamagnetic’ field scale. For fields H H ∗ the heavy quasiparticle state is destroyed by breaking the Kondo singlet state. For QPTs the hyperscaling relation which relates critical exponents to the effective dimension is given by94 2 − α = νdeff ,

deff = d + z.

(4.17)

In the case of a Gaussian fix point appropriate for deff > 4 one has ν = 12 . In the free energy of Eq. (4.16) which is a generalization of the one used in126–128 the characteristic temperature (T ∗ ) and metamagnetic field (H ∗ ) have scaling relations T ∗ ∼ |r|νz ,

H ∗ ∼ |r|φh .

(4.18)

In the magnetically ordered regime T ∗ has to be replaced by the magnetic transition temperature which scales as Tc ∼ |r|ψ where ψ is the shift exponent. Below the upper critical dimension, i.e., for deff < dc = 4 the hyperscaling relation Eq. (4.17) is equivalent to the assumption ψ = νz.125 In this case Tc (r) and T ∗ (r) 126 R. Takke, M. Niksch, W. Assmus, B. Lüthi, R. Pott, R. Schefzyk, and D. K. Wohlleben, Z. Phys. B

44, 33 (1981). 127 P. Thalmeier and P. Fulde, Europhys. Lett. 1, 367 (1986). 128 A. B. Kaiser and P. Fulde, Phys. Rev. B 37, 5357 (1988). 129 L. Zhu, M. Garst, A. Rosch, and Q. Si, Phys. Rev. Lett. 91, 066404 (2003).

STRONGLY CORRELATED ELECTRONS

47

scale symmetrically around the QCP (Figure IV.6), however for deff > 4 in general one has ψ = νz. This is known as ‘breakdown of hyperscaling’. Within a generalized Landau–Ginzburg–Wilson approach this may be understood as the effect of a dangerously irrelevant quartic interaction. Although it scales to zero for deff > 4, it changes nevertheless the scaling behavior at finite T leading to a modified shift exponent ψ = z/(deff − 2) for deff > dc . From an experimental viewpoint the most interesting aspect is the temperature dependence of physical properties at the QCP (r = 0) in the non-Fermi liquid regime. Very useful quantities are specific heat C = (T /V )(∂S/∂T )p and thermal expansion α = (1/V )(∂V /∂T )p .119,129 At the QCP (r = 0) they scale with temperature like C(T ) ∼ T d/z ,

1

α(T ) ∼ T (d− ν )/z

and =

1 α ∼ T − νz . C

(4.19)

This means that the temperature dependence of the critical ‘Grüneisen ratio’ (r = 0) is controlled by the exponent which directly determines the time scale of quantum fluctuations in Eq. (4.16). Using this important relation a consistent explanation of experiments in the NFL compound CeNi2 Ge2 can indeed be given (Figure IV.7). Tables of the scaling behavior of the quantities in Eq. (4.19) for various d, z have been given in Ref. [129]. The exponent νz determines at the same time pressure scaling (Eq. (4.18)) of the characteristic temperature T ∗ on the nonmagnetic side of the QCP. On the other hand the pressure scaling exponent φh of the characteristic field H ∗ is an independent quantity within the scaling ansatz. Experimentally it has been investigated in detail for CeRu2 Si2 which has a metamagnetic field scale H ∗ (p = 0) = 7.8T (H c). It was found empirically that φh = 2 − α = νz is fulfilled. According to the free energy in Eq. (4.16) this implies with m = (∂f/∂H ) that m(H ∗ ) = const independent of pressure. This was indeed found experimentally.130 The empirical relation 2 − α = νz may be interpreted as quantum hyperscaling relation with dimension d = 0 according to Eq. (4.17). The empirical validity of such a relation points to a dimensional crossover as function of pressure close to the QCP which is caused by the different divergence of spatial and temporal correlations.125 An explicit calculation of scaling exponents close to the QCP demands the use of effective field theories based on Ginzburg–Landau type action functionals for the spatial and temporal order parameter fluctuations. Such theories are not specific for strongly correlated electron systems and therefore are beyond the scope of this review. As mentioned before they have indeed first been constructed for 130 A. Lacerda, A. de Visser, P. Haen, P. Lejay, and J. Flouquet, Phys. Rev. B 40, 8759 (1989).

48

P. FULDE ET AL.

F IG . IV.7. Thermal expansion showing the suppression of NFL behavior as function of field. The inset shows that for B = 0 the critical contribution to the Grüneisen ratio of CeNi2 Ge2 scales like ∼ 1/T νz with νz = 1. According to Eq. (4.19) this means (assuming z = 2 for AF SDW) a mean field correlation length exponent ν = 1/2 which is in agreement with deff = d + z = 5 for the effective dimension. (After Ref. [119].)

weakly correlated metals in Refs. [48,100,101] and Ref. [102] and have been reinvestigated later in hindsight of QPTs in strongly correlated metals.131 Until now the results and even starting assumptions of these field theoretical approaches are controversial and will not be discussed here. V. Partial Localization

The concept of orbital-selective localization applies to correlated systems with orbital degeneracies. Important examples are transition metal oxides132–135 and 5f compounds. In these materials, the intra-atomic correlations as described by Hund’s rules play an important role. Nevertheless the physics of partial localization in transition metal oxides and 5f systems is quite different. In compounds 131 A. J. Millis, Phys. Rev. B 48, 7183 (1993). 132 V. I. Anisimov, I. A. Nekrasov, D. E. Kondakov, T. M. Rice, and M. Sigrist, Eur. Phys. J. B 25,

191 (2002). 133 A. Koga, N. Kawakami, T. M. Rice, and M. Sigrist, Phys. Rev. Lett. 92, 216402 (2004). 134 A. Liebsch, Phys Rev. Lett. 95, 116402 (2005). 135 M. S. Laad, L. Craco, and E. Müller-Hartmann, Europhys. Lett. 69, 984 (2005).

STRONGLY CORRELATED ELECTRONS

49

with d electrons the large crystalline electric field (CEF) set up by the surroundings of a transition metal ion plays a major role. It is often larger than the bandwidth as, for example in the manganites (Section VI.15). In case of a cubic lattice it splits the five d orbitals into a t2g triplet and an eg doublet and the corresponding subbands are well separated. When the Hund’s rule energy is larger than this splitting and when the orbital energy of the t2g is lower than that of the eg states the t2g states will be occupied by the first three d electrons. Those three d electrons remain localized in a high-spin state with S = 3/2. Additional d electrons occupy eg states and remain delocalized. The situation differs when the CEF splitting is larger than Hund’s rule coupling. In that case the t2g subband can accommodate six electrons. When the d electron count per ion nd is larger than six, i.e., nd > 6 only (nd − 6) d electrons will be itinerant and contribute to metallic behavior. In 5f compounds we are facing a different situation. Since the 5f atomic wavefunctions are closer to the nuclei than d electron wavefunctions are, CEF splittings are smaller and less important. But Hund’s rule energies are larger. Therefore when we deal with a situation where the 5f count per actinide ion nf exceeds two, i.e., nf > 2 only those 5f electrons will delocalize which enable the remaining ones to form a Hund’s rule state. Otherwise the Coulomb interaction is increased so much that delocalization is disadvantageous as far as energy is concerned. Therefore Hund’s rule correlations may strongly enhance anisotropies in the kinetic energy and eventually lead to the co-existence of band-like itinerant 5f states with localized atomic-like ones. The central focus of the present section is the dual model for actinide-based heavy fermion compounds which assumes the co-existence of delocalized and localized 5f electrons. Initially, the dual character has been conjectured for UPd2 Al3 where the variation with temperature of the magnetic susceptibility points to the coexistence of CEF-split localized 5f states in a heavy fermion system with 5f -derived itinerant quasiparticles. Direct experimental evidence for the co-existence of 5f -derived quasiparticles and local magnetic excitations is provided by recent neutron scattering experiments.136 There is clear evidence that the presence of localized 5f states is responsible for the attractive interaction leading to superconductivity.137 In addition the dual model could allow for a rather natural description of heavy fermion superconductivity co-existing with 5f -derived magnetism. For a recent review of experimental facts see Refs. [53,54]. Heavy quasiparticles have been observed by de Haas–van Alphen (dHvA) experiments in a number of U compounds. The experiments unambiguously confirm 136 A. Hiess, N. Bernhoeft, N. Metoki, G. H. Lander, B. Roessli, N. K. Sato, N. Aso, Y. Haga, Y. Koike, T. Komatsubara, et al., cond-mat/0411041 (2004). 137 N. Sato, N. Aso, K.. Miyake, R. Shiina, P. Thalmeier, G. Varelogiannis, C. Geibel, F. Steglich, P. Fulde, and T. Komatsubara, Nature 410, 340 (2001).

50

P. FULDE ET AL.

that some of the U 5f electrons must have itinerant character. It has been known for quite some time that the 5f -states in actinide intermetallic compounds cannot be considered as ordinary band states. Standard bandstructure calculations based on the Local Density Approximation (LDA) to Density Functional Theory fail to reproduce the narrow quasiparticle bands. On the other hand the LDA bandwidths are too small to explain photoemission data.138,139 These shortcomings reflect the inadequate treatment of local correlations within ordinary electron structure calculation. Theoretical studies aiming at an explanation of the complex low-temperature structures lay emphasis on the partitioning of the electronic density into localized and delocalized parts.140,141 Concerning the low-energy excitations it has been shown that the dual model allows for a quantitative description of the renormalized quasiparticles—the heavy fermions—in UPd2 Al3 . The measured dHvA frequencies for the heavy quasiparticle portions as well as the large anisotropic effective masses can be explained very well by treating two of the 5f electrons as localized. The central goal of the present section is (1) to demonstrate that the dual model allows to determine the heavy quasiparticles in U compounds without adjustable parameters and (2) to give a microscopic justification for the underlying assumptions. Before turning to a discussion of the dual model, its results and their implications we should like to add a few comments. In referring to the dual model one has to keep in mind that the latter provides an effective Hamiltonian designed exclusively for the low-energy dynamics. As such it seems appropriate for typical excitation energies hω ¯ below ∼ 10 meV. In general, effective low-energy models are derived from the underlying microscopic Hamiltonians—to borrow the language of Wilson’s renormalization group— by integrating out processes of higher energies. In the case of 5f systems the conjecture is that the hybridization between the conduction electrons and the 5f states effectively renormalizes to zero for some channels while staying finite for others. We shall show that the physical mechanism leading to the orbital-dependent renormalization of the hybridization matrix elements are the intra-atomic correlations which are often described by Hund’s rules. To focus on the role of the intra-atomic correlations we consider model Hamiltonians for the 5f subsystem where the hybridization with the conduction 138 J. W. Allen, in Synchrotron Radiation Research: Advances in Surface and Interface Science, Plenum Press, New York (1992), vol. 1, chap. 6, p. 253. 139 S. Fujimori, Y. Saito, M. Seki, K. Tamura, M. Mizuta, K. Yamaki, K. Sato, T. Okane, A. Tanaka, N. Sato, et al., J. Electron Spectrosc. Relat. Phenom. 101–103, 439 (1999). 140 L. Petit, A. Svane, W. M. Temmerman, Z. Szotek, and R. Tyer, Europhys. Lett. 62, 391 (2003). 141 J. M. Wills, O. Eriksson, A. Delin, P. H. Andersson, J. J. Joyce, T. Durakiewicz, M. T. Butterfield, A. J. Arko, D. P. Moore, and L. A. Morales, J. Electron Spectrosc. Relat. Phenom. 135, 163 (2004).

STRONGLY CORRELATED ELECTRONS

51

electrons is accounted for by introducing effective 5f hopping. The orbitaldependent suppression of hybridization then translates into orbital-selective localization. The concept of correlation-driven partial localization in U compounds has been challenged by various authors (see, e.g., Ref. [142]). The conclusions are drawn from the fact that conventional band structure calculations within the Local Density Approximation (LDA) which treat all 5f -states as itinerant can reproduce ground state properties like Fermi surface topologies and densities. The calculation of ground state properties, however, cannot provide conclusive evidence for the delocalized or localized character of the 5f -states in actinides. First, the presence of localized states can be simulated in standard band calculations by filled bands lying (sufficiently far) below the Fermi level. Second, the Fermi surface is mainly determined by the number of particles in partially filled bands and the dispersion of the conduction bands which, in turn, depends mainly on the geometry of the lattice. A change in the number of band electrons by an even amount does not necessarily affect the Fermi surface since a change by an even number may correspond to adding or removing a filled band. As such, the Fermi surface is not a sensitive test of the microscopic character of the states involved. Unambiguous proof of the dual character can be provided by an analysis of the spectral function. Of particular importance are characteristic high-energy features associated with transitions into excited local multiplets. A detailed discussion of these features will be given in Section VIII. 9. H EAVY Q UASIPARTICLES IN UP D 2 A L 3 Within the dual model the strongly renormalized quasiparticles in U -based heavy fermion compounds are described as itinerant 5f electrons whose effective masses are dressed by low-energy excitations of localized 5f states. We refer to Refs. [33,54] for a detailed description which proceeds in three steps. The latter include (a) a band structure calculation to determine the dispersion of the bare itinerant 5f states (b) a quantum chemical calculation which yields the localized 5f multiplet states and, in particular, their coupling to their itinerant counterparts and, finally, (c) a standard (self-consistent) many-body perturbation calculation to determine the renormalized effective mass. We should like to emphasize, however, that we treat all 5f electrons as quantum mechanical particles obeying Fermi anticommutation relations. The scheme has been successfully applied to UPd2 Al3 and UPt3 as can be seen from the comparison between the calculated and measured dHvA frequencies and 142 I. Opahle, S. Elgazzar, K. Koepernik, and P. M. Oppeneer, Phys. Rev. B 70, 104504 (2004).

52

P. FULDE ET AL.

the effective masses in Figure V.1 and Table V.1, respectively. It is important to note that the data are derived from a parameter-free calculation. To show this we examine the individual steps as described above. First, the bare 5f band dispersion is determined from a parameter-free ab initio calculation by solving the Dirac equation for the self-consistent LDA potentials

F IG . V.1. Upper panel: Fermi surface of UPd2 Al3 calculated within the dual model.33 The main cylinder part has effective masses with m∗ = 19–33m, the highest masses are found on the torus. Lower panel: Comparison of experimental dHvA frequencies (black symbols) from Ref. [143] and calculated frequencies (open symbols) (After Ref. [33]). The large parabola corresponds to the main FS cylinder. 143 Y. Inada, H. Yamagani, Y. Haga, K. Sakurai, Y. Tokiwa, T. Hinma, E. Yamamoto, Y. Onuki, and T. Yanagisawa, J. Phys. Soc. Jpn. 68, 3643 (1999).

STRONGLY CORRELATED ELECTRONS

53

TABLE V.1. E FFECTIVE M ASSES IN UP D 2 A L 3 FOR H c. N OTATION FOR FS S HEETS AND E X VALUES FROM R EF. [143], m0 I S THE F REE E LECTRON M ASS . T HEORETICAL VAL UES FROM R EF. [33]

PERIMENTAL

FS sheet

m∗ /m (exp.)

ζ γ β 2 3 β

65 33 19 18 12 5.7

m∗ /m (theory) 59.6 31.9 25.1 17.4 13.4 9.6

but excluding two U 5f (j = 52 ) states from forming bands. The apparent absence of Kramers’ degeneracy in this compound suggests to treat an even number of 5f electrons as localized. The calculations yield the dHvA frequencies which can be directly compared with experimental data. At this point we should like to briefly comment on the strategy to account for long-range antiferromagnetic order. The two examples, UPd2 Al3 and UPt3 , represent two different categories. In UPd2 Al3 localized 5f moments order antiferromagnetically at TN 14.5 K with the induced moment being 0.83μB per U. The heavy quasiparticles form in the magnetically ordered state. As a consequence, the calculation of the bare 5f bands employs the experimentally observed antiferromagnetic structure. The superstructure strongly affects the Fermi surface topology for the heavy quasiparticles. The corresponding paramagnetic model cannot reproduce the heaviest orbit. In the second step, the localized U 5f states are calculated by diagonalizing the Coulomb matrix in the restricted subspace of the localized 5f states. Assuming the j -j coupling scheme, the Coulomb matrix elements are evaluated using the radial functions of the ab initio band structure potentials. The coupling between the localized and delocalized 5f electrons is directly obtained from the expectation values of the Coulomb interaction in the 5f 3 states. Finally, the renormalization of the effective masses which results from the coupling between the two 5f subsystems is estimated. The itinerant 5f states scatter off the low-energy excitations of the localized 5f 2 configurations. The situation resembles that in Pr metal where a mass enhancement of the conduction electrons by a factor of 5 results from virtual crystal field (CEF) excitations of localized 4f 2 electrons.144 The effective masses in Table V.1 are obtained from an isotropical renormalization of the band mass mb is given by m∗ ∂ |ω=0 . =1− mb ∂ω 144 R. White and P. Fulde, Phys. Rev. Lett. 47, 1540 (1981).

(5.1)

54

P. FULDE ET AL.

F IG . V.2. Self-energy diagram due to local intra-atomic excitations leading to a mass enhancement. Solid double line: full Green’s function of the conduction electrons. Dashed lines: effective intra-atomic two-level states |α, |β separated by an excitation energy δ¯ = 7 meV. Triangles: matrix elements a|M|.

The local self-energy of the delocalized 5f states (ω) is displayed in Figure V.2. The explicit expressions are given in.33 The mass enhancement is calculated selfconsistently inserting values for the density of states at the Fermi level N (0) = 2.76 states/(eV cell spin) obtained from the bandstructure, when two 5f electrons are kept localized. The vertex is given by a|M| = 0.084 eV where the prefactor a denotes the 5f weight per spin and U atom of the conduction electron states near EF . The matrix element M describes the transition between the localized states |4 and |3 due to the Coulomb interaction UCoul with the delocalized 5f electrons. These are the two lowest eigenstates of the localized 5f 2 system in the presence of the CEF. They have J = 4 in accordance with Hund’s rule and are combinations of |Jz = | ± 3. Finally, the dynamical susceptibility is approximated by that of an effective two-level system with an excitation energy δ¯ 7 meV. 10. M ICROSCOPIC M ODEL C ALCULATION To illustrate the orbital selection by intra-atomic correlations we consider a simple molecular model consisting of two actinide atoms at sites a and b. The strong Coulomb interaction among the 5f electrons at the same site leads to well-defined ionic configurations f n with energies E(f n ). To model U compounds we assume that the total number of 5f electrons in the cluster be five corresponding to an averaged f -occupation of 2.5 per U site. The ground state will be a linear combination of states |a; f 3 |b; f 2 and |a; f 2 |b; f 3 , respectively. These two sets of states are coupled by the hopping term. Since both atoms have more than one

STRONGLY CORRELATED ELECTRONS

55

electron in their 5f shells intra-atomic correlations come into play. The two sets of basis functions split into groups of states characterized by the total angular momenta J (a) and J (b), respectively, the energy differences being of the order of the 5f exchange constant, i.e., approximately 1 eV. Since the spin-orbit interaction is large we use j -j coupling and restrict ourselves to 5f states with j = 5/2. We are aiming at the low-energy subspace which is spanned by the states |a; f 3 , J (a) = 9/2|b; f 2 , J (b) = 4 and |a; f 2 , J (a) = 4|b; f 3 , J (b) = 9/2, in close analogy to Hund’s rules. Transferring an electron from site a to site b changes the local f occupation and the total angular momenta a; f 3 , J (a) = 9/2 b; f 2 , J (b) = 4 → a; f 2 , J (a) b; f 3 , J (b) (5.2) and the resulting final state will usually contain admixtures from excited multiplets. The transfer of a 5f electron from site a to site b causes intra-atomic excitations against which the gain in kinetic energy has to be balanced. The crucial point is that the overall weight of the low-energy contributions to the final state depends upon (a) the orbital symmetry of the transferred electron, i.e., on jz and (b) on the relative orientation of J(a) and J(b). The latter effect closely parallels the “kinetic exchange” well-known from transition metal compounds. The requirement that the gain in energy associated with the hopping be maximal leads to orbital selection. The dynamics in the low-energy subspace is described by an effective single-particle Hamiltonian where some of the transfer integrals are renormalized to zero while others are reduced yet remain finite. These qualitative considerations are the basis for microscopic model calculations which proceed from the simple model Hamiltonian H = Hband + HCoul . The local Coulomb repulsion part 1

HCoul = Ujz1 ,jz2 jz3 jz4 cj†z (a)cj†z (a)cjz3 (a)cjz4 (a) 1 2 2 a

(5.3)

(5.4)

jz1 ,...,jz4

is written in terms of the usual fermionic operators cj†z (a) (cjz (a)) which create (annihilate) an electron at site a in the 5f -state with total angular momentum j = 5/2 and z-projection jz . Considering the fact that the spin-orbit splitting is large we neglect contributions from the excited spin-orbit multiplet j = 7/2 and adopt the j -j coupling scheme. The Coulomb matrix element Ujz1 jz2 jz3 jz4 for jzi = −5/2, . . . , 5/2

J Jz JJ Ujz1 jz2 jz3 jz4 = UJ C5/2,j C z (5.5) z1 ;5/2,jz2 5/2,jz3 ;5/2,jz4 J ... and the Coulomb are given in terms of the usual Clebsch–Gordan coefficients C... parameters UJ . Here J denotes the total angular momentum of two electrons

56

P. FULDE ET AL.

and Jz = jz1 + jz2 = jz3 + jz4 . The sum is restricted by the antisymmetry of the Clebsch–Gordan coefficients to even values J = 0, 2, 4. The kinetic energy operator describes the hopping between all pairs at neighboring sites ab

tjz cj†z (a)cjz (b) + h.c. + f cj†z (a)cjz (a). (5.6) Hband = − ab,jz

a,jz

We assume the transfer integrals tjz to be diagonal in the orbital index jz . While this is certainly an idealization it allows us to concentrate on our main interest, i.e., the interplay of intra-atomic correlations and kinetic energy. Finally, we account for the orbital energy f which determines the f -valence of the ground state. Due to the local degeneracy, the Hilbert space increases rapidly with the number of lattice sites and exact (numerical) solutions are possible only for relatively small clusters. For extended systems, i.e., for periodic solids the ground state and the low-lying excitations can be determined within a mean-field approximation.145 The slave-boson functional integral method allows for a discussion of various ground states and co-operative phenomena starting from realistic bare electronic band structures. The orbital-dependent separation of the low-energy excitations into dispersive quasiparticle bands and incoherent background is observed in the spectral functions of a linear chain calculated by means of Cluster Perturbation Theory.146 Itineracy is reflected in a discontinuity of the orbital-projected momentum distribution function (5.7) njz (k) = dω f (ω)Ajz (k, ω) where Aj z (k, ω) is the single-particle spectral function while f (ω) denotes the Fermi distribution. Here we discuss the qualitative features derived for two-site clusters where we can find simple approximate forms for the ground-state wavefunction in limiting cases. In order to quantify the degree of localization or, alternatively, of the reduction of hopping of a given jz orbital by local correlations, the ratio of the jz -projected kinetic energy Tjz and the bare matrix element tjz

Tjz = gs | cj†z (a)cjz (b) + h.c. |gs (5.8) tjz ab,

The ground-state wavefunction |gs contains the strong on-site is correlations. A small ratio of Tjz /tjz indicates partial suppression of hopping for electrons in the ±jz orbitals. Two kinds of correlations may contribute to that calculated.33

145 J. Jedrak and G. Zwicknagl, preprint (2005). 146 F. Pollmann, and G. Zwicknagl, Phys Rev. B 73, 035121 (2006).

STRONGLY CORRELATED ELECTRONS

57

process. The first one is based on the reduction of charge fluctuations due to the large values of the isotropically averaged Coulomb repulsion which results in an isotropic renormalization of the kinetic energy. As this is a typical high-energy effect we defer the discussion to Section VIII. In the strong-coupling limit the reduction of charge fluctuation is accounted for by restricting the ground state to the well-defined atomic configurations. The quantity of interest here is the orbitaldependent reduction Tjz /tjz which is due to intra-atomic correlations. As the latter are local in nature, even small clusters should adequately describe the important qualitative features. The results for Tjz /tjz 33 —initially obtained perturbatively for a two-site cluster—as well as their interpretation are confirmed by detailed calculations based on exact diagonalization for small clusters.147 Figure V.3 displays the reduction factors for a two-site cluster. The model parameters U4 = UJ =4 − UJ =0 = −3.79 eV U2 = UJ =2 − UJ =0 = −2.72 eV.

(5.9)

are chosen appropriate for UPt3 . These findings demonstrate that in particular Hund’s rule correlations strongly enhance anisotropies in the hopping. For a certain range of parameters this may result in a complete suppression of the effective hopping except for the largest one, which remains almost unaffected. This provides a microscopic justification of partial localization of 5f electrons which is observed in a number of experiments on U intermetallic compounds. As the relevant correlations are local, the general results qualitatively agree with those found for a three-site cluster and four-site clusters.148 The magnetic character, however, is affected by finite size effects. This can be seen by varying the cluster sizes and the boundary conditions. Although the total angular momentum component Jz may be different for periodic and open boundary conditions we can identify the following different regimes in the strong-coupling limit. In the strongly anisotropic limit with dominating transfer integral |t3/2 | |t1/2 | = |t5/2 | the high-spin states with ferromagnetic inter-site correlations are energetically most favorable. In the two-site cluster, the ground state has a very simple form

1 t † † † † † † | = √ c3/2 (a) + c3/2 (b) c5/2 (a)c1/2 (a)c5/2 (b)c1/2 (b)|0 |t| 2

(5.10)

being simultaneously an eigenstate of the Coulomb energy and of the kinetic energy. It can be considered as a bonding jz = 3/2 state in a ferromagnetically aligned background. The high-spin phases are followed by complicated 147 D. V. Efremov, N. Hasselmann, E. Runge, P. Fulde, and G. Zwicknagl, Phys. Rev. B 69, 115114 (2004). 148 M. Reese, F. Pollmann, and G. Zwicknagl (2006), unpublished.

58

P. FULDE ET AL.

F IG . V.3. Left panel: Values Tjz /tjz for a two-site cluster along a line connecting linearly the points written below the figure. (After Ref. [147].) Right panel: Variation with wave number of (Ajz (k , ω) + A−jz (k , ω)) in the low-energy regime calculated for a two-site cluster with five electrons. The corresponding values of the transfer integrals are those of the left panel. The full line and the dotted line refer to k = 0 and k = π , respectively. Spectral weight is transferred to local excitations (valence transitions and transitions into excited atomic multiplets) which are not displayed here. The Lorentzian broadening is η = 0.03 (After Ref. [146].)

intermediate-spin phases as the isotropic limit t1/2 = t3/2 = t5/2 is approached. In the case with subdominant |t3/2 | |t1/2 | = |t5/2 | low-spin phases with antiferromagnetic intersite correlations are formed. In a two-site cluster, they involve linear combinations of † † † † † (a)c±5/2 (a)c±3/2 (a)c∓5/2 (b)c∓1/2 (b)|0, c1/2 † † † † c±5/2 (a)c±3/2 (a)c∓5/2 (b)c1/2 (b)|0.

The splitting of the low-energy excitations into dispersive quasiparticle states and incoherent background is reflected in the single-particle spectral functions Ajz (k , ω) where the discrete set of quantum numbers k = 0, π labels the singleparticle eigenstates of the two-site cluster. The variation with the transfer integrals is displayed in Figure V.3. The jz -channels with dominant hopping exhibit dispersive narrow peaks while those with subdominant hopping yield an incoherent background. Considerable spectral weight is transferred to the high-energy excitations not shown here.

STRONGLY CORRELATED ELECTRONS

59

11. S UPERCONDUCTIVITY M EDIATED BY I NTRA -ATOMIC E XCITATIONS Since the discovery of the isotope effect149,150 and the work of Fröhlich151 the electron–phonon interaction has been considered the main cause of Cooper-pair formation. By exchanging virtual phonons, electrons may attract each other and form Cooper pairs. Later it was pointed out that phonons need not be the only bosons the exchange of which results in electron attraction. Also magnetic excitations such as paramagnons were considered as candidates for generating superconductivity, although not necessarily in a conventional s-wave pairing state.97,152 Also it had been pointed out that crystalline electric field (CEF) excitations in rareearth ions like Pr have a pronounced effect on superconductivity153–155 when such ions are added to a conventional superconductor and furthermore, that those excitations can be either pair-breaking or pair forming depending on matrix elements between different CEF levels. The experimental observation of those effects, e.g., in doped LaPb3 and LaSn3 156,157 demonstrated not only the reality but also the magnitude of that kind of boson exchanges between conduction electrons. After the discovery of high-temperature superconductivity in some of the cuprate perovskites and even before for some of the heavy-fermion superconductors numerous suggestions of non-phononic pairing interactions were made.158–166 But they were mainly qualitative rather than quantitative and therefore remained inconclusive. For reviews see Refs. [54,167]. Therefore it is of interest that for UPd2 Al3 experimental evidence exists for a non-phononic mechanism causing superconductivity. It has a transition temperature Tc of Tc = 1.8 K; which is 149 E. Maxwell, Phys. Rev. 78, 477 (1950). 150 C. A. Reynolds, B. Serin, W. H. Wright, and L. B. Nesbitt, Phys. Rev. 78, 487 (1950). 151 H. Fröhlich, Phys. Rev. 79, 1950 (845). 152 D. Fay and J. Appel, Phys. Rev. B 16, 2325 (1977). 153 P. Fulde, L. L. Hirst, and A. Luther, Z. Phys. 238, 99 (1970). 154 J. Keller and P. Fulde, J. Low Temp. Phys. 4, 289 (1971). 155 J. Keller and P. Fulde, J. Low Temp. Phys. 12, 63 (1973). 156 F. Heiniger, E. Bucher, J. P. Maitra, and L. D. Longinotti, Phys. Rev. B 12, 1778 (1975). 157 R. W. McCallum, W. A. Fertig, C. A. Luengo, M. B. Maple, E. Bucher, J. P. Maitra, A. R.

Schwedler, L. Mattix, P. Fulde, and J. Keller, Phys. Rev. Lett. 34, 1620 (1975). 158 D. J. Scalapino, E. Loh, and J. E. Hirsch, Phys. Rev. B 34, 8190 (1986). 159 K. Miyake, S. Schmidt-Rink, and C. M. Varma, Phys. Rev. B 34, 6554 (1986). 160 P. W. Anderson, Science 235, 1196 (1987). 161 J. Spalek, Phys. Rev. B 38, 208 (1988). 162 T. Moriya, Y. Takahashi, and K. Ueda, J. Phys. Soc. Jpn. 59, 2905 (1990). 163 P. Monthoux, A. V. Balatsky, and D. Pines, Phys. Rev. Lett. 67, 3448 (1991). 164 P. Monthoux and G. G. Lonzarich, Phys. Rev. B 59, 14598 (1999). 165 P. Monthoux and G. G. Lonzarich, Phys. Rev. B 63, 054529 (2001). 166 P. Monthoux and G. G. Lonzarich, Phys. Rev. B 66, 224504 (2002). 167 N. M. Plakida, High-Temperature Superconductivity, Springer, Berlin, Heidelberg (1995).

60

P. FULDE ET AL.

below the onset of antiferromagnetic (AF) order with a Néel temperature of TN = 14.3 K. Some evidence for a non-phononic pairing mechanism is provided by UPd2 Al3 –Al2 O3 –Pb tunneling measurements.168 The differential conductivity dI /dV shows structure in the regime of 1 meV demonstrating that there are low-energy bosons which result in a frequency dependence (ω) of the order parameter. For phonons this structure would be an order of magnitude higher in energy. The Debye energy of UPd2 Al3 is 13 meV. In addition inelastic neutron scattering (INS) experiments show that the CEF based magnetic excitation energy ωE (q) at q = Q is between 1–1.5 meV depending on temperature.136,137,169,170 It has been argued that these excitations show up in (ω) and cause superconductivity. This is seen in Figure V.4 which shows the INS data as well as the tunneling density of states. The strong coupling of those AF excitons to conduction electrons is also demonstrated in these experiments. The AF structure of UPd2 Al3 consists of ferromagnetic hexagonal planes with a moment of μ = 0.83μB per U ion pointing in [100] direction and stacked antiferromagnetically along the c-axis.171,172 This corresponds to an AF wave vector Q = (0, 0, 1/2). The large moment supports the dual model with two localized 5f electrons. As discussed before the Hund’s rule ground-state multiplet of the 5f 2 localized electrons is J = 4. In a CEF only the two lowest singlets |3 and |4 have to be taken into account. The Hamiltonian is then of the form

† H= kσ ckσ ckσ + δ |4 4 |i kσ

− Jff

i

Ji Jj − 2I0 (geff − 1)

ij

si Ji

(5.11)

i

where kσ = ⊥ (k⊥ σ ) − 2t cos kz

(5.12)

serves as a model for the Fermi surface of UPd2 Al3 in the paramagnetic state. Figure V.3 shows that the Fermi surface in the AF state consists of a cylindrical part and a torus. The torus has the highest effective mass. For simplicity we will neglect it here and model the paramagnetic Fermi surface by a cylinder. The 168 M. Jourdan, M. Huth, and H. Adrian, Nature 398, 47 (1999). 169 N. Sato, N. Aso, G. H. Lander, B. Roessli, T. Komatsubara, and Y. Endoh, J. Phys. Soc. Jpn. 66,

1884 (1997). 170 N. Bernhoeft, N. Sato, B. Roessli, N. Aso, A. Hiess, G. H. Lander, Y. Endoh, and T. Komatsubara,

Phys. Rev. Lett. 81, 4244 (1998). 171 A. Krimmel, P. Fischer, B. Roessli, H. Maletta, C. Geibel, C. Schank, A. Grauel, A. Loidl, and F. Steglich, Z. Phys. B 86, 161 (1992). 172 H. Kita, A. Dönni, Y. Endoh, K. Kakurai, N. Sato, and T. Komatsubara, J. Phys. Soc. Jpn. 63, 726 (1994).

STRONGLY CORRELATED ELECTRONS

61

F IG . V.4. Upper panel: Magnetic exciton dispersion from INS along c∗ (0, 0, ql ) and a ∗ (qh , 0, 0.5) around the AF zone center Q = (0, 0, 0.5) for T = 2 K just above Tc = 1.8 K. A flat dispersion with a corresponding high DOS is observed for q Q. For T < Tc the additional quasielastic response (open circles at zero energy) evolves into sharp resonance peaks within the gap. (After Ref. [136].) Lower panel: Differential conductivity dI /dV for tunneling current along c. The additional hump at V 1.5 meV has been associated with the magnetic exciton mode at Q in the upper panel. This feature is due to a frequency dependent gap (ω) caused by a strong coupling of quasiparticles to magnetic excitons. However the evaluation of the tunneling data needs additional justification (J. Geerk, private communication). (After Ref. [168].)

antiferomagnetic coupling to the conducting electrons is considerably larger than in systems like TbMo6 S8 173 and HoNi2 B2 .174 One should also keep in mind that 173 M. Ishikawa and Ø. Fischer, Solid State Comm. 24, 747 (1977). 174 A. Amici, P. Thalmeier, and P. Fulde, Phys. Rev. Lett. 84, 1800 (2000).

62

P. FULDE ET AL.

in accurate determination of Tc is anyway out of reach and that the aim is here to demonstrate that the non-phononic pairing mechanism yields the right order of magnitude for Tc . Returning to Eq. (5.12) we note that t determines the amount of corrugation of the cylinder. The second term in Eq. (5.11) denotes the CEF splitting with δ = 6–7 meV. The coupling between localized 5f electrons on nearest-neighbor sites is given by Jff and the on-site exchange between localized and itinerant electrons is described by the last term of Eq. (5.11). The effective Landé factor geff refers to the localized 5f electrons. The total intersite exchange is therefore J (q) = Jeff (q) + I02 (geff − 1)2 χe (q)

(5.13)

where χe (q) is the spin susceptibility of the itinerant electrons. Due to that intersite interaction the susceptibility of the system becomes χ(q, ω) =

u(ω) 1 − J (q)u(ω)

(5.14)

where u(ω) is the single-ion susceptibility175 and the CEF excitation energy goes over into an excitation band (magnetic exciton). When J (q) has its maximum value at q = Q and J (Q) ≡ Je exceeds a critical value, i.e., Je > Jcrit the system becomes an induced AF. In that case the Néel temperature TN is given by TN =

δ 2

tanh−1 (J

c /Je )

.

(5.15)

UPd2 Al3 is an induced AF and one finds that Je /Jc = 1.015. The critical value is given by Jc = δ/2M 2 where M = 24 |Jx |3 i . For temperatures T < TN the susceptibility is again of a form similar to Eq. (5.14) but now the single-ion susceptibility contains the effect of the AF molecular field acting on the |4 , |3 states. In that case the magnetic excitations form a band of AF magnons. For a review see, e.g., Refs. [109,176]. They have originally been measured177 with relatively low resolution and later with much better one, see Refs. [136,137] and [178]. Their dispersion has also been derived theoretically in Ref. [179] by in175 B. R. Cooper, Phys. Rev. 163, 444 (1967). 176 J. Jensen and A. R. Mackintosh, Rare Earth Magnetism, Structures and Excitations, Clarendon

Press, Oxford (1991). 177 T. E. Mason and G. Aeppli, Matematisk-fysiske Meddelelser. 45, 231 (1997). 178 N. Bernhoeft, Eur. Phys. J. B 13, 685 (2000). 179 P. Thalmeier, Eur. Phys. J. B 27, 29 (2002).

STRONGLY CORRELATED ELECTRONS

63

cluding the molecular field as well as the anisotropic exchange and agreed nicely with the measured ones. An approximate form is (5.16) ωE (qz ) = ωex 1 + β cos(cqz ) with ωex = 5 meV, β = 0.8 and c denoting the lattice constant perpendicular to the hexagonal planes. The corresponding boson propagator K(qz , ων ) in Matsubara frequency notation (ων = 2πT , ν = integer) replaces the phonon propagator when the superconducting properties are calculated.180 It is of the form K(qz , ων ) = g

2 ωex (ωE (qz ))2 + ων2

(5.17)

where g denotes the coupling constant between conduction electrons and magnetic excitons. Their interaction Hamiltonian Hc−f can be written in a pseudospin notation by introducing for the two levels |3 i and |4 i of a U site i the + 1 pseudospin τ i , so that τiz |3(4) i = (−) 2 |3(4) i . Then we may write

Hc−f = I σiz τix (5.18) i

where σi refers to the itinerant 5f electron. The two coupling constants g and I are related through

I 2 1 p02 1 (5.19) g= 4 c 2π ωex where p0 is the radius of the circle in the px , py plane which contains the same area as the hexagon defining the Brillouin zone. We are now in the position to write down and solve Eliashberg’s equations for the conduction electron self-energy (pz , ωn ) and order parameter (pz , ωn ). (pz , ωn ) =

dp⊥ T

K(pz − pz ; ωn − ωm ) G(p⊥ , pz , ωm ) Nz (2π)2 pz ,m

(pz , ωn ) = −

T

K(pz − pz ; ωn − ωm )(pz , ωm ) Nz

×

pz ,m

dp⊥ G(p , p , ωm )2 ⊥ z 2 (2π)

180 P. McHale, P. Fulde, and P. Thalmeier, Phys. Rev. B 70, 014513 (2004).

(5.20)

64

P. FULDE ET AL.

where Nz is the number of lattice sites along the z-axis and ωn = 2πT (n + 1/2). It has been assumed that the order parameter has even parity (singlet channel). The electron Green function has the usual form G−1 (p, ωn ) = iωn − p − (pz , ωn )

(5.21)

with p given by Eq. (5.12). integration in Eq. (5.20) has been done the equations reduce After the dp⊥ to a one-dimensional problem. Thereby it is essential that the kernel K(qz , ων ) is strongly peaked at qz = π/c and ων = 0. Therefore, loosely speaking the gap equation is of the form

π (pz , πT ) = −C(pz ) pz − , πT (5.22) c where C(pz ) is a smooth positive function. This suggests the form (p) = cos(cpz )

(5.23)

with A1g symmetry. The symmetry allows also for a multiplication of the righthand side by a fully symmetric function f (px , py ). The order parameter has lines of nodes at the AF zone boundary pz = ±Qz /2 = ±π/(2c). One finds that Eliashberg’s equations yield also an odd-parity solution of the form (pz ) = sin(cpz )

(5.24)

|χ = (2)−1/2 (|↑ ↓ + |↓ ↑)

with a spin part and the same Tc . Note that because of the Ising-like interaction (5.18) rotational symmetry in spin space is broken. A more general study of possible order parameters due to pair potentials based on magnetic excitons was undertaken in Ref. [179]. It turned out that in the weak coupling limit, i.e., without taking retardations into account, one of the odd-parity triplet states has lower energy than the singlet one. However this could be a consequence of the weak coupling assumption which does not apply to UPd2 Al3 . There is strong experimental evidence discussed below that the order parameter has indeed A1g symmetry (see Eq. (5.23)) and therefore we discard the A1u solution (5.24). In the following we discuss the parameters which are required within this simplified model to explain the anisotropic effective mass and the ones which are needed to explain the observed Tc . For the DOS at the Fermi energy a value of N (EF ) 2 states/(eV-cell-spin) seems appropriate. This includes also the torus. The local intra-atomic excitations responsible for the mass enhancement are characterized by δ 7 meV33 and ωex 5 meV.180 With these values it turns out that a value of I 2 N (EF ) = 0.026 eV

(5.25)

STRONGLY CORRELATED ELECTRONS

65

F IG . V.5. Left panel: The dependence of the superconducting Tc on the electron-magnetic exciton coupling constant g (Eq. 5.19). Parameter values are ωex = 0.01⊥ , α = −0.1, β = 0.8. The full curve corresponds to opposite spin pairing states |χ (Sz = 0) A1g and A1u with gap functions given in Eqs. (5.23), (5.24) and node lines at kz = ± πc and kz = 0 respectively. The dashed curve is a less favorable state with |Sz | = 1 and more node lines. For a value g/⊥ ∼ 2 which leads to the observed mass enhancement m∗ /mb 10 one obtains a calculated Tc 2.9 K (from the full curve). This value is somewhat larger than the experimental Tc = 1.8 K. (After Ref. [180].)

corresponding to g/⊥ = 2 is required in order to reproduce the experimentally observed mass enhancement within the simplified scheme applied to Eliashberg’s equations. With this value a superconducting transition temperature Tc = 2.9 K is obtained while the true value is 1.8 K. The dependence of the superconducting Tc on the dimensionless coupling strength g/⊥ is shown in Figure V.4. Taking into account that the strong mass anisotropies were derived theoretically without adjustable parameters (see Table V.1) it is gratifying to find that when the parameter I 2 N (EF ) (or g/⊥ ) of a simplified model is adjusted so as to reproduce the mass anisotropies, a superconducting transition temperature of the right order of magnitude is obtained. As regards the experimental situation the superconducting state of UPd2 Al3 has been studied in great details for which we refer to the review Ref. [54]. Here we point out merely those experiments which allow for a determination of the symmetry of the order parameter. This applies in particular to the studies of the anisotropic thermal conductivity in an applied magnetic field. As pointed out in Ref. [181] measurements of the thermal conductivity under rotating magnetic field with heat current perpendicular to the rotation plane yield information on 181 K. I. T. Watanabe, Y. Kasahara, Y. Haga, Y. Onuki, P. Thalmeier, K. Maki, and Y. Matsuda, Phys.

Rev. B 70, 184502 (2004).

66

P. FULDE ET AL.

the k-space position of gap nodes. Corresponding measurements on single crystals of UPd2 Al3 181 and their analysis182 have indeed shown that (p) has node lines perpendicular to the c-axis. However these experiments cannot distinguish π at the AF zone boundary or at pz = 0 at the zone between a node line at pz = ± 2c center, i.e., which one of the theoretically favored gap functions of Eq. (5.23) or Eq. (5.24) is realized. Other evidence for node lines was pointed out by Bernhoeft.178 He argued that the symmetry property (p ± Q) = −(p) is required in order to explain the large intensity of a low energy quasiparticle-like peak in the inelastic neutron scattering spectrum below Tc . This again implies a line of nodes perpendicular to the c axis but cannot distinguish between the two candidates. However already before these results became available a pronounced Knight shift reduction below Tc was found in UPd2 Al3 .183 A naive interpretation of this result advocates for the even parity A1g gap function in Eq. (5.23) whose antisymmetric spin function corresponds to the spin singlet state in models with isotropic pairing interaction. In concluding this section we want to summarize the above findings. It has been shown that in UPd2 Al3 superconductivity is due to non-phononic bosons. Intraatomic excitations of localized 5f electrons in U ions, a consequence of strong correlations and described within the dual model provide the glue for the Cooper pairs. We want to stress that their interaction with the itinerant 5f electrons (see Eq. (5.18)) is not time-reversal invariant. Nevertheless Cooper pairs may form but a sign change of the order parameter along the c-direction is mandatory. Otherwise the interaction would not be pair forming but rather act as a pair breaker. It is likely that a similar pairing mechanism, mediated by the exchange of quadrupolar excitons, is operative in the Pr-skutterudite cage compound. VI. Charge Ordering

The concept of charge order in electronic systems was introduced by Wigner in the early 1930s.9 He considered a homogeneous electron gas, i.e., a system in which the positively charged background is distributed uniformly over the sample. Wigner showed that in the limit of low densities the Coulombic repulsion energy between the electrons will always dominate their gain in kinetic energy due to delocalization. Therefore at sufficiently low temperatures electrons will form a lattice. This way they minimize their mutual repulsions. Following the original proposal of Wigner a number of systems have been discovered which show electronic charge order. The cleanest realization of Wigner 182 P. Thalmeier, T. Watanabe, K. Izawa, and Y. Matsuda, Phys. Rev. B 024539, 72 (2005). 183 Y. Kitaoka, H. Tou, K. Ishida, N. Kimura, Y. Onuki, E. Yamamoto, Y. Haga, and K. Maezawa,

Physica B 281–282, 178 (2000).

STRONGLY CORRELATED ELECTRONS

67

crystallization is observed in a classical 2D sheet of electrons generated on a liquid-He surface where the electron density can be varied by an applied electrical field.184 In constrained geometries like quantum dots clear signatures of Wigner crystallization may be found already for small electron numbers.185 The most common systems which exhibit this type of electronic charge order have an underlying atomic lattice as an important ingredient in distinction to Wigner’s homogeneous positive background. When valence electrons are situated close to an atomic nucleus the overlap with orbitals from neighboring sites is expected to be small. This implies that the associated kinetic energy gain is small when electrons delocalize. Therefore the mutual repulsions between electrons on neighboring sites will dominate the kinetic energy gain at a higher density than it is the case for a uniformly distributed positive background. But a resulting electronic charge order must here be commensurate with the underlying atomic lattice. The 3d-valence electrons of transition metal compounds are most amenable to this kind of charge order. The latter may occur within a metallic (or at least conducting) state as in the prominent example of magnetite Fe3 O4 or within an already insulating state as in α -NaV2 O5 . Since the number of d-electrons in 3dcompounds may commonly be changed by doping, a large variety of commensurate 3d-charge ordered states can be achieved, for example in the cuprate (parent compound LaCu2 O4 ) and single layer and bilayer manganite families (parent compound LaMnO3 and half-doped compound LaSr2 Mn2 O7 , respectively). The amplitude of the total charge order parameter or charge disproportionation on the inequivalent 3d-sites is typically small of the order 0.1 electron per site or less. This is due to the screening of the large 3d-orbital occupation changes by the valence electrons of ligands, as can be clearly seen from LSDA+U calculations. Experimentally the amount of charge disproportionation is extremely difficult to determine. This is mostly done via the empirical valence-bond analysis of X-ray results in the ordered phase, where the change in bond distances is linked to the valence charge disproportionation. In some 3d-oxide compounds like, e.g., the bilayer-manganites one must be aware that 3d-charges are dressed by strong distortions of the surrounding lattice leading to (small) polaron formation. It is then the latter which exhibit the ordering transition. Charge ordering is less common in 4f -compounds, because the intersite Coulomb interaction necessary for charge order is well screened and in genuine metallic compounds the hybridization with conduction electrons tends to favor a site-independent 4f -occupation. This leads to a metallic mixed-valent or heavy fermion state. There is however an important case where 4f -charge order may occur. In insulating or semimetallic 4f compounds which are homogeneous valence fluctuators at high temperatures, the intersite Coulomb interaction may be 184 G. Adams, Phys. Rev. Lett. 42, 795 (1979). 185 A. V. Filinov, M. Bonitz, and Y. E. Lozovik, Phys. Rev. Lett. 17, 3851 (2001).

68

P. FULDE ET AL.

strong enough to lead to a 4f -charge disproportionation, i.e., an inhomogeneous mixed-valent state at low temperatures with different 4f -orbital occupations on inequivalent sites. Again the amplitude of the total charge order including the effect of ligand screening charges is much smaller than the bare 4f -charge disproportionation. An important class of compounds where this charge-order (CO) transition occurs are members of the R4 X3 series (R = rare earth Yb, Sm, Eu and X = As, Bi, P, Sb), notably the semimetal Yb4 As3 discussed in Section VI.13. An attractive feature of CO transitions in these 3d or 4f compounds is the possibility of lowering the effective dimension of the arrangement of magnetic ions, for example to a family of 1D chains, planes of zig-zag chains or ladders and stripes. The effect of low dimensionality has then important consequences for the spin excitation spectrum, e.g., the appearance of a two-spinon continuum in the case of spin chains. When this type of electronic charge order in 3d and 4f systems is compared with the original suggestion of Wigner one notices two differences. As pointed out before, the lattice structure of the positive background is very important but also the repulsions between electrons on neighboring sites are not purely Coulombic. Instead they may be modified due to the electrons in inner closed shells which leads to strongly screened Coulomb interactions that usually extend only to nearest and next nearest neighbors. Another type of charge ordering which does not break spatial symmetries is obtained in systems which can be described by a Hubbard Hamiltonian at half filling. Here it is the on-site Coulomb interaction expressed by an energy U which is competing with electron hopping processes and the associated energy gain. While the repulsion energy U favors single occupancy of sites, and suppresses double occupancies the kinetic energy gain favors a sizeable fraction of sites with double occupations. Without electron correlations 25% of them would be doubly occupied in order to optimize the kinetic energy. For sufficiently large values of U charge order in the form of strongly suppressed on-site charge fluctuations will take place leading to a Mott–Hubbard metal to insulator (M-I) transition. Again, similarities to the previously considered cases are obvious but so are the differences. Repulsions between electrons on different sites are completely neglected in the Hubbard model and it is crucial to have precisely one electron per site in order to obtain charge order. A similar requirement does not exist in the previously considered cases. Finally, charge order can also occur via formation of a charge density wave (CDW) in metals. In this case the instability is driven by minimizing the kinetic (band) energy of conduction electrons leading to a reconstruction of the Fermi surface. A prerequisite is the presence of nesting properties in the Fermi surface. The generally incommensurate vector Q which connects the nesting parts determines wavelength and direction of a corresponding CDW. Note that strong elec-

STRONGLY CORRELATED ELECTRONS

69

tron correlations are not required for a CDW to form. Summarizing we distinguish between the following electronic charge ordering processes: (a) (b) (c) (d) (e)

Wigner crystallization in the homogeneous electron gas or liquid Charge order due to weak hybridizations and strong intersite interactions Mott–Hubbard charge order due to strong on-site interaction Charge density waves due to nesting properties of the Fermi surface Charge ordering in polaronic systems

In this overview we will not address the genuine Mott–Hubbard M-I transition which is reviewed in existing articles, e.g., Ref. [186]. It demands a considerable technical effort based on the recently developed dynamical mean field theory (DMFT). Low dimensional metallic CDW systems will also not be included, since this topic is well represented in the literature187 and should be discussed together with spin-density waves and superconductivity which is beyond the scope of this chapter. 12. W IGNER C RYSTALLIZATION IN H OMOGENEOUS 2D E LECTRON S YSTEMS The electron gas may be subject to many different instabilities depending both on the background (lattice) potential and the resulting shape of the Fermi surface as well as the strength and range of the screened Coulomb interactions. A convenient way to characterize the relevant regime is the Brueckner parame− 13 ter rs = a10 ( 4π which is the ratio of average electron distance to the Bohr 3 n) radius a0 (n = electron density). In the two limits of small and large rs the electron system exhibits radically different behavior. At large density (small rs ) the system is in a metallic state dominated by the kinetic (Fermi) energy and the Coulomb interactions between electrons are well screened. If the Fermi surface has parallel (quasi-1D) sections, ‘nested’ by a wave vector Q, the residual Coulomb interactions may lead to a condensation of electron–hole (Peierls) pairs into a charge- or spin-density wave state with translational and possibly other symmetries broken. Part or all of the nested Fermi surface sheets are then removed by the self-consistent potential in the condensed state. For a conventional density wave spontaneous modulation of the charge- or spin density with period 2π/Q takes place which may be identified by common methods like X-ray or neutron diffraction. Since real metallic materials have high densities and small or moderate rs this type of instability is frequently encountered. It often competes or coexists with an alternative condensation mechanism, 186 A. Georges, G. Kotliar, W. Krauth, and M. J. Rosenberg, Rev. Mod. Phys. 68, 13 (1996). 187 G. Grüner, Density Waves in Solids, Addison-Wesley (1994).

70

P. FULDE ET AL.

namely electron–electron (Cooper) pair formation leading to a superconducting state. In the opposite limit of small density and large rs the long range Coulomb interaction is badly screened and it dominates the small kinetic energy gain due to delocalizations. At low enough temperatures the electron liquid condenses in real space, forming a Wigner solid9 which also breaks translational symmetry. This is complementary to condensation in the k-space as found in the previous density wave case. For a two dimensional (2D) homogeneous electron liquid in a uniform positive background the appropriate Hamiltonian H = T + V is

1

† † † (k)ckσ ckσ + vq cp+qσ ck−qσ (6.1) H= ckσ cpσ 2 kσ

pkq;σ σ

2

where (k) = k2 /2m is the kinetic energy and vq = 4πe (1 − δq0 ) is the Coulomb q2 interaction. The Kronecker delta δq0 ensures that due to the positive background vq = 0. Furthermore is the volume. For practical calculations on a lattice and for finite systems the Ewald summation technique has to be used to obtain the real space Coulomb potential V (r). The qualitative shape of the n–T phase boundary for the liquid-solid transition has been given in Ref. [188]. It is derived from the intuitive notion that at the phase transition the average potential and kinetic energies of electrons should be comparable, i.e., V /T ≡ 0 . This leads to a parametrically (z = exp(−βμ)) determined n–T phase boundary (μ = chemical potential) shown in Figure VI.1. In 2 √πn. Then the classical limit (kT μ) one has T = kT , furthermore V = e √ the melting curve is simply given by n(T ) = (kT 0 / π e2 )2 with an unknown parameter 0 . In a homogeneous background the 2D electron liquid solidifies in a trigonal (hexagonal) lattice structure.189 In the static approximation without ki−1/2 which is lower netic energy the ground-state energy is EGS = −3.921034e2 ac √ than for any other of the five 2D Bravais lattices. (Here ac = ( 3/2)a02 is the hexagonal cell area with a0 denoting the lattice constant, the density is n = 1/ac .) This result is simple to understand because of all 2D lattices the trigonal one has the largest lattice spacing for a given density and therefore minimizes the total energy if the latter is dominated by the Coulomb repulsion as in the small density regime. Stability analysis shows that the trigonal lattice is stable under longitudinal and transverse (shear) distortions and the corresponding two phonon branches have real frequencies. In the long wavelength limit they are isotropic, i.e., they depend only on q = (qx2 + qy2 )−1/2 and are given by ω1 (q) = ωp (a0 q)1/2 and ω2 (q) = 0.19ωp a0 q for longitudinal and transverse modes respectively. Here 188 P. M. Platzmann and H. Fukuyama, Phys. Rev. B 10, 3150 (1974). 189 L. Bonsall and A. A. Maradudin, Phys. Rev. B 15, 1959 (1977).

STRONGLY CORRELATED ELECTRONS

71

F IG . VI.1. Schematic Fermi liquid–Wigner solid phase diagram of the 2D electron system. Estimates of critical density and temperature are given by nc = (4/πa02 )(1/ 02 ) and Tc = (2e4 m/ 02 ). (After Ref. [188].) 2

−1 is the 3D plasma frequency of a slab of thickness 2a. While ωp = 4πe m∗ (2ac a0 ) the Wigner lattice structure and stability is well understood, the melting into the liquid state, both classical melting (as function of T ) and quantum melting at T = 0 (as function of the control parameter rs ) is much less clear. The situation sketched in Figure VI.1 is certainly oversimplified in one aspect: In both cases presumably an intermediate phase between Wigner solid and Fermi liquid appears which is characterized by the loss of long range translational order but preserves quasi-long range orientational order. In the case of classical melting of 2D trigonal lattices this intermediate phase is known as the ‘hexatic phase’.190 In the case of quantum melting (at T = 0) as function of density (rs ) a similar precursor phase to the liquid seems to appear. This can only be investigated by numerical techniques like Quantum Monte Carlo (QMC) simulations. It was known from earlier QMC results191 that for rs > 37 ± 5 the Fermi liquid state becomes instable. A more recent investigation of phases as function of rs was undertaken in Ref. [192] with a fixed-node QMC approach. A variational trial or guiding wave function for the ground state of H (Eq. (6.1)) on a grid (Lx , Ly ) was used. It has the following 190 B. I. Halperin and D. R. Nelson, Phys. Rev. Lett. 41, 121 (1978). 191 B. Tanatar and D. M. Ceperley, Phys. Rev. B 39, 5005 (1989). 192 H. Falakshahi and X. Waintal, Phys. Rev. Lett. 94, 046801 (2005).

72

form

P. FULDE ET AL.

J |ri − rj | . (r1 , r2 , . . . rN ) = Det φi (rj )

(6.2)

i<j

The single particle wave functions φi (rj ) in the Slater determinant Det[φi (rj )] are taken as plane waves in the liquid state and localized Gaussian orbitals on trigonal sites in the Wigner lattice case. The Jastrow function J (|ri − rj |) describes correlations and consists of modified Yukawa functions. It takes the Coulomb correlations into account by keeping the electrons apart. √ The range of correlations scales with the average electron distance d = 1/ πn where n = N/Lx Ly denotes the density. With this trial wave function one would obtain indeed the instability of the liquid state at rs∗ 40 since for rs > rs∗ its energy exceeds that of the Wigner solid (see Figure VI.2). However, the latter with its localized wave functions is still not the most stable state in that range of rs . This may be seen if one uses instead trigonal lattice Bloch states for the single particle functions φi (rj ) but with k constrained to the first BZ. This implies an orientational symmetry breaking in k space, i.e., a trigonally shaped Fermi surface. But the static density correlation function has still no fully developed Bragg peaks like in the crystal in analogy to the classical melting scenario. This intermediate or hybrid state has indeed a lower energy than the Wigner solid in the range rs∗ < r < rs∗∗ with rs∗ 30 and rs∗∗ 80. For still higher values of rs the Wigner solid with fully

F IG . VI.2. Energy differences in units of 2π N nt (t = hopping energy, n = N/Lx Ly = average density) of liquid and intermediate (or hybrid) phases with respect to the Wigner crystal phase. Here Eliquid –Ecrystal (circles) and Ehybrid –Ecrystal (triangles) are plotted as function of rs for N = 72 electrons on a Lx = 48 × Ly = 84 grid. Critical values are rs∗ ∼ 30 and rs∗∗ ∼ 80. Inset: density–density correlation function with reference particle in the center. (After Ref. [192].)

STRONGLY CORRELATED ELECTRONS

73

localized functions φi (rj ) finally becomes stable. There is no symmetry change involved in going from the intermediate to the Wigner solid state. Therefore it is not clear whether there is a real quantum phase transition at rs∗∗ , as there is at rs∗ , or simply a crossover to more pronounced density correlations (see inset of Figure VI.2). The picture of the intermediate phase is also supported by QMC calculations for mesoscopic 2D electron systems in a harmonic trap. There a similar two-step transition is found from liquid to orientational and finally to fully developed lattice correlations.185 Finally we note that at even larger values of rs the Wigner lattice becomes spin-polarized due to a ferromagnetic ring exchange in the trigonal lattice.193 The experimental realization of the genuine Wigner lattice formation in the 2D electron liquid has been attempted along two alternative approaches. The more successful route is the accumulation of electrons in a monolayer on the surface of liquids such as helium. The accumulation is achieved by applying an electrical pressing field perpendicular to the surface. Its strength allows to vary the electron density in the monolayer over several orders of magnitude. The lower part of the classical melting curve in Figure VI.1 has been determined in Ref. [184] by a rfresonance method. For the ratio of potential to kinetic energy at the phase boundary a surprisingly large value of 0 ∼ 137 was found in agreement with early MC simulations. Due to a finite surface tension the pressing field deforms the liquid surface around the electrons thereby leading to single electron ‘dimples’. This induces an effective attraction between electrons which has to be added to the Coulomb repulsion. It has been proposed that this attraction may lead to a structural phase transition of the Wigner lattice from trigonal to square lattice for sufficiently low density and high pressing fields.194 The second route to generate 2D electron systems are semiconductor heterojunctions. It has been much less conclusive because the evidence for Wigner lattice formation in transport properties is obscured by the 2D localization effects caused by impurities.195 Computational results presented before show that the genuine Wigner lattice formation takes place at rs values which are more than an order of magnitude larger than those found in real solids. But in real crystals with inhomogeneous electron densities the condition for a Wigner type of lattice formation may be much easier to fulfill. In case that the overlap of atomic wavefunctions of neighboring atoms is small the gain in kinetic energy due to electron delocalization is also small. The mutual Coulomb repulsion of electrons on neighboring sites can become more easily dominant in that case than in a homogeneous electron gas. 193 D. M. Ceperley, The Electron Liquid Paradigm in Condensed Matter Physics, IOS Press, Amsterdam (2004), p. 3. 194 M. Haque, I. Paul, and S. Pankov, Phys. Rev. B 68, 045427 (2003). 195 E. Abrahams, Rev. Mod. Phys. 73, 251 (2001).

74

P. FULDE ET AL.

Neighboring rare earth ions have a particularly small overlap of their 4f wavefunctions. Therefore they are particularly good candidates for the formation of charge ordered Wigner like lattices196 as will be discussed in the next section. Furthermore in 3d/4f compounds the Coulomb interactions are strongly screened whereas in the two-step classical and quantum melting of a 2D Wigner lattice the long range part of the Coulomb interactions is most important. Indeed, charge ordering in compounds usually takes place at a well defined temperature and is mostly of first order. It is driven by a competition between short range next and next nearest neighbor Coulomb interactions and the kinetic energy. Also some compounds are already in a Mott–Hubbard insulating state due to large on-site Coulomb repulsion before charge order caused by the inter-site Coulomb interactions appears. Therefore, for real compounds like vanadates and manganites the extended Hubbard type models are a better starting point than the Hamiltonian in Eq. (6.1) to describe the multitude of charge ordering phenomena in solids. Nevertheless, loosely speaking one may refer to them as a kind of generalized Wigner lattice formation.196 13. G ENERALIZED W IGNER L ATTICE : Y B 4 A S 3 The intermetallic compound Yb4 As3 is a perfect example of a system in which charge order takes place, here of 4f holes. Yb4 As3 has a cubic anti-Th3 P4 struc¯ ture with a I 43d space group. Due to the special lattice structure charge order in this three-dimensional system results in the formation of well separated chains of Yb3+ ions. They act like one-dimensional spin chains. The net result is that Yb4 As3 shows all the signs of a low-carrier-density heavy fermion system which here is due to the properties of the spin chains. This is a good example for the formation of heavy quasiparticles caused by electronic charge order. The Kondo effect plays no role in this compound. We start out by summarizing some experimental facts and results. Yb4 As3 and other family members of R4 X3 were first systematically investigated by Ochiai et al.43 A compilation of more recent results may be found in Ref. [197]. By counting valence electrons one notices that since As has a valency of −3, three of the Yb ions must have a valency of +2 while one ion has a valency of +3, i.e., one expects Yb4 As3 → (Yb2+ )3 (Yb3+ )(As3− )3 . But Yb2+ has a filled 4f shell. Thus there is one 4f hole per formula unit. The Yb ions occupy four families of 196 P. Fulde, Ann. Phys. (Leipzig) 6, 178 (1997). 197 B. Schmidt, H. Aoki, T. Cichorek, J. Custers, P. Gegenwart, M. Kohgi, M. Lang, C. Langhammer,

A. Ochiai, S. Paschen, et al., Physica B 300, 121 (2001).

STRONGLY CORRELATED ELECTRONS

75

F IG . VI.3. Left panel: Anti-Th3 P4 structure of Yb4 As3 . Large and small spheres symbolize Yb and As ions, respectively. The Yb ions are residing on four interpenetrating families of chains oriented along cubic space diagonals. Right panel: Dense rod packing representation of the Yb-chains. In the CO structure only one family of chains carries Yb3+ ions with pseudo-spin S = 1/2 whereas the other three families are occupied with S = 0 Yb2+ ions. (After Ref. [197].)

interpenetrating chains which are pointing along the diagonals of a cube (see Figure VI.3). This is often referred to as body-centered cubic rod packing.198 It is important to notice that the distance between two neighboring Yb ions along a chain is larger than the distance between ions belonging to different chains. This implies that nearest neighbor Yb ions belong to different families of chains. At sufficiently high temperatures, i.e., above 300 K the 4f holes move freely between sites and the system is metallic. Measurements of the Hall coefficient RH confirm that the carrier concentration is approximately one hole per unit cell in that temperature range. The situation is different at low temperatures where the measured Hall coefficient has a value of RH = 7 · 1018 cm−3 implying approximately one hole per 103 Yb ions (see Figure VI.4). Thus the system changes from a metal to a semimetal as the temperature decreases. This is particularly seen in measurements of the resistivity ρ(T ) (see Figure VI.4). While for T > 300 K a linear temperature dependence is observed, one notices that near Tc 292 K a first-order phase transition is taking place with a corresponding increase in resistivity. At low temperatures ρ(T ) = ρ0 + AT 2 is found, i.e., the semimetal is a Fermi liquid. Despite the low carrier concentration of order n 10−4 per cell obtained from the Hall constant, Yb4 As3 shows all the signs of a heavy-quasiparticle system at low temper198 Y. M. Li, N. d’Ambrumenil, and P. Fulde, Phys. Rev. Lett. 78, 3386 (1997).

76

P. FULDE ET AL.

F IG . VI.4. Left panel: Hall coefficient RH (T ) for Yb4 As3 . The inset shows the change at the phase transition temperature Tc . Right panel: resistivity ρ(T ). At Tc = 295 K a phase transition due to charge ordering is taking place. Solid line: extrapolation of ρ(T ) ∼ T . (After Ref. [43].)

atures. The γ -coefficient of the specific heat is γ 200 mJ/(mol K2 ), the Sommerfeld–Wilson ratio is RW = 4π 2 kB2 /3(gμB )2 (χ/γ ) 1 implying an equally enhanced spin susceptibility and the Kadowaki–Woods ratio A/γ 2 is similar to that of other heavy quasiparticle systems. If one were to postulate an origin of the heavy mass within the Kondo lattice mechanism, this may seem very strange in view of the fact that this semimetal has a very low density of charge carries. The phase transition at Tc 300 K is accompanied by a trigonal distortion and a change of the space group to R3c. This structural transition is volume conserving and is triggered by charge order of the 4f holes. The angle between orthogonal axes in the cubic phase changes to α = 90.8◦ in the trigonal phase for T Tc (Figure VI.5). Associated with this change is a spontaneous elastic strain below Tc which is proportional to the charge order parameter. The structural instability is accompanied by a softening of the c44 elastic mode above Tc .199 This suggests that the trigonal elastic strain yz , zx , xy with 5 symmetry plays a crucial role. The temperature dependence of the c44 mode may be obtained from a Ginzburg–Landau expansion of the free energy in terms of the strains and the charge ordering parameter components (Qyz , Qzx , Qxy ).199 The latter are defined by expanding the charge ρ = ρ0 + ρ in the form ρ = Qyz ρyz (5 ) + Qzx ρzx (5 ) + Qxy ρxy (5 ).

(6.3)

Here ρ0 is the part of the charge distribution which remains unchanged by the phase transition while ρij (5 ) are the charge fluctuation modes of 5 symmetry. 199 T. Goto, Y. Nemoto, and A. Ochiai, Phys. Rev. B 59, 269 (1999).

STRONGLY CORRELATED ELECTRONS

77

F IG . VI.5. Upper panel: Unit cell angle α = 90◦ + δ (open symbols) as function of T showing first order trigonal distortion at the CO transition temperature Tc 288 K together with linear thermal expansion a/a (full symbols). After Ref. [200]. Lower panel: temperature dependence of the elastic constant c44 (T ). Above the structural phase transition temperature Tc a strong softening is observed described by Eq. (6.6) and caused by coupling to the 5 type charge order parameter. Due to the first-order nature of the transition the theoretical mean-field transition temperature Tc0 = 247 K is smaller than the actual Tc . (After Ref. [199].)

It is Qij = 0 for T > Tc and Qij = 0 for T < Tc . Up to a constant the free energy contains three different contributions. One (FQ ) is due to the order parameter, a second one (Fel ) is due to the elastic energy of the lattice and the third one (FQ-el ) describes the interactions of the order parameter with the lattice. For the 200 K. Iwasa, M. Kohgi, N. Nakajima, R. Yoshitake, Y. Hisazaki, H. Osumi, K. Tajima, N. Wakabayashi, Y. Haga, A. Ochiai, et al., J. Mag. Mag. Mat. 177–181, 393 (1998).

78

P. FULDE ET AL.

c44 elastic constant we obtain201 α FQ = F0 + Q2xy + Q2xz + Q2yz 2

β 3 2 4 4 4 2 2 2 Qxy + Qxz + Qyz − Qxy + Qxz + Qyz + 4 5 Fel =

0 c44 2 2 2 xy + xz + yz 4

FQ-el = −g(Qxy xy + Qxz xz + Qyz yz ).

(6.4)

Near a phase transition α = α0 (T − ) changes sign at a characteristic temperature . The fourth-order terms in Qij stabilize the ordered state of the system. For T > the softening of the elastic constant is obtained by neglecting the terms ∼ Q4ij in the free energy and minimizing F = FQ + Fel + FQ-el by setting ∂F /∂Qij = 0. For β > 0 this leads to a trigonal charge order parameter Qt = √1 (Qxy , Qxz , Qyz ). It also leads to a proportionality between Qij and the 3 strain ij which may be used to rewrite the free energy in the form

2 1 0 g2 2 2 c − xy + xz . (6.5) + yz F = F0 + 2 44 α0 (T − ) Therefore the renormalized elastic constant is

T − Tc0 g2 0 where Tc0 = + c44 = c44 0 T − α0 c44

(6.6)

denotes the theoretical mean-field transition temperature in the presence of the strain interaction. The explanation of a first-order phase transition at Tc > Tc0 requires the inclusion of higher order terms in Qij in (6.4). A detailed grouptheoretical analysis of different measured elastic constants is found in Ref. [199]. At temperatures T > Tc the 4f holes are equally distributed over the chains. But at low temperatures the system avoids nearest-neighbor Yb3+ –Yb3+ sites in order to minimize the mutual short-range inter-site repulsion of 4f holes. This is accomplished by an accumulation of 4f holes in one family of chains, i.e., by charge order. This way nearest-neighbor repulsions of 4f holes are reduced. In the idealized case one expects that for T → 0 one family of chains consists of Yb3+ sites while in the three remaining families of chains all sites are in a Yb2+ configuration. This explains the trigonal distortion (Figure VI.5) which is accompanying charge ordering of the 4f holes. Since Yb3+ ions have a smaller ionic radius than Yb2+ ions the sample is shrinking in the direction of the chains containing the Yb3+ ion. In order to keep the volume of the unit cell constant (other201 T. Goto and B. Lüthi, Adv. Phys. 52, 67 (2003).

STRONGLY CORRELATED ELECTRONS

79

wise a too large amount of elastic energy would be necessary) the remaining three families of chains must expand correspondingly. It was first pointed out in Ref. [31] that the origin of the heavy quasiparticles are spin excitations (spinons) in the chains of Yb3+ ions and that it is not due to the Kondo effect as previously thought. This physical model was beautifully confirmed by inelastic neutron scattering experiments (INS).32,202 They demonstrated that the magnetic excitations are those of an isotropic antiferromagnetic Heisenberg chain. They agree with the spectrum of two-spinon excitations lying within the lower and upper boundaries ωL (q) and ωU (q) respectively, given by

π 1 (6.7) ωL (q) = J sin(q) and ωU (q) = πJ sin q 2 2 with q measured in units of inverse lattice constants d −1 . The lower boundary ωL (q) was calculated long before by des Cloizeaux and Pearson203 (see Figure VI.6). Note that unlike in the classical spin chain there is no sharp spin wave excitation for a given momentum q but instead a two-spinon continuum. Its corresponding dynamic spin-structure factor (Figure VI.6) is proportional to the INS

F IG . VI.6. Spectral function S(q, ω) of the two-spinon excitation spectrum of a Heisenberg chain in the q, ω-plane. It is nonzero in the shaded region above the lower bound ωL (q) calculated by Ref. [203] and the below the upper bound ωU (q) given by Eq. (6.8). S(q, ω) diverges at ωL (q) approximately with a root singularity. The step-like cutoff at ωU (q) is an artefact of the approximate form in Eq. (6.8). The lattice constant is set equal to unity. (After Ref. [204].) 202 M. Kohgi, K. Iwasa, J.-M. Mignot, N. Pyka, A. Ochiai, H. Aoki, and T. Suzuki, Physica B 259– 261, 269 (1999). 203 J. des Cloizeaux and J. J. Pearson, Phys. Rev. 128, 2131 (1962). 204 M. Karbach, G. Müller, and A. H. Bougourzi, Phys. Rev. B 55, 12510 (1997).

80

P. FULDE ET AL.

cross-section and may be approximated by204 S(q, ω) =

(ω − ωL (q))(ωU (q) − ω) . 2 (q) ω 2 − ωL

(6.8)

This spectrum diverges at the lower boundary with a square root singularity and therefore has a very asymmetric appearance as function of energy transfer ω (see Figure VI.6). The total integrated intensity, i.e., the frequency integral of S(q, ω) is linear in q for q π and diverges like [− ln(1 − q/π)]α for q → π , where α = 1 for the approximation in Eq. (6.8) and α = 3/2 is the exact result. Therefore the two-spinon continuum should appear in INS as a spectrum strongly peaked at ωL (q) with an asymmetric tail reaching up to ωU (q) and a strongly increasing total intensity for q → π . This is precisely what has been found in the INS experiments of Kohgi et al. (see Figure VI.7) and constitutes a proof for the 1D character of spin excitations in Yb4 As3 . That the interacting crystal field ground-state doublets of Yb3+ behave like an isotropic Heisenberg system is not immediately obvious. It was shown

F IG . VI.7. Left panel: Experimental S(q, ω) from INS202 for momenta q = 1 and 0.8 (here q is given in units of π/d where d is the Yb distance in the chain). The asymmetric shape of the two-spinon spectrum in Figure VI.6 is clearly observed. For q < 1 the resolution limited peak position corresponds to the lower boundary ωL (q) of the spinon spectrum. Right panel: Dispersion of ωL (q) from INS experiments for different directions of the momentum transfer. Here q is the projection of momenta on the 111 chain direction. All data points fall on the dashed curve which is the theoretical ωL (q) = π2 J sin dq with J /kB = 25 K. In addition to the asymmetric shape of S(q, ω) this proves the 1D character of magnetic excitations in Yb4 As3 . (After Ref. [32,202].)

STRONGLY CORRELATED ELECTRONS

81

independently in Refs. [205] and [206]. Thereby the local symmetry of the crystalline electric field was properly accounted for. Spin fluctuations of Heisenberg chains can explain the observed heavy quasiparticle excitations as they appear in the specific heat C = γ T and spin susceptibility χS . They are given by γ=

2 kB R 3 J

and χS =

4μ2eff R (π 2 J )

(6.9)

(see Ref. [207]). Here J is the AF coupling constant of nearest-neighbor sites in the effective S = 12 spin chain described by the 1D Heisenberg Hamiltonian

H =J Si Sj . (6.10) ij

Furthermore, R is the gas constant and μeff is the effective magnetic moment of a Yb3+ site. Therefore one finds RW = 2 for the Sommerfeld–Wilson ratio. When the experimental value of J /kB = 25 K (from Figure VI.7) is used in (6.9) the observed size of the γ coefficient is well reproduced. Having described the underlying physics we discuss a model description for the compound. For that purpose we neglect the electron hopping terms between different chains as it was done, e.g., in the Labbé–Friedel model for A-15 compounds like V3 Si or Nb3 Sn.208 There one is dealing with three families of intersecting chains while here we have four types of chains. The effective 4f -model Hamiltonian31 is then written as

+ fiμσ fj μσ + h.c. + U niμ↑ niμ↓ H = −t μ ij σ

+

μ

iσ

μ

μ niμσ +

i

N c 2 . 4

(6.11)

The first term describes effective 4f -hole hopping due to hybridization with As 4p ligand states within a chain of a family μ = 1–4 from site i to a nearest neighbor site j . From LDA calculations one can deduce that 4t 0.2 eV. The second + fiμσ term is due to the on-site Coulomb repulsion of 4f holes with niμσ = fiμσ 4+ 12 and ensures that in the large U limit Yb states with 4f configurations are excluded. The third term describes the volume conserving coupling of the f bands 205 G. Uimin, Y. Kudasov, P. Fulde, and A. Ovchinnikov, Eur. Phys. J. B 16, 241 (2000). 206 H. Shiba, K. Ueda, and O. Sakai, J. Phys. Soc. Jpn. 69, 1493 (2000). 207 D. C. Mattis, The Theory of Magnetism, vol. 17 of Springer Series in Solid State Sciences, Springer-Verlag, Berlin (1981), 2nd ed. 208 J. Labbé and J. Friedel, Journ. Phys. (Paris) 27, 153, 303 (1966).

82

P. FULDE ET AL.

to the trigonal strain > 0 with = 5 . It leads to a deformation potential of the form (6.12) μ = (4δμ1 − 1) 3 for 4f holes situated in chains, e.g., in [111] direction denoted by μ = 1. Since the Yb3+ ions are smaller than the Yb2+ ions, the distance between Yb ions shrinks for μ = 1 while it expands in the other chain directions denoted by μ = 2, 3, 4. As previously pointed out the origin of the deformation potential is the Coulomb repulsion between holes on neighboring sites. It is treated here as an effective attraction Veff between holes on nearest-neighbor sites of a chain. The fourth term in (6.11) is the elastic energy in the presence of a trigonal distortion, where N is the number of sites and c is the background elastic constant. A reasonable value is c / = 4 · 1011 erg/cm3 where denotes the volume of a unit cell with a lattice constant of a0 = 8.789 Å. The Hamiltonians for chains μ with an interaction Veff can be written in the form

+ Hμ = −tμ fiμσ fj μσ − Veff (niμ − n)(n ¯ j μ − n) ¯ (6.13) ij σ

ij

where n¯ is the average occupancy of all sites in the system. Within a molecularfield approximation the Hamiltonian reduces to

N + fiμσ fj μσ − 2Veff (n¯ μ − n) (niμ − n) ¯ + Veff (n¯ μ − n) ¯ 2. HμMF = −tμ 4 ij σ

ij

(6.14) We denote the distinct chains with μ = 1 and note that with the correspondence 4 = −2Veff (n¯ 1 − n); ¯ 3

2 9 = Veff c 4

(6.15)

the Hamiltonians (6.14) and (6.11) become the same. This serves as a justification for the band Jahn–Teller type of description chosen above. When a distortion is taking place the hopping matrix elements also depend on μ, according to tμ = t+ δμ1 + t− (1 − δμ1 ) t+ = teλ ,

t− = teλ /3 .

(6.16)

But this μ dependence of t is not essential. The Hamiltonian (6.11) is well suited for describing the lattice distortion caused by charge ordering. The distortion is described here like a collective band Jahn– Teller effect. The four-fold degeneracy of the f bands is lifted by the spontaneous appearance of a trigonal strain which lowers the symmetry. For the purpose of

STRONGLY CORRELATED ELECTRONS

83

F IG . VI.8. Temperature dependence (T ) of the (secondary) strain order parameter. Shown in the inset are the corresponding changes in the population of the different families of chains. Q = n1 − n2 is the primary charge order parameter. (After Ref. [31].)

demonstration we consider first the case of U = 0. This neglects the effects of strong on-site correlations on the band Jahn–Teller effect. Near the charge ordering transition where each of the chains contains nearly 25% of Yb3+ sites this approximation is justified. However, it is no longer acceptable for low temperatures when nearly all of the sites in the μ = 1 chains are Yb3+ . The condition for a collective band Jahn–Teller effect taking place is 2 /(t ) > 3.31 Choosing = 5 eV results in a transition temperature of Tc 250 K which is close to the experimental value of 300 K. This value of corresponds to a Grüneisen parameter of G ≡ /(4t) = 25 which is of a comparable size found in other 4f -mixed valence systems. The symmetry strain as function of reduced temperature T /Tc is shown in Figure VI.8. As a consequence of a finite strain the four degenerate onedimensional f bands split into a lower and three upper bands. Their centers of gravity differ by (4/3)| | with the equilibrium strain given by = −/(2c ) 0.02. The changes in the population of the chains with μ = 1 and μ = 1 with decreasing temperature are shown in the inset of Figure VI.8. The transition is of first order due to the singular DOS of the effective 1D f-bands. Let us reemphasize that those changes are caused by the Coulomb repulsion of holes and drive (T ) and not vice versa. Band refillings by a band Jahn–Teller transition and crystallization of holes are alternative points of view of the respective descriptions here.

84

P. FULDE ET AL.

F IG . VI.9. Yb4 As3 : Site selective values of Yb valence/hole concentration (data points) as obtained from the 303¯ reflection in the vicinity of the Yb L3 X-ray absorption edge. Full line: guide to the eye. Dashed line: model calculation from Ref. [198]. Dotted line: from the angular deviation δ(T )200 in Figure VI.5. (After Ref. [209].)

There have been experiments which directly observed one-dimensional charge order.209 This was achieved, e.g., by resonant X-ray diffraction on the Yb L3 absorption edge. Below Tc forbidden reflections appear in the slightly rhombohedrally distorted cube. From their intensity one can deduce an effective valency for the short and long chains (see Figure VI.9). The discontinuities at the first-order phase transition are even larger than the above model calculation predicts. We return to the Hamiltonian in Eq. (6.11) and consider the effects of a large on-site interaction U in the charge ordered state for T Tc . For this purpose we transform to a t–J Hamiltonian for the chains μ = 1. The exclusion of Yb4+ configurations (2 holes) due to U is taken into account by a projector P which projects onto 0 and 1 hole occupations of sites. To lowest order in t/U we obtain

1 + Si Sj − ni1 nj 1 (6.17) P fi1σ fj 1σ + h.c. P + J Hμ=1 = −t 4 ij σ

ij

+ where J = 4t 2 /U and furthermore Si = αβ fi1α σ αβ fi1β , ni1 = σ ni1σ . For U = 10 eV we find J = 1·10−3 eV. A slight band-narrowing effect due to the 209 U. Staub, B. D. Patterson, C. Schulze-Briese, F. Fauth, M. Shi, L. Soderholm, G. B. M. Vaughan, and A. Ochiai, Europhys. Lett. 53, 72 (2001).

STRONGLY CORRELATED ELECTRONS

85

lattice distortion (see Eq. (6.16)) has been neglected here. The Hamiltonian Hμ=1 can be treated within the slave-boson approximation. Thereby the projector P is replaced by an auxiliary boson bj+ which generates a configuration without a hole, i.e., a Yb2+ site. By treating the boson field in mean-field approximation one obtains an effective mass of the quasiparticles m∗ t = mb tδ + (3/4)χJ

(6.18)

where mb is the bare band mass and χ = ( π2 ) sin( π2 (1 − δ)). Furthermore, δ is the deviation of the chains μ = 1 from half filling. When δ = 0, i.e., for the half-filled case we find (J = 4t 2 /U ) m∗ π U 2π t = = mb 6 t 3 J

(6.19)

which is a large mass enhancement of order 102 . In this case the heavy quasiparticles are spinons as we are dealing with an antiferromagnetic Heisenberg chain. The low temperature thermodynamics is completely determined by these spin degrees of freedom and we have an example of spin-charge separation here. A de Haas–van Alphen experiment should not yield heavy quasiparticle masses here and the Fermi-liquid relation between the γ coefficient and a renormalized mass of (nearly) free electrons is violated. This becomes obvious when Yb4 (As1−x Px )3 (x = 0.3–0.4)210,211 is considered. In distinction to Yb4 As3 this is a charge ordered insulator but it has nevertheless a similar large linear specific heat coefficient γ . The latter is caused by spin excitations in Heisenberg chains as in Yb4 As3 . It is interesting to note that the Hamiltonian (6.11) can be solved exactly by adaptation of Lieb and Wu’s solution of the one-band Hubbard model. The solution is based on the Bethe ansatz. This is possible since the different bands are not coupled directly with each other. One interesting finding is that the increase in the strain order parameter just below Tc is much steeper than in Figure VI.8 and therefore in better agreement with experiments. For more details we refer to the original literature.212 This brings us to the question: why is Yb4 As3 at low temperatures still a semimetal and not an insulator? From the present model we would naively expect that at zero temperature Yb4 As3 is an insulator. Charge order should be complete and a half-filled Hubbard chain is an insulator at sufficiently low temperatures for any positive value of U . In reality this is not the case due to incomplete charge order, 210 H. Aoki, T. Suzuki, and A. Ochiai, unpublished (2005). 211 A. Ochiai, H. Aoki, T. Suzuki, R. Helfrich, and F. Steglich, Physica B 230–232, 708 (1997). 212 Y. M. Li, N. d’Ambrumenil, and P. Fulde, Phys. Rev. B 57, R14016 (1998).

86

P. FULDE ET AL.

F IG . VI.10. LDA+U energy bands for Yb4 As3 . A small number of As 4p holes appears at the -point. The flat band has Yb 4f -character. (After Ref. [45].)

i.e., the Hubbard chains are not half-filled but doped. Within the model one possible explanation for incomplete charge order would be self-doping. Indeed, as function of U the exact solution of the Hamiltonian (6.11) shows a regime in the c vs. total electron concentration n0 plane where charge ordering is incomplete. However, in Yb4 As3 the true reason for the observed semimetallic behavior is found when bandstructure calculations within the local spin-density approximation plus U approach (LSDA+U) are performed. They show a rigid pinning of the Fermi energy to states close to the top of the As 4p band (see Figure VI.10). The filled 4f shell of Yb2+ is treated as a core shell and the interaction U = 9.6 eV between two 4f holes was adjusted to obtain the proper number of charge carriers. Because of a large gap between the As 4p and Yb 5d bands, the 4f hole band is pinned to the top of the As 4p band. This allows for charge transfer between Yb and As. As a result a small amount of As 4p holes is created, which act as mobile charge carriers with a corresponding reduction of Yb 4f holes. The calculated cyclotron masses of the almost spherical hole sheet of the As p states are in the range of 0.6 to 0.8 times the free electron mass m0 , in good agreement with the value of mexp = 0.72m0 obtained from cyclotron-resonance experiments while a value of 0.275m0 was obtained from Shubnikov–de Haas oscillations.213 However, the calculated mass should still be renormalized due to electron–phonon interactions. We want to draw attention to the fact that the relation between the large γ coefficient in the specific heat and the mass of the charged quasiparticles responsible for charge transport is lost here. This calls in question one fundamental requirement 213 P. Gegenwart, H. Aoki, T. Cichorek, J. Custers, N. Harrison, M. Jaime, M. Lang, A. Ochiai, and F. Steglich, Physica B 312–313, 315 (2002).

STRONGLY CORRELATED ELECTRONS

87

of Landau’s Fermi liquid theory. Its basis is a one to one correspondence between the excitations of an interacting electron system and those of a free electron system with renormalized parameters such as the quasiparticle mass. In the case of Yb4 As3 this correspondence holds only when the charge of the free electrons is renormalized to zero, i.e., when we deal with neutral fermions. This is due to the fact that the low-lying excitations are those of a Heisenberg chain which are of magnetic origin and can be described either by bosons or alternatively by neutral fermions. In addition to the neutral fermionic excitations in the chains which are spinon-like there are charged fermions (the As 4p-holes), i.e., electrons with a low density of states which provide for charge transport. The large A coefficient in ρ(T ) results from scattering of the charged fermions by the neutral ones, while the thermal conductivity is dominated by the neutral ones (spinons). This special feature is amplified when instead of Yb4 As3 semiconducting mixed crystals Yb4 (As1−x Px )3 with x = 0.3–0.4 are considered. These crystals also exhibit charge order like Yb4 As3 forming spin chains below the ordering temperature. The Sommerfeld constant is γ = 250 mJ/(mol K2 ) despite the fact that at T = 0 there are no charge carriers in the system.211 The LSDA+U calculations also show that one must be careful in finding the correct ordered structure by comparing Madelung energies. In competition with the trigonal phase considered here is a cubic P21 3 phase with chains of sequence – Yb3+ –Yb2+ –Yb2+ –Yb2+ –Yb3+ –Yb2+ – . The Madelung energy of this structure is slightly lower than the one of the trigonal structure. It does not couple to the 5 strain and therefore cannot explain the observed softening of the elastic constant c44 . But when the self-consistent charges are calculated one finds a slight charge disproportionation of 0.05 electrons between the center Yb2+ ion and the two adjacent Yb2+ ions. This changes the Madelung energy difference in favor of the trigonal structure. When a magnetic field H is applied to an isotropic antiferromagnetic spin chain (S = 12 , g = 2), the excitations remain gapless as long as the field remains smaller than gμB HS = J beyond which the system becomes a fully polarized ferromagnet with a Zeeman gap.214 It was therefore a surprise when it was found that the specific heat of Yb4 As3 depends strongly on H.215 Experimental results for γ (H) are shown in Figure VI.11. Likewise strong anomalies in the thermal expansion were found215 which is related to the specific heat via the Ehrenfest relation. A number of possible explanations of these observations have been proposed. One is based on magnetic interchain interactions.216 Another model calcu214 J. D. Johnson, J. Appl. Phys. 52, 1991 (1981). 215 M. Köppen, M. Lang, R. Helfrich, F. Steglich, P. Thalmeier, B. Schmidt, B. Wand, D. Pankert,

H. Benner, H. Aoki, et al., Phys. Rev. Lett. 82, 4548 (1999). 216 B. Schmidt, P. Thalmeier, and P. Fulde, Europhys. Lett. 35, 109 (1996).

88

P. FULDE ET AL.

F IG . VI.11. Yb4 As3 : Experimental field dependence of the specific heat γ coefficient (full circles) at T 0.5 K and theoretical results based on interchain interactions: lower and upper solid lines: H ⊥[111] and H [111]. The dashed curve is for T = 5 K. A ratio J /J = 10−4 was used. (After Ref. [216].)

lation advocates a staggered field mechanism due to the Dzyaloshinsky–Moriya interaction206 and a third one suggests that the dipolar interactions within a chain are responsible for the decrease of γ with increasing external field.205 In all three cases a magnetic field applied perpendicular to the Yb3+ chains is opening a gap in the excitation spectrum while the excitations remain gapless when the field is pointing along the chains. But they differ in details, e.g., in the way the gap opens. When a small interchain coupling J is assumed between adjacent Yb3+ chains a field perpendicular to the chains induces a gap ∼ (|J J |)1/2 . For J /J = 10−4 one obtains a decrease of the γ coefficient with increasing field of the observed size (see Figure VI.11). The two other models are based on independent Heisenberg chains. The model based on the Dzyaloshinsky–Moriya interaction exploits the fact that the Yb3+ sites are not centers of inversion (see Figure VI.12). The local C3 symmetry together with a glide reflexion and a glide vector parallel to the chains allows for the following features: a uniaxial anisotropy for the symmetric part of the spin– spin interaction and an antisymmetric Dzyaloshinsky–Moriya (DM) interaction. However due to the hidden symmetry they are not independent.206 A transformation consisting of staggered rotations with angle θ around the chain direction (z) makes this more apparent: The pseudo-spin Hamiltonian for the lowest Yb3+

STRONGLY CORRELATED ELECTRONS

89

F IG . VI.12. Yb4 As3 : Absence of a center of inversion in Yb3+ chains. The distance Yb(1)–As(1) (or Yb(2)–As(2)) is smaller than the distance Yb(1)–As(2) (or Yb(2)–As(1)). Atoms with equal gray scale are equivalent. (After Ref. [206].)

Kramers’ doublet, expressed in rotated spin operators, is then given by

Heff = J g Siz Hz + cos θg⊥ (Six Hx + Siy Hy ) Si Sj − ij

i

+ (−1)i sin θg⊥ (Siy Hx − Six Hy ) .

(6.20)

Here the C3 doublet wavefunction has associated anisotropic g-factors g,⊥ whose ratio is 2.5.206 The angle θ is adjustable and in principle determined by the C3 CEF parameters. Thus for zero field one has indeed an isotropic spin chain (S = 1/2) Hamiltonian despite involving strongly anisotropic wave functions of the lowest Kramers’ doublet state. This leads to the gapless spinon excitation spectrum discussed previously. When a magnetic field is applied perpendicular to the chain a staggered field perpendicular to both chain and applied field is induced by the DM interaction described by the last term in Eq. (6.20): Hs = g⊥ sin θ [n × H].

(6.21)

Here n is a unit vector in chain direction and g⊥ = 1.3 is the corresponding g factor. Due to the staggered field the uniform physical susceptibility χ⊥ (0) is a mixture of q = 0 (uniform) and q = π (staggered) susceptibilities χ1D of the (S = 12 , g = 2) isotropic Heisenberg chain according to 2 2 χ⊥ (0) = g⊥ cos (θ )χ1D (0) + sin2 (θ )χ1D (π) . (6.22) Since the latter diverges ∼ 1/T at low temperatures this should lead to a Curielike upturn also in the homogeneous χ⊥ (0, T ). This behavior was indeed found and in principle the value of tan2 (θ ) = 0.04 may be extracted from the analysis of

90

P. FULDE ET AL.

F IG . VI.13. Upper panel: Spin excitations (ωL (q)) from INS in an Yb3+ chain in a magnetic field perpendicular to the chains and without it. Note the gap opening at q = π/d. After Ref. [217]. Lower panel: Gap as function of applied field. A scaling exponent 2/3 corresponding to quantum sine-Gordon equation is found (full line: (H ) ∼ Es (H ) ∼ H 2/3 ). Here Es (H ) is the gap from thermodynamic and transport quantities and (H ) is the gap obtained in INS. (After Ref. [197].)

the upturn. The most important effect of the staggered field is the appearance of an induced gap in the excitation spectrum with a field dependence 2/3

(H ) 1.8J 1/3 Hs

∼ H 2/3 .

(6.23)

This gap was seen in thermodynamic and transport properties like specific heat, thermal expansion, etc.215,213 and the field scaling exponent 2/3 was indeed identified (Figure VI.13). A field dependence of this form has also been directly observed by inelastic neutron scattering (INS) on a single crystal at T = 1.9 K. A gap 217 M. Kohgi, K. Iwasa, J.-M. Mignot, B. Fak, P. Gegenwart, M. Lang, A. Ochiai, H. Aoki, and T. Suzuki, Phys. Rev. Lett. 86, 2439 (2001).

STRONGLY CORRELATED ELECTRONS

91

was found to open up at q = πd when the field was perpendicular to the short, i.e., Yb3+ chains (see Figure VI.13). This supports the above model. In passing we note that the above excitations can also be described by a sine-Gordon equation associated with moving domain walls as applied to Cu-benzoate.218 But when the magnetic field is parallel to the chain, gapless modes at finite q = πd (1±2σ ) (σ = magnetization) are expected219,220 which so far have not been seen and this casts some doubt on the theory. This brings us to the third model which is based on the weak dipolar interaction of the Yb3+ sites. For that purpose the DM interaction is neglected. The dipolar interaction is

Ji Jj − 3(Ji e)(Jj e) Hdip = g 2 μ2B (6.24) |Ri − Rj |3 i<j

where e = (Ri − Rj )/|Ri − Rj | and only the ground state doublet of the Yb3+ is taken into account. This leads to an effective, slightly anisotropic Heisenberg antiferromagnet in an applied field. In a transverse field a gap opens up.221 A special feature is that at high fields the gap should close again. Measurements up to H = 30 T reveal this effect. Indeed a strong reduction of the gap below the (H ) ∼ H 2/3 scaling curve (Figure VI.13) was observed already above H = 10 T.213 When H is parallel to the chains a Zeeman splitting is expected and there should be no incommensurate peaks appearing, in agreement with experiments. In summary it seems that the magnetic field effects are not yet fully understood. 14. C HARGE O RDERING AND 1D S PIN E XCITATIONS IN α -NAV 2 O 5 In quasi-1D metals such as organic charge transfer salts or the famous KCP chain compound187 it is known that the ground state exhibits a spontaneous dimerization due to the instability of the 1D Fermi surface. It is signified by a diverging electronic susceptibility at wave number q = 2kF . In real compounds this instability, the ‘Peierls-transition’ takes place at a finite transition temperature controlled by the interchain-coupling. Amazingly a similar ‘spin-Peierls’ transition may occur in insulating quasi-1D spin chains with antiferromagnetic nearest neighbor (n.n.) coupling. This is most conveniently understood for an xy-type exchange interaction model which can be exactly mapped by a Jordan–Wigner transformation 218 D. C. Dender, P. H. Hammar, D. N. Reich, C. Broholm, and G. Aeppli, Phys. Rev. Lett. 79, 1750 (1997). 219 G. Müller, H. Thomas, H. Beck, and J. C. Bonner, Phys. Rev. B 24, 1429 (1981). 220 H. Shiba, K. Ueda, O. Sakai, and S. Qin, Physica B 312–313, 309 (2002). 221 D. V. Dmitriev, V. Y. Krivnov, and A. A. Ovchinnikov, Phys. Rev. B 65, 172409 (2002).

92

P. FULDE ET AL.

(JW) to a model of free spinless 1D fermions at half filling.222 Naturally this leads to a chain dimerization via the same ‘electron’–phonon coupling as in the case of real conduction electrons. Adding the z-term of the Heisenberg exchange interaction one obtains an interacting fermion model after the JW transformation but the basic mechanism of dimerization is unchanged. The spin-Peierls transition has originally been found in a number of organic spin chain compounds and has been theoretically investigated first in Ref. [223] within a mean-field treatment and later in Ref. [224] using the Heisenberg exchange and its coupling to the lattice in the fermionic (JW) representation. Surprisingly the spin-Peierls transition rarely occurs in inorganic 1D-spin chain compounds, presumably because magnetic order due to interchain–exchange is preferred in most cases. The only such spin-Peierls compound known until recently was CuGeO3 225 where the S = 12 spins of Cuchains undergo dimerization at TSP = 14 K. The corresponding dimerization of the exchange integral along the chain then creates an isotropic spin excitation gap. The ensuing isotropic drop in the spin susceptibility below the transition temperature is therefore the most direct method to identify the spin-Peierls mechanism. Actually this is not unambiguous because the presence of n.n.n exchange interactions J with a ratio J /J > 0.24 where J is the n.n. exchange also leads to a spin gap and this issue is still controversial in CuGeO3 . Therefore the discovery of a structural phase transition in the layered perovskite insulator α -NaV2 O5 at Tc 34 K with a corresponding isotropic spingap formation226 has created enormous interest and activity, both experimental and theoretical. This compound was seen as a second candidate for an inorganic spin-Peierls system which seemed to be consistent with the original crystal structure determination227 that suggested the existence of S = 1/2 V4+ spin chains along the crystal b-axis (every second V chain in Figure VI.14), isolated by intervening nonmagnetic V5+ (S = 0) chains. Both belong to V-V ladders formed by the oxygen pyramids, where neighboring ladders are shifted by b/2. In the ab-plane this leads to a Trellis lattice structure shown in Figure VI.14. Exchangedimerization of the S = 1/2 V chains due to the spin-Peierls mechanism below Tc would then lead to the isotropic spin gap. This interpretation was however much too naive as became clear subsequently. It turned out that the structural phase transition is not of the simple chain dimerization type but leads to a very low symmetry (monoclinic) structure that can only be understood if in addition a charge 222 G. Beni and P. Pincus, J. Chem. Phys. 57, 3531 (1972). 223 E. Pytte, Phys. Rev. B 10, 4637 (1974). 224 M. C. Cross and D. S. Fisher, Phys. Rev. B. 19, 402 (1979). 225 M. Hase, I. Terasaki, and K. Uchinokura, Phys. Rev. Lett. 70, 3651 (1993). 226 M. Isobe and Y. Ueda, Phys. Soc. Jpn. 65, 1178 (1996). 227 A. Carpy and J. Galy, Acta Crystallogr. B 31, 1481 (1975).

STRONGLY CORRELATED ELECTRONS

93

F IG . VI.14. Upper panel: Layered perovskite structure of α -NaV2 O5 consisting of chains of oxygen pyramids that contain the V atoms aligned along the crystal b axis. The layers are stacked along c axis. Na atoms (grey spheres) are centered above the ladder plaquettes. Lower panel: ab-plane Trellis lattice structure of V-V ladders alternatingly shifted along b by half a lattice constant. This leads to a quasi-‘triangular’ structure for V-V rung units. Orthorhombic high temperature unit cell is indicated.

ordering transition of V4+ /V5+ is present, starting from a homogeneous high temperature insulating mixed valence (V4.5+ ) state, in contrast to the first assumption in Ref. [227]. Nevertheless above Tc the susceptibility exhibits the typical Bonner–Fisher maximum of 1D spin chains.226,228 This compound therefore is another example of an intricate relation between charge ordering and quasi-1D spin excitations which in the present case are gapped. In this section we first discuss the result of the increasingly more detailed X-ray analysis of the high and low temperature structure of α -NaV2 O5 , nevertheless no final agreement on the low-T structure has been reached. Electronic structure calculations are essential to construct an effective Hamiltonian for the charge ordering. We will argue that this transition and the ensuing spin 228 P. Horsch and F. Mack, Eur. Phys. J. B 5, 367 (1998).

94

P. FULDE ET AL.

gap formation requires the inclusion of lattice degrees of freedom which lead to the appearance of two inequivalent V-V ladder types in the perovskite layers. The gapped spin excitation spectrum in the distorted CO phase will be discussed within a simple dimer-RPA approach and a comparison with INS results is given which also advocates the inequivalent ladder model. Finally we briefly mention the stacking of CO layers along c and the destruction of CO by Na deficiency doping or substitution of Na by Li or Ca and in connection with the nature of the insulating state in α -NaV2 O5 . In this section we will not review the various alternative theoretical models that have been proposed for α -NaV2 O5 . We also will exclude the discussion of most optical experiments, since this is not the ideal method to investigate spin excitations. The determination of the crystal structure of α -NaV2 O5 , both above and below Tc , is fundamental for constructing a microscopic model for the phase transition and spin gap mechanism. This was surprisingly controversial and has led to much confusion, mostly for the low- but even for the high-temperature structure. The latter was originally thought to have non-centrosymmetric symmetry227 already above Tc leading to the assumption of V5+ /V4+ in-line charge disproportionation on each V-V rung of the ladders from the outset. However later it was discovered229 that the proper high temperature structure belongs to the centrosymmetric Pmmn space group. Due to the reflection plane containing y both V-sites in the rungs must be equivalent, i.e., they are in a mixed valence state V4.5+ . The structure of the low temperature phase (T Tc ) proved even more controversial. In Refs. [230–232] an orthorhombic space group Fmm2 with a 2a × 2b × 4c supercell was proposed. In the low temperature phase the modulation (atomic shifts of V, O and Na atoms with respect to high temperature structure) strongly differs for neighboring ladders A and B. Loosely speaking the atomic positions on A are modulated while on B they are not (see Figure VI.17). Subsequently it was shown233 that the symmetry is even lower, characterized by the monoclinic space group A112 which does not contain an inversion symmetry. This implies the existence of a spontaneous dipole moment (induced ferroelectric order parameter) below the phase transition which has indeed been observed by measuring the dielectric function. The two space groups differ in the number of inequivalent atoms 229 H. G. von Schnering, Y. Grin, M. Knaupp, M. Somer, R. K. Kremer, O. Jepsen, T. Chatterji, and

M. Weiden, Z. Kristallographie 213, 246 (1998). 230 J. Lüdecke, A. Jobst, S. van Smaalen, E. Morré, C. Geibel, and H. G. Krane, Phys. Rev. Lett. 82, 3633 (1999). 231 S. van Smaalen and J. Lüdecke, Europhys. Lett. 49, 250 (2000). 232 J. L. deBoer, S. A. Meetsma, J. Baas, and T. T. M. Palstra, Phys. Rev. Lett. 84, 3962 (2000). 233 H. Sawa, E. Ninomiya, T. Ohama, H. Nakao, K. Ohwada, Y. Murakami, Y. Fuji, Y. Noda, M. Isobe, and Y. Ueda, J. Phys. Soc. Jpn. 71, 385 (2002).

STRONGLY CORRELATED ELECTRONS

95

per unit cell, e.g., 6 V sites in two inequivalent layers a, b for Fmm2 and 8 V sites again in two layers for A112. Likewise there are 6 vs. 8 inequivalent Na atoms and 16 vs. 20 inequivalent O atoms in both cases respectively. Nevertheless, the full refinement of the modulated crystal structure with A112 and Fmm2 space group leads to almost identical atomic positions.233 This raises the question how the valences, most importantly of V-atoms should be assigned in the low temperature structure. Unfortunately the modulated structure has not yet been investigated within LDA+U calculations. Therefore one has to resort to the empirical valence-bond method.234 In this approach every atom at an inequivalent site is assigned a formal valence Vi (or oxidation number) which may be thought of as the number of electrons it contributes to all the bonds connected to ligand atoms according to the prescription

R0 − Rij (6.25) vij with vij = exp |Vi | = B j

where vij is the valence of a given central atom-ligand bond which depends on the bond length. Here R0 and B are empirical parameters characteristic of a given type of chemical bond, e.g., V–O bond, independent of the material. The optimal parameters R0 and B may however be weakly temperature dependent. Using the sum rule in Eq. (6.25) and identifying valence with the number of electrons contributing to bonds the valence of constituents may be determined. In α -NaV2 O5 we are primarily interested in the number of electrons in the V-dxy orbital because the 3dxy -bands are well separated from all other bands as seen below. Its orbital occupation is then given by ndxy = 5–Vi , assuming that bonding takes place mainly with the lower lying O3p orbitals. This quantity is the most interesting to study in view of possible charge ordering. We now discuss a few basic observations that prove the connection between charge ordering and spin gap formation at the structural phase transition. It has been proposed early from thermal expansion measurements235 that actually there are two separate but close by phase transitions at Tc1 33 K and Tc2 32.7 K which are of first and second order respectively. These values depend considerably on sample quality and may be higher (see Figure VI.15) than those given above. Detailed investigation of NMR frequencies and Knight shifts have shown236 that Tc1 and Tc2 may be associated with charge ordering on V-sites and a spin-gap formation respectively (Figure VI.15). In the following we will denote the whole 234 J. D. Brown, Acta Cryst. B 48, 553 (1992). 235 M. Köppen, D. Pankert, R. Hauptmann, M. Lang, M. Weiden, C. Geibel, and F. Steglich, Phys.

Rev. B 57, 8466 (1998). 236 Y. Fagot-Revurat, M. Mehring, and R. K. Kremer, 84, 4176 (2000).

96

P. FULDE ET AL.

F IG . VI.15. Upper panel; V-Knight shift 51 Kcc and Na-Knight shift 23 Kcc as well as quadrupolar frequency 23 νcc of α -NaV2 O5 . The first reflects charge order, the second the opening of the spin gap and the third the lattice distortion around Na-sites. Since 23 Kcc and 23 νcc behave synchronously below Tc2 this suggests that spin gap formation is connected with exchange dimerization due to Na-shifts. After Ref. [236]. Lower panel: Magnetic susceptibility for single crystalline α -NaV2 O5 showing the isotropic spin gap opening below Tc2 . (After Ref. [237].)

region of these close transitions simply by ‘Tc ’. At the lower transition the critical exponent of the spin-gap opening SP ∼ (1 − T /Tc )β is β ∼ 0.34 close to 2 the theoretical value 0.33 obtained from SP ∼ δ 3 (see Ref. [224]) and a mean1 field chain and exchange dimerization behavior δ ∼ (1 − T /Tc ) 2 . This suggests indeed a spin-Peierls dimerization at the lower transition. The first transition on 237 M. Weiden, R. Hauptmann, C. Geibel, F. Steglich, M. Fischer, P. Lemmens, and G. Güntherod, Z. Phys. B 103, 1 (1997).

STRONGLY CORRELATED ELECTRONS

97

the other hand has a 2D-Ising character, as indicated by a logarithmic peak in the specific heat superposed by the jump of the second transition. Furthermore, according to temperature dependence of X-ray satellites the total lattice distortion has a temperature exponent β ∼ 0.2 closer to the Ising value 1/8 than to the mean-field exponent. In summary, these findings suggest that the Tc1 -transition leads to charge ordering on the V-sites and has partly 2D Ising character. Its field dependence is smaller than for an Ising transition but larger than for a pure structural transition. At Tc1 the main lattice distortion takes place. At the slightly lower Tc2 the spin gap opens with a spin-Peierls like exponent and connected with an additional exchange dimerization along the charge ordered chains. Before discussing microscopic models for these peculiar transitions results of the electronic structure calculations for α -NaV2 O5 have to be summarized. So far they were only done for the undistorted structure. Both LDA calculations238 and spin polarized LDA+U calculations239 for the charge ordered (but undistorted) case have been performed. In both cases it is found that the planar V dxy bands are well separated from hybridized Vd-Op-bands which are fully occupied or empty as shown in Figure VI.16. In the LDA calculation the Fermi level is centered in the dxy band predicting a metallic state, contrary to the fact that even without CO above Tc α -NaV2 O5 is an insulator. As in the undoped cuprates this is due to a neglect of on-site Coulomb correlations in LDA. In the LDA+U treatment they are simulated by breaking the orbital symmetry, i.e., by using an orbital-occupation dependent one-electron potential

1 LDA+U LSDA (6.26) − nασ |ασ ασ | = Vσ + (U − J ) Vσ 2 α where U, J are the on-site Hubbard and exchange energy and α denotes the 3dorbitals. In a charge ordered state the different orbital occupations of inequivalent V-sites cause relative shifts of their orbital energies. As shown in Figure VI.16 this leads to a dxy subband splitting with a charge transfer gap CT . It moves the Fermi level to the top of the lower subband, thus creating a charge transfer insulator in the CO phase. The size of the gap is CT 0.5–1 eV. A gap of this size was indeed found in optical conductivity measurements.240 Calculation of the total LDA+U energy for various CO structure favors the zig-zag structure in one ladder,239 however so far it cannot say anything on the arrangement of adjacent CO ladders or whether only every second ladder exhibits CO as proposed in 238 H. Smolinsky, C. Gros, W. Weber, U. Peuchert, G. Roth, M. Weiden, and C. Geibel, Phys. Rev. Lett. 80, 5164 (1998). 239 A. N. Yaresko, V. N. Antonov, H. Eschrig, P. Thalmeier, and P. Fulde, Phys. Rev. B 62, 15538 (2000). 240 C. Presura, D. van der Marel, M. Dischner, C. Geibel, and R. K. Kremer, Phys. Rev. B. 62, 16522 (2000).

98

P. FULDE ET AL.

F IG . VI.16. Left panel: LDA+U DOS of α -NaV2 O5 with U = 4.1 eV and J = 1.1 eV exhibits two isolated 3dxy subbands due to enforced charge order with a charge transfer gap CT ∼ 0.5–1 eV between them. Right panel: Tight binding (TB) fit to LDA bands (CT = 0) with full V-O basis corresponding to effective hopping elements tR = 0.380 eV, tL tD = 0.085 eV for the effective V-V TB model with only dxy -states included. Note that within LDA a metallic state is predicted with EF lying in the lower dxy band. (After Ref. [239].)

the structure model of Ref. [230] and others. The nature of the insulating phase above Tc is an unsolved problem since every rung is only singly occupied, i.e., one has quarter filled V-ladders. Even without CO when CT vanishes there is an excitation gap for double occupancy of V-V rungs. An interpretation as a simple Mott–Hubbard insulator in an effective dxy -one band model based on the molecular orbital (bonding) state of a rung seems inadequate. An interpretation of the insulating state in terms of an extended Hubbard model has been proposed in Ref. [241]. Such microscopic models require as an input the effective hopping parameters obtained from a mapping of LDA band structure to a tight binding model. It was shown in Ref. [239] that an adequate mapping requires a basis of both V dxy and O px , O py orbitals. The result is shown in Figure VI.16 for the full basis. Nevertheless in a crude approximation this may be further simplified by mapping to an effective dxy model containing only three hopping parameters tR , tL and tD along the rung, leg and diagonal of a single ladder (inset of Figure VI.17). Their values are given in Figure VI.16. It is found that tL tD . This leads to the essentially flat upper band in Figure VI.16 (right) and therefore tD cannot be neglected. It is also essential to obtain the proper exchange Hamiltonian for the zig-zag CO structure [111] which will be discussed now. The description of the coupled CO and exchange dimerization in α -NaV2 O5 starts from an extended Hubbard model containing hopping terms discussed before, the on-site effective Coulomb energy Ueff 3 eV and unknown intersiteCoulomb energies VR , VL and VD for the same bonds as the hopping integrals 241 A. Bernert, Ph.D. thesis, TU Dresden (2001).

STRONGLY CORRELATED ELECTRONS

A

B

A

99

B

F IG . VI.17. Charge order and dimerization in α -NaV2 O5 . Left panel: Shift of V-positions in distorted a-layer below Tc1 . Stacking along c is of aaa a type. In a -layers A shifts have the same phase and B shifts are moved by one lattice constant along b (ladder direction). Each layer has three inequivalent V (full, open and gray circles), leading to 6 inequivalent V. Charge order (zig-zag) happens mainly on A, ladder dimerization on B. Below Tc2 the A ladders also dimerize and V sites on B become inequivalent leading to 8 inequivalent V sites altogether. Right panel: Variation of effective spin exchange along the ladder (b-direction) with V charge order parameter 2δCO for zig-zag CO (A). 0 is the actual charge order parameter for α -NaV O on A-ladders corresponding to J = 440 K δCO A 2 5 (37.9 meV). Inset shows TBA hopping elements tR (along rung a), tL (along leg b) and tD (along diagonal) on a ladder plaquette. The same convention for inter-site Coulomb interactions VR , VL and VD is used. (After Ref. [242].)

(inset of Figure VI.17). For an investigation of CO, this model may be reduced to a much simpler one taking for granted an insulating state with double occupancies of rungs prohibited. Then the charge degrees of freedom are described by a pseudo spin T = 12 where Tz = ± 12 describes a dxy electron that occupies the left (− 12 ) or right (+ 12 ) V-atom of a rung.243 The projected Hamiltonian in the charge sector then has the form244

ij

ij HITF = KLz Tiz Tjz + KI L Tiz Tjz + 2t˜Ri Tix (6.27)

i,j L

i,j I L

i

which is the Ising model in a transverse field (ITF) whose role is plaid by the renormalized intra-rung hopping t˜Ri . In the spin sector one has a Heisenberg Hamiltonian with exchange between the spins on neighboring rungs and legs ij ij (Eq. (6.30)). Like the Ising interaction ‘constants’ KLz (intra-ladder) and KI L 242 A. Bernert, P. Thalmeier, and P. Fulde, Phys. Rev. B 66, 165108 (2002). 243 P. Thalmeier and P. Fulde, Europhys. Lett. 44, 242 (1998). 244 A. Bernert, T. Chatterji, P. Thalmeier, and P. Fulde, Eur. Phys. J. B 21, 535 (2001).

100

P. FULDE ET AL.

(inter-ladder) t˜Ri is related to the original Hubbard parameters which are renormalized by terms that depend on the spin configuration:242 ij

KLz = 2VL + δKLz (Si , Sj ) ij

KI L = −VI L + δKI L (Si , Sj )

δ t˜R (Si , Sj ). t˜R = tR +

(6.28)

ij L

In this model the charge (T) degrees of freedom and spin (S) degrees of freedom are coupled through the renormalized interaction constants of Eq. (6.28) that depend on the spin configuration. As a consequence, even above Tc the optical conductivity which probes the (rung) charge excitations also shows a signature of coupled spin excitations.245 For the moment, considering only the possibility of charge ordering we may freeze the spins in an AF or FM configuration along or between the ladders according to the sign of the spin exchange obtained in LDA+U calculations.239 This leads to values t˜R = −0.19 eV and KLz −KI L = 0.68 eV.242 One might expect that the Hamiltonian in Eq. (6.27) on the rigid Trellis lattice describes charge order in a natural way, however this is not so obvious. It is true that the ITF on a single ladder (first and last term in Eq. (6.27)) has a (doubly degenerate) ground state with staggered ‘AF’ (KLz > 0) pseudo-spins corresponding to zig-zag charge order along the ladder if the magnitude of the ‘transverse field’ t˜R is smaller than a critical value 4t˜Rc = KLz . This value defines the quantum critical point λc = 1 of the ITF model93 with the dimensionless control parameter λ = KLz /4t˜R . For λ > λc , and assuming an infinitesimal staggered field to lift the twofold ground-state degeneracy, the order parameter of zig-zag CO is given by the exact solution of the 1D ITF:

2 1 8 z λc i1 1− Ti = (−1) = (−1)i δCO (λ). (6.29) 2 λ However due to the Trellis lattice structure (Figure VI.14) the rungs of a ladder form a trigonal covering lattice and therefore the inter-ladder coupling KI L frustrates the zig-zag charge ordering on a given ladder. Therefore the critical λc (KI L ) increases monotonously with the inter-ladder coupling which defines a quantum critical line for zig-zag CO at T = 0 in the KLz –KI L plane. At finite temperature the presence of frustration prevents zig-zag CO to occur. If KI L becomes equal to the intra-ladder KLz , CO melts and for some range of KI L even at T = 0 a disordered state appears. Finally if KI L increases even further one obtains again a CO state, but now with in-line order with parallel alignment of pseudo spins 245 M. V. Mostovoy, D. I. Khomskii, and J. Knoester, Phys. Rev. B 65, 064412 (2002).

STRONGLY CORRELATED ELECTRONS

101

along a ladder, i.e., V4+ configurations are on one side of the ladder and V5+ on the other side. These conclusions have been drawn from an exact diagonalization study of the 2D model with finite KI L .246 The LDA+U results for α -NaV2 O5 (see Ref. [239]) imply a relation 2VL − VI L 0.027 eV meaning KLz KI L . Therefore α -NaV2 O5 is indeed close to the quantum critical line for zig-zag charge order and purely Coulombic interactions cannot lead to a phase transition at finite temperature in this compound due to geometric frustration. This is rather similar to the charge ordering in the pyrochlore- or spinel lattices (or their 2D analogue, the checkerboard lattice) where charge ordering is also prohibited by the inherent geometric frustration due to corner sharing tetrahedra of V- or other 3d ions of different valencies (Section VII). In such structures CO requires the lifting of macroscopic degeneracy of the charge configurations by a lattice distortion as is the case in AlV2 O4 (see Section VII.17). Something similar happens in α -NaV2 O5 . The driving mechanism for the lattice distortion is here the spin superexchange energy between singly occupied rungs along a ladder. Due to the quarter-filled ladders the superexchange does not only contain terms coming from intermediate states with doubly occupied sites but also contributions from rungs with two singly occupied sites. The latter depend on the pseudospin configurations, which is the complementary effect as compared to Eq. (6.28). Therefore the effective spin exchange constants will depend on the degree of charge order. One obtains

Jij Sij Si+1j Hex = i,j

Jij = 1 +

α

uαi+ 1 ,j ∇ αi+ 1 ,j 2 2

z J Tijz , Ti+1j

ij z z J Tijz , Ti+1j = J0 1 + f Tijz , Ti+1j uij =

λq

λ† 1 λ . exp iqRij bqj + bqj 1/2 (mN )

(6.30)

The summation runs over the atomic shifts uij of neighboring atoms (α = O, Na) with respect to V which modulate the superexchange. In addition the latter depends on the charge configuration. Therefore spin (Si ), charge (Ti ) and lattice λ ) degrees of freedom are now coupled via Eq. (6.30). The spin exchange in (bqj Eq. (6.30) has to be added to Eq. (6.27) to get the total Hamiltonian HISSP of the z ) Ising-spin Peierls model for α -NaV2 O5 . To simplify the model the J (Tijz , Ti+1j 246 A. Langari, M. A. Martin-Delgado, and P. Thalmeier, Phys. Rev. B 63, 144420 (2001).

102

P. FULDE ET AL. ij

dependence is approximated by Jij = J0 (1 − 4Tjz 2 ). This reduction of superexchange (Figure VI.17) with increasing charge order was explained before. The remaining spin-lattice part is treated within the Cross–Fisher theory.224 The combined spin-Peierls transition and charge ordering takes place at Tc1 . At that temperature the renormalized frequency of the VO-bond dimerization mode with wave vector q0 = π/b along the ladder given by 2 (6.31) ω˜ q20 (T ) = ωq20 − 0.26gVO (q0 ) T −1 − 4gI2s χq0 (T ) becomes soft, i.e., when ω˜ q20 (Tc1 ) = 0. Here the last term is determined by the pseudo-spin susceptibility χq0 (T ) of HITF where gI s is a coupling constant that describes the change of the transverse pseudo-spin field with lattice distortion. It may be shown that inclusion of a spin-Zeeman term leads to the proper field dependence of Tc1 (H ) observed in experiment. It is found to be much weaker than for a pure spin Peierls transition. The choice of the precise order parameter and distortion pattern between the ladders below Tc1 is determined by the minimization of the total free energy. On a given ladder there is a competition between the exchange dimerization energy gain of the spin Peierls distortion and the zig-zag charge order because the former is proportional to J and the latter reduces J as just discussed (Figure VI.17). This can be avoided by generating two inequivalent types of ladders A and B below Tc1 where one (A) is mainly charge ordered and the other (B) mainly dimerized.242 At the same time this reduces the symmetry of the Trellis lattice in such a way that geometric frustration is reduced and long range charge order is stabilized at a finite temperature. Indeed, X-ray results230,233 show that the distortion of B-type ladders is much stronger as of Atype ladders, independent of whether orthorhombic Fmm2 or monoclinic A112 space groups are used for the structure refinement (Figure VI.17, left panel). At this stage, slightly below Tc1 one has a large spin gap on B ladders but none on the zig-zag spin chains on the A ladders. However the rapidly growing charge order δCO (T ) on A-type ladders below Tc1 modulates the hopping integrals and orbital energies via Na- and rung O- shifts. This occurs in such a way that an additional but smaller exchange dimerization is also induced on the A-type ladders. It grows with δCO (T ). Once it is big enough it leads to a further dimerization below Tc2 on the A-type ladders which is now of the pure spin-Peierls type and opens the spin gap seen in experiment (Figure VI.15). This interpretation is supported by the appearance of additional Na-NMR splittings caused by the shifts of Na atoms on top of the A-ladders for T < Tc2 . They correspond to 8 instead of 6 inequivalent Na positions below Tc2 which is indeed compatible with the monoclinic A112 structure from X-ray analysis.233 Although the mechanism for the phase transitions is intricate, involving charge, spin and lattice degrees of freedom and their competing coupling effects, the low temperature (T Tc ) spin dynamics is quite simple again. With charge order and

STRONGLY CORRELATED ELECTRONS

103

lattice distortion saturated only the pure spin part in Eq. (6.30) of the original ISSP Hamiltonian remains. Thereby the existence of two inequivalent A,B-type ladders and their low temperature (T Tc1 ) distortions in the parameterization of exchange constants has to be taken into account. Since the B ladders are strongly exchange dimerized with a δB ∼ 0.25 and J = JB (1 ± δB ) they have a large spinexcitation gap B = 38 meV.242 It is not visible in the inelastic neutron scattering (INS) results which show a minimum excitation energy around 10 meV. It must therefore result from excitations on the more weakly dimerized (δA δB ) A-type CO ladders. Consequently the low temperature spin Hamiltonian comprises only slightly dimerized 1D zig-zag S = 1/2 spin chains (on A) with an intra-chain exchange JA (1 ± δA ) along the b-direction. Since they are separated by intervening B-ladders the A-ladders are only weakly coupled with Ja JA in the transverse a-direction. One therefore would expect gapped quasi-1D spin excitations in α NaV2 O5 . Indeed it was found that their dispersion is much stronger along b than along a.247,248 As mentioned earlier the stacking of layers along c is of the aaa a type.249 Therefore the zig-zag chains on A are in-phase on aa (and a a ) bilayers and out-of-phase between aa . In the c-direction one may therefore assume an exchange Jc within the bilayers and neglect coupling between them. Using this effective exchange model with parameter set (JA , δA , Ja , Jc ), where Ja = Ja − 4JD is an effective intra-chain exchange along a, the magnetic excitations have been calculated within a local dimer approach. It is applicable here since JA Ja , Jc . The susceptibility of an isolated dimer pair in the bilayer is given by u± (ω) =

2(JA (1 + δA ) ∓ Jc ) . (JA (1 + δA ) ∓ Jc )2 − ω2

The collective susceptibility of the bilayers in RPA is then expressed as −1 q , ω) = 1 − J ( q )u± (ω) u± (ω). χ ± (

(6.32)

(6.33)

The dispersion of spin excitations in the ab plane may be obtained from the poles q , ω) as of χ ± ( 2 2 ω± (qx , qy ) = JA (1 + δA ) ∓ Jc − JA (1 + δA ) ∓ Jc × JA (1 − δA ) cos 2qy ± Ja cos(qx − qy ) − 4JD cos qx cos qy . (6.34) 247 B. Grenier, L. P. Regnault, J. E. Lorenzo, T. Ziman, J. P. Boucher, A. Hiess, T. Chatterji, J. Jegoudez, and A. Revcolevschi, Phys. Rev. Lett. 86, 5966 (2001). 248 T. Yosihama, M. Nishi, K. Nakajima, K. Kakurai, Y. Fuji, M. Isobe, C. Kagami, and Y. Ueda, J. Phys. Soc. Jpn. 67, 744 (1998). 249 K. Ohwada, Y. Fuji, K. Y. J. Muraoka, H. Nakao, Y. Murakami, H. Sawa, E. Ninomiya, M. Isobe, and Y. Ueda, Phys. Rev. Lett. 94, 106401 (2005).

104

P. FULDE ET AL.

The comparison of mode dispersions with experimental results is shown in Figure VI.18. Using the low temperature JA = 440 K (see Ref. [248]) which corresponds to the charge order parameter 2δCO = 0.32 in Figure VI.17 the remaining parameters may be determined from three of the four observed gaps ω± (0, 12 ) and ω± (0, 1) in Figure VI.18. The fourth (lowest) gap is then correctly calculated as ω− (0, 1) = 8.14 meV. The exchange dimerization obtained is δA = 0.03 δB . The model calculation explains a number of observations from INS:

F IG . VI.18. Dispersion of spin excitations in α -NaV2 O5 (qx a and qy b given in r.l.u. 2π/a and 2π/b respectively). Comparison of theoretical fit after Eq. (6.34) with experimental results from Ref. [247]. Full lines: qy0 = 12 , broken lines q0y = 1. Upper panel: ω+ (qx )-dispersion (top) and ω− (qx )-dispersion (bottom). From extremal values at qx = 0 model parameters δA = 0.03, Ja = 0.21 meV and Jc = 0.43 meV are obtained. Lower panel: Dispersion along b with exchange JA = 37.9 meV (440 K) along zig-zag chain on A. (After Ref. [242].)

STRONGLY CORRELATED ELECTRONS

105

(i) The dispersion along b is much larger than along a because Ja JA due to weak coupling of A-ladders through intervening B-ladders. (ii) The a-dispersion of ω+ (qx , qy0 ) is considerably smaller than for ω− (qx , qy0 ) with qy0 = 12 or 1. (iii) Contrary to earlier results248 the high resolution experiments247 presented in Figure VI.18 show a finite gap between lower and upper mode +− 1 meV which is determined by a combination of JA and Jc . It provides strong evidence for the inequivalent A-B ladder model. If only equivalent A-ladders were present, the gap should vanish, i.e., ω+ (qx , qy0 ) and ω− (qx , qy0 ) would touch with their minima and maxima and the dispersion would have twice the observed period along a.250 We conclude that α -NaV2 O5 presents another example where charge ordering may lead to pronounced 1D character of spin excitations below Tc , here they are gapped due to exchange dimerization caused by the complicated nature of the associated lattice distortions. It has become clear that CO in α -NaV2 O5 is severely inhibited by effects of geometric frustration. In fact its comparatively low Tc 33 K indicates that it is close to the quantum critical point of the ITF model, where the CO is of essentially 1D Ising type. The true 2D ordered state at finite T is then established by a staggered longitudinal pseudo spin field set up by the distortions of the neighboring ladders. In this scenario it is suggestive that even small perturbations of the 1D Ising spin correlations along the ladder might suppress the CO state in α -NaV2 O5 . This can be achieved by reducing the filling factor n of the 1D ladders below 14 by doping with holes. This introduces “empty” rungs into the ladder which cut the Ising bonds. The ensuing destruction of long-range 1D correlations should then strongly reduce Tc as function of the hole concentration δh (n = 14 − δh ). This has indeed been found by introducing holes into the ladders through Na-deficiency doping251 where a few per cent holes are sufficient to destroy the CO state and the associated spin Peierls transition. Rapid suppression of charge order has also been found in various other doping series, i.e., replacing Na by Li and K (isoelectronic) or Ca (electron-doping).252 This may be observed directly by specific heat measurements252 which show a progressive suppression of C(Tc ) with increasing doping. It is also seen in the susceptibility251 which exhibits a closing of the spin gap associated with CO. Most importantly, in this doping range α -Nax V2 O5 remains an insulator. This is not easy to understand within a Hubbard like model for the quarter filled ladder.244,242 Possibly 1D localization and polaronic effects play a role, indeed the conductivity was found to exhibit variable-range hopping behavior251 for hole doping. It was shown in 250 C. Gros and R. Valenti, Phys. Rev. Lett. 82, 976 (1999). 251 M. Isobe and Y. Ueda, J. Alloys Compounds 261–263, 180 (1997). 252 M. Dischner, C. Geibel, E. Morré, and G. Sparn, J. Magn. Magn. Mat. 226–230, 405 (2001).

106

P. FULDE ET AL.

Ref. [253] that even for the (hole-) doped case the CO problem may be treated with an extended pseudo-spin model. In order to incorporate the possibility of empty rungs on a ladder a pseudo spin T = 1 is introduced where the |Tz = ±1 states describe occupation of the right or left V dxy orbital of a rung respectively, and in addition |Tz = 0 the empty (hole-doped) rung. The total effective T = 1 Hamiltonian of a single ladder is then given by

H= ( − μ)Tzi2 + tR Txi2 − Tyi2 − h0si Tzi i

+ 2tL

j† i i† j Ozy Ozy + Ozy Ozy ij

+ V−

Tzi Tzj + V+

ij

Tzi2 Tzj2 .

(6.35)

ij

= h0s (−1)i is a longitudinal stagHere is the on-site orbital energy and gered pseudo-spin field that simulates the effect of distortion connected with CO and the coupling to neighboring ladders, ij denotes n.n. rungs along the ladder. Here Ozy = iTz Ty may be interpreted as a quadrupolar operator in the T = 1 pseudo-spin space. Furthermore is the dxy orbital energy and μ, a ‘chemical potential’ to fix the number of holes δ = 1 − n (n = number of d-electrons per rung) at a value determined by the doping. Interaction parameters are defined as V± = 12 (VL ± VD ). If the ladder diagonal term VD is neglected then V± = 12 VL leads to a control parameter λ = 2tR /VL (to stay in accordance with Ref. [253] the inverse value of the previous definition for λ is used here). In isospin language the (staggered) CO parameter δCO and the hole doping δh are given by δCO = Tz1 = −Tz2 , (6.36) δh = 1 − Tz2 . h0s (i)

Here i = 1, 2 denote the two 1D sublattices along the ladder direction b. The selfconsistent mean-field solution of the model is shown in Figure VI.19 (lower panel). Its usefulness relies on the Ising type nature of the ordered state. It shows that close to the QCP λc = 1 the charge order parameter is rapidly suppressed with increasing doping which is also evident from the δh -dependence of the slope shown in the inset. This behavior corresponds qualitatively to the rapid reduction of CO in Na-deficiency doped α -Nax V2 O5 where the spin-gap and hence the associated charge order is suppressed by a few per cent Na-deficiency 1 − x. For small doping one may assume that the latter is equal to the average hole concentration δh in the V-rungs. 253 P. Thalmeier, Physica B 334, 60 (2003).

STRONGLY CORRELATED ELECTRONS

107

F IG . VI.19. Upper panel: Melting of charge order by Na-deficiency (1 − x) (hole) doping seen from the rapid closing of the spin gap in χ(T ) with increasing 1 − x (corresponding nominally to δh ). (After Ref. [251].) Lower panel: Calculated melting of CO with hole doping δh for various λ = 2tR /VL given in decreasing order. The absolute slope value −(dδCO /dδh ) increases strongly when approaching the quantum critical point λc = 1 of CO; this is shown in the inset. (After Ref. [253].)

Finally we briefly discuss the β-vanadium bronzes β-Na0.33 V2 O5 with large but stoichiometric (1 − x = 2/3) Na deficiency doping. Their crystal structure is different but it still contains the Trellis lattice layers. For high temperatures these compounds are 1D metals (only in the stoichiometric case) along the b-axis and

108

P. FULDE ET AL.

exhibit a CDW-instability at TCDW = 136 K into an insulating state.254 While the Wigner-lattice type CO transition discussed for α -NaV2 O5 is due mostly to intersite Coulomb interaction energies of localized 3d electrons, the CDW Fermisurface instability in β-Na0.33 V2 O5 is driven by the kinetic energy of 1D conduction electrons. Under pressure the CDW transition may be suppressed again and around pc 8 GPa the TCDW (p)-line ends in a quantum critical point with an associated superconducting dome around a maximum superconducting Tc of about 10 K. 15. R EENTRANT C HARGE O RDERING AND P OLARON F ORMATION IN D OUBLE E XCHANGE B ILAYER M ANGANITES L A 2−2x S R 1+2x M N 2 O 7 The layered perovskite manganites have been at the center of 3d-oxide research since the discovery of the colossal magnetoresistance effect (CMR).255 Its signature is a change in the resistivity over several orders of magnitude under comparatively small magnetic field changes for doped metallic manganites close to the ferromagnetic phase transition. The investigation of CMR has led to a global survey of doped manganite compounds. Their structures consist of MnO6 octahedra corner-linked to layers that may be stacked in different fashions. As in the cuprates, the parent compounds are AF Mott–Hubbard insulators and hole doping destroys the AF order. However, the metallic state is not superconducting but ferromagnetic. In the manganites the doping with holes only reduces the Mn-moments, rather than creating non-magnetic Zhang–Rice singlets as in the cuprates. The Mn moments then order ferromagnetically via the double exchange (DE) mechanism256,257 that lowers kinetic energy of eg conduction electrons when their spins are aligned with spins of localized Mn-t2g spins (see Figure VI.25). The physics of manganites, especially those derived from the infinite layer parent compound LaMnO3 , has been reviewed in many articles, e.g., Ref. [22]. In this chapter we shall focus exclusively on aspects of the bilayer manganites with half-doped insulating compound LaSr2 Mn2 O7 that are related to charge ordering and possible polaronic effects. In addition we discuss magnetic excitations in the doped metallic ferromagnetic bilayer compounds which give evidence for the double exchange mechanism that is central to the physics of magnetic phases and magnetotransport. This topic has also been more extensively reviewed in 254 K. Okazaki, A. Fujimori, T. Yamauchi, and Y. Ueda, Phys. Rev. B 69, 045103 (2004). 255 Y. Moritomo, Z. Asamitsu, and Y. Tokura, Nature 380, 141 (1996). 256 C. Zener, Phys. Rev. B 82, 403 (1951). 257 P. W. Anderson and H. Hasegawa, Phys. Rev. B 100, 675 (1955).

STRONGLY CORRELATED ELECTRONS

109

F IG . VI.20. Left panel: Crystal structure of LaSr2 Mn2 O7 and La2−2x Sr1+2x Mn2 O7 consisting of MnO6 octahedra and (La,Sr)-cations (circles). Lattice constants are (x = 0.5) a = 3.874 Å, c = 19, 972 Å. The space group is I4/mmm. Right panel: Structural and magnetic phase diagram of bilayer La2−2x Sr1+2x Mn2 O7 in the doping range 0.3 < x < 1.0. Charge order (CO) appears for 0.5 x 0.65. Around x = 0.7 magnetic order is absent. (After Ref. [258].)

Ref. [259]. We first give a brief summary of structural properties. The manganites belong to the Ruddlesden–Popper phases which may be described by intergrowth of rock-salt like MnO slabs and n slabs of the perovskite LaMnO3 . For n = ∞ one has the infinite layer LaMnO3 perovskite, while n = 2 corresponds to the bilayer manganite La2−2x Sr1+2x Mn2 O7 considered here. Its structure is shown in Figure VI.20. In the (hypothetical) compound with x = 0 La and Sr are tri- and divalent cations which implies a Mn3+ (S = 2) state for the magnetic cations. Replacing La by Sr according to the chemical formula La2−2x Sr1+2x Mn2 O7 is equivalent to hole doping and creates Mn4+ (S = 3/2) with a nominal concentration of x holes/Mn site. For x = 0.5 one has a stoichiometric mixed-valent compound LaSr2 Mn2 O7 with a 1:1 ratio of Mn3+ /Mn4+ ions. This suggests the possibility of charge (and orbital) ordering leading to an insulating state. In the possible concentration range 0.2 < x < 1 the crystal structure remains the same although the Mn–O bond lengths depend on x due to the Jahn–Teller distortion of 258 X. Qiu, S. J. L. Billinge, C. R. Kmety, and J. F. Mitchell, cond-mat/0307652 (2003). 259 T. Chatterji, G. Jackeli, and N. Shannon, in Colossal Magnetoresistance Manganites, Kluwer Aca-

demic Publishers (2004), chap. 8, p. 321.

110

P. FULDE ET AL.

the octahedrons containing Mn3+ . The AF (x = 0.5) and FM (x < 0.4) structures are shown later in Figure VI.25. Electronic structure calculations for LaSr2 Mn2 O7 within LSDA+U (see Ref. [260]) lead to a quasi-2D band structure that is close to that of a half metal. The gap between majority and minority spin bands is ↑↓ = 2.7 eV. The influence of possible charge ordering has been neglected in this calculation. Due to the CEF splitting of 3d states into t2g and eg states, the lower lying t2g bands, which are ∼ 1 eV below EF are almost dispersionless while the bands crossing EF have mainly eg character. This allows one to use a simple model for the electronic structure: While the eg electrons are described in a nearest neighbor (n.n.) tight-binding (TB) approximation, the t2g electrons are treated as localized with the intra-atomic exchange aligning their spins to a total spin S (S = 3/2) (see Figure VI.25). Furthermore, there is a Hund’s rule coupling of strength JH which tries to align localized t2g and itinerant eg spins. Finally on-site (U ) and inter-site (V ) Coulomb interaction terms for the eg electrons have to be added. Then one obtains the total Hamiltonian

†

H= tij ciσ cj σ + h.c. + U ni↑ ni↓ + V ni nj ij σ

− JH

i

Si si + J

i

ij

Si Sj .

(6.37)

ij

Here the first three terms describe eg conduction electrons (ciσ ) where niσ = † ciσ ciσ and ni = ni↑ + ni↓ , the fourth term describes FM Hund’s rule coupling (JH > 0) between eg -spins (s) and t2g spins (S) and the last one a superexchange between the localized t2g spins. Note that i = (l, λ) where λ = 1, 2 is the bilayer index and l the site within a layer. The model is able to describe both the charge ordering and magnetism in the manganites. The orbital degree α = 1, 2 of eg electrons is still missing. It is too complex to be solved in full generality, we therefore treat CO and magnetic aspects separately and disregard the possibility of simultaneous orbital order. To investigate charge order as function of the eg band filling n we take into account only the first three terms which constitute an extended Hubbard model (EHM) for the eg electrons. Assuming identical CO in both layers the problem reduces to the EHM on a 2D square lattice. Magnetic order will be suppressed and two-sublattice (A,B) charge order is assumed. In the limit U t > V this model may be treated261 by a combination of Hartree–Fock approximation for the inter-site term (V ) and a CPA approximation for the on-site Hubbard term (U ). 260 P. K. de Boer and R. A. de Groot, Phys. Rev. B 60, 10758 (1999). 261 A. T. Hoang and P. Thalmeier, J. Phys. Condens. Matter 14, 6639 (2002).

STRONGLY CORRELATED ELECTRONS

111

The latter rests on the alloy-analogy, i.e., the EHM is replaced by a single-particle Hamiltonian with diagonal (sites 1,2 within each layer) disorder of eg orbital en(1,2) (1,2) ergies EA/Bσ and corresponding probabilities pA/Bσ on each sublattice. Accordingly, (1)

EA/Bσ = zV nA/B (2)

(1)

with pA/Bσ = 1 − nA/B−σ

EA/Bσ = zV nA/B + U

(2)

with pA/Bσ = nA/B−σ .

(6.38)

The Green’s functions of the equivalent single-particle Hamiltonian is then configuration averaged within CPA, i.e., requiring the average T -matrix of the system to vanish. This leads to averaged Green’s functions tk2 ¯ A/B (k, ω) = ω − A/B (ω) − (6.39) G ω − B/A (ω) where tk = (t/2)(cos kx + cos ky ). The corresponding self-energies are given by ¯ A/B (ω) zV NB/A A/B (ω) = E¯ A/B − zV nB/A − A/B (ω) G + U − A/B (ω) . (6.40) Here E¯ A/B = zV nB/A + 12 U nA/B are the effective orbital energies on A/B sublattices. On the bipartite lattice CO has to be symmetric which leads to the restriction nA/B = n ± nCO . This requires only a single averaged Green’s function defined ¯ A/B (ω). From the above equations the self energies may be by G(±nCO , ω) = G eliminated. One obtains a cubic equation for G from which the order parameter nCO may be calculated as function of filling n and Coulomb interaction parameters U, V by requiring charge conservation. Setting nCO = 0 the phase boundary between CO and homogeneous phase is obtained as a surface in (n, U, V ) space. It is obtained as an implicit solution of the equations 2 n=− dω f (ω) Im G(0, ω) and π 2 (6.41) dω f (ω) Im G (0, ω) 1=− π where the derivative is defined as G (ω) = ∂G(nCO , ω)/∂nCO |nCO =0 and f (ω) is the Fermi function. The self-consistent solution for charge order has been determined for the 2D square lattice (z = 4 and W = 4t = half bandwidth). The resulting n–V and V –T phase diagrams for CO are shown in the left and right part of Figure VI.21 respectively. In the n–V phase diagram we notice two regions. For n < n∗ ∼ 0.67 the CO boundary Vc (n) is almost independent of U while for n > n∗ when the half filled case n = 1 is approached CO is strongly suppressed with increasing U . This is due to the fact that in a Mott–Hubbard in-

112

P. FULDE ET AL.

F IG . VI.21. Left: n–V phase diagram of charge order (CO) for the 2D EHM (T = 0, W = 4t ≡ 1) and U = 0, 0.5, 1.5, ∞ corresponding to dotted, long-dashed, dashed and solid lines respectively. Right: V –T phase diagram of CO for U = 2 and various band filling n = 0.3, 0.5, 0.65 and 0.8 corresponding to solid, dash-dotted, dotted and dashed curves respectively. The CO regime is to the right of the boundary for each value of n. Energies and temperature are given in units of t . (After Ref. [261].)

sulator charge fluctuations are already strongly suppressed and additional spatial symmetry breaking CO then needs a larger threshold value Vc . On the other hand for n < n∗ , e.g., quarter filling n = 1/2 the Vc ∼ 0.25W = t is determined essentially by the hopping t. The minimum Vc where CO is most easily achieved is obtained around n = n∗ . The V –T phase diagram shows an interesting aspect: For each value of U a range of V values exists for which the CO transition is reentrant as function of temperature. For such a V value the ground state is homogeneous while CO appears in an intermediate temperature range. This behavior cannot be obtained by treating the EHM in Hartree–Fock approximation and thus it is a genuine correlation effect. However, as we shall see, another mechanism based on polaron formation may also lead to reentrant CO. In the present model the absolute value of transition temperatures is unrealistically large because only the n.n. interaction V is assumed. This may be improved by including also a competing n.n.n. Coulomb repulsion which reduces the CO temperature as shown later. The predicted phase diagram of charge order qualitatively agrees with experimental observations, keeping in mind that due to electron–hole symmetry the calculated phase diagram can be used for the hole doped case of La2−2x Sr1+2x Mn2 O7 (x = 1 − n). One must note however that there is no unanimous agreement on doping range and temperature behavior of CO in this compound. Both depend considerably on the experimental method used to detect CO, e.g., X-ray, electron diffraction or transport measurements. In the latter case one

STRONGLY CORRELATED ELECTRONS

113

F IG . VI.22. Structure of charge and orbital order in stoichiometric (x = 0.5) LaSr2 Mn2 O7 corresponding to wave vector Q = ( 14 , 14 , 0). (After Ref. [262,263].)

finds CO in a broad range of doping (0.44 x 0.8) at TCO ∼ 200 K.264 Another observation is the collapse of CO or reentrance of the homogeneous phase at lower temperatures. Surprisingly a second reentrance of CO appears below 50 K as concluded from an upturn in the resistivity. From diffraction experiments the doping range of CO is somewhat smaller (0.5 x 0.65).258 For the stoichiometric case x = 0.5 (Mn3+ /Mn4+ = 1) the CO has first been observed in Ref. [262] by X-ray diffraction. If one had only CO one would expect a simple two-sublattice structure with Mn3+ /Mn4+ ordering corresponding to a commensurate superstructure with Q = ( 12 , 12 , 0). However one rather observes Q = ( 14 , 14 , 0). This is due to additional orbital ordering of Mn3+ eg orbitals in a staggered fashion (d3x 2 −r 2 /d3y 2 −r 2 ) on top of CO (see Figure VI.22). The Q = ( 14 , 14 , 0) superlattice reflexions are then due to the associated JT distortion of the crystal structure. The additional orbital order is not contained in the above single-orbital model. Below 100 K the superstructure reflections vanish, indicating melting of both CO and orbital order as conjectured from transport.264 Later X-ray experiments on LaSr2 Mn2 O7 (x = 0.5) have shown that there is also evidence for a CO reentrance below 50 K (see Ref. [265]) in agreement with Ref. [264]. This evidence for the second (CO) reentrance is seen in Figure VI.23. The intensity of reflexions in the reentrant CO region below 50 K is however much smaller, indicating much weaker CO. In fact, it seems sample dependent since it was not observed in other experiments. The possible existence of the second CO reentrance cannot be 262 T. Kimura, R. Kumai, Y. Tokura, J. Q. Li, and Y. Matsui, Phys. Rev. B 58, 11081 (1998). 263 Y. Wakabayashi, Y. Murakami, I. Koyama, T. Kimura, Y. Tokura, Y. Moritomo, Y. Endoh, and

K. Hirota, J. Phys. Soc. Jpn. 72, 618 (2003). 264 J. Dho, W. S. Kim, H. S. Choi, E. O. Chi, and N. H. Hur, J. Phys. Condens. Matter 13, 3655 (2001). 265 T. Chatterji, G. J. McIntyre, W. Caliebe, R. Suryanarayanan, G. Dhalenne, and A. Revcolevschi, Phys. Rev. B 61, 570 (2000).

114

P. FULDE ET AL.

F IG . VI.23. Temperature variation of superlattice reflexion intensities in LaSr2 Mn2 O7 corresponding to wave vector Q = ( 14 , 14 , 0) (cf. inset of Figure VI.24). Right: CO and first reentrance of homogeneous state. Left: second possible reentrance of CO below 50 K. (After Ref. [265].)

explained by the purely electronic EHM model. In fact around x = 1 − n∗ there is not even the first reentrance found to the homogeneous phase. Instead the charge order parameter increases monotonously with decreasing temperature as may be inferred from the V –T phase diagram (n = 0.65) in Figure VI.21. We note that Mn3+ /Mn4+ charge order has also been observed in the infinitelayer manganites, typically around the half-doped (x = 0.5) compounds, e.g., in La0.5 Ca0.5 MnO3 and R0.5 Sr0.5 MnO3 (R = Pr, Nd). For the Pr-compound CO was observed in a large doping range (0.3 x 0.7) similar as in the bilayer La2−2x Sr1+2x Mn2 O7 . The reentrance into the homogeneous phase was also observed in Pr0.5 Sr0.5 MnO3 , again only away from half doping (x = 0.5). It becomes especially pronounced in the presence of magnetic fields up to 10 T.266 There is no evidence for a second CO reentrance in the infinite layer compounds. To explain these phenomena in the stoichiometric bilayer LaSr2 Mn2 O7 a more extended but still single-orbital based theory is apparently needed. It was proposed in Ref. [267] that in this case CO is profoundly affected by polaron formation caused by a strong coupling to the lattice. This is suggestive since polaron formation changes the ratio of kinetic vs. intersite Coulomb energy of the holes and thus affects the conditions of CO. The electron–lattice coupling is due to the modulation of pd-hybridization along the in-plane bond directions caused by vibrations of oxygen atoms that form corner-sharing octahedra around the Mn ions. 266 Y. Tomioka, A. Asamitsu, H. Kuwahara, Y. Moritomo, and Y. Tokura, Phys. Rev. B 53, R1689

(1996). 267 Q. Yuan and P. Thalmeier, Phys. Rev. Lett. 83, 3502 (1999).

STRONGLY CORRELATED ELECTRONS

115

Effectively this leads to a coupling of the Mn3+ -eg level shift to a bond-stretching vibration of the oxygen. The latter may be assumed dispersionless with a frequency ω0 . We note that this refers to conventional Holstein-type polarons. They differ from the Jahn–Teller (JT) type polarons where the eg level is split by coupling to the JT symmetry distortions of the whole oxygen octahedron. The latter have been proposed for the slightly doped infinite layer La1−x Srx MnO3 in the region 0.1 x 0.2.268 The present Holstein-type model for the x 0.5 bilayer LaSr2 Mn2 O7 is described by

† † He−ph = g bi,δ + bi,δ (ni+δ − ni ) + ω0 bi,δ bi,δ . (6.42) i,δ

i,δ

† bi,δ

is the local vibration at oxygen site δ associated with Mn site i and g Here is the coupling constant. This has to be added to the EHM part, i.e., to the first three terms of Eq. (6.37). The latter is also generalized by including both n.n. interactions (V1 ) and n.n.n. interactions (V2 ) to achieve a realistic TCO which is controlled by the ratio (V1 − V2 )/t. In the limit of strong coupling (α ≡ g 2 /ω02 ∼ 1) the phonon coordinates may be eliminated by a combined Lang–Firsov (LF) transformation

† (ni+δ − ni ) g/ω0 bi,δ − bi,δ U1 = exp − i,δ

(see Ref. [269]), and squeezing transformation

† † U2 = exp γ bi,δ bi,δ − bi,δ bi,δ . i,δ

Here γ > 0 is a variational parameter270 determined by minimization of the ground-state energy. This leads again to an effective electronic model, but with renormalized hopping and interaction parameters. Furthermore, the on-site correlation problem is simplified by using the limit U → ∞ where the layers are fully spin polarized and we may assume spinless fermions. For x = 0.5 this implies the spinless half-filled band is realized in LaSr2 Mn2 O7 . Then, after applying U2 U1 the effective Hamiltonian reads, up to a constant,

†

Heff = −t˜ ci ci+δ + h.c. + (V1 + 2αω0 ) ni ni+δ i,δ

+ V2

i,δ

ni ni+η .

i,η 268 Y. Yamada, O. Hino, S. Nohdo, and R. Kanao, Phys. Rev. Lett. 77, 904 (1996). 269 I. G. Lang and Y. A. Firsov, Sov. Phys. JETP 16, 1301 (1963). 270 H. Zheng, Phys. Rev. B 37, 7419 (1988).

(6.43)

116

P. FULDE ET AL.

The first term describes hopping of small polarons. The essential point is that the effective hopping element t˜ = t exp[−5ατ coth(ω0 /2T )] with τ = exp(−4γ ) is strongly temperature dependent. It is small compared to the bare hopping t when T ω0 and increases for T ω0 because the occupation of the n-phonon modes decreases with T eventually until only the effect of zero-point fluctuations in t˜ is left. This T -dependent renormalization of t˜ is very important for charge ordering to take place, since the latter is determined by the balance of kinetic and intersite Coulomb energies. Treating the intersite Coulomb terms for two sublattices A,B in Hartree–Fock approximation as before and choosing ni = 1/2 ± nCO , i ∈ A, B, the condition for the CO instability line is 2V 1 tanh[2 (t˜z)2 + (V nCO )2 /T ] K( 1 − z2 ) dz (6.44) 1= 2 π 0 (t˜z)2 + (V nCO )2 where K is the complete elliptic function of the first kind and z = ε 2 − (4V nCO )2 /4t˜ with V = V12 + 2αω, V12 = V1 − V2 . For T → 0 this equation has always a solution with nCO > 0. For a reasonable parameter set (t, ω0 , V12 ) its solution leads to the α–T phase diagram shown in Figure VI.24. Depending on the size of α, both the non-reentrant and double-reentrant scenarios are possible. There is an intermediate region for α ∼ 0.65 where on lowering the temperature one obtains

F IG . VI.24. α–T phase diagram for the spinless (half-filled) case of the Holstein–EHM model with parameters V12 = 0.1, ω0 = 0.05 in units of t = 4 · 103 K. For comparison, the thin line corresponds to a t˜ which is kept constant (cf. Figure VI.23). The inset shows nCO (T ). The dotted, solid and dashed lines correspond to the three possible types of diagrams with α = 0.60, 0.65 and 0.68 respectively. (After Ref. [267].)

STRONGLY CORRELATED ELECTRONS

117

a CO phase, then a first reentrance into the homogeneous phase and subsequently a second reentrance into the CO phase. The corresponding variation of the order parameter nCO (T ) is shown in the inset of Figure VI.24 (full line). The other possible cases are also illustrated. Physically the behavior around α ∼ 0.65 may be explained as follows. First the effective hopping t˜ is reduced from the bare value and polaronic CO appears at relatively high temperatures. With decreasing temperature the kinetic energy (∼ t˜) increases until CO can no longer be maintained and the homogeneous state is stable again. For even lower temperatures CO always reappears because the n.n. tight binding Fermi surface has a nesting instability to CO for the half filled (spinless) case for arbitrary small values of V . The reentrance behavior discussed here is entirely due to the temperature dependence of the effective polaron hopping t˜ = t exp[−5ατ coth(ω/2T )]. Without it only the lowest CO transition does occur. This agrees with the previous study where no reentrance was observed for quarter filling including spin or spinless half filling. In the discussion of the reentrance behavior in La2−2x Sr1+2x Mn2 O7 we have so far invoked electronic correlation effects and polaron formation as origin but neglected the influence of coexisting magnetic order. A treatment of the full problem of CO would require the inclusion of spin degrees of freedom for finite values of U together with the last two exchange terms in Eq. (6.37) and the electron–lattice coupling. This is still an open problem. In the last part of this chapter we therefore focus on a rather complementary case: When the doping is large enough Coulomb correlation effects are less prominent and CO is absent for all temperatures. Then only the exchange terms in Eq. (6.37) are important. Double exchange (DE) illustrated in Figure VI.25 favors FM order within and between layers by optimizing kinetic energy gain for parallel eg (s = 1/2) conduction and t2g (S = 3/2) localized spins. In contrast superexchange (last term in Eq. (6.37)) favors AF orientation of moments between layers leading to the AF order in Figure VI.25 for x = 0.5. For 0.4 < x < 0.5 its competition with FM double exchange along the c-axis leads to a canting of moments out of the plane271 (CAF region in Figure VI.20) which may be interpreted as a superposition of an AF and FM structure. For x 0.4 the eg conduction bands become increasingly two-dimensional with d3z2 −r 2 character. Therefore double exchange along c increases significantly as discussed below. Consequently only the FM structure with FM bilayers remains and the last term in Eq. (6.37) may be neglected. The less than half-doped (x 0.4) metallic La2−2x Sr1+2x Mn2 O7 compounds are then described by the ferromagnetic (JH > 0) Kondo-lattice Hamil271 K. Hirota, S. Ishihara, H. Fujioka, M. Kubota, H. Yoshizawa, Y. Moritomo, Y. Endoh, and S. Maekawa, Phys. Rev. B 65, 64414 (1998).

118

P. FULDE ET AL.

F IG . VI.25. Left: AFM structure of stoichiometric (x = 0.5) CO insulator LaSr2 Mn2 O7 consisting of AF stacked FM layers along c. Right: FM structure of metallic (x = 0.4) La2−2x Sr1+2x Mn2 O7 . Moments are parallel to [110] in both cases. Center: Illustration of FM double exchange mechanism in doped manganites. FM polarization of itinerant eg spins (s = 1/2) leads to kinetic energy gain (∼ t ) due to FM Hund’s rule coupling (∼ JH ) to localized t2g spins (S = 3/2).

tonian HK = −t

† ciλα cj λα − t⊥

ij λα

− JH

† ci1α ci2α + h.c. iα

† Siλ · ciλα sαβ ciλβ .

(6.45)

iλαβ

Here t, t⊥ > 0 are the nearest neighbor hopping parameters within a layer and between the two partners (λ = 1, 2) of a bilayer along c respectively. Furthermore S and s are localized and conduction electron spins respectively with α, β =↑, ↓. In La2−2x Sr1+2x Mn2 O7 the lattice constants (x = 0.4) are a = 3.87 Å and c = 20.14 Å. The intra-bilayer splitting d a is much smaller than the distance D = 6.2 Å between adjacent bilayers (Figure VI.20). Therefore inter-bilayer hopping or exchange has been neglected above. Diagonalization of the hopping term leads to bonding and antibonding tight binding bands split by t⊥ with identical in-plane dispersion and a DOS given by σ ± (k) = − ±t⊥ + t (cos kx + cos ky ) N± () = N ( ± t⊥ );

2 1 2 2 1 N () = 2 K 1 − . W π W

(6.46)

The justification for this model and the size of its parameters can be obtained by considering the spin wave excitations below the Curie temperature TC . They have

STRONGLY CORRELATED ELECTRONS

119

been investigated by inelastic neutron scattering by various groups271–274 and analyzed in Refs. [275,276] both in the classical limit and with quantum corrections. In the manganites the condition JH t, t⊥ is fulfilled because the Hund’s rule coupling JH ∼ 2 eV is quite large. This greatly simplifies spin wave calculations because firstly the eg bands σ ± (k) will be spin-split such that only majority bands are occupied, i.e., n↑± = 1 and n↓± = 0 and secondly the large S = 3/2 local t2g spins allow for a 1/S expansion. This approach has been first applied to the cubic manganites277 and later used for the bilayer manganites.275,276 It turns out that in the limit JH → ∞, and to order 1/S one obtains classical spin waves of an effective Heisenberg model for t2g spins. The effective exchange constants are determined by the eg conduction band dispersion and filling. One obtains ωA (q) = zJ DE S[1 − γq ] ωO (q) = zJ DE S[1 − γq ] + 2J⊥DE S.

(6.47)

In two dimensions γq = 12 (cos qx + cos qy ) and ωA (q) and ωO (q) are the dispersion of acoustic (A) and optical (O) spin wave branches respectively. They have equal dispersion in the ab-plane and are split by the A-O gap AO = 2SJ⊥DE . In this approximation there is no spin-space anisotropy and therefore the A branch has no gap at k = 0. The effective Heisenberg exchange constants J DE , J⊥DE for t2g spins are given by F ±t⊥ 1 1 J DE = − 2 (0 + π ) with 0,π = N () d 2S 2z −W F ±t⊥ 1 t⊥ J⊥DE = 2 (n0 − nπ ) with n0,π = N () d. (6.48) 2S 2 −W The effective t2g exchange parameters J DE , J⊥DE termined by the eg band parameters in the limit simple result for the spin waves in the double good agreement with inelastic neutron scattering

are therefore completely deJH → ∞. This surprisingly exchange ferromagnet is in experiments on the x = 0.4

272 T. Chatterji, P. Thalmeier, G. J. McIntyre, R. van de Kamp, R. Suryanarayanan, G. Dhalenne, and

A. Revcolevschi, Europhys. Lett. 46, 801 (1999). 273 T. Chatterji, L. P. Regnault, P. Thalmeier, R. Suryanarayanan, G. Dhalenne, and A. Revcolevschi, Phys. Rev. B 60, R6965 (1999). 274 T. G. Perring, D. T. Adroja, G. Chaboussant, G. Aeppli, T. Kimura, and Y. Tokura, Phys. Rev. Lett. 87, 217201 (2001). 275 T. Chatterji, L. P. Regnault, P. Thalmeier, R. van de Kamp, W. Schmidt, A. Hiess, P. Vorderwisch, R. Suryanarayanan, G. Dhalenne, and A. Revcolevschi, J. Alloys Compounds 326, 15 (2001). 276 N. Shannon, T. Chatterji, F. Ouchni, and P. Thalmeier, Eur. Phys. J. B 27, 287 (2002). 277 N. Furukawa, J. Phys. Soc. Jpn. 65, 1174 (1996).

120

P. FULDE ET AL.

F IG . VI.26. Left panel: Acoustic and optic spin wave branches along [100] direction with a splitting AO = 6 meV and overall dispersion of 40 meV. Full lines are obtained from the classical dispersion expression in Eq. (6.47). Right panel: Acoustic spin wave dispersion along [001]. An extrapolated anisotropy gap A (0) = 0.04 meV is obtained. (After Ref. [275].)

La2−2x Sr1+2x Mn2 O7 . This is seen in the left panel of Figure VI.26. Two parallel A and O modes are observed with a maximum zone-boundary energy of ωA (qx = πa ) ∼ 40 meV and an A-O splitting of AO = 6 meV. From these values one obtains SJ DE = 10 meV and SJ⊥DE = 3 meV. Using Eqs. (6.48) this leads to eg band parameters t = 0.175 meV and t⊥ = 0.1 eV. In the present theory there is no double exchange between adjacent bilayers and hence no spinwave dispersion along the c-axis. But experimentally a small dispersion along c was found (Figure VI.26, right panel) although it is two orders of magnitude smaller than the one along the a-axis. This requires an inter-bilayer DE constant J⊥DE with J⊥DE /J⊥DE 1.5 · 10−2 (see Ref. [272]) and shows that La2−2x Sr1+2x Mn2 O7 is an almost ideal two dimensional double exchange ferromagnet. This conclusion was supported by an analysis of diffuse neutron scattering which exhibits long range FM in-plane correlations far above the Curie temperature (∼ 2.3TC ).278 Finally, Figure VI.26 shows that a small extrapolated anisotropy gap A (0) ∼ 0.04 meV for the acoustic mode exists at the zone center whose microscopic origin is not clear. The double exchange model based on the FM Kondo lattice Hamiltonian is able to describe ferromagnetism and basic properties of spin wave excitations quite well. However it has its limits. Firstly quantum corrections of order 1/S 2 can278 T. Chatterji, R. Schneider, J. U. Hoffmann, D. Hohlwein, R. Suryanarayanan, G. Dhalenne, and A. Revcolevschi, Phys. Rev. B 65, 134440 (2002).

STRONGLY CORRELATED ELECTRONS

121

not be completely neglected as discussed in Refs. [259,276] and references cited therein. They lead to two effects: (i) reduction of the overall dispersion of spin waves. In the effective Heisenberg model this would necessitate a rescaling of the parameters J DE , J⊥DE or possibly an inclusion of more parameters; (ii) the local spin moment is coupled to density fluctuations in the itinerant system which leads to damping effects not present in the classical (1/S) approximation. Comparison with experiment shows that (1/S 2 ) corrections provide still insufficient damping and also cannot explain the observed deviations from the classical q-dependence of spin waves.276 It has also been proposed that a crossing with a phonon branch might be involved in these anomalies. Another shortcoming of the model is the neglect of orbital degeneracy of eg states. This has indeed dramatic effects on the doping dependence of the A-O spin wave splitting and the resulting effective exchange constants in the FM regime x = 0.3–0.4 as shown in Ref. [274]. When x decreases from the present value x = 0.4 the effective J⊥DE strongly increases while J DE stays almost constant. In the above double exchange model the anisotropy ratio is given by

J⊥DE t⊥ W (n0 − nπ ) = − . (6.49) DE J t 0 + π Assuming a doping independent t⊥ /t the above ratio changes at most by ∼ 10% in the doping range x = 0.3–0.4, which is much too small to explain experimental observations. Therefore another mechanism must be invoked. It has been found279 that for decreasing x the MnO6 octahedra elongate significantly along the c axis due to the JT effect on eg orbitals which leads to a lower energy and hence larger occupation for d3z2 −r 2 orbitals as compared to dx 2 −y 2 orbitals. Since the former have larger overlap along the c axis, the effective t⊥ strongly increases with decreasing x. Thus it is really the prefactor (t⊥ /t) in the above equation which leads to the dramatic increase of J⊥DE and the A-O spin wave splitting with decreasing x. This effect was described phenomenologically in Ref. [276] and within a microscopic model in Ref. [280]. In our discussion of bilayer manganites we have focused on models for charge ordering which can be described as simple periodic superstructures caused by inter-site but short range Coulomb interactions supplemented by small polaron formation. We have also discussed the importance of the double exchange mechanism for explaining the spin excitations in the metallic ferromagnet away from half-doping. We have mostly neglected the complications of orbital order, JT distortions and the effect of longer range Coulomb interactions in the low doping 279 M. Kubota, H. Fujioka, K. Hirota, K. Ohoyama, Y. Moritomo, H. Yoshizawa, and Y. Endoh, J. Phys. Soc. Jpn. 69, 1606 (2000). 280 G. Jackeli and N. B. Perkins, Phys. Rev. B 65, 212402 (2002).

122

P. FULDE ET AL.

DE F IG . VI.27. Upper panel: Doping dependence of effective exchange parameters. Note that J⊥ is proportional to A-O spin wave splitting and J DE to the overall dispersion. Lower panel: Doping dependence of JT distortion JT (elongation along c) of MnO6 octahedra. (After Ref. [274].)

regime. This may lead to the important possibility of an inhomogeneous state due to phase separation of ferromagnetic metallic and charge ordered insulating regions. Such states may consist of metallic droplets or stripes of holes in an insulating environment. This possibility has been reviewed in Ref. [281]. These aspects may also be of great importance for explaining the giant magnetoresistance of the manganites.22 VII. Geometrically Frustrated Lattices

Usually the concept of frustration is used in connection with magnetic systems. When Ising spins with an antiferromagnetic interaction are placed onto certain lattices like a triangular one, the pair-wise interactions cannot be satisfied simultaneously and therefore are frustrated. Here we will associate the concept of frustration with lattice structures. We call a lattice geometrically frustrated when in case that its sites are occupied by antiferromagnetically coupled Ising spins the interactions are frustrated. Examples are in two dimensions the just mentioned triangular, the checkerboard or the Kagomé lattice. In three dimensions the pyrochlore lattice (see Figure VII.1) is the one most frequently investigated. For those lattices we want to study charge degrees of freedom, i.e., when the electron number at a lattice site is fluctuating. A frustrated 281 A. Moreo, S. Yunoki, and E. Dagotto, Science 283, 2034 (1999).

STRONGLY CORRELATED ELECTRONS

123

F IG . VII.1. Pyrochlore lattice consisting of corner-sharing tetrahedra.

lattice structure can have a degenerate ground state for special band fillings when electron correlations are strong. In fact, in the limit of large on-site and nearest-neighbor electron repulsions there exists an exponentially large number of configurations with minimal potential energy. This is particularly so when the number of electrons equals half the number of lattice sites. It is not surprising that this special feature which is closely related to a frustrated geometry leads to new theoretical models and special effects when the electrons are strongly correlated. In the center of our attention will be the above mentioned pyrochlore lattice and a two-dimensional projection of it, the checkerboard lattice. A pyrochlore lattice is a substructure of the spinels which have the composition AB2 O4 . They can be considered as face-centered cubes of O2− ions. The B ions are surrounded by an octahedron of O2− ions, i.e., BO6 and are positioned on corner-sharing tetrahedra which define the pyrochlore lattice. Here we want to consider metallic spinels in which the electrons are itinerant. They may undergo metal to insulator transitions which are usually accompanied by a structural distortion. The most studied example has been magnetite Fe3 O4 . A transition to an insulator already indicates that electron correlations may be strong in spinels but an unambiguous proof is the observed heavy-fermion behavior of LiV2 O4 at low temperatures.282 Another interesting case is AlV2 O4 . This material is either a poor metal or a semiconductor at low temperatures. It undergoes a structural phase transition at lower temperatures which apparently is caused by strong electron correlations. Finally, LiTi2 O4 is a metallic spinel which becomes supercon282 S. Kondo, D. C. Johnston, and L. L. Miller, Phys. Rev. 59, 2609 (1999).

124

P. FULDE ET AL. TABLE VII.1. S PINELS WITH A H ALF -I NTEGER VALENCY OF d I ONS M=

Li(Al)M2 O4

Ti

V

V(Cr)

Mn

LiTi2 O4

LiV2 O4

AlV2 O4

LiMn2 O4

(LiCr2 O4 ) average d-electron count per M-atom

d0.5

d1.5

d2.5

d3.5

ducting at a relatively high transition temperature of Tc = 13.7 K.283,284 Table VII.1 summarizes these materials with half-integer valency of the cations. In the following we start out with a reminder on Fe3 O4 for which a huge literature does exist. For references see, e.g., Ref. [285]. The purpose is to merely recall some of the basic facts in order to understand better the special features of strong electron correlations in LiV2 O4 , AlV2 O4 and other spinels. This is followed by a discussion of fractional charges. They are found when a model Hamiltonian describing strongly correlated electrons with strong on-site and nearest-neighbor repulsions is used and applied to a frustrated lattice. Magnetite Fe3 O4 has been much investigated because of the important role it has played in the development of magnetism and magnetic materials. It is a spinel of the form AB2 O4 with A = Fe3+ and B = Fe2.5+ sites. We assume that 50% of the B sites are in a Fe2+ and Fe3+ configuration each, i.e., that electron correlations are so strong that Fe+ or Fe4+ configurations are suppressed. Magnetite undergoes at 120 K a phase transition from a metallic high-temperature phase to an insulating low-temperature phase. This transition was first observed by Verwey and Haayman8 and is usually referred to as Verwey transition. Verwey presented also a model for its description in terms of an order-disorder transition, which is entropy driven. The implicit assumption regarding B sites is thereby that the repulsions of electrons on neighboring sites are so strong that the kinetic energy term of the electrons plays only a minor role and may be neglected when the phase transition is considered. With an average valence of the B sites of +2.5 this implies that two neighboring Fe2+ sites and also two Fe3+ sites repel each other, while Fe2+ –Fe3+ sites attract. Let us denote by Vαβ the interaction between two neighbors Feα+ –Feβ+ . An order-disorder phase transition will take place when δV = V33 + V22 − 2V23 > 0.

(7.1)

Verwey suggested a particular charge ordering for the insulating low-temperature phase in which the Fe2+ and Fe3+ sites of the pyrochlore lattice order in form of 283 D. C. Johnston, J. Low Temp. Phys. 25, 145 (1976). 284 R. W. McCallum, D. C. Johnston, C. A. Luengo, and M. B. Maple, J. Low Temp. Phys. 25, 177

(1976). 285 M. Isoda and S. Mori, J. Phys. Soc. Jpn. 69, 1509 (2000).

STRONGLY CORRELATED ELECTRONS

125

two families of chains pointing in the [110] and [110] direction, respectively. However, the situation is more complicated than that. First one should realize that in the absence of electron hopping the ground state is highly degenerate. In order to minimize the Coulomb interactions Vαβ , two of the sites of each tetrahedron of the pyrochlore structure must be occupied by a Fe2+ and two by a Fe3+ ion (tetrahedron rule). There is an exponentially large number of different configurations which satisfy this rule.286 When a small hopping of electrons is taken into account this degeneracy is partially lifted. How that is taking place remains an unsolved problem. It is possible that the electronic ground state would remain disordered, i.e., liquid like as long as the lattice is unchanged. In that case charge order could result from a structural distortion which is accompanying the metal-insulator transition. Indeed, the experimental determination of the electronic low-temperature phase has been a challenging and controversial subject as has been a proper theoretical interpretation. A recent review287 describes the development of different theoretical models starting from a Hubbardlike Hamiltonian including nearest-neighboring repulsions288 up to inclusion of electron–phonon interactions together with the tetrahedron rule.289 Calculations in the frame of density functional theory based on LDA+U and the observed low temperature lattice structure produce charge order which agrees with estimates based on a valence bond analyses.290 They also conclude that the tetrahedron rule is not strictly fulfilled. This is due to the kinetic energy, i.e., electronic hopping terms which lead to violations of that rule. Nevertheless, for a simple reason the tetrahedron rule must be satisfied to a high degree. Without considerable short-range order it would be difficult to understand the relatively low transition temperature of the Verwey transition. For a conventional order– disorder phase transition the transition temperature is given by TV = 2δV /kB , where kB is Boltzmann’s constant. This would imply a TV of several thousands of Kelvin.286 16. M ETALLIC S PINELS : L I V 2 O 4 — A M ETAL WITH H EAVY Q UASIPARTICLES In order for a spinel oxide to be conducting, the electron count of the B ions in AB2 O4 should differ from an integer number. The compounds listed in Ta286 P. W. Anderson, Phys. Rev. 102, 1008 (1956). 287 F. Walz, J. Phys. Cond. Matt. 14, R285 (2002). 288 J. R. Cullen and E. Callen, J. Appl. Phys. 41, 879 (1970). 289 D. Ihle and B. Lorenz, Phil. Mag. 42, 337 (1980). 290 I. Leonov, A. N. Yaresko, V. N. Antonov, M. A. Korotin, and V. I. Anisimov, Phys. Rev. Lett. 93,

146404 (2004).

126

P. FULDE ET AL.

ble VII.1 are therefore of special interest. As mentioned before LiTi2 O4 with d 0.5 per Ti ion is a superconductor with a transition temperature of Tc = 13.7 K. LiV2 O4 with d 1.5 per V ion is a metal with heavy quasiparticle excitations. At ambient pressure no spin- or charge order has been observed down to the lowest temperature. The compound LiCr2 O4 is not stable and therefore AlV2 O4 with d 2.5 per V ion is particularly interesting. This system becomes a charge ordered insulator by so-called valence skipping (see the next section). Finally LiMn2 O4 with d 3.5 per Mn ion is an antiferromagnetic insulator with a Néel temperature of TN = 280 K. Charge ordering is taking place in that material which has been used in batteries. In the following we will discuss LiV2 O4 in more detail. As pointed out above LiV2 O4 shows at low temperatures heavy-fermion behavior, i.e., it supports heavy quasiparticle excitations.282,291 It has been the first system where the heavy quasiparticles originate from d electrons. Experiments show that the γ coefficient of the low temperature specific heat C = γ T is strongly enhanced and of order γ 0.4 J mol−1 K−2 . The spin susceptibility is equally enhanced at low T . Over a large temperature regime it shows a behavior χS = χ0 +

C , T +

= 63 K

(7.2)

i.e., of Curie–Weiss type. The Sommerfeld–Wilson ratio RW = πkB2 χS (T = 0)/(3μ2B γ ) is found to be RW = 1.7. The temperature independent term χ0 = 0.4 · 10−4 cm3 /mol and the Curie constant is C = 0.47 cm3 K/(mol V). The sign of indicates antiferromagnetic interactions between V sites but no magnetic ordering was found down to 4.2 K. In view of the frustrated lattice this is understandable. The resistivity is found to be ρ(T ) = ρ0 + AT 2 with a large coefficient A = 2μ cm K−2 . The Kadowaki–Woods ratio A/γ 2 ,292 a hallmark of heavy quasiparticles is in the range of other heavy-quasiparticle materials.293 These findings are typical signatures of heavy fermion systems. From the specific heat data one may determine the entropy S(T ). One finds that S(T = 60 K) − S(T = 2 K) = 10 J/(mol · K) which is close to 2R ln 2 where R is the gas constant. The implication is that at 60 K the system has almost one excitation per V ion. This is inconceivable with a conventional band description of the d electrons. According to Pauli’s principle only a small fraction of them is participating in the excitations 291 S. Kondo, D. C. Johnston, C. A. Swenson, F. Borsa, A. V. Mahajan, L. L. Miller, T. Gu, A. I. Goldman, M. B. Maple, D. A. Gajewski, Phys. Rev. Lett. 78, 3729 (1997). 292 K. Kadowaki and S. B. Woods, Solid State Comm. 58, 507 (1986). 293 C. Urano, M. Nohara, S. Kondo, F. Sakai, H. Takagi, T. Shiraki, and T. Okubo, Phys. Rev. Lett. 85, 1052 (2000).

STRONGLY CORRELATED ELECTRONS

127

F IG . VII.2. Energy bands for electrons in a pyrochlore lattice with one orbital per site in the presence of nearest neighbor hopping. The upper flat band is two-fold degenerate. (After Ref. [285].)

when a one-electron picture is applied. Calculations based on the LDA show that the electrons near the Fermi energy have t2g character.294–296 These states are well separated from the eg states as well as from the oxygen states (see Figure VII.3). The width of the t2g bands is of order 2 eV and therefore at 60 K only a small fraction of the electrons in t2g states would contribute to the excitations. In fact, the calculated density of states must be multiplied by a factor of 25 in order to account for the large γ value. This provides convincing evidence for strong electron correlations in LiV2 O4 . Further support is given by the observation that the material undergoes a phase transition into a charge ordered state at approximately 6 GPa.297,298 Presumably this metal–insulator transition is again accompanied by a structural distortion as in Fe3 O4 . It is worth pointing out that the band structure of a pyrochlore lattice has interesting features, which are simple to derive when only nearest-neighbor hopping is taken into account. The Hamiltonian of noninteracting electrons with nearestneighbor hopping t is given in diagonal form by

† α (k) − μ akασ akασ (7.3) H0 = kασ

294 J. Matsuno, A. Fujimori, and L. F. Mattheiss, Phys. Rev. B 60, 1607 (1999). 295 D. J. Singh, P. Blaha, K. Schwarz, and I. I. Mazin, Phys. Rev. B 16, 359 (1999). 296 V. Eyert, K.-H. Höck, S. Horn, A. Loidl, and P. S. Riseborough, Europhys. Lett. 46, 762 (1999). 297 K. Takeda, H. Hidaka, H. Kotegawa, T. C. Kobayashi, K. Shimizu, H. Harima, K. Fujiwara,

K. Miyoshi, J. Takeuchi, Y. Ohishi, et al., Physica B 359–361, 1312 (2005). 298 K. Fujiwara, K. Miyoshi, J. Takeuchi, Y. Shimaoka, and T. Kobayashi, J. Phys.: Condens Matter 16, S615 (2004).

128

P. FULDE ET AL.

F IG . VII.3. Partial densities of states (DOS) for LiV2 O4 calculated in LDA. The flat band of Figure VII.2 corresponds to the spike at 1 eV. (After Ref. [296].)

where α = 1, . . . , 4 is a band index due to 4 atoms/unit cell and one orbital per site is assumed. The band energies are 2t, α = 3, 4 1 α (k) = 2 α = 1, 2 −2t 1 ± (1 + ηk ) ηk = cos(2kx ) cos(2ky ) + cos(2ky ) cos(2kz ) + cos(2kz ) cos(2kx ) (7.4) where kν is given in reciprocal lattice units 2π a . The bandstructure is shown in Figure VII.2. One notices a two-fold degenerate flat band which is unoccupied provided t > 0. Hopping processes beyond nearest neighbors do not give the flat band a dispersion. This is only the case when the hopping matrix elements differ for different orbitals. The essential features of the simplified bands are still visible in the bands calculated by LDA (see Figure VII.3). As regards heavy quasiparticles the crucial question is which degrees of freedom are associated with their formation. Usually one relates spin degrees of freedom with the low energy excitations giving rise to the heavy quasiparticles. This has been discussed at length, e.g., in Sections III, V and VI. However, in a frustrated lattice one might also think of charge degrees of freedom giving rise to a large number of low energy excitations. The high degeneracy of the ground state in the absence of a kinetic energy term in the Hamiltonian is lifted when hopping processes are included and the entropy can be released over a small temperature range. This is discussed in one of the next sections for the strong correlation limit. Nonetheless, the finding that the entropy at 60 K is close to 2R ln 2 suggests that here too spin degrees of freedom are responsible for the large low temperature specific heat coefficient γ .

STRONGLY CORRELATED ELECTRONS

129

In the following we give an estimate which shows that spin degrees of freedom in the pyrochlore structure are indeed able to explain the size of γ in LiV2 O4 . In setting up the Hamiltonian we include repulsive interactions between electrons on neighboring sites. In view of the observed charge ordering under pressure, the following Hamiltonian seems appropriate

†

H =− tν ciνσ cj νσ + h.c. + U niν↑ niν↓ + U niν niμ ij ν

+ J˜

iνμ

siν siμ + V

iν

ni nj +

ij

i;ν>μ

Jij (Si , Sj )Si Sj .

(7.5)

ij

Here i is a site and ν is an orbital index (ν = 1, 2, 3) denoting the different t2g orbitals. The first term is the kinetic energy or electronic hopping term. For the purpose of the intended estimate for γ we will later neglect it. The following three terms describe the intra-atomic Coulomb repulsions and spin interactions. For simplicity we have neglected the differences in the repulsions when different orbitals at site i are involved. Otherwise we would have to introduce an additional parameter U (compare with Eq. (7.7) below). Finally, the last two terms are due to the Coulomb repulsions and antiferromagnetic spin spin interactions between neighboring sites. Hereby Si = ν siν . For an estimate of the spin contributions to the γ coefficient we assume that the tν are very small so that they do not play a role. Then the d 2 configurations have spin S = 1. The Coulomb repulsions are minimized if on each tetrahedron two sites are in a d 1 configuration with S = 1/2 and two are in a d 2 configuration with S = 1. Let us pick out one of the exponentially large number of degenerate ground-state configurations (see Figure VII.4). One notices that all S = 1/2 sites form chains and rings and the same holds true for the sites with spin 1. The smallest rings consist of six sites. These features are independent of the chosen configuration. By means of constrained LDA+U calculations one can determine the nearest-neighbor spin coupling constants Jij (Si Sj ).299 One finds for J (1/2, 1/2) = 3 meV and J (1, 1) = 24 meV implying that the spin 1 sites are much stronger coupled to each other than the spin 1/2 sites. Note that spin 1 chains have a gap in the expectation spectrum, i.e., the Haldane gap H .300,301 Therefore spin 1/2 chains and rings are virtually uncoupled from each other. They can be coupled only via spin 1 chains. But the coupling between the two is frustrated and it takes a considerable energy H 0.41J (1, 1) to excite the spin 1 chains and rings. Therefore the spin 1/2 chains remain essentially uncoupled and 299 P. Fulde, A. N. Yaresko, A. A. Zvyagin, and Y. Grin, Europhys. Lett. 54, 779 (2001). 300 F. D. M. Haldane, Phys. Lett. A 93, 464 (1983). 301 F. D. M. Haldane, Phys. Rev. Lett. 50, 1153 (1983).

130

P. FULDE ET AL.

F IG . VII.4. Pyrochlore lattice: Example of a configuration satisfying the tetrahedron rule. Occupied sites with S = 1 (black dots) are connected by thick solid lines which form chains or rings. The same may be done for occupied sites with S = 1/2 (yellow dots).

we can determine directly the γ coefficient of the specific heat and the susceptibility from the relations.302 γ=

kB R 2 , 3 J (1/2, 1/2)

χs =

4μ2eff R . π 2 J (1/2, 1/2)

(7.6)

Note that the Sommerfeld–Wilson ratio is RW = 2. An experimental fit of γexp would require J (1/2, 1/2) = 1.2 meV instead of the calculated 3 meV. It is known that spin interactions are overestimated by a LDA+U calculation. But in any case, the improvement which is needed by applying the above localized electron picture to determine the γ coefficient is much less than the factor of 25 which is missing when a band approach is used. The above estimate suggests that a description of electrons in LiV2 O4 should start from the localized limit instead from the band limit because in the former case the required corrections by including tν = 0 are much less. There have been also a number of attempt to explain the heavy quasiparticle in LiV2 O4 with an on-site Hubbard interaction U only, i.e., without including Coulomb repulsions between neighboring sites. Thereby one of the t2g electrons is kept as localized while the remaining 0.5 electron per V site is treated as delocalized. The following argument is used to justify this distinction. Due to a slight 302 J. C. Bonner and M. E. Fisher, Phys. Rev. A 135, 640 (1964).

STRONGLY CORRELATED ELECTRONS

131

distortion of the oxygen octahedra surrounding the V sites the t2g states split into a lower a1g and two eg states. The splitting is much smaller than the corresponding bandwidths. Indeed, a LDA bandstructure calculation294–296 finds the total occupancies n(eg ) = 1.1 and n(a1g ) = 0.4 implying a similar population of the different t2g orbitals. But when instead a LDA+U calculation is performed303 the a1g state is singly occupied while the remaining 0.5 electrons per V site are of eg character. However, this seems to be a typical mean-field result. From an atomic point of view there is no reason why an a1g electron should not be able to hop to a neighboring site like an eg type electron. The following Hamiltonian based on the LDA+U findings has been used and investigated beyond mean-field approximation304

†

H =− t12 ci1σ cj 2σ + h.c. + U niα↑ niα↓ + U ni1 ni2 ij

− J˜

Si (σi1 + σi2 ) + J

i

iα

i

(7.7)

Si Sj .

ij

The indices 1 and 2 refer to the two eg orbitals. Due to Hund’s rule the coupling at site i between a localized a1g electron with spin Si and an eg electron with spin 1 2 σiα (α = 1, 2) is ferromagnetic. The spin–spin interactions between neighboring sites i and j are antiferromagnetic. Otherwise the system would order ferromagnetically. The on-site Coulomb repulsion of eg electrons is chosen to be different when the electrons are in the same orbital and when they are not. The spin–spin interaction between the eg electrons is neglected. A strong Hund’s rule coupling is assumed between the a1g and the eg electrons by taking the limit J˜ → ∞. The nearest neighbor spin correlations between the localized a1g electrons imply that the effective hopping matrix element t12 (S) of the eg electrons depends on the relative spin orientation of the a1g electrons, i.e., 1 + Si Sj t12 (S) = t12 . (7.8) 2S 2 The determination of Si Sj takes into account the frustrated lattice, here the pyrochlore structure 305 With the above simplification the Hamiltonian (7.7) reduces to

† † H =− t12 (S) ci1 cj 2 + ci2 cj 1 + h.c. + U ni1 ni2 . (7.9) ij

i

303 V. I. Anisimov, M. A. Korotin, M. Zölfl, T. Pruschke, K. L. Hur, and T. M. Rice, Phys. Rev. Lett. 83, 364 (1999). 304 M. S. Laad, L. Craco, and E. Müller-Hartmann, Phys. Rev. B 67, 033105 (2003). 305 B. Canals and C. Lacroix, Phys. Rev. Lett. 80, 2933 (1998).

132

P. FULDE ET AL.

The ci operators have only one additional index which takes the values 1 and 2 and acts like a pseudospin. Therefore Eq. (7.9) has the form of a Hubbard Hamiltonian with a spin dependent hopping matrix element. This Hamiltonian has been treated for the 1/4 filled case by iterated perturbation theory.304 When U is increased a Kondo-like sharp resonance is obtained at the Fermi surface resulting in heavy quasiparticles at low temperatures. Thermodynamic as well as transport properties can be expressed in terms of a cross-over temperature T ∗ , going from a heavy Fermi liquid to a spin liquid at T > T ∗ . There have been also a number of other attempts to explain the heavy quasiparticles which we want to mention. One approach starts from a Hamiltonian similar to (7.7) but replacing the two eg orbitals by a single one.306 Nearestneighbor spin correlations are treated by a mean-field ansatz Si Sj = − 32 2 and so are Hund’s rule correlations Si σ i = u2 . The mean field u is determined from a pseudo-hybridization between the a1g electron and the itinerant, i.e., eg electron. A subsidiary condition ensures that there is one a1g electron per site. Two temperatures characterize that approach. Above T = Tmag the quantity = 0 and the susceptibility is Curie–Weiss like because the intersite correlations have vanished. Similarly, a vanishing mean field u marks the second temperature THF ( 20 K) below which a narrow a1g band at EF appears giving rise to heavy quasiparticles. More details are found in Ref. [306]. The mean-field approach has been generalized by treating also the a1g electron as itinerant. The on-site Coulomb repulsion between the eg and a1g electrons is taken into account in a slave boson mean-field approximation.307 In effect the a1g bandwidth is strongly renormalized and gives rise to a sharp resonance at EF . There have been also weak coupling approaches to explain the heavy quasiparticles. One suggestion is based on multicomponent fluctuations due to the t2g and spin degrees of freedom.308 One of the consequences of the large orbital contributions to the γ coefficient of the specific heat is a small Sommerfeld–Wilson ratio of RW 0.1. Another approach treats the pyrochlore structure of the V ions as a network of Hubbard chains.309 Due to this one-dimensional feature electron correlations have strong effects on electron-hole excitations and hence on the selfenergy.

306 C. Lacroix, in Proceed. HFM 2000, Canad. J. Phys. 79, 135 (2000). 307 H. Kusunose, S. Yotsuhashi, and K. Miyake, Phys. Rev. B 62, 4403 (2000). 308 Y. Yamashita and K. Ueda, Phys. Rev. B 67, 195107 (2003). 309 S. Fujimoto, Phys. Rev. B 65, 155108 (2002).

STRONGLY CORRELATED ELECTRONS

133

17. S TRUCTURAL T RANSITION AND C HARGE D ISPROPORTIONATION : A LV 2 O 4 The spinel AlV2 O4 is of interest because the average d-electron number per V ion is 2.5 and therefore the configurations are expected to fluctuate between 3d 2 and 3d 3 . However, what actually happens is that the system undergoes a phase transition at approximately Tc = 700 K to a charge ordered state. It is associated with a change of the lattice structure from pyrochlore to alternating Kagomé and triangular planes. This is shown in Figure VII.5. In the low temperature rhombohedral phase the [111] axis is elongated while the perpendicular axes are shortened in order to keep the volume of the unit cell nearly constant. Experimental results are shown in FigureVII.6. The figure contains also a plot of the observed changes of the angle between two unit vectors of the rhombohedral lattice as the temperature

F IG . VII.5. Distortion of a pyrochlore lattice by elongation along the [111] axis. The resulting rhombohedral lattice consists of Kagomé and triangular planes.

F IG . VII.6. AlV2 O4 : Dependence of the V–O bond lengths on temperature. V1 and V2 refer to V2+ and V4+ ions while O1 and O2 are different oxygen ions. (After Ref. [310].) 310 J. Matsuno, T. Katsufuji, S. Mori, Y. Moritomo, A. Machida, E. Nishibori, M. Takata, M. Sakata, N. Yamamoto, and H. Takagi, J. Phys. Soc. Jpn. 70, 1456 (2001).

134

P. FULDE ET AL.

F IG . VII.7. Resistivity and magnetic susceptibility at 1 Tesla as function of temperature for AlV2 O4 . The left inset shows the low temperature field cooled (FC) and zero field cooled (ZFC) susceptibility in a field of 10−2 Tesla. (After Ref. [310].)

is lowered below the phase transition temperature. Note that there are three times as many sites on the Kagomé lattice than there are on the triangular one. In a simplified description the V ions have a valency of V4+ on the triangular and V2+ on the Kagomé sites corresponding to d 1 and d 3 configurations, respectively. The charge disproportionation is often called valence skipping. Of course, this is a simplified view since in reality the disproportionation is considerably less than the separation 4 × d 2.5 → 3 × d 3 + 1 × d 1 would suggest. The system avoids frustration by distorting. Unfortunately the experimental results are still sparse. It is not even clear whether AlV2 O4 is a poor metal or a small gap semiconductor at low temperatures. Resistivity measurements as well as those of the susceptibility are shown in Figure VII.7. The structural phase transition shows up in both quantities, i.e., by a small but steep increase in the resistivity and a pronounced decrease of the magnetic susceptibility. For a description of the phase transition one must set up a model Hamiltonian. It should also allow for explaining differences of charge ordering in AlV2 O4 and in LiV2 O4 under pressure. While AlV2 O4 is a semiconductor or a metal in the charge ordered state, LiV2 O4 becomes an insulator.297 Electronic structure calculations based on LDA+U provide a realistic description of magnetic insulators but are not suitable for strongly correlated paramagnetic metals. Therefore we exclude them here and start from a microscopic model Hamiltonian at the price of having to introduce adjustable parameters. Nevertheless, we can uncover this way the processes which lead to the observed structural transition and the accompanying charge order. From standard band-structure calculations it is known that only t2g states are near the Fermi energy (compare with Figure VII.3). All other bands

STRONGLY CORRELATED ELECTRONS

135

are well above or below EF . Therefore it suffices to include only t2g electrons in the model Hamiltonian. We write it in the form H = H0 + Hint + He−p , with

νν † H0 = tμμ (l, l )clμνσ cl μ ν σ lμ,l μ

(U + 2J ) Hint = nlμν↑ nlμν↓ + U nlμνσ nlμν σ¯ ν

lμ

+ (U − J )

ν>ν

nlμνσ nlμν σ +

ν>ν

V 2

nlμνσ nl μ ν σ

lμ,l μ νν σ σ

1 δμ,1 − (1 − δμ,1 ) nlμνσ + K He−p = l2 . 3 μ lνσ

(7.10)

l

Here H0 describes the kinetic energy. The electron creation and annihilation operators are specified by four indices, i.e., for the unit cell (denoted by l), the sublattice (μ = 1−4), the t2g orbital (ν = dxy , dyz , dzx ), and the spin (σ = ↑, ↓). The brackets . . . indicate a summation over nearest-neighbor sites. The term Hint describes the on-site Coulomb and exchange interactions U and J among the t2g electrons. The last term contains the Coulomb repulsion V of an electron with those on the six neighboring sites. Finally He−p describes the coupling to lattice distortions. The deformation potential is denoted by . It is due to a shift in the orbital energies of the V sites caused by relative changes in the oxygen positions. While the energy shift is positive for the V (1) sites it is negative for the V (2) sites. The elastic constant K refers to the c44 mode and describes the energy due to the rhombohedral lattice deformation. It is reasonable to assume that like in Fe3 O4 311 and Yb4 As3 199 only the c44 mode is strongly coupled with the charge disproportionation. One can give at least approximate values for all parameters except for V and . Their ratio will be fixed by the charge-ordering transition temperature while keeping the constraint V U . For the on-site Coulomb- and exchange integrals we set U = 3.0 eV and J = 1.0 eV which are values commonly used for vanadium oxides.312 Band structure calculations which we have νν between different performed demonstrate that the hopping matrix elements tμμ orbitals ν = ν are negligible. For simplicity we can therefore omit ν, ν . Then 311 H. Schwenk, S. Bareiter, C. Hinkel, B. Lüthi, Z. Kakol, A. Koslowski, and J. M. Honig, Eur. Phys. J. B 13, 491 (2000). 312 A. Fujimori, K. Kawakami, and N. Tsuda, Phys. Rev. B 38, R7889 (1988).

136

P. FULDE ET AL.

tμμ (l, l ) = −t when l, l are nearest neighbors. We will take into account the orbital dependent hopping matrix elements coming from a tight-binding fit of LDA calculations. Furthermore the c44 elastic constant is neither known for AlV2 O4 nor for LiV2 O4 , while computational methods for its ab initio calculation in the case of materials with strong electronic correlations are not mature enough. (0) Therefore a representative value c44 / = 6.1 · 1011 erg/cm3 is used for AlV2 O4 where is the volume of the cubic unit cell with a lattice constant of a = 5.844 Å. This value is close to the experimental value for Fe3 O4 which has also the spinel structure. This leads to K 1.1 · 102 eV. The deformation potential is not known but is commonly of the order of the band width. For convenience we introduce the dimensionless coupling constant λ = 2 /Kt and lattice distortion δL = /t. From LDA calculations the bandwidth is 8t = 2.7 eV, and therefore a reasonable value is λt = 2 /K = 1 eV. This means = 10.5 eV which is twice the value of Yb4 As3 .31 Not contained in the Hamiltonian (7.10) is a spin–spin interaction term between the V ions. This might turn out a shortcoming since bandstructure calculations based on a local spin-density approximation (LSDA) to density functional theory find effective exchange constants which are strongly enhanced in the low temperature phase. Estimates are Jkk = Jkt = 202 K for the high temperature phase where the subscripts k and t refer to Kagomé and triangular sites. For the low temperature phase the corresponding estimates are Jkk = 360 K and Jkt = 167 K.313 Let us first consider H0 which is easily diagonalized. With four V ions per unit cell and three t2g orbitals there are altogether 24 bands, assuming that the spin symmetry is broken. Of those twelve are dispersionless and degenerate. Furthermore, there are two sixfold degenerate dispersive bands (compare with Figure VII.2). The Fermi energy is in a region of high density of states. More details are found in Ref. [285]. The next term we discuss is He−p which describes the deformation potential coupling. When it is sufficiently strong it leads to charge ordering. There is no opening of a gap though, but only a sharp decrease of the density of states near EF , i.e., the system remains a metal. This feature does not change when the interactions U and V are included in mean-field approximation, provided we deal with a paramagnetic state. Generally U suppresses charge ordering while V enhances it. Again, no gap opens at EF but the density of states decreases in its neighborhood. In mean-field approximation the relation between the homogeneous lattice distortion δL along [111] and charge disproportionation is given by δL =

λ(n2 − n1 ) 2

313 A. Yaresko, I. Leonov, and P. Fulde, Physica B, in press.

(7.11)

STRONGLY CORRELATED ELECTRONS

137

where n1 = νσ nl1νσ is the occupational number of the triangular sites while n2 = n3 = n4 with n2 = νσ nl2νσ is the one of the Kagomé sites. A shortcoming of the mean-field analysis is that it leads to a second-order phase transition instead of the observed first-order one. This is almost certainly due to strong correlations which suppress charge fluctuations between different vanadium sites. In order to incorporate them at least approximately, one must allow for unrestricted mean-field solutions by breaking the spin symmetry. But the constraint of zero total magnetic moment has to remain. This is done by ascribing to the sites μ of a tetrahedron an occupational number nμ and a magnetization mμ = νσ nlμνσ σ . The spins are assumed to be directed towards the center of the tetrahedron in the undistorted phase. For them the [111] direction is a convenient quantization axis. In the distorted phase the spins of the V (1) sites are slightly tilted with respect to this axis so that the net magnetization remains zero. The free energy is a function of the different nμ and mμ and must be minimized with respect to both. The energy bands do now depend on spin σ . The hopping matrix elements between nearest neighbor sites must be transformed accordingly, so that the different spin directions are accounted for. For details see Ref. [314]. As a result the charge disproportionation is found as function of the various parameters. We show in Figure VII.8 the results for T = 0 as function of the ratio V /t. As usual the calculated disproportionation is larger, here by a factor of 2.5 than

F IG . VII.8. Charge disproportionation based on Eq. (7.10) as function of V /t . The nμ denote the occupation numbers of the four sites of a tetrahedron. In the inset the changes in the density of states are shown when V /t is just below and above the critical value at which charge ordering sets in. For V /t = 1.67 one has n1 = 2.5 − 3δ and ni = 2.5 + δ (i = 2–4) with a charge disproportionation δ 0.25. Here U = 3.0 eV, J = 1.0 eV, λt = 1.0 eV and 8t = 2.7 eV. (After Ref. [314].) 314 Y. Z. Zhang, P. Fulde, P. Thalmeier, and A. Yaresko, J. Phys. Soc. Jpn. 74, 2153 (2005).

138

P. FULDE ET AL.

the one obtained from a valence band analysis of the measured distorted structure. This is due to the simplified model Hamiltonian which does not allow for screening by non-d electrons. The same difficulty was found for Yb4 As3 .31,315 Also shown in Figure VII.8 as an inset is the change in the density of states in the vicinity of the critical ratio (V /t)crit = 1.6 at which the transition to a charge ordered state does occur. The strong change which one can notice might explain the observed small but steep increase in the resistivity when charge ordering sets in. The phase transition is found to be of first order when the free energy is evaluated. For V /t = 1.67 the calculated transition temperature is Tc = 660 K which is reasonably close to the observed one of Texp = 700 K. Of course, there is some arbitrariness in the particular choice of V /t. It should be pointed out that the LSDA calculations yield a value of δ = 0.17 for the disproportionation and a small hybridization gap. In the undistorted phase the point symmetry of the vanadium ions is D3d and the t2g degeneracy is reduced to an a1g singlet and an eg doublet. In the distorted, i.e., charge ordered phase the symmetry of the triangular sites remains D3d while the one of the Kagomé sites is lowered to C2h . This lifts also the eg degeneracy. It is due to an elongation of the crystal in [111] direction and a contraction perpendicular to it. While in the distorted phase of AlV2 O4 the energies of the three orbitals are nearly the same because of a very small distortion of the oxygen octahedra one expects that in LiV2 O4 the energy of the a1g orbital is highest. There the distortion of the octahedra is fairly large. Since the changes in orbital energies are small in AlV2 O4 one expects that the system remains gapless even in the charge ordered state in agreement with LDA calculations. The LDA band structure can be reproduced by a proper choice of the hopping parameters. By determining self-consistently the occupational numbers of the three V (1) sites one xy yz xy yz yz xy zx zx finds that n2 = nzx 2 > n2 , n3 = n3 > n3 and n4 = n4 > n4 in the t2g basis. This shows that the ordered orbitals on sublattices 2, 3 and 4 are perpendicular to each other. There is no orbital ordering on the V (2) sites in the charge ordered state because of the small energy difference between the a1g and eg orbitals as compared with the bandwidth. The sharp decrease of the density of states near EF as well as the order of the charge ordering phase transition are not influenced by orbital order. The same holds true for the absence of an energy gap at EF . Therefore orbital ordering is of little importance for AlV2 O4 . These findings should be compared with charge ordering observed in LiV2 O4 under pressure. A crucial difference is the average d-electron number per V site which is 1.5 for LiV2 O4 as compared with 2.5 in the case of AlV2 O4 and the distinct role of the a1g orbital. Consequently in the limit t → 0 the a1g orbital is 315 U. Staub, B. D. Patterson, C. Schulze-Briese, F. Fauth, M. Shi, L. Soderholm, G. B. M. Vaughan, E. Dooryhee, J. O. Cross, and A. Ochiai, Physica B 318, 284 (2002).

STRONGLY CORRELATED ELECTRONS

139

empty at the V (1) sites of LiV2 O4 while the split eg orbitals are singly occupied with S = 1. On the V (2) sites with d 0 also the split eg orbitals are unoccupied. Therefore a gap at EF is expected in the charge ordered state. This is what is found when the Hamiltonian (7.5) is treated in mean-field approximation with a filling factor of 1/4 instead of 5/12 as in the case of AlV2 O4 . The opening of a gap can also be inferred from measurements of ρ(T ).297 Orbital ordering is obviously not relevant here. For further details we refer to Ref. [314]. The structure in the distorted phase on which the above theory has been based was recently called into question in Ref. [316]. Instead of a low-temperature structure consisting of triangular and Kagomé planes those authors interpret their data in terms of V7 molecular clusters. The future has to show which structure is the correct one. 18. F RACTIONAL C HARGES D UE TO S TRONG C ORRELATIONS Consider the pyrochlore lattice with half as many electrons than there are number of sites. We take the limit U → ∞ and neglect for simplicity the electron spin so that we are dealing with spinless fermions. In that case half of the lattice sites are singly occupied and half of them are empty. Restricting the inter-site Coulomb repulsion to nearest neighbors the Hamiltonian is

†

H = −t ci cj + h.c. + V ni nj . (7.12) ij

ij

The ci† create spinless fermions at sites i and as usual ni = ci† cj . As discussed before, the repulsion V is minimized when in each tetrahedron two sites are occupied and two sites are empty (tetrahedron rule). Let us now add one particle to the system. Since each site belongs to two tetrahedra, the above rule is violated for two neighboring tetrahedra which now contain three electrons each. The interaction energy is increased by 4V . But when one of the four nearest neighbors of the added particle hops onto an empty site the two tetrahedra violating the rule are separated. This is shown in Figure VII.9. The important point is that the interaction energy remains unchanged by this separation, i.e., it is still 4V . When the charge of the added particle is e, each fragment must be assigned a charge e/2. Taking into account the kinetic energy term of the Hamiltonian lifts the exponentially large degeneracy of the ground state which is present when the kinetic energy term is absent. Deconfinement of the charges e/2 remains intact provided 316 Y. Horibe, M. Shingu, K. Kurushima, H. Ishibashi, N. Ikeda, K. Kato, Y. Motome, N. Furukawa, S. Mori, and T. Katsufuji, Phys. Rev. Lett. 96, 086406 (2006).

140

P. FULDE ET AL.

F IG . VII.9. Separated tetrahedra on a pyrochlore lattice after an electron has been added to the system. Occupied sites are connected by solid red lines and empty by green lines (courtesy of F. Pollmann).

t/V is sufficiently small.317–319 Since a numerical study of a pyrochlore lattice is difficult we shall investigate instead the simpler checkerboard lattice. The latter can be considered a projection of the pyrochlore lattice onto a plane. But one must keep in mind that the lower dimension of the checkerboard lattice may result in different behaviors as regards confinement or deconfinement of the fractional charges e/2. This is known from lattice gauge theories which are closely related to the present problem317,320 Also the statistics of fractionally charged excitations may differ in two and three dimensions. In two dimensions the wavefunction of the particles belongs to a representation of the braid group while in three dimensions it is one of the permutation group. Figure VII.10 shows one of the ground state configurations. They have the form of string nets (see also Ref. [321]). In the absence of hopping the degeneracy is Ndeg = (4/3)3N/4 where N = Nx Ny and Nx , Ny are the number of lattice sites in x and y direction. In order to study numerically the ground state of the system for large ratios of V /t it is advantageous to introduce an effective Hamiltonian42 which acts on the different configurations obeying the tetrahedron rule. They form what will be called the allowed subspace 317 A. M. Polyakov, Gauge Fields and Strings, vol. 3 of Contemporary Concepts in Physics, Harwood Academic Publ. (1993), 5th print. 318 P. Fulde, K. Penc, and N. Shannon, Ann. Phys. (Leipzig) 11, 892 (2002). 319 J. Betouras, F. Pollmann, and P. Fulde, to be published (2006). 320 E. Fradkin, Field Theories of Condensed Matter Systems, Addison-Wesley Publ., Redwood City (1991). 321 M. Levin and X.-G. Wen, Phys. Rev. B 73, 035122 (2006).

STRONGLY CORRELATED ELECTRONS

141

F IG . VII.10. Ground-state configuration of a checkerboard lattice with half-filling of spinless fermions. Occupied sites are connected by solid lines and empty sites by dashed lines. Hopping takes place along thin lines with matrix element −t .

of all configurations. An effective Hamiltonian allows for the diagonalization of much larger clusters than does the full H . To leading order in t/V one finds that the energy is lowered for all allowed configurations by an amount of 4t 2

ni . (7.13) E = − V i

Therefore it does not lift the degeneracy and one has to go to the next higher order term. Different allowed configurations are connected through ring hopping processes. The smallest non-vanishing process is 3 − 6t (7.14) + Heff = (+) 2 V where filled dots denote occupied and empty dots empty sites, respectively. The site in between can be empty or occupied. The arrows stand for particle hopping. With tring = this Hamiltonian can be written as Heff = tring

12t 3 V2

(7.15)

cj†6 cj†4 cj†2 cj5 cj3 cj1 .

(7.16) 7 Hopping on larger rings implies higher orders in t/V . The matrix elements of Heff with respect to different allowed configurations |i and |j are j |Heff |i = (−1)n0 tring

(7.17)

142

P. FULDE ET AL.

where n0 is the occupation number of the site inside the ring. It is worth realizing that the sign dependence of j |Heff |i is absent when instead of a checkerboard lattice the pyrochlore lattice is considered. In the latter structure there is no lattice site inside a 6-ring loop. The partial lifting of the degeneracy of the ground-state manifold by Heff can be understood with the help of the height representation. For that purpose one divides the crisscrossed squares of the checkerboard lattice into sublattices A and B and assigns a clockwise and counter-clockwise orientation to them. To each occupied site is attached a unit vector the direction of which is in accordance with the orientation of the corresponding crisscrossed squares. At each empty site the vector is pointing into opposite direction. This defines a vector field f(r) where r is defined with respect to the uncrossed plaquettes. Because of the tetrahedron rule, i.e., two sites are occupied and two are unoccupied on a crisscrossed square, the vector sum over a closed loop vanishes, implying curl f = 0. Therefore f can be written as the gradient of a scalar field h(r), i.e., a potential which is called height field. It allows for the introduction of two topological quantum numbers κx and κy . They quantify the difference in the potential at the upper and lower boundary and at the right and left one. Their values cover the range −Nx /2 κx Nx /2 and −Ny /2 κy Ny /2. In Figure VII.11 an example is given of the change of the height field h(r) defined on the uncrossed squares. On a torus κx and κy are winding numbers. An important point is that the application of Heff does not change the topological quantum numbers of a configuration. Therefore the degenerate ground-state configurations are divided into different classes according to (κx , κy ). The matrix i|Heff |j reduces into block matrices characterized by (κx , κy ). It turns out that Heff does not necessarily connect all configurations within a class. Therefore the matrix (Heff )ij for the class (κx , κy ) may reduce further to irreducible blocks (κx(α) , κy(α) ). This holds true in particular for the class (0, 0) which has the largest

F IG . VII.11. Values of the height field h for a part of a given configuration: solid and empty dots mark occupied and empty sites, respectively.

STRONGLY CORRELATED ELECTRONS

143

number of elements. It is found that for a system of size 8 × 8 with Nf = 32 spinless fermions the ground state has topological quantum numbers (0, 0). The subclass to which it belongs has more than 105 elements. The ground state is twofold degenerate and the two states are related by particle–hole symmetry. Note that Heff has this symmetry while H does not have it. The two states are charge ordered along one of the diagonals and can be transformed into each other by a rotation of 90 degrees. This invalidates a supposition in Ref. [42]. The participation ratio (PR) of a wavefunction is a measure of how extended that function is. With

|ψ = αν |ν (7.18) ν

where |ν denotes different configurations the participation ratio is 1 . 4 ν |αν |

PR[ψ] =

(7.19)

For the ground state |ψ0 of the 8 × 8 system this ratio is very large, i.e., PR[ψ0 ] = 46.9 · 103

(7.20)

indicating that many configurations contribute to it. The largest possible value of PR[ψ0 ] in a Hilbert space of dimension N is PR[ψ0 ] = N . The total density of state is

ρtot (E) = δ(E − El ) (7.21) l

where El are the eigenvalues of H . From it we can compute the specific heat C(T ) according to ∂ dE Eρtot (E)e−βE C(T ) = . (7.22) ∂T dE ρtot (E)e−βE Numerical results for different system sizes are shown in Figure VII.12. One notices an almost linear in T behavior. This suggests that a large quasiparticle mass in geometrically frustrated lattices may possibly be due to charge instead of spin degrees of freedom, the usual source of heavy quasiparticles. The large number of low lying excitations causing the steep linear increase of the specific heat with temperature is here due to a release of entropy (3/4) ln(4/3) ≈ 0.22 per site over a temperature range of kB T 2tring . In the following we want to go beyond the space of allowed configurations which obey the tetrahedron rule. When a particle is hopping to a neighboring empty site (vacuum fluctuation) the tetrahedron rule is broken for two tetrahedra: now one tetrahedron contains three particles, while another contains one only (see

144

P. FULDE ET AL.

F IG . VII.12. Specific heat per particle for a checkerboard lattice of spinless fermions at half filling for various system sizes. Inset: corresponding entropies, the arrow marks the value of 2(3/4) ln(4/3). (After Ref. [42].)

Figure VII.13a). For the corresponding uncrossed squares curl f = 0. By subsequent hopping these two objects can separate carrying a charge of ±e/2 each. As a result of the vacuum fluctuation the vector field f(n) contains a vortex–antivortex pair. An insulator to metal transition may be viewed as a proliferation of such pairs and resembles a Kosterlitz–Thouless transition. It is difficult to compute numerically the ratio V /t at which this transition takes place, but an estimate yields a critical ratio of (V /t)cr 7. This is considerably larger than the value obtained by conventional equations of motion methods in Hubbard I-type approximation.322

F IG . VII.13. (a) Vacuum fluctuation. One criss-crossed square (tetrahedron) contains three particles while another one contains one particle only; (b) particle added to the otherwise half-filled checkerboard lattice; (c) after a hop of one of the electrons the two squares with three particles each have separated. (After Ref. [318].) 322 Y. Z. Zhang, M.-T. Tran, V. Yushankhai, and P. Thalmeier, Eur. Phys. J. 44, 265 (2005).

STRONGLY CORRELATED ELECTRONS

145

When an extra particle is added to the system two neighboring criss-crossed squares contain three occupied sites each (see Figure VII.13b). These two special squares separate from each other when one of the electrons is hopping to a neighboring site (see Figure VII.13c). There is no change in the particle repulsions associated with this separation of the two. Since the charge of the added particle is e, each of the separated squares must have charge e/2. The reason for that is easily seen. When a square with three particles moves in the checkerboard lattice plane, the squares left behind must again satisfy the tetrahedron rule. Inspection shows that this requires the backflow of a charge e/2, thus reducing the charge flow due to hopping of an electron from e to e/2. For the checkerboard lattice it turns out that ring hopping processes cause a (weak) restoring force on the two particles with fractional charge e/2.323 We have not discussed the issue of the spin here but instead have considered spinless or fully polarized fermions. In passing we point out that not only do we have spin-charge separation when the spin is included but also is the spin distributed over parts of the sample. For more details we refer to Ref. [318]. The spectral density is a quantity which is expected to show signatures of fractional charges. For that reason we determine the integrated spectral density

ψ N +1 c† ψ N .2 δ ω − E N +1 + E N . S(ω) = (7.23) 0 kν 0 kν kν kν N +1 |ψkν

are the different excited states characterized by momentum k Here N +1 are the corresponding and band index ν of the N + 1 particle system and Ekν † create particles energies. The energy of the N -particle ground state is E0N . The ckν in quantum states k, ν. For a 32 sites checkerboard cluster with N = 16 spinless fermions and V /t = 25 the integrated spectral density is shown in Figure VII.14a. When one includes only configurations of the N + 1 particle system in which the added particle is not disintegrated like in Figure VII.14a one obtains the spectral density shown in Figure VII.14b. A comparison with Figure VII.14a shows a considerable reduction of the width of the excitation spectrum and an absence of the low frequency part. Therefore we may conclude that hopping processes leading to a separation of the charge e into two parts have an important effect on the spectral density and constitute further evidence for the appearance of fractional charges. The above considerations suggest that in 2D there are also other lattices than the checkerboard one allowing for charge fractionalization. That holds particularly true for the Kagomé lattice which at 1/3 filling can support excitations with charge e/3 and 2e/3 when a spinless fermion is added.323 The requirement hereby is a short-range repulsion V ni nj when i and j are on the same hexagon. 323 F. Pollmann and P. Fulde, Europhys. Lett., in print.

146

P. FULDE ET AL.

F IG . VII.14. Integrated spectral density as function of energy for a 36 sites checkerboard system with 18 particles and V /t = 25. (a) When the excited states are fully accounted for and (b) when only configurations are used in which the added particle remains an entity. (After Ref. [324].)

The fermionic character of the particles discussed here makes the present model different from related spin models and models for hard core bosons. Nevertheless, there exist also similarities between the problem of fractional charges and resonating valence bonds (RVB). For example, Kalmeyer and Laughlin325 have shown that the ground-state wavefunction of an antiferromagnetic Heisenberg Hamiltonian with nearest-neighbor interactions on a triangular lattice is practically the same as the fractional quantum Hall effect (FQHE) wavefunction for bosons. As the ground-state of a Heisenberg Hamiltonian on a frustrated lattice is of the RVB type, the two phenomena, i.e., FQHE effect and RVBs are closely related. RVB systems support spinons, i.e., a spin flip with sz = 1 breaks up into two spinons with spin 1/2 each.326–329 The situation resembles the one in Figure VII.13 in particular when an Ising Hamiltonian us used. Spins up and down on a checkerboard lattice correspond to occupied and unoccupied sites and a state with total z = 0 has a half-filled lattice of hard-core bosons as analogue. While a spin Stot large body of work exists connecting RVB models with confined and deconfined phases of compact gauge theories (see, e.g., Refs. [320,326,330]) corresponding work for fermionic systems is still missing. 324 F. Pollmann, E. Runge, and P. Fulde, Phys. Rev. B 73, 125121 (2006). 325 V. Kalmeyer and R. B. Laughlin, Phys. Rev. B 39, 11879 (1989). 326 R. Moessner and S. L. Sondhi, Phys. Rev. B 63, 224401 (2001). 327 L. Balents, M. P. A. Fisher, and S. M. Girvin, Phys. Rev. B 65, 224412 (2002). 328 O. I. Motrunich and T. Senthil, Phys. Rev. Lett. 89, 277004 (2002). 329 G. Misguish and C. Lhuillier, Frustrated Spin Systems, World Scientific, Singapore (2004). 330 M. Hermele, M. P. A. Fisher, and L. Balents, Phys. Rev. B 69, 064404 (2004).

STRONGLY CORRELATED ELECTRONS

147

F IG . VII.15. String (marked in red) of an odd number of sites (here five) connecting two particles with charge e/2.

Finally we want to comment on some modifications which occur when the spin of the fermions is included. The question may be asked where the spin of an added electron goes when the excitation falls into two parts with charge e/2 each. The answer is found by looking at Figure VII.15 where periodic boundary conditions are used. The two charges e/2 are connected by a spin chain containing an odd number of sites. The ground state of that chain is two-fold degenerate and represents the spin degrees of freedom. Thus one may state that the spin is smeared over parts of the system as is the connected spin chain. This is a rather novel feature which we have not met before in condensed matter physics to the best of our knowledge. It should be also noticed that in the presence of spins the lowest order ring exchange process on a checkerboard lattice involves four sites instead of six. This is different for the pyrochlore lattice where the smallest possible ring involves six sites (see Figure VII.4). So the ground-state degeneracy is lifted in order t 2 /V . VIII. High-Energy Excitations

In Section II we demonstrated that strong electron correlations generate characteristic low energy scales. They are much smaller than the Fermi energy, the typical energy scale in a metal. But it is well known that strong correlations influence high-energy excitations as well. Hereby the expression high energy is used quite flexible. For example, it may include satellite structures or peaks as they are found in the photoelectron spectra of Ni metal331,332 or of the high temperature superconducting cuprates. But it also includes energies which are larger than the one 331 S. Hüfner and G. K. Wertheim, Phys. Lett. A 47, 349 (1974). 332 W. Eberhardt and E. W. Plummer, Phys. Rev. B 21, 3245 (1980).

148

P. FULDE ET AL.

at which Fermi liquid behavior breaks down. In practice this may be a rather low energy or temperature. These effects are best studied by investigating the oneparticle Green’s function. In Dyson’s representation it reads Gν (k, z) =

1 . z − ν (k) − ν (k, z)

(8.1)

The energy ν (k) describes the dispersion of electrons in band ν within an effective single-electron approximation while the self-energy ν (k, ω) contains all effects beyond that approximation. In case that ν (k) describes the Hartree– Fock bands, ν (k, ω) contains the electronic correlations. When Landau’s Fermi liquid theory does apply, the low-energy excitations near the Fermi energy are quasiparticles. They are obtained from G(k, ω) =

Z + Ginc (k, ω). ω − qp (k) − iγk sgn ω

(8.2)

For convenience we have omitted the band index ν. The first term contains the quasiparticle pole at ω = qp (k) + iγk

(8.3)

with the quasiparticle dispersion qp (k) and lifetime γk . The second term is the incoherent part which is of special interest here. Usually it is not further discussed but we want to draw attention to its importance and to significant features when electron correlations are strong. We may think of it as being due to the internal degrees of freedom of the correlation hole which is surrounding an electron. The bare electron has weight Z < 1 in the quasiparticle. The reduction is due to the interaction of the electron (or hole) with the surroundings. The internal degrees of freedom of the modified surroundings, i.e., the correlation hole shows up in the integrated spectral density in form of quasiparticle damping and satellite structures. Those structures have generally a k dependence which is much weaker than the one of the quasiparticles. An example is the shadow band in the Hubbard model when the Hubbard I approximation7 is made. The internal degrees of freedom of the correlation hole are best described by the projection operator method. The idea is to select those particular operators which describe the most important microscopic processes in setting up the correlation hole. Green’s function is determined within that restricted operator space. The Hubbard I approximation to the Hubbard model is the simplest example. Here + only one operator, i.e., ciσ ni−σ where i is the site index is used in order to describe the correlation hole. More interesting cases are discussed in the following subsections.

STRONGLY CORRELATED ELECTRONS

149

We want to draw attention to the zero-point fluctuations of internal excitation modes of the correlation hole. A well known example is Gaskell’s ansatz333 for the ground-state |ψ0 of a homogeneous electron gas. It is of the form

† |ψ0 = exp (8.4) τ (q)ρ ρq SCF q

0

q

where |SCF 0 is the Hartree–Fock ground state and ρq are the density fluctuations of wavenumber q. Furthermore τ (q) ∼ q −2 when q → 0. Here the zero-point fluctuations of plasmons are taken into account which are the internal excitation modes of the correlation hole when the latter is described within the random phase approximation (RPA). It is well known that the RPA models very well the longrange part of the correlation hole but fails to describe properly the short-range part. Zero-point fluctuations of other modes, in particular of those associated with the short-range part of the correlation hole enter in a similar way the (Jastrow) prefactor in Eq. (8.4). We start out by describing the projection operator formalism before we discuss a number of applications. 19. P ROJECTION O PERATORS In the following we shall use the retarded Green function in order to determine the excitations of the system. It is given by † (8.5) GR νσ (k, t) = −i(t) ψ0 cνσ (k, t), cνσ (k) + ψ0 where |ψ0 is the exact ground state and (t) is the step function, i.e., (t) = 1 for t 0 and zero otherwise. The superscript R will be left out in the following discussion for simplicity. We assume that the Fourier transforms of the most important microscopic processes for the generation of the correlation hole are represented by a set of operators {Aμ (k)}, the dynamical variables. But we want to † (k). Explicit examples for proper include in this set also the original operators cνσ choices of the Aμ (k) will be given when specific applications of this method are discussed. Within that reduced operator space 0 spanned by the {Aν (k)} we define the Green function matrix (8.6) Gμν (k, t) = −i(t) ψ0 A†μ (k, t), Aν (k, 0) + ψ0 . Note that the Green function (8.5) is just a diagonal element of that matrix. It is convenient to introduce the following notation (8.7) (A|B)+ = ψ0 A† , B + ψ0 . 333 T. Gaskell, Proc. Phys. Soc. 72, 685 (1958).

150

P. FULDE ET AL.

This enables us to rewrite (8.6) after a Fourier transformation in the condensed form

1 Aν Gμν (k, z) = Aμ (8.8) z−L + where z = ω + iη and η is a positive infinitesimal number. The Liouvillian L corresponds to H and is defined by its action on an arbitrary operator A through LA = i

dA = [H, A]− dt

(8.9)

so that A(t) = eiLt A(0).

(8.10)

By making use of the identity 1 1 1 1 = − b a+b a a a+b we can rewrite (8.8) in the form of the following matrix equation z1 − L + M(z) χ−1 G(z) = χ

(8.11)

with matrix elements χμν = (Aμ |Aν )+ Lμν = (Aμ |LAν )+ ,

1 QLAν . Mμν (z) = Aμ LQ z − QLQ +

(8.12)

The matrix M(z) is called memory function.334,335 It couples the relevant operators {Aν } to the remaining degrees of freedom. The operator Q

Q=1− |Ai )+ χij−1 (Aj | (8.13) ij

projects onto those remaining degrees, i.e., onto an operator space perpendicular to the {Aν }, i.e., Q|Aν )+ = 0. Setting M(z) = 0 implies that the dynamics of the system is approximated by the {Aν } and takes place within 0 . One may either choose a large basis {Aν } and set M(z) = 0 or work with a small basis and keep M(z). Examples are given below. If not stated otherwise we shall set M(z) = 0. The dimension of the matrix Eq. (8.11) equals the number of dynamical variables Aν (k). The energy resolution of the excitation spectrum depends on the size of the set {Aν (k)}. For high-energy excitations a relatively small number of dynamical variables is sufficient. By increasing their number one can increase the energy resolution of the spectral density calculated from Eq. (8.8). 334 H. Mori, Progr. Theor. Phys. 33, 423 (1965). 335 R. Zwanzig, Lectures in Theoretical Physics, Interscience, New York (1961), vol. 3.

STRONGLY CORRELATED ELECTRONS

151

20. T HE H UBBARD M ODEL : A PPEARANCE OF S HADOW BANDS The Hubbard model shows particularly well a number of generic features caused by strong electron correlations. Among them are the appearance of satellite structures, shadow bands and a marginal Fermi liquid like behavior close to half filling. The Hamiltonian is of the well known form

† ciσ cj σ + h.c. + U ni↑ ni↓ H = −t ij

i

= H0 + HI

(8.14)

in standard notation. In the following we discuss solely for pedagogical and illustrative reasons the spin-density wave (SDW) and Hubbard I approximation by applying projection operators. The simplest case in which a shadow band does appear, is a square lattice at half filling when a spin-density wave (SDW) approximation is made. This simple approximation leads to an antiferromagnetic ground state |AF . Charge fluctuations are suppressed here on a mean-field level by symmetry breaking. Breaking a symmetry can reduce intersite charge fluctuations similarly as strong correlations do without symmetry breaking. Therefore features of strong correlations show up already in this simple mean-field scheme. From the kinetic energy term in (8.14) one obtains the dispersion (k) = −2t (cos kx + cos ky ). The lattice constant has been set equal to unity. Therefore, at half filling the Fermi surface is nested and the ground state in mean-field approximation is a spin density wave. One finds † † uk ckσ + σ vk ck+Qσ |0 (8.15) |AF = kσ † † where Q is a reciprocal lattice vector and ckσ is the Fourier transform of ciσ . Furthermore u2k + vk2 = 1 with

(k) (k) 1 1 2 2 1− , vk = 1+ uk = 2 E(k) 2 E(k) 1

m2 U 2 2 E(k) = (k)2 + 0 . (8.16) 4

Here m0 is the staggered magnetization. The latter has to be calculated selfconsistently. In order to calculate the excitations we choose for the relevant dynamical variables {Aν } † A1 (k) = ckσ ,

† A2 (k) = ck+Qσ .

(8.17)

152

P. FULDE ET AL.

When the 2 × 2 matrix (8.11) with M(z) = 0 is evaluated one finds G11 (k, z) =

u2k z − ( U2 − E(k))

+

vk2 z − ( U2 + E(k))

and for the spectral density

U U D(k, ω) = u2k δ ω − + E(k) + vk2 δ ω − − E(k) . 2 2

(8.18)

(8.19)

For each k point there are two contributions to D(k, ω), i.e., one δ-function peak with a large weight and one with a small one. The peaks with the smaller weight form a shadow band Esb (k) = −E(k) which complements the band resulting from the peaks with large weight.336,337 Because of the mean-field level the shadow band disappears for temperatures higher than the Néel temperature. This is in reality not the case and therefore one would like to reproduce a shadow band also for arbitrary filling factors and for the paramagnetic state. This can be done, of course, only by accounting for the strong correlations. They are described in the simplest way by the Hubbard I7 approximation. In that case the following choice is made for the dynamical variables {Aν } 1 ikRi † † , A2 (k) = √ e ciσ δni−σ (8.20) A1 (k) = ckσ N0 i with δni−σ = ni−σ − ni−σ . The Ri denote the positions of the N0 lattice sites. Again, we want to determine G11 (k, ω) from (8.8) by setting M(z) = 0. The 2 × 2 matrix equation can be easily solved and one finds −1

U Uˆ G11 (k, z) = z − (k) − n 1 + (8.21) 2 z − Uˆ where n is the number of electrons per site and Uˆ = U (1 − n/2). G11 (k, ω) has two poles centered at z = 0 and z = U . Neglecting terms of order U −1 we can rewrite (8.21) as G11 (k, z) =

n 1 − n2 2 . n + z − (k)(1 − 2 ) z − U − (k) n2

(8.22)

The poles give raise to two bands, i.e., the upper and the lower Hubbard band. Their widths differ except for n = 1. For n = 0.25 the upper Hubbard band is reduced to a satellite structure with a k-dependent dispersion. This is illustrated in Figure VIII.1 and is well known. The reason for repeating these facts here is 336 A. P. Kampf and J. R. Schrieffer, Phys. Rev. B 42, 7967 (1990). 337 A. P. Kampf, Phys. Rev. 249, 219 (1994).

STRONGLY CORRELATED ELECTRONS

153

F IG . VIII.1. Schematic representation of the two bands resulting from the two variables of Eq. (8.20), i.e., the upper and the lower Hubbard band. The electron number per site is n, the broadening is artificial.

that we want to proceed similarly when we discuss the satellite structure in Ni or the spectral density of electrons in Cu–O planes. We want to emphasize the point of view that the incoherent part of a Green function is the superposition of satellite peaks which have a small k-dependence each. But before, we demonstrate that for special band fillings a Hubbard model can exhibit marginal Fermi liquid behavior. This is shown explicitly for a square lattice. 21. M ARGINAL F ERMI L IQUID B EHAVIOR AND K INK S TRUCTURE The Coherent Potential Approximation (CPA) has been widely used in electronic structure calculations of disordered systems.338–343 Here we want to combine it with the projection operator technique and apply it to the Hubbard model. We remind the reader that a CPA was introduced first by Hubbard when treating his 338 P. Soven, Phys. Rev. 156, 809 (1967). 339 D. W. Taylor, Phys. Rev. 156, 1017 (1967). 340 B. Velický, S. Kirkpatrick, and H. Ehrenreich, Phys. Rev. 175, 747 (1968). 341 F. Yonezawa, Progr. Theor. Phys. 40, 734 (1968). 342 R. J. Elliott, J. A. Krumhansl, and P. L. Leath, Rev. Mod. Phys. 46, 465 (1974). 343 H. Ehrenreich and L. M. Schwartz, in Solid State Physics, vol. 31, Academic Press, New York

(1976).

154

P. FULDE ET AL.

Hamiltonian.20 In the following we want to treat the many-electron problem as accurately as possible for a number of sites which need not be connected. This ˜ cluster is embedded in a medium with a coherent potential (ω). The potential is determined self-consistently so that it agrees with the momentum integrated selfenergy (k, ω) of the cluster. It is known344,345 that the local projection operator method combined with the CPA346 is equivalent to the Many-Body CPA,347 the Dynamical CPA348,349 as well as to the Dynamical Mean Field Theory (DMFT) which is based on many-body physics in infinite dimensions.350,351 For reviews of the latter, see Refs. [186,352]. Here we want to discuss the more general nonlocal version of the projection operator method353 combined with the CPA. It is based on a decomposition of the scattering matrix of the system into one-site, two-site etc. scattering matrices. This way the scattering matrix can be calculated successively in terms of increments, a method successfully applied in the theory of wavefunction based electronic structure calculations of solids. For a review of that method, see Refs. [354,41]. We apply the theory to the Hubbard model on a square lattice near half filling.7,20 The results are interesting. A marginal Fermi liquid behavior is found for large U values and small hole doping and a corresponding phase diagram is worked out.355 It is also found that for similar parameters the excitation spectrum (or real part of the self-energy) has a kink near EF .356 Such a structure was observed in a number of underdoped cuprates like Bi2 Sr2 CaCuO8+δ or La2−δ Srδ CuO4 .357,358 It has been attributed to electron– phonon interactions358–361 and also to the interaction with a magnetic resonance 344 Y. Kakehashi, Adv. Physics 53, 497 (2004). 345 Y. Kakehashi, Phys. Rev. B 66, 104428 (2002). 346 Y. Kakehashi and P. Fulde, Phys. Rev. B 69, 045101 (2004). 347 S. Hirooka and M. Shimizu, J. Phys. Soc. Jpn. 43, 70 (1977). 348 Y. Kakehashi, J. Magn. Magn. Mater. 104–107, 677 (1992). 349 Y. Kakehashi, Phys. Rev. B 45, 7196 (1992). 350 W. Metzner and D. Vollhardt, Phys. Rev. Lett. 62, 324 (1989). 351 E. Müller-Hartmann, Z. Phys. B: Cond. Matt. 74, 507 (1989). 352 T. Pruschke, M. Jarrell, and J. Freericks, Adv. Phys. 44, 187 (1995). 353 Y. Kakehashi and P. Fulde, Phys. Rev. B 70, 195102 (2004). 354 H. Stoll, B. Paulus, and P. Fulde, J. Chem. Phys. 123, 144108 (2005). 355 Y. Kakehashi and P. Fulde, Phys. Rev. Lett. 94, 156401 (2005). 356 Y. Kakehashi and P. Fulde, J. Phys. Soc. Jpn. 74, 2153 (2005). 357 P. V. Bogdanov, A. Lanzara, S. A. Keller, X. J. Zhou, E. D. Lu, W. J. Zheng, G. Gu, J.-I. Simoyama,

K. Kishio, H. Ikeda, et al., Phys. Rev. Lett. 85, 2581 (2000). 358 T. Chuk, D. H. Lu, X. J. Zhou, Z.-X. Shen, T. P. Devereaux, and N. Nagaosa, Phys. Stat. Sol. (b) 242, 11 (2005). 359 Z.-X. Shen, A. Lanzara, S. Ishihara, and N. Nagaosa, Philos. Mag. B 82, 1349 (2002). 360 S. Verga, A. Knigavko, and F. Marsiglio, Phys. Rev. B 67, 054503 (2003). 361 S. Ishihara and N. Nagaosa, Phys. Rev. B 69, 144520 (2004).

STRONGLY CORRELATED ELECTRONS

155

mode observed by inelastic neutron scattering.362–365 But as it turns out, also strong electron correlations in a 2D Hubbard model can produce it. To reach our goal we start out by choosing for the {Aν } simply the operators † but we keep this time the memory matrix, i.e., M(z) = 0. In that case we write ciσ for a paramagnetic system G(k, z) =

1 . z − (k) − U 2 M(k, ω)

(8.23)

The matrix L in (8.11) gives only a constant energy shift and is neglected here. For convenience a factor U 2 has been extracted from M(k, z). We decompose

M(k, z) = Mj0 (z)eikRj (8.24) j

and write for the reduced memory matrix according to (8.12)

1 † † Mij (z) = ciσ δni−σ c δnj −σ , z − L¯ j σ +

(8.25)

† † where L¯ = QLQ with the projector Q = 1 − iσ |ciσ )+ (ciσ |. Stopping at this stage, i.e., neglecting the new memory function in the denominator of (8.25) would bring us back to the Hubbard I approximation. In order to establish a connection to the CPA we define the Hamiltonian of an effective medium through

˜ H˜ (z) = H0 + (z) ni (8.26) i

˜ i.e., LB ˜ = [H˜ (z), B]− for arbitrary operawith the corresponding Liouvillian L, tors B. The aim is to account efficiently for local as well as nonlocal correlations ˜ by means of an effective medium characterized by (z). ˜ The coherent potential (z) is determined self-consistently from ˜ (z) =

U2

M(k, z) N

(8.27)

k

362 M. Eschrig and M. R. Norman, Phys. Rev. Lett. 85, 3261 (2000). 363 P. D. Johnson, T. Valla, A. V. Fedorov, Z. Yusof, B. O. Wells, Q. Li, A. R. Moodenbaugh, G. D.

Gu, N. Koshizuka, C. Kendziora, et al., Phys. Rev. Lett. 87, 177007 (2001). 364 M. Eschrig and M. R. Norman, Phys. Rev. B 67, 144503 (2003). 365 E. Schachinger, J. J. Tu, and J. P. Carbotte, Phys. Rev. B 67, 214508 (2003).

156

P. FULDE ET AL.

where N is the number of sites. With this in mind we decompose

˜ + ˜ Q U δni↑ δni↓ − (z)n L¯ = QLQ i Q i

= L0 (z) +

(i)

LI (z)

i

= L0 (z) + LI (z).

(8.28)

¯ −1 in terms of a scattering (super)operator T as Next we express (z − L) 1 1 1 1 + T = z − L0 z − L0 z − L0 z − L¯ = g0 (z) + g0 (z)T g0 (z)

(8.29)

with T = LI + L I g 0 L I + · · · . The T -operator can be decomposed into a sequence of many-sites increments

T= Ti + δTij + δTij k + · · · . (8.30) i

ij

ij k

Those increments are closely related to the T operators Ti , Tij , Tij k , . . . of single-site, 2-sites, 3-sites, etc. clusters. It is δTij = Tij − Ti − Tj δTij k = Tij k − δTij − δTik − δTj k − Ti − Tj − Tk .. .

(8.31)

This enables us to introduce retarded memory functions for clusters

1 (c) † † Mij (z) = ciσ δni−σ c δnj −σ . z − L¯ (c) j σ +

(8.32)

These matrices have dimensions 1 × 1 when c = i (one-site cluster) and 2 × 2 when c = (i, j ), i.e., in the 2-site cluster approximation. The Liouvillian L¯ (c) (z) is given by L¯ (c) = L0 (z) +

Nc

(n)

LI (z).

(8.33)

n∈c

The sum over n involves all Nc sites belonging to a given cluster c. Within (n) zeroth-order renormalized perturbation theory (RPT-0) only that part of LI (z)

STRONGLY CORRELATED ELECTRONS

157

(n) † is used which projects onto the operators ciσ δni−σ , i.e., P¯ LI (z)P¯ with the projector.

† c δni−σ χ −1 c† δni−σ (8.34) P¯ = iσ iσ + i iσ

and χi = ni−σ (1 − ni−σ ). With this simplification the memory matrix can be expressed in terms of a “screened” one as −1 Mij(c) (z) = g · 1 − L(c) . (8.35) I g ij The screened memory matrix is given by

1 † gij (z) = ciσ cj†σ δnj −σ . δni−σ z − L0 (z) +

(8.36)

(c)

The cluster memory matrix Mij (z) describes a Hubbard cluster embedded in a uniform medium with a Hamiltonian H˜ (z) (see the left side in Figure VIII.2). The ˜ interactions in the embedded cluster are given by ic (U δni↑ δni↓ − (z)n i ). We start from a uniform medium described by H˜ (z) (see Eq. (8.28) and the right side of Figure VIII.2). An alternative would have been to start from the same medium but with cavities at the sites of the cluster (see the middle of Figure VIII.2), i.e., from a Hamiltonian H˜ (c) with ˜ H˜ (c) = H˜ (z) − (z)

Nc

ni .

(8.37)

n∈c

In this case the interaction in the cluster would be n∈c U δni↑ δni↓ . (c) The diagonal matrix LI in (8.35) describes the atomic excitations. The ma(j ) (i) (i) trix elements are given by [LI , LI , . . .]. It has one element LI = U (1 − (j ) 2ni−σ )/[ni−σ (1 − ni−σ )] when c = i and a second one LI when c = (i, j ). The incremental cluster expansion is depicted in Figure VIII.3. With the above approximations the theory reproduces two limiting cases exactly, i.e., the limit of

F IG . VIII.2. Left side: Cluster with on-site Coulomb repulsion U embedded in a medium. Middle: ˜ Cavities replacing the sites of the cluster. Right side: Uniform medium with self-energy (ω). (After Ref. [353].)

158

P. FULDE ET AL.

F IG . VIII.3. Schematic drawing of the multisite cluster expansion of Green’s function. From left to right: single-site, two-sites and three-sites contributions. Note that the sites of a cluster need not be nearest neighbors.

small U when perturbation theory is applicable as well as the atomic limit. This is an important feature of the present theory. In the limit of large clusters the memory functions are independent of the medium. But since the cluster expansion must be truncated in practical applications there is a dependence of the memory functions on the medium and we must make an optimal choice for it. When correlation effects on the static matrix elements are neglected one can write down an explicit expression for the screened memory function of the form gij(c) (z) = Aij

d d d ρ (c) ()ρ (c) ( )ρ (c) ( )χ(, , ) ij ij ji z − − +

(8.38)

with Aii = [ni−σ (1 − ni−σ )]/[ni−σ c (1 − ni−σ c )] and Ai=j = 1. Here (c) ρij () is the density of states of a system with one or two empty sites (depending ˜ on the cluster c) embedded in a medium with a coherent potential (z). More specifically ρij(c) (z) = −

−1 1 Im z − H˜ (c) . ij π

Furthermore

niσ c =

(8.39)

(c)

d ρii ()f ()

where f () is the Fermi function. Moreover χ(, , ) = f (−)f (− )f (− ) + f ()f ( )f (− ). These approximations are used in order so solve Eq. (8.27) self-consistently whereby M(k, z) is replaced by Eq. (8.35). We reemphasize that in the two-site cluster approximation for fixed site i, all sites j are taken into account until convergence is achieved. For the Hubbard model on a square lattice this includes sites which are more than ten lattice vectors apart! In this respect the present theory resembles incremental schemes which

STRONGLY CORRELATED ELECTRONS

159

have been applied in the treatment of solids by quantum chemistry methods.366 For a review see Ref. [41]. The self-consistent projection method (SCPM) provides an interesting link between treatments of model Hamiltonians in solid state theory and true ab initio calculations with controlled approximations based on methods used in quantum chemistry. Our theory differs from extensions of the DMFT such as the Dynamical Cluster Approximations367 or the Cellular Dynamical Mean-Field Theory368 where clusters of connected sites are treated. They require a truly impressive amount of numerical work and have been carefully reviewed in Ref. [369]. Determining M(k, ω) might look like a very demanding computational problem too, but that is not really the case. In fact, we can calculate M(k, ω) directly without a numerical analytic continuation from the imaginary axis as is the case in other schemes.369 Therefore a high numerical resolution as regards energy and momentum can be obtained. The following results are obtained for U = 8|t| and T = 0 in the underdoped regime, i.e., for n 1. At half-filling, the system will always be an antiferromagnetic insulator due to nesting. But in the effective medium approach described here one finds in addition also a paramagnetic metallic solution. We use the latter here, being aware of the fact that an arbitrarily small temperature or doping concentration will destroy antiferromagnetic order in two dimensions (Mermin– Wagner theorem). A metallic solution does exist only for U < Ucrit where in single-site approximation Ucrit 14|t| is obtained. Therefore with a value of U = 8|t| we are still in the metallic regime. We find that a flat quasiparticle band is crossing the Fermi energy EF . There is also an empty upper Hubbard band found which is centered around the M point and there is incoherent spectral density near the point resulting from the lower Hubbard band. The results compare well with those of Quantum Monte Carlo (QMC) calculations for finite temperatures.370–372 This is seen in Figure VIII.4. The Fermi surface for n = 0.95 (underdoped regime) is found to be hole like. This is due to a collapse of the lower Hubbard band which causes a portion of the flat quasiparticle band near the X point to sink below EF . These findings are contrary to expectations from the Hubbard I approximation. From (8.22) it is seen that within that approximation the spectral weight of the lower Hubbard band increases while that of the upper Hubbard band decreases in case of hole doping n < 1. In the present, improved approximation this is not the 366 H. Stoll, Phys. Rev. B 46, 6700 (1992). 367 M. H. Hettler, M. Mukherjee, M. Jarrell, and H. R. Krishnamurthy, Phys. Rev. B 61, 12739 (2000). 368 G. Kotliar, S. Savrasov, G. Pallson, and G. Biroli, Phys. Rev. Lett. 87, 186401 (2001). 369 T. Maier, M. Jarrell, T. Pruschke, and M. H. Hettler, Rev. Mod. Phys. 77, 1027 (2005). 370 N. Bulut, D. J. Scalapino, and S. R. White, Phys. Rev. Lett., Phys. Rev. 73, 50, 748, 7215 (1994). 371 R. Preuss, W. Hanke, and W. von der Linden, Phys. Rev. Lett. 75, 1344 (1994). 372 C. Gröber, R. Eder, and W. Hanke, Phys. Rev. B 66, 4336 (2000).

160

P. FULDE ET AL.

F IG . VIII.4. Single-particle excitations at zero temperatures for the Hubbard model on a square lattice in units of the nearest-neighbor transfer integral t . Dashed line: Hartree–Fock result. Open circles with error bars: QMC results for T = 0.33.372 (After Ref. [355].)

case for small hole doping and implies that Luttinger’s Theorem30 does not apply here. It would require a reduction of the volume enclosed by the Fermi surface with increasing hole concentration. For n = 0.8 (overdoped regime) an electronlike Fermi surface is found. These results are in agreement with the Dynamical Cluster Approximation373 and with QMC calculations.370–372 An important finding is that for doping less than 2% the effective mass mk changes strongly between the M point, i.e., [π, π] where it is minimal and the X point, i.e., [π, 0] where it has its maximum. It is computed numerically from mk = 1 − U 2 Re ∂M(k, ω)/∂ω|ω=0+ . Near the X point one finds that the smaller the δω steps are in computing the derivative, the larger becomes mk=X . One finds that approximately mk ∼ ln δω, indicating marginal Fermi liquid behavior. The marginal Fermi liquid theory46,47,374,375 had been designed in order to explain a number of features, observed in the normal state of the high-Tc cuprates where electron correlations are strong. They deviate from normal Fermi liquid behavior. Most noticeable is a linear temperature dependence of the resistivity ρ(T ) ∼ T which has been observed, e.g., in doped La2 CuO4 materials. It is suggestive to associate this dependence with a quasiparticle scattering rate 1/τ (T ) ∼ ρ(T ), i.e., τ −1 ∼ Im (T ) ∼ T . Then it is plausible to assume that for T < |ω| the corresponding expression is Im (ω) ∼ |ω|. Indeed, optical reflectivity measurements 373 T. A. Maier, T. Pruschke, and M. Jarrell, Phys. Rev. B 66, 075102 (2002). 374 C. M. Varma, P. B. Littlewood, S. Schmitt-Rink, E. Abrahams, and A. Ruckenstein, Phys. Rev.

Lett. 64, 497 (1990). 375 G. T. Zimanyi and K. S. Bedell, Phys. Rev. B 48, 6575 (1993).

STRONGLY CORRELATED ELECTRONS

161

F IG . VIII.5. Phase diagram for the Hubbard model on a square lattice as function of hole doping δn. In the upper shaded region two self-consistent solutions are found one of which corresponds to a marginal and the other to a normal Fermi liquid. In the lower shaded region two slightly different marginal Fermi liquid solutions are found. (After Ref. [355].)

on YBa2 Cu3 O4 are in accordance with this form.376 But also the frequencydependent spin susceptibility at low T shows marginal Fermi liquid behavior. Real and imaginary part of (k, ω) are related to each other via a Kramers– Kroning relation from which is follows that Re (ω) ∼ ω ln(ω/ω0 ) where ω0 is a cut-off parameter. From this form of Re (ω) we conclude that the residuum of the Green’s function pole (see Eq. (8.2)) is Z(ω) ∼ 1/| ln(ω/ω0 )| and that the quasiparticle mass mk diverges at the Fermi energy like mk ∼ | ln(ω/ω0 )|. The above treatment shows that a marginal Fermi liquid type of behavior can be obtained from a Hubbard Hamiltonian on a square lattice, provided one is in a certain U dependent doping regime. We expect that this region will be enlarged when long-range antiferromagnetic correlations are taken into account which have been neglected here. The phase diagram in the U vs. δn plane is shown in Figure VIII.5, where δn denotes hole doping. There are two small regions in which two self-consistent solutions are found. They separate the marginal Fermi liquid regime from the normal Fermi liquid one. For smaller U values the cross-over between the two regimes is continuous. It is instructive to consider the origin of the marginal Fermi-liquid like behavior of the self-energy. For half-filling a van Hove singularity shows up in the density of states at EF which leads, as is well known, to a self-energy of marginal Fermi liquid type. With hole doping this singularity moves rather fast away from EF pro376 R. T. Collins, Z. Schlesinger, F. Holtzberg, P. Chaudhari, and C. Feild, Phys. Rev. B 39, 6571

(1989).

162

P. FULDE ET AL.

F IG . VIII.6. Schematic drawing of the dispersion ω(k) near kF in the presence of a kink.

vided correlation effects are small.377–379 But when U is large as assumed here, and for small hole doping spectral density moves to high energies and therefore EF remains virtually pinned to the van Hove singularity. This changes at higher doping concentrations where EF moves to lower energies and normal Fermi liquid behavior is recovered. It is interesting that for small hole doping the calculations for U = 8|t| show a kink in the excitation spectrum at approximately ωkink = −0.8|t|. A kink has been observed in high-resolution photoemission experiments in the quasiparticle band dispersion of high-Tc cuprates.357,358 It was found that along the nodal direction (0, 0) − (π, π) the effective Fermi velocity vF as defined by the form ω(k) = vF (k)(|k| − kF ) is neither sensitive to the type of cuprate, nor to doping concentration or isotope substitution380 as long as ω < ωkink (= 60–70 meV). But when ω > ωkink a strong dependence of vF on those quantities as well as on k is observed. The form of the dispersion is schematically shown in Figure VIII.6. There have been two possible explanations advanced for this experimental observation. One is based on a coupling of electrons to the longitudinal optical phonon mode found in inelastic neutron scattering experiments.358 The other is based on a coupling of the electronic quasiparticles to spin fluctuations, in particu377 A. Virosztek and J. Ruvalds, Phys. Rev. B 42, 4064 (1990). 378 H. Schweitzer and G. Czycholl, Z. Phys. B 83, 93 (1991). 379 G. Kastrinakis, Physica C 340, 119 (2000). 380 G.-H. Gweon, T. Sasagawa, S. Y. Zhou, J. Graf, H. Takagi, D.-H. Lee, and A. Lanzara, Nature

430, 187 (2004).

STRONGLY CORRELATED ELECTRONS

163

F IG . VIII.7. Hubbard model on a square lattice near half-filling. Contours of spectral function of excitations along M– for hole doping δn = 0.01 showing a kink. (After Ref. [356].)

lar to an observed resonance mode.362,363,381 No consensus has been reached yet. So it is interesting to note that a kink is also obtained from the Hubbard model on a square lattice for small doping concentrations. Here it is based on long-ranged electron correlations. In Figure VIII.7 we show the excitation spectrum near EF for a small hole concentration of δn = 0.01 and U = 8|t| as before356 (compare with Figure VIII.4). As before, the calculations assume a paramagnetic ground state. The kink structure becomes weaker as the doping concentration increases while the kink position changes little with δn. For δn = 0.05 the kink has disappeared together with the remnants of the lower Hubbard band. The ratio of the Fermi velocities vF /vF above and below ωkink is found to be vF /vF = 1.8 for δn = 0.01 and 1.5 for δn = 0.02. The kink is caused by a hybridization of the quasiparticle excitation with short-range antiferromagnetic fluctuations. With decreasing antiferromagnetic correlations, e.g., by hole doping the kink structure does also decrease and eventually disappears. Whether or not it provides an explanation for the observed kink in the underdoped regime of La2−x Srx CuO4 remains an open question. 22. N ICKEL AND ITS S ATELLITE Photoelectron spectroscopy has revealed a pronounced satellite structure in Ni metal which is approximately 6 eV below the Fermi energy EF .331 It is due to 381 A. V. Chubukov and M. R. Norman, Phys. Rev. B 70, 174505 (2004).

164

P. FULDE ET AL.

strong electron correlations and a number of different theoretical model calculations have been performed to explain it. The simplest way of including correlations is by calculating the self-energy in second-order perturbation theory.382,383 This results in a d-band narrowing effect as well as in a satellite structure. However, for a quantitative comparison with experiments this is not sufficient. Another well known method is the t-matrix approach of Kanamori.21 It accounts for multiple scattering of two d-holes, but it is strictly valid only in the cases of small or almost complete band filling. It has been used to explain the satellite structure384,385 and was subsequently extended to include also multiple electronhole scattering.386–388 These calculations establish also a link to calculations based on couplings of a hole to magnons.389–392 There have been also numerical diagonalizations based on a 4-sites tetrahedral cluster with five d-orbitals per site.393 A correctly positioned multiplet structure was obtained for ferromagnetic Ni but more detailed information is beyond the scheme of that approach. Other calculations were based on a LDA+DMFT approach394 and on a Gutzwiller projected wavefunction.395 In the latter case band narrowing but no satellite structure was obtained. Here we want to start from a five-band Hubbard model and to calculate the spectral density for paramagnetic Ni with the help of the projection operator method.396 It gives good insight into the relevant microscopic processes which contribute to the satellite and are described by the set of operators {Aν } (see Eq. (8.6)). The results are found to be similar to those obtained when the twohole one-electron t matrix is solved by employing Faddeev’s equations.397

382 G. Treglia, F. Ducastelle, and D. Spanjaard, J. Phys. (Paris) 41, 281 (1980). 383 G. Treglia, F. Ducastelle, and D. Spanjaard, J. Phys. (Paris) 43, 341 (1982). 384 D. R. Penn, Phys. Rev. Lett. 42, 921 (1979). 385 A. Liebsch, Phys. Rev. Lett. 43, 1431 (1979). 386 A. Liebsch, Phys. Rev. B 23, 5203 (1981). 387 J. Igarashi, J. Phys. Soc. Jpn. 52, 2827 (1983). 388 J. Igarashi, J. Phys. Soc. Jpn. 54, 260 (1985). 389 L. Roth, Phys. Rev. B 186, 428 (1969). 390 J. A. Hertz and D. M. Edwards, J. Phys. C 3, 2174 (1973). 391 J. A. Hertz and D. M. Edwards, J. Phys. C 3, 2191 (1973). 392 H. Matsumoto, L. Umezawa, S. Seki, and M. Tachiki, Phys. Rev. B 17, 2276 (1978). 393 R. H. Victora and L. M. Falicov, Phys. Rev. Lett. 55, 1140 (1985). 394 A. I. Lichtenstein, M. I. Katsnelson, and G. Kotliar, Phys. Rev. Lett. 87, 067205 (2001). 395 J. Bünemann, F. Gebhard, T. Ohm, R. Umstätter, S. Weiser, W. Weber, R. Claessen, D. Ehm, A. Harasawa, A. Kakizaki, et al., Europhys. Lett. 61, 667 (2003). 396 P. Unger, J. Igarashi, and P. Fulde, Phys. Rev. B 50, 10485 (1994). 397 J. Igarashi, P. Unger, K. Hirai, and P. Fulde, Phys. Rev. B 49, 16181 (1994).

STRONGLY CORRELATED ELECTRONS

165

We write the five-band Hubbard Hamiltonian for the d electrons of Ni in the following form

H1 (l) H = H0 + H0 =

l

ν (k)nνσ (k)

kνσ

H1 (l) =

1

† † Vij mn aiσ (l)amσ (l)anσ (l)aj σ (l). 2

(8.40)

ij mn σ σ

Here l is a site index and i, j, m, n denote different d orbitals. The ν (k) with ν = 1, . . . , 5 are the energy dispersions of canonical d-bands obtained by solving a one-particle equation. We use for them the LDA bands being aware of the † ckνσ fact that they contain already some correlation effects. The nνσ (k) = ckνσ are number operators for Bloch states with quantum numbers k, ν and σ . Their † (l) through creation operators are expressed in terms of the basis operators aiσ 1

† † ckνσ =√ ανn (k)eikRl anσ (l) (8.41) N0 ln where N0 is the number of sites. The interaction matrix elements in (8.40) are of the form Vij mn = Uim δij δmn + Jij (δin δj m + δim δj n ) Uim = U + 2J − 2Jim

(8.42)

where U and J are average values of the Coulomb- and exchange interaction, respectively. The matrix Jij can be expressed in terms of J and a single anisotropic parameter J provided we deal with a cubic lattice as is the case here. For more details we refer, e.g., to Refs. [398,399]. When electronic correlations are neglected the ground state is of the form † ckνσ |0. (8.43) |0 = |k| 0 n n jz 0 n0 Ajz (k, ω) = (8.47) (N −1) cj (k) (N ) 2 δ ω + ω(−) , ω < 0 z n n 0 n0 with cjz (k) =

a

eika cjz (a),

(±) ωn0 = En(N ±1) − E0(N ) .

(8.48)

STRONGLY CORRELATED ELECTRONS

169

F IG . VIII.10. Configurational energies vs. 5f -valence for the microscopic model adopted to describe the U sites. For a qualitative discussion, the value U0 is treated as a parameter since it is screened in a metal and concomitantly will depend upon the crystallographic environment of the U site.

It yields the probability for adding (ω > 0) or removing (ω < 0) a 5f electron with energy ω in a state characterized by momentum k and angular momentum (N ) (N ) projection jz to the N -particle ground state |0 with energy E0 . The states (N ±1) (N ±1) and En , respectively. with N ± 1 and their energies are denoted by |n The notation was introduced in Section V. The structure of the spectra in the strong-coupling limit can be understood by considering the atomic limit where the system is modeled as a statistical ensemble of isolated 5f atoms. The absence of pronounced valence peaks in the photoemission and inverse photoemission spectra suggests that the energies of the f 2 - and f 3 -configurations, are (almost) degenerate i.e., E(5f 2 ) = E(5f 3 ). The variation with 5f -valence of the configurational energies E(f n ) is shown schematically in Figure VIII.10. The ground state will mainly involve 5f 2 and 5f 3 configurations. The corresponding spectral functions are obtained in close analogy to the classical work of Hubbard.7 Let us first consider the zero configuration-width approximation which neglects intra-atomic correlations. The valence transitions f 2 → f 1 and f 3 → f 4 occur at high energies set by the isotropic average of the Coulomb interaction and, concomitantly, do not affect the low-temperature behavior. The latter is determined by the low-energy peak resulting from the transitions f 2 ↔ f 3 within the f 2 - and f 3 -configurations. This peak is a direct consequence of the intermediate-valent ground state. The distribution among the peaks can be estimated from combinatorial considerations. The weight Z(f 2 → f 1 ) of the transition f 2 → f 1 equals the probability that a state with a given jz is occupied in that

170

P. FULDE ET AL.

F IG . VIII.11. Left panel: Multiplets for f 2 and f 3 configurations of the U model in the atomic limit. The levels are obtained by diagonalizing the Coulomb matrix using j -j coupling and Coulomb parameters of UPt3 . Right panel: Spectral function for the model in the atomic limit.

f 2 contribution of the mixed-valent ground-state. Following these lines one finds 1 Z f2 →f1 = , 6 3 1 Z f →f2 = , 4

1 Z f2 →f3 = 3 3 1 Z f →f4 = 4

(8.49)

The central focus is the evolution of the low-energy peak whose spectral weight sums up to 7/12 (= 1/3 + 1/4). Intra-atomic correlations which are usually described by Hund’s rules yield the multiplets displayed schematically in Figure VIII.11. The values for the excitation energies are calculated from the Coulomb parameters of UPt3 adopting j -j -coupling. In the atomic limit the model spectral function has a low-energy peak resulting from transitions between the Hund’s rule ground-state manifolds |f 2 , J = 4, Jz and |f 3 , J = 9/2, Jz as well as peaks corresponding to transitions into excited multiplets. Due to the rotational invariance of the Coulomb interaction, the spectral functions do not despectral weights for the phopend upon the magnetic quantum number jz . The 1 2 3 toemission and inverse photoemission parts, 10 Jz |f , J , Jz − jz |cjz |f , J = † 9/2, Jz |2 and 19 Jz |f 3 , J , Jz + jz |cjz |f 2 , J = 4, Jz |2 are easily obtained by expressing the matrix elements in terms of reduced matrix elements and Clebsch– Gordan coefficients. The excitation energies as well as the corresponding spectral weights are listed in Table VIII.1. We should like to mention that there is no transition into the excited multiplet |f 2 , J = 0. The model therefore predicts 5f spectral weight at 1 eV binding energy in the photoemission spectra from U-based heavy fermion compounds. The position of these 5f structures should not depend sensitively on the actual crystalline environment since they result from intra-atomic excitations. The weights, however,

STRONGLY CORRELATED ELECTRONS

171

TABLE VIII.1. P OSITIONS AND S PECTRAL W EIGHTS OF THE ATOMIC T RANSITIONS IN U RA AT Z ERO E NERGY P OSITION THE PARTICLE AND H OLE P EAKS H AVE A T OTAL W EIGHT 0.414

NIUM .

PES Position/[eV] Spectral weight

−1.06 0.054

BIS 0.00 0.196

0.00 0.218

1.60 0.032

2.73 0.083

will be altered by the reconstruction of the ground state and the low-energy excitations in an extended solid and may vary with chemical composition and temperature. These predictions seem to be in agreement with recent experiments.403 Recent photoemission studies by Fujimori et al.404 seem to indicate the presence of features in the proper energy range. The fact that they cannot be attributed to LDA energy bands further supports our interpretation in terms of multiplet side bands. An unambiguous identification, however, will require resonant photoemission experiments. 24. E XCITATIONS IN C OPPER -OXIDE P LANES It is well known that the copper-oxide based perovskites which play a major role in high-temperature superconductivity are strongly correlated electron systems. This is immediately obvious by realizing that, e.g., La2 CuO4 is an insulator and not a metal despite the fact that with one hole per unit cell one would expect a half-filled conduction band. Note that insulating behavior is found also above the antiferromagnetic transition temperature and therefore is unrelated to the doubling of the unit cell when the material becomes an antiferromagnet. Indeed, LDA calculations give an effective Coulomb repulsion of two d holes on a Cu site of Ud = 10.5 eV and a hopping matrix element of a hole from a Cu 3dx 2 −y 2 orbital to an O 2px(y) orbital of tpd = 1.3 eV. Therefore the bandwidth is small as compared with Ud . The strong correlations lead to a single-particle spectral density which is quite distinct from the one of weakly correlated electrons. In fact, the excitations are dominated by the internal degrees of freedom of the correlation hole so that the one-particle or coherent part of Green’s function plays a secondary role here. This will become clear towards the end of this section. We shall use again a model Hamiltonian although an ab initio calculation would be highly desirable. We want to write it in hole representation in the form of a 403 R. Eloirdi, T. Gouder, F. Wastin, J. Rebizant, and F. Huber, preprint (2005). 404 S. Fujimori, private communication (2005).

172

P. FULDE ET AL.

F IG . VIII.12. Cu and O orbitals accounted for in the 3-band Hubbard Hamiltonian (8.53).

three-band Hubbard or Emery model. The unit cell consists of one Cu 3dx 2 −y 2 orbital and two O 2px(y) orbitals (see Figure VIII.12). The orbital energies are d and p . Two holes on a Cu site repel each other with Ud and on a O site with Up . The hopping matrix element between a Cu orbital and an O orbital is tpd and tpp between the orbitals of the two O atoms. The parameter values can be derived from a constrained LDA calculation405 with the following results: Ud = 10.5 eV, Up = 4.0 eV, tpd = 1.3 eV, tpp = 0.65 eV, p − d = 3.6 eV. It is helpful to first introduce a basis of oxygen orbitals which is diagonal with respect to oxygen– oxygen hopping processes tpp . Let us denote the corresponding creation operators † by cmkσ where m is an oxygen band index. Those bands have a dispersion (m = 1, 2) (8.50) m (k) = p ± 2tpp cos k(r1 + r2 ) − cos k(r2 − r1 ) where the vectors r1 and r2 are shown in Figure VIII.12. Due to the different orientations of the O 2px(y) orbitals, the sign of tpp depends on the direction. It is positive in the direction r1 + r2 , −(r1 + r2 ) and negative in the direction r1 − r2 , r2 − r1 . Next we introduce a linear combination of oxygen orbitals which possesses the same symmetry on a CuO4 plaquette as the tpd -matrix elements, i.e.,

† † = φmk cmkσ , (8.51) pkσ m

with i φmk = − √ [sin kr1 ± sin kr2 ]. 2 405 M. S. Hybertsen, M. Schlüter, and N. E. Christensen, Phys. Rev. B 39, 9028 (1989).

(8.52)

STRONGLY CORRELATED ELECTRONS

173

The model Hamiltonian we shall be using can thus be written as

† m (k)cmkσ cmkσ + Up np↑ (J )np↓ (J ) H= mkσ

+ d

† dkσ dkσ + Ud

kσ

+ 2tpd

J

nd↑ (I )nd↓ (I )

I

† pkσ dkσ + h.c. .

(8.53)

kσ

As usual npσ (J ) and ndσ (I ) are the occupation number operator of the O 2px(y) orbital on site J and of the Cu 3dx 2 −y 2 orbital on site I , respectively. With the help of the above Hamiltonian we calculate the spectral density of the Cu–O planes, with and without hole doping. For that purpose we have to choose the right set of relevant operators {An (k)}. They must include the most important microscopic processes in the strongly correlated system which generate the correlation hole of an electron. First of all, the hole operators † , Ap (m, k) = pmk

† Ad (k) = dk↑ ,

m = 1, 2

(8.54)

must be part of the set. They are supplemented by a number of local operators. In order to suppress double occupancies of the d and p orbitals due to the large values of Ud and Up , we must include d¯↑† = d↑† (I )nd↓ (I ) and p¯ ↑† = pJ† ↑ np↓ (J ), i.e., their Fourier transforms 1 −ikRI ¯ † e dI ↑ Ad (k) = √ N J Ap (k) = √

1 2N

e−ikRJ p¯ J† ↑

(8.55)

J

where N is the number of Cu sites and there are two O sites per Cu site. In addition we want to account for spin flips of d holes at Cu sites in combination with spin flips at neighboring O sites. Those processes are important for the formation of a Zhang–Rice singlet.406 This is a singlet state formed by a hole at a Cu site and another one at a nearest-neighbor O site. The corresponding microscopic operator is 1 −ikRI † + e p˜ I ↑ SI Af (k) = √ N I 406 F. C. Zhang and T. M. Rice, Phys. Rev. B 37, 3759 (1988).

(8.56)

174

P. FULDE ET AL.

where 1 † † † † p1σ + p2σ (8.57) − p3σ − p4σ 2 is a superposition of the four O 2p orbitals which surround the 3d orbital of Cu site I . The operator SI+ = dI+↑ dI ↓ . For a possible formation of triplet states also the operator 1 −ikRI † Aa (k) = √ e p˜ I ↑ nd↓ (I ) (8.58) N I p˜ I†σ =

is needed. In order to describe charge transfer in the vicinity of an added hole we also include 1 −ikRI † † Ac (k) = √ e pI ↑ pI ↓ d I ↓ . (8.59) N I This completes the choice of the set {Aν (k)}. With 9 operators Aν (k) we have to diagonalize for each k point (9 × 9) matrices Lμν and χμν (see (8.12)). The static expectation values which enter the matrix elements are determined from the spectral functions to which they are related via +∞ † ψ0 Am (k)An (k) ψ0 = dω f (ω)Amn (k, ω) (8.60) −∞

with β = (kB T )−1 is the Fermi distribution function. where It can be replaced by a step function. By solving Eq. (8.60) self-consistently the static correlation functions are obtained. For more details we refer to the original literature.407,408 The resulting density of states are shown in Figure VIII.13 for the half-filled case as well as for 25% of hole doping. The two cases are supposed to simulate La2 CuO4 and La2−x Srx CuO4 , respectively. The agreement with results of exact diagonalization of a small cluster containing four CuO2 units409 is very good. It is noticed that at half filling the system is insulating and a gap is present. Around ω = 0 one notices the O 2p band and a 3d component due to hybridization. The upper Hubbard band is centered at 5tpd . The structure near −7tpd results mainly from Ad (k) and is interpreted as the lower Hubbard band. The peak near −4tpd comes mainly from Ac (k), i.e., from charge fluctuations. The structure close to 2.5tpd marks the Zhang–Rice singlet state. It is important for the interpretation of spectroscopic experiments.410 When the system is doped f (ω) = [eβω

+ 1]−1

407 P. Unger and P. Fulde, Phys. Rev. B 48, 16607 (1993). 408 P. Unger and P. Fulde, Phys. Rev. B 47, 8947 (1993). 409 T. Tohyama and S. Maekawa, Physica C 191, 193 (1992). 410 H. Romberg, M. Alexander, N. Nücker, P. Adelmann, and J. Fink, Phys. Rev. B 42, 8768 (1990).

STRONGLY CORRELATED ELECTRONS

175

F IG . VIII.13. Spectral density of Cu–O planes described by the Hamiltonian (8.53); (a) at half-filling; (b) for 25% hole doping. Solid and dashed lines show the Cu and O contributions. In the hole doped case spectral density has been shifted from the upper Hubbard band to the region near EF (dotted line). Parameters are Ud = 8, Up = 3, tpp = 0.5, tpd = 1, p − d = 4. Compare also with Figure VIII.14. (After Ref. [407].)

with holes the Fermi energy moves into the Zhang–Rice singlet band. Simultaneously there is a transfer of spectral density taking place from the upper Hubbard band to energies below EF . As mentioned at the beginning of this section we are dealing here with a situation where the internal degrees of freedom of the correlation hole dominate the spectral density. This is most clearly seen by comparing the density of states for the half-filled case with the one obtained in the independent electron approximation. The latter is shown in Figure VIII.14a. It consists of a bonding, nonbonding and antibonding part. The splitting of the d electron contributions into a lower and upper Hubbard band is schematically shown in Figure VIII.14b and the singlettriplet splitting in Figure VIII.14c. The difference between Figures VIII.13a and b demonstrates nicely the effect of the excitations of the correlation hole.

176

P. FULDE ET AL.

F IG . VIII.14. Schematic representation of the density of states of a Cu–O plane described within a 3-band Hubbard model. (a) Independent electron approximation. A, B, NB denote antibonding, bonding and nonbonding part. (b) Splitting of the d band into a lower (LHB) and upper (UHB) Hubbard band. (c) Singlet-triplet splitting (S, T) S = Zhang–Rice singlet.

IX. Summary and Outlook

The different topics we have discussed in this review concern mainly low energy effects of strongly correlated electrons, though not exclusively. In Section VIII we have also given examples of high energy features like shadow bands, satellites and kink effects which originate from strong electron correlations. Low energy effects are mainly due to heavy quasiparticles consisting of an electron with its (rigid) correlation hole. The latter is very pronounced when correlations are strong and therefore an electron moves with a reduced Fermi velocity through the system dragging the correlation hole with it. Low temperature properties are strongly influenced by the effective mass of the quasiparticles. Important examples are Ce-based heavy fermion metals where an interplay of strong on-site 4f Coulomb correlations and hybridization with conduction electrons leads to the heavy quasiparticle mass. These features may be described within Renormalized Band Theory by assuming periodic scattering with a resonant phase shift. This way one obtains the proper heavy quasiparticle bands and the Fermi surface. In recent years it has been realized that in U-based heavy fermion compounds like, e.g., UPd2 Al3 heavy quasiparticles originate from a special mechanism: the 5f electrons form a two-component system with some itinerant and some localized

STRONGLY CORRELATED ELECTRONS

177

orbitals and the renormalization of the former via intra-atomic excitations of the localized 5f electrons leads to strong mass enhancements. In fact, this mechanism has also been identified as the origin of superconductivity in UPd2 Al3 which is not based on electron–phonon interactions. We have also given examples where the low energy excitations cannot simply be described by a Fermi liquid of heavy quasiparticles. In general, even in weakly correlated metals, one expects non-Fermi liquid behavior close to quantum phase transitions. The earliest examples are the logarithmic corrections to the linear specific heat term coming from electrons dressed by paramagnon excitations close to a ferromagnetic quantum critical point. By now numerous examples of mostly Ce-based heavy fermion metals have been found where the vicinity to an AF quantum phase transition leads to pronounced non-Fermi liquid anomalies. Their microscopic understanding is still at an early stage. A different type of deviation from the Fermi liquid picture emerges in strongly correlated electron compounds which exhibit Wigner-lattice type charge order as is the case, e.g., in Yb4 As3 . Here spin and charge degrees of freedom which are responsible for low energy excitations may belong to different types of electrons, i.e., they appear to be separated. In the example of Yb4 As3 the spin degrees of freedom involve 4f holes of Yb while the charge degrees of freedom were found to be due to As 4p holes. The spins of 4f holes are aligned along chains and the 1D neutral spinon excitations cause the large linear specific heat term while light 4p holes carry the current. Quite generally charge ordering in 3d or 4f mixed-valent systems is a promising route to obtain low-dimensional spin structures. An example is NaV2 O5 . There the 1D spin excitations that emerge via charge ordering interact with the lattice leading to a spin-Peierls type dimerization and spin-gap formation. An even stronger kind of lattice coupling occurs in the manganites which leads to polaron formation. The intersite Coulomb correlations then drive charge order of polaronic quasiparticles as observed in the bilayer-manganites. The nonstoichiometric compounds of this class are examples of strong Hund’s rule correlations of itinerant (eg ) and localized (t2g ) electrons. This leads to almost ideal 2D ferromagnetic order driven by kinetic or double exchange mechanisms. Another deviation from a simple Fermi liquid heavy-quasiparticle description was found for the Hubbard model on a square lattice at a particular range of doping and for U above the critical value of the metal–insulator transition at half filling. Here the excitations were of a form previously termed marginal Fermi liquid and suggested to explain some of the properties of layered cuprates. High-energy features of strongly correlated electrons result on the other hand from excitations of internal degrees of freedom of the correlation hole. While the slowly moving quasiparticle has a low excitation energy the internal excitations of its cloud correspond to high energies and show up as satellite structures in photoelectron spectroscopy. Examples were given in Section VIII.

178

P. FULDE ET AL.

In which direction will research on the theory of strongly correlated electrons develop in the future? Here one can only speculate at the risk of being completely wrong. Firstly, there is the field of electronic structure calculations. After LDA based density functional calculations turned out to describe insufficiently strongly correlated electrons they were combined successfully with other approaches to improve on the shortcomings. As discussed in this review Renormalized Band Structure calculations showed considerable predictive power. But also LDA+U and LDA+GW schemes have been applied and yielded insight into strongly correlated electrons. However the more corrections are added to the original approximation to density functional theory like LDA, the less controlled the results are. Double counting of correlation contributions or screening is one of the uncertainties, accounting for the spatial extend of the correlation hole is another. The latter is a problem which also dynamical mean-field theory (DMFT) is facing in its present form. Extensions of that theory to clusters369 are desirable but difficult to realize in practice. This suggests that over the long run wavefunction-based approaches using quantum chemical methods may be a possible solution to the problem. They are technically very demanding but they are well controlled and allow for a detailed understanding of different correlation processes. They may have a great future.41 Exact diagonalizations will certainly also play their role in the future. Usually they use model Hamiltonians with model parameters obtained from single particle LDA(+U) calculations. With increasing possibilities to treat larger clusters they will lead to much new insight into the nature of the correlated ground state as well as the excitations responsible for low temperature thermodynamic anomalies. Analyses of the excitation spectrum of correlation holes seem to be a very promising field. By projecting the calculations onto a few selected variables which represent the most important degrees of freedom, insight may be gained about the relative importance of different correlations. We expect considerable extensions of our understandings of elementary excitations here. As was shown in Section VII in special lattices (here geometrically frustrated ones) it may happen that an electron added to the system may separate into two parts when correlations are strong. This may give raise to charge fractionalization, a phenomenon known from the fractional quantum Hall effect (FQHE).40 Even if there is a weak restoring force between the two parts we would have “quasiparticles” of considerable spatial extent. They would have little in common with the usual picture of an electron surrounded by a correlation hole. Interestingly enough, certain analogies to field theories in elementary particle physics do appear here when dealing with confinement and deconfinement.317,320 After all, why should nature restrict itself to realize certain basic properties only in one particular field of physics and not in others too?

STRONGLY CORRELATED ELECTRONS

179

Acknowledgment

We thank Prof. Y. Kakehashi for a critical reading of Section VIII and for helpful comments. Last not least we thank Mrs. Regine Schuppe for carefully preparing the manuscript. L IST OF ACRONYMS AF ARPES BEC BZ CDW CEF CMR CO CPA DE dHvA DOS DM DMFT EHM e-p FL FM FQHE FS HF ICM INS ISSP ITF JT JW KS LDA LSDA n.n. n.n.n.

antiferromagnet angle resolved photoemission spectroscopy Bose–Einstein condensation Brillouin zone charge density wave crystalline electric field colossal magnetoresistance charge order coherent potential approximation double exchange de Haas–van Alphen density of states Dzyaloshinsky–Moriya dynamical mean-field theory extended Hubbard model electron–phonon Fermi liquid ferromagnet fractional quantum Hall effect Fermi surface heavy fermion or Hartree–Fock incommensurate magnet inelastic neutron scattering Ising-spin-Peierls Ising model in transverse field Jahn–Teller Jordan–Wigner Kondo singlet local density approximation local spin density approximation nearest neighbor next nearest neighbor

180

NCA NFL NMR ODLRO PM QCP QMC QPT RPA RKKY SCF SCPM SDW TB WFM

P. FULDE ET AL.

non-crossing approximation non-Fermi liquid nuclear magnetic resonance off-diagonal long range order paramagnet quantum critical point quantum Monte Carlo quantum phase transition random phase approximation Ruderman–Kittel–Kasuya–Yoshida self-consistent field self-consistent projection method spin density wave tight binding weak ferromagnet

SOLID STATE PHYSICS, VOL. 60

Defect-Induced Dynamic Pattern Formation in Metals and Alloys

Y VES B RÉCHET Laboratoire de Thermodynamique et Physico-Chimie Métallurgiques, Institut National Polytechnique de Grenoble, 38402, St. Martin D’Hères, France

C HRISTOPHER H UTCHINSON Department of Materials Engineering, Monash University, Clayton, 3168, Vic, Australia

I. Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1. Chemical Patterning . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2. Structural Patterning in Systems Prepared Far from Equilibrium . . . . . . . . . . . 3. Structural Patterning in Systems Maintained Far from Equilibrium . . . . . . . . . . 4. Spatio-Temporal Patterning in Plasticity . . . . . . . . . . . . . . . . . . . . . . . . . II. Free Energy Changes, Driving Forces and Energy Input . . . . . . . . . . . . . . . . . . 5. Systems Prepared Far from Equilibrium . . . . . . . . . . . . . . . . . . . . . . . . . 6. Systems Maintained Far from Equilibrium by the Continuous Input of Energy . . . . III. Chemical Patterning: Interface-Mediated Transformations: Eutectoid Decomposition and Discontinuous Precipitation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7. Steady State Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8. The Spacing Selection Problem . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9. Non-Steady State Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10. Coarsening and Related Morphological Evolution . . . . . . . . . . . . . . . . . . . 11. Multilayer Stability . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . IV. Structural Defect Patterning: Grain Growth, Recovery and Recrystallization . . . . . . . 12. Grain Growth . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13. Recovery and Recrystallization of Dislocation Structures . . . . . . . . . . . . . . . V. Structural Defect Patterning: Irradiation and Plastic Deformation . . . . . . . . . . . . . 14. Irradiation Induced Patterning . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15. Plasticity Induced Patterning . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . VI. Spatio-Temporal Patterning in Plasticity: The Portevin–Le Chatelier Effect . . . . . . . . 16. Phenomenology of Portevin–Le Chatelier Effect . . . . . . . . . . . . . . . . . . . . 17. Statistical Analysis of Serrated Flow: An Example of Self Organized Criticality (SOC) 18. Portevin–Le Chatelier Effect: An Example of Deterministic Chaos . . . . . . . . . . VII. Concluding Remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

182 185 186 187 187 188 188 191 192 197 213 218 225 232 233 234 240 248 249 255 273 274 276 282 285

181 ISBN 0-12-607760-6 ISSN 0081-1947/06

© 2006 Elsevier Inc. (USA) All rights reserved.

182

Y. BRÉCHET AND C. HUTCHINSON

I. Introduction

There has recently developed within the non-linear physics community, a deep interest in the formation of ‘patterns’ in condensed matter systems driven far from equilibrium. Patterns are a concept somewhat vague and subjective. We will speak of spontaneous pattern formation when a spatial distribution of matter, or the temporal response of a solid to an external stimulus presents some sort of regularity which has a lower symmetry than its cause. The ideal regularity is periodicity, but one may also consider the possible order in apparently chaotic behavior, or the length scales appearing in an initially homogeneous body. After the extensive work done in fluid mechanics where numerous examples of spontaneous pattern formation may be found (e.g., see Refs. [1,2]), and where the non-linear equations to be solved are well established, solidification seemed to be another of these areas to which the non-linear physicist could apply his methods to model the spontaneous emergence of patterns (dendritic forms and cellular and eutectic structures). Since the classic review paper by Langer,3 a number of new mathematical techniques (e.g., solvability theory) or numerical methods (phase field, cellular automata)4 have been developed to describe and predict the shapes and scales observed when going from the liquid to the solid. For both fluid mechanics and solidification, the dynamic equations to be solved (Navier–Stokes equation, and mass and heat transfer equation) are defined without ambiguity, and the problem is primarily to analyze and solve them. Similarly, the spontaneous patterning (both in space and time) that can be observed in chemical reactions has also attracted significant recent attention, particularly from the ‘Belgian school’. These systems have been labeled ‘dissipative structures’5–7 and in such situations, the transport of matter is often by a diffusion mechanism. The variety of possible ‘intermediate reactions’ leads to a much wider range of partial differential equations than in fluid mechanics or solidification, but the methods currently used to find the conditions for instabilities and their development are quite similar. 1 S. Chandrasekhar, Hydrodynamic and Hydromagnetic Stability, Dover (1981). 2 P. Berge, Y. Pomeau, and C. Vidal, Order within Chaos: Towards a Deterministic Approach to

Turbulence, Wiley, New York (1987). 3 J. S. Langer, Rev. Mod. Phys. 52, 1 (1980). 4 H. Muller-Krumbhaar, W. Kurz and E. A. Brener, in Phase Transformations in Materials, ed. G. Kostorz, Wiley–VCH, Weinheim (2001), p. 81. 5 G. Nicolis and I. Prigogine, Self-Organization in Nonequilibrium Systems: From Dissipative Structures to Order Through Fluctuations, Wiley, New York (1977). 6 D. Walgraef, Spatio-Temporal Pattern Formation: With Examples from Physics, Chemistry, and Materials Science, Springer, New York (1997). 7 C. Vidal and H. Lemarchand, La Reaction Creatrice, Hermann, Paris (1988).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 183

Comparatively less studied by the physics community is the spontaneous patterning in the solid state. This field is also very rich in examples, but there is no equivalent of a ‘Navier–Stokes equation’ which would apply to all the patterns observed. In addition, unlike liquids, crystalline solids also contain structural defects of various dimensions (point defects (0d), dislocations (1d), grain boundaries (2d)), and these defects bring both a new complexity and a new richness to the field. The approach we will take is to present an outline of the relevant phenomena and, where they exist, to summarize the possible equations used to describe the observations and the current models developed by materials scientists to capture the complexity of the problem. The guide line of this chapter, which at the same time gives it its unity and limits its scope, is ‘spontaneous pattern formation’ in solids driven far from equilibrium, involving explicitly the role of structural defects. It is well recognized that there is an energetic cost associated with pattern formation that involves a multiplication of interfaces. This is one fundamental reason for which being far from equilibrium seems to be a necessary condition for obtaining patterns. Solids can be either prepared out of equilibrium, or maintained out of equilibrium by a continuous injection of energy from outside the system. Both cases are possible for metallic alloys, and both lead to pattern formation. For example, preparing a solid far from equilibrium can be achieved by rapidly cooling below a phase boundary of the phase diagram: the high temperature structure is then out of equilibrium. Maintaining a system out of equilibrium can be accomplished either by plastic deformation or by irradiation: we refer to such systems as ‘driven systems’ and again, in these cases, patterns may spontaneously appear. In metallic alloys, pattern formation in space can be manifested in two ways: it can be a patterning of phases of different chemical composition, such as in the decomposition of solid solutions, or it can be a patterning of the structural defects themselves as in the case of plastically deformed materials. Pattern formation in time is well know in chemistry, and ‘chemical clocks’ have been central to the development of the methods of non-linear physics.5,8 To our knowledge there is no equivalent in the solid state (except perhaps in periodic oxidation, but it is translated in space under the form of layered oxides9 ). However, under special circumstances, we can observe an equivalent in the plastic behavior of materials: ‘serrated yielding’. 8 H. Haken, Synergetics: An Introduction: Nonequilibrium Phase Transitions and Self-Organization in Physics, Chemistry, and Biology, Springer, New York (1983). 9 G. Bertrand, Solid State Phenomena 3–4, 257 (1988).

184

Y. BRÉCHET AND C. HUTCHINSON

TABLE I.1. C LASSIFICATION OF THE PATTERNING E XAMPLES P RESENTED IN THIS C HAPTER Structural defects patterning

Chemical patterning

Systems prepared far Grain growth, recovery and from equilibrium recrystallization (Section IV)

Interface-mediated phase transformations: Pearlite and Discontinuous precipitation (Section III)

Systems maintained far from equilibrium

Driven systems10 Irradiation induced precipitation and order/disorder transition, Ball milling amorphization11 Fatigue induced dissolution12

Spatial patterning (Section V) Dislocation and void self organization under irradiation. Pattern formation in plasticity (creep, fatigue...) Temporal patterning (Section VI) Serrated yielding (Portevin–Le Chatelier effect)

We have classified the various phenomena to be presented in this chapter in Table I.1. We do not claim to be exhaustive (e.g., neither pattern formation in dynamic fracture nor pattern formation in martensitic transformations is treated here, and the case of chemical patterning under irradiation has recently been reviewed in the same series10 ), but we aim to present examples which are representative both of the phenomena occurring in the solid state involving structural defects as central actors, and of the current tools used for their understanding. For systems prepared far from equilibrium that produce patterns whilst approaching the equilibrium state, thermodynamics is a natural guide: it indicates the end point of the transformation, and computing the ‘driving force’ for the evolution is meaningful. For systems maintained far from equilibrium, the situation is much more confusing, and the input of energy into the system is a key parameter, together with the ability of the system to store it or to dissipate it as heat. In these driven systems, the kinetics of the defects becomes a central issue, and therefore the modelling is bound to be much more ‘system and problem specific’. Depending on the nature of the departure from equilibrium (initially imposed or constantly maintained) the questions of driving forces and energy input must be addressed differently along with the consequences on relevant kinetic mechanisms. In a driven system, besides the natural atomic movements due to thermal activation, extra mobilities associated either with irradiation damage or with 10 G. Martin and P. Bellon, in Solid State Physics, vol. 50, eds. H. Ehrenreich and F. Spaepen, Acad-

emic Press (1997), p. 189. 11 P. Pochet, L. Chaffron, P. Bellon, and G. Martin, Ann. Chimie 22, 363 (1997). 12 Y. Brechet, F. Louchet, C. Marchionni, and J. L. Vergergaugry, Phil. Mag. A 56, 353 (1987).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 185

dislocation motion must also be taken into account. The evaluation of the contributions to the driving force and the relative magnitudes compared to the input energies will be discussed in Section II. Within this scheme, the examples to be treated can be put into perspective with other systems more familiar to the physics community. We will consider successively: chemical patterning, structural defect patterning, and spatio-temporal patterning in plasticity. 1. C HEMICAL PATTERNING There is often a thermodynamic requirement that alloys decompose, i.e., to produce, from an initially homogeneous mixture of different atomic species, phases with different compositions well separated in space. This process of decomposition, which reflects the competition between the entropic term which wins at high temperature and the enthalpic terms which dominate at low temperature, tends to bring the alloy closer to thermodynamic equilibrium. In these situations, there is a thermodynamic potential which ‘shows the way’, the free energy, and the possible kinetic paths for the alloy lead to a succession of microstructures that are spatially heterogeneous. One class of these phenomena, the diffusional decomposition of a solid solution by precipitation and/or spinodal decomposition, is familiar to the physics community. The process generates length scales and kinetic scaling laws which have been extensively studied, experimentally, theoretically, and with computer simulations (for a review, see Refs. [13,14]). At this level of generality, it does not really matter if the decomposition is in a solid or in a liquid. However, the specificity of the solid being able to sustain shear and usually having a crystalline structure introduces a new richness through the elastic effects and crystal anisotropy. Pattern formation under these conditions has been extensively studied,15–17 and leads to specific behavior as far as coarsening rates and shapes are concerned. Again, the classical tools of statistical mechanics and computer simulations have led this field to a state of maturity, and it will not be reviewed here. When decomposition is thermodynamically possible, there are various possible kinetic pathways, all compatible with the thermodynamics. One of them is to 13 R. Wagner, R. Kampmann, and P. W. Voorhees, in Phase Transformations in Materials, ed. G. Kos-

torz, Wiley–VCH, Weinheim (2001), p. 309. 14 K. Binder and P. Fratzl, in Phase Transformations in Materials, ed. G. Kostorz, Wiley–VCH, Wein-

heim (2001), p. 409. 15 P. Fratzl, O. Penrose, and J. Lebowitz, J. Stat. Phys. 95, 1429 (1999). 16 F. Larche, in Dislocations in Solids, ed. F. R. N. Nabarro, North-Holland, Amsterdam, Netherlands

(1979), p. 135. 17 A. G. Khachaturian, Theory of Structural Transformations in Solids, Wiley, New York (1983).

186

Y. BRÉCHET AND C. HUTCHINSON

take advantage of the defects in the material to find short circuits toward thermodynamic equilibrium. The decomposition, instead of taking place by a homogeneous nucleation and growth process, may take advantage of existing interfaces in the solid (most often grain boundaries) or it may proceed by creating an interface and propagating a front into the non-transformed region, to approach thermodynamic equilibrium more closely. These interface-mediated transformations lead to very nice regular patterns, which bear some similarities to those observed in solidification.18 These patterns have attracted considerable interest in materials science and we will attempt to summarize this form of solid state patterning in Section III. 2. S TRUCTURAL PATTERNING IN S YSTEMS P REPARED FAR FROM E QUILIBRIUM Metals and alloys are rarely in their state of thermodynamic equilibrium. This would be given by the phase distributions predicted by the phase diagram, and given an infinite length scale, would, in principle, lead to an interfacial energy contribution equal to zero. Even the simplest case of a solidified pure metal, usually consists of a polycrystalline structure, i.e., it contains grain boundaries which are surface defects with an associated surface energy. This is the simplest possible out of equilibrium situation which may lead to defect patterning. The phenomenon of grain growth, in spite of its simplicity, presents some features of pattern forming systems which are worth further investigations.19,20 The difference with the classical ‘domain growth with non-conserved order parameter’ familiar to the statistical physicist will be reviewed. Relying on recent simulations, some open questions on grain growth will be addressed in Section IV.12. Another way of introducing extra energy in a simple system is through plastic deformation. The dislocations stored in the material after a deformation step tend to annihilate during further annealing, bringing the system closer to thermodynamic equilibrium. This procedure may be smooth and lengthy, or it may be discontinuous and rapid. The two phenomena, referred to as recovery and recrystallization,21 are different pathways to thermodynamic equilibrium, and although they do not generate organized patterns, they lead to the evolution of patterns which in itself reveals some important differences between deformation 18 G. R. Purdy and Y. J. M. Brechet, in Phase Transformations in Materials, ed. G. Kostorz, Wiley–

VCH, Weinheim (2001), p. 481. 19 D. Weaire and S. McMurry, Solid State Physics 50, 1 (1997). 20 C. V. Thompson, Solid State Physics 55, 269 (2000). 21 F. J. Humphreys, Recrystallization and Related Annealing Phenomena, Elsevier Science, New York

(2003).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 187

structures and equilibrium structures. These aspects will be discussed in Section IV.13 with a view to understanding the patterns formed during plastic deformation (Section V.15). 3. S TRUCTURAL PATTERNING IN S YSTEMS M AINTAINED FAR FROM E QUILIBRIUM A system may be maintained out of equilibrium by a continuous input of energy. Two cases will be investigated in this section. In Section V.14 we investigate the remarkable patterns arising from irradiation damage. The input of energy is transformed at least partially into point defects and the dynamical evolution of this population (its aggregation into dislocation loops or cavities) leads to patterns which are striking by their regularity (both in scale and in crystallographic orientation). The regular networks of dislocation loops or voids and bubbles is one of the most convincing cases of pattern formation in driven systems in metallurgy. The classical methods of ‘chemical kinetics’ have been remarkably successful in explaining them. This ‘success story’ is to be contrasted with the case described in Section V.15: pattern formation in plasticity. The patterns observed are also very nice although less regular, but our understanding of them is much less complete. The comparison with pattern formation under irradiation will help in identifying both the necessary ingredients to be included in a future theory for pattern formation during plastic deformation, and the limits of the ‘chemical reaction’ approach. Recent developments from intensive computer simulations as well as stochastic approaches will be presented. 4. S PATIO -T EMPORAL PATTERNING IN P LASTICITY Patterning at the microstructural scale is only one feature of plasticity. The distribution of plastic deformation in space may not be homogeneous, and in some situations, well defined ‘plastic waves’ may travel through the sample. The stressstrain curve is then no longer smooth and the observation of ‘serrated yielding’ presents some complex features strongly reminiscent of ‘stick-slip’ behavior. We will focus our attention on the Portevin–Le Chatelier (PLC) effect, and illustrate the existence of a regime of self-organized criticality (SOC),22 and of deterministic chaos.2 22 H. J. Jensen, Self-Organized Criticality, Cambridge University Press, Cambridge (1998).

188

Y. BRÉCHET AND C. HUTCHINSON

II. Free Energy Changes, Driving Forces and Energy Input

We have classified the different flavors of defect-induced solid state patterning according to whether they occur in systems prepared far from equilibrium whilst approaching equilibrium or whether they occur in systems that are maintained far from equilibrium by some external input of energy (Table I.1). This classification not only provides a nice physical picture of the differences between the two types of patterning systems but also highlights the important fundamental difference that necessitates different theoretical approaches. As we shall see in the coming chapters, the relative success we have had in describing and explaining the patterning observed in the solid state, accurately reflects the relative maturity of the theoretical framework available for the two types of systems. 5. S YSTEMS P REPARED FAR FROM E QUILIBRIUM The systems in which patterning is observed during an approach to equilibrium include interface-mediated chemical patterning and defect patterning in grain growth, recrystallization and recovery. Under isothermal conditions, these systems can be considered to be ‘closed’ in a thermodynamic sense and well defined initial and final states can be identified using classical thermodynamics. A thermodynamic potential, ‘the free energy’, can be defined and the change in this potential in going from the initial state to the final state can be quantified. The contributions to this free energy change that are interest to us are usually classified as chemical energy, strain energy and interfacial (surface) energy and we shall discuss these further in a moment. However, we are interested in dynamic pattern formation. This is the spontaneous patterning that occurs during the change from the initial to the final state and these changes are intrinsically irreversible. Even though the initial and final states may be well defined, classical thermodynamics tells us nothing about these irreversible changes. To describe the changes we resort to kinetic descriptions of the underlying physical processes (diffusion, dislocation glide, etc.) and then the theory of irreversible thermodynamics23–25 provides us with a means of linking these irreversible microstructural changes to the equilibrium descriptions of the initial and final states. Our ability to describe the changes that occur depends on our ability to describe the initial and final states and on our understanding and ability to accu23 W. Yourgrau, A. van der Merwe, and G. Raw, Treatise on Irreversible and Statistical Physics, MacMillan, New York (1966). 24 S. R. DeGroot and P. Mazur, Non-Equilibrium Thermodynamics, North-Holland, Amsterdam, (1962). 25 R. Haase Thermodynamics of Irreversible Processes, Addison-Wesley, Reading, MA (1969).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 189

rately describe the fundamental physical processes underlying the changes that occur within the material. This approach has been very successful at describing, for example, the kinetics of phase transformations13,14 where mass transport by diffusion is the primary process governing change. The kinetic descriptions of the underlying physical processes are usually based on the assumption that the rate of the process is linearly related to the gradient in a relevant thermodynamic potential. This is not a consequence of the theory of irreversible thermodynamics, but is a hypothesis that appears to be experimentally well supported. Fick’s first law of diffusion (Eq. (2.1)) in an n component system is a good example: Ji =

n

−Lij grad(μj ),

(2.1)

j =1

Lij are phenomenological coefficients and μj is the chemical potential of component j . In this case the solute flux is proportional to the gradient in the chemical potential of the solute species. We usually refer to the gradient in the thermodynamic potential as the ‘driving force’ and the gradient in the chemical potential is the driving force for solute diffusion. These driving forces are not independent of the free energy change associated with the initial and final states of the material but neither are they the same. The driving forces are locally defined and should be associated with some particular physical process. Nevertheless, we usually categorize the driving forces in the same way as we categorize the free energy changes and it is worthwhile summarizing these different contributions.

a. Chemical Energy: The Free Energy of Strain-Free Regions of a Phase When the compositions and/or the structures of the phases in a system deviate from the equilibrium values under the conditions examined a driving force for solute redistribution and/or crystal structure change arises. The classic example may be the cooling of pure Fe below the allotriomorphic phase transformation temperature of 1183 K. The change in free energy associated with the crystal structure change is of the order of 1 kJ/mol (140 MJ/m3 ). Other microstructural changes driven by chemical free energy familiar to the physicist include the precipitation of a second phase from a metastable homogeneous solid solution.13 In this case the chemical free energy change attending the reaction is typically somewhere in the range 0.1–3 kJ/mol (∼10–300 MJ/m3 ) and is used to drive both the crystal structure change and the necessary solute redistribution.

190

Y. BRÉCHET AND C. HUTCHINSON

b. Strain Energy: The Increase in Free Energy Caused by Short and Long Range Elastic Strains When a metal or alloy is deformed most of the work done is liberated as heat. However, a small amount (which is less than 10% and decreases with increasing strain) is stored within the material in the form of lattice strains and imperfections. The most important of these are dislocations which have a long range strain field. In most cases the entropic contribution to the free energy of the material from dislocations is negligible compared with the strain energy contribution and we can approximate the increase in free energy with the strain energy of the dislocation ensemble. The elastic stored energy of a single isolated edge dislocation is:

μb2 r ED = , (2.2) Ln 4π(1 − ν) r0 μ is the shear modulus of the material, b is the burgers vector, r is the outer cut-off radius (which could be the specimen surface), r0 is the inner cut-off radius and ν is Poisson’s ratio. In addition to the elastic stored energy of the long range strain field, we also associate a ‘core’ energy with the dislocation with a magnitude similar to the elastic contribution. Often, the total is approximated as 12 ρμb2 . An ensemble of dislocations, ρ, can reduce its free energy contribution from ρED by reducing r through the rearrangement into stress-screening arrays. Clearly both the density and the distribution of dislocations must be known to calculate the free energy contribution from the dislocations. For a typical metal deformed at room temperature and containing a high dislocation density of 1 · 1015 m−2 we may estimate the upper limit to the total strain energy (ρED ) as of the order of 10–20 J/mol (1–3 MJ/m3 ). It is this free energy that drives the recovery and recrystallization processes to be discussed in Section IV.13. Unlike solute diffusion, where the kinetic processes are relatively well described (Eq. (2.1)), dislocation motion is much more problematic. Dislocations motion is restricted to well defined crystallographic planes and dislocations are non-conserved quantities. They move by a dislocation glide process which occurs more readily than diffusion. These kinetic aspects as well as the difficulty in defining a local driving force for dislocation motion (which depends on the density and distribution of all other dislocations) will be discussed in later chapters and highlights the difficulties faced in describing dislocation patterning.

c. Interfacial (Surface) Energy: The Extra Free Energy of Atoms at Interfaces Between Phases and at Grain Boundaries The extra energy associated with the atoms at the interfaces between phases and at grain boundaries is a free energy. This excess free energy is usually expressed

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 191

as an energy per unit area of interface and gives rise to a driving force to reduce the interfacial area. This reduction occurs through interface migration and the local driving force is usually expressed in terms of a chemical potential difference on either side of an interface: 2σ μ = , (2.3) r σ is the interfacial free energy per unit area and r is the radius of curvature of the interface (which can be generalized to two principle radii of curvature for an arbitrary boundary). It is the interfacial contribution to the free energy of the system that drives the grain growth processes to be discussed in Section IV.12. A typical grain boundary energy in a metal may be expected to lie somewhere between 0.4–1 J/m2 and for a grain size of 10 µm, this would give rise to a local driving force acting over the interface of the order of 1 J/mol (0.1 MJ/m3 ). The kinetic description of interface motion is usually based on an assumed proportionality between this driving force and the interface velocity. The above separation of the driving forces into chemical, strain and interfacial energies is useful for discussion purposes but it is of course artificial. Not only is there usually more than one type of contribution present, but the contributions often also represent retarding forces that need to be overcome for the physical process to proceed. For example, a concentration gradient in an otherwise perfect crystal will have contributions to the driving force from both chemical and strain energies. The latter arises from the concentration dependence of the molar volume of the lattice. In the case of the interface-mediated transformations to be discussed in Section III, the transformation (which is driven by the chemical free energy change) results in the generation of interfaces and strains (because of differences in molar volumes of the phases). The associated interfacial and strain energies must be ‘paid for’ by the chemical free energy driving the transformation. When considering the contributions (driving or retarding) from chemical, strain and interfacial energies, it is useful to bear in mind the relative magnitudes. Although the driving forces usually evolve in time, in general we find that the typical chemical contribution is one or two orders of magnitude larger than a typical strain energy contribution which is usually at least an order of magnitude larger than the interfacial energy contribution. 6. S YSTEMS M AINTAINED FAR FROM E QUILIBRIUM BY THE C ONTINUOUS I NPUT OF E NERGY For those systems that are continuously maintained far from equilibrium by the input of energy, no general framework such as that offered by classical and irreversible thermodynamics discussed above exists. It is not meaningful to define

192

Y. BRÉCHET AND C. HUTCHINSON

an initial and final state of the material. The system is dynamic and the external input of energy input plays a vital role in the identification and the stability of any stationary states. The defect patterning that occurs during irradiation and during plastic deformation both belong to these types of systems. The energetic contributions to the driving forces discussed above (chemical, strain and interfacial) all still apply to driven systems but an additional two factors must also now be considered. The first is the input of energy into the systems and the means of storing this energy. In the case of plastic deformation, the energy is stored in the form of dislocations and represents less than 10% of the energy expended in deformation. In the case of irradiation, the equivalent quantity is the displacement per atom induced by irradiation. The energy is stored in the form of point defects (vacancies and interstitials) and the only way to evaluate the quantities in an irradiation cascade is through molecular dynamics simulations. This continuous input of energy during plastic deformation or irradiation modifies the ‘potential landscape’ in which the system evolves. Any attempts at identifying stationary states must consider the effect of this input energy on the landscape being sampled. In addition, the defects introduced by plastic deformation and irradiation modify the kinetic processes governing the changes in the material. Therefore, not only is the ‘potential landscape’ modified but the kinetic pathways available for searching the landscape are also changed. Both of these aspects must be considered in dealing with microstructural evolution in driven systems. As we shall see in Section V.14, some success has been achieved in dealing with patterning under irradiation. In these cases a ‘chemical kinetics’ approach was adopted which shows some good agreement with experiment. In Section V.15, we discuss patterning during plastic deformation and we shall see that our understanding is much less complete. The difficulties in identifying the local driving force for dislocation motion and in mimicking the dislocation transport (glide) process currently present some barriers to progress. III. Chemical Patterning: Interface-Mediated Transformations: Eutectoid Decomposition and Discontinuous Precipitation

Probably the best known of all solid state patterns formed in the science of metals and alloys, and certainly the most thoroughly studied, is that arising from the pearlite phase transformation in steels. The reaction belongs to the class of eutectoid transformations (the solid state equivalent of the eutectic transformation) and involves the decomposition of the face-centered cubic austenite (γ ) phase into a lamellar pattern of body-centered cubic carbon-poor ferrite (α) and carbon-rich orthorhombic cementite (Fe3 C) behind a migrating interphase boundary. γ → α + Fe3 C

(3.1)

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 193

In this case, the defect involved in the pattern formation is the interface which is created between the growing product phases and the parent phase. The transformation usually begins at the prior γ grain boundaries or other structural heterogeneities and an example taken from an Fe-0.8C (wt.%) alloy is shown in Figure III.126 together with the phase diagram illustrating the three phases involved in the transformation. Although the pearlite transformation in steels is by far the best known and studied of the eutectoid transformations, the formation of lamellar patterns from eutectoid decomposition in systems other than those based on Fe-C are also well known (e.g., Cu-Al,27–30 Zn-Al,31 Cu-In,32 Au-In33 ). In all cases, the parent phase transforms into two different product phases and growth involves the redistribution of solute from the solute-poor product phase to the solute-rich phase. An important input into the theoretical treatments of growth is an identification of the ‘path’ taken by the redistributing solute. In some cases, such as in the Cu-Al system,29 it has been quite well established that the diffusion occurs in the parent phase ahead of the migrating interface. In other cases (e.g., Cu-In32 ), it has been concluded that the solute redistribution occurs by shortcircuit diffusion within the migrating interphase boundary itself where the atomic arrangement is comparatively disordered.34,35 In the overwhelming majority of cases of pearlite growth, the necessary solute redistribution from the solute poor phase to the solute rich is restricted to the vicinity of the transformation interface and no long range solute diffusion either to or from the parent phase is observed. The pearlite aggregate forms with the same overall composition as the parent phase and growth occurs at a constant rate with a constant interlamellar spacing. It is these two characteristics of the pattern formation in eutectoid decomposition that have attracted the interest of researchers in materials science. In the solid state, a lamellar pattern resembling the pearlite transformation in appearance can also arise as the product of a simple precipitation reaction involving only two crystallographically distinct phases. The transformation is referred 26 L. S. Darken and R. M. Fisher, in Decomposition of Austenite by Diffusional Processes, eds.

V. F. Zackay and H. I. Aaronson, Interscience, New York (1962), p. 249. 27 G. V. T. Ranzetta and D. F. R. West, J. Inst. Metals 92, 12 (1964). 28 M. K. Asundi and D. F. R. West, J. Inst. Metals 94, 19 (1966). 29 D. Cheetham and N. Ridley, Metall. Mater. Trans. A 4, 2549 (1973). 30 M. J. Whiting and P. Tsakiropoulos, Acta mater. 45, 2027 (1997). 31 D. Cheetham and N. Ridley, J. Inst. Metals 99, 371 (1971). 32 A. Das, S. K. Pabi, I. Manna, and W. Gust, J. Mat. Sci. 34, 1815 (1999). 33 A. Das, W. Gust, and E. J. Mittemeijer, Mat. Sci. and Tech. 16, 593 (2000). 34 Y. Mishin, C. Herzig, J. Bernardini, and W. Gust, Int. Mat. Rev. 42, 155 (1997). 35 I. Kaur and W. Gust, Diff. and Def. Data A 66–69, 765 (1989).

194

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.1. (a) Optical micrograph of a pearlite colony in an Fe-0.8C (wt.%) alloy partially transformed at 700 ◦ C. The lamellar pattern consists of alternating plates of Fe3 C (dark) and α (light) separated from the parent γ phase by an interphase boundary. (b) The Fe-rich end of the binary Fe-C phase diagram illustrating the three phases involved in eutectoid decomposition. The C content of the α phase is so low that the single α phase field cannot be resolved for the domain of C contents chosen for illustration.

to as ‘discontinuous’ precipitation to distinguish it from the competitive ‘continuous’ mode of relieving the supersaturation of the parent phase, familiar to the physicist.13,14 Discontinuous precipitation also usually begins at grain bound-

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 195

F IG . III.2. (a) Bright field transmission electron microscopy image of discontinuous precipitation in an Al-22Zn (at.%) alloy partially transformed at 478 K. The lamellar pattern consists of alternating plates of β-Zn and a solute depleted α-Al phase separated from the supersaturated α0 phase (parent phase) by a grain boundary. (b) The binary Al-Zn phase diagram illustrating the two phases involved in discontinuous precipitation.

aries in the supersaturated parent phase (α0 ) and forms as a regular aggregate of alternating compound phase (β) and a solute depleted matrix phase (α) growing behind a migrating grain boundary which separates the product from the parent phase (e.g., Figure III.2a). α0 → α + β

(3.2)

196

Y. BRÉCHET AND C. HUTCHINSON

The solute depleted matrix phase (α) is identical in structure to the parent phase (α0 ) and differs only in solute content and crystal orientation across the transformation interface. The solute content and orientation appear to change ‘discontinuously’ across the grain boundary and it is from this change that the transformation derives its name. The solute redistribution from the solute depleted product phase to the solute rich compound phase occurs by short circuit diffusion within the transformation interface and volume diffusion in the parent phase is thought to play little role in the transformation. Like most cases of the pearlite transformation, under isothermal conditions the discontinuous precipitation product usually forms with the same overall composition as the parent phase and growth at a constant rate with a constant interlamellar spacing is observed. Discontinuous precipitation has now been identified in more than 150 binary and ternary systems. A comprehensive review of theses systems was recently compiled by Manna et al.36 and a thorough discussion of many aspects of the reaction can be found in the monograph by Pawlowski and Zieba37 and in several recent reviews.18,38 An example taken from the Al-Zn system39 is shown in Figure III.2 along with a section of the corresponding binary phase diagram. In the transmission electron micrograph shown, discontinuous precipitation of the β-Zn phase and the Zn poor α-Al matrix lamellar phase grow behind a migrating grain boundary into the parent phase. Unlike eutectoid decomposition, where pearlite formation is associated with a definite feature of the phase diagram (the eutectoid), it is not well understood under which conditions a supersaturated solution will decompose solely in a discontinuous manner, solely in a continuous manner or both together in a competitive manner. The result depends on the competition between the nucleation and growth of the continuous and discontinuous products. Although the growth aspects of both of these problems are now reasonably well understood, a reliable quantitative understanding of the rates of nucleation of the two products is lacking. This is especially true for the initiation of the discontinuous reaction. Several initiation mechanisms have been proposed over the years36,37,39–42 but so far no single origin is consistent with all of the experimental observations. 36 I. Manna, S. K. Pabi, and W. Gust, Int. Mat. Rev. 46, 53 (2001). 37 A. Pawlowski and P. Zieba, Phase Transformations: Controlled by Diffusion at Moving Boundaries,

Polish Academy of Sciences, Warszawa (1991). 38 D. B. Williams and E. P. Butler, Int. Metals Rev. 26, 153 (1981). 39 I. G. Solorzano, G. R. Purdy, and G. C. Weatherly, Acta metall. 32, 1709 (1984). 40 G. Meyrick, Scripta metall. 10, 649 (1976). 41 S. F. Baumann, J. Michael, and D. B. Williams, Acta metall. 29, 1343 (1981). 42 H. I. Aaronson and C. S. Pande, Acta mater. 47, 175 (1998).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 197

The pearlite and discontinuous reactions shown in Figures III.1 and III.2 give rise to lamellar patterns. The pattern takes the form of alternating plates of the product phases and this is indeed the most commonly observed morphology. Less frequently, products of both the discontinuous and eutectoid decomposition reactions have also been observed to adopt ‘rod-like’ morphology; examples include the discontinuous precipitation reaction in Cu-Co43 and the pearlite (α + Mo2 C) formed in Fe-C-Mo.44 As is the case for eutectic solidification, the choice of morphology depends on the relative volume fraction of phases formed and the energy of the interface between the product phases.4 In the following discussion, we shall restrict ourselves to treatments of the more common lamellar morphology. The regularity of the patterns formed from the pearlite and discontinuous precipitation reactions has led many theoreticians to search for a quantitative description of the pattern repeat distance and the growth rate. In Section III.7, we review the most popular treatments and then in Section III.8 consider the attempts to resolve the central unanswered growth related question: ‘the spacing selection problem’. A brief discussion of lamellar pattern formation under non-steady state conditions is presented in Section III.9 and some illustrations of the resulting patterns are provided. Since the products of both the pearlite and the discontinuous precipitation reactions are highly non-equilibrium structures, a significant driving force exists for coarsening processes. In Section III.10 we summarize the known mechanisms responsible for the changes in shape and scale of the lamellar products during coarsening. Finally, a short discussion on the possibility of using artificially created metallic multilayers to investigate some of the fundamental aspects of the selection and evolution of solid state patterns in interface-mediated transformations is presented. 7. S TEADY S TATE G ROWTH

a. Theoretical Treatments The pearlite and discontinuous precipitation products shown in Figures III.1 and III.2 were formed isothermally under steady state conditions with an approximately constant (average) growth rate and interlamellar spacing. This problem of the steady state growth of a lamellar pattern has a long history and has been

43 A. Perovic and G. R. Purdy, Acta metall. 29, 53 (1981). 44 R. E. Hackenberg and G. J. Shiflet, Acta mater. 51, 2131 (2003).

198

Y. BRÉCHET AND C. HUTCHINSON

considered by many authors.45–66 In the following, we will present a selection from the sequence of models which have appeared in the literature, each model representing a response to the limitations of its predecessors. The reason for this approach is not only to provide a clearer insight into the necessary ingredients for a full solution of the problem, but also to give the reader access to the simplest model possible for interpreting their experimental observations. If only the growth kinetics and length scales are to be interpreted, then Zener’s47 approach is sufficient. If local chemical analysis between lamellae is to be analyzed, then the full solution of the diffusion equation provided by Cahn50 is necessary. If the shapes of the moving boundaries are available to experimental investigation, then the treatment developed by Hillert49,57,60,64 is necessary. If the full selection problem is to be investigated, then a complete solution of the diffusion equations, coupled with appropriate thermodynamic data and a local force balance at every position along the transformation interface is required. We start with the simplest approaches and progressively proceed toward the more sophisticated ones, but want to emphasize that for a given set of experimental observations the appropriate theory may not be the most sophisticated one. At the outset it is worth emphasizing the difference between the pearlite and discontinuous precipitation reactions. Even though both processes give rise to a lamellar pattern and the diffusion geometry is similar in both cases, one reaction is 45 W. H. Brandt, J. Appl. Phys. 16, 139 (1945). 46 E. Scheil, Z. Metallkd. 37, 123 (1946). 47 C. Zener, Trans. AIME 167, 550 (1946). 48 D. Turnbull, Acta metall. 3, 55 (1955). 49 M. Hillert, Jernkont. Ann. 141, 757 (1957). 50 J. W. Cahn, Acta metall. 7, 18 (1959). 51 K. A. Jackson and J. D. Hunt, Trans. AIME 236, 1129 (1966). 52 K.-N. Tu and D. Turnbull, Scripta metall. 1, 173 (1967). 53 H. I. Aaronson and Y. C. Liu, Scripta metall. 2, 1 (1968). 54 B. E. Sundquist, Acta metall. 16, 1413 (1968). 55 J. M. Shapiro and J. S. Kirkaldy, Acta metall. 16, 579 (1968). 56 J. Petermann and E. Hornbogen, Z. Metallkunde 59, 814 (1968). 57 M. Hillert, in Mechanism of Phase Transformations in Solids, vol. 33, The Institute of Metals

(1968), p. 231. 58 B. E. Sundquist, Acta metall. 17, 967 (1969). 59 M. Hillert, Acta metall. 19, 769 (1971). 60 M. Hillert, Metall. Mater. Trans. A 3, 2729 (1972). 61 M. P. Puls and J. S. Kirkaldy, Metall. Mater. Trans. A 3, 2777 (1972). 62 G. Bolze, M. P. Puls, and J. S. Kirkaldy, Acta metall. 20, 73 (1972). 63 B. E. Sundquist, Metall. Trans. A 4, 1919 (1973). 64 M. Hillert, Acta metall. 30, 1689 (1982). 65 A. Bogel and W. Gust, Z. Metallkd. 79, 296 (1988). 66 L. Klinger, Y. J. M. Brechet, and G. R. Purdy, Acta mater. 45, 5005 (1997).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 199

a precipitation reaction and involves only two different phases, whereas the eutectoid decomposition reaction involves three different phases. The thermodynamic situation in the two cases is very different and this difference must be considered in the development of models that attempt to explain the observed growth. Nevertheless, there are many common assumptions made in the derivations and it is also worth summarizing these commonalities. In all cases, the model derivations are based on the isothermal growth of a perfectly regular lamellar aggregate. The isothermal assumption includes all areas of the transformation interface and it is assumed that the heat liberated by the reaction can be conducted away from the transformed volume quickly enough that any local rises in temperature can be ignored. It is usually assumed that all of the phases involved in the reaction have equal molar volumes and that any local stresses developed upon transformation have a negligible influence upon the growth. Finally, it is usually assumed that any interfacial energies that enter into the derivation are isotropic. One of the earliest theoretical treatments was due to Zener47 who was interested in describing the kinetics of the pearlite transformation in steels (Eq. (3.1), Figure III.1). Zener provided an approximate treatment that assumed the growth rate of the pattern was controlled by the redistribution of carbon from the ferrite (α) to the cementite (Fe3 C) and that this occurred entirely by volume diffusion in the parent austenite (γ ) phase, Figure III.3. The diffusion was driven by the difference in carbon composition in the γ at the γ /α and γ /Fe3 C interfaces, (X γ /α − X γ /Fe3 C ). If the γ /α and γ /Fe3 C interfaces are planar and assuming dilute solution thermodynamics, then the driving force for carbon redistribution is given by the difference in interfacial carbon contents which are usually assumed to be the equilibrium values (local equilibrium assumption) found from the metastable extensions of the γ /(γ + α) and γ /(γ + Fe3 C) phase boundaries into the (α + Fe3 C) two phase field of the phase diagram (dotted lines, Figure III.1b). Zener realized that not all of this driving force could be used to drive the C diffusion because during growth some must be spent on the creation of the new α/Fe3 C interfaces. The driving force, G, spent on the creation of the interlamellar interface is 2σ Vm , (3.3) λ λ is the interlamellar spacing (pattern repeat distance), σ is the surface energy of the α/Fe3 C interface and Vm is the molar volume assumed to be the same for all phases. A critical interlamellar spacing, λc , can be identified for which all the free energy available would be spent on creating α/Fe3 C interfaces and the growth rate of the aggregate would fall to zero. For interlamellar spacings greater than λc , = Gsurface m

200

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.3. Schematic illustration of the diffusion geometry for lamellar pattern formation under conditions where the solute redistribution occurs by volume diffusion in the parent phase.

the net driving force for diffusion could then be approximated by multiplying the total driving force for the reaction by a scaling factor, (1 − λc /λ). Combining this driving force for C diffusion with a characteristic diffusion distance (which was assumed proportional to the lamellar thickness), a carbon flux can be evaluated and when combined with a solute mass balance across the interface, an expression for the growth rate of the regular lamellar aggregate can be written:47,60

γ /α γ /Fe C λc Xe − Xe 3 1 2D γ 1− , (3.4) ν = α Fe C λ λ f f 3 X Fe3 C − X α v is the growth rate, D γ is the C diffusivity in γ , λα and λFe3 C are thicknesses of the α and Fe3 C lamellae respectively, the interlamellar spacing λ = λα + λFe3 C , f α and f Fe3 C are the mol fractions of α and Fe3 C in the aggregate, X α and X Fe3 C are the C compositions of the growing α and Fe3 C phases, both assumed to be γ /α γ /Fe C constant, and Xe and Xe 3 are the C compositions in the γ at the γ /α and γ /Fe3 C interfaces, usually assumed to be the local equilibrium values found from the phase diagram. Zener’s treatment, like almost all subsequent treatments, provides a relationship between the growth velocity, the interlamellar spacing and the boundary

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 201

conditions of the diffusion problem. After a choice of appropriate interfacial compositions, an additional criterion is still required to decouple the interface velocity from the interlamellar spacing to obtain a unique velocity/spacing pair. This is referred to as the ‘spacing selection’ problem. Zener invoked a maximum growth rate hypothesis to remove the degeneracy of the problem and it is clear from Eq. (3.4) that the maximum growth rate occurs at an interlamellar spacing, λ = 2λC , (i.e., when half of the free energy driving the process is stored as interfacial energy). According to Zener’s reasoning this would be the real pearlite growth rate. A consequence of Zener’s assumed proportionality between the observed lamellar spacing and the critical spacing (Eq. (3.3)) is that we should expect a plot of the reciprocal interlamellar spacing versus the driving force to give a straight line. The driving force usually shows good proportionality with the undercooling from the eutectoid temperature and indeed plots of the reciprocal spacing versus undercooling do fall on a straight line describing well the smaller interlamellar spacings that are observed in pearlite formed at lower and lower temperatures (e.g., Figures III.6b and III.8b). In principle, either the interlamellar interfacial energy (σ ) or the proposed proportionality between the observed lamellar spacing and the critical spacing (and therefore the optimization principle) could be extracted from the slope of such plots but unfortunately neither is currently known with sufficient certainty for meaningful conclusions to be drawn. Certainly, reliable theoretical calculations of the interlamellar interfacial energy could shed some valuable light on the question of optimization principles. The first treatment applicable to discontinuous precipitation appeared in 1955 by Turnbull48 who was interested in interpreting his growth kinetic results for a Pb-Sn alloy.67 Turnbull first used Zener’s treatment for the pearlite transformation with boundary conditions for the diffusion problem appropriate for discontinuous precipitation and found that his kinetics was around eight orders of magnitude faster that those calculated assuming volume diffusion of Sn. Turnbull subsequently modified Zener’s treatment by assuming that the diffusion path for the solute was the transformation interface itself (Figure III.4) instead of volume diffusion in the parent phase as assumed by Zener for the pearlite transformation. He neglected the effect of surface energy and made some approximations in his evaluation of the net driving force for diffusion and obtained an expression for the pattern growth rate in discontinuous precipitation:

α/β D i δ X bulk − Xe , (3.5) ν= α 2 (λ ) X bulk X bulk is the initial composition of the supersaturated parent phase, D i is the solute diffusivity within the reaction interface and δ is the width of the interface itself. 67 D. Turnbull and H. N. Treaftis, Acta metall. 3, 43 (1955).

202

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.4. Schematic illustration of the diffusion geometry for lamellar pattern formation under conditions where the solute redistribution occurs by short-circuit diffusion within the migrating interface. α/β

λα is the width of the solute depleted lamella and Xe is the local equilibrium solute concentration in the α at the α/β interface. Turnbull found satisfactory agreement with his experimentally observed growth rates when using an activation energy for grain boundary diffusion that was a little less than half of that for bulk diffusion. This was consistent with the early findings for other metals and has since been found to be typically representative.34,35,68 However, the experimentally observed lamellar spacing was much larger than that predicted using Zener’s maximum growth rate hypothesis. Even though the diffusional treatment of the problem seemed adequate, Zener’s solution to the spacing selection problem did not appear to be satisfactory. Furthermore there was an indication that the discontinuous precipitation reaction resulted in an incomplete relief of the supersaturation of the parent phase and therefore the local equilibrium assumption for the boundary conditions of the diffusion problem may not be appropriate. The next steps in the theoretical treatments of lamellar growth came very soon after Turnbull’s treatment and represented major theoretical advances that put the diffusion problem on a much sounder mathematical basis. Hillert49 was the first 68 P. Zieba and W. Gust, Interface Sci. 10, 27 (2002).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 203

to present his treatment which was developed with the pearlite transformation in mind, again assuming that the C redistribution occurred only through the γ . He realized that in solving the diffusion problem all the carbon concentrations in the austenite should be considered and not only the compositions at the γ /α and γ /Fe3 C interface (Figure III.3) as was done in Zener’s approximate treatment. Hillert, building on the work of Brandt45 and Scheil46 obtained a Fourier series expression for the C diffusion field in the γ as a solution to the steady state twodimensional carbon diffusion equation. He included the effect of capillarity from the curved γ /pearlite transformation interface but to apply the boundary condition at the interface and solve for the unknown Fourier coefficients in the C field expression required knowledge of the shape of the transformation interface which was, a priori, unknown. By assuming a relatively flat interface and mechanical equilibrium at the γ /α/Fe3 C triple junction (Figure III.3), Hillert was able to obtain an analytic growth rate expression which turned out to be very similar to the approximate expression obtained by Zener (Eq. (3.4)): ν=

γ /α γ /Fe C λc π 3 D γ f α f Fe3 C Xe − Xe 3 1 1 − , b λ λ X Fe3 C − X α

(3.6)

b is a constant that depends on the ratio of the lamellar widths and typically has a value ∼ 0.5. Furthermore, Hillert’s treatment allowed for a detailed calculation of the interphase boundary shape. This had previously only been calculated by Brandt.45 To solve the spacing selection problem, Hillert, like Zener, assumed a maximum growth rate hypothesis. Soon after Hillert’s treatment, Cahn50 provided a general treatment for lamellar growth applicable to both pearlite and discontinuous transformations under conditions where it was assumed that the solute redistribution occurs solely by shortcircuit diffusion in the migrating interface (Figure III.4). Turnbull’s experiments in the Pb-Sn system67 had provided an indication that during the discontinuous precipitation reactions, the solute redistribution between the growing phases was incomplete and a non-negligible supersaturation remained in the matrix lamellar phase. With this in mind, Cahn wrote his differential equation for grain boundary interface solute transport but solved it under conditions where the composition of the product phases could vary across the lamellar (i.e., perpendicular to the growth direction). Cahn realized that equilibrium could not be maintained at the moving curved interface and that this resulted in non-equilibrium solute partitioning between the product phases. He solved his steady state diffusion problem and obtained an expression for the solute concentration profile within the solute depleted lamellae as a function of the growth rate, v, the interlamellar spacing, λ,

204

Y. BRÉCHET AND C. HUTCHINSON

and the solute transport properties of the interface (Figure III.4): √

y α X bulk − X α (y) cosh λα √ = X bulk − X α/β cosh 2α

where α =

kvλ2 , Di δ

(3.7)

X(y) is the solute content in the solute depleted α lamellae behind the migrating interface as a function of position, X α/β is the solute concentration in the α at the α/β interlamellar interface which is usually taken as the equilibrium value from the phase diagram, D i is the solute diffusivity in the migrating boundary, δ is the boundary width and k is a proportionality constant that relates the concentration in the thin slab of interface, X i , to the solute concentration inherited by the product phase, X α . Cahn assumed that the interface velocity was simply proportional to the net Helmholtz energy change across the interface, F , which can be calculated from a knowledge of the system thermodynamics, the solute profiles retained within the lamella and the interfacial energy of the interlamellar interfaces: ν = MF,

(3.8)

M is a macroscopic kinetic parameter (friction) which is a measure of the response of the interface to the applied driving force. Again, Cahn adopted an optimization principle (optimal rate of free energy dissipation) to remove the degeneracy of the problem and select a velocity/spacing pair. Cahn’s derivation of the solute profile left behind the migrating interface is applicable to both pearlite and discontinuous precipitation products. However, by nature of the system thermodynamics, the composition gradients which can be sustained in pearlite, and still result in a net free energy decrease during growth, are very limited. In contrast, in the discontinuous reaction, the ranges of available compositions allowed for a supersaturated solution are much wider. The difference is shown in Figure III.5. In the top figure the free energy curves for the precipitation reaction are shown. For a bulk alloy composition X0 , the chemical part of the free energy will decrease in a precipitating system as long as the precipitate, β, forms with a composition greater than X , regardless of how little precipitates and therefore how little the α phase changes composition. For the eutectoid composition shown below, the new α and β phases cannot take compositions anywhere near the original γ matrix composition. Segregation to at least Xα and Xβ is necessary to give a decrease in the free energy of the system. The exact solution for the solute diffusion profile between two lamellae provided by Cahn’s approach proved to be both theoreti-

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 205

F IG . III.5. Schematic free energy curves for (a) precipitating and (b) eutectoid systems.50

cally important, and possible to test experimentally by local chemical analysis, in discontinuous reaction products, e.g., see Refs. [69–73]. Hillert criticized Cahn’s treatment because it did not consider the force actually pulling the grain boundary in the first place and therefore did not really explain how discontinuous precipitation occurs. In addition, Cahn prescribed a flat interface, whereas, in principle, not only the spacing between lamellae, but also the shape of the moving grain boundary should be part of the solution of the problem. Hillert57,60,64 then provided treatments for the pearlite and discontinuous transformations under conditions where the solute redistribution was restricted to the 69 D. A. Porter and J. W. Edington, Proc. Roy. Soc. London A 358, 335 (1977). 70 P. Zieba and W. Gust, Int. Mat. Rev. 43, 70 (1998). 71 P. Zieba and W. Gust, Mikrochimica Acta 132, 295 (2000). 72 P. Zieba and W. Gust, Z. Metallkd. 92, 645 (2001). 73 P. Zieba Mat. Chem. and Phys. 62, 183 (2000).

206

Y. BRÉCHET AND C. HUTCHINSON

transformation interface, by considering the necessary diffusion and a detailed balance of surface tensions across the interface during growth. The treatments of Cahn and Hillert can respectively be characterized as ‘global’ and ‘detailed’ in the sense that, in Cahn’s treatment the interface is a high diffusivity reaction path and its mobility controls the rate at which the interface moves in response to the existing driving force; whilst in Hillert’s treatments of lamellar growth, detailed knowledge of the interface and its properties is often necessary for application of the growth rate expressions. The theoretical treatments of Hillert and Cahn, made in the 1950s and 1960s, remain to this day the treatments used most frequently. Since this time, contributions to the theory of lamellar growth have concentrated on extending these original treatments to include such effects as: ternary solute additions,58,59 non-uniformity in the compositions of the lamella phases in pearlite,62 coherency stresses60 and resolution of the spacing selection problem.61,66,74

b. Experimental Observations Many aspects of the theoretical treatments discussed above can be compared with experimental data. These include metallographic measurements of lamellar growth rates and interlamellar spacings and more recently, analytical electron microscopy measurements of the solute concentrations inherited by the growing phases. For both the pearlite transformation and the discontinuous precipitation reaction, much of the experimental data has been collected and compared with the theoretical predictions in periodical reviews of the subject (pearlite: see Refs. [61, 75,76]; discontinuous precipitation: see Refs. [36–38]). Here we present a couple of selected examples to illustrate the types of comparisons that are usually made. Pearlite. Traditionally, researchers have been interested in describing both the growth rate and the repeat distance of the evolving pattern. These are the two quantities that are experimentally measured. The growth rates are usually calculated from a representative width of the pearlite colonies in a series of isothermally transformed specimens and the results are then compared with the predictions of one of the models discussed above. The first example is taken from the Cu-Al system. The transformation rate in a Cu-12Al (wt.%) alloy has been measured by several authors27–29 and the experimental growth rates and interlamellar spacings as a function of temperature are shown in Figure III.6. 74 J. S.Kirkaldy, Phys. Rev. B 30, 6889 (1984). 75 R. F. Mehl and W. C. Hagel, Prog. Met. Phys. 6, 74 (1956). 76 J. W. Cahn, in Decomposition of Austenite by Diffusional Processes, eds. V. F. Zackay and H. I. Aaronson, Interscience, New York (1962), p. 131.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 207

F IG . III.6. Experimentally measured (a) pearlite growth rates and (b) interlamellar spacings in a Cu-11.8Al (wt.%) alloy as a function of temperature.29 .

For the data shown, Cheetham and Ridley29 then applied Hillert’s volume diffusion growth rate equation (Eq. (3.4)) using the experimentally observed interlamellar spacings to examine the agreement between theory and observation. To

208

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.7. Comparison of the growth rate data in Figure III.6a with the theoretical predictions calculated assuming local equilibrium interfacial compositions, volume diffusion of the components and using the experimentally observed interlamellar spacings.29 The results using both the maximum growth rate hypothesis of Zener47 and the optimal rate of entropy production of Kirkaldy61 are shown.

make the comparison, a choice must be made concerning the relationship between the observed lamellar spacing and the critical spacing. The calculated results using both Zener’s maximum growth rate hypothesis (λ = 2λc ) and Kirkaldy’s maximum rate of entropy production (λ = 3λc ) are compared with the experimental results in Figure III.7. The agreement in both cases is considered to be quite good. On the basis of such comparisons it is now fairly well accepted that the solute redistribution in this reaction occurs predominantly by volume diffusion in the parent phase ahead of the interface but considering the uncertainty in experimental measurements and the thermodynamic and kinetic quantities entering into Eq. (3.4), solid conclusions cannot be drawn concerning the operative optimization principle. The second example concerns the pearlite reaction in binary Fe-C steels. There has been much discussion in the literature concerning the diffusion path for C in this reaction.47,49,50,54,57,76 During the 50s, 60s and 70s when much of the experimental work was carried out, the accuracy with which the relevant thermodynamic and kinetic data was known was insufficient to draw any solid conclusions about the C diffusion path through comparisons with theory. Nevertheless, many authors had tentatively suggested that the experimental growth rates appear to be at least an order of magnitude faster than those predicted by the volume diffusion con-

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 209

F IG . III.8. Experimentally observed pearlite (a) growth rates and (b) interlamellar spacings in a series of binary Fe-C alloys as a function of temperature. The theoretical predictions assuming local equilibrium interfacial conditions, a maximum growth rate hypothesis and both volume diffusion control and boundary diffusion control are shown in (a). The volume diffusion controlled kinetics is approximately an order of magnitude slower than the experimental observations. The boundary diffusion controlled kinetics was calculated using a sD i δ triple product with an activation energy ∼ 0.5 of that for bulk C diffusion. (Continued on next page.)

trolled models.47,49,54,76 Today, our knowledge of the relevant thermodynamic and kinetic parameters is much better and we have carried out a new series of calculations using the existing data to shed some light on this issue. The experimentally measured growth rates77–79 and interlamellar spacings79 are shown in Figure III.8. The theoretical prediction using the experimental lamellar spacings and assuming both volume diffusion of C and Zener’s maximum growth rate hypothesis is also shown. It is clear that the kinetics are indeed at least an order of magnitude slower than the experimental values, suggesting a diffusion path for C other than the parent γ phase must be contributing to solute redistribution. Hillert49 77 F. C. Hull, R. A. Colten, and R. F. Mehl, Trans. AIME 150, 185 (1942). 78 J. H. Frye, E. E. Stansbury, and D. L. McElroy, Trans. AIME 197, 219 (1953). 79 D. Brown and N. Ridley, J. Iron and Steel Inst. 204, 811 (1966).

210

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.8. (Continued.)

and Cahn76 have discussed the possibility of different diffusion paths for the C and it now seems the most likely candidate is the moving interphase boundary itself (as is the case for the discontinuous precipitation reaction). The theoretical treatments of growth according to this diffusion path have also been made but the problem lies in the lack of knowledge of the thermodynamic and kinetic quantities of the moving boundary region. Hillert’s57 expression for the growth rate of pearlite according to boundary diffusion control is:

γ /α

γ /Fe C 12sD i δ Xe − Xe 3 λc 1 ν = α Fe C . (3.9) 1 − λ f f 3 X Fe3 C − X α λ2 Our problem is that neither D i , δ or s are known with any certainty. Instead, what is usually done, is to extract an effective triple product, sD i δ, from the experimental results using one of the models for growth and then to make a judgment about whether this seems reasonable for boundary diffusion control. If so, it is then usually concluded that the diffusion path for the solute is probably the moving boundary. We have made such calculations and find that using a segregation coefficient (s) of 1 and a grain boundary width (δ) of 0.5 nm, the experimental data can be adequately described by assuming Zener’s maximum growth rate hypothesis (λ = 3λc /2 in the case of boundary diffusion control) with an activation

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 211

energy for boundary diffusion of C that is approximately 0.7 of that for C diffusion in the bulk (Figure III.8a). In the case of substitutional elements diffusing in migrating interfaces, experimental measurements have found that the activation energy for diffusion is indeed approximately 0.5–0.7 of the corresponding value in the bulk.34,35,68 Whether the same should be true for C which diffuses interstitially in the bulk it is not clear. Nevertheless, this example illustrates the difficulty encountered in making any solid conclusions about the transformation when considerable uncertainty exists in the knowledge of either the optimization principle or the interlamellar interfacial energy and the relevant thermodynamic and kinetic data for the migrating boundary region. Kaur et al.80 have compiled a large set of interphase boundary diffusion data for those systems that have been experimentally examined and as we shall see in the next section, much of this data is obtained through back calculation from the results obtained in discontinuous precipitation reactions. During the last 20 years, it has become possible to use advanced electron microscopy techniques to directly measure solute concentrations in the vicinity of the transformation interface. Indeed, the state of the art instruments today are capable of making measurements in the sub-nm range. This would be an ideal, direct way of identifying the solute diffusion path in these reactions. This has been done for several cases and it has recently been shown that for the pearlite formed in Fe-C-Mn alloys,81 the diffusion path for the redistributing substitutional Mn element is the reaction interface itself and volume diffusion of Mn plays little role in the reaction. However, because of the very low C contents that are encountered in eutectoid steels and the contamination of the surface of the thin-foil samples for electron microscopy during preparation, it is currently not possible to measure with sufficient accuracy the C concentrations in these specimens. In this respect, progress in our understanding of some of the fundamental aspects of the pearlite transformation in steels has not been able to take advantage of the technological advances that techniques like analytical electron microscopy have been able to bring to other transformations, such as the discontinuous precipitation reaction to be discussed below. Discontinuous Precipitation. In making comparisons between theory and experiment in the discontinuous precipitation reaction we are not faced with the question of the solute diffusion path. From the earliest theoretical treatments it 80 I. Kaur and W. Gust, Fundamentals of Grain and Interphase Boundary Diffusion, John Wiley &

Sons, New York (1995). 81 C. R. Hutchinson, R. E. Hackenberg, and G. J. Shiflet, Acta mater. 52, 3565 (2004).

212

Y. BRÉCHET AND C. HUTCHINSON

was assumed that the path was the reaction interface itself and this is now experimentally well established. However, the comparisons are complicated by the nonequilibrium segregation of solute at the transformation interface. The solute depleted matrix lamella does retain some level of residual supersaturation. For comparisons between experimentally measured growth rates and interlamellar spacings with theoretical predictions, many of the models proposed require a quantification of this non-equilibrium segregation. Cahn provided an expression describing the solute profile across the lamella behind the transformation interface as a function of the growth rate, the interlamellar spacing, the bulk solute content and the transport properties of the boundary. This is one area where progress in our understanding has benefited from recent advances in analytical electron microscopy. There are now many experimental studies that have directly measured the solute profiles behind the migrating boundary and have found that Cahn’s equation is well obeyed. Many of these studies have recently been summarized in a series of reviews, e.g., Refs. [36,37,72]. An example taken from the work of Duly et al.82 on the discontinuous precipitation reaction in an Mg-18.8Al (at.%)) alloy is shown in Figure III.9. The data shows solute profiles measured at two distances behind the reaction interface and the solid curve is the best-fit (in α and Xα/β , Eq. (3.7)) using Cahn’s equation. From the value of α obtained, and the experimental measurements of the growth rate and interlamellar spacing of the lamellar pattern, values for the sD i δ, triple product can be extracted and a judgment can be made concerning the reasonableness of these values. Clearly, depending on which of the theoretical models for growth is chosen for comparison, different values of this triple product can be obtained. Amir and Gupta83 have nicely presented the possible differences calculated for each of the different models using data for an Mg-7Al (at.%) alloy. They metallographically measured the growth rate and interlamellar spacing as a function of temperature and used X-ray diffraction techniques to estimate the level of nonequilibrium solute segregation, all as a function of temperature. They then extracted the triple products necessary to reproduce the experimental data for each of the different models and compared these. They are shown in Figure III.10. The three most sophisticated models (Cahn,50 Hillert60,64 and Sundquist63 ) all give quite similar activation energies for boundary diffusion, ∼ 70 kJ/mol. The activation energy for chemical diffusion in dilute Mg-Al alloys is reported to be ∼ 143 kJ/mol. The proposed boundary diffusion value is then ∼ 0.5 of that for volume diffusion and is consistent with the findings in other alloys. The extraction of boundary diffusion parameters from the analysis of the discontinuous precipitation reaction has now become one of the prime sources of boundary diffusion data. However, as is clear from Figure III.10, the values obtained depend on the model used to describe the discontinuous reaction. 82 D. Duly, M. C. Cheynet, and Y. Brechet, Acta metall mater. 42, 3843 (1994). 83 Q. M. Amir and S. P. Gupta, Can. Metall. Qrty 34, 43 (1995).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 213

F IG . III.9. Plots of Al composition as a function of position across the solute depleted lamellae at two distances behind the reaction interface; (a) at 380 nm and (b) at 200 nm during discontinuous precipitation in an Mg-18.8Al (at.%) alloy treated at 220 ◦ C for 16 h. The profiles were measured using electron energy loss spectroscopy and a scanning transmission electron microscope.82 In both cases, the profiles are well described by Cahn’s equation (solid line) using the same Xα/β and α values.

8. T HE S PACING S ELECTION P ROBLEM In each of the theoretical treatments of steady state lamellar pattern growth discussed above, a relation between the growth velocity, ν, the interlamellar spacing, λ, and the boundary conditions for the diffusion problem is obtained. After ap-

214

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.10. Extracted triple product (sD i δ) values as a function of 1/T (K−1 ) according to each of the different discontinuous precipitation models for experimental growth rate and interlamellar spacing data from a Mg-7Al (at.%) alloy treated at a variety of temperatures.83

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 215

propriate boundary conditions have been chosen, an additional criterion must still be invoked to decouple the growth velocity, ν, and the interlamellar spacing, λ. This problem of ‘spacing selection’ is the central unanswered question in the formation of lamellar patterns in the solid state. Traditionally a global optimization principle has been invoked. Zener47 and Hillert49 used the maximum growth rate hypothesis, Kirkaldy61 has considered an optimal rate of entropy production and Cahn50 has considered an optimal rate of free energy dissipation. If we consider, for example, the pearlite transformation, according to volume diffusion control, the optimal lamella spacing according to Zener’s maximum growth rate hypothesis and Kirkaldy’s maximum rate of entropy production are λ = 2λc and λ = 3λc . For boundary diffusion controlled growth, the corresponding values are λ = 1.5λc and λ = 2λc . The differences in spacing predicted by the two hypotheses differ only by a small factor. The accuracy with which diffusion coefficients are known does not allow us to differentiate between these two heuristic principles and, as is often the case with these pattern selection problems, the very question of the existence of a selected spacing is still open. Gust et al.84 have carefully measured the interlamellar spacing in selected discontinuous precipitation reactions and found that under isothermal conditions, not a single spacing but a Gaussian distribution of spacings is experimentally observed (Figure III.11). Similar observations were made by Duly et al.85 in their investigations of the discontinuous reaction in Mg-Al alloys. Solorzano and Purdy86 have examined Cahn’s maximum rate of free energy dissipation hypothesis by comparing the theoretical predictions with experimental results from the Mg-Al system. These authors calculated a dissipation function, GNET · ν as a function of interface velocity and interlamellar spacing. They did indeed find a maximum in the dissipation function for a particular velocity and that this maximum was highest for a particular interlamellar spacing. Example calculations for the Mg-9Al (wt.%) alloy at two temperatures are shown in Figure III.12. The numbers on the curves refer to the interlamellar spacings. Given the experimentally observed growth rates and interlamellar spacings and an estimate of the thermodynamic and kinetic properties of the boundary extracted from experimentally measured solute concentration profiles, Solorzano and Purdy estimated the remaining supersaturation in the lamella behind the moving interface and calculated GNET . The observed interlamellar spacings could then be compared with those predicted by a maximum rate of free energy dissipation by identifying the theoretical spacing which gave the highest value in the dissipation function for the 84 W. Gust, B. Predel, and U. Roll, Z. Metallkd. 68, 117 (1977). 85 L. Klinger, Y. Brechet, and D. Duly, Scripta mater. 37, 1237 (1997). 86 I. G. Solorzano and G. R. Purdy, Metall. Trans. A 15A, 1055 (1984).

216

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.11. Experimentally measured distribution of lamellar spacings in a Ni-31.7Zn (at.%) alloy treated for 24 h at 600 ◦ C.84 The distribution is well described as Gaussian.

experimentally observed velocity. It was found that from the myriad of possible kinetic states, the velocity/spacing pair selected were within a factor of ∼ 2 of that which would give a maximum in the rate of free energy dissipation. Considering the uncertainties in the thermodynamic quantities, in particular interfacial energies, the agreement was deemed encouraging.

a. Klinger’s Alternative for Discontinuous Precipitation Only recently, an alternative treatment of the diffusion problem for the discontinuous precipitation reaction has been supplied by Klinger et al.66 which provides a unique velocity/spacing pair and for which an additional ‘optimization’ criteria is not necessary. Klinger et al. realized that the degeneracy of the problem could be removed by invoking an additional local condition in the derivation rather than imposing an optimization principle on a relation between the interface velocity and the lamella spacing. The conditions imposed were all local in nature and relied on thermodynamic assumptions of local equilibrium, which may be arguable, but are at least clearly stated. The starting point of the approach is that both the α and the β lamellae must grow at the same rate, and that both these rates are diffusion controlled. The thermodynamic difference between the α0 /α interface and the α0 /β interfaces, which parallels the previously stated difference between

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 217

F IG . III.12. Computed variation of the dissipation function, (GNET .ν), as a function of discontinuous precipitation cell velocity in an Mg-9Al (wt.%) alloy. The calculations are performed at (a) 485 K and (b) 550 K for a range of interlamellar spacings (labelled).86

218

Y. BRÉCHET AND C. HUTCHINSON

pearlite and discontinuous precipitation, requires different treatments for the diffusion problem. In previous treatments of the reaction, the solute diffusion from the solute poor lamella to the solute rich lamellae was assumed to occur within the α/α0 grain boundary and was driven by concentration gradients. The nature of the β/α0 interface and the driving force for solute diffusion within this interface was not usually considered. Klinger et al. treated the growth of the α and β phases simultaneously, subject to conditions of equal growth velocities, but assumed that the diffusion in the α/α0 grain boundary was driven by concentration gradients and diffusion within the β/α0 interface boundary was driven by gradients in curvature. Such an assumption for the β/α0 interface boundary is physically based since the compound phase in discontinuous precipitation is very often a stoichiometric phase which offers very little range for concentration gradients. The treatment of the grain boundary followed the classical treatments of Cahn50 and Hillert57 and that of the interphase boundary followed the treatment of Mullins.87 An assumption of local equilibrium and diffusional flux continuity at the α/β/α0 triple junction was sufficient to remove the degeneracy of the problem and select a unique velocity/spacing pair. Klinger et al. compared their treatment with the available experimental data in the Al-Zn system and found good agreement using reasonable values of the unknown parameters. Klinger’s approach can be seen as an idealized, but tractable version of the problem. Each of the assumptions made can be relaxed through a more sophisticated treatment: local equilibrium assumptions can be modified to account for attachment kinetics, the thermodynamic model for the solid solution can be made more realistic, the shape of the moving interface can be left free: however, the solution is no longer analytic and numerical calculations are needed which show a rich variety of behavior. The important issue is that the intrinsic degeneracy of the spacing selection problem can be relieved by local assumptions and does not require the introduction of an additional optimization principle. 9. N ON -S TEADY S TATE G ROWTH In each of the theoretical treatments of growth discussed above, it is assumed that the lamellar pattern formed under steady state conditions of constant interlamellar spacing and growth rate. There are at least two sets of circumstances where the steady state hypothesis has been called into question and each will be briefly discussed. The first concerns the recent suggestions that growth is not a continuous process with a constant rate but rather a ‘stop and go’ process and as a result, the average growth rate, determined for example from metallographic measurements, 87 W. W. Mullins, J. Appl. Phys. 28, 333 (1957).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 219

must be differentiated from the instantaneous growth rate. The second case concerns the formation of so-called divergent lamellar aggregates. Observations of isothermal lamellar growth with a rate that decreases in time and an interlamellar spacing that increases in time have been observed in both the pearlite and discontinuous precipitation reactions and the theory is qualitatively well understood.

a. ‘Stop and Go’ Interface Motion On the basis of preliminary in-situ high voltage electron microscopy studies of the discontinuous precipitation reaction in an Al-Zn alloy, Bogel and Gust65 proposed that the reaction interface does not migrate in a continuous manner with a constant velocity but rather by a ‘stop and go’ process. Subsequent electron microscopy studies88 showed that this was observed experimentally and the plot of interface displacement versus time in Figure III.13 clearly shows the start-stop nature of the interface.

F IG . III.13. Interface migration distance as a function of time during discontinuous precipitation in an Al-15Zn (at.%) alloy transformed at 160 ◦ C.88 The measurements were made during the in-situ elevated temperature high-voltage electron microscopy observations. The stop-start nature of the interface migration is clearly shown in the plot. 88 S. Abdou, G. Solorzano, M. ElBoragy, W. Gust, and B. Predel, Scripta mater. 34, 1431 (1996).

220

Y. BRÉCHET AND C. HUTCHINSON

Bogel and Gust claim that the difference between the instantaneous interface velocity and the average value can be up to three orders of magnitude. Further indirect experimental evidence in support of the ‘stop and go’ motion was collected in Duly’s studies of the discontinuous precipitation reaction in the Mg-Al system.85 They found, as with previous investigators, that within a given lamellar colony, a range of lamella spacings is observed. When the solute profiles within the lamellae behind the reaction interface were measured, they could be fitted to Cahn’s equation (Eq. (3.7)) using an approximately constant α parameter. If cooperative motion does occur in a continuous and constant manner, then everywhere along a reaction front where the lamellar spacing changes, so too should the α parameter necessary to describe the solute profile left behind. For lamellar spacings that range from S/2 to 2S, we should expect to see a variation in the α parameter of a/4 to 4a, a factor of 16. Klinger et al.85 reinterpreted the observed chemical profiles in terms of a ‘stop and go’ motion of the interface and found that the approximately constant α parameter across a lamellar colony with varying lamellar spacing could be rationalized assuming the non-steady state type of growth proposed by Bogel and Gust.65

b. Divergent Lamellar Growth The second case of non-steady state lamella growth worth considering is the formation of aggregates with diverging lamellae. The lamellar product of eutectoid decomposition or discontinuous precipitation usually inherits the same overall composition as the parent phase and therefore it is assumed that a constant (average) growth prevails. Indeed, this is experimentally confirmed in most cases. However, if for some reason the growing aggregate is constrained to inherit a composition different from that of the parent phase then long range solute diffusion is necessary between the growing lamellar aggregate and the parent phase and growth with a constant rate cannot prevail. Non-steady state growth of both pearlite and discontinuous precipitation is possible and both have been observed. These observations are restricted to multi-component systems and the examples considered below are each taken from Fe-based systems containing both a substitutional and interstitial solute. We first consider non-steady state growth of pearlite, using the Fe-C-Mn system as an example before examining a counterpart discontinuous precipitation reaction found in high N austenitic stainless steels. Pearlite. Under conditions of constant temperature and pressure, the three phase equilibrium between the γ , α, and Fe3 C in the binary Fe-C system occurs at a single ‘eutectoid’ temperature (Figure III.1b). At temperatures below the eutectoid, the γ phase is unstable and the growing (α + Fe3 C) pearlitic aggregate consumes 100% of the parent γ phase and therefore is obliged to inherit the bulk

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 221

composition. However, in multi-component systems, the three phase equilibrium between the γ , α and M3 C (M = Fe + X), exists over a temperature range and a (γ + α + M3 C) three phase field is observed. It is within this (γ + α + M3 C) three phase field that non-steady state pearlite formation can occur. Two sections of the ternary Fe-C-Mn phase diagram are shown in Figure III.14.

F IG . III.14. (a) Isoplethal section of the Fe-C-Mn system sectioned at 5.42 (wt.%) Mn. The (γ + α + M3 C) three phase field is clearly labelled. (b) Fe-rich corner of an isothermal section of the Fe-C-Mn phase diagram sectioned at 625 ◦ C. Two alloy compositions are labelled. Alloy A lies within the (γ + α + M3 C) three phase field and Alloy B, within the (α + M3 C) two phase field.

222

Y. BRÉCHET AND C. HUTCHINSON

The isopleth shown in (a) is taken at a constant Mn content of 5.4 (wt.%) and the isotherm shown in (b) corresponds to a temperature of 625 ◦ C. In both diagrams the (γ + α + M3 C) three phase field is clearly labelled. For an alloy with the composition labelled A in Figure III.14b, the equilibrium compositions of the three phases correspond to the three corners of the three phase tie-triangle (bold). It is clear that for equilibrium to be achieved, significant Mn redistribution must occur from the α to the M3 C, and to a lesser degree to the γ and substantial C redistribution must occur from the α to the M3 C and a smaller redistribution from the γ to the growing lamellar aggregate. The case of Fe-C-Mn is a little more complicated because C diffusion in γ occurs 106 times faster than Mn at these temperatures and, in practice, the growing pearlite colony does inherit the bulk Mn content of the austenite (there is no long range Mn diffusion to or from the γ ). The Mn redistribution from the α to the M3 C occurs via short circuit diffusion in the reaction interface. Nevertheless, the short circuit Mn redistribution is still much slower than the significant long range C diffusion which must occur from the γ to the growing pearlite aggregate in addition to the short range C redistribution from the α to the M3 C, and the lamellar aggregate grows into what it sees to be a parent phase with a C content that decreases in time. As a result, the local equilibrium interfacial compositions (the boundary conditions of the diffusion problem) at the pearlite/γ interface change in time. The consequence is that the compositions inherited by both phases in the lamellar aggregate also continually changes in time and growth occurs with a rate that decreases in time and an interlamellar spacing that increases in time. The effect was first observed by Cahn and Hagel in 196276 and has since been observed in Fe-C-Si89 and Fe-C-Mo90 systems and has been discussed in detail by Hillert.91 If instead, an alloy composition such as B in Figure III.14b is chosen, which lies within the (α + M3 C) two phase field

F IG . III.15. (a) Optical micrograph of ‘divergent pearlite’ formed in an Fe-0.55C-5.42Mn (wt.%) alloy transformed for 384 h at 625 ◦ C. The M3 C phase contrast is dark and the α phase is light. The alloy composition is marked, A, in the Fe-C-Mn isothermal section (Figure III.14b). Pearlite growth for compositions lying within the (γ + α + M3 C) three phase field occurs with an interlamellar spacing that increases in time and a growth rate that decreases in time. (b) Scanning electron microscopy secondary electron image of a section of a pearlite colony in an Fe-0.54C-3.51Mn (wt.%) alloy treated at 625 ◦ C for 5 h. In this case, the M3 C phase contrast is light and the α phase is dark. The alloy composition, B, lies within the (α + M3 C) two phase field as marked in the isothermal section (Figure III.14b). For such alloy compositions, growth occurs with an approximately constant interlamellar spacing and rate. 89 J. Fridberg and M. Hillert, Acta metall. 18, 1253 (1970). 90 J. Fridberg and M. Hillert, Acta metall. 25, 19 (1977). 91 M. Hillert, in Solid Solid Phase Transformations, eds. H. I. Aaronson, D. E. Laughlin, R. F. Sekerka,

and C. M. Wayman, AIME (1981), p. 789.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 223

224

Y. BRÉCHET AND C. HUTCHINSON

of the phase diagram, γ is not stable, and as was the case for the binary Fe-C system, the growing pearlite is obliged to inherit the bulk alloy composition and steady state growth can be established. The Fe-C-Mn system has recently been analyzed in detail81 and micrographs of the pearlite formed in alloys A and B (Figure III.14b) and measurements of their growth rates at 625 ◦ C are shown in Figures III.15 and III.16, respectively. The divergency of the lamellar spacing of alloy A (Figure III.15a) and a growth rate which decreases in time (Figure III.16) are clearly contrasted with the steady state conditions which prevail for Alloy B (Figure III.15b). Discontinuous Precipitation. As was the case for the non-steady state pearlite growth described above, the occurrence of non-steady state discontinuous precipitation arises from conditions that result in the growing aggregate inheriting an overall composition different from the bulk parent phase (i.e., long range diffusion to or from the parent phase is necessary in addition to the short range redistribution between the lamella phases). The most thoroughly studied case

F IG . III.16. Experimentally measured pearlite growth rates as a function of time at 625 ◦ C in the alloy compositions marked A and B in the Fe-C-Mn isothermal section in Figure III.14b. Alloy A, located within the (γ + α + M3 C) three phase field forms with a growth rate that decreases in time. Alloy B, located within the (α + M3 C) two phase field, forms with an approximately constant growth rate.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 225

is the precipitation of Cr2 N in some Cr-Ni austenitic stainless steels. In a series of studies, Kikuchi92–94 examined the discontinuous precipitation of Cr2 N in several Fe-20Ni-25Cr (wt.%) alloys with varying N contents and measured the growth rates and interlamellar spacings at several temperatures. These are shown for a series of alloys treated at 1073 K in Figure III.17. For a given alloy, the isothermal growth rate of the lamellar aggregate can change by 4 orders of magnitude and the interlamellar spacing can increase four fold during the reaction. Using arguments based on Hillert’s theoretical discussion of the formation of divergent pearlite,91 Kikuchi et al.94 argues that for the alloys examined, under conditions where no long range diffusion of Ni or Cr occurs between the parent γ and the growing lamellar aggregate, to maintain local equilibrium between the lamellar phases, long range diffusion of N from the parent γ phase to the aggregate is necessary. Kikuchi et al.93,94 have shown experimentally that indeed no bulk diffusion of the substitutional solutes is observed for most of the reaction time and that the N content of the parent phase does decrease with time. As a result of the long range N diffusion, the lamellar aggregate grows into a parent phase whose composition is continually changing. The consequence is a continuous change in both the interfacial conditions at the moving boundary and the compositions inherited by the growing phases and results in lamellar aggregate growth with a velocity that decreases in time and an interlamellar spacing that increases in time. 10. C OARSENING AND R ELATED M ORPHOLOGICAL E VOLUTION The lamellar patterns arising from eutectoid decomposition and discontinuous precipitation are highly non-equilibrium structures. In both cases, energy is stored in the form of the interlamellar interfaces. In the case of the pearlite transformation, the compositions of the phases formed are usually relatively close to the equilibrium compositions found from the phase diagram and little chemical supersaturation generally exists (Figure III.5). However, the solute depleted lamellar phase in the discontinuous reaction necessarily retains some level of supersaturation and the non-equilibrium nature of this product is due to both the free energy stored in the interfaces and the residual chemical supersaturation. The relative contribution to the driving force from the chemical and surface terms will be system specific 92 M. Kajihara, S. Choi, M. Kikuchi, R. Tanaka, Y. Seo, T. Okumura, and Y. Kondoh, Z. Metallkd. 77, 515 (1986). 93 M. Kikuchi, T. Urabe, G. Cliff, and G. W. Lorimer, Acta metall. 38, 1115 (1990). 94 M. Kikuchi, M. Kajihara, and S. Choi, Mat. Sci. and Eng. A 146, 131 (1991).

226

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.17. (a) Experimentally measured discontinuous precipitation growth rates in a series of N containing Fe-25Cr-20Ni (wt.%) alloys transformed at 800 ◦ C.94 The growth rate decreases during growth. (b) Corresponding interlamellar spacings showing an increase in spacing during growth.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 227

and depend on the primary transformation conditions, but in most cases it is expected that the volumetric chemical term will dominate the surface term. Fournelle95 has estimated the magnitudes of the two contributions to the driving force for coarsening in a Fe-30Ni-6Ti (wt.%) alloy and found that for his conditions, the chemical term was two orders of magnitude larger than the surface term. For both types of lamellar products, the available stored energy provides a driving force for coarsening processes. The return towards equilibrium can take on two aspects: (a) the decrease in interfacial energy and (b) additionally for the discontinuous precipitation product, a decrease in the remaining supersaturation. The decrease in interface energy has obvious consequences in terms of the morphology and scale of the product phases. Just as is the case for precipitation, it can occur either continuously, or discontinuously through the migration of an interface.

a. Spheroidization The reduction in total interface area can be obtained at almost constant scale through a shape change. Since Lord Rayleigh’s96 seminal work on the stability of fluid jets, it is known that a cylinder can reduce its surface area by a continuous growth of perturbations towards the production of a series of spheres: this process is spontaneous (i.e., there is no energy barrier to be overcome) and is called ‘spheroidization’. The equivalent in the solid state has been analyzed by Nicols and Mullins.97 By contrast, a perfect lamellar structure of infinite extent is stable with respect to infinitesimal fluctuations (although the sphere of equivalent volume has an obvious advantage in terms of reduced surface energy). However, real lamellar structures are not perfect: the lamellae contain both boundaries and defects. The morphological instabilities of lamellar structures are bound to initiate at boundaries and defects and several different types of instabilities leading to spheroidization have been observed. Werner98 has recently reviewed these processes. By nature of the difference in interface curvature, a driving force exists for solute transport from the edge of a lamella plate to the flat face of the plate. This solute transport in itself can lead to the direct cylinderization of a plate, and the cylinder is then unstable with respect to the type of perturbations discussed by Lord Raleigh, giving rise to the formation of an aligned row of spheres, Figure III.18a.99 95 R. A. Fournelle, Acta metall. 27, 1147 (1979). 96 Lord Rayleigh, Proc. Lon. Math. Soc. 10, 4 (1879). 97 F. A. Nichols and W. W. Mullins, Trans. AIME 233, 1840 (1965). 98 E. Werner, Z. Metallkd. 81, 790 (1990). 99 T. H. Courtney and J. C. M. Kampe, Acta metall. 37, 1747 (1989).

228

Y. BRÉCHET AND C. HUTCHINSON

F IG . III.18. Schematic illustration of the primary instability modes for an isolated plate.99 (a) A terminated plate may evolve into a cylinder as a result of capillarity driven mass transfer from the edges to the broad faces of the plate. Following ‘cylinderization’, a Raleigh instability causes the cylinder to decompose into a row of spheres. (b) The shape evolution gives rise to the pinching-off of a row of spheres along the edges of the plate (edge spheroidization). The spheres form as a result of perturbations developed along the ridge which forms at the edges during the first stages of mass transfer to the broad faces. (c) If boundaries are present in the plate, plate splitting may occur by sustained mass transport from boundary grooves to the broad face of the plate. Cylinderization and Raleigh instabilities can then follow.

Alternatively, part way through the cylinderization process of a plate, ridges may form along the edges and the partial cylinders at the edge of the plate may then decompose to rows of spheres directly on either side of the plate through the Raleigh instability. This process is shown schematically in Figure III.18b and is usually referred to as ‘edge spheroidization’. Both of these processes lead to a change in shape at approximately the same scale and arise naturally from the solute transfer driven from the curved boundaries of plates to the flat faces. Clearly, the boundaries from which transport occurs could equally be holes in the plates themselves rather than external edges. Lamella plates also often contain boundaries. These can be the result of faulting during growth, or boundaries formed during recovery and recrystallization. In either case, these boundaries can also act as sites for the splitting of plates through a ‘boundary grooving’ mechanism which has been discussed in detail by Mullins.87,100,101 The curvature of the 100 W. W. Mullins, Acta metall. 6, 414 (1958). 101 W. W. Mullins, Trans. AIME 218, 354 (1960).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 229

F IG . III.19. Schematic illustration of ‘fault migration’ during coarsening of lamellar structures.102 (a) Initial geometry, (b) migration of the faults and (c) bulged plate. The driving force for mass transfer is the difference in curvature at the termination and the branch.

surface of the plate in the vicinity of the boundary can be sufficient to drive solute away from the boundary region. To maintain the balance of surface tensions at the triple point between the boundary and the interlamellar interface, in the presence of solute transfer, the groove continually deepens along the boundary until it is entirely removed and the plate is split in two. This process is shown schematically in Figure III.18c. Each of the instabilities shown in Figure III.18 involves the splitting of individual plates; it is a change is shape at approximately the same scale and we shall refer to them all under the umbrella of spheroidization. The reduction in surface energy can also be obtained by increasing the scale of the microstructure. This increase in scale requires diffusional mass transport and the standard means is by bulk diffusion. This is the process of Oswald ripening which has been extensively studied, both experimentally and theoretically, and has been excellently reviewed many times (e.g., see Ref. [103]). An additional mechanism for accomplishing the change in scale involves the interactions between adjacent plates and is referred to as fault migration.102 In this case, the difference in curvature at the end of a terminated plate and on the broad face of an adjacent plate drives the dissolution of the faulted plate and the 102 H. E. Cline, Acta metall. 19, 481 (1971). 103 P. W. Voorhees, Ann. Rev. Mat. Sci. 22, 197 (1992).

230

Y. BRÉCHET AND C. HUTCHINSON

thickening of the adjacent plate by volume diffusion of the atomic species until the faulted region is entirely removed (Figure III.19). As we shall see below, when volume diffusion of solute is too slow, an alternative mechanism can take over.

b. Discontinuous Coarsening When bulk diffusion is too slow, the change in scale can be accomplished through discontinuous coarsening. This is a solution involving interface migration and interface diffusion and can take over from continuous coarsening (Ostwald ripening), just as discontinuous precipitation can take over from continuous precipitation in similar situations. Discontinuous coarsening is a moving boundary reaction that converts a fine lamellar pattern into a structurally and morphologically similar, but distinctly coarser pattern. As is the case for the very similar discontinuous precipitation, the solute redistribution during the discontinuous coarsening reaction occurs via short circuit diffusion in the migrating boundary and a discontinuous change in crystal orientation is observed across the boundary. Coarsening by this mode has been observed for lamellar products of both discontinuous precipitation and eutectoid decomposition and Manna et al.36 reports that it has been identified in more than 30 different alloy systems. A classic example104 of the discontinuous coarsening of a eutectoid lamellar aggregate in the Co-Si system is shown in Figure III.20. The kinetics of the coarsening process were first treated theoretically by Livingston and Cahn104 who were interested in the thermal stability of Co-Si, Cu-In and Ni-In aligned eutectoids. They were able to derive an expression for the velocity of the interface based on a solution to the diffusion equation and considering the change in interlamellar spacing, λ.

λOR sδD b σ Vm 8X β νDC = β , (3.10) 1 − X − X e fα2 fβ2 λ2DC λOR RT λDC X β is the equilibrium composition of the β phase, λOR is the lamellar spacing of the initial pattern and λDC is the spacing of the coarsened pattern. Livingston and Cahn were considering the coarsening of eutectoid products. They assumed that the driving force in this case arises mostly from a reduction in the interfacial energy stored in the interlamellar interfaces. However, for discontinuous coarsening of discontinuously precipitated lamellar aggregates the driving force for the coarsening process must include the contribution from the chemical 104 J. D. Livingston and J. W. Cahn, Acta metall. 22, 495 (1974).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 231

F IG . III.20. An optical micrograph of the discontinuous coarsening reaction in a Co-Si alloy treated for 4 days at 1000 ◦ C.104 The direction of grain boundary motion is indicated by the arrows.

supersaturation remaining in the aggregate. Fournelle,95 modified a previous treatment for discontinuous precipitation,56 and derived an expression for the coarsening rate that allows for the inclusion of both contributions to the driving force. νDC =

8GDC sδD b , RT λ2DC

(3.11)

GDC is the total driving force for the coarsening process and includes contributions from both the remaining chemical supersaturation and the interlamellar interfaces. Under conditions where the chemical supersaturation remaining in the lamellar aggregate after the initial reaction is very close to zero, Eq. (3.11) reduces to an expression very similar to that derived by Livingston and Cahn (Eq. (3.10)). It is clear from Eqs. (3.10) and (3.11), that a relation between the interface velocity and the interlamellar spacing is obtained. The two quantities are coupled and an identical spacing selection problem exists for the discontinuous coarsening reaction as for the discontinuous precipitation and pearlite transformations discussed in Section III.8.

232

Y. BRÉCHET AND C. HUTCHINSON

11. M ULTILAYER S TABILITY The pearlite and discontinuous precipitation reactions discussed in this chapter give rise to a solid state lamellar pattern with a characteristic spacing behind a migrating interphase or grain boundary. Some aspects of the problems are still not well understood (especially aspects concerning the initiation processes) and in an effort towards this goal, Klinger et al.105–107 has suggested that several fundamental questions could be addressed through studies of the thermal stability of multilayers. Carefully controlled multilayer fabrication using techniques such as molecular beam epitaxy (MBE) provide a convenient means of examining the evolution of heterogeneous systems far from equilibrium. To date, much of the work has concentrated on the evolution of the systems controlled by bulk diffusion (an example is the precise determinations of low temperature solute diffusivities108,109 ), but multilayer growth on bi-crystal substrates that would result in a boundary that penetrates the entire structure could provide a means of examining interface-mediated pattern evolution under conditions where the boundary can act as a short circuit diffusion path for solute. Klinger et al.105 have considered the homogenization of a fully miscible multilayer by boundary migration and have computed the boundary shape and velocity (pattern selection) as a function of the system dimensions and the relevant thermodynamic and kinetic parameters. They identify different homogenization ‘modes’ illustrated schematically in Figure III.21. At one extreme (a) the homogenization may occur by the steady state motion of the boundary and at the other (c) through the instability of the boundary and a resulting ‘fingering’ solution. They were concerned with the conditions that would lead to the different patterns. More recently, they have considered cases were a third phase may form at the interfaces in the multilayer and have calculated the resulting shape and velocity of the interface between the three phases.107 Experiments of the type proposed by Klinger et al. may well provide a means of addressing such questions as velocity and pattern selection in well controlled systems as a function of the thermodynamics and kinetics of the system chosen and could certainly lead to a deeper understanding of the evolution of the lamellar patterns discussed in this chapter. 105 L. Klinger, Y. Brechet, and G. Purdy, Acta mater. 45, 4667 (1997). 106 L. Klinger, Y. Brechet, and G. Purdy, Acta mater. 46, 2617 (1998). 107 L. Klinger, Y. Brechet, and G. Purdy, Acta mater. 47, 325 (1999). 108 A. L. Greer, Curr. Opin. Sol. State. Mat. Sci. 2, 300 (1997). 109 A. L. Greer, Ann. Rev. Mat. Sci. 17, 219 (1987).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 233

F IG . III.21. The different possibilities for discontinuous homogenization of a multilayer containing a moving grain boundary:105 (a) steady state motion of the grain boundary, (b) sinusoidal instability of the grain boundary and (c) fingering instability of a moving grain boundary.

IV. Structural Defect Patterning: Grain Growth, Recovery and Recrystallization

In the previous section, the patterning examined was of a chemical nature. The structural defect involved was an interface which separated the transformed (patterned) region from the untransformed and in some cases provided a short-circuit diffusion path for solute. In the following sections we will consider the patterning of the structural defects themselves in systems that can be considered to be nominally chemically homogeneous. The structural defects encountered in metals and alloys are of three types: point defects (vacancies and interstitials), line defects (dislocations), and planar defects (grain boundaries, interfaces and surfaces). Point defects have a low energetic cost and a high configurational entropy: they are weakly interacting and only at short distances. Vacancies have a finite equilibrium concentration which can be reached when the material is cooled very slowly. Transport occurs by diffusion, in response either to a gradient in concentration, or to a gradient in stress (the latter being responsible for diffusional creep). Line defects (dislocations) are much more disturbing for the theoretician: they have a high energetic cost and their configurational entropy is restricted by topological requirements (a dislocation line can’t end within the crystal). Their equilibrium density is virtually zero at any temperature, but nevertheless, even if the material is cooled very slowly, dislocations are almost always present (e.g., Frank

234

Y. BRÉCHET AND C. HUTCHINSON

network). The reason for their persistence is the threshold force required to move them. The existence of this ‘solid friction’, together with the topological requirements and the crystallographic constraints to their motion (glide and cross slip on definite planes) prevents the simple definition of a relevant thermodynamic potential which drives their evolution. To make the things worse, dislocations are associated with a long range stress field (which decreases as 1/r) and present short range reactions (junctions). Both of these aspects are crucial to the theory of plasticity: the long range stress field couples to the applied stress to give the Peach–Kohler force for dislocation motion under stress and the short range interaction and junction formation are responsible both for the work hardening of the material and for the very existence of the sources which produce the dislocations. Any physicist interested in plasticity should absolutely resist the temptation to forget either of these aspects. We have to deal both with out of equilibrium, long range interacting, non-conserved entities, and with short range reactions. The natural mode of dislocation motion is to glide in well defined crystallographic planes in response to a local stress which results from the superposition of the applied stress and of the stress arising from all of the surrounding dislocations. Grain boundaries are somewhat more tractable. Like dislocations, they are nonequilibrium entities, but they have no long range stress field. Except for some very special grain boundaries which have a limited mobility and a low energy, their structure is such that they can have enough flexibility and ability to move so that the thermodynamic situation of having no boundary is, in principle, attainable. The specific differences in these three basic defect entities will help explain the characteristics of the patterns they produce and the ease with which they can be explained. 12. G RAIN G ROWTH Grain growth is the simplest of the pattern forming systems.110 There is a well defined thermodynamic state to be reached (infinite grain size) and the entities to be eliminated have no long range interaction. This apparent theoretical simplicity is less obvious from the experimental investigations. Grain growth is a 3D phenomenon, however very few 3D experimental studies have been reported in the literature.111,112 Most experimental studies are made using 2D slices. In addition, the theoretical predictions are derived under the assumption of a linear relation between the boundary mobility and the local driving force (which is the 110 A. P. Sutton and R. W. Balluffi, Interfaces in Crystalline Solids, Oxford University Press, Oxford (1996). 111 F. N. Rhines and B. R. Patterson, Metall. Trans. A 13A, 985 (1982). 112 F. C. Hull, Mat. Sci. and Tech. 4, 778 (1988).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 235

reduction in grain boundary curvature, cf. Section II). Under these assumptions, the theories113–115 predict that the length scale should behave as t 1/2 and that the size distribution of the grains, when scaled with the average grain size, should be invariant. Experimentally, the 1/2 exponent is almost never observed, although numerical simulations predict it, regardless of whether the boundary mobilities and energies depend on boundary misorientation. This suggests that the linear relationship between the velocity and the driving force is not valid. Natural reasons could be the impurity drag on moving boundaries116 or the reduced mobility of triple junctions and quadruple points.117 However, in spite of the disagreement between the predicted and experimentally observed exponents, the existence of an invariant scaled grain size distribution is observed both experimentally and in computer simulations. Patterning in grain growth is to be understood as the characteristics of this self-similar behavior: (i) The existence and shape of an invariant scaled size distribution. (ii) Topological relations such as the relation between the average size of the neighboring grains, or the number of neighbors of a grain of given size. Since all simulations relying on a linear relation between local driving force and velocity must give a kinetic law in t 1/2 , the issues on patterning are rather on these two characteristics. Extensive reviews of the topological characteristics of ‘cellular structures’ can be found in the articles by Weaire and McMurry19 and Thompson.20 Here we will focus on some of the open questions related both to theoretical pattern formation, and to some of the specifics of ‘real systems’. Two types of computer simulations dominate the literature on grain growth. On one side are those based on an adaptation of the Potts model,118–120 and on the other are those based on a discretization of grain boundaries, called the ‘vertex model’.121–125 Both models have been run in 2D and 3D and give similar results, 113 J. E. Burke and D. Turnbull, Prog. Met. Phys. 3, 220 (1952). 114 W. W. Mullins, J. Appl. Phys. 27, 900 (1956). 115 M. Hillert, Acta metall. 13, 227 (1965). 116 J. W. Cahn, Acta metall. 10, 789 (1962). 117 G. Gottstein and L. S. Shvindlerman, Acta mater. 50, 703 (2002). 118 M. P. Anderson, D. J. Srolovitz, G. S. Grest, and P. S. Sahni, Acta metall. 32, 783 (1984). 119 M. P. Anderson, G. S. Grest, and D. J. Srolovitz, Phil. Mag. B 59, 293 (1989). 120 A. D. Rollett, D. J. Srolovitz, and M. P. Anderson, Acta metall. 37, 1227 (1989). 121 K. Fuchizaki, T. Kusaba, and K. Kawasaki, Phil. Mag. B 71, 333 (1995). 122 F. J. Humphreys, Scripta metall. mater. 27, 1557 (1992). 123 C. Maurice and F. J. Humphreys, in Proceedings of an International Conference on Thermomechanical Processing in Theory, Modelling and Practice, ed. B. Hutchinson, The Society, Stockholm (1997), p. 201. 124 D. Weygand, Y. Brechet, and J. Lepinoux, Phil. Mag. B 78, 329 (1998). 125 D. Weygand, Y. Brechet, J. Lepinoux, and W. Gust, Phil. Mag. B 79, 703 (1999).

236

Y. BRÉCHET AND C. HUTCHINSON

as far as the size distribution and topological relations are concerned. We will place emphasis on the vertex models since the input quantities are continuum ones (such as boundary energies or mobilities) which, in principle, can be derived from experimental measurements. In both 2D and 3D, a scaled grain size distribution is obtained in the computer simulations as shown in Figure IV.1. However, this distribution does not corresponds to Hillert’s distribution which is a sort of mean field distribution (i.e., it assumes that the average size around a given grain is the average grain size in the system). It seems that Louat’s distribution, which relies on the unrealistic assumption of the totally random motion of a grain in the space of grain sizes126 is much closer to the simulated distribution, whereas the experimental distributions are often observed to be Log Normal. The ubiquity of Log Normal distributions (also observed in precipitation) is a puzzle in metallurgy. It seems that, although they do not correspond to steady state solutions of the Normalized Fokker–Planck equation, the transient to depart from them is very long. However, the reason for their appearance in the first place remains unknown. The second item used to characterize the patterns, are local correlations. Two may be considered: (i) Grains larger than average are more likely to be surrounded by grains smaller than average (Figure IV.2a). (ii) Grains larger than average tend to have a larger number of neighbors (Figure IV.2b). The correlations captured in item (i) are not included in Hillert’s derivation and may be the reason for the discrepancies between computer simulations and Hillert’s prediction. The correlations included in item (ii) are necessary in the Ryum–Hunderi scaling theory127 which makes use of the Mullins–Von Neumann equation114 to calculate the growth rate of an individual grain. The scaling theory of Ryum–Hunderi127 describes very accurately the distribution observed in the simulation (Figure IV.3), but there is currently no analytical derivation of the correlation given in Figure IV.2b. Even in this simplest case of pattern formation (scaling in grain growth), the distributions predicted both by the theory and the simulations are not in agreement, and they both disagree with the experimental data which appears to be a Log Normal distribution. Besides the pure ‘statistical physics’ problem, which amounts to investigating domain sizes in a conserved order parameter system, one can also consider 126 N. P. Louat, Acta metall. 22, 721 (1974). 127 O. Hunderi and N. Ryum, J. Mat. Sci. 15, 1104 (1980).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 237

F IG . IV.1. (a) Scaled grain size distribution obtained from a 2D vertex dynamics simulation.124 The log normal distribution as well as the distributions predicted by Hillert115 and Louat126 are shown for comparison. (b) Scaled grain size distribution obtained from a 3D vertex dynamics simulation125 and the comparison with the log-normal distribution and a previous simulation by Fuchizaki et al.121

238

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.2. 2D vertex dynamics simulations illustrating: (a) the average size of the neighbors of a grain of a given size128 and (b) the average number of neighbors of a grain of given size.124

materials science specific issues: the anisotropy of grain boundary energies and mobilities, the finite mobility of triple junctions, pinning points, etc. For the sake 128 D. Weygand, PhD, Institut National Polytechnique de Grenoble, Grenoble (1998).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 239

F IG . IV.3. Grain size distribution of the 2D vertex dynamics simulation compared to the distribution from the Ryum–Hunderi scaling theory.128

of illustration, let us consider the effect of particle pinning on the patterns formed by an evolving grain structure.129 Of course, the pinning by particles (Zener Pinning) is known to lead to a stabilized grain size. The kinetics, as simulated by the vertex model, saturate toward this ultimate grain size according to a kinetic law corresponding to a subtraction from the capillary forces due to Zener pinning (which in itself is a surprising result since Zener pinning is in principle a threshold force). The simulated kinetics and the results of an analytical expression are shown in Figure IV.4. The distributions are of course non-scale invariant, but the final distributions can be accurately fitted by a log normal distribution (Figure IV.5). A perhaps more striking result is the behavior of the topological characteristics.128,130 As shown in Figure IV.6, the correlation between the grain size of the neighbors and the average grain size is expected to be exactly opposite that predicted for grain growth in the absence of particles. For this simple patterning system it seems that two ingredients are missing for a complete understanding: the analytical derivation of the local spatial correlations, and the reasons for the apparent stability of the Log Normal distribution for grain sizes. However, the tools developed for understanding the evolution of capillary driven structures does allow us to obtain a new insight into recrystallization and 129 D. Weygand, Y. Brechet, and J. Lepinoux, Acta mater. 47, 961 (1999). 130 D. Weygand, J. Lepinoux, and Y. Brechet, in ed. J. Driver, Annecy, France, in press (2004).

240

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.4. Vertex dynamics simulation of the kinetics of grain growth in the presence of pinning particles.129 The grain size has been normalized to its saturation value and the time has been rescaled accordingly.

recovery, which in turn will provide some important inputs for the understanding of pattern formation in plasticity. 13. R ECOVERY AND R ECRYSTALLIZATION OF D ISLOCATION S TRUCTURES When heavily deformed, metals store large quantities of dislocations, in more or less organized structures (see Section V for the origin of this patterning). This certainly increases the free energy of the system, and provided some sufficient mobility is available to the defects, they will tend to move in order to reduce this energy. Accordingly, the dislocation density decreases, the substructures evolves and the hardness of the material decreases. This evolution of the structural defects during annealing can be followed by the evolution of the hardness of the material. Two situations are possible: either the evolution is slow in time (typically logarithmic) and occurs approximately everywhere at the same time and is referred to as ‘recovery’, or it is rapid in time, occurs heterogeneously, and corresponds to the nucleation of new grains free from defects (recrystallization). A detailed review of these mechanisms and their experimental studies can be found in Refs. [21,131]. 131 R. D. Doherty, D. A. Hughes, F. J. Humphreys, J. J. Jonas, D. J.Jensen, M. E. Kassner, W. E. King, T. R. McNelley, H. J. McQueen, and A. D. Rollett, Mat. Sci. and Eng. A A238, 219 (1997).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 241

F IG . IV.5. Vertex dynamics simulations of the grain size distribution in the presence of particles, compared to the initial distribution.129

In the following, we will highlight some observations which may lead to a better insight into plastically induced patterning from their further thermal stability. The first remark concerns the role of fluctuations, whereas the second and third remarks concern the definition of a driving force for structural evolution. The first set of comments concerns the nucleation of recrystallization. It is tempting to consider the nucleation of a dislocation free grain as a classical nucleation process where the gain in bulk energy pays for the cost in surface energy. The size of nuclei is such that the classical theory would predict a ridiculously low nucleation rate.21 Recrystallization nucleation is often associated with preexisting heterogeneities in the material: undeformable particles or initial grain boundaries. It seems natural to assume that gradients in stored energy are responsible for the motion of a grain boundary which delimits the new grain. This is perfectly understandable for particle nucleated grains, since geometrically necessary dislocations accumulate around the undeformable particles. However, it is more difficult to envisage in the vicinity of the grain boundary. Even if there is some crystalline anisotropy which may lead to different stored energies depend-

242

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.6. The grain size correlation function for particle inhibited grain growth compared to the correlation for normal grain growth.128 With increasing grain size, the average grain size of the neighboring grains increases in the presence of particles. The opposite behavior is observed for normal grain growth.

ing on the crystallographic orientation of the grains, these differences would tend to vanish when plastic deformation increases to the level attained in cold rolling. The paradox is that it is precisely when the strain increases that the nucleation of new grains at the boundary becomes easier. The dislocations stored in the material during cold rolling organize themselves into subgrains. The subgrain misorientations will increase, and their size will decrease when the strain in increased. An estimate of the stored energy can be obtained from the average subgrain size and the average misorientation. A vertex type simulation was performed in a situation where, across a grain boundary, a difference in stored energy was mimicked by a difference in subgrain size.132 Sure enough, the bowing of the grain boundary was triggered by this somewhat artificial gradient. But another simulation can be made, with no macroscopic gradient between the two grains, but simply accounting for the fact that sub-boundaries have a lower energy and a lower mobility that a general grain boundary.133 With these simple ingredients, it is found that, below a critical subgrain size or above a critical subgrain misorientation (which both can be understood as a critical strain) the nucleation of new grains by bowing out 132 F. J. Humphreys, Acta mater. 45, 4231 (1997). 133 D. Weygand, Y. Brechet, and J. Lepinoux, Phil. Mag. B 80, 1987 (2000).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 243

occurs naturally (Figure IV.7). It is not the gradient in the average quantity, but the fluctuation in the quantity which drives the nucleation of a new pattern. The importance of the fluctuations, and the fact that they have been too neglected in the current treatments, is a remark we will come back to. The second remark comes from measurements of the kinetics of recovery. If the sub-boundaries arising from deformation were low energy equilibrium structures, then the subsequent evolution of the microstructure would be simple subgrain growth. There would be no qualitative difference between subgrain growth and grain growth (it has been shown that the introduction of the dependence of the energy and mobility on grain boundary misorientation may change the prefactor, but the power law in t 1/2 should survive). Since the yield stress scales as the inverse subgrain size, the decrease in hardness should also follow a power law behavior, and not logarithmic kinetics. The experimentally observed logarithmic kinetics indicates that subgrain growth is slower, and suggests that the sub-boundary energy is decreasing during recovery. From this fact we can infer that (i) the sub-boundaries formed during plastic deformation where not a minimum in energy, and (ii) the sub-boundaries probably tend to a structure with minimum energy during recovery. The third set of remarks relies on some experimental observations of recovery in Al-2.5%Mg alloys. These observations will also be useful to understand the nature of the patterns emerging from deformation. Recovery processes are in principle simple in the sense that the main parameter governing the evolution is time and not strain, and the system is out of equilibrium but not maintained far from equilibrium. The pertinent questions are: What is the evolution of dislocation density? How is it correlated to the evolution of internal stresses? What is the remaining stored energy in a system having undergone static recovery? Microdensity and resistivity134 can be used to measure dislocation densities, the analysis of X-ray broadening allows us to evaluate the screening of dislocations in their substructure and calorimetry allows us to measure the stored dislocation energy which is released during recrystallization. Combining these measures on deformed samples, recovered for different times, provides information both on the pattern emerging from deformation, and its subsequent stability.135–138 134 M. Verdier, PhD, Institut National Polytechnique de Grenoble, Grenoble (1992). 135 M. Verdier, I. Groma, L. Flandin, J. Lendvai, Y. Brechet, and P. Guyot, Scripta mater. 37, 449

(1997). 136 M. Verdier, M. Janecek, Y. Brechet, and P. Guyot, Mat. Sci. and Eng. A 248, 187 (1998). 137 M. Verdier, Y. Brechet, and P. Guyot, Acta mater. 47, 127 (1998). 138 M. Verdier, F. Bley, M. Janecek, F. Livet, J. P. Simon, and Y. Brechet, Mat. Sci. and Eng. A 234,

258 (1997).

244

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.7. The bulging mechanism for the nucleation of recrystallization calculated with 2D vertex dynamics simulations with no subgrain size misfit.133 (a) Initial configuration and (b)–(f) evolution sequence.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 245

The evolution of the dislocation density as a function of the cold rolling strain (ε) in an Al-Mg alloy is shown in Figure IV.8a. The dislocation storage is not simply proportional to the strain but involves also dynamic recovery taking place during deformation. As a consequence, the net dislocation storage rate decreases at large strains. Figure IV.8b shows the evolution of the dislocation density during recovery annealing. The behavior of the dislocation density with annealing time is characteristic of the recovery kinetics: a fast initial decrease followed by a slower decay at longer annealing times. The results from resistivity and from microdensity measurements are consistent. For each sample deformed and recovered, the density of dislocations is known. In order to check that the broadening of the Bragg peak was mainly due to dislocations, the line width at half maximum has been measured for various peaks. After recovery annealing, the broadening of the peak decreases. In order to extract some useful information about the dislocation microstructure from the X-ray broadening, one has to postulate a model for the spatial arrangement of the dislocations. Instead, some information can be obtained directly from the behavior of the tail of the peak. Ideally, for an infinite straight dislocation the asymptotic decay of the intensity at large scattering vectors (q) would behave as q −3 , whereas for a dislocation dipole configuration, because of the screening of the strain fields, the intensity would decrease more slowly, as q −2 . The asymptotic behavior of the intensity for large q therefore gives information about the screening of the dislocation interactions. After static recovery, the tails at large q exhibit a slower decrease. This evolution can be interpreted as a consequence of the rearrangement of the dislocations into self screened structures of lower energy (Figure IV.9). The density of dislocations can be estimated via the resistivity measurements which are directly related to the total length of dislocation core. The stored energy in a given state can be measured by the total energy released in the calorimeter when a sample is fully recrystallized. Figure IV.10 shows the stored energy as function of the dislocation density for increasing strains. Not only does the rough estimation of the stored energy given by ρμb2 /2 (ρ is the dislocation density, μ is the shear modulus and b is the burgers vector) tend to overestimate the true value, but including the logarithmic correction term (Ln(bρ 1/2 )) is also insufficient. This clearly shows that, while deformation increases, and as dislocation structures become better defined, the dislocation stress fields are more and more efficiently screened. This effect parallels the screening effect evidenced by the X-ray analysis. During recovery, the dislocation density decreases, as expected. But the decrease in energy is much lower than would be expected from the simple estimates from the relation between dislocation density and energy in a cold rolled sample. Everything behaves as if there was a ‘marginal cost’ to incorporate and remove a dislocation from a given structure. This ‘chemical potential’ for dislocations governs the decrease of stored energy during recovery, as seen in Figure IV.11.

246

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.8. The evolution of the dislocation density (a) as a function of the cold rolling strain, ε, in an Al-Mg alloy and (b) during annealing of deformed Al-Mg samples at 160 ◦ C and 220 ◦ C.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 247

F IG . IV.9. Evolution of the X-ray Bragg peak during recovery of a deformed Al-Mg alloy after cold rolling to ε = 3.

F IG . IV.10. Comparison between the measured stored energy (EDSC ) and the calculated E(ρ) using the classical expression with a cut-off radius Re = 1/vρ, as a function of the dislocation density at different cold rolling strains in an Al-Mg alloy.

248

Y. BRÉCHET AND C. HUTCHINSON

F IG . IV.11. Evolution of the stored energy during cold rolling and after recovery of ε = 3 at T = 220 ◦ C as a function of the dislocation density in an Al-Mg alloy.

The main points to be retained from these results are the following: (i) The dislocations structures emerging from cold deformation are not low energy structures: recovery leads to lower energy structures as well as to the reduction of their number per unit volume. (ii) Dislocation density is not a sufficient variable to characterize a deformed state and the associated microstructure: as far a stored energy is concerned, the self screening of dislocations is an essential parameter. These facts will provide guidelines to evaluate the existing models for dislocation patterning. V. Structural Defect Patterning: Irradiation and Plastic Deformation

From the previous statements, one can infer that two factors will plague the understanding of patterns associated with dislocations. On one hand, the screening of the long range interactions between dislocations must be considered and this will be a key issue for understanding patterning. On the other hand, the motion of dislocations in response to an applied stress field must also be adequately addressed. Both of these aspects present current difficulties for the theoretician. In this sense, irradiation and plasticity are quite different. Irradiation induced dislocations are loops whose far field elastic stresses are much smaller than those

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 249

associated with long dislocations generated by plasticity. Furthermore, whereas the point defects generated by irradiation are mobile entities, irradiation loops are effectively immobile. As a result of these two ‘simplifications’ our understanding of patterning in irradiation is more advanced than our understanding of patterns obtained during plastic deformation. 14. I RRADIATION I NDUCED PATTERNING The main effect of irradiation is the generation of point defects (both interstitials and vacancies139 ). These defects, far in excess of the equilibrium concentrations, tend to agglomerate140 in the form of either irradiation loops or voids.139,141 An example in an irradiated stainless steel142 is shown in Figure V.1. The defects visible in Figure V.1 are clearly not well organized. However, under particular conditions, these structural defects generated from the excess point defects do tend to self-organize into strikingly regular patterns as shown in Figure V.2.143,144

a. The Experimental Facts: Dislocation Carpets and Void Lattices Detailed accounts of the experimental characteristics of irradiation patterns can be found in numerous reviews (Refs. [145–148] for voids and bubble lattices, Refs. [149–152] for dislocation patterning). We will focus our attention on the main features relevant to the modeling of irradiation patterns as dynamic instabilities. The patterns shown in Figure V.2 have two seemingly contradictory characteristic features: their scale is very small, but still much larger than the interatomic 139 M. T. Robinson, J. Nucl. Mat. 216, 1 (1994). 140 A. Barbu and G. Martin, Solid State Phenomena 30–31, 179 (1993). 141 A. Barbu, G. Martin, and L. Howe, in Basic Mechanical Properties and Lattice Defects of Inter-

metallic Compounds, eds. J. Westbrook and R. Fleisher, Wiley and Sons, New York (2000), p. 181. 142 C. Pokor, Y. Brechet, P. Dubuisson, and J. P. Massoud, J. Nucl. Mat. 326, 19 (2004). 143 W. Jager, P. Ehrhart, and W. Schilling, Solid State Phenomena 3–4, 279 (1988). 144 G. L. Kulcinski and J. L. Brimhall, in Effects of Irradiation on Substructure and Mechanical Properties of Metals and Alloys, ed. J. Mateff, ASTM (1973), p. 258. 145 J. H. Evans, Nature 229, 403 (1971). 146 J. H. Evans, Solid State Phenomena 3–4, 303 (1988). 147 J. H. Evans, Rad. Eff. 10, 55 (1971). 148 S. L. Sass and B. L. Eyre, Phil. Mag. 27, 1447 (1973). 149 D. J. Mazey and J. H. Evans, J. Nucl. Mat. 138, 16 (1986). 150 J. O. Stiegler and K. Farrell, Scripta metall. 8, 651 (1974). 151 W. Jager, P. Ehrhart, and W. Schilling, Rad. Eff. Def. Solids 113, 201 (1990). 152 R. Bullough, B. L. Eyre, and K. Krishan, Proc. Roy. Soc. London A 346, 81 (1975).

250

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.1. (a) Irradiation loops and (b) irradiation voids in an irradiated stainless steel.142

F IG . V.2. Self-organizing patterns under irradiation. (a) Dislocation carpets in Cu (periodic arrays of vacancy loops).143 (b) Nb void lattices: electron micrograph showing a BCC void superlattice in Nb irradiated with Ta+ ions at 800 ◦ C.144 The foil orientation is near 111.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 251

252

Y. BRÉCHET AND C. HUTCHINSON

spacing (at least two orders of magnitude) and their alignment reflects the underlying crystallography of the lattice. In Figure V.2a, the dislocation vacancy loops generating the ‘carpet pattern’ in irradiated Cu are aligned along (001) planes. The 3D void lattice in irradiated Nb shown in Figure V.2b has the same symmetry and orientation as the underlying crystalline host lattice. The obvious question is what mechanism could transfer anisotropy at the atomistic level into patterns at a scale two orders of magnitude larger. These well organized patterns are not observed under all irradiation conditions. The dislocation patterns become regular when the irradiation flux exceeds some critical value which is an increasing function of the irradiation temperature. However, the wave length developed seems to depend little on the irradiation conditions. If the flux exceeds a second critical value, the dislocation microstructure loses its regular patterning. The values of these two critical fluxes depend on the system and on the material purity. The void lattice (Figure V.2b) seems to nucleate first at random, and then to order at a later stage when the irradiation dose has become sufficiently high. The conditions for void ordering also depend on the level of purity of the alloys and on their gas content. The void lattice parameter seems to depend on temperature and irradiation flux mainly through the total fraction of voids generated after a given irradiation dose.

b. The Framework of a ‘Reaction Diffusion’ Approach The main effect of irradiation is to generate point defects (and possibly gases). These entities interact to create the mesoscopic defects whose patterning is of interest here: the point defects can generate dislocation loops and vacancies and gases can form bubbles. The point defects can also interact with the defects they have already formed. For example, the diffusion of vacancies or interstitials to the stationary dislocation loops and voids can give rise to absorption events. These mechanisms provide a framework for a ‘chemical kinetics’ approach to the evolution of the population of defects. A set of rate equations can be written to describe the evolution of the defect populations. The point defects (vacancies or interstitials) will be indexed by r, and the microstructural features (dislocation loops, vacancies clusters, voids) by q. Each defect in concentration, Cr , will be generated at a rate Pr by irradiation damage, and can be annihilated or created on either pre-existing sinks (such as grains boundaries) or those created by irradiation. Annihilation may also occur by pairs of vacancies/interstitials. A further feature of the rate equations is that the absorption of point defects by features such as dislocations presents a bias in favor of the interstitials. The rate of absorption is related to the mobility of point defects and therefore to their diffusion coefficients, whereas the relevant microstructural features are the defect densities and sizes.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 253

The volume fraction Qq occupied by a given type of microstructural feature (e.g., voids) may either grow or decay from the absorption or emission of point defects. The details of these equations will depend on the nature of the microstructural features under consideration, but the form of the equations is quite general. The form of the ‘rate equations’ for the point defects and the microstructural features can be written: C˙ r = Pr − AC1 C2 + r (Cr , Qq ) (5.1) ˙ q = Pq + (Cr , Qq ). Q These general ‘rate equations’, initially defined by Bullough et al.,152–154 can be used to study the evolution of the specific features one is attempting to describe. For example, if the evolution of the distribution of dislocation loops is of concern, a detailed solution of the problem, using a Fokker–Plank approach, allows for a description of the number and size distribution.142 If patterning (dislocation patterning or void patterning) is the phenomenon which has to be described, a spatial variable must be added. This appears as a diffusion term in the rate equation for the point defects. The microstructural features such as voids and dislocations are not supposed to move in space and their patterning reflects only the patterning in the field of the point defects. An example of such an approach was proposed by Murphy154 for the patterning of vacancy loops. The technique used is always the same: one searches for a homogeneous steady-state solution to the rate equations, and then performs a linear stability analysis with respect to infinitesimal perturbations periodic in space. When at least one eigenvalue of the linearized equations in Fourier space has a positive real part, the corresponding eigenmode will grown and lead to a periodic pattern. This very simple linear stability analysis is able to provide a qualitative understanding of dislocation loop patterning, but is unable to provide a quantitative prediction for the selected wavelength. In order to go further, a non-linear analysis of the same set of rate equations must be performed. In a series of papers, Ghoniem and Walgraef155–158 have thoroughly investigated this problem, both with weakly non-linear analysis (the next term in the expansion in terms of the amplitude of the perturbation) and with numerical simulations. They investigated the influence of defect densities (initial dislocation network) on the wavelength. The values of the parameters which lead to patterning have been derived and the ratio of the absorption bias to the emission bias 153 K. Krishan, Solid State Phenomena 3–4, 267 (1988). 154 S. M. Murphy, Solid State Phenomena 3–4, 295 (1988). 155 N. M. Ghoniem, D. Walgraef, and S. J. Zinkle, J. Comp. Aid. Mat. Des. 8, 1 (2002). 156 D. Walgraef and N. M. Ghoniem, Phys. Rev. B 39, 8867 (1989). 157 N. M. Ghoniem and D. Walgraef, Mod. Sim. Mat. Sci. and Eng. 1, 569 (1993). 158 D. Walgraef, J. Lauzeral, and N. M. Ghoniem, Phys. Rev. B 53, 14782 (1996).

254

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.3. Comparison between experimental data and theoretical predictions for the temperature and dose rate dependence of defect cluster wall observations in irradiated Ni.155 The filled symbols denote conditions where defect cluster wall formation was observed.

seems to play a key role. The anisotropy of diffusion of self interstitial atoms is held responsible for the crystallographic nature of the patterning of both the dislocation loops and the voids. It was also shown that this anisotropy need not to be larger than 1% to give a very well defined crystallographic organization. The conditions for patterning appear to be that the rate of point defect absorption exceeds their mutual annihilation, and that cascade induced vacancy cluster densities are above some critical value. These conditions lead to the prediction of the ranges in temperature and irradiation conditions for which dislocation patterning is expected (Figure V.3).155 When the temperature is too high, the cluster evaporation decreases the net absorption rate by dislocation loops and when the temperature is too low the recombination between vacancies and interstitials dominates. Dislocation patterning is observed only within these two limiting temperatures. The case of void formation is somewhat different: voids seem to nucleate ‘at random’, and progressively organize.146 The crystallographic organization of the void lattice has also been interpreted as a consequence of the anisotropy of self interstitial diffusion. Furthermore, it has been shown that when a void is slightly displaced from its position in a regular lattice, it will tend to grow in an anisotropic

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 255

manner, to bring it back to a central position.159 This amounts to having a drift force on the void mediated by the diffusion field of point defects. In the case of the dislocation carpets discussed above it is assumed that spatial motion is only possible for the point defects. The dislocations themselves are assumed stationary. Such models are bound to fail in describing pattern formation for entities which are nucleated at random with a substantial size. For void patterning, it seems that the long range repulsive forces described above play a key role, more so than a diffusional instability. A similar situation will be suggested for dislocation patterning in plasticity. 15. P LASTICITY I NDUCED PATTERNING The first feature which arises from dislocation patterning in plasticity, especially when compared to the dislocation patterns issued from irradiation, is their relatively coarse scale (for an overview of experimental results for F.C.C. metals, see Ref. [160]). The scale is at least one order of magnitude larger than the ‘carpet structures’ developed under irradiation. This in itself can be seen as a sign of the long range elastic interactions between dislocations, and as a consequence of the dislocation glide transport mechanism which is far more efficient than diffusion.

a. The Experimental Facts When plastic deformation takes place in a polycrystal, multiple slip systems are generally activated. The dislocations generated on these different slip systems interact and the material hardens. Eventually the flow stress reaches a saturation level where the annihilation of dislocations balances the accumulation. At large enough strains (or more accurately for large enough dislocation densities, i.e., when the interaction between dislocations exceeds the lattice friction) a cellular structure will form. The material is a composite structure of regions virtually free of dislocations (cell interiors) separated by regions of high dislocation densities (cell walls). The experimental conditions (T , ε) for the emergence of a cell structure in Fe are shown in Figure V.4.161 At low temperatures the lattice friction is difficult to overcome and the dislocation pattern remains planar rather than cellular. For F.C.C. materials, the lattice friction stress is generally negligible and cellular patterns emerge more readily than in BCC and HCP metals. When alloying 159 P. Benoist and G. Martin, in Proceedings of an Internations Conference on Fundamental Aspects of Radiation Damage in Metals, Gatlinberg, Tennessee (1975), p. 1236. 160 B. Bay, N. Hansen, D. A. Hughes, and D. Kuhlmann-Wilsdorf, Acta metall mater. 40, 205 (1992). 161 A. S. Keh and S. Weissmann, in Electron Microscopy and Strength of Metals, eds. G. Thomas and G. Washburn, Interscience, New York (1963), p. 231.

256

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.4. The transition between uniform and cellular dislocation structures in α-Fe as a function of strain and temperature.161

elements are added, any phenomenon which promotes the planarity of the slip (e.g., decreases the stacking fault energy, presence of shearable precipitates, etc.) will postpone to larger strains and larger dislocation densities the emergence of a cellular structure. The higher the deformation temperature, the better defined are the cells, i.e., the narrower are the cell walls.162 Some examples taken from Ni, Cu and Al are shown in Figure V.5.163 The cell structure has a scale D which is inversely proportional to the flow stress, as shown in Figure V.6.164 The relation between D (normalized by the Burgers vector b) and σ (normalized by the shear modulus μ) is given by Eq. (5.2). The constant K is close to 20. b σ =K μ D

(5.2)

The 3D patterns developed during large strains have been extensively reviewed. They show the emergence of patterns elongated in the direction of cold rolling and the initiation of bands of intense localization of plastic strains, probably associated with crystalline rotations.160 In addition to this self imposed ‘scale’, more recent detailed examination of the apparent length scales at different magnifications have revealed the existence of a 162 M. R. Staker and D. L. Holt, Acta metall. 20, 569 (1972). 163 I. Barker, N. Hansen, and B. Ralph, Mat. Sci. and Eng. A A113, 449 (1989). 164 S. V. Raj and G. M. Pharr, Mat. Sci. and Eng. 81, 217 (1986).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 257

(a)

(b)

(c)

F IG . V.5. Bright field transmission electron microscope images of some FCC metals deformed to a true strain of 0.1.163 (a) Ni, (b) Cu and (c) Al.

258

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.6. The relation between reduced cell size, D/b, and reduced flow stress, σ/μ, in (a) Fe and (b) Al.164

fractal structure in the dislocation cells.165 The scaling works over two orders of magnitude for the cell sizes and the fractal dimension of the 2D slices of the cell structure ranges between 1.6 to 1.8 (with increasing flow stress), Figure V.7. As pointed out by Kubin,166 the scaling relation between the flow stress and the dislocation cell size (Eq. (5.2)) can be readily obtained either from the dependence in 1/r of the dislocation stress field, or from the dependence in 1/D of the activation stress for a source whose pinning points are separated by a distance D. Therefore, any acceptable theory for pattern formation should lead to this scaling law. The differentiation between the different theories should be made on the basis of both their predictions for the constant K and their ability to predict the conditions under which patterning is observed.

b. The Limits of Classical Approaches for Pattern Formation Let us begin by summarizing a few key features of the formation of dislocation cells. • Since dislocation patterning occurs during plastic deformation, and well before the saturation stress is reached, it should be considered as a dynamic instability, not an organization of a given number of dislocations. 165 P. Hähner, K. Bay, and M. Zaiser, Phys. Rev. Letts. 81, 2470 (1998). 166 L. P. Kubin, in Materials Science and Technology: Vol. 6 Plastic Deformation and Fracture of

Materials, ed. H. Mughrabi, VCH, Weinheim (1993), p. 138.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 259

F IG . V.7. (a) Bright field transmission electron micrograph of the dislocation cell structure in a Cu single crystal after tensile deformation along a [100] direction at room temperature to a stress of 75.6 MPa. (b) Analysis of the cell structure shown in (a) by determining the ‘box dimension’ DB .165

260

Y. BRÉCHET AND C. HUTCHINSON

• Since cell formation is postponed by planarity of slip, and multiple slip seems necessary for the appearance of cells, the local reactions between different dislocation families must be a key ingredient for pattern formation. • Since cellular patterns are observed only when the long range stresses between dislocations overcome the short range lattice friction stress, it is also necessary to include the stress field of a dislocation distribution as a crucial ingredient for pattern formation. The classical approaches to dislocation patterning all fail in at least one of the above respects. The first theory for dislocation patterning, due to Holt,167 considers the formation of a cellular structure as an instability in a population of a given density of dislocations. He considers a two-dimensional distribution of supposedly infinite dislocation lines, and no short range reactions are allowed. The correlation function between dislocations is assumed to vanish on distances which are of the order of ρ −1/2 where ρ is the dislocation density. Under these conditions, the system is expected to spontaneously ‘un-mix’ by a spinodal-like instability, the fastest growing wavelength being proportional to the cut-off radius. Since the flow stress is proportional to ρ 1/2 , this gives the expected scaling law. However, besides the simplistic 2D realization, the model is fundamentally flawed in two respects: (a) the dislocations are assumed to respond to the internal stress only, whereas they should also be responding to the applied stress, and (b) the dislocation density is assumed to be constant, whereas this is obviously not generally the case during plastic deformation. Furthermore, in order to write the appropriate ‘diffusion-like’ equation for dislocation motion, the existence of a cut-off radius is crucial, and this gives the emergence of a characteristic length. The question of the spontaneous emergence of the screening length appears as a crucial issue in the problem of patterning and must be solved in a self consistent manner, not imposed ‘a priori’. The Holt model is, in essence, a model to minimize the energy of a closed system, whereas dislocation patterning is a dynamic instability in an open system. Along similar lines of a minimization of the total energy at constant dislocation density and in the absence of an external applied stress, is the family of models known as LEDS (Low Energy Dislocation Structures).168–172 These 167 D. L. Holt, J. Appl. Phys. 41, 3197 (1970). 168 D. Kuhlmann-Wilsdorf, Metall. Trans. A 16A, 2091 (1985). 169 D. Kuhlmann-Wilsdorf, Trans. AIME 224, 1047 (1962). 170 N. Hansen and D. Kuhlmann-Wilsdorf, Mat. Sci. and Eng. 81, 141 (1986). 171 D. Kuhlmann-Wilsdorf, Mat. Sci. and Eng. A A113, 1 (1989). 172 U. F. Kocks, T. Hasegawa, and R. O. Scattergood, Scripta metall. 14, 449 (1980).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 261

models describe the scaling law, which only means that they are dimensionally correct, but they cannot describe the dynamic nature of the instability. A completely different route was proposed by Kocks.173,174 Whereas the previous models insisted on the forces acting on the dislocations, Kocks insisted on including the short range reactions between dislocations in their glide plane when they interact with the forest made by dislocations from other glide planes. The key idea is that the building up of a cell structure is intrinsically a statistical problem: regions where the forest trees are to narrowly spaced will not be penetrable by the gliding dislocations, which will leave around these regions loops which will make them even more impenetrable. Since the only length scale in the problem is ρ −1/2 , the distance between hard points will scale as this distance, which will indeed give the correct scaling law, since the flow stress scales as ρ 1/2 . The simulations performed by Kocks confirm this finding. However the flaw in the approach is in two respects. On the one hand, dislocation patterning occurs in multiple slip and the forest dislocation density is certainly not constant, as is assumed in stage II work hardening. On the other hand, the hard points created by the mere fact that forest dislocations are too close together, are not really so hard. They may be too hard to be penetrated by the applied stress, but once a loop is left behind, they may be penetrated by the combined effect of the applied stress and the line tension. In order to stabilize these hard points, local reactions due to recovery are necessary to create sessile obstacles. The dynamic nature of dislocation patterning and the non-conserved character of dislocations (i.e., their ability to annihilate by pairs or to multiply via various source mechanisms) has triggered interest in a ‘chemical kinetics’ approach. Various detailed sets of equations have been proposed,174–182 but the framework always remains the same. The density of dislocations is divided into different ‘species’, ρi , each with a flux, Ji . The reaction terms (annihilation, 173 U. F. Kocks, in Dislocations and Properties of Real Materials, The Institute of Metals, London

(1985), p. 125. 174 U. F. Kocks, A. S. Argon, and M. F. Ashby, Prog. Mat. Sci. 19, 1 (1975). 175 D. Walgraef and E. C. Aifantis, J. Appl. Phys. 58, 688 (1985). 176 L. P. Kubin and J. Lepinoux, in Proceedings of an International Conference of the Strength of Metals and Alloys (ICSMA8), Vol. 1, eds. P. O. Kettunen, T. K. Lepisto, and M. E. Lehtonen, Pergamon, Tampere, Finland (1988) p. 35. 177 U. Essmann and K. Differt, Scripta metall. 22, 1337 (1988). 178 K. Differt and U. Essmann, Mat. Sci. and Eng. A A164, 295 (1993). 179 G. Malygin, Soviet Physics State Solid 31, 96 (1989). 180 G. Malygin, Physics-Uspekhi 42, 887 (1999). 181 Y. Estrin and L. P. Kubin, Acta metall. 34, 2455 (1986). 182 L. P. Kubin, in NATO ASI Series: Stability of Materials, eds. A. Gonis, P. E. A. Turchi, and J. Kudrnovsky, Plenum, New York (1995), p. 99.

262

Y. BRÉCHET AND C. HUTCHINSON

multiplication. . .) are embedded into a function R(ρi , ρj , σ ) and the evolution equations can then be written as: ∂ρi + div(Ji ) = R(ρi , ρj , σ ) ∂t

(5.3)

In some cases, when only dynamic processes are involved (i.e., when R is proportional to the velocity of dislocations), the differential equation can be written in terms of derivatives with respect to ε. The difficulty in the approach is in the expression of Ji . The flux is obviously related to the dislocation densities and velocities, and the velocities are related to the applied stress, σa , and to the internal stress, σint , due to the other dislocations by an ‘effective’ dislocation mobility, M. Ji = ρi V = ρi M(σa − σint )

(5.4)

All the difficulty lies in the evaluation of the internal stress. Since the dislocation field is long ranged, the expression for the internal stress is given by an integral, and only an expansion of this integral in terms of gradients in ρ allows us to reach an expression for σint which is local. Under this very questionable assumption, the basic equation can be reduced to a ‘reaction diffusion’ approach for which the standard techniques can be applied. Another simplified condition under which a ‘diffusion’ term can be obtained is the case of spreading of the dislocation density via random events such as double cross-slip. But again, this procedure hides the fundamental fact that dislocations are gliding and not diffusing, and that the long range fields cannot be assumed to be screened without further justification. This is probably the reason why ‘reaction diffusion’ approaches have never been able to present for dislocation patterning the same success they have shown for irradiation patterning. In spite of these pitfalls, the various ‘classical approaches’ presented above have brought to the forefront the key issues that need to be addressed by a future ‘theory of dislocation patterning’: – local reactions must be accounted for, and in particular, the non-conservative nature of dislocation densities; – long range stresses have to be accounted for, and the self-screening of dislocations, which can even be measured experimentally,183,184 must be derived as part of the solution of the problem. 183 T. Ungar, L. S. Toth, J. Illy, and I. Kovacs, Acta metall. 34, 1257 (1986). 184 T. Ungar, H. Mughrabi, D. Ronnpagel, and M. Wilkens, Acta metall. 32, 333 (1984).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 263

As a result of the difficulty in addressing these questions in an analytical manner, without making unreasonable assumptions, computer simulations of dislocation dynamics have been proposed to investigate the collective behavior of dislocation populations, and in particular, their tendency to patterning.185

c. Computer Simulations of Pattern Formation The principle of all simulations described below is first to compute for each dislocation segment the local stress arising from the applied stress and from the interactions with other dislocations in the system. Under this local stress, each dislocation will move at a particular velocity. The simulations differ in the variety of local reactions allowed (multiplications, annihilation, junction formation), on the degree of naivety with which they are described and in the range of strains (or equivalently dislocation densities, or volume simulated) they can treat in a reasonable computing time. The first simulation,186,187 a cellular automaton carried out in two dimensions, included, for reasons of computational efficiency, a cut-off radius for dislocation interactions. Calculations were made with and without an externally applied stress. When no external stress was applied, but with the dislocation interactions artificially screened, the instabilities occur, and a length scale emerges which is related to the cut-off radius. When the long range interactions were accounted for without an imposed cut-off radius, as was done in another group of simulations using Molecular Dynamics techniques,188,189 the patterning disappears. In any case, a partial self-screening is observed, in the sense that during relaxation, the net interaction stress with other dislocations is decreasing. When an external stress is applied, and no cut-off radius is artificially imposed, no clear patterning seems to occur. The definitions of the local rules for multiplication, which are randomly positioned in an artificial manner, are obviously too naïve to capture the spatial organization. In spite of the numerical and topological difficulties associated with the 3D aspect of dislocation dynamics, it seemed necessary to go one step further and to explicitly include the long range dislocation interactions, the friction stress, the junction formation, dislocation multiplications and the various glide and cross 185 L. P. Kubin, Y. Estrin, and G. Canova, in NATO ASI: Patterns, Defects and Material Instabilities,

ed. D. Walgraef, Kluwer (1989). 186 J. Lepinoux and L. P. Kubin, Scripta metall. 21, 833 (1987). 187 J. Lepinoux, Solid State Phenomena 3–4, 389 (1988). 188 N. M. Ghoniem and R. J. Amodeo, Solid State Phenomena 3–4, 377 (1988). 189 R. J. Amodeo and N. M. Ghoniem, Phys. Rev. B 41, 6958 (1990).

264

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.8. (a) Thin (111) slice (1 μm thickness) extracted from the simulated dislocation structure of a [100] aluminium crystal after deformation. (b) The corresponding mapping of the internal shear stress field resolved in the same plane.196

slip processes.190–195 The details of the 3D dislocation simulation, known as DDD (Discrete Dislocation Dynamics) can be found in Ref. [196]. This ambitious program has been developed over the years and has finally led to the simulation of an emerging dislocation structure associated with a spatial patterning of the internal stress.196,197 An example is shown in Figure V.8. The limitations in terms of plastic strain attainable in a reasonable computational time, as well as the rather poorly defined cellular structure, prevents testing of the scaling law for cell size as function of the flow stress, although the length scale observed is reasonable. The lesson to be learnt from both the 2D and the 3D simulations is that both long range stresses and short distance reactions are necessary to obtain patterning, and that the short range reactions must be described with a sufficient spatial accuracy. The fact that a source is unlikely to operate 190 L. P. Kubin and G. Canova, Scripta metall. mater. 27, 957 (1992). 191 L. P. Kubin and G. Canova, in Electron Microscopy in Plasticity and Fracture Research of Mate-

rials, eds. F. Appel and U. Messerschmidt, Akademie-Verlag, Berlin (1989), p. 23. 192 L. P. Kubin, G. Canova, M. Condat, B. Devincre, V. Pontikis, and Y. Brechet, Diff. and Def. Data B 23–24, 455 (1992). 193 B. Devincre and L. P. Kubin, Mod. Sim. Mat. Sci. and Eng. 2, 559 (1994). 194 H. M. Zbib, M. Rhee, and J. P. Hirth, Int. J. Mech. Sci. 40, 113 (1998). 195 D. Weygand, L. H. Friedman, E. Van der Giessen, and A. Needleman, Mod. Sim. Mat. Sci. and Eng. 10, 437 (2002). 196 L. P. Kubin and B. Devincre, in Deformation-Induced Microstructures: Analysis and Relation to Properties. Proceedings of 20th International Symposium on Materials Science, 6–10 Sept. 1999, Riso Nat. Lab, Roskilde, Denmark (1999), p. 61. 197 R. Madec, B. Devincre, and L. P. Kubin, Scripta mater. 47, 689 (2002).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 265

when dislocations in the surrounding region are closely spaced must be taken into account (e.g., distributing sources randomly will not be sufficient). More recently, 2D simulations have been revised198–201 with the idea of incorporating information from the 3D simulations, to simultaneously benefit from the much greater speed of the 2D calculations and the possibility of rigorously treating the mechanical boundary conditions, together with the necessity of relating the local rules to the local environment. Furthermore, lattice rotations can be naturally included.202 Figure V.9 illustrates an emerging dislocation pattern in Cu

F IG . V.9. (a) Evolution of the bulk dislocation structure in [110] tension of crystal A at a strain of ε = 0.03. (b) The corresponding contours of lattice rotation, θ (in degrees).202 198 H. H. M. Cleveringa, E. Van der Giessen, and A. Needleman, Acta mater. 45, 3163 (1997). 199 A. Needleman, Acta mater. 48, 105 (2000). 200 A. Needleman and E. Van der Giessen, Mat. Sci. and Eng. A 309, 1 (2001). 201 J. Y. Shu, N. A. Fleck, E. Van der Giessen, and A. Needleman, J. Mech. Phys. Solids 49, 1361

(2001). 202 A. A. Benzerga, Y. Brechet, A. Needleman, and E. Van der Giessen, Mod. Sim. Mat. Sci. and Eng.

12, 159 (2004).

266

Y. BRÉCHET AND C. HUTCHINSON

together with the local lattice rotations for a plastic strain of 3%. In this simulation, no artificial cut-off radius was imposed. When the rules for multiplication and annihilation are not defined according to the local environment, dislocation patterning does not emerge.

d. Necessary Ingredients for a Theory of Plastically Induced Pattern Formation The situation concerning our understanding of dislocation patterning during plastic flow can be summarized in the following way. The energetic models and statistic models capture only one part of the problem and both fail to account for the long range interactions between dislocations which is a key ingredient. The local reactions must be explicitly accounted for, including their dependence on the local environment. The ‘reaction diffusion’ approaches oversimplify the dynamics of dislocation glide. In addition, one aspect which is not accounted for is the appearance, together with cell formation, of lattice rotations which may modify the dislocation dynamics on either side of a cell wall. Each of these ingredients are necessary for a future theory for pattern formation. Recent work by Hähner and collaborators203–211 has highlighted a completely new feature that may also need to be considered in the problem of dislocation patterning. Hähner emphasizes the importance of the stochastic aspect in dislocation dynamics. The local fluctuations in the shear rate, γ˙ , and the effective shear stress, τeff , are related to the internal shear stress, τint , and to the strain rate sensitivity, S, in the following way: S = γ˙

∂τa ∂γ˙

(5.5)

Through an equivalent of the fluctuation dissipation theorem: (δτeff )2 = Sτint

and δ γ˙ 2 /γ˙ 2 = τint /S.

(5.6)

203 P. Hähner, Appl. Phys. A 62, 473 (1996). 204 M. Zaiser, Mat. Sci. and Eng. A 309, 304 (2001). 205 S. Bross and P. Hähner, in NATO ASI Series: Thermodynamics, Microstructures and Plasticity, eds. A. Finel, D. Maziere, and M. Veron, Kluwer, Dordrecht (2002), p. 313. 206 P. Hähner, Acta mater. 44, 2345 (1996). 207 M. Zaiser, M. Avlonitis, and E. C. Aifantis, Acta mater. 46, 4143 (1998). 208 M. Zaiser, K. Bay, and P. Hähner, Acta mater. 47, 2463 (1999). 209 M. Zaiser and P. Hähner, Mat. Sci. and Eng. A 270, 299 (1999). 210 P. Hähner and M. Zaiser, Mat. Sci. and Eng. A 272, 443 (1999). 211 P. Hähner, Scripta Materialia 47, 415 (2002).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 267

Zaiser, Bay and Hähner208 then write an evolution equation for the dislocation density which is in fact a stochastic equation incorporating the noise in the local strain rate. The detailed form of the deterministic equation can be discussed, but the key feature is the following: the probability distribution of the dislocation density changes from a peaked distribution for small values of the noise (i.e., small internal stresses compared to the applied stress) to a power law distribution at larger values of the noise. In this approach, the cell size distribution is expected to show a fractal like behavior, and is to be understood as a noise induced phase transition, where the strain-rate sensitivity and the internal stress compared to the applied stress play a crucial role.208,211 In addition to the requirements concerning long range stresses and local reactions, the theory for dislocation cell formation still to be discovered will have to incorporate these stochastic aspects.

e. The Special Case of Patterning in Fatigue Fatigue loading is quite special in plasticity. By a periodic reversal of the applied stress, dislocations are forced to move back and forth, and the resulting microstructure depends on the degree of irreversibility of this motion. As fatigue cycles accumulate, dislocation dipoles are formed, and these entities have elastic fields which are less extended in space. By the very construction of the fatigue dislocations, the long range interaction stresses tend to be naturally screened. The patterns observed in fatigue are very regular, much more so than the patterns obtained in monotonic plasticity. Since the phenomenon of plastic localization in fatigue was discovered,212 the dislocations structures associated with intense localization have been extensively studied,213–219 both by conventional TEM to characterize the structure, and by in-situ deformation, to observe the mode of operation.220 We will summarize only the main features, since they have

212 A. T. Winter, Phil. Mag. 30, 719 (1974). 213 J. G. Antonopoulos, L. M. Brown, and A. T. Winter, Phil. Mag. 34, 549 (1976). 214 U. Essmann and H. Mughrabi, Phil. Mag. A 40, 731 (1979). 215 U. Essmann, U. Gosele, and H. Mughrabi, Phil. Mag. A 44, 405 (1981). 216 F. Ackermann, L. P. Kubin, J. Lepinoux, and H. Mughrabi, Acta metall. 32, 715 (1984). 217 R. Wang, H. Mughrabi, S. McGovern, and M. Rapp, Mat. Sci. and Eng. 65, 219 (1984). 218 J. Lepinoux and L. P. Kubin, Phil. Mag. A 54, 631 (1986). 219 H. Mughrabi, Acta metall. 31, 1367 (1983). 220 J. Lepinoux and L. P. Kubin, Phil. Mag. A 51, 675 (1985).

268

Y. BRÉCHET AND C. HUTCHINSON

been extensively reviewed in Refs. [221–226]. Since the motion of dislocations is responsible for pattern formation, the most informative studies have been performed by applying a constant plastic strain amplitude to single crystals oriented for single slip. Below a threshold amplitude, the dislocation structure is formed of ‘veins’ rich in dislocations separated by ‘channels’ of equivalent volume fraction, poor in dislocations. This is referred to as the ‘matrix structure’, and the plastic deformation at the macroscopic level is homogeneous in space. When a critical threshold amplitude is attained, plastic deformation becomes strongly localized into so-called ‘persistent slip bands’ (PSB) which exhibit a very regular ‘ladder structure’. This strikingly regular structure shown in Figure V.10214 has been thoroughly studied and is one of the nicest and simplest examples of dislocation patterning in plasticity. It is especially simple compared to the cellular patterns discussed in Section V.15.a–c since it is a structure developed while single crystals are fatigued so that a single burgers vector is activated. This dislocation structure appears to be extremely efficient at carrying the important strains in the Persistent Slip Bands (PSB). Furthermore, the situation corresponds to a true steady state: in a test with constant applied plastic strain amplitude, it corresponds to the saturation of the applied stress amplitude, and to a steady state in the dislocation density. This implies that any creation of dislocation length has to be balanced by an equivalent annihilation process. The overall functioning of the structure is now well understood. The rungs in the ladder structure are of edge character, and the dislocations moving in the channels are of screw character (Figure V.10b). The rungs are formed by dislocation dipoles. Under the applied stress, the dipoles act as sources and emit dislocations in the channels. The screw dislocations moving in the channels leave new edge dislocations in the walls. The creation processes just described are counterbalanced by annihilation processes: dipoles in the walls can collapse by climb, annihilating edge dislocations, and two screw dislocations of opposite signs in the channels can annihilate by cross slip. The annihilation by climb in the walls requires the emission of point defects, which is the origin of the ‘swelling’ of the PSB as a whole, creating extrusions and intrusions. The operating stress of the structure is governed by the stress necessary to emit a dislocation from the wall and to propagate it in the channel. 221 L. M. Brown, in Proceedings of an International Conference on the Dislocation Modelling of

Physical Systems, eds. M. Ashby, R. Bullough, C. S. Hartley, and J. P. Hirth, Pergamon, Gainesville, Florida, USA (1980), p. 51. 222 Z. S. Basinski and S. J. Basinski, Prog. Mat. Sci. 36, 89 (1992). 223 T. Magnin, J. Driver, J. Lepinoux, and L. P. Kubin, Rev. de Phys. 19, 467 (1984). 224 T. Magnin, J. Driver, J. Lepinoux, and L. P. Kubin, Rev. de Phys. 19, 483 (1984). 225 L. M. Brown, Mat. Sci. and Eng. A A285, 35 (2000). 226 L. P. Kubin, C. Fressengeas, and G. Ananthakrishna, in Dislocations in Solids, Vol. 11, eds. F. R. N. Nabarro and M. S. Duesbery, Elsevier, Amsterdam (2002), p. 101.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 269

F IG . V.10. (a) Persistent slip bands (PSB) formed in Cu crystal subject to fatigue loading. The PSB and ‘matrix’ structures are clearly labeled.214 (b) Schematic representation of the dislocation arrangement within a PSB.215

270

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.11. Saturation peak resolved shear stresses of Cu crystals fatigued at various constant plastic strain amplitudes and temperatures.227

Therefore the structure operates at a stress amplitude which scales as the inverse spacing of the ladder rungs. In the domain of strain amplitude where the PSBs are observed, the applied saturation stress amplitude is constant and the volume fraction of PSBs is proportional to the strain227 (Figure V.11). This qualitative description of the functioning of the structure has been cast into the format of a ‘chemical kinetics approach’ for the density of dislocations in the walls and in the channels by Differt and Essmann.177,178 Even though the functioning of the structure is well understood, its spontaneous emergence is still not clear. It has been studied in the framework of the ‘reaction diffusion approach’ in a series of papers by Walgraef and Aifantis, which can be seen as the most sophisticated examples of this type of modeling in plasticity.175,228–232 Two dislocation populations, the fast and the slow, 227 Z. S. Basinski, A. S. Korbel, and S. J. Basinski, Acta metall. 28, 191 (1980). 228 D. Walgraef and E. C. Aifantis, Int. J. Eng. Sci. 23, 1351 (1985). 229 D. Walgraef and E. C. Aifantis, Int. J. Eng. Sci. 23, 1359 (1985). 230 D. Walgraef and E. C. Aifantis, Int. J. Eng. Sci. 23, 1365 (1985). 231 D. Walgraef and E. C. Aifantis, Int. J. Eng. Sci. 24, 1789 (1986). 232 E. C. Aifantis, Solid State Phenomena 3–4, 397 (1988).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 271

F IG . V.12. Bifurcation diagram in the WA model.175 A is the amplitude of the modulation of the immobile dislocation density and is the stress at saturation during cycling. The heavy lines indicate the range of stability of each of the three possible solutions, a uniform structure (0), a ‘vein’ structure (1) and a ‘ladder’ structure (2).

with two different ‘effective diffusion coefficients’ evolve in a coupled manner. In fact, the exact form of the reaction terms is more inspired by the so called ‘Brussellator’5,6 than by any precise dislocation mechanism. The control parameter in this model is the applied stress and a sequence of instabilities is predicted via a ‘Turing-type’ scenario: from a homogeneous distribution, to a ‘rod-like’ distribution (identified as the so-called ‘vein structure’) to a ‘ladder-like’ distribution (Figure V.12). Qualitatively, the sequence is indeed the observed one. However one may be surprised that in the set of equations studied by Walgraef and Aifantis, there are no terms specific to fatigue. It would predict the same kind of patterning in monotonic loading in single slip, which is known not to occur. In the current framework, the only difference in fatigue would be the ability to maintain the strain long enough so that saturation can indeed be reached and the control parameter increased sufficiently. However, very large flow stresses can be obtained in monotonic loading, and the PSB structure is never observed. This highlights the limitations of phenomenological approaches such as those developed in the reaction diffusion approach: it is necessary to incorporate some of the microstructural features which are known to be important.

272

Y. BRÉCHET AND C. HUTCHINSON

F IG . V.13. Simulated dipolar pattern viewed in a section perpendicular to the slip plane and parallel to the slip direction.233

One of these features specific to fatigue is the existence of a large density of dipoles. These dipoles are naturally created by the back and forth motion of dislocations during fatigue loading. An attempt to propose a working mechanism to generate dipole clusters, as incipient features of pattern formation, has been proposed by Kratochvil et al.233–237 The basic idea is that a dipole drifts in a stress gradient generated by the moving screw dislocations. This drift tends to accumulate dipolar loops which in turn enhance the bowing of the dislocations and provoke further accumulation. This mechanism has been seen to operate in the 3D dislocation simulations,233 and the simulation of dipole clustering shown in Figure V.13 shows that it may be considered as a possible mechanism for generating structures. However, we are still far from the nice regular structures we have described for the PSB.

233 A. Franek, R. Kalus, and J. Kratochvil, Phil. Mag. A 64, 497 (1991). 234 J. Kratochvil, Rev. de Phys. 23, 419 (1988). 235 J. Kratochvil and M. Saxlova, Scripta metall. mater. 26, 113 (1992). 236 V. Gregor, J. Kratochvil, and M. Saxlova, Mat. Sci. and Eng. A 234, 209 (1997). 237 J. Kratochvil, Mat. Sci. and Eng. A 309, 331 (2001).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 273

VI. Spatio-Temporal Patterning in Plasticity: The Portevin–Le Chatelier Effect

After having examined the spatial organization of dislocations under various loading conditions, we finally consider a case of spatio-temporal instability in mechanical behavior. In this section, we consider patterning at scales which are much larger (∼mm) than typical dislocation spacings. At this scale, plastic deformation is normally homogeneous. Two stabilizing factors ensure this homogeneity: work hardening and a positive strain-rate sensitivity. When a material deforms, it hardens, and therefore a region which is more deformed tends to deform less easily. This is true for low strains (up to 10%) and is referred to as work hardening. When the strain is larger, and therefore when the stress has increased, the reduction in sample area associated with enhanced plastic deformation may overcome the work hardening rate (which decreases as deformation proceeds): this is the origin of the macroscopic instability called ‘Necking’ which ends any tensile test of a ductile material. Similarly, the textural evolutions associated with large strains may lead to a ‘strain softening’ and to the formation of deformation bands where deformation is much higher than in the rest of the sample. These are both instabilities in mechanical behavior. When a material is deformed at a faster rate, the stress necessary is in general higher and this is referred at as ‘positive strain-rate sensitivity’. However, in some alloys, a negative strain-rate sensitivity can be observed, leading at the same time to a serrated stress-strain curve and to the spatial localization of plastic deformation. This phenomenon, called the ‘Portevin–Le Chatelier’ (PLC)238 effect has been interpreted239 as the interplay between the diffusion of impurity solutes toward dislocations, and de-pinning of the dislocations. The underlying physics is relatively clear. For a given applied strain rate, a given dislocation density spends part of the time waiting at obstacles (other dislocations), and part of the time flying towards another obstacle. While arrested at obstacles, dislocations attract mobile impurity solutes. The greater the concentration of impurities segregated to the dislocation core, the higher the stress necessary to unpin it for further flight. Therefore two characteristic times have to be considered: the diffusion time for impurities, and the waiting time for dislocations. When the diffusion time is very large compared to the waiting time, dislocations move with almost no solute interaction, with a high mobility, and a positive strain-rate sensitivity is observed. When the diffusion time is very small compared to the waiting time, dislocations are permanently loaded with solute, they will have a low mobility, but still a positive strain-rate sensitivity. When the two times are of the same order, the longer the waiting time (lower strain rate), 238 H. Le Chatelier, Rev. de Metall. 6, 914 (1909). 239 A. Cottrell, Dislocations and Plastic Flow in Crystals, England, Carendon, Oxford (1953).

274

Y. BRÉCHET AND C. HUTCHINSON

the greater the concentration of impurities that will segregate to the dislocation, and the lower will be its mobility, meaning a higher stress is needed to make it move at a given velocity: this results in a negative strain rate sensitivity. Since the waiting time depends on the dislocation density and the applied strain rate, and the diffusion time depends on both the temperature and dislocation density, this simple analysis allows for a basic understanding of why the PLC effect is observed only in a closed domain of strain-rates and temperatures, and only beyond a critical strain. This approach has been thoroughly explored, using rate equations for dislocation densities (mobile and immobile) and well established segregation kinetics for impurities at dislocations. The questions of conditions for serrated yielding (another name for PLC) in terms of strain rate, temperature and critical strain can be considered to be solved.240,241 Similarly, a formal description of the range of negative strain-rate sensitivity,242 together with spatial dependences in gradients of the stress or the strain rate243,244 have allowed for a continuum description of the propagative plastic waves. The recent advances in the subject are related to the non-periodic serrated flow, and with the associated spatial aspects of strain localization. In this section we will consider only the detailed features of the spatial organization of plasticity and the statistics of the serrated flow. After summarizing the variety of experimentally observed phenomena, we will outline two recent approaches: PLC as an example of self organized criticality (SOC), and PLC as an example of deterministic chaos. 16. P HENOMENOLOGY OF P ORTEVIN –L E C HATELIER E FFECT The PLC effect has two manifestations: a serrated stress-strain curve and a localized deformation pattern. Three types of stress strain curves are commonly distinguished, and they correspond to three different types of spatial organization of plasticity.245–247 Type A serrations are associated with repetitive continuous propagation of deformation bands, nucleated at one end of the sample. Type B serrations correspond to a hopping propagation of localized bands in the axial direction of the sample. Type C serrations correspond to the nucleation of bands in a spatially non-correlated manner. The typical appearances of the various types of serrations are shown in Figure VI.1. 240 L. P. Kubin and Y. Estrin, Acta metall. 33, 397 (1985). 241 L. P. Kubin and Y. Estrin, Acta metall mater. 38, 697 (1990). 242 P. Penning, Acta metall. 20, 1169 (1972). 243 V. Jeanclaude and C. Fressengeas, Comp. Rendue Acad. des Sci. 315, 7 (1992). 244 V. Jeanclaude and C. Fressengeas, Comp. Rendue Acad. des Sci. 316, 867 (1993). 245 K. Chihab, Y. Estrin, L. P. Kubin, and J. Vergnol, Scripta metall. 21, 203 (1987). 246 E. Pink and A. Grinberg, Mat. Sci. and Eng. 51, 1 (1981). 247 L. P. Kubin, K. Chihab, and Y. Estrin, Acta metall. 36, 2707 (1988).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 275

F IG . VI.1. Examples of the different types of serrated yielding seen in an Al-5Mg (wt.%) polycrystal deformed at room temperature with different imposed strain rates, ε˙ .226 Type C serrations: ε˙ = 5 × 10−6 /s. Type B serrations: ε˙ = 5 × 10−4 /s. Type A serrations: ε˙ = 5 × 10−3 /s.

The stress drops during serrated yielding have also been examined and the statistical analysis248 in various situations can also lead to three types of histograms: the peak shaped distribution (type p), the asymmetric distribution (type as) and an intermediate distribution which presents both a peak and an asymmetry (type i) (Figure VI.2).

F IG . VI.2. Examples of ‘stress-drop’ histogram shapes for room temperature deformation:249 (a) polycrystalline specimen, ε˙ = 1.3 × 10−5 /s (type p); (b) single crystal, ε˙ = 1.3 × 10−5 /s (type i); (c) polycrystalline specimen, ε˙ = 6.1 × 10−4 /s (type as). 248 M. A. Lebyodkin, Y. Brechet, Y. Estrin, and L. P. Kubin, Phys. Rev. Letts. 74, 4758 (1995). 249 M. Lebyodkin, L. Dunin-Barkowskii, Y. Brechet, Y. Estrin, and L. P. Kubin, Acta mater. 48, 2529

(2000).

276

Y. BRÉCHET AND C. HUTCHINSON

F IG . VI.3. Classification of the types of serrations and stress drop statistics in an (˙ε, 1/T) map.249 The boundaries between various regions are drawn in a semi-schematic way. The area where the PLC effect occurs is delineated by the horseshoe-shaped curve.

The parameters to be considered in a first approximation as controlling the characteristics of the PLC effect are the strain rate and temperature. It is convenient to map the domain in which serrated yielding occurs in terms of the type of instability and the type of stress-drop distribution. An example for the Al-Mg system is shown in Figure VI.3. In the following sections we will consider two types of models developed to describe this rich phenomenology. The first (Section VI.17) relies on a phenomenological description, and considers as essential ingredients the negative strainrate sensitivity and the spatial coupling between slices of material deforming at different rates. The second model (Section VI) delves deeper into the detailed dynamics of dislocations responsible for the phenomena. 17. S TATISTICAL A NALYSIS OF S ERRATED F LOW: A N E XAMPLE OF S ELF O RGANIZED C RITICALITY (SOC) The existence of a negative strain-rate sensitivity, which is the origin of the PLC instabilities, is reminiscent of the behavior of a dynamic friction coefficient which decreases when the sliding velocity increases. This behavior itself generates a similar type of instability during the sliding of two solids, the ‘stick-slip’

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 277

F IG . VI.4. The distribution density function D(s) for an Al-Mg single crystal deformed at 120 ◦ C and ε˙ = 1.3 × 10−5 /s.249 The dotted line corresponds to the exponent α ≈ 1 in the dependence D(s) ≈ s −α .

instability.250–252 This sliding instability is characterized by a power law distribution for the jump in the force/displacement curve. Similarly, the distribution of stress drops, when the distribution is asymmetrical, also exhibits a power law behavior as shown in Figure VI.4. A simple model for the power law behavior in stick-slip has been proposed in the physics community: a set of blocks coupled by springs, with an appropriate friction law.250–252 By analogy a simple model has been proposed for the PLC effect:252,253 the material is ‘sliced’ into layers which may each deform at different rates. The relation between the local stress and the strain-rate is an N shaped curve which is obtained from the theory of dynamic strain aging (Figure VI.5). The local stress is the applied one corrected for ‘incompatibility stresses’ stemming from the difference in local strains. The equivalent of the position in Langer’s ‘stick-slip’ model is the strain, and the equivalent of the friction law is the N-shaped stress-strain-rate curve. The equation governing the strain in each slice (εi ) can be written: σ = hεi + F (˙εi ) − K (εi−1 − εi ) + (εi+1 − εi ) . (6.1) 250 R. Burrige and L. Knopoff, Bull. Seis. Soc. Amer. 57, 341 (1967). 251 J. M. Carlson and J. S. Langer, Phys. Rev. Letts. 62, 2632 (1989). 252 J. M. Carlson and J. S. Langer, Phys. Rev. A 40, 6470 (1989). 253 M. Lebyodkin, Y. Brechet, Y. Estrin, and L. Kubin, Acta mater. 44, 4531 (1996).

278

Y. BRÉCHET AND C. HUTCHINSON

F IG . VI.5. (a) Schematic illustration of the coupled block model sliding with a strain-rate dependent friction (F (˙ε)) and deformed with a constant total imposed strain rate ε˙ a . (b) The viscoplastic Penning’s function F (˙ε) for an Al-Mg alloy.226 In the intermediate range of strain rates, the portion of the negative slope of F describes the negative strain-rate sensitivity associated with the PLC effect.

F IG . VI.6. Schematic phase diagram of the computer model behavior illustrating the types of plastic localization and stress drop statistics.249 The dashed line separates domains of different spatial nature of strain localizations. ε˙ a1 and ε˙ a2 denote the lower and upper bounds of the applied strain rate interval where the PLC effect occurs.

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 279

F IG . VI.7. The normalized distribution D(s) of stress drops for a simulated deformation curve.249 The dotted line corresponds to the exponent α ≈ −1 in the dependence D(s) ≈ s −α .

The first term is the work hardening of the slice, the second describes the strainrate sensitivity, and the third term describes the spatial coupling. This model should be able to describe not only the power law behavior in the stress drops, but also the conditions under which the PLC effect is observed (in terms of applied strain rate and test temperature). It should also predict the type of spatial localization expected. The model is solved numerically, and indeed presents the same variety of behavior as observed experimentally. When the strain-rate is increased, the stress drop distribution changes from bell-shaped to a continuously decreasing one (cf. Figure VI.2). The asymmetric distribution is indeed a power law, and the exponent depends on the coupling constant between the blocks (slices of material). The value of this coupling constant is of the order of the elastic modulus and confirms the interpretation of the coupling as resulting mainly from elastic incompatibilities. The plastic localization which is observed in the numerical simulation also evolves with increasing applied strain-rate, from spatially uncorrelated (Type C) to spatially correlated, hopping or propagating (Type B and A). The band structure predicted in each of the three cases, in relation with the stress strain curve is shown in Figure VI.8. The velocity of the propagating band has also been computed with this simple model and it is found to exhibit a non-monotonic behavior. Within this framework, the statistical behavior of the PLC instability, namely the existence of a power law distribution of stress drops can be seen, in certain

280

Y. BRÉCHET AND C. HUTCHINSON

F IG . VI.8. Stress versus time curve and the attendant deformation band patterns for (a) ε˙ a = 10−5 s −1 , (b) ε˙ a = 5 · 10−5 s −1 and (c) ε˙ a = 4 · 10−4 s −1 .253 (Continued on the next page.)

domains, as an example of Self Organized Criticality.22,254–256 However, some other experimental findings suggest another type of analysis. 254 P. Bak, C. Tang, and K. Wiesenfeld, Phys. Rev. Letts. 59, 381 (1987). 255 P. Bak, C. Tang, and K. Wiesenfeld, Phys. Rev. A 38, 364 (1988). 256 P. Bak, How Nature Works: The Science of Self-Organized Criticality, Oxford University Press,

Oxford, England (1997).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 281

F IG . VI.8. (Continued.)

F IG . VI.9. Dependence of the band propagation velocity on the imposed strain rate for three values of the coupling constant for h = 103 MPa. Curve 1: k = M, Curve 2: k = 0.5M and Curve 3: k = 0.27M. A demarcation line between the regions of the true and apparent (relay-race) propagation is shown.253

282

Y. BRÉCHET AND C. HUTCHINSON

18. P ORTEVIN –L E C HATELIER E FFECT: A N E XAMPLE OF D ETERMINISTIC C HAOS The details of the stress strain curve appear to be ‘noisy’ but what is the structure of this noise? As detailed in Ref. [226], this curve is considered as a scalar time series on which the standard techniques of chaos analysis are applied. From a series of N values of stress taken at regular intervals of time t, {σ (kt), k = 1 to N}, one constructs a vector X(k) of M values corresponding to a sampling every Lt, starting from the point σ (kt), X(k) = {σ (k + nL)t, n = 0 to M − 1}. The mapping X(k + 1) = F (X(k)) in the M-dimensional space is known as the ‘reconstructed attractor’. The embedding dimension M is a priori unknown. If M is smaller than the space in which the ‘true attractor’ lives, two points which have different orbits in the ‘true attractor’ will seem to be on the same orbit on the ‘reconstructed one’. This will influence the correlation function, C(r) namely the fraction of vectors X(k) in the M dimensional space which are closer than a distance r. When we have a fractal attractor, C(r) shows a power law behavior C(r) = r ν . The correlation dimension ν depends on the dimension M of the space in which the reconstructed attractor is built. When this space is made larger and larger (M increasing), ν tends towards a limiting value. The value of M above which the correlation dimension ceases to evolve indicates the number of variables necessary to describe the deterministic chaos. This method257 has been applied to experimental data on Portevin–Le Chatelier serrated flow. The dimension of the attractor, as obtained from the correlation function in the phase space, is shown to converge toward a value of 3.2 when the dimension M is increased beyond 5 (Ref. [258], Figure VI.10). This indicates that indeed the behavior of the time series studied is an example of deterministic chaos, and that no more than 5 variables are required to analyze this behavior. Well before this experimental proof of deterministic chaos in PLC (serrated yielding) was given, a model was proposed by Ananthakrishna,259–264 with evolution equations for the densities of mobile dislocations, of immobile dislocations and of dislocations interacting with impurity clouds, to which an equation for the stress was added. These four variables indeed show chaotic behavior. 257 F. Takens, Dynamical Systems and Turbulence, Springer-Verlag (1981). 258 S. J. Noronha, G. Ananthakrishna, L. Quaouire, C. Fressengeas, and L. P. Kubin, Int. J. Bifur.

Chaos 7, 2577 (1997). 259 G. Ananthakrishna and M. C. Valsakumar, J. Physics D 15, 171 (1982). 260 G. Ananthakrishna and M. C. Valsakumar, Phys. Letts. A 95A, 69 (1983). 261 G. Ananthakrishna, Solid State Phenomena 3–4, 357 (1988). 262 G. Ananthakrishna, Solid State Phenomena 23–24, 417 (1992). 263 G. Ananthakrishna, Scripta metall. mater. 29, 1183 (1993). 264 M. S. Bharathi, S. Rajesh, and G. Ananthakrishna, Scripta mater. 48, 1355 (2003).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 283

F IG . VI.10. Log-log plot of the correlation integral C(r) as a function of distance r in the phase space.258 Note the convergence of the slope to 3.2 (dotted line) as the embedding dimension is increased (arrow) from two to five.

A systematic statistical analysis of experimental data has shown that, depending on the loading conditions, the stress drops showed either deterministic chaos, or power law behavior, the transition being the two regimes being characterized by a multi-fractal behavior.265–269 The attractor reconstructed from experimental data on Al-Mg polycrystals, and the prediction of the model proposed by Ananthakrishna, shown in Figure VI.11 shows striking similarities, indicating that the non-linearities in this set of equations are relevant to capture the physics of the problem.270 265 G. Ananthakrishna, C. Fressengeas, M. Grosbras, J. Vergnol, C. Engelke, J. Plessing, H. Neuhauser, E. Bouchaud, J. Planes, and L. P. Kubin, Scripta metall. mater. 32, 1731 (1995). 266 G. Ananthakrishna, S. J. Noronha, C. Fressengeas, and L. P. Kubin, Phys. Rev. E 60, 5455 (1999). 267 G. Ananthakrishna, S. J. Noronha, C. Fressengeas, and L. P. Kubin, Mat. Sci. and Eng. A 309, 316 (2001). 268 M. Lebyodkin, C. Fressengeas, G. Ananthakrishna, and L. P. Kubin, Mat. Sci. and Eng. A 319, 170 (2001). 269 M. S. Bharathi, M. Lebyodkin, G. Ananthakrishna, C. Fressengeas, and L. P. Kubin, Phys. Rev. Letts. 8716, (2001). 270 S. Kok, M. S. Bharathi, A. J. Beaudoin, C. Fressengeas, G. Ananthakrishna, L. P. Kubin, and M. Lebyodkin, Acta mater. 51, 3651 (2003).

284

Y. BRÉCHET AND C. HUTCHINSON

F IG . VI.11. Type B bands. Strange attractor from experiment (a) and from model (b) in a 3D space.270 Note the striking similarity.

The spatial features of the chaotic regime need further investigation to be fully understood, as well as the mechanisms for the cross over between chaos and SOC with increasing strain rate.270–272

271 G. Ananthakrishna, M. S. Bharathi, et al., Phys. Rev. E, in press (2004). 272 P. Hähner, A. Ziegenbein, E. Rizzi, and H. Neuhauser, Phys. Rev. B 65 (2002).

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 285

VII. Concluding Remarks

As we bring this chapter to a close, we wish to stress some features of the patterning problems we have examined which would certainly benefit from the input of the physics community. However, before these ‘open problems’ are outlined, we want to insist on the necessity to incorporate in any modelling those specific features which are experimentally well established. Non-linear physics has justly shown that some universal behavior can be derived without knowledge of the precise details of the equations involved and of the microscopic mechanisms. Bifurcation theory, in both its linearized and non-linear (amplitude equations) versions and Chaos theory have shown that it is possible to generate a large variety of behavior with a limited number of ingredients. Similarly, Self Organized Criticality has been claimed to provide a very general framework. However, as outlined in the previous examples, some specific features of the problems have to be incorporated: the N shape of the stress/strain rate curve in Portevin–Le Chatelier modelling brings some new features to the richness of the observed behavior and the fact that the lamellar structure in discontinuous precipitation involves two different driving forces depending on the nature of the interface has important consequences on the removal of the velocity/spacing degeneracy. The analogies between problems (PLC and solid friction, discontinuous precipitation and eutectic solidification, dislocation self-screening and ion screening in a 2D coulomb gas) have both their strengths and weaknesses. Part of the challenge in applying the methods of non-linear physics is to identify the necessary ingredients provided by a detailed knowledge of the underlying mechanisms, without being overflowed by too many details. In the problems of patterning of lamellar structures in the solid state, a key issue is to identify precisely the differences (and implication) between the solid state structures and those resulting from solidification. One of the aspects certainly lies in the difference between solids and liquids, both in their ability to sustain shear, and in the requirements imposed by crystallography. Misfit stresses may modify the driving forces, but may also drive the details of the geometry of the pattern. The crystallography of the interface determines both its energy and its mobility. In a crystalline solid, depending on the driving force, an interface can move either by lateral propagation of steps, or by normal growth. This behavior is probably associated with the ‘stop and go’ motion which has been described in Section III.7.a, but the macroscopic consequences on the patterning are still to be explored. Another feature is of course the fact that, not a single wavelength but a range of wavelengths is experimentally observed. The limited data available in the literature indicates a scaling behavior for the population of spacings observed. These results are still waiting to be modelled. Another feature, also related to the spacing selection problem, is the transition between the patterns which are nucleated and those which are growing, or the adjustment mechanisms when a change

286

Y. BRÉCHET AND C. HUTCHINSON

in the transformation conditions requires a modification of the interlamellar spacing (pattern repeat distance). Are the mechanisms operating in eutectic spacing selection still valid in systems where the anisotropy of the interface properties would make difficult any ‘tilt wave’? On the whole, patterning in phase transformations in the solid state is nevertheless on relatively solid grounds, in the sense that the relevant equations are available, and agreed upon by the community. Comparatively less advanced is the spatial patterning of structural defects. In spite of decades of experimental work and many attempts to developed models for these problems, the state of ‘irradiation patterning of dislocations’ outlined in Section V.14, where there is a relative consensus on the equations to be solved, is far from general. The role of long range stresses seems to be central to many of these ‘structural patterning’ problems. It seems crucial to explain how random nucleation of voids can lead, above a critical density, to a well organized lattice. The case of dislocation patterning in plasticity is far from being solved. The ‘reaction diffusion’ approaches have shown their limitations, due to the difficulty in mimicking a glide process by a diffusion-like description. The energetic approaches, as long as they ignore the fact that the system is maintained far from equilibrium, are unlikely to provide further contributions. Both the short range interactions and the long range interactions must be accounted for. A key issue seems to be the self-screening of dislocations. Like in ionic solutions, one could envisage a population of dislocations as a set of positive and negative entities, in principle able to screen each others field. Due to the specific forces between dislocations, it would be a sort of ‘Coulomb Gas’ with logarithmic interaction energies. But unlike ionic solution, this screening cannot be obtained from standard statistical physics: the motion of dislocations is mainly restricted to glide in certain directions, their number is not conserved since they can annihilate by pairs, and since they are generated, not spontaneously, but by source mechanisms. A proper theory of screening under such restrictions is still to be developed. Another issue put forward recently, which brings a new light to these problems, is a systematic method to account for fluctuations in plasticity. Already these approaches have led to interesting results (e.g., Refs. [133,206]). The incorporation of these ingredients together with the local events which control both the pinning and the annihilation and multiplication of dislocations is a promising route. It is likely that the intensive computer simulations developed in the last decade for dislocation dynamics will have to incorporate these stochastic features to overcome their current limitations. In the cases we have reported, spatio-temporal patterning in plasticity known as the Portevin–Le Chatelier phenomena is specially encouraging and interesting. The set of equations at the level of dislocation dynamics can be seen as sufficiently consensual to provide a realistic description of macroscopic data such as the critical strain to observe the phenomenon of serrated flow. A continuum description of band propagation has been proposed, so the ‘simplified regular PLC

DEFECT-INDUCED DYNAMIC PATTERN FORMATION IN METALS AND ALLOYS 287

effect’ can be said to be reasonably well understood. When one delves deeper into the details of the statistics of stress jumps, two regimes have been identified, corresponding respectively to a type of ‘Self Organized Criticality’ with well defined scaling laws, and to a regime of deterministic chaos, corresponding to a correctly reproduced ‘strange attractor’. However, the transition from a regime in which an infinite number of variables is required to describe the statistics, to a regime where a finite and small number of variables is sufficient, is still not understood. The phenomenon being well studied experimentally and the models to describe it at a microscopic level being reasonably safe, it could be very promising to use this problem as a prototype for understanding the transition from deterministic chaos to SOC. In any case, the variety of the patterning phenomena observable in the solid state, and associated with structural defects is certainly a driving force for new modelling approaches which could be both respectful of the underlying mechanisms but not obsessed by them.

This page intentionally left blank

Author Index

Numbers in parentheses are reference numbers and indicate that an author’s name is not cited in the text.

Asamitsu, A., 114(266) Asamitsu, Z., 108(255) Ashby, M. F., 261(174) Aso, N., 49(136, 137), 60(169, 170) Assmus, W., 46(126) Asundi, M. K., 193(28) Avella, A., 6(23) Avlonitis, M., 266(207)

A Aaronson, H. I., 196(42), 198(53) Aarts, J., 2(2) Abdou, S., 219(88) Abrahams, E., 13(46), 73(195), 160(374) Abrikosov, A. A., 9(28) Acker, F., 34(106) Ackermann, F., 267(216) Adams, G., 67(184) Adelmann, P., 12(35), 174(410) Adrian, H., 60(168) Adroja, D. T., 119(274) Aeppli, G., 62(177), 91(218), 119(274) Aifantis, E. C., 261(175), 266(207), 270, 271 Albessard, A. K., 17(64), 20(72, 73) Alexander, M., 174(410) Allen, J. W., 17(66, 67), 50(138) Amici, A., 61(174) Amir, Q. M., 212 Amodeo, R. J., 263(188, 189) Ananthakrishna, G., 268(226), 282, 283, 284(271) Anderson, M. P., 235(118–120) Anderson, P. W., 59(160), 108(257), 125(286) Andersson, P. H., 50(141) Andres, K., 2 Anisimov, V. I., 48(132), 125(290), 131(303) Antonopoulos, J. G., 267(213) Antonov, V. N., 13(45), 97(239), 125(290) Aoki, H., 17(64), 20(72, 73), 74(197), 79(202), 85(210, 211), 86(213), 87(215), 90(217) Appel, J., 59(152) Argon, A. S., 261(174) Arko, A. J., 50(141) Armstrong, P. E., 17(66, 67)

B Baas, J., 94(232) Bak, P., 280(254–256) Balatsky, A. V., 59(163) Balents, L., 146(327, 330) Balluffi, R. W., 234(110) Barbu, A., 249(140, 141) Bareiter, S., 135(311) Barker, I., 256(163) Basinski, S. J., 268(222), 270(227) Basinski, Z. S., 268(222), 270(227) Baumann, S. F., 196(41) Bay, B., 255(160) Bay, K., 258(165), 266(208), 267 Beaudoin, A. J., 283(270) Beck, H., 91(219) Bedell, K. S., 160(375) Bednorz, J. G., 2(5) Bellon, P., 184(10, 11) Beni, G., 92(222) Benner, H., 87(215) Benoist, P., 255(159) Benzerga, A. A., 265(202) Berge, P., 182(2) Berk, N. F., 33(97) Bernardini, J., 193(34) Bernert, A., 98(241), 99(242, 244) Bernhoeft, N., 49(136), 60(170), 62(178), 66 Bernhoeft, N. R., 34(108) 289

290

AUTHOR INDEX

Bertrand, G., 183(9) Bethe, H., 8, 85 Betouras, J., 140(319) Bharathi, M. S., 282(264), 283(269, 270), 284(271) Billinge, S. J. L., 109(258) Binder, K., 185(14) Biroli, G., 159(368) Blaha, P., 127(295) Bley, F., 243(138) Bogdanov, P. V., 154(357) Bogel, A., 198(65), 219, 220 Bolze, G., 198(62) Bonitz, M., 67(185) Bonner, J. C., 91(219), 93, 130(302) Bonsall, L., 70(189) Borsa, F., 126(291) Bouchaud, E., 283(265) Boucher, J. P., 103(247) Bougourzi, A. H., 79(204) Bozorth, R. M., 34(107) Brandt, W. H., 198(45), 203 Brechet, Y., 184(12), 212(82), 215(85), 232(105–107), 235(124, 125), 239(129, 130), 242(133), 243(135–138), 249(142), 264(192), 265(202), 275(248, 249), 277(253) Brechet, Y. J. M., 186(18), 198(66) Bredl, C. D., 2(2) Brener, E. A., 182(4) Brimhall, J. L., 249(144) Brodsky, M. B., 34(105) Broholm, C., 91(218) Bross, S., 266(205) Brown, D., 209(79) Brown, J. D., 95(234) Brown, L. M., 267(213), 268(221, 225) Brugger, T., 12(35) Bruls, G., 24(84) Bucher, E., 59(156, 157) Budnick, J. I., 34(104) Bullough, R., 249(152), 253 Bulut, N., 159(370) Bünemann, J., 164(395) Burke, J. E., 235(113) Burrige, R., 277(250) Butler, E. P., 196(38) Butterfield, M. T., 50(141)

C Cahn, J. W., 198, 203–206, 210, 212, 213, 215, 218, 220, 222, 230, 231, 235(116) Caliebe, W., 113(265) Callen, E., 125(288) Canals, B., 131(305) Canfield, P. C., 17(66) Canova, G., 263(185), 264(190–192) Carbotte, J. P., 155(365) Carlson, J. M., 277(251, 252) Carpy, A., 92(227) Cavadini, N., 38(115) Ceperley, D. M., 71(191), 73(193) Chaboussant, G., 119(274) Chaffron, L., 184(11) Chandrasekhar, S., 182(1) Chatterji, T., 94(229), 99(244), 103(247), 109(259), 113(265), 119(272, 273, 275, 276), 120(278) Chaudhari, P., 161(376) Cheetham, D., 193(29, 31), 207 Cheynet, M. C., 212(82) Chi, E. O., 113(264) Chihab, K., 274(245, 247) Choi, H. S., 113(264) Choi, S., 225(92, 94) Christensen, N. E., 20(71), 172(405) Chubukov, A. V., 163(381) Chuk, T., 154(358) Cichorek, T., 22(79), 39(119), 74(197), 86(213) Claessen, R., 164(395) Cleveringa, H. H. M., 265(198) Cliff, G., 225(93) Cline, H. E., 229(102) Coldea, R., 38(117) Coleman, P., 39(120) Collins, R. T., 161(376) Colten, R. A., 209(77) Condat, M., 264(192) Continentino, M. A., 32(94), 45(125) Cooper, B. R., 59, 62(175), 66, 70 Cottrell, A., 273(239) Courtney, T. H., 227(99) Cox, D. L., 15(52) Craco, L., 48(135), 131(304) Cross, J. O., 138(315) Cross, M. C., 92(224), 102

AUTHOR INDEX Cullen, J. R., 125(288) Custers, J., 39(120), 74(197), 86(213) Czjzek, G., 12(35) Czycholl, G., 162(378) D Dagotto, E., 122(281) Daliachaouch, Y., 17(66) d’Ambrumenil, N., 75(198), 85(212) Darken, L. S., 193(26) Das, A., 193(32, 33) de Boer, P. K., 110(260) de Groot, R. A., 110(260) de Visser, A., 24(84), 47(130) deBoer, J. L., 94(232) DeGroot, S. R., 188(24) Delin, A., 50(141) Dender, D. C., 91(218) Denlinger, J. D., 17(66, 67), 21 des Cloizeaux, J., 79 Devereaux, T. P., 154(358) Devincre, B., 264(192, 193, 196, 197) Dhalenne, G., 113(265), 119(272, 273, 275), 120(278) Dho, J., 113(264) Differt, K., 261(177, 178), 270 Dischner, M., 97(240), 105(252) Dmitriev, D. V., 91(221) Doherty, R. D., 240(131) Doniach, S., 14(49), 33(98), 39, 40(121) Donnevert, L., 23(82) Dönni, A., 60(172) Dooryhee, E., 138(315) Driver, J., 268(223, 224) Dubuisson, P., 249(142) Ducastelle, F., 164(382, 383) Duly, D., 212, 215, 220 Dunin-Barkowskii, L., 275(249) Durakiewicz, T., 50(141) Dzyaloshinski, I. E., 9(28) E Eberhardt, W., 147(332) Ebihara, T., 20(72) Eder, R., 159(372) Edington, J. W., 205(69)

291

Edwards, D. M., 164(390, 391) Efremov, D. V., 57(147) Ehm, D., 16(55), 164(395) Ehrenreich, H., 153(340, 343) Ehrhart, P., 249(143, 151) ElBoragy, M., 219(88) Elgazzar, S., 51(142) Elliott, R. J., 153(342) Eloirdi, R., 171(403) Endoh, Y., 60(169, 170, 172), 113(263), 117(271), 121(279) Engelke, C., 283(265) Engelsberg, S., 33(98) Enz, C. P., 33(99) Eriksson, O., 50(141) Erkelens, W. A. C., 20(70) Eschrig, H., 13(45), 97(239) Eschrig, M., 155(362, 364) Essmann, U., 261(177, 178), 267(214, 215), 270 Estrin, Y., 261(181), 263(185), 274(240, 241, 245, 247), 275(248, 249), 277(253) Evans, J. H., 249(145–147, 149) Eyert, V., 127(296) Eyre, B. L., 249(148, 152) F Fagot-Revurat, Y., 95(236) Fak, B., 90(217) Falakshahi, H., 71(192) Falicov, L. M., 164(393) Farrell, K., 249(150) Faulhaber, E., 22(79) Fauth, F., 84(209), 138(315) Fay, D., 59(152) Fedorov, A. V., 155(363) Feild, C., 161(376) Fertig, W. A., 59(157) Filinov, A. V., 67(185) Fink, J., 174(410) Firsov, Y. A., 115 Fischer, M., 96(237) Fischer, Ø., 61(173) Fischer, P., 60(171) Fisher, D. S., 92(224) Fisher, M. E., 93, 102, 130(302) Fisher, M. P. A., 146(327, 330) Fisher, R. M., 193(26)

292

AUTHOR INDEX

Fisk, Z., 2(3, 4), 17(66, 67), 34(106) Flandin, L., 243(135) Fleck, N. A., 265(201) Flouquet, J., 20(70), 47(130) Fournelle, R. A., 227, 231 Fradkin, E., 140(320) Franek, A., 272(233) Franz, W., 2(2) Fratzl, P., 185(14, 15) Freeman, A. J., 34(105) Freericks, J., 154(352) Fressengeas, C., 268(226), 274(243, 244), 282(258), 283(265–270) Freye, D. M., 39(118) Fridberg, J., 222(89, 90) Friedel, J., 6, 81 Friedman, L. H., 264(195) Fröhlich, H., 59 Frye, J. H., 209(78) Fuchizaki, K., 235(121), 237 Fuji, Y., 94(233), 103(248, 249) Fujimori, A., 6(22), 108(254), 127(294), 135(312) Fujimori, S., 50(139), 171 Fujimoto, S., 132(309) Fujioka, H., 117(271), 121(279) Fujiwara, K., 127(297, 298) Fukuyama, H., 70(188) Fulde, P., 5(14), 9(29), 11(31, 33), 12(36), 13(41, 42, 45), 17(62), 27(88, 89), 35(109), 46(127, 128), 49(137), 53(144), 57(147), 59(153–155, 157), 61(174), 63(180), 74(196), 75(198), 81(205), 85(212), 87(216), 97(239), 99(242–244), 129(299), 136(313), 137(314), 140(318, 319), 145(323), 146(324), 154(346, 353–356), 164(396, 397), 165(401), 174(407, 408) Furrer, A., 38(115) Furukawa, N., 119(277), 139(316) G Gajewski, D. A., 126(291) Galy, J., 92(227) Garst, M., 46(129) Gaskell, T., 149 Gebhard, F., 164(395)

Geerk, J., 61 Gegenwart, P., 23(82, 83), 39(119, 120), 74(197), 86(213), 90(217) Geibel, C., 16(55), 22(79), 23(82, 83), 39(119, 120), 49(137), 60(171), 94(230), 95(235), 96(237), 97(238, 240), 105(252) Georges, A., 69(186) Gerhardt, W., 34(103) Ghoniem, N. M., 253, 263(188, 189) Girvin, S. M., 146(327) Gogolin, A. O., 12(37) Goldman, A. I., 126(291) Goremychkin, E. A., 22(77) Gorkov, L. P., 9(28) Gosele, U., 267(215) Goto, T., 76(199), 78(201) Gottstein, G., 235(117) Gottwick, U., 20(69) Gouder, T., 171(403) Graebner, J. E., 2 Graf, J., 162(380) Grauel, A., 60(171) Greer, A. L., 232(108, 109) Gregor, V., 272(236) Grenier, B., 103(247) Grest, G. S., 235(118, 119) Grewe, N., 20(69) Grin, Y., 94(229), 129(299) Grinberg, A., 274(246) Gröber, C., 159(372) Groma, I., 243(135) Gros, C., 97(238), 105(250) Grosbras, M., 283(265) Grosche, F. M., 39(118) Grüner, G., 69(187) Gu, G., 154(357) Gu, G. D., 155(363) Gu, Q., 40(122) Gu, T., 126(291) Güdel, H. U., 38(115) Güntherod, G., 96(237) Gupta, S. P., 212 Gust, W., 193(32–35), 196(36), 198(65), 202(68), 205(70–72), 211(80), 215, 219, 220, 235(125) Gutzwiller, M. C., 6, 164 Guyot, P., 243(135–137) Gweon, G. -H., 17(66, 67), 162(380)

AUTHOR INDEX H Haase, R., 188(25) Haayman, P. W., 3(8), 124 Habicht, K., 38(115) Hackenberg, R. E., 197(44), 211(81) Haen, P., 47(130) Haga, Y., 49(136), 52(143), 65(181), 66(183), 77(200) Hagel, W. C., 206(75), 222 Hähner, P., 258(165), 266, 267, 284(272) Haken, H., 183(8) Haldane, F. D. M., 129 Halperin, B. I., 71(190) Hammar, P. H., 91(218) Hanke, W., 159(371, 372) Hansen, N., 255(160), 256(163), 260(170) Haque, M., 73(194) Harasawa, A., 164(395) Harima, H., 127(297) Harrison, N., 86(213) Hase, M., 92(225) Hasegawa, H., 108(257) Hasegawa, T., 260(172) Hasselmann, N., 57(147) Hauptmann, R., 95(235), 96(237) Hayden, S. M., 34(108) Heeger, A. J., 12(38) Heiniger, F., 59(156) Heitler, W., 3 Held, K., 17(59) Helfrich, R., 23(82), 85(211), 87(215) Hermele, M., 146(330) Hertz, J. A., 34, 164(390, 391) Herzig, C., 193(34) Hettler, M. H., 159(367, 369) Hewson, A. C., 15(50) Hidaka, H., 127(297) Hiess, A., 49(136), 60(170), 103(247), 119(275) Hillert, M., 198, 202, 203, 205–207, 209, 210, 212, 215, 218, 222, 225, 235(115), 236, 237 Hinkel, C., 135(311) Hinma, T., 52(143) Hino, O., 115(268) Hinze, P., 23(83) Hirai, K., 164(397) Hirooka, S., 154(347)

293

Hirota, K., 113(263), 117(271), 121(279) Hirsch, J. E., 59(158) Hirst, L. L., 59(153) Hirth, J. P., 264(194) Hisazaki, Y., 77(200) Hoang, A. T., 110(261) Höck, K. -H., 127(296) Hoffmann, J. U., 120(278) Hohlwein, D., 120(278) Holt, D. L., 256(162), 260 Holtzberg, F., 161(376) Honig, J. M., 135(311) Horibe, Y., 139(316) Horn, R., 23(82) Horn, S., 127(296) Hornbogen, E., 198(56) Horsch, P., 93(228) Howe, L., 249(141) Huang, C. Y., 34(106) Hubbard, J., 2, 6–8, 14, 27, 32, 68, 69, 74, 85, 86, 97, 98, 100, 105, 108, 110, 111, 125, 130, 132, 144, 148, 151–155, 157–161, 163–165, 167, 169, 172, 174–177, 179 Huber, F., 171(403) Hückel, E., 3 Hüfner, S., 16(55), 147(331) Hughes, D. A., 240(131), 255(160) Hull, F. C., 209(77), 234(112) Humphreys, F. J., 186(21), 235(122, 123), 240(131), 242(132) Hunderi, O., 236, 239 Hunt, J. D., 198(51) Hur, K. L., 131(303) Hur, N. H., 113(264) Hüser, D., 34(103) Hutchinson, C. R., 211(81) Huth, M., 60(168) Hybertsen, M. S., 172(405) I Igarashi, J., 164(387, 388, 396, 397) Ihle, D., 125(289) Ikeda, H., 154(357) Ikeda, N., 139(316) Illy, J., 262(183) Imada, M., 6(22) Inada, Y., 52(143)

294

AUTHOR INDEX

Ishibashi, H., 139(316) Ishida, K., 66(183) Ishihara, S., 117(271), 154(359, 361) Ishikawa, M., 61(173) Isobe, M., 92(226), 94(233), 103(248, 249), 105(251) Isoda, M., 124(285) Iwasa, K., 11(32), 77(200), 79(202), 90(217) Izawa, K., 66(182) J Jackeli, G., 109(259), 121(280) Jackson, K. A., 198(51) Jaclic, G., 42(123) Jager, W., 249(143, 151) Jaime, M., 86(213) Janecek, M., 243(136, 138) Jarrell, M., 154(352), 159(367, 369), 160(373) Jayprakash, C., 16(56, 57) Jeanclaude, V., 274(243, 244) Jedrak, J., 56(145) Jeevan, H., 22(79) Jegoudez, J., 103(247) Jensen, D. J., 240(131) Jensen, H. J., 187(22) Jensen, J., 35(110, 111), 62(176) Jepsen, O., 94(229) Jobst, A., 94(230) Johnson, J. D., 87(214) Johnson, P. D., 155(363) Johnston, D. C., 123(282), 124(283, 284), 126(291) Jonas, J. J., 240(131) Jones, B., 16(58) Jourdan, M., 60(168) Joyce, J. J., 50(141) Julian, S. R., 17(65), 20(74), 39(118) K Kadowaki, K., 76, 126 Kagami, C., 103(248) Kaganov, M. I., 23(81) Kaiser, A. B., 46(128) Kajihara, M., 225(92, 94) Kakehashi, Y., 154(344–346, 348, 349, 353, 355, 356), 165(401), 179

Kakizaki, A., 164(395) Kakol, Z., 135(311) Kakurai, K., 60(172), 103(248) Kalmeyer, V., 146 Kalus, R., 272(233) Kampe, J. C. M., 227(99) Kampf, A. P., 152(336, 337) Kampmann, R., 185(13) Kanamori, J., 6, 164 Kanao, R., 115(268) Karbach, M., 79(204) Kasahara, Y., 65(181) Kassner, M. E., 240(131) Kastrinakis, G., 162(379) Kasuya, T., 13(43), 17(60), 180 Kato, K., 139(316) Katsnelson, M. I., 164(394) Katsufuji, T., 133(310), 139(316) Kaur, I., 193(35), 211 Kawabata, A., 14(48), 34(100) Kawakami, K., 135(312) Kawakami, N., 48(133) Kawasaki, K., 235(121) Kawatra, M. P., 34(104) Keh, A. S., 255(161) Keller, J., 9(29), 59(154, 155, 157) Keller, S. A., 154(357) Kendziora, C., 155(363) Khachaturian, A. G., 185(17) Khomskii, D. I., 100(245) Kikuchi, M., 225 Kim, W. S., 113(264) Kimura, N., 66(183) Kimura, T., 113(262, 263), 119(274) King, C. A., 20(75) King, W. E., 240(131) Kirkaldy, J. S., 198(55, 61, 62), 206(74), 208, 215 Kirkpatrick, S., 153(340) Kishio, K., 154(357) Kita, H., 60(172) Kitaoka, Y., 15(51), 66(183) Kleinmann, L., 165(398) Klinger, L., 198(66), 215(85), 216, 218, 220, 232 Kmety, C. R., 109(258) Knaupp, M., 94(229) Knigavko, A., 154(360) Knoester, J., 100(245)

AUTHOR INDEX Knopoff, L., 277(250) Kobayashi, T., 127(298) Kobayashi, T. C., 127(297) Kocks, U. F., 260(172), 261 Koepernik, K., 51(142) Koga, A., 48(133) Kohgi, M., 11(32), 74(197), 77(200), 79(202), 80, 90(217) Koike, Y., 49(136) Koitzsch, A., 21(76) Kok, S., 283(270) Komatsubara, T., 49(136, 137), 60(169, 170, 172) Kondakov, D. E., 48(132) Kondo, S., 11, 14–17, 21, 32, 38–43, 45, 46, 74, 76, 79, 117, 120, 123(282), 126(291, 293), 132, 179 Kondoh, Y., 225(92) Konno, R., 28(91) Köppen, M., 87(215), 95(235) Korbel, A. S., 270(227) Korotin, M. A., 125(290), 131(303) Koshizuka, N., 155(363) Koslowski, A., 135(311) Kotegawa, H., 127(297) Kotliar, G., 69(186), 159(368), 164(394) Kovacs, I., 262(183) Kovrizhin, D., 38(117) Koyama, I., 113(263) Krämer, K., 38(115) Krane, H. G., 94(230) Kratochvil, J., 272 Krauth, W., 69(186) Kremer, R. K., 94(229), 95(236), 97(240) Krimmel, A., 60(171) Krishan, K., 249(152), 253(153) Krishna-murthy, H. -R., 16(56, 57) Krishnamurthy, H. R., 159(367) Krivnov, V. Y., 91(221) Kroha, J., 16(55) Krumhansl, J. A., 153(342) Kubin, L., 277(253) Kubin, L. P., 258, 261(176, 181, 182), 263(185, 186), 264(190–193, 196, 197), 267(216, 218, 220), 268(223, 224, 226), 274(240, 241, 245, 247), 275(248, 249), 282(258), 283(265–270) Kubota, M., 117(271), 121(279) Küchler, R., 39(119)

295

Kudasov, Y., 81(205) Kuhlmann-Wilsdorf, D., 255(160), 260(168–171) Kulcinski, G. L., 249(144) Kumai, R., 113(262) Kuramoto, Y., 15(51) Kurushima, K., 139(316) Kurz, W., 182(4) Kusaba, T., 235(121) Kusunose, H., 132(307) Kuwahara, H., 114(266) L Laad, M. S., 48(135), 131(304) Labbé, J., 81(208) Lacerda, A., 47(130) Lacroix, C., 11(34), 131(305), 132(306) Landau, L. D., 7, 9–11, 13, 18, 32, 45, 47, 76, 87, 148 Lander, G. H., 49(136), 60(169, 170) Lang, I. G., 115 Lang, M., 23(82, 83), 74(197), 86(213), 87(215), 90(217), 95(235) Langari, A., 101(246) Langer, J. S., 182, 277 Langhammer, C., 23(82, 83), 74(197) Lanzara, A., 154(357, 359), 162(380) Larche, F., 185(16) Laughlin, R. B., 13(40), 146 Lauzeral, J., 253(158) Le Chatelier, H., 184, 187, 273, 274, 282, 286 Leath, P. L., 153(342) Lebowitz, J., 185(15) Lebyodkin, M., 275(249), 277(253), 283(268–270) Lebyodkin, M. A., 275(248) Lee, B. -W., 17(66) Lee, D. -H., 162(380) Lejay, P., 20(70), 47(130) Lemarchand, H., 182(7) Lemmens, P., 96(237) Lendvai, J., 243(135) Leonov, I., 125(290), 136(313) Lepinoux, J., 235(124, 125), 239(129, 130), 242(133), 261(176), 263(186, 187), 267(216, 218, 220), 268(223, 224) Levin, M., 140(321)

296

AUTHOR INDEX

Lhuillier, C., 146(329) Li, J. Q., 113(262) Li, Q., 155(363) Li, Y. M., 75(198), 85(212) Lichtenstein, A. I., 164(394) Lieb, E., 36(112), 85 Liebsch, A., 48(134), 164(385, 386) Liecke, W., 2(2) Lifshits, I. M., 23(81) Link, A., 23(82) Littlewood, P. B., 13(46, 47), 160(374) Liu, Y. C., 198(53) Livet, F., 243(138) Livingston, J. D., 230, 231 Loewenhaupt, R., 22(79) Loh, E., 59(158) Löhneysen, H. v., 34(108) Loidl, A., 60(171), 127(296) London, F., 3 Longinotti, L. D., 59(156) Lonzarich, G. G., 17(63, 65), 20(74, 75), 34(108), 39(118), 59(164–166) Lorenz, B., 125(289) Lorenzo, J. E., 103(247) Lorimer, G. W., 225(93) Louat, N. P., 236, 237 Louchet, F., 184(12) Lozovik, Y. E., 67(185) Lu, D. H., 154(358) Lu, E. D., 154(357) Lüdecke, J., 94(230, 231) Luengo, C. A., 59(157), 124(284) Lühmann, T., 23(83), 38(117) Luther, A., 13(44), 59(153) Lüthi, B., 24(84), 46(126), 78(201), 135(311) Luttinger, J. M., 10, 12, 17, 160 M Machida, A., 133(310) Machida, K., 28(92) Mack, F., 93(228) Mackintosh, A. R., 35(111), 62(176) Madec, R., 264(197) Maekawa, S., 117(271), 174(409) Maezawa, K., 66(183) Magnin, T., 268(223, 224) Mahajan, A. V., 126(291)

Maier, T., 159(369) Maier, T. A., 160(373) Maitra, J. P., 59(156, 157) Maki, K., 65(181) Maletta, H., 60(171) Malygin, G., 261(179, 180) Mancini, F., 6(23) Manna, I., 193(32), 196, 230 Maple, M. B., 17(66, 67), 59(157), 124(284), 126(291) Maradudin, A. A., 70(189) Marchionni, C., 184(12) Marsiglio, F., 154(360) Martin, G., 184(10, 11), 249(140, 141), 255(159) Martin-Delgado, M. A., 101(246) Mason, T. E., 62(177) Massoud, J. P., 249(142) Mathur, N. D., 39(118) Matsuda, Y., 65(181), 66(182) Matsui, Y., 113(262) Matsumoto, H., 164(392) Matsumoto, M., 38(116) Matsuno, J., 127(294), 133(310) Mattheiss, L. F., 127(294) Matthias, B. T., 34(107) Mattis, D., 36(112) Mattis, D. C., 81(207) Mattix, L., 59(157) Maurice, C., 235(123) Maxwell, E., 59(149) Mayer, H. M., 20(69) Mazey, D. J., 249(149) Mazin, I. I., 127(295) Mazur, P., 188(24) McCallum, R. W., 59(157), 124(284) McElroy, D. L., 209(78) McEwen, K. A., 35(110) McGovern, S., 267(217) McHale, P., 63(180) McIntyre, G. J., 113(265), 119(272) McMahan, A. K., 17(59) McMullen, G. J., 17(65), 20(74) McMurry, S., 186(19), 235 McNelley, T. R., 240(131) McQueen, H. J., 240(131) Medrick, K., 165(398) Meetsma, S. A., 94(232) Mehl, R. F., 206(75), 209(77)

AUTHOR INDEX Mehring, M., 95(236) Menovsky, A., 24(84) Meschede, D., 2(2) Metoki, N., 49(136) Metzner, W., 154(350) Meyrick, G., 196(40) Michael, J., 196(41) Mignot, J. -M., 11(32), 79(202), 90(217) Miller, L. L., 123(282), 126(291) Millis, A. J., 48(131) Misguish, G., 146(329) Mishin, Y., 193(34) Mitchell, J. F., 109(258) Mittemeijer, E. J., 193(33) Miyake, K., 59(159), 132(307) Miyake, K. ., 49(137) Miyoshi, K., 127(297, 298) Mizuta, M., 50(139) Moessner, R., 146(326) Monthoux, P., 59(163–166) Moodenbaugh, A. R., 155(363) Moore, D. P., 50(141) Morales, L. A., 50(141) Moreo, A., 122(281) Mori, H., 150(334) Mori, S., 124(285), 133(310), 139(316) Moritomo, Y., 108(255), 113(263), 114(266), 117(271), 121(279), 133(310) Moriya, T., 14, 34, 59(162), 88, 179 Morré, E., 94(230), 105(252) Mostovoy, M. V., 100(245) Motome, Y., 139(316) Motrunich, O. I., 146(328) Mott, N. F., 2, 68, 69, 74, 98, 108, 111 Mughrabi, H., 262(184), 267(214–217, 219) Mukherjee, M., 159(367) Müller, G., 79(204), 91(219) Müller, K. A., 2(5) Müller-Hartmann, E., 48(135), 131(304), 154(351) Muller-Krumbhaar, H., 182(4) Mullins, W. W., 218, 227, 228, 235(114), 236 Murakami, Y., 94(233), 103(249), 113(263) Muraoka, K. Y. J., 103(249) Murata, K. K., 14(49) Murphy, S. M., 253 Mutka, H., 38(115) Mydosh, J. A., 34(103, 104), 39(119)

297 N

Nagaosa, N., 154(358, 359, 361) Nakajima, K., 103(248) Nakajima, N., 77(200) Nakao, H., 94(233), 103(249) Needleman, A., 264(195), 265(198–202) Neef, M., 26(86, 87) Nekrasov, I. A., 48(132) Nelson, D. R., 71(190) Nemoto, Y., 76(199) Nersesyan, A. A., 12(37) Nesbitt, L. B., 59(150) Neuhauser, H., 283(265), 284(272) Neumaier, K., 39(119, 120) Nichols, F. A., 227(97) Nicolay, G., 16(55) Nicolis, G., 182(5) Niksch, M., 46(126) Ninomiya, E., 94(233), 103(249) Nishi, M., 103(248) Nishibori, E., 133(310) Noda, Y., 94(233) Nohara, M., 126(293) Nohdo, S., 115(268) Norman, M. R., 155(362, 364), 163(381) Normand, B., 38(116) Noronha, S. J., 282(258), 283(266, 267) Nücker, N., 174(410) O Ochiai, A., 11(32), 13(43), 74, 76(199), 77(200), 79(202), 84(209), 85(210, 211), 86(213), 90(217), 138(315) Oeschler, N., 39(119) Ohama, T., 94(233) Ohishi, Y., 127(297) Ohm, T., 164(395) Ohoyama, K., 121(279) Ohwada, K., 94(233), 103(249) Okane, T., 50(139) Okazaki, K., 108(254) Okubo, T., 126(293) Okumura, T., 225(92) Ole´s, A., 5(14), 165(399) Olson, C. G., 17(66, 67)

298

AUTHOR INDEX

Onuki, Y., 17(64), 20(72, 73), 52(143), 65(181), 66(183) Opahle, I., 51(142) Oppeneer, P. M., 13(45), 51(142) Osborn, R., 22(77) Osumi, H., 77(200) Ott, H. R., 2 Ouchni, F., 119(276) Ovchinnikov, A., 81(205) Ovchinnikov, A. A., 91(221) Ozaki, M., 28(92) P Pabi, S. K., 193(32), 196(36) Pallson, G., 159(368) Palstra, T. T. M., 94(232) Pande, C. S., 196(42) Pankert, D., 87(215), 95(235) Pankov, S., 73(194) Paschen, S., 74(197) Patterson, B. D., 84(209), 138(315) Patterson, B. R., 234(111) Paul, I., 73(194) Paulus, B., 154(354) Pawlowski, A., 196 Pearson, J. J., 79 Penc, K., 140(318) Penn, D. R., 164(384) Penning, P., 274(242), 278 Penrose, O., 185(15) Pepin, C., 39(120) Perkins, N. B., 121(280) Perlov, A. Y., 13(45) Perovic, A., 197(43) Perring, T. G., 119(274) Peschel, I., 13(44) Petermann, J., 198(56) Petit, L., 50(140) Peuchert, U., 97(238) Pfeuty, P., 36(113) Pfleiderer, C., 34(108) Pharr, G. M., 256(164) Pincus, P., 92(222) Pines, D., 59(163) Pinettes, C., 11(34) Pink, E., 274(246) Plakida, N. M., 59(167) Planes, J., 283(265)

Platzmann, P. M., 70(188) Plessing, J., 283(265) Plummer, E. W., 147(332) Pochet, P., 184(11) Pokor, C., 249(142) Pollmann, F., 56(146), 57(148), 140, 145(323), 146(324) Polyakov, A. M., 140(317) Pomeau, Y., 182(2) Pontikis, V., 264(192) Poppe, U., 20(69) Porter, D. A., 205(69) Pott, R., 46(126) Predel, B., 215(84), 219(88) Prelovsek, N. B., 42(123) Presura, C., 97(240) Preuss, R., 159(371) Prigogine, I., 182(5) Pruschke, T., 131(303), 154(352), 159(369), 160(373) Puls, M. P., 198(61, 62) Pulst, U., 22(78), 23(80) Purdy, G., 232(105–107) Purdy, G. R., 186(18), 196(39), 197(43), 198(66), 215 Pyka, N., 79(202) Pytte, E., 92(223) Q Qin, S., 91(220) Qiu, X., 109(258) Quaouire, L., 282(258) R Radu, T., 38(117) Raj, S. V., 256(164) Rajesh, S., 282(264) Ralph, B., 256(163) Ranzetta, G. V. T., 193(27) Rapp, M., 267(217) Rauchschwalbe, U., 20(69) Raw, G., 188(23) Rayleigh, Lord, 227 Razavi, F., 34(103) Rebizant, J., 171(403) Reese, M., 26(87), 57(148)

AUTHOR INDEX Regnault, L. P., 20(70), 103(247), 119(273, 275) Reich, D. N., 91(218) Reinert, F., 16(55) Revcolevschi, A., 103(247), 113(265), 119(272, 273, 275), 120(278) Reynolds, C. A., 59(150) Rhee, M., 264(194) Rhines, F. N., 234(111) Rice, T. M., 38(116), 48(132, 133), 108, 131(303), 173–176 Ridley, N., 193(29, 31), 207, 209(79) Riseborough, P. S., 127(296) Rizzi, E., 284(272) Robinson, M. T., 249(139) Roessli, B., 49(136), 60(169–171) Roll, U., 215(84) Rollett, A. D., 235(120), 240(131) Romberg, H., 174(410) Ronnpagel, D., 262(184) Rosch, A., 46(129) Rosenberg, M. J., 69(186) Rossat-Mignot, J., 20(70) Roth, G., 12(35), 97(238) Roth, L., 164(389) Ruckenstein, A., 13(46), 160(374) Rudigier, H., 2(3) Ruegg, C., 38(115) Runge, E., 13(42), 20(71), 57(147), 146(324) Ruvalds, J., 162(377) Ryum, N., 236, 239 S Sachdev, S., 32(93) Sahni, P. S., 235(118) Saito, Y., 50(139) Sakai, F., 126(293) Sakai, O., 81(206), 91(220) Sakata, M., 133(310) Sakurai, K., 52(143) Sarrao, J. L., 17(67) Sasagawa, T., 162(380) Sass, S. L., 249(148) Sato, K., 50(139) Sato, N., 23(83), 49(137), 50(139), 60(169, 170, 172) Sato, N. K., 49(136) Satoh, K., 20(72)

299

Savrasov, S., 159(368) Sawa, H., 94(233), 103(249) Sawatzky, G., 166(402) Saxlova, M., 272(235, 236) Scalapino, D. J., 59(158), 159(370) Scalettar, R. T., 17(59) Scattergood, R. O., 260(172) Schachinger, E., 155(365) Schäfer, H., 2(2) Schank, C., 60(171) Schefzyk, R., 46(126) Scheil, E., 198(46), 203 Schilling, J. S., 34(103) Schilling, W., 249(143, 151) Schlesinger, Z., 161(376) Schlüter, M., 172(405) Schmidt, B., 11(31), 42(124), 74(197), 87(215, 216) Schmidt, S., 16(55) Schmidt, W., 119(275) Schmidt-Rink, S., 59(159) Schmitt-Rink, S., 13(46), 160(374) Schneider, R., 120(278) Schreiner, T., 12(35) Schrieffer, J. R., 12(38, 39), 33(97), 152(336) Schultz, T., 36(112) Schulze-Briese, C., 84(209), 138(315) Schwartz, L. M., 153(343) Schwarz, K., 127(295) Schwedler, A. R., 59(157) Schweitzer, H., 162(378) Schwenk, H., 135(311) Seki, M., 50(139) Seki, S., 164(392) Senthil, T., 146(328) Seo, Y., 225(92) Serin, B., 59(150) Shannon, N., 109(259), 119(276), 140(318) Shapiro, J. M., 198(55) Shen, Z. -X., 154(358, 359) Shi, M., 84(209), 138(315) Shiba, H., 81(206), 91(220) Shiflet, G. J., 197(44), 211(81) Shiina, R., 49(137) Shimaoka, Y., 127(298) Shimizu, K., 127(297) Shimizu, M., 154(347) Shimizu, T., 20(72)

300

AUTHOR INDEX

Shingu, M., 139(316) Shiraki, T., 126(293) Shu, J. Y., 265(201) Shvindlerman, L. S., 235(117) Si, Q., 39(119), 46(129) Sigrist, M., 28(90), 38(116), 48(132, 133) Simon, J. P., 243(138) Simoyama, J. -I., 154(357) Singh, D. J., 127(295) Skalski, S., 34(104) Slater, J. C., 6, 72 Smith, J. L., 2(3, 4), 34(106) Smolinsky, H., 97(238) Soderholm, L., 84(209), 138(315) Solorzano, G., 219(88) Solorzano, I. G., 196(39), 215 Somer, M., 94(229) Sommerfeld, A., 8, 76, 81, 87, 126, 130, 132 Sondhi, S. L., 146(326) Soven, P., 153(338) Spalek, J., 59(161) Spanjaard, D., 164(382, 383) Sparn, G., 16(54), 20(69), 23(82, 83), 105(252) Srolovitz, D. J., 235(118–120) Staker, M. R., 256(162) Stansbury, E. E., 209(78) Staub, U., 84(209), 138(315) Steglich, F., 2(2), 16(54), 20(69), 22(79), 23(82, 83), 38(117), 39(119, 120), 49(137), 60(171), 85(211), 86(213), 87(215), 95(235), 96(237) Steiner, M. J., 39(118) Stewart, G. R., 2(4) Stiegler, J. O., 249(150) Stirling, W. G., 35(110) Stockert, O., 16(54), 22(79) Stoll, H., 154(354), 159(366) Stollhoff, G., 165(399–401) Stoner, E., 32–34 Stuesser, N., 22(79) Su, W. P., 12(38, 39) Sundquist, B. E., 198(54, 58, 63), 212 Suryanarayanan, R., 113(265), 119(272, 273, 275), 120(278) Sutton, A. P., 234(110) Suzuki, T., 11(32), 13(43), 79(202), 85(210, 211), 90(217) Svane, A., 50(140)

Swenson, C. A., 126(291) Szotek, Z., 50(140) T Tachiki, M., 164(392) Tajima, K., 77(200) Takagi, H., 126(293), 133(310), 162(380) Takahashi, Y., 59(162) Takata, M., 133(310) Takeda, K., 127(297) Takens, F., 282(257) Takeuchi, J., 127(297, 298) Takke, R., 46(126) Tamura, K., 50(139) Tanaka, A., 50(139) Tanaka, R., 225(92) Tanatar, B., 71(191) Tang, C., 280(254, 255) Tautz, F. S., 17(65), 20(74) Tayama, T., 23(83) Taylor, D. W., 153(339) Tegus, O., 39(119) Temmerman, W. M., 50(140) Terasaki, I., 92(225) Thalmeier, P., 11(31), 13(45), 16(53, 54), 24(84), 37(114), 42(124), 46(127), 49(137), 61(174), 62(179), 63(180), 65(181), 66(182), 87(215, 216), 97(239), 99(242–244), 101(246), 106(253), 110(261), 114(267), 119(272, 273, 275, 276), 137(314), 144(322), 165(400) Thomas, H., 91(219) Thompson, C. V., 186(20), 235 Tohyama, T., 174(409) Tokiwa, Y., 39(120), 52(143) Tokura, Y., 6(22), 108(255), 113(262, 263), 114(266), 119(274) Tomioka, Y., 114(266) Toth, L. S., 262(183) Tou, H., 66(183) Tran, M. -T., 144(322) Treaftis, H. N., 201(67) Treglia, G., 164(382, 383) Trovarelli, O., 16(55), 39(120) Tsakiropoulos, P., 193(30) Tsuda, N., 135(312) Tsvelik, A. N., 12(37) Tu, J. J., 155(365)

AUTHOR INDEX Tu, K. -N., 198(52) Turnbull, D., 198(48, 52), 201–203, 235(113) Tyer, R., 50(140)

301

Vollmer, R., 34(108) von der Linden, W., 159(371) von Schnering, H. G., 94(229) Voorhees, P. W., 185(13), 229(103) Vorderwisch, P., 38(115), 119(275)

U W Uchinokura, K., 92(225) Ueda, K., 28(90, 91), 59(162), 81(206), 91(220), 132(308) Ueda, Y., 92(226), 94(233), 103(248, 249), 105(251), 108(254) Uhlarz, M., 34(108) Uimin, G., 81(205) Uji, S., 17(64), 20(72, 73) Umehara, I., 20(72) Umezawa, L., 164(392) Umstätter, R., 164(395) Ungar, T., 262(183, 184) Unger, P., 164(396, 397), 174(407, 408) Urabe, T., 225(93) Urano, C., 126(293) V Valenti, R., 105(250) Valla, T., 155(363) Valsakumar, M. C., 282(259, 260) van de Kamp, R., 119(272, 275) Van der Giessen, E., 264(195), 265(198, 200–202) van der Marel, D., 97(240), 166(402) van der Merwe, A., 188(23) van Smaalen, S., 94(230, 231) Varelogiannis, G., 49(137) Varma, C. M., 13(46, 47), 16(58), 59(159), 160(374) Vaughan, G. B. M., 84(209), 138(315) Velický, B., 153(340) Verdier, M., 243(134–138) Verga, S., 154(360) Vergergaugry, J. L., 184(12) Vergnol, J., 274(245), 283(265) Verwey, E. J. W., 3, 124, 125 Victora, R. H., 164(393) Vidal, C., 182(2, 7) Virosztek, A., 162(377) Vleck, J. H. V., 6 Vollhardt, D., 154(350)

Wagner, R., 185(13) Waintal, X., 71(192) Wakabayashi, N., 77(200) Wakabayashi, Y., 113(263) Walgraef, D., 182(6), 253, 261(175), 270, 271 Walker, I. R., 39(118) Walz, F., 125(287) Wand, B., 87(215) Wang, R., 267(217) Ward, J. C., 10(30) Wastin, F., 171(403) Watanabe, K. I. T., 65(181) Watanabe, T., 66(182) Weaire, D., 186(19), 235 Weatherly, G. C., 196(39) Weber, D., 24(84) Weber, W., 97(238), 164(395) Weickert, F., 24(85) Weiden, M., 94(229), 95(235), 96(237), 97(238) Weiser, S., 164(395) Weissmann, S., 255(161) Wells, B. O., 155(363) Wen, X. -G., 140(321) Werner, E., 227 Wertheim, G. K., 147(331) West, D. F. R., 193(27, 28) Weygand, D., 235(124, 125), 238(128), 239(129, 130), 242(133), 264(195) White, R., 53(144) White, S. R., 159(370) Whiting, M. J., 193(30) Wiesenfeld, K., 280(254, 255) Wigner, E., 3, 7, 40, 66–74, 91, 108, 177, 179 Wildes, A., 38(115) Wilhelm, H., 38(117), 39(120) Wilkens, M., 262(184) Wilkins, J. W., 16(56, 57) Williams, D. B., 196(38, 41)

302

AUTHOR INDEX

Willis, J. O., 2(4) Wills, J. M., 50(141) Winter, A. T., 267(212, 213) Wohlleben, D. K., 46(126) Wolf, B., 24(84) Woods, S. B., 76, 126 Wright, W. H., 59(150) Y Yamada, Y., 115(268) Yamagami, H., 17(67) Yamagani, H., 52(143) Yamaki, K., 50(139) Yamamoto, E., 52(143), 66(183) Yamamoto, N., 133(310) Yamashita, Y., 132(308) Yamauchi, T., 108(254) Yanagisawa, T., 52(143) Yaresko, A., 136(313), 137(314) Yaresko, A. N., 13(45), 97(239), 125(290), 129(299) Yonezawa, F., 153(341) Yoshitake, R., 77(200) Yoshizawa, H., 117(271), 121(279) Yosihama, T., 103(248) Yotsuhashi, S., 132(307) Yourgrau, W., 188(23) Yu, L., 40(122) Yuan, Q., 114(267) Yunoki, S., 122(281) Yushankhai, V., 37(114), 38(117), 144(322) Yusof, Z., 155(363)

Z Zaanen, J., 5(14) Zaiser, M., 258(165), 266(204, 207–210), 267 Zawadowski, A., 15(52) Zbib, H. M., 264(194) Zener, C., 108(256), 198–203, 208–210, 215, 239 Zerec, I., 42(124) Zevin, V., 12(36) Zhang, F. C., 108, 173–176 Zhang, G. M., 40(122) Zhang, Y. Z., 137(314), 144(322) Zheng, H., 115(270) Zheng, W. J., 154(357) Zhou, S. Y., 162(380) Zhou, X. J., 154(357, 358) Zhu, L., 39(119), 46(129) Zieba, P., 196, 202(68), 205(70–73) Ziegenbein, A., 284(272) Ziman, T., 103(247) Zimanyi, G. T., 160(375) Zinkle, S. J., 253(155) Zölfl, M., 131(303) Zvyagin, A. A., 129(299) Zwanzig, R., 150(335) Zwicknagl, G., 9(29), 11(33), 12(36), 16(53, 54), 17(61), 18(68), 20(71), 22(78, 79), 26(87), 27(88, 89), 56(145, 146), 57(147, 148)

Subject Index

phase diagram, 112–114 physics of, 108–110 in 3D-valence elections, 67, 68 in homogeneous 2D electron systems, 69–74 original proposal, 66–67 quasi-1D spin excitations α -NaV2 O5 , 91–107 electronic structure, 97–98 Hubbard model, 98–99 Ising-spin Peierls model, 101–107 ITF model, 99–101 Jordan–Wigner mapping, 91–92 β-vanadium bronzes, 107–108 structural phase transition, 92–93 temperature structure, 93–97 Wigner crystallization 4f model Hamiltonian, 81–87 Dzyaloshinsky–Moriya interaction, 88–91 experimental summary, 74–76 Labbé–Friedel model, 81 underlying physics, 77–81 Chemical patterning characterization, 185–186, 192–193 coarsening discontinuous, 230–231 overview, 225, 227 spheroidization, 227–230 discontinuous precipitation characterization, 194–196 divergent lamellar growth, 224–225 interface motion, 219–220 multilayer stability, 232 spacing selection, 216, 218 morphological evolution, 225, 227–230 non-steady state growth concerns, 218–219 divergent lamellar, 220–222, 224–225 interface motion, 219–220 spacing selection, 213, 215–218 steady state growth Cahn’s treatment, 204–206 discontinuous precipitation, 211–213

A AF structures, 60–61 ALV2 O4 characterization, 133–134 charge disproportionation, 136–139 structural transitions, 134–136 V ions, 134 α -NaV2 O5 coupled CO, 98–107 crystal structure, 94–95 electronic structure, 97–98 exchange dimerization in, 98–107 ground state, 91 Jordan–Winger mapping, 91–92 structural phase transition, 92–93 temperature structure, 93–97 B Bands persistent slip, 268–272 shadow, 151–153 theory, 18–19 BEC. See Bose–Einstein condensation Bilayer manganites. See Double exchange bilayer manganites Bose–Einstein condensation, 38 C Cahn’s treatment, 204–206 CeCu2 Si2 heavy fermions, 19–23 phase diagram, 23–30 CEF. See Crystalline electric fields CeRu2 Si2 , 19–23 Charge ordering 4f compounds, 67–68 concept of, 66 density in metals, 68–69 double exchange bilayer manganites as function of eg , 110–112 model, 117–122 303

304

SUBJECT INDEX

Chemical pattering (Continued) Hillbert’s treatment, 202–203 pearlite observations, 206–211 theoretical history, 197–199 Turnbull’s treatment, 202–203 Zener treatment, 199–202 transformations -discontinuous precipitation, comparison, 198–199 characterization, 193–195 divergent lamellar growth, 220–222, 224 experimental observations, 206–207 Fe-C steels, 208–208 identification, 196 multilayer stability, 232 regularity of, 193, 197 steady state growth, 206–211 CMR. See Colossal magnetoresistance effect Co-Si system, 230–231 Coarsening discontinuous, 230–231 overview, 225, 227 spheroidization, 227–230 Coherent potential approximation, 153–154 Colossal magnetoresistance effect, 108 Condensation, Bose–Einstein, 38 Cooper pairs, 59 Copper-oxide planes, 171–176 Correlated systems with orbital degeneracies, 48–51 CPA. See Coherent potential approximation Creation operators, 26–27 Crystalline electric fields characterization, 15 doublet-quartet scheme, 23, 35 in rare earth ions, 59 singlet states, 36–38 Crystallization. See Wigner crystallization Cu-Al systems, 206–207 Cuprates perovskite structures, 13–14 D Discontinuous precipitation -transformation, comparison, 198–199 chemical patterning characterization, 194–195 identification, 196

interface motion, 219–220 Klinger’s alternative, 216, 218 theory/experiment comparisons, 211–213 divergent lamellar growth, 224–225 Dislocations characterization, 233–234 patterning cell formation, 258 dynamic nature of, 261–262 first theory, 260 Hähner model, 266–267 Holt model, 260–261 Kocks model, 261 structures carpets, 249, 252 density of, 245 in PSB, 268–272 recovery density decreases, 245 kinetics, 243 processes, 243 study results, 248 recrystallization evolution of, 240–241 nucleation of, 241–243 study results, 248 void lattices, 249, 252 Divergent lamellar growth, 220–222, 224 Double exchange bilayer manganites reentrant charge ordering as function of eg , 110–112 electronic structure calculations, 110 model, 117–122 phase diagram, 112–114 physics of, 108–110 polaron formation, 114–117 structural properties, 109–110 Dynamical mean field theory, 17 Dzyaloshinsky–Moriya interaction, 88–91 E Elastic strains, 190 Energy chemical, 188–189 free, 77–78 free energy, 189–191

SUBJECT INDEX high (See High-energy excitations) interfacial, 190–191 low, scales, 10–12 madelung, 87 strain, 190 Equilibrium systems maintained far from, 191–192 systems prepared far from chemical energy, 188–189 interfacial energy, 190–191 strain energy, 190 structural patterning in, 186–187 Eutectoid decomposition, 220–222, 224–225

F Fatigue loading, 267–268, 270–272 Fault migration, 229 Fe-C steels, 208–208 Fe-C-Mn systems, 222, 224 Fe-C-Mo systems, 222, 224 Fe-C-Si systems, 222, 224 Fe3 /O4 , 124–125, 130 Fermi-liquid state CeCu2 Si2 , 19–23 CeRu2 Si2 , 19–23 high-energy excitations combined models, 153–154 findings, 159–163 methodology, 154–159 mean-field theory, 16–17 renormalized band theory, 18–19 strongly correlated electrons deviations, 12–14 Wigner crystallization, 69, 71 Fermions, heavy, 19–23 Five f systems, 168–171 Free energy at phase/grain boundary interface, 190–191 elastic strain-induced, 190 strain-free regions, 189 Free energy changes systems continuously maintained, 191–192 systems preparation characterization, 188–189 chemical energy, 189

305 interfacial energy, 190–191 strain energy, 190 G

Geometrically frustrated lattices characterization, 123 charge disproportionation, 133–139 fractional charges, 139–147 function, 122–123 metallic spinels, 124–133 structural transition, 133–139 Grain growth characterization, 234 computer models, 235–236 experiments, 234–235 log normal distributions, 236–240 Green function, 7–8 H Hähner model, 266–267 Heavy quasiparticles in U compounds dual model application, 51–54 dual model theory, 50–51 superconductivity, 59–66 High-energy excitations copper-oxide planes, 171–176 energies, 147–148 Hubbard model, 151–153 in 5f systems, multiplet effects, 168–171 kink structure, 153–163, 154–159 marginal Fermi liquid behavior combined models, 153–154 findings, 159–163 methodology, 154–159 Ni satellite structure, 163–168 projection operators, 148, 149–150 research summary, 176–178 zero-point fluctuations, 149 Hillbert’s treatment, 202–203 Holt model, 260–261 Hubbard model for high-energy excitations, 151–153 quasi-1D spin excitations, 98–99 Hückel theory, 3

306

SUBJECT INDEX I

Interatomic correlations, 3–4 Interface motion, 219–220 Interfaces at phases/grain boundaries, 190–191 Intra-atomic correlations function, 4 in superconductivity, 59–66 strength measure, 5–6 Irradiation main effect of, 252 rate equations, 253 structural defect patterning experimental characteristics, 249, 252 rate equations, 253 reaction diffusion approach, 252–255 void formation, 254–255, 258 Ising model in transverse field, 99–101 ITF. See Ising model in transverse field Itinerant ferromagnetism models, 32–37

Lamellar patterning characterization, 225, 227 discontinuous precipitation, 224–225 pearlite, 220–222, 224 spheroidization, 227–230 LaMnO3 electronic structure calculations, 110 physics, 108 structural properties, 109–110 Landau theory, 9–10 LaSr2 Mn2 O2 electronic structure calculations, 110 physics of, 108 structural properties, 109–110 LDA. See Local density approximations Line defects. See Dislocations LiV3 /O4 , 125–133 Local density approximations, 51 Log normal distributions, 236–240 Low-energy scales, 10–12

J M Jordan–Wigner transformation, 91–92 K Kink excitations, 12–13 Kink structure, 153–163 Klinger’s alternative, 216, 218 Kocks model, 261 Kondo lattice systems Ce-based compounds, 15–16 CeCu2 Si2 , 19–23 CeRu2 Si2 , 19–23 Fermi-liquid state, 18–19 function, 14–15 heavy fermions, 19–23 heavy quasiparticles, 18–19 magnetic ions, 16–17 quantum criticality in, 38–45 renormalized band theory, 18–19 scaling theory, 45–48 Kondo necklace model, 40 L Labbé–Friedel model, 81 Lamellar growth, divergent, 220–222, 224

Madelung energy, 87 Magnetic ion lattice, 16–17 Magnets, itinerant, 32–38 Magnets, localized, 32–38 Manganites. See Double exchange bilayer manganites Metallic spinels Fe3 /O4 , 124–125 LiV3 /O4 , 125–133 Metals. See also specific metals density in, charge ordering, 68–69 Landau theory, 9–10 quasiparticle energies, 8–9 transitions, 6 N Nickel satellite structure, 163–168 Non-steady state growth chemical patterning concerns, 218–219 divergent lamellar, 220–222, 224–225 interface motion, 219–220

SUBJECT INDEX O Orbital degeneracies in correlated systems dual model, 49–51 examples, 48–49 P Partial localization concept of, 48–49 in U compounds heavy quasiparticles in, 51–54 LDA, 51 microscopic model calculations, 54–58 Patterns Belgian school, 182–183 chemical (See Chemical patterning) concept of, 182 energetic costs, 183 equilibrium departure, 184 in metallic alloys, 183–184 spatio-temporal (See Spatio-temporal patterning) structural (See Structural defect patterning) Pearlite transformations -discontinuous precipitation, comparison, 198–199 characterization, 193–195 divergent lamellar growth, 220–222, 224 experimental observations, 206–207 Fe-C steels, 208–208 identification, 196 regularity of, 193, 197 steady state growth, 206–211 Persistent slip bands, 268–272 Phase diagrams CeCu2 Si2 , 23–30 charge ordering, 112–114 Phase transitions CeCu2 Si2 , 23–30 free energy, 190–191 quantum broken symmetry state, 30–32 in itinerant magnets, 32–38 in localized magnets, 32–38 structural, 92–93 Plasticity in structural defect patterning

307

classical approaches, 258, 260–263 computer simulations, 263–266 experimental facts, 255–256 fatigue loading, 267–268, 270–272 spatio-temporal patterning in chaotic behavior of, 282–284 characterization, 273–274 phenomenology of, 274–276 serrated flow, statistical analysis, 276–280 stress-strain curve, 187 PLC. See Portevin–Chatelier effect Polarons formation in double exchange bilayer manganites, 114–117 hopping element, 116 JT type, 115 Polyacethylene, 12–13 Portevin–Chatelier effect chaotic behavior of, 282–284 characterization, 273–274 phenomenology of, 274–276 serrated flow, statistical analysis, 276–280 PSB. See Persistent slip bands Pyrochlore lattice band structure, 127–128 characterization, 123 spin degrees of freedom, 129 Q QCP. See Quantum critical point QCT. See Quantum phase transitions QPC. See Quantum critical point Quantum critical point non-Fermi behavior in, 14 QPT in, 31 scaling theory, 45–48 Quantum criticality, 38–45 Quantum phase transitions broken symmetry state, 30–32, 31–32 in itinerant magnets, 32–38 in localized magnets, 32–38 onset of, 35–36 Quasi-1D spin excitations charge ordering α -NaV2 O5 , 91–107 electronic structure, 97–98 Hubbard model, 98–99

308

SUBJECT INDEX

Quasi-1D spin excitations (Continued) ITF model, 99–101 β-vanadium bronzes, 107–108 structural phase transition, 92–93 temperature structure, 93–97 Ising-spin Peierls model, 101–107 Jordan–Wigner mapping, 91–92 Quasiparticles. See Heavy quasiparticles R Raleigh instability, 227–228 Rate equations, 253 Reaction diffusion approach, 252–255 Recrystallization, 240–243 S β-Vanadium bronzes, 107–108 SDW. See Spin-density wave Self organized criticality, 276–280 Serrated flow, 276–280 Shadow bands, 151–153 SOC. See Self organized criticality Spacing selection chemical patterning discontinuous precipitation, 216, 218 problems, 213, 215–218 Spatio-temporal patterning PLC effect chaotic behavior of, 282–284 characterization, 273–274 phenomenology of, 274–276 serrated flow, statistical analysis, 276–280 stress-strain curve, 187 Spheroidization, 227–230 Spin excitations. See Quasi-1D spin excitations Spin-change separation, 12–13 Spin-density wave, 24 Steady state growth. See also Non-steady state growth chemical patterning Cahn’s treatment, 204–206 discontinuous precipitation, 211–213 Hillbert’s treatment, 202–203 pearlite observations, 206–211 theoretical history, 197–199

Turnbull’s treatment, 202–203 Zener treatment, 199–202 Stick-slip model, 277, 279 Stoner–Wolfarth theory, 32 Strain energy, 190 Strain-free regions, 189 Strong correlations, 139–147 Strongly correlated electrons charge ordering α -NaV2 O5 , 91–108 concept of, 66–69 generalized Wigner lattice, 74–91 homogeneous 2D systems, 69–74 ID spin excitations, 91–108 reentrant, 108–122 Wigner crystallization, 69–74 Yb4 As3 , 74–91 Fermi-liquid behavior deviations, 12–14 geometrically frustrated lattices characterization, 122–124 charge disproportionation, 133–139 fractional changes, 139–147 metallic spinels, 124–133 structural transitions, 133–139 high-energy excitations 5f systems, 168–171 characterizations, 147–149 copper-oxide planes, 171–176 future research, 176–178 Hubbard model, 151–153 kink structure, 153–163 marginal Fermi liquid behavior, 153–163 Ni satellites, 163–168 projection operators, 149–150 shadow bands, 151–153 Kondo lattice systems band theory, 18–19 CeCu2 Si2 , 19–30 CeRu2 Si2 , 19–23 characterization, 14–18 Fermi-liquid state, 18–19 heavy fermions, 19–23 heavy quasiparticles, 18–19 low-temperature phase, 23–30 quantum criticality, 38–45 low-energy scales, 10–12 overview, 2–8 partial localization

SUBJECT INDEX characterization, 48–51 intra-atomic excitations, 59–66 microscopic model calculation, 54–59 quasiparticles, 51–54 superconductivity, 59–66 UPd2 Al3 , 51–54 quantum phase transitions characterization, 30–32 critical point, 45–48 criticality, 38–45 itinerant magnets, 32–38 localized magnets, 32–38 scaling theory, 45–48 theories, 8–10 Structural defect patterning characterization, 233–234 dislocation structures cold rolling stain, 245, 248 density of, 245, 248 evolution, 240–241 nucleation of, 241–243 recovery kinetics, 243, 248 recovery observations, 243 grain growth characterization, 234 computer models, 235–236 experiments, 234 Log Normal distributions, 236–240 irradiation-induced experimental characteristics, 249, 252 rate equations, 253 reaction diffusion approach, 252–255 void formation, 254–255 plasticity-induced classical approaches, 258, 260–263 computer simulations, 263–266 experimental facts, 255–256, 258 fatigue loading, 267–268, 270–272 Hähner model, 266–267 Structural patterning, 186–187 Structural transition, 133–139 Superconductivity A phase interplay, 24–26 CeCu2 S2 , 24–29 intra-atomic excitations, 59–66

309 T

Transformations. See Pearlite transformations Transitions metals, 6 Turnbull’s treatment, 202–203 U U compounds AF structures, 60 heavy quasiparticles dual model application, 51–54 dual model theory, 50–51 microscopic model calculations, 54–58 superconductivity, 59–66 V Void formation, 254–255 W Wigner crystallization charge ordering 4f model Hamiltonian, 81–87 Dzyaloshinsky–Moriya interaction, 88–91 experimental summary, 74–76 Labbé–Friedel model, 81 underlying physics, 77–81 in homogeneous 2D electrons, 69–74 Y Yb4 , change ordering 4f model Hamiltonian, 81–87 elastic constant, 78–80 free energy, 77–78 interacting chains, 81 lattice structure, 74–76 Madelung energy, 87 Z Zener treatment, 199–202

This page intentionally left blank

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close